D Y N A M I C
P LASTICITY
This page intentionally left blank
% : / " . * $
1 -"45*$*5: /%$SJTUFTDV 6OJWFSTJUZ...

Author:
N. D. Cristescu

This content was uploaded by our users and we assume good faith they have the permission to share this book. If you own the copyright to this book and it is wrongfully on our website, we offer a simple DMCA procedure to remove your content from our site. Start by pressing the button below!

D Y N A M I C

P LASTICITY

This page intentionally left blank

% : / " . * $

1 -"45*$*5: /%$SJTUFTDV 6OJWFSTJUZPG'MPSJEB 64"

World Scientiﬁc / & 8 + & 3 4 & : t - 0 / % 0 / t 4 * / ( " 1 0 3 & t # & * + * / ( t 4 ) " / ( ) " * t ) 0 / ( , 0 / ( t 5" * 1 & * t $ ) & / / " *

Published by World Scientific Publishing Co. Pte. Ltd. 5 Toh Tuck Link, Singapore 596224 USA office: 27 Warren Street, Suite 401-402, Hackensack, NJ 07601 UK office: 57 Shelton Street, Covent Garden, London WC2H 9HE

British Library Cataloguing-in-Publication Data A catalogue record for this book is available from the British Library.

DYNAMIC PLASTICITY Copyright © 2007 by World Scientific Publishing Co. Pte. Ltd. All rights reserved. This book, or parts thereof, may not be reproduced in any form or by any means, electronic or mechanical, including photocopying, recording or any information storage and retrieval system now known or to be invented, without written permission from the Publisher.

For photocopying of material in this volume, please pay a copying fee through the Copyright Clearance Center, Inc., 222 Rosewood Drive, Danvers, MA 01923, USA. In this case permission to photocopy is not required from the publisher.

ISBN-13 978-981-256-747-5 ISBN-10 981-256-747-X

Printed in Singapore.

YHwa - Dynamic Plasticity.pmd

1

12/26/2006, 11:42 AM

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

IN MEMORIAM I would like to mention, with all the sadness possible, the memory of my wife Cornelia, which disappeared meantime, and which helped me always so much.

v

dynamic

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

This page intentionally left blank

dynamic

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Preface

The present book is not simply a new addition of the book Dynamic Plasticity, initially published in 1967, a long time ago. Certainly this edition is not only a new version, containing the essential of the old book and what has been done meantime. Why again Dynamic Plasticity? Well because very many books published meantime on the subject are not mentioning the waves which are to be considered in Dynamic Plasticity. Also, generally, the plastic waves are slower than the elastic one. Thus, when considering a simple problem of propagation of waves in thin bars, for any loading at the end, the plastic waves are reached by the elastic ones, and will not propagate any more. Only a part of the bar is deforming plastically. Examples of this kind are very few. I thought that this new version is too restrictive for the today students which know little of static plasticity, diﬀerential equations, dynamic elastic–plastic properties, etc. Therefore, I thought to write a simpler book, containing the main concepts of dynamic plasticity, but also something else. Thus I thought that this new version would contain the elementary concepts of static plasticity, etc., which would be useful to give. Also it would be good to give other problems, not directly related to dynamic plasticity. Thus I started with some classical problems on static plasticity, but only the simplest things, so that the readers would afterwards understand also the dynamic problems. Also, since in dynamic problems the soils and rocks played a fundamental role, I thought to write a chapter on rocks and soils. Then were expressed several chapters about dynamic plasticity, as propagation of elastic–plastic waves in thin bars, the rate inﬂuence and the propagation of waves in ﬂexible strings. It is good to remember here that all problems related to dynamic problems, are to be considered using the mechanics of the wave propagation; without the wave propagation mechanics all results concerning constitutive equations, rate eﬀect, etc. are only informative. Such problems are mentioned however in the book. We have presented mainly the diﬀerent aspects on constitutive equations of materials, as resulting from dynamic problems. Rate eﬀects are considered in this way. They have been used by a variety of authors. The same with the mechanics of ﬂexible strings, presented afterwards. Not very many authors have considered till now the mechanics of deformable cables. vii

dynamic

January 12, 2007

viii

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Dynamic Plasticity

Therefore I thought to write a very simple book, which can be read by the students themselves, without any additional help. They can understand what “plasticity” is after all. Then several other problems have been presented. Not trying to remove the fundamentals, I have thought also to add some additional problems, which are in fact dynamic, though the inertia eﬀect is disregarded. They are the stationary problems, quite often met in many applications. It is question obviously, about problems involving Bingham bodies, as wire drawing, ﬂoating with working plug, extrusion, stability of natural inclined plane, etc. Further I have considered various problems of plastic waves, using various theories. Also the perforation problems, was presented, using various symmetry assumptions, or any other assumption made. The last chapter is on hypervelocity impact. To keep it simple, I have given only very few information about. Thus I wished to show what hypervelocity is and how is it considered now. Though the book is a very simple one, I wished to ask any author to disregard possible missing of some papers. All literature is certainly incomplete. One has done today much more than given here. It was impossible for me to mention “all” authors in this ﬁeld. N. D. Cristescu [email protected]ﬂ.edu

dynamic

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

dynamic

Contents

Preface

vii

Introduction 1 Diagnostic Tests . . . . . . . . . . . . . . . . . . . 2 Tests Performed at Long and Short Term Intervals 3 Long-Term Tests . . . . . . . . . . . . . . . . . . . 4 Temperature Inﬂuence . . . . . . . . . . . . . . . . 5 The Inﬂuence of the Hydrostatic Pressure . . . . . 6 Variation of Elastic Parameters with Plastic Strain

. . . . . . . . . . . . . . . . . . . . . . . . . (Metals)

. . . . . .

. . . . . .

. . . . . .

. . . . . .

1. Yield Conditions 1.1 1.2 1.3 1.4 1.5 1.6 1.7 1.8 1.9 1.10 1.11 1.12 1.13 1.14

15

Stresses . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Yield Conditions . . . . . . . . . . . . . . . . . . . . . . . . . . The Classical Constitutive Equation for Perfectly Plastic Materials . . . . . . . . . . . . . . . . . . . . . . . . . . Work-Hardening Materials . . . . . . . . . . . . . . . . . . . . . Isotropic Hardening . . . . . . . . . . . . . . . . . . . . . . . . The Universal Stress Strain Curve . . . . . . . . . . . . . . . . Constitutive Equation for Isotropic Work-Hardening Materials The Drucker’s Postulate . . . . . . . . . . . . . . . . . . . . . . Kinematical Work-Hardening . . . . . . . . . . . . . . . . . . . Further Developments . . . . . . . . . . . . . . . . . . . . . . . Experimental Tests . . . . . . . . . . . . . . . . . . . . . . . . . Viscoplasticity . . . . . . . . . . . . . . . . . . . . . . . . . . . Rate Type Constitutive Equations . . . . . . . . . . . . . . . . General Principles . . . . . . . . . . . . . . . . . . . . . . . . .

. . . .

15 19

. . . . . . . . . . . .

22 25 27 29 30 31 32 34 35 38 42 43

. . . . . . . . . . . .

2. Rocks and Soils 2.1 2.2

1 1 5 9 11 12 12

53

Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Experimental Foundation . . . . . . . . . . . . . . . . . . . . . . . ix

53 59

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

x

dynamic

Dynamic Plasticity

2.3 2.4 2.5 2.6

The Constitutive Equation Failure . . . . . . . . . . . . Examples . . . . . . . . . . Viscoelastic Model . . . . .

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

3. The Propagation of Longitudinal Stress Waves in Thin Bars 3.1 3.2 3.3 3.4 3.5 3.6 3.7

The Equation of Motion . . . . . . . . . . . . . . . . The Finite Constitutive Equation . . . . . . . . . . . The Unloading Problem . . . . . . . . . . . . . . . . Determination of the Loading/Unloading Boundary The Finite Bar . . . . . . . . . . . . . . . . . . . . . Examples . . . . . . . . . . . . . . . . . . . . . . . . The Elastic Solution . . . . . . . . . . . . . . . . . .

105 . . . . . . .

. . . . . . .

. . . . . . .

. . . . . . .

. . . . . . .

. . . . . . .

. . . . . . .

. . . . . . .

4. Rate Inﬂuence 4.1 4.2 4.3 4.4 4.5

Experimental Results . . . . . The Constitutive Equation . . Instantaneous Plastic Response Numerical Examples . . . . . . Other Papers . . . . . . . . . .

. . . . .

. . . . .

. . . . .

. . . . .

. . . . .

. . . . .

. . . . .

. . . . .

. . . . .

. . . . .

. . . . .

. . . . .

. . . . .

. . . . .

. . . . .

. . . . .

. . . . .

. . . . .

. . . . .

. . . . .

Introduction . . . . . . . . . . . . . . . . Equations of Motion . . . . . . . . . . . The Finite Constitutive Equation: Basic The Order of Propagation of Waves . . Boundary and Initial Conditions . . . . Numerical Examples . . . . . . . . . . . Rate Inﬂuence . . . . . . . . . . . . . . Shock Waves . . . . . . . . . . . . . . . Other Papers . . . . . . . . . . . . . . .

6.3 6.4

. . . . . . . . . . . . Formulae . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . .

. . . . . . . . .

. . . . . . . . .

. . . . . . . . .

. . . . . . . . .

Flow of a Bingham Fluid Through a Tube . . . . . . . . . . Flow of a Bingham Fluid Between Two Circular Concentric Cylinders (Reiner [1960]) . . . . . . . . . . . . . . . . . . . A Model for Slow Motion of Natural Slopes (Cristescu et al. [2002]) . . . . . . . . . . . . . . . . . . . . How to Measure the Viscosity and Yield Stress . . . . . . .

7. Axi-Symmetrical Problems 7.1

169 176 181 189 194 217

6. Flow of a Bigham Fluid 6.1 6.2

105 108 124 127 134 144 155 169

5. Mechanics of Extensible Strings 5.1 5.2 5.3 5.4 5.5 5.6 5.7 5.8 5.9

71 76 88 94

. . . . . . . . .

. . . . . . . . .

. . . . . . . . .

. . . . . . . . .

217 221 223 226 227 230 232 237 240 251

. . . . 251 . . . . 259 . . . . 268 . . . . 290 315

Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 315

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

dynamic

Contents

7.2 7.3 7.4

7.5

7.6

Enlargement of a Circular Oriﬁce . . . . . . . . . . Thin Wall Tube . . . . . . . . . . . . . . . . . . . . Wire Drawing . . . . . . . . . . . . . . . . . . . . . 7.4.1 Introduction . . . . . . . . . . . . . . . . . 7.4.2 Basic Equations . . . . . . . . . . . . . . . 7.4.3 Friction Laws . . . . . . . . . . . . . . . . 7.4.4 Drawing Stress . . . . . . . . . . . . . . . . 7.4.5 Comparison with Experimental Data . . . 7.4.6 Other Papers . . . . . . . . . . . . . . . . . Floating Plug . . . . . . . . . . . . . . . . . . . . . 7.5.1 Formulation of the Problem . . . . . . . . 7.5.2 Kinematics of the Deformation Process . . 7.5.3 Friction Forces . . . . . . . . . . . . . . . . 7.5.4 Determination of the Shape of the Floating 7.5.5 The Drawing Force . . . . . . . . . . . . . 7.5.6 Numerical Examples . . . . . . . . . . . . Extrusion . . . . . . . . . . . . . . . . . . . . . . . 7.6.1 Formulation of the Problem . . . . . . . . 7.6.2 Kinematics of the Process . . . . . . . . . 7.6.3 The Approximate Velocity Field . . . . . . 7.6.4 The Extrusion Pressure . . . . . . . . . . . 7.6.5 Numerical Examples . . . . . . . . . . . .

xi

. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Plug . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . .

8. Plastic Waves. Perforation 8.1 8.2 8.3 8.4 8.5

Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . Various Theories . . . . . . . . . . . . . . . . . . . . . . . Perforation with Symmetries . . . . . . . . . . . . . . . . Modeling of the Taylor Cylinder Impact Test. Anisotropy Analysis of the Steady-State Flow of a Compressible Viscoplastic Medium Over a Wedge (Cazacu et al. [2006])

9. Hypervelocity Impact (Information) 9.1 9.2

317 321 332 332 334 336 337 339 342 346 346 347 349 351 354 357 366 366 368 372 374 375 383

. . . .

. . . .

. . . .

. . . .

. . . .

383 384 393 407

. . . . . 410 425

Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 425 Further Studies . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 434

Author Index

447

Subject Index

457

This page intentionally left blank

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Introduction

Theory of Plasticity studies the distribution of stresses and particle velocities (or displacements) in a plastically (irreversible) deformed body, when are known the external factors which have acted upon him and the history of variation of these factors. The theory was applied to metals to describe working processes both at cold (drawing, rolling, etc.) and warm (extrusion, forging, etc.), to describe term behavior (high and law) involving also temperatures, to short term behavior, to describe impact, shocks, perforation, etc. It was applied to geomaterials, as soils, rocks, sands, clays, etc., with the description of civil engineering applications as tunnels, wells, excavations of all sorts, etc. It was applied to other materials as concrete, asphalt, ceramics, ice, powder-like materials, various pastes, slurries, etc. In the classical sense the Plasticity Theory is time independent. However a time dependent theory was also developed and called Viscoplasticity. Besides Rheology deals with any ﬂow or deformation in which time is the main parameter. From the point of view of formulation of problems, in plasticity one considers in some of the problems, as in elasticity, that the strains are small; whoever in some other problems the consideration of the problems are as in nonlinear ﬂuid mechanics when the strain are ﬁnite. 1

Diagnostic Tests

These are the slow tests in compression or in tension (ε˙ ≤ 10−2 s−1 , say) so as the strain is uniform along the specimen. We denote by σPK =

F A0

and by

σC =

F A

the Piola–Kirchhoﬀ and the Cauchy’s stresses. Here F is the total force applied axially to the specimen, and A the current area, and by A0 the initial area of the cross section of the specimen. We also denote by εH = ln

l l0

and by 1

εc =

l − l0 l0

dynamic

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

2

Dynamic Plasticity

Stress

Q

σY

σP

0

εP

R

εE Fig. 1

Strain

Typical diagram of a diagnostic test.

the Henchy’s strain or the Cauchy’s strain. Here again l is the length of the working area of the specimen, and l0 is the initial length of the same area. As a sign convention, σ > 0 in tension for metals, but it is a reverse convention for rocks and soils (see Fig. 1). σP is the proportionally limit of the specimen where we apply the Hooke’s law σ = Eε with E the Young’s modulus which is constant, and independent on the loading rate and on the loading history. Up to σP we apply the Hooke’s law in both loading und unloading. σY is a conventional or oﬀset yield limit . deﬁned by the permanent εY , generally 0.1% = 0.5% of the total strain. Essentially is that εY is deﬁned by a convention. Thus for ε < εY the unloading is perfectly elastic without hysteresis loop, as σ = σQ + E(ε − εQ ) . Thus we assume small strains and ε = εE + εP . In elasticity we apply the Hooke’s law written as σ = C[ε] or σij = Cijkl εkl where C is a fourth order tensor. We apply this law during loading and unloading and the natural reference conﬁguration is the stress-free strain-free state. If we introduce the two deviators by: tr σ tr ε l and ε = ε − l, σ = σ − 3 3 the Hooke’s law can be written σ = 2Gε

and tr σ = 3Ktr ε ,

dynamic

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

Introduction

dynamic

3

σ

ε

0 Fig. 2

Nonlinear elastic curve.

σ E

A

σ

∆σ

D

F

σ∗ 0

B

εP

Fig. 3

C

εE ∆ε P

ε

Stress work per unit volume.

where G and K are the two elastic constants. The above relations are applied for any elastic isotropic body. There are nonlinear elastic bodies as for instance rubber (see Fig. 2). The stress– strain curve is nonlinear but reversible. The unloading is according to some other law, exhibiting a signiﬁcant hysteresis loop. We cannot describe this behavior by the Hooke’s law but with a nonlinear law, giving a one-to-one correspondence. Since the material remembers his initial conﬁguration, the reference conﬁguration is the initial one. For dissipative materials as the plastic ones, we can deﬁne an irreversible stress work per unit volume by: T σ(t)ε˙P (t) dt . W (T ) = 0

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

4

Dynamic Plasticity

σ

σ∗

• •

•

•

• ε

0 Fig. 4

Lack of one-to-one correspondence.

σ

σY

0

ε

εY

Fig. 5

Linear work-hardening.

That is shown in Fig. 3; it is the total irreversible area under the curve. The remaining area is the potential energy of deformation reversible for the reversible elastic materials (conservative). In order to deﬁne work-hardening, we start with the Fig. 3. In a loading loop BAEDC producing the irreversible strain ∆εP and returning to the same stress σ ∗ , we deﬁne by: (σ − σ ∗ )∆εP > 0 irreversibility , ∆σ∆εP > 0 stability . These two conditions are known as the Drucker’s postulate and are used to deﬁne the plastic work-hardening. Another postulate is due to Iliushin’s; it says that the loading–unloading FAEDF must be positive. In plasticity there is no one-to-one stress–strain correspondence. That is very clear in Fig. 4. The loading history must be known; to a single stress correspond several strains. Plasticity starts with unloading, as compared with nonlinear elastic behavior; and with the plastic strains which can develop only if σ > σY . The linear work-hardening is deﬁned by two straight lines (Fig. 5): σ = Eε

if σ ≤ σY ,

σ = σY + E1 (ε − εY ) if σ ≥ σY . Here E1 is the constant work-hardening parameter, and E1 E.

dynamic

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Introduction

dynamic

5

σ B 2σ Y 2σ Y C 0

ε

K G M Fig. 6

Various hardening laws.

If the stress is increasing very slowly, in the so-called “soft” machines, one is observing some steps on the stress–strain curve. It is question of the so-called Savart–Masson eﬀect, later rediscovered by Portevin–Le Chatelier eﬀect. It was shown that this eﬀect can by described by a rate-type constitutive equation (Suliciu [1981]). The viscosity coeﬃcient has strong variation in some regions of the ε, σ plane that lie above the equilibrium curve. For most materials, if σ is on a plastic state, then −σ is also on the plastic state. As it is well known, there are a lot of materials which do not satisfy this condition. For rocks for instance, if σY t is the yield stress in tension, then σY c is in compression, and |σY c | |σY t |. That is also for concrete, cast iron, soils, glass, powders, etc. That is called Bauschinger eﬀect, discovered in 1886. In Fig. 6 it is along BCK, that is the segment 2σY stays more or less constant during loading. For metals the elastic domain has a constant size 2σY during loading. If during unloading we follow BCGM then the hardening is said to be isotropic. If during unloading we follow the path BCK we say that the hardening is kinematic. Generally, if the yield stress in one direction is diminished by a previous plastic deformation in the opposite direction we have a Bauschingr eﬀect. It introduces anisotropy, sough it can be removed by annealing at high temperature. If we do a loading in a single direction, we cannot distinguish between the two hardening.

2

Tests Performed at Long and Short Term Intervals

If dx is a material element in current conﬁguration, and dX in the initial conﬁg˙ uration, we call λ = dx/dX elongation. The rate of elongation is D = λ/λ (= ε˙ sometimes).

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

6

Dynamic Plasticity

σ

ε→

+∞

local increase of ε (dynamic ) ε2 > ε1 ε1 > ε0 ε0

&

ε→

−∞

σ = const. creep ε = const.

&

stress relaxation

ε

0 Fig. 7

Eﬀect of change of rate of elongation.

Table 1

Variation of ε. ˙

ε˙ < 10−20 s−1 10−8 s−1 ≥ ε˙ ≥ 10−12 s−1

slow tectonic motion, creep tests,

10−4 s−1 ≥ ε˙ ≥ 10−1 s−1

testing machines,

ε˙ 1 s−1 ε˙ 10 s−1

hammer drop, the strain is not uniform, wave propagation is needed,

ε˙ 102 s−1 ε˙ 104 s−1

metal drawing, air gun bullet, high speed impact, ballistics,

ε˙ 106 s−1 − 107 s−1

high speed drawing of very ﬁne wires, or very fast tests.

The change of rate of deformation is shown in Fig. 7. An increase of ε˙ is raising the curves. But this raise in technically limited by the machine we have. For an additional increase, we need dynamic curves, with an local increase ˙ This of ε. increase is done by elastic waves propagating with the velocity c0 = E/ρ. A table of approximate increase of ε˙ is given in Table 1. This is a very approximate table of variation of ε. ˙ For constant stress we have creep, but for constant strain we have stress relaxation. Any other intermediate variation of the strain rate is possible. For |ε| ˙ → ∞ we have very fast variation of the strain rate, impossible to realize practically. In order to have a representation we take into account that mainly the plastic properties are inﬂuenced by the change of the rate of strain (see Fig. 8). A relationship was proposed by Ludwik from 1909, and is of the kind shown on Fig. 8. Thus we have for a ﬁxed strain: σ = σY + σ0 ln

ε˙P ε˙P 0

and σ > σY > 0

dynamic

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

Introduction

dynamic

7

σ ε2 > ε1 ε1 > ε0

σY

0

Fig. 8

ε0

•

ε

Inﬂuence of the strain rate on the stress–strain curve.

with σ0 = constant. If the elastic strains are disregarded, the stress–strain curves are σ − σY if σ > σY , 3η ε˙ = 0 if 0 ≤ σ ≤ σY , where σ − σY is the overstress. σY is the yield stress for a conventional small ε˙0 obtained in very slow performed tests, when ﬂow starts being possible. η is a viscosity coeﬃcient; if two tests are performed with the strain rates ε˙1 and ε˙2 we have: σ2 − σ1 , 3η = ε˙2 − ε˙1 to determine η. If η is constant for any strain rates, the relation is linear, otherwise nonlinear. Since in this relation there is no strain, the reference conﬁguration is the actual one. For work-hardening materials (Malvern): σ − f (ε) if σ > f (ε) , 3η ε˙ = 0 if 0 ≤ σ ≤ f (ε) . The reference conﬁguration is the initial one or a relative one, corresponding to the state when the test started (for geomaterials, for instance). Let as give several examples. In Fig. 9 is given the stress–strain curves for schist. One can see that the inﬂuence of the strain rate is felt from the beginning. The hole curve is inﬂuenced, not only the plastic part. Also, the last points correspond to failure. Thus with an increase of loading rate the stress at failure is increased, while the strain at failure is decreased. Thus a theory of failure expressing in stresses only, would not work. In order to see that the inﬂuence of the strain rate is not always to be seen always on the stress–strain curves. In Fig. 10 are given the curves for granite, obtained in

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

8

Dynamic Plasticity

Fig. 9

Fig. 10

Stress–strain curves for schist.

Inﬂuence of the strain rate on granite.

triaxial tests (after Sano, Ito, Terada [1981]). One can see that the inﬂuence of the strain rate is practically zero on the axial stress strain curves. But the inﬂuence on the radial strain is remarkable on the other curves. Failure is the last point, but for the lowest radial curve is extended until −0.064, thus extending very much outside the ﬁgure. Concerning failure one can see that stress at failure is increased with the strain rate, while the strain is decreased. Thus failure would be impossible to describe with a condition written in stresses only.

dynamic

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Introduction

3

dynamic

9

Long-Term Tests

In order to ﬁnd out the principal properties of creep and relaxation, one is doing long-terms tests. If the stress applied is relative small, the creep is transient, i.e., stabilizing after a certain time. In Fig. 11 is shown the creep curves for schist. One can see that the ﬁrst curves correspond to transient creep only. The stresses are too small. The fact that the stresses are small, on the right side is given the ε˙ − t curves. The curves corresponding to the transient case come quite fast at the origin (ε˙ → 0). For higher stresses, we obtain a steady state creep, with ε˙ = const. That is obtained generally for σ ≥ 0.6σc , where σc is the short-term failure strengths. Temperature has a strong inﬂuence on creep. With increasing temperature the creep curves start at a lower stresses and extend very much. When the applied stress is still increased, we arrive at the tertiary creep, where ε¨ > 0. That means that soon failure will take place. From the right side of the diagram, the tertiary creep is not bringing the curves at zero. From the very many laws existing, the most known is the Norton law where ε˙ ∼ σ n . Generally we describe creep by ε˙ = f (σ, ε), the temperature being also inﬂuenced. For relaxation one is describing it with σ˙ = g(σ, ε), the temperature being again present. Jugging only from the creep curves, it is diﬃcult to see if they correspond to a viscoelastic model or to a viscoplastic one. The only things we can say is the diﬀerence in the history dependent principle. Figure 12 is showing the diﬀerence. If one is loading with the stress σ1 and then increase it to σ2 , or applied from the beginning the stress σ2 , we obtain the same thing (at left) if there are no internal changes, or obtain something diﬀerent (at right), with possibly internal changes. In the ﬁrst case the loading is history independent, while in the second we have a history dependency. The history dependency is probably viscoplastic.

Fig. 11

Creep curves for schist.

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

10

dynamic

Dynamic Plasticity

ε σ2

ε

σ2

σ2 σ2 σ1

σ1 t 0

t 0

Fig. 12

Fig. 13

Principle of history dependency.

The method used for the determination of the elastic parameters.

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Introduction

dynamic

11

Thus we have to consider plasticity only if: • • • • •

the stresses σ > σY , we obtain an irreversible strain, we have a history dependence, generally, we have a initial reference conﬁguration, generally, the deviator relationship (σ ∼ ε ) is distinct from the volumetric (tr σ ∼ tr ε).

Concerning the procedure used to measure the elastic parameters for various materials, for metals there are no problems. The problem is for the powder-like materials, or for rocks, for instance. The idea is that for such materials the hysteresis loop is quite important, so that if one is doing the unloading immediately, it is diﬃcult to determine the elastic parameters directly. Figure 13 (after a PhD of Niandou [1994]) is showing such a problem. If one is trying to determine the elastic parameters directly immediately after loading, one obtains the hysteresis loops shown. One has to wait after each re-loading a number of minutes during which the rock is creeping. On the last ﬁgure shown one can see that the rate of deformation is decreasing wary much. Thus after a period of time if one is doing the unloading, no hysteresis loops are observed any more. This method is to separate the rheological properties from the unloading. That is the method proposed for rocks since 1988 (Cristescu). It was applied to many other materials since that time.

4

Temperature Inﬂuence

A temperature increases will decrease: • • • •

the the the the

elastic parameters, yield stress, work-hardening modulus, ultimate strength.

It is important to mention here the Zener–Hollomon parameter for metals: ∆H , Z = ε˙ exp RT where ∆H is the activation energy which may depend on temperature, R is a universal gas constant and T the absolute temperature. For ε = const. the stress can be obtained from ∆H . σ = f (Z) = f ε˙ exp RT That is we can change the rate of strain or temperature according to this relation.

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

12

Dynamic Plasticity

Fig. 14

5

Triaxial stress–strain curves for alumina powder.

The Inﬂuence of the Hydrostatic Pressure

It was shown that with an increase of pressure: the yield stress slight increases, the ultimate strength increases, the elastic modules G and K increase (increase of wave velocities), the work-hardening modulus increase and the ductility increases signiﬁcantly. The last increase has lead to new methods of metal working, where an additional pressure was used. Generally, for metals the constitutive equations is written in deviators. The above is not true for: rocks, soils, wood, cast iron, powder like materials, granular like materials, etc. For all these materials the pressure plays an important role. In Fig. 14 is shown the stress–strain curves for alumina powder, obtained in triaxial tests. One can see that all curves, the axial, diameter, and volumetric curves, are strongly dependent on the pressure (written along the curves). 6

Variation of Elastic Parameters with Plastic Strain (Metals)

During plastic deformation the elastic parameters vary. That has a signiﬁcance for the expression of wave velocities (say). For cylindrical specimens subjected to uniaxial tests ε2 = ε3 = −νε1

dynamic

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Introduction

dynamic

13

with ν the Poisson’s ratio. For isotropic elastic materials 0 ≤ ν ≤ 0.5. If ν ≈ 0 no lateral strain is to be expected. For ν ≈ 0.5 we have an incompressible material ε11 + ε22 + ε33 = 0. For rubber ν = 0.47, steel 0.25 ≤ ν ≤ 0.30, aluminum 0.26 ≤ ν ≤ 0.36, cork ν = 0.00, polyethylene and paraﬃn ν ≈ 0.5. In the plastic domain for aluminum ν is very close to 0.5, thus shoving plastic incompressibility. Thus the variation of the volume is elastic only: σ = 3KεE and εP = 0. This result is true for metals, only. For rocks, granular materials, etc. it is not. Bibliography Niandou H., 1994, Th´ese de Doctorat, Lab. de M´ecanique de Lille URA 1441 CNRS. Sano O., Itˆ o I. and Terada M., 1981, Inﬂuence of strain rate on dilatancy and strength of oshima granite under uniaxial compression, J. Geophys. Res. 86, B10, 9299–9311. Suliciu I., 1981, On the Savart–Masson eﬀect, J. Applied Mech. 48, 426–428.

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

This page intentionally left blank

dynamic

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

dynamic

Chapter 1

Yield Conditions

1.1

Stresses

In order to understand well the problem we have to show several concepts which are helping. We choose an octhaedrical plane and its normal (see Fig. 1.1.1). For a point of stress (σ 1 , σ 2 , σ 3 ) we have the stress vector tn which must be projected on the hydrostatic line and on a normal to the hydrostatic line. Since σ1 0 0 tn = [n1 , n2 , n3 ] 0 σ2 (1.1.1) 0, 0

0

σ3

its components are i1 i2 i3 tn = n · T = σ1 √ + σ2 √ + σ3 √ 3 3 3 so that the projection of this vector on the hydrostatic line is σ2 σ3 σ1 + + = σ, tn · n = 3 3 3 where σ is the mean stress. The projection on the hydrostatic line is now

(1.1.2)

(1.1.3)

i2 i3 i1 (tn · n)n = σ √ + σ √ + σ √ 3 3 3 with absolute value |(tn · n)n| = |σ| . The projection normal to the octhaedrical line is tτ = tn − (tn · n)n σ σ σ σ2 σ3 σ1 i1 + √ − √ i2 + √ − √ i3 = √ −√ 3 3 3 3 3 3 1 = √ (σ1 i1 + σ2 i2 + σ3 i3 ) 3 15

(1.1.4)

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

16

dynamic

Dynamic Plasticity

Fig. 1.1.1

Octahedral plane and all other associated concepts.

with the absolute value

|tτ | = τoct =

2 IIσ . 3

(1.1.5)

We got thus the interpretation of Roˇs and Eichinger [1926]: the absolute value of the vector tensor normal to the linear hydrostatic axes is equal to the square root of the second invariant of the deviatoric stress tensor. For notation we give IIσ =

1 2 3 2 1 2 [(σ ) + (σ2 )2 + (σ3 )] = τoct ¯ = σ 2 1 2 3

(1.1.6)

= σij − σδij is the stress deviator. and σij Since the vector tτ in entirely in the octahedral plane, one can try to project it on various directions in this plane. Thus projecting on the π plane is giving (see Fig. 1.1.2): σ1 2 σ2 2 σ3 2 i1 + √ i2 + √ i3 . tn |π = √ 3 3 3 3 3 3

Now projecting on the σ 3 direction we have, σ2 2 1 σ3 2 σ1 2 1 +√ −√ tn · (−i3 ) = √ 3 32 3 32 3 3 1 = √ (σ1 + σ2 − 2σ3 ) 3 2 σ = − √3 . 2

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

Yield Conditions

dynamic

17

σ3'

π 2π 3

i3' 0 i'2

i1'

π 3

α ωσ

σ1'

σ2' tτ

Fig. 1.1.2

Octahedral plane with the assumption σ2 > σ1 > σ3 .

Thus we can write: σ tn · i2 = τoct cos α = √2 , 2 2π = tn · i3 = τoct cos α + 3 2π = tn · i1 = τoct cos α − 3

σ √3 , 2

(1.1.7)

σ1

√ , 2

σ1 σ2 σ3 = IIIσ . Taking into account that

2π 1 2π cos α − = cos 3α , cos α cos α + 3 3 4

we arrive at the relation

cos 3α =

3 IIσ

3

IIIσ , 2

(1.1.8)

α ∈ [0, π/3] deﬁnes the orientation in the octahedral plane of the stress vector t(x, n) and is the angle with ii corresponding to σi maximum. tτ is located between ii corresponding to σi maxim and ij corresponding to σj intermediate.

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

18

Dynamic Plasticity σ3 1 1 1 , , n 3 3 3

σ3′

σ2′

α τoct

P

σ σ1′

σ2

0

σ1

Fig. 1.1.3

Possible use of the invariants.

i3′ i3

arc cos

1 3

= 54 $73 n

0 Fig. 1.1.4

Projection on the octahedral plane.

If we write √ √ cos α σ2 / 2 = m, − 3 σ3 − σ1 sin α we obtain the Lode parameter, which is deﬁning the orientation in the octahedral plane.

dynamic

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

Yield Conditions

dynamic

19

From (1.1.7) we get:

3 τoct sin α − 2 σ2 − σ3 3 = τoct sin α + 2 2 σ3 − σ1 3 =− τoct sin α . 2 2 σ1 − σ2 = 2

π , 3 π , 3

(1.1.9)

Since we have chosen σ2 > σ1 > σ3 we have: σ1 − σ2 < 0

or

σ2 − σ3 > 0

or

σ3 − σ1 < 0

or

π π ≤ α ≤ 2π + , 3 3 π π − ≤α≤π− , 3 3

π+

0 ≤ α ≤ π.

Therefore we have 0 ≤ α ≤ π/3 which is satisfying all the inequalities. Since τmax = τ1 = (σ2 − σ3 )/2, we have: τmax π = sin α + 3 (3/2)τoct and since we have to choose only half of the interval 0 ≤ α ≤ π/6 to get diﬀerent values for the ratio, we get: √ 3 τmax ≤√ (0.866 =) ≤1 (1.1.10) 2 IIσ √ for α = π/6 and α = 0. The conclusion is that τmax and IIσ is quite close to each other. Thus a point of coordinates σ1 , σ2 , σ3 can be replaced by a point σ, τ, α, introducing the three invariants: the ﬁrst invariant of the stress, and the second and third invariants of the stress deviator (Fig. 1.1.3). We have still show howa quantity is projected on the octahedral plane. We have cos(i3 , i3 ) = 2/3, and just any quantity which is projected on the octahedral plane is to be multiplied by 2/3 (Fig. 1.1.4).

1.2

Yield Conditions

It is assumed that when deforming plastically all materials are satisfying a condition called yield condition. At least most metals satisfy this condition. The yield conditions satisfy a few general conditions. Let us describe them.

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

20

dynamic

Dynamic Plasticity

Assumption 1. We assume that for each material a yield function f (σ) exists so that: f (σ) < 0

or if f (σ) = 0 and ∂f σ˙ = 0 ∂σ ij

f (σ) = 0

and

∂f σ˙ ij < 0 the material is elastic ; ∂σij for loading in perfect plasticity ,

ij

∂f σ˙ ij > 0 ∂σij

for loading for work-hardening plasticity .

In order to give an example let us consider the yield criteria of von Mises which can be written f (σ) := IIσ − k 2 . Here k if it is constant the material is perfectly plastic; if however k is changing when the plastic deformation takes place, that is k(εP ), the material is work-hardening. Assumption 2. For metals the yield is independent of the spherical part of the stress. Thus f depends on the stress deviator f (σ). That means that the yield conditions are cylindrical in the stress space. Assumption 3. The material is initially isotropic. Therefore f (Iσ , IIσ , IIIσ ) = k 2 the yield function depends on invariants only. There are no preferred directions; f does not depend on the orientation of the principal axes. Taking into account the previous assumption, f depends on the deviator invariants: f (IIσ , IIIσ ) = k 2 .

(1.2.1)

Assumption 4. Since for most metals the curves σ–ε are symmetric with respect to the origin of axes, we must have f (σ) = f (−σ). Because IIσ = II(−σ ) the third deviator invariant must be involved in even powers. The Tresca [1868] Yield Condition. It is, in the octhaedrical plane, a regular hexagon as shown in Fig. 1.2.1. Thus the Tresca hexagon is deﬁne as τmax = k = const. It can be expressed in terms of invariants as described previously. Thus we can write (σ1 − σ2 ) = 4k 2 , σ1 σ2 + σ2 σ3 + σ3 σ1 = −IIσ , σ1 σ2 σ3 = IIIσ , σ1 + σ2 + σ3 = 0 . We can eliminate all the deviator stress components to get 2 27IIσ3 4 IIIσ2 3IIσ − − 1 − = 0, 64k 6 27 IIσ3 4k 2

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

Yield Conditions

dynamic

21

σ3' σ3 > σ1 > σ2

σ3 > σ2 > σ1 2 −σ

k =2

σ3 −

2 σ 3 Y

σ1 −

σ1'

σ

3

σ1 > σ2 > σ3 Fig. 1.2.1

Fig. 1.2.2

σ1

=2 k

σ2− σ1 = 2k

σ1 > σ3 > σ2

σ1− σ2 = 2k

σ3

0

π 3

=2 k

σ3 σ 2−

k =2

σ2 > σ3 > σ1

σ2'

σ2 > σ1 > σ3

The Tresca hexagon.

The plane Tresca hexagon.

which is due to Reuss. That is a complicated way of expressing the Tresca yield condition, so that today it is expressed also as τmax = k. For the plane problems it is expressed in a simpler way as in Fig. 1.2.2. For the Tresca condition the relationship between the yield stresses in shear and tension is 2τY = σY . The number 1/2 is a little too small, experimentally it is ranging somewhere between 0.55 and 0.6.

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

22

Dynamic Plasticity

The Mises [1913] Yield Condition. The von Mises yield condition is expressed as IIσ = k 2 , where IIσ = =

1 2 2 2 [(σ11 − σ22 )2 + (σ22 − σ33 )2 + (σ33 − σ11 )2 ] + σ12 + σ23 + σ31 6 1 2 [(σ ) + (σ2 )2 + (σ3 )2 ] . 2 1

The von Mises yield condition is represented in the three axial stress space as a circular cylinder shown in the last two ﬁgures. For the plane case it is an ellipse. For the von Mises yield condition the relationship between the yield stress in shear √ ∼ and tension is τY = σY / 3 = 0.557σY . That is a much better value. All the correspondences of the two yield condition and the tests are shoving a better ﬁtting of the von Mises than that of Tresca. Also, any generalization of this condition to for anisotropic materials is a combination of the two conditions.

1.3

The Classical Constitutive Equation for Perfectly Plastic Materials

Saint-Venant–Mises Constitutive Equation The ﬁrst law of plasticity is due to Barr´e de Saint-Venant [1870]. He has done several assumptions which have been inspired from metal working theories but the meaning of the plastic ﬂow was changed. They are: εE = 0

the elastic part of the strain rate is negligible

since εP V ≈ 0 plastic incompressibility is assumed, i.e., D = D , σ = λD as in Newtonian viscosity, but λ is variable, λ is determined from a plasticity condition; squaring the above law we have √ σ : σ 2 σ : σ = λ D : D or λ = √ D:D

and for a von Mises plasticity condition IIσ = k 2 = conts. for perfect plasticity: k λ= √ . IID Thus the constitutive equation is:

√

k σ = √ D IID IIσ < k

and tr D = 0 if IIσ = k 2

or IID = 0

for perfectly plastic , for rigid behavior .

The meaning of k follows from the yield conditions. For von Mises yield conditions

dynamic

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Yield Conditions

dynamic

23

1 1 2 2 2 2 2 2 σ : σ = (σ11 + σ22 + σ33 ) + σ12 + σ23 + σ31 = k2 2 2 2 if all σij = 0 besides σ12 = 0 we obtain σ12 = k 2 or, if the yield stress in pure shear is τ , τ = k.√ In uniaxial tensile tests σ11 = 0 all other σij = 0, we obtain Y 2 /3 = k 2 , or k = Y / 3, where Y is the yield stress in uniaxial tensile (or compressive) tests. Thus we arrive at the relation σY τY = √ , 3

for the yield stresses in pure shear and tensile, for the von Mises yield condition. The classical constitutive equation seems to be a non-Newtonian ﬂuid, but it is not, since it is time-independent (nonviscous). To show that we write the constitutive equation as D σ √ , = k IID and we change v with µv, with µ > 0, that is we change the time. We have D → µD, and IID → µ2 IID thus µ disappears from the constitutive equation. Thus the main properties of the constitutive equation are time independent, the reference conﬁguration is the present one (in the case we have no internal changes) D is involved as for ﬂuids; it is used when the plastic deformation are signiﬁcant, the elastic part of the strain rate are negligible, as in some metal working problems. The Prandtl–Reuss Constitutive Equation This is a constitutive equation developed by Prandtl [1924] for two-dimensional cases and extended by Reuss [1930] for the three-dimensional case. Assuming small deformations the constitutive equations are: ε˙ = ε˙ E + ε˙ P ,

ε˙ E =

1 σ˙ , 2G

tr σ˙ = 3K tr ε˙ ,

(1.3.1)

λ σ˙ , tr ε˙ P = 0 . 2G Thus the strain rates are additive, the reference conﬁguration is usually the initial one, G is the shearing modulus, and K is the bulk modulus with G = E/2(1 + v) and K = E/3(1 − 2v). From there one receive ε˙ P =

+ λσij . 2Gε˙ij = σ˙ ij

(1.3.2)

In (1.3.2) we have 10 variables, 3 velocities, 6 stresses and λ. If we assume the von Mises yield condition IIσ = k 2 , we obtain either σ˙ ij IIε˙ P + σij ε˙ij = 2G k

January 12, 2007

24

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

dynamic

Dynamic Plasticity

or ε˙ij =

˙P σ˙ ij W + σ 2G 2k 2 ij

˙ P = σij ε˙P the stress work per unit volume. with W ij With all these the Prandtl–Reuss constitutive materials is √ σ˙ ij IIε + σij ε˙ij = 2G k if IIσ = k 2 tr σ˙ = 3K tr ε˙ σ˙ ij if IIσ < k 2 ε˙ij = 2G tr σ˙ = 3K tr ε˙ if IIσ = k 2

equation for perfectly plastic

and σij σ˙ ij = 0 ,

(1.3.3) or and σij σ˙ ij < 0 .

σ˙ ij = 0 is called consistency condition. The reference conﬁguration The relation σij is either the actual one or the conﬁguration after unloading from current conﬁguration. Also, εE does not satisfy the Saint-Venant compatibility conditions, since there may be no single valued continuous displacement ﬁeld that would take the whole body from deformed conﬁguration to an unstressed conﬁguration. Thus ε˙ P is not explicitly integrable. It is easy to show that the Prandtl–Reuss constitutive equation is time-independent, i.e., they are nonviscous.

The Hencky Constitutive Equation This is a constitutive equation developed by H. Hencky [1924], tough A. Nadai [1923] has used it for torsion problems, and afterwards it was used by A. A. Iliushin [1961]. The main assumption is that one can write it as for Hooke law, but the “plastic” parameters are variable, not constant. Thus: σ = 2GP ε , σ = 3KP ε . But KP coincides with K because the volume behavior is elastic. So it is only G which can be written: √ IIσ S = , 2GP = √ E IIε if one uses the Sokolovsckii notation. Thus for work-hardening condition: S = F (E) , σ =

F (E) ε , E

σ = 3Kε ,

(1.3.4)

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Yield Conditions

dynamic

25

or, E = F −1 (S) , ε =

F −1 (S) σ , S

(1.3.5)

σ˙ for all cases . 3K One has to observe that this constitutive equation was extensively used because it is easily reversible; it is written in ﬁnite form and called constitutive equation of “plastic deformation”; it was used when the strain are increasing continuously; for proportional loading paths σ(X, t) = λ(t)σ 0 (X), the Prandtl–Reuss constitutive equation coincides with the Hencky (Iliushin [1961]); the reference conﬁguration is the initial one. We can think to another variant of the Hencky constitutive equation by assuming: ε˙ =

ε = ε E + εP , εE satisfy the Hooke constitutive equation, the plastic strain satisﬁes −1 1 F (S) − σ . εP = S 2G

(1.3.6)

If we diﬀerentiate the constitutive equation we can write: −1 F (S) d F −1 (S) σ˙ + σ for E = F −1 (S) and S˙ > 0 for loading , dt S S ε˙ = for unloading elastic ˙ σ for E = F −1 (S) and S˙ ≤ 0 or E < F −1 (S) 2G σ for all cases . ε˙ = 3K The Hencky’s constitutive equation is obviously time independent. 1.4

Work-Hardening Materials

We assume for work-hardening materials small strains so that ε = ε E + εP . The elastic rate of deformation components satisfy ε˙E ˙ kl . ij = Aijkl σ The yield function F exists which satisfy F (σij , εP kl , χ) = 0

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

26

Dynamic Plasticity

Fi = 0

∂Fi ∂σ kl Fj = 0 ∂F j ∂σ kl Fig. 1.4.1

The Koiter generalization.

P with F (0, εP ij , χ) < 0 at reference conﬁguration with εij and χ ﬁxed at a particle. χ is a scalar called work-hardening parameter. If F (σij , χ), i.e., εP ij is not explicitly involved the work-hardening is called isotropic. If however, F (σij , εP kl ) the work-hardening is inducing anisotropy. The plastic rate of deformation is given by: P F (σij , εkl , χ) < 0 or for ∂F 0 F (σij , εP σ˙ ij ≤ 0 . P kl , χ) = 0 and ε˙ij = ∂σij ∂F ˙ ij ) for F (σij , εP σ˙ ij > 0 . Bij (σkl , εP mn , χ, σ kl , χ) = 0 and ∂σij

The initial data are deﬁned by εP (0) = εP 0 , and χ(0) = χ0 , thus a reference conﬁguration in assumed, not necessarily the stress-free, strain-free conﬁguration. Since it is assumed that both at time t and t + ∆t the yield condition is satisﬁed during a loading, we have ∂F ∂F ∂F χ˙ = 0 , σ˙ ij + P ε˙P ij + ∂σij ∂χ ∂εij which shows that all the increments are not independent. This is the consistency condition. Because when approaching the yield condition by continuity, we must have: lim Bij (σkl , εP ˙ ij ) = 0 , mn , χ, σ ∂F σ˙ ij → 0 , ∂σij which is the continuity condition. That means that only the normal component of the increment of the stress tensor is giving a plastic increment of the strain ﬁeld. Thus we have ε˙P ˙ mn ) ij = λ(σkl , σ

∂F ∂σij

dynamic

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

Yield Conditions

dynamic

27

and we call the constitutive law associated to the yield condition. That is true for most metals, but not true for rocks or soils, for instance. For such materials we have to introduce a plastic potential following the idea of von Mises from 1928: ε˙ij = µ(σkl , σ˙ mn )

∂H , ∂σij

where H is the plastic potential. For such materials the constitutive equation is called nonassociated. There are yield conditions which have several constitutive equation meeting at a point. For instance the Tresca yield condition is of this kind (see Fig. 1.4.1). In this case we use the idea of Koiter [1953]: ε˙P ij = λk

∂Fk ∂σij

with the constants λk deﬁned by: ∂Fk σ˙ = 0 for perfect plasticity ∂σ ij λk > 0 if

Fk (σmn ) = 0 Fk (σmn ) < 0

λk = 0 if

Fk (σmn ) = 0

ij

and

∂Fk σ˙ ij > 0 for working-hardening ∂σij

or

∂Fk ∂σmn σ˙ mn < 0

for perfect plasticity

∂Fk σ˙ mn ≤ 0 ∂σmn

for working-hardening .

and

Thus, only at the corner are involved several values of λk .

1.5

Isotropic Hardening

For the isotropic hardening the yield condition is written F (σij , χ) : f (σij ) − H(χ), and in a speciﬁc form f (IIσ , IIIσ ) = H(χ). It is interesting to follow the way in which the work-hardening parameter is determined. It can be the irreversible stress work per unit volume (Fig. 1.5.1), i.e.,

t

χ(t) = W P (t) =

σij (X, s)ε˙P ij (X, s) ds 0

or

t χ(t) = 0

4 II P ds = 3 ε˙

t 0

t 2 P P dεij dεij ds = ε¯˙P (s) ds , 3 0

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

28

Dynamic Plasticity

σ3'

A

0

σ2'

σ1' Fig. 1.5.1

The isotropic hardening.

where ε¯˙P is not a derivative. In this case χ(t) is the history of the eﬀective plastic strain increment. However we can still consider by deﬁnition: 2 P P ε (t)εP χ(t) = ε¯ (t) = ij (t) 3 ij and the work-hardening parameter is equivalent to the plastic strain. For the von Mises yield condition written as: √ σ ¯ = 3k with σ ¯ the equivalent stress: 3 2 (σ1 + σ22 + σ32 )1/2 = 3IIσ σ ¯= 2 =

1/2 1 2 2 2 [(σ11 − σ22 ) + (σ22 − σ33 ) + · · · ] + 3(σ23 + · · · ) . 2

If only one component, say, σ11 = 0, and all the others σij = 0, then σ ¯ = |σ11 |. For such a component we write: σ ¯ (t) = F (W P (t)) , t P ¯ σ ¯ (t) = H ε˙ (s) ds , 0

σ ¯ (t) = G(¯ εP (t)) , which describe various possible variants of the isotropic work-hardening.

dynamic

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

Yield Conditions

29

σ1 = H σ1

dynamic

( ∫ ε ds ) P 1

σ

σ = H ( χ ( t )) ∆σ

σ1

t

W P (t ) = ∫0 σ 1

dl σ 12 (t ) − l0 2E

t

χ (t ) = ∫0 ε P ( s ) ds

0

∆χ

dl dσ 1 dW P = σ 1 − E l0

ε 1P

Fig. 1.6.1

1.6

The universal stress–strain curve.

The Universal Stress Strain Curve

If we do a single test we have σ ¯ = σ11 = σ1 (assume that σ11 is positive). If = εP the specimen is cylindrical, εP 2 3 , and if we assume plastic incompressibility P P ε1 = −2ε2 . Thus if we take all these into account we have (Fig. 1.6.1): 2 P P 2 1 P2 2 dεij dεij = dεP dε = ε˙P + 1 ds . 1 3 3 2 1 Thus if we are doing a single test we discover a three-dimensional law to be applied generaly. We have to apply the general law since the function H is already known. If the constitutive equation is ε˙P ij (t) = λ(t)σij (t) with λ ≥ 0, i.e., the principal directions of ε˙P ij and of σij coincide, then we have

˙ P (t) = σ W ¯ (t)ε¯˙P (t) . That is easy to show since

σij λσij

=

3 σ σ 2 ij ij

Thus the work-hardening law is

σ ¯ (t) = F 0

t

2 P P ¯ ε¯˙P . ε˙ ε˙ = σ 3 kl kl

¯˙ ds . σ ¯ (s)ε(s)

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

30

Dynamic Plasticity

We have the suggestion to write this law t P ¯ σ ¯ (t) = H ε˙ (s) ds 0

and it is easy to pass from one to the other. If the variation of the plastic strains is proportional, i.e., P εP ij (t, X) = h(t)εij0 (X)

at every particle X. Then dεP dh ij = εP ij0 dt dt i.e., dh . ε¯˙P = ε¯P 0 dt By integration with respect to time at a ﬁxed particle X with h(0) = 0, we get t ε¯˙P (s) ds = ε¯P 0 h(t) . 0

Generally a proportional variation of εP ij in every point of the body is not possible, but in very special designed laboratory test. The equality t ε¯˙P (s) ds = ε¯P (t) 0

do not hold for all practical cases. Thus the work-hardening condition σ ¯ (t) = G(¯ εP (t)) is generally not correct, though extensively used. It disregards the history dependence of the plastic deformation. This is a closed relation to nonlinear elasticity. 1.7

Constitutive Equation for Isotropic Work-Hardening Materials

From the work-hardening condition f (σij ) = F (χ) ,

we get the consistency condition ∂f ∂F λ ∂F χ˙ = σ σ . ˙ ij = σ ∂σij ∂χ ∂χ kl 2G kl If we solve with respect to λ and we introduce in the constitutive equation ε˙P ij =

λ σ . 2G ij

dynamic

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

Yield Conditions

We get ε˙P ij

1 = 2IIσij (∂F/∂χ)

dynamic

31

∂f ˙ kl σij . σ ∂σkl

Thus the general constitutive equation is σ˙ ij 1 + ε˙ij = 2G 2IIσ (∂F/∂χ)

∂f ˙ kl σij σ ∂σkl

with the bracket deﬁned by A if f (σij ) = F (χ) and A = ) = F (χ) and f (σij 0 if ) < F (χ) . f (σij

∂f ˙ ij > 0 σ ∂σij ∂f ˙ ij ≤ 0 or σ ∂σij

If we write the yield condition in the form F (σij , χ) := f (σij ) − H(χ) ,

then the constitutive equation is ε˙P ij =

)σ˙ kl

∂F (∂F/∂σkl (∂F/∂χ)(∂F/∂σmn )σmn ∂σij

with a similar deﬁnition of the bracket . 1.8

The Drucker’s Postulate

For stable work-hardening materials Drucker [1951] has established the following postulate. Assume that a stress–strain curve is built. It is showing as in the Fig. 1.8.1. We start from a stress σ0 . We load by producing also some plastic deformation ∆εP 1 . Then we unload, up to the initial stress σ0 . If the material is a stable work-hardening, then two conditions are to be satisﬁed: ε˙P ˙ ij ≥ 0 , ij σ 0 ε˙P ij (σij − σij ) ≥ 0 .

Thus the plastic work done by external agency during the application of an additional stress is positive and the net total work performed by the external agency during the cycle of adding and removing stress is non-negative. The Drucker’s postulate has signiﬁcant consequences for metal plasticity. Thus the yield condition must be convex, nowhere concave. That is shown in Fig. 1.8.2. Another similar postulate was invented by Iliushin, but it is connected to the strain concept. One is starting from a certain strain εij and one make a loading

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

32

Dynamic Plasticity

Fig. 1.8.1

The Drucker’s postulate.

F (σ ij , χ ) = 0

εijP

F (σ ij , χ ) = 0

σ ij0

σ ij

σ ij

σ ij0

Fig. 1.8.2

εij

Consequences of the Drucker’s postulate.

and unloading until one reaches the same strain (see Fig. 1.8.1). A weakened form of Iliushin’s postulate, which says that the changing rate of the stress work done along every standard strain cycle should be non-negative, whenever the incorporated plastic sub path tends to vanish, is due to Bruhns et al. [2005]. The Drucker’s postulate has been extensively considered in the literature. It is a nonenergetic and equivalent to associated ﬂow rule (see Stoughton and Yon [2005] for literature). 1.9

Kinematical Work-Hardening

Another work-hardening law is the kinematical work-hardening. It is shown in Fig. 1.9.1 for a plastic rigid model. The yield surface does not change shape; it translates in the stress space. The size of the elastic domain remains constant and

dynamic

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

Yield Conditions

dynamic

33

σ1

arc tan c1

σY

σ Y + c1ε 0' c1ε

0

σ Y − c1ε

−σY

Fig. 1.9.1

The work-hardening model.

F ( t + ∆t ) = 0

F (t ) = 0

M

σ ij cεijP

0' P

α ij

N

α ij

σ ij

0

σ ij Fig. 1.9.2

The kinematical work-hardening assumptions.

equal to 2σY (rigid). The origin translates with c1 ε in the case of linear workhardening/rigid model. c1 is a constant work-hardening modulus. This model is describing an idealized Bauschinger eﬀect. For the general three-dimensional case the initial surface is F (σij ) = 0. The translated surface is F (σij − αij ) = 0, where the coordinates of the new origin are αij . Some additional postulates are to be satisﬁed by αij in order to satisfy the history of the plastic deformation. It must satisfy the initial condition α = 0 if εP = 0. It is called sometimes “back stresses”.

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

34

Dynamic Plasticity

Prager [1959] postulated that the yield surface translates in the direction normal ∂F/∂σij at the current stress state σij in the nine-dimensional space, i.e., in the direction of PM. That is α˙ ij = cε˙P ij if we assume ε˙P ij ∼ ∂F/∂σij . Consideration in spaces with smaller dimensions than nine, may lead to mistakes since the normal may not remain normal. The constitutive equation is (Fig. 1.9.2) ∂F (σ − α) . ∂σ The scalar η is obtained from the consistency condition ˙ = η(σ, εP , σ) ˙ ˙ ε(σ, εP , σ)

∂F (σ − α) ˙ = 0, : (σ˙ − α) ∂σ where, if one takes into account the above relations we have ε˙P ij =

∂F (σkl − αkl ) (∂F (σkl − αkl )/∂σmn )σ˙ mn . c(∂F (σkl − αkl )/∂σgh )(∂F (σkl − αkl )/∂σgh ) ∂σij

If we make the assumption that the yield surface translates in the direction PN, i.e., ˙ = (σ − α)µ˙ , α where µ˙ > 0 is an additional unknown. It is a diﬃcult problem with this additional unknown. 1.10

Further Developments

Combined Isotropic and Kinematical Hardening. Some authors have combined the two models to get a combination in the form f (σ − α, χ) = 0 , where α and χ are the two work-hardening coeﬃcients, the kinematical and workhardening. As an example one can consider yield surfaces of the form f=

1 1 (σ − α)(σ − α) − σY2 = 0 . 2 3

Mr´ oz [1969] has introduced the multi-surface model to describe the cyclic eﬀect and the nonlinearity of stress–strain loops. There are several such surfaces fi (σ − α, χi ) = 0 ,

i = 1, 2, . . . , n .

Dafalias and Popov [1975] have reduced the number of surfaces at two, one corresponding to the conventional yield surface and the other is a bounding surface.

dynamic

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

Yield Conditions

dynamic

35

Thus the two surfaces are f = (σ − α)2 − σY2 = 0 ,

f ∗ = (σ ∗ − α∗ )2 − σY∗2 = 0 ,

with α and α∗ the two centers σY and σ ∗ their respective sizes. Valanis [1971] has proposed a new theory in which the present state of the material depends on the present values and the past history of observable variables. The theory is called endochronic and is expressed by z deP ρ(z − z ) dz , σ = 2G dz 0 where the yield surface is a derivable result of the theory. ρ(z) is a material function and z is the intrinsic time deﬁned by dz =

dζ , f (ζ)

where f (ζ) is the non-negative intrinsic time scale, with f (0) = 1 and ζ deﬁned by √ dζ = dεP dεP . Some other further developments will no more be cited. 1.11

Experimental Tests

Some authors have tested the yield surfaces in plasticity or the work-hardening surfaces. Thus Lode [1926] has tested the yield surfaces of Tresca and Mises. Some of his results are shown in Fig. 1.11.1. One can see that he found mostly the Mises yield condition to be satisﬁed. He has tried steel, copper and nickel, and he ﬁnd all to better satisfy the Mises condition. Also from the old results are to be mentioned the Taylor and Quinney [1931] results. They have tested copper, aluminum and mild steel. From their results we

Fig. 1.11.1

The Lode’s tests results.

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

36

Dynamic Plasticity

give here Fig. 1.11.2. As one can see according to Taylor and Quinney the Mises yield condition is in better agreement with the data, than the Tresca. From the old papers devoted to tests is also the paper of Roˇs and Eichinger [1929]. They have also compared the Tresca and Mises yield condition. Generally they ﬁnd the Mises yield condition in better agreement with experimental data. That is shown on Fig. 1.11.3 given below. From more recent papers in which the authors tried to compare the initial and subsequent yield surfaces in plasticity is the paper of Naghdi et al. [1958]. The initial surface is an ellipse, while the next ones, when only an shearing stress is applied, are deformed, trying to form an pointed corner at a thin walled tube (Fig. 1.11.4). Outer tests are reported by Phillips [1986]. Figure 1.11.5 is shoving some of his results, obtained at several temperatures shown. No lateral inﬂuence is shown but a signiﬁcant Bauschinger eﬀect is there. The surfaces are translated and deformed. The last authors are Williams and Svensson [1970] [1971]. In the ﬁrst paper they try to apply a tensile plastic strain to 1100-F aluminum. They found again a

Fig. 1.11.2

Experimental results of Taylor and Quinney [1931].

Fig. 1.11.3

Experiments of Roˇs and Eichinger [1929].

dynamic

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Yield Conditions

Fig. 1.11.4

The tests of Naghdi et al. [1958] for initial and subsequent yield loci.

Fig. 1.11.5

Second, third and fourth subsequent yield surfaces (Phillips [1986]).

dynamic

37

considerable Bauschinger eﬀect, but they found also a cross eﬀect. They found also corners in tension, as shown in Fig. 1.11.6. In another paper they apply a torsion plastic prestrain. This time they do not ﬁnd corners, but strong Bauschinger eﬀect is still there.

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

38

Dynamic Plasticity

Fig. 1.11.6

Comparison of initial and subsequent yield loci (Williams and Svensson [1970]).

Fig. 1.12.1

1.12

Tests done with various velocities.

Viscoplasticity

In all the constitutive equations of plasticity, they are time-independent. Thus several phenomena cannot be represented. For instance, if one is doing the same experiment with various speeds, one is obtaining distinct curves as a result (see Fig. 1.12.1). That cannot be described with a time-independent constitutive equation. Also, if we stop the test at a certain stress level, and we quip the stress constant, we observe a phenomena which is creep (Fig. 1.12.2). Also, if we quip the strain constant we observe that the stress relaxes. Any other behavior intermediate is possible. There are a number of materials which have such mechanical propriety which cannot be described: waxes, heavy oils, pastes, butter, creams, tooth pastes, etc. For such materials a new type of model was developed. It is called Bingham body.

dynamic

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

Yield Conditions

dynamic

39

σ creep

relaxation

ε 0 Fig. 1.12.2

Curves for creep or stress relaxation.

The assumptions for Bingham bodies are: Incompressibility, i.e., tr ε˙ = 0 . A viscoplastic function is deﬁned as g(σ ij ) :=

(1.12.1)

IIσ − k .

The constitutive equation is: 0 ε˙ij = 1 k √ 1 − σ˙ ij 2η IIσ

(1.12.2)

if IIσ ≤ k 2 if IIσ > k 2 .

(1.12.3)

Here k and η are two constants which characterize the model. They are absolute constants or relative constants, i.e., they may depend on the particle X. From (1.12.3) we get: σ = K + G ,

(1.12.4)

Gij = 2η ε˙ij

(1.12.5)

G is due to a Newtonian viscosity

with η a viscosity coeﬃcient. K is a plastic deviatory stress in the sense of Saint-Venant: f (K) : = IIK − k 2 ≤ 0 yield condition ε˙ij = 2λKij .

(1.12.6) (1.12.7)

We assume η > 0 and λ ≥ 0 with λ

= 0 if f (Kij ) < 0 > 0 if f (Kij ) = 0 .

(1.12.8)

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

40

dynamic

Dynamic Plasticity

II σ ′

overstress

II σ ′ = k 2

σ′

0 '

ε′ij

0

Rigid Viscoplastic

Fig. 1.12.3

The Bingham model.

From (1.12.7), (1.12.5) and (1.12.4) we get = (1 + 4ηλ)Kij σij

(1.12.9)

and for the invariants IIσ = (1 + 4ηλ)2 IIK .

(1.12.10)

If IIK < k 2 from these formulae follows λ = 0, and from (1.12.10) we have IIσ = IIK < k 2 . If IIK = k 2 from (1.12.8)2 and (1.12.10) follows √ IIσ 1 −1 > 0. (1.12.11) λ= 4η k From here we have IIσ > k 2 . Thus the constitutive equation is if IIσ < k 2 0 ε˙ij = 1 k 1− √ σ if IIσ > k 2 . 2η IIσ

(1.12.12)

The states IIσ = k 2 are not in the constitutive equation, so that strain rates for those states are not deﬁned. However, when IIσ k 2 , from (1.12.12) it follows. From here follows that if IIσ is increased the strain rate is also increasing. If IIσ is decreased, the strain rate is decreasing. If IIσ is decreased towards k 2 the strain rates decreases towards zero ε˙ij → 0. Thus we obtain the constitutive equation (1.12.3) (Fig. 1.12.3). If IIσ > k 2 from (1.12.12)2 we get 2 k (2η)2 IIε˙ = 1 − √ IIσ , IIσ

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Yield Conditions

and from here 2η

IIε˙ + k = IIσ .

dynamic

41

(1.12.13)

If IIσ < k 2 from (1.12.12)1 we have ε˙ij = 0 or IIε˙ = 0. (1.10.12) can be used to inverse the constitutive equation. We obtain √ undetermined with IIσ ≤ k for ε˙ij = 0 σij = (1.12.14) k ε˙ij for ε˙ij = 0 . 2η + √ IIε˙ Since in some of the problems one is giving the velocity (experimentally suggested) it is useful to get also the stress power. For ε˙ij = 0 from (1.10.14) we obtain ε˙ij = 2k IIε˙ + 4ηIIε˙ (1.12.15) σij and it is expressed in terms of kinematics variables only. Concerning the reference conﬁguration it is the actual one, since strain is not involved. If the model is used with variable k and η (nonhomogeneous) then the reference conﬁguration is the initial one. The generalization of this constitutive equation is presented in the next chapters. There are very many generalizations based on the concept of “overstress” due especially to Krempl and his collaborators (Krempl [1979]). For instance in the paper of Ho and Krempl [2000], the constitutive equation for small strain, for volume preserving inelastic deformation is 3 s−g 1+v 3 s−g 1+v s˙ + = s˙ + F [Γ] , e˙ = e˙ el + e˙ in = E 2 Ek[Γ] E 2 Γ where s and e are the deviator stress and strain tensors, respectively. The inelastic part of the ﬂow law can either be written using the decreasing, positive viscosity function k[Γ] with k[0] = 0 having the dimension of time, or in terms of the increasing, positive ﬂow function F [Γ] with F [0] = 0 having the dimension of 1/time. The overstress invariant is 3 tr ((s − g)(s − g)) Γ= 2 and g is the deviator of the equilibrium stress. The elastic volumetric relation augments the deviator law by 1 − 2v tr σ˙ . tr ε˙ = E The new growth law for the deviator state variable equilibrium stress g is s−g ψ[Γ] ˙ ψ[Γ] g−f s˙ + + 1− f. g˙ = − E p˙ E k[Γ] A + βΓ E For the deviator kinematics stress f we have ˆt s − g E f˙ = E k[Γ]

January 12, 2007

42

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

dynamic

Dynamic Plasticity

and ﬁnally a simple growth law for the secular isotropic stress is A˙ = Ac (Af − A)p˙ . The positive, decreasing shape function ψ[Γ] controls the transition from the initial quasi linear behavior to ﬁlly established ﬂow and is bounded by E > ψ[Γ] > Et where Et is the tangent modulus at the maximum strain of interest. It is related ˆt = Et (1 − (Et /E)). The ˆt by E to the tangent modulus based on inelastic strain E eﬀective inelastic strain rate is given by p˙ = Γ/(Ek[Γ]) = F [Γ]. The quantities Ac and Af are constants with no dimension and of the dimension of stress, respectively. Ac controls the speed with witch the ﬁnal value of A, i.e., Af , is reached. The model is slightly changed to describe various eﬀects, as: relaxation, the cyclic Swift eﬀect, the pre-necking and post-necking relaxation, creep, free-end torsion, rate-dependent deformation behavior of metals and solid polymers, high temperature applications, etc. 1.13

Rate Type Constitutive Equations

From now on, we will assume that always exists an instantaneous elastic response. It always exists for one-dimensional rate-type models, i.e., for any given state. If a jump in strain is produced, the stress also jumps and its jump is uniquely determined by the strain alone. For several components of stress it is no more so evident. We will assume however that the instantaneous response is path independent. From physical point of view one can accept this assumption, and from experimentally point of view one is not able to imagine tests which will contradict. The purpose of this section is (Suliciu [1989]), to examine the consistency of a simpliﬁed form of the instantaneous modules with the requirement of existence of instantaneous elastic response. The constitutive equation we deal with is of the form ˙ = ε(E, T)E ˙ + G(E, T, k) , T

ˆ k˙ = k(E, T, k) ,

(1.13.1)

where E and T are symmetric and objective strain and stress tensors conjugated with respect to the stress power w: w=

1 ˙ , T·E ρ0

(1.13.2)

where ρ0 is the mass density in the reference conﬁguration, and k is a isotropic workhardening parameter. T is the Cauchy stress tensor and E is the strain tensor. For a body modeled by constitutive equation (1.13.1), a process starting at a state (E0 , T0 , k0 ) ∈ D is a curve (E(t), T(t), k(t)) in D for t ∈ [0, t0 ), t0 ≥ 0 with E(0) = E0 , T(0) = T0 , k(0) = k0 which veriﬁes (1.13.1). One may term the set De from D where both G and kˆ vanish the equilibrium set of the model since a process starting at such a state, and generated by the

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Yield Conditions

dynamic

43

constant strain E(t) = E0 for all t ≥ 0 will be the constant process (E(t) = E0 , T(t) = T0 , k(t) = k0 ) for all t ≥ 0. Depending on the structure of the equilibrium set De we may classify the models described by the constitutive equation of the form (1.13.1) as viscoelastic or viscoplastic models. If the function G in (1.12.1) is independent of k and if there is a function of strain TR (E) for E in some strain domain DE ⊂ S such that (E, TR (E)) ∈ D for all E ∈ DE and G(E, T) = 0 if and only if T = TR (E) then the model may be called viscoelastic (the evolution equation for k may be disregarded). In other terms, the model is called viscoelastic if the equilibrium state of stress is determined by the state of strain alone. The model (1.13.1) may be called viscoplastic if the equilibrium set De contains an open set in D and De ⊂ D is a strict inclusion. The inﬂuence of the temperature in one-dimensional stress–strain curves are described by many authors. For stainless steel it is given in Xue et al. [2004] which wave used an explosion technique to study the thick-walled cylinder under highstrain deformation of ∼ 104 s−1 . The shear-band initiation and propagation were examined. Several grain size were considered. 1.14

General Principles

For the general principles, see Malvern [1969], Mase and Mase [1999] and Fung and Tong [2001]. Let us consider a volume V bounded by a ﬁxed surface S. Conservation of Mass. ! The mass is M = V ρ dV . The rate of increase of mass is (Fig. 1.14.1): ∂ρ ∂M = dV (1.14.1) ∂t V ∂t if no mass is created or destroyed inside. That ! ! must be equal to ! the rate of inﬂow ˆ dS = − V ∆ · (ρv) dV , the trough the surface which is S −ρvn dS = − S ρv · n last one is coming from the divergence theorem. Combining with (1.14.1) we have ∂ρ + ∆ · (ρv) dV = 0 . ∂t V Thus must be true for arbitrary V , thus ∂ρ + ∆ · (ρv) = 0 ∂t or, in rectangular Cartesian coordinates ∂ρ ∂(ρvi ) + = 0. ∂t ∂xi Since ∂ρ ∂vi ∂(ρvi ) = vi + ρ , ∂xi ∂xi ∂xi

(1.14.2)

(1.14.2a)

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

44

dynamic

Dynamic Plasticity

nˆ

v

P V dS

S

Fig. 1.14.1

The reference volume in space.

and from the material derivative ∂ρ ∂ρ dρ = + vi , dt ∂t ∂xi the above law is dρ ∂vi +ρ =0 dt ∂xi

(1.14.3)

or in vector form dρ + ρ div v = 0 . (1.14.3a) dt That is the continuity equation due to Euler in 1757. If the density of all the particles is constant, then div v = 0 ,

(1.14.4)

which is the condition of incompressibility. The continuity condition can be written in material form. If V is the volume of material at time t, and V0 the volume at the same material at time t0 , we have (Fig. 1.14.2) ρ(X, t0 ) dV0 = ρ(x, t) dV = ρ(x(X, t), t)|J| dV0 V0

V

V0

with |J| the absolute value of the Jacobian determinant " " ∂x ∂x " " ∂x " " " ∂X ∂Y ∂Z "" " " " ∂y ∂y " " ∂y J ≡" ". " ∂X ∂Y ∂Z "" " " " ∂z ∂z " " ∂z " " ∂X ∂Y ∂Z

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

Yield Conditions

dynamic

45

x = χ ( X , t ).

m0 V0

m

R

V

Fig. 1.14.2

The material form of continuity condition.

ρbdV

dV

tdS

V dS

S Fig. 1.14.3

The momentum balance.

! We have from conservation of mass V0 [ρ0 − ρ|J|] dV0 = 0. But for arbitrary volume V0 we have ρ|J| = ρ0 , and since at t = t0 we have no empty spaces, ρ = ρ0 > 0 it follows J = 1 and therefore J > 0 for t > t0 . Therefore we have ρJ = ρ0 .

(1.14.5)

This is also due to Euler in 1762. Equation of Motion. Let us consider a body V (see Fig. 1.14.3), which is a closed thermodynamic system, which is not exchanging matter. We postulate that d t dS + ρb dV = ρv dV , dt V S V

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

46

dynamic

Dynamic Plasticity

! ˆ · T, where (d/dt) is the material derivative of the integral. If we replace here t = n we have in Cartesian coordinates d Tji nj dS + ρbi dV = ρvi dV . dt v S V Using the divergence theorem to pass to a volume integral, and since ρ dV = const ., we can write dvi ∂Tji dV = 0 . + ρbi − ρ ∂xj dt V For an arbitrary V , ∂Tji dvi , + ρbi = ρ ∂xj dt

(1.14.6)

which are the equations of motion of Cauchy’s. In vector form, they can be written ∆ · T + ρb = ρ

dv dt

(1.14.6a)

independent of the system of coordinates. For the equilibrium problems we have ∆ · T + ρb = 0. Moment of Momentum Principle. The total moment of momentum is

(r × t) dS + S

(r × ρb) dV = V

d dt

(r × ρv) dV V

and in Cartesian components d ermn xm tn dS + ermn xm bn ρ dV = ermn xm vn ρ dV . dt V S V Here we take care that tn = Tjn nj , we use the divergence theorem

xm Tjn nj dS = S

V

∂(xm Tjn ) dV , ∂xj

and ρ dV = const., to obtain d(xm vn ) ∂(xm Tjn ) ρ dV . ermn + xm bn ρ dV = ermn ∂xj dt V V If we develop the derivatives ∂Tjn dvn dxm vn + xm dV . ermn xm + δmj Tjn + ρxm bn dV = ermn ∂xj dt dt V V

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

Yield Conditions

dynamic

47

Grouping now the terms we have dvn ∂Tjn + δmj Tjn dV = ermn xm + ρbn − ermn vm vn dV . ∂xj dt V V We ! take into account that ermn vm vn = 0 since vm vn is symmetric in mn, so that e T dV = 0, or of any V , ermn Tmn = 0. Thus for r = 1 we have T23 − T32 = V rmn mn 0, and so on. Thus the stress tensor is symmetric. Energy Balance. We chose again a closed thermodynamic system not exchanging mater with the surroundings. The work is on the system, not by the system. Power input is t · v dS + ρb · v dV . Pinput = S

In Cartesian coordinates

V

Pinput =

Tji nj vi dS +

S

ρbi vi dV V

∂vi ∂Tji vi dV = + ρbi + Tji ∂xj ∂xj V dvi = + Tji [Dij + Wij ] dV vi ρ dt V 1 d (vi vi ) ρ dV + = Tji Dij dV dt V 2 V d 1 = Tij Dij dV . ρvi vi dV + dt V 2 V In vector form we have Pinput =

d dt

V

1 ρv · v dV + T : D dV . 2 V

Thus the rate of work which is the power input is equal to the variation of the kinetic energy plus the total stress power. The heat input rate is ˆ dS + ρr dV , Qinput = − q · n S

V

where the ﬁrst integral is the heat ﬂux through the surface of contact S (q is the heat ﬂux vector), while the second is the distributed internal heat source of strength r per unit mass. The total energy E is E˙ total = K˙ + U˙ = Pinput + Qinput ,

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

48

dynamic

Dynamic Plasticity

where K is the kinetic energy and U the internal energy (elastic stored energy, and all other nonspeciﬁed energies). Thus we have dK d dK + + ρu dV = T : D dV dt dt V dt V ˆ dS + ρr dV . + − q·n S

V

Simplifying and transforming the surface integral in a volume integral, we have for arbitrary V in vector form and coordinate form: ρ

du = T : D + ρr − ∆ · q , dt

(1.14.7) du ρ = Tij Dij + ρr − qj,j , dt which is the energy equation due to Kirchhoﬀ in 1894. Here ρ du/dt is the rate of increase of the internal energy ρu per unit volume, ρr is the internal supply of heat per unit volume, and −qi,i the inﬂow per unit volume of heat through the boundaries of the element. In elasticity the heat transfer is insigniﬁcant. But in plasticity we have a heating due to the plastic deformation, a heating at the tectonic plates, volcanoes, etc. The Second Law of Thermodynamics. If we introduce the Piola–Kirchhoﬀ stress tensor 1 ˜ S = ρ−1 T(FT )−1 = S , (1.14.8) ρ0 the energy balance can be written ρe˙ − ρSij F˙ij +

∂qi = ρr . ∂xi

(1.14.9)

The entropy rate γ is deﬁned as ρr q + div , (1.14.10) θ θ where η = η(X, t) is the entropy per unit mass while θ = θ(X, t) > 0 is the absolute temperature. The second law of thermodynamics, or the Clausius–Duhem inequality (not used here), states that (Truesdell and Toupin [1960]) ργ = ρη˙ −

γ ≥ 0.

(1.14.11)

From (1.14.9), (1.14.10) and (1.14.11) follows γ = η˙ −

e˙ 1 ∂θ + θ−1 Sij F˙ij − 2 qi ≥ 0. θ ρθ ∂xi

If one introduces the free energy ψ = e − θη ,

(1.14.12)

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Yield Conditions

dynamic

49

then (1.14.12) can be expressed as θγ = −ψ˙ − η θ˙ + Sij F˙ij −

1 ∂θ qi ≥ 0. ρθ ∂xi

(1.14.13)

˜ given by (1.14.8), we can write the balance equations in initial Using the tensor S coordinates ρ0

∂vi ∂ S˜ij − = ρ0 b i , ∂t ∂Xj

(1.14.14)

∂ q˜i ∂e ∂Fij − S˜ij + ρ0 = ρ0 r , ∂t ∂t ∂Xi ˜ = JF−1 q (see Green and Rivlin [1964a,b]). with q A regular surface Σ with equation ϕ(X, t) = 0, is called an acceleration wave through the body if ϕ is continuous and their derivatives may have jump discontinuities across Σ, while being continuous at all points. The quantities U =−

∂ϕ/∂t , |Grad ϕ|

ni =

∂ϕ/∂Xi , |Grad ϕ|

(1.14.15)

are called the propagation speed and the direction of propagation of the acceleration wave, respectively. ˜ ψ, . . . cannot be independent; they have The jumps of the derivatives of v, F, θ, S, to satisfy three types of conditions. The geometric and kinematics compatibility conditions give those relations between the jumps of ∂v/∂t, ∂v/∂X, etc., that are due to the continuity of v or follow from the fact that v and F are the partial derivatives of the same vector function χ. These compatibility conditions can be written as ∂Fkl ∂Fkl ∂vk ∂vk = U 2 ak , = −U ak nl , = ak n l n j , = ∂t ∂Xj ∂Xl ∂t ∂θ ∂θ = −U v , = vnj , (1.14.16) ∂t ∂Xj # $ $ # ∂ S˜ij ∂ S˜ij = −U sij , = sij nk , etc. ∂t ∂Xk Here [f ] = f + − f − , f + being the limit value of f at a point on the surface Σ, reached from the positive side of the normal (n, −U ) to Σ at that point, and f − being the limit value of f at the same point but reached from the other side of the surface. The vector a = (a1 , a2 , a3 ) is called the mechanical amplitude of the wave, the scalar v is called the thermal amplitude of the wave and sij may be called the stress amplitude, etc.

January 12, 2007

10:41

50

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Dynamic Plasticity

The second group of restrictions imposed on the jumps comes from the balance equations. They are called dynamic compatibility equations and they are obtained from (1.14.14) as follows: one considers (1.14.14) on each side of the surface Σ and then, after taking limit values at a point on Σ, one calculates the diﬀerence between the two obtained relations. Since b and r are assumed continuous, one obtains the following homogeneous dynamic compatibility conditions. # ˜ $ ∂ Sij ∂vi − = 0, ρ0 ∂t ∂Xj (1.14.17) ∂ q ˜ ∂e ∂F ij j − S˜ij + = 0. ρ0 ∂t ∂t ∂Xj The third group of restrictions is imposed by the constitutive equations, i.e., ˜ η, ψ and q. These restricthose relations that must exist between F, θ, Grad θ, S, tions will be discussed in the other chapters. In case of an isolated discontinuity surface, the geometric-kinematic and dynamic compatibility conditions have been presented for the ﬁrst time by Hadamard [1903] for the general three-dimensional case. Bibliography Bruhns O. T., Xiao H. and Meyers A., 2005, A weakened form of Ilyushin’s postulate and the structure of self-consistent Eulerian ﬁnite elastoplasticity, Int. J. Plasticity 21, 199–219. Dafalias Y. F. and Popov E. P., 1976, Plastic internal variables formalism of cyclic plasticity, J. Appl. Mech. 43, 645–651. Drucker D. C., 1951, A more fundamental approach to plastic stress–strain relations, Proc. 1st U.S. Natl. Cogr. Appl. Mech., 487–491. Fung Y. C. and Tong P., 2001, Classical and Computational Solid Mechanics, World Scientiﬁc, 930 pp. Green A. E. and Rivlin R. S., 1964a, Simple force and stress multipoles, Arch. Rational Mech. Anal. 16, 5, 325–353. Green A. E. and Rivlin R. S., 1964b, Multipolar continuum mechanics, Arch. Rational Mech. Anal. 17, 2, 113–147. Hadamard J., 1903, Le¸cons sur la Propagation des Ondes et les Equations de l’Hydrodynamique, Herman, Paris. Hencky H., 1924, Zur Theorie plastischer Deformationen und der hierdurch hervorgerufenen Nachspannungen, Zeits. Angew. Math. U. Mech. 4, 323–334. Ho K. and Krempl E., 2000, Modeling of positive, negative and zero rate sensitivity by using the viscoplasticity theory based on overstress (VBO), Mech. Time-Dep. Materials 4, 21–42. Iliushin A. A., 1961, On the postulate of plasticity, Prikl. Mat. Mech. 25, 503. Koiter W. T., 1953, Stress–strain relations, uniqueness and variational theorems for elastic, plastic materials with a singular yield surface, Q. Appl. Math. 11, 350–354. Krempl E., 1979, Viscoplasticity based on total strain: The modeling of creep with special considerations of initial strain and aging, J. Eng. Mat. Tech. 101, 380–386.

dynamic

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Yield Conditions

dynamic

51

Lode W., 1926, Versuche uber den Einﬂuss der mittleren Hauptspannung auf das Fliessen der Metalle Eisen, Kupfer, und Nickel, Z. Physik 36, 913–939. Malvern L. E., 1969, Introduction to the Mechanics of a Continuous Medium, PrenticeHall, Inc., 713 pp. Mase G. Th. and Mase G. E., 1999, Continuum Mechanics for Engineers, CRC Press, 377 pp. Mises R. von, 1913, Mechanik der festen K¨ orper in plastisch deformable Zustand, Nachr. Akad. Wiss. G¨ ottingen Math.-Phis. K1 H.4, 582–592. Mr´ oz Z., 1969, An attempt to describe behaviour of metals under cyclic loads using a more general workhardening model, Acta. Mech. 7, 199–212. Nadai A., 1923, Der Beginn des Fliessvorganges in einem tortierten Stab, Zeits. Angew. Math. Mech. 3, 442–456. Naghdi P. M., Essenburg F. and Koﬀ. W., 1958, An experimental study of initial and subsequent yield surfaces in plasticity, J. Appl. Mech. 25, 201–209. Phillips A., 1986, A review of quasistatic experimental plasticity and viscoplasticity, Int. J. Plasticity 2, 315–328. Prager W., 1959, An Introduction to Plasticity, Addison-Westley Publishing Co. Prandtl L., 1924, Spannungsgsverteilung in plastischen Koerpern, Proc. 1st Int. Congr. Appl. Mech. (Delft), 43–54. Reuss E., 1930, Beruecksichtigung der elastischen Formaenderungen in der Plasizitaets theorie, Zeits. Angew. Math. U. Mech. 10, 266–274. Ros M. and Eichinger A., 1926, Proc. 2nd Int. Congr. Appl. Mech. (Z¨ urich), 315. Ros M. and Eichinger A., 1929, Metalle Diskussionsbericht No. 34 der Eidgenossen Materialprufungsanstalt, Zurich, 315. Saint-Venant, Barr´e de., 1870, M´emoire sur l’´etablissement des ´equations diﬀ´erentielles des mouvements int´erieure op´er´es das les corps solides ductiles au del` a des limite o` u l’´elasticit´e pourrait les ramener ` a leur premier ´etat, C. R. Ac. Sci. (Paris) 70, 473–480. Stoughton T. B. and Yon J. W., 2005, Review of Drucker’s postulate and the issue of plastic stability in metal forming, Int. J. Plasticity (in print). Suliciu I., 1989, Some remarks on the instantaneous response in rate-type viscoplasticity, Int. J. Plasticity 5, 173–181. Taylor G. I. and Quinney H., 1931, The plastic distortion of metals, Philos. Trans. Roy. Sos. London A 230, 323–362. Tresca H., 1868, Memoire sur l’ecoulment des corps solides, M´em. Sav. Acad. Sci. Paris, 733–799. Truesdell C. and Toupin E. R., 1960, The Classical Field Theories, Handbuch der Physik, Vol. III/1, Springer Verlag, Berlin. Valanis K. C., 1980, Fundamental consequences of a new intrinsic time measure plasticity as a limit of the endoshronic theory, Arch. Mech. 32, 171. Williams J. F. and Svensson N. L., 1970, Eﬀect of tensile prestrain on the yield locus of 1100-F Aluminium, J. Strain Analysis 5, 2, 128–139. Williams J. F. and Svensson N. L., 1971, Eﬀect of torsional prestrain on the yield locus of 1100-F Aluminium, J. Strain Analysis 6, 4, 263–272. Xue Q., Meyers M. A. and Nesterenco V. F., 2004, Self organization of shear bands in stainless steel, Mater. Sci. Eng. A 384, 35–46.

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

This page intentionally left blank

dynamic

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

dynamic

Chapter 2

Rocks and Soils

2.1

Introduction

The constitutive equation for rocks or soils is much more complicated. The reason is that the experimental results are much more involved. Even the elastic constants are no more what they were for metals, and the methods of ﬁnding them from tests are diﬀerent from what we know from metals. The yield conditions are diﬀerent. While for metals a cylindrical constitutive yield condition, independent of the mean stress is quite normal, such a yield condition for rocks is not acceptable. One has tried to introduce a yield condition depending also on mean stress and on the third deviator stresses F (Iσ , IIσ , θ) = 0 , where θ=

√ 3 3IIIσ 1 sin−1 3 3 2 IIσ

is the Lode angle. The most familiar are the Mohr–Coulomb and Drucker–Prager yield conditions. The ﬁrst condition is written τ = c − σ tan φ with 1√ σc σt c= 2

−1

and φ = sin

σc − σt σc + σt

with 0 ≤ φ

0, σ > 0. We write the displacement on one side and another side and because this displacement is the same (du)− = v − dt + ε− dx (du)+ = v + dt + ε+ dx or [v] = −c[ε] .

(3.5.2)

This is the kinematics condition. c X1

X2

+

ε + [ε ] v + [v ] Fig. 3.5.4

− Y (t )

ε v

Formation of shock waves.

→x

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

138

dynamic

Dynamic Plasticity

We write now the balance of linear momentum. We have d Y (t) d X2 ρv(X, t) dX + ρv(X, t) dX dt X1 dt Y (t)

X2

=

ρb(X, t) dX + σ(X2 , t) − σ(X1 , t)

X1

or making the derivatives Y (t) X2 ∂v(X, t) ∂v(X, t) dX − ρv − (Y (t), t)Y˙ (t) + dX ρ ρ ρv + (Y (t), t)Y˙ (t) + ∂t ∂t Y (t) X1

X2

=

ρb(X, t) dX + σ(X2 , t) − σ(X1 , t) .

X1

We introduce new notations when X1 → Y (t), X2 → Y (t) and v + (Y (t), t) = lim v(X, t) X → Y (t) X < Y (t) and the velocity of propagation c = Y˙ (t). With these notations we obtain cρ[v] = −[σ] which is the dynamic jump condition. We obtain also from here 1 [σ] c= ρ [ε]

(3.5.3)

(3.5.4)

for the velocity of propagation. It is certainly not independent and does not coincide with the velocity of the acceleration waves. We have a total of four unknown functions σ, ε, v, c but we have only three equations. Another condition is obtained from boundary conditions or some other condition which may result from the problem. This is a very simple theory, which replaces the diﬀerential relations with algebraic linear equations. It allows an elementary study of the interaction between elastic (loading and unloading) and plastic waves. It also allows a very simple description of reﬂection and refraction of waves. Reﬂection of waves. When waves are reﬂected from the end of the bar, many situations may arise, depending on whether the end of the bar is free, ﬁxed, or whether the bar continues with another bar, with diﬀerent material proprieties. If an impact is produced at one end x = −l of the bar, the ﬁrst wave to reach the other end x = 0 is always an elastic wave and σ = −ρc0 v. The displacement due to this elastic wave is u1 = f1 (c0 t − x) ,

(3.5.5)

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

The Propagation of Longitudinal Stress Waves

dynamic

139

where f1 is an arbitrary function to be determined by the initial conditions. The corresponding stress is σ1 = E(∂u1 /∂x) = −ρc0 (∂u1 /∂t)

(3.5.6)

for the inverse waves (propagating in the opposite direction) u2 = f2 (c0 t + x) ,

(3.5.7)

σ2 = E(∂u2 /∂x) = ρc0 (∂u2 /∂t) .

(3.5.8)

and

Let us consider the case when the end x = 0 of the bar is free. After the reﬂection of the elastic wave, the total stress will be σ = σ1 + σ2 = E{f2 (c0 t + x) − f1 (c0 t − x)} .

(3.5.9)

But at the end x = 0 the stress vanishes for all t f2 (c0 t) − f1 (c0 t) = 0 .

(3.5.10)

One can therefore conclude that f1 (z) = f2 (z) = f (z), and the displacement after reﬂection will be u = u1 + u2 = 2f (c0 t) .

(3.5.11)

Furthermore, due to reﬂection at the free end the displacement produced by the wave is doubled, as is also the velocity. With regard to stress, we have in this case σ1 = −σ2 , i.e., a compressive wave is reﬂected as a tensile one and vice versa. If we now assume that the second end of the bar is ﬁxed rigid, then the displacement of this end is zero for all t f1 (c0 t) + f2 (c0 t) = 0 , and therefore f1 (z) = −f2 (z), i.e., the displacement produced by the reﬂected wave is equal to that produced by the incident wave, but in the reverse direction. This stress σ = σ1 + σ2 = 2Ef2 (c0 t)

(3.5.12)

is doubled due to reﬂection from the ﬁxed end. For this reason, an elastic wave can be reﬂected a plastic one, if on reﬂection, the stress carried by the reﬂected wave exceeds the yield stress. If the bar is continued with another one, possessing diﬀerent mechanical properties the situation is more complicated: a reﬂected wave of intermediate intensity will propagate from the end of the bar, but at the same time a wave will also be reﬂected in the other medium (see Kolsky [1953]). The previous arguments are generally also valid for plastic waves. The ﬁnite bar. Many authors have considered the problem of normal impact of a ﬁnite bar against a rigid target. Let us examine the problem as done by Lenski [1949]. A bar of length l moves with velocity V from right to left (Fig. 3.5.4).

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

140

dynamic

Dynamic Plasticity

−εY

−ε

0

−σ Y −σ Fig. 3.5.5

Elastic linearly work-hardening plastic bar striking a rigid target.

x=

c1 t

t

x=

c 0t

σ =0 0

x Fig. 3.5.6

The ﬁrst waves to propagate in the bar.

At time t = 0 the bar strikes a rigid wall x = 0. It is assumed that the impact velocity is suﬃciently high to produce elastic-plastic strains and that the material of the bar is linear work-hardening. Due to the sudden impact and linear workhardening only shock waves are considered. Thus, after impact two shock waves, one elastic and one plastic will propagate. Their wave fronts delimitate three distinct regions in the bar. In the ﬁrst region (Fig. 3.5.6) ε0 = 0, v0 = −V , in the second region ε1 = −εY , σ1 = −EεY and v1 = −V + c0 εY . In the third region v2 = 0 and ε2 = (1/c1 )(c0 εY − V ) − εY ,

σ2 = (E1 − E)εY + E1 ε2 .

(3.5.13)

Therefore, for the plastic strains to appear, the velocity of impact must satisfy the condition V > c0 εY . After the time t = l/c0 the elastic wave front is reﬂected from the free end. Behind this front σ3 = ε3 = 0 ,

v3 = 2c0 εY − V .

(3.5.14)

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

dynamic

The Propagation of Longitudinal Stress Waves

141

σ t

ε2

4′′

ε 4′′

ε 4′

ε σ4

4′ 3

2 1

0

S Fig. 3.5.7

σ2

l

x

Stresses and strains during unloading after the ﬁrst reﬂexion.

When the wave fronts of the plastic and of the elastic unloading waves meet at the section S (Fig. 3.5.7) several situations are possible, depending on the magnitude of the velocity V . Let us consider ﬁrst the case when, after the two wave fronts have met, the plastic wave does not propagate any more. In this case the elastic waves will spread in both directions from S (Fig. 3.5.10). The leftward wave is always an elastic one. On both sides of the section S the particle velocities are equal to v4 = v4 , otherwise the bar will break. From the balance of the force it also follows that, σ4 = σ4 (the stresses are initial stresses). The strains in the two regions will be diﬀerent. In the region 4 the material is in an elastic state, the yield point was never reached, while in the region 4 the material is also in an elastic state, but is being unloaded after a plastic deformation. This situation is shown in Fig. 3.5.7. Thus the stress–strain relation that acts on the two sides of the section S is σ = Eε

and σ = σ2 + E(ε − ε2 ) . σ4

σ4 ,

v4

(3.5.15)

v4

From these relations and the conditions = = and the jump conditions, we obtain c 0 + c1 2c2 + c0 c1 − c21 ε4 = (c0 εY − V ) , ε4 = 0 (c0 εY − V ) , 2 2c0 2c20 c1 3c0 − c1 (c0 εY − V ) + V . 2c0 Thus the strain is discontinuous across the section S. This is a non-propagable discontinuity surface. If the plastic wave stops at S (Fig. 3.5.10), the strain for x > xS must be bigger than the strain corresponding to the yield stress ε4 > −εY . From this condition it follows that 2c0 ε Y c0 . V < 1+ c 0 + c1 v4 = v4 =

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

142

dynamic

Dynamic Plasticity

σ

t

ε2

ε5 σ5

5 4′′

ε

4′ 3

2 1 0 0

S Fig. 3.5.8

l

x

Possible separation from the wall at the ﬁrst reﬂection.

If we have also v4 = v4 > 0 when the elastic wave propagating to the left reaches the end of the bar, this end can possibly be pulled away from the wall (Fig. 3.5.8). If the separation takes place σ5 = 0 and c20 − c21 (c0 εY − V ) , v5 = 2c0 εY − V , c20 c1 where εP is the plastic strain. The plastic strain is constant in the part of the bar to the left of section S, whose length is ε5 = −εP =

xS = 2c1 l/(c0 + c1 ) . From here we obtain also the separation condition V < 2c0 εY . The time during which the bar is in contact with the wall is 2l/c0. After the separation the bar will have a sudden change of diameter. If the inequality 2c0 c0 ε Y 2c0 εY < V < 1 + c 0 + c1 is satisﬁed, then the elastic waves will again propagate from S in both directions, but the bar will continue to touch the wall for a little longer: 4l/(c0 + c1 ). Now the elastic wave propagating to the right is reﬂected and when it arrives at the impact end separation takes place. If ﬁnally the inequality 2c0 c0 ε Y V > 1+ c 0 + c1 holds, then ε4 < −εY and the plastic wave continues to propagate to the right from the section S (Fig. 3.5.10). There are two possibilities. Either the elastic wave which

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

dynamic

The Propagation of Longitudinal Stress Waves

143

σ ε2 ε6

t S1

S

σ3 E

C B

6 2

5

ε 4 = −ε Y

D

4

•

•

ε

σ 4 = −σ Y σ5 =σ6

A

σ2 1 0 x

Fig. 3.5.9

Characteristic ﬁeld for the case when two stationary discontinuities occur.

propagates to the left from S is reﬂected from the end x = 0 and then meets the plastic wave at S1 , which in the meantime continues to propagate. Or the elastic wave which propagates from S to the right and is reﬂected from the end x = l meets the plastic wave ﬁrst. That depends on the velocities of propagation of the elastic and plastic waves. In Fig. 3.5.9 the ﬁrst of these two possible cases is represented, when c0 /c1 > 4.236. Now the length of the plastically deformed portion of the bar, the abscissa of the section S1 , is xS1 = 2lc1 /(c0 + c1 ) . The magnitudes of the strain and velocity in regions 1, 2 and 3 coincide with those given in the previous example. In region 4, since ε = −εY , it follows that v4 = 3c0 εY − V . The stresses in regions 5 and 6 are equal and satisfy the relations: σ5 + σY = E(ε5 + εY ) and σ6 − σ2 = E(ε6 − ε2 ) . Using the momentum equation for shock waves together with the condition v6 = v5 and the previous relation we obtain (Fig. 3.5.10) ε5 =

3c20 − c21 V εY − , c1 (c0 + c1 ) c1 v5 = v6 =

ε6 =

c21 + c20 V εY − , c1 (c0 + c1 ) c1

2c0 c1 εY . c 0 + c1

Finally the bar will possess two stationary discontinuity fronts. If necessary the analysis can be continued in a similar way for greater impact velocities. Many such kinds of problems, described only by shock waves, can be found in the papers by De Juhasz [1949a], [1949b] and in the book by Rakhmatulin and Demianov [1961].

January 12, 2007

10:41

144

Dynamic Plasticity

Fig. 3.5.10

3.6

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Elastic linearly work-hardening plastic bar striking a rigid target.

Examples

The examples given are the impact of two identical aluminum 1100 bars (Cristescu and Bell [1970], Cristescu [1970]). The bars are 25 cm in length and one inch in diameter. The experimental results are due to J. F. Bell published in several papers and the books by Bell [1968, 1973]. Numerical integration method. The constitutive equation is written σ = F (ε) or in an inverse ε = F −1 (σ). F is a strictly increasing function. We consider σ and ε positive in compression. The density is ρ = 0.002757 g cm−4 sec2 . The plastic deformation is εP = F −1 (σ) − σ/E. The characteristics are

dynamic

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

The Propagation of Longitudinal Stress Waves

dynamic

145

dx = ±c = ± dt

E ρ(1 + Eϕ)

(3.6.1)

and dσ = ∓ρcdv .

(3.6.2)

The diﬀerential relations along the characteristics are: dx = 0 (twice)

(3.6.3)

and dεP = ϕdσ

(3.6.4)

EdεE = dσ . The constitutive equation is written as σ˙ 1 σ˙ −1 + χ (F (σ)) − σ˙ = + ϕ(σ)σ˙ ε˙ = E E E and χ=

1

if σ = σm (x)

0

if σ ≤ σY or σY < σ < σm (x) .

(3.6.5)

We introduce the dimensionless variables v kx σ , T = kt , X = . S= , V = E c0 c0 Now we choose the highest value of dx/dt in the whole ﬁeld, i.e., dx/dt = ±c0 or dX/dT = ±1 the bar velocity, with c0 = 5080 m/sec. The principle of the method is an integration along characteristic lines. We will not give details. The method is convergent since the monotone bounded sequence F (ε) < c(i) (σ, ε) ≤ c(i−1) (σ, ε) ≤ · · · ≤ c0 ρ is always satisﬁed. It is very rapid, since we do 2-3 iterations in one point. Initial and boundary conditions. The initial conditions are for the specimen (S): & t=0 :σ=ε=v=0 0≤x≤l and for the hitter (H): t=0

&

−l ≤ x ≤ 0

: σ = ε = 0,

v=V .

The boundary conditions are, if v(0, t) is prescribed: x = l,

t ≥ 0 : σ = 0,

x = −l ,

t ≥ 0 : σ = 0,

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

146

dynamic

Dynamic Plasticity

2l V 0 ≤ t ≤ t∗ = : vH = vS = vmax = c0 2 x=0

t∗ ≤ t < Tc : vH = −vS

or σH = σS = σmax ,

symmetry of motion ,

Tc ≤ t : σS = 0 .

Here Tc is the time of contact between the two bars. The boundary conditions can be prescribed for σ(0, t) if the stress is measured in a hard transmitter bar or with a piezocrystal, and v = −ϕ(σ). The initial conditions are formulated to make economy of computer time and to avoid the singular point O. The ﬁrst initial conditions are named S from shock. An initial shock wave is propagating and reﬂecting from the free end (see Fig. 3.6.1). Thus AR is a tensile unloading shock wave. For a constitutive equation of the form σ = βε1/2 we have along this line: 1 β2 ∗ t. x = −c0 (t − t ) and x = c(σ)t = ρ 2σ From here we get: t2 β2 2 ∗ 2ρc0 (t − t)2 2 3/2 2√ 2 1 2 σ vb (t) = + − σY σY 3β ρ ρc0 3β ρ

σb (t) =

(i)

where “b” stands for “before”. We now use the jump condition to pass at “after” the shock.

t

Tc t

V max

M A

V ! VY

V

0 , t

V max VY

0

Fig. 3.6.1

xM

xA

The initial condition S.

R

VY

l

x

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

dynamic

The Propagation of Longitudinal Stress Waves

147

We have: jump condition : σa − σb = −ρc0 (va − vb ) , after : −σa + ρc0 va = const. , in R : σb = σY = ρc0 vb , σa = 0 . From here we get: 1 σa − σb = − {2σY − (ρc0 vb − σb )} , 2 va = vb −

1 (σa − σb ) , ρc0

(ii)

σa P , εP a = εb . E Though along the line x = −c0 (t − t∗ ) for the data “after” we have: 0 ≤ x ≤ xM : σ = σmax = const. εE a =

xM ≤ x < xA : (i) , xA ≤ x ≤ l : (ii) . These are the initial data along the reﬂected shock wave. We have tested also a second type of initial data called L (linear). There are no shocks now and we have the boundary conditions: t 0 ≤ t ≤ tm = 20 µ sec : σ = σmax , tm x=0 tm ≤ t < Tc : vH = vS , Tc ≤ t : σS = 0 .

Tc

t

σm

ax

t*

σY

tm ty

σ (0, t )

σ max σ Y

σ=

0

x

0

Fig. 3.6.2

l The initial boundary conditions L.

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

148

dynamic

Dynamic Plasticity

Tc t A

V ! VY tm

V (o,t) V max V

0

Fig. 3.6.3

R

σ = σY xA

x

l

x

The initial data of a mixed type M.

Now we get along the line:

∗

x = −c0 (t − t )

and x =

1 β2 ρ 2σ

tm t− σ . σm

From here:

√ √ − 2ρc0 (t∗ − t) + 2ρc20 (t∗ − t)2 + 4β 2 (tm /σmax )t (i) σb = 2β(tm /σmax ) and a similar formula for vb . A mixed initial condition called M (mixed) has also been considered. It is a one dimensional simulation of the three dimensional wave initiations at the end of the bar: a sudden shock up to σ ¯ = 0.794σmax after which follows a linear variation up to σmax reached at tm = 40 µ sec. Thus t ¯+ (σm − σ ¯) , 0 ≤ t ≤ tm = 40 µ sec : σ = σ tm x=0 tm ≤ t < Tc : vH = vS , Tc ≤ t : σS = 0 . We have to ﬁnd x ¯ from

x=

1 β2 t and x = c0 (t∗ − t) . ρ 2¯ σ

We obtain x ¯=

c0 t∗ √ , 1 + c0 2ρ¯ σ /β

from where x ¯ = 2.64D < xA for V = 40 m/sec.

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

The Propagation of Longitudinal Stress Waves

For

dynamic

149

∗ x = c0 (t − t) 0≤x≤x ¯: 1 β2 x = ρ 2¯ σ

we have: √ √ σb = σa √ ¯ )[t − σ ¯ tm /(σmax − σ ¯ )]} −c0 2ρ(t∗ − t) + 2ρc20 (t∗ − t)2 + {4β 2 tm /(σmax − σ = 2βtm /(σmax − σ ¯) and a similar formula for va . In the interval where the reﬂected wave is still felt: x ¯ ≤ x ≤ l : σb =

t2 β2 2ρc20 (t∗ − t)2

if

σb > σa → (ii) ⇒ σa σb ≤ σa → (i) ⇒ σa .

Concerning the constitutive equation we have used three. First was used the dynamic curve σ = Eε ,

σ = σY 1 = 307.5 psi

σ = βε1/2 ,

σ ≥ σY 1 .

with β = 5.6 × 104 psi , E = 10.2 × 106 psi , c0 = 5080 m/sec , εY 1 = 0.00003014 . That was the fundamental constitutive equation. Since the yield stress was not correct, we have translated the parabola to get the correct yield stress. Thus σ = Eε ,

σ ≤ σY 2 = 1100 psi

σ = β(ε + ε0 )1/2 ,

σ ≥ σY 2

and εY 2 = 0.00010784, and ε0 = 0.0002779988 (the translation on horizontal). The quasi-static stress–strain curve is σ = 3.32 × 104 ε3/8 from where: σ = Eε ,

σ ≤ σY 0 = 1068.24 psi

σ = 3.32 × 104 ε3/8 ,

σ ≥ σY 0 .

In the examples σmax is given while vmax is computed. First comparison was for the time of contact Tc which is obtained by observing the interruption of the longitudinal beam of light from a source on one side of the impact faces before, during, and after collision, by means of a photomultiplier tube on the opposite side (Fig. 3.6.4).

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

150

Fig. 3.6.4

Dynamic Plasticity

Time of contact versus velocity; a comparison of theoretical and experimental data.

Fig. 3.6.5

Coeﬃcient of restitution versus impact velocity.

dynamic

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

The Propagation of Longitudinal Stress Waves

dynamic

151

A second comparison with the experimental data is the coeﬃcient of restitution deﬁned e = (2vf − V )/V with vf the ﬁnal velocity (travel time of the free end of specimen after separation) (Fig. 3.6.5). The characteristic planes for the impact for more than 34 m/sec are given in Fig. 3.6.6. L means “loading”, while U means “unloading”. The time of contact coincides with the experiment.

(a)

(b)

Fig. 3.6.6 (a) Characteristic plane for σY = σY 1 and V = 35.85 m/sec. (b) Characteristic plane for σY = σY 2 and V = 34.98 m/sec.

January 12, 2007

10:41

152

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Dynamic Plasticity

Fig. 3.6.7

A comparison of computed strain-time proﬁles with experimental data.

The best comparison with the experiment is on the graph of variation of strain at various cross sections. The graph given is only for the higher yield stress. All three theoretical solutions are shown. Also the time of contact is given (Fig. 3.6.7). The displacement variation is given in Fig. 3.6.8 for the two yield stresses and the three initial boundary conditions. The diameters where the variation is measured are shown. The variation of the stress at the impacted end is shown in Fig. 3.6.9. The initial rise of the stress at the impacted end is not given. The stress plateau is shown very clearly. One has compared also the cross section xA when the reﬂected shock wave is completely absorbed. Both theoretically and experimentally one have found xA between 4 and 5 diameters.

dynamic

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

The Propagation of Longitudinal Stress Waves

dynamic

153

Fig. 3.6.8 Computed displacement-time curves compared with experimental values obtained with an optical displacement technique.

The velocity of propagation is checked by Swegle and Ting [1982]. They have tested if the waves travel with the velocity predicted by the one-dimensional theory, although they have larger rise-times. That was what they have found. In a paper by Jones et al. [1987], a one-dimensional analysis is presented that leads to the appropriate equation of motion for the undeformed portion of a plastic, rigid rod after impact with a rigid anvil. This equation is used as a basis for deducing material properties of the rod material from post-test measurements. Data

January 12, 2007

154

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Dynamic Plasticity

Fig. 3.6.9 Variation of stress in time at the impact end of the bar. The experiment data were obtained with piezo crystal measurements. The dynamic overstress is not included in the present discussion.

for copper, for depleted uranium, for iron and steel are given for velocity surpassing 300 m/s. The impact of a solid cylinder (aluminum) by a compressible ﬂuid (water) is considered by Lush [1991]. The speeds of impact are 10, 100 and 350 m s−1 . The main modiﬁcation of the model is to incorporate the unloading of the plastic wave which is produced by the multiple reﬂections of the elastic release wave. In general the agreement between penetration, rate, contact pressure and depth of penetration is good.

dynamic

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

The Propagation of Longitudinal Stress Waves

dynamic

155

The formation, propagation, and reﬂection of shock waves is studied for synthetic curved cables by Tjavaras and Triantafyllou [1996]. First, analytical solutions are derived for weightless cables with nonlinear stress–strain relation, which are then compared with numerical solutions. For very small curvature the analytical and numerical solutions show that synthetic lines can form shock waves when loaded impulsively. The tension is ampliﬁed signiﬁcantly when a reﬂection occurs, pointing to a probable mechanism of failure. The examples are on Catenary. In another paper by Nonaka et al. [1996] the integration is done again, trying to explain some damage that appeared after earthquakes. One considers ﬁnite thin elastic bars and assumes that the second end is free, then ﬁxed, and in ﬁnal assuming that at the second end the rod is miss-matched impedance. The mechanical impedance is expressed by the change of the velocity by αρc with α > 0. For α very large one obtains various examples for steel: E = 206 GPa, ρ = 7850 kg/m3 , c = 5120 m/s. Several strengths measurements are presented by several papers by Kanel [1999]. The presented experimental data for engineering metals and alloys and for metals single crystals demonstrate the eﬀects of material grain structure and temperature on the resistance to high-rate rupture. Several ﬁgures are given, showing this inﬂuence. A technique for rapid two-stage dynamic tensile loading of polymers, based on a tensile Hopkinson bar apparatus, was developed by Shim et al. [2001]. In this technique, the initial incident wave and its reﬂection are used to load a specimen in quick succession. Consequently, the specimen is stressed, momentarily unloaded, and then reloaded until fracture. A procedure to obtain the associated stress–strain curves for such double-stage loading is formulated. This procedure is examined experimentally and analytically to substantiate their validity. To verify the proposed approach, a relatively rate-insensitive material was subjected to two-stage dynamic tension. The stress–strain curves obtained via the procedure established were compared with results from static loading. A ﬂat-nosed cylinder moving at a suﬃciently high impact velocity is assumed to fracture by Teng et al. [2005]. The fracture mechanism is investigated numerically using ABAQUS/Explicit. The impact velocity of the projectiles ranges from 240 m/s to 600 m/s. It is found that a more ductile cylinder tends to fail by petalling while a less ductile one by shear cracking.

3.7

The Elastic Solution

D’Alembert solution. For the progressive waves which translate in space we have the equation 2 ∂2u 2∂ u = c ∂t2 ∂x2

(3.7.1)

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

156

dynamic

Dynamic Plasticity

with c = const. If we change the variables α = x − ct ,

β = x + ct

where α, β are characteristic variables, we have ∂u ∂u ∂u ∂u ∂u ∂u = + , = −c +c ∂x ∂α ∂β ∂t ∂α ∂β ∂2u ∂2u ∂2u ∂2u + = + 2 ,··· . ∂x2 ∂α2 ∂α∂β ∂β 2 If we introduce in the equation we receive ∂2u =0 ∂α∂β from where we get the solution u = f (x − ct) + g(x + ct) which is the d’Alembert solution. It gives the general solution with f and g to be determined from initial data. u = f (x − ct) are the direct waves, propagating towards the right. Let us introduce a mobile system of coordinates, for an observer which translates with the speed ct. In the new system of coordinates x ¯ = x − ct, t¯ = t we have u(¯ x, t¯) = f (¯ x) i.e., the observer sees the same stationary wave. The Cauchy problem for the equation (3.7.1) with initial data: ∂u u(x, 0) = h(x) and (x, 0) = k(x) (3.7.2) ∂t with h of class C2 (h and ﬁrst two derivatives are continuous) and k of class C1 along −∞ < x < ∞ and the solution u = f (x − ct) + g(x + ct)

(3.7.3)

2

with f and g arbitrary and of class C . For t = 0 we have f (x) + g(x) = h(x) . By derivation of (3.7.3) ∂u (x, 0) = −cf (x) + cg (x) = k(x) . ∂t Integrating (3.7.5): 1 x −f (x) + g(x) = k(ξ) dξ + g(x0 ) − f (x0 ) . c x0 From (3.7.4) and (3.7.6) we obtain 1 1 f (x) = h(x) − 2 2c 1 1 g(x) = h(x) + 2 2c

x

x0

x

x0

(3.7.4)

(3.7.5)

(3.7.6)

1 k(ξ) dξ − [g(x0 ) − f (x0 )] 2 1 k(ξ) dξ + [g(x0 ) − f (x0 )] . 2

(3.7.7)

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

dynamic

The Propagation of Longitudinal Stress Waves

157

t

x0 − ct0

x0

ct =

xP

xP ct = x+

x−

x−

+ ct 0

ct = x

0

− ct

0

t = x0 x+c

0

domain of influence of P

Q ( x0 , t 0 )

t0

x0 + ct0

x

P domain of dependence of Q ( x0 , t0 )

domain of determin acy of the segment x 0 − ct0 ≤ x ≤ x0 ≤ ct0 Fig. 3.7.1

The various domains existing.

We replace x by x − ct in the ﬁrst relation and x by x + ct in the second, and by adding: u(x, t) = f (x − ct) + g(x + ct) 1 x−ct 1 x+ct 1 h(x − ct) + h(x + ct) − k(ξ) dξ + k(ξ) dξ . = 2 c x0 c x0 The last two terms can be written in the form: 1 h(x − ct) + h(x + ct) + u(x, t) = 2 2c

x+ct

k(ξ) dξ .

(3.7.8)

x−ct

The ﬁrst term corresponds to the solution with initial zero velocities (k(0) = 0) and the last term to the solution with initial zero displacements (h(0) = 0). The various domains which are involved in various problems and haw are they called are shown in Fig. 3.7.1. The prescribed data in P are not enough for the determination of the solution. One can put the problem if the solution is unique? Let us assume that u1 (x, t) and u2 (x, t) are two distinct solutions which satisfy the initial data (3.7.2). It follows that u = u1 − u2 is also a solution of (3.7.1) with the initial values u(x, 0) = 0

and

∂u (x, 0) = 0 ∂t

corresponding to h = k = 0. It follows from (3.7.8) that u(x, t) = 0 for any x and t ≥ 0. Thus u1 = u2 and the solution is unique. We have to study the dependence of the solution on the initial data. From (3.7.8) it follows that the solution u(x0 , t0 ) at Q(x0 , t0 ) depends on the Cauchy data along x0 − ct0 ≤ x ≤ x0 + ct0 and t = 0.

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

158

dynamic

Dynamic Plasticity

Let us show the continuous dependence of the solution (3.7.8) on the Cauchy data. Let us assume two sets of Cauchy data: u1 (x, 0) = h1 (x) , u2 (x, 0) = h2 (x) ,

∂u1 (x, 0) = k1 (x) ∂t ∂u2 (x, 0) = k2 (x) ∂t

(3.7.9)

and let us assume that |h1 (x) − h2 (x)| < ε ,

|k1 (x) − k2 (x)| < δ

(3.7.10)

for −∞ < x < ∞ and ε > 0, δ > 0 arbitrary. From (3.7.8) we have: h1 (x − ct) − h2 (x − ct) h1 (x + ct) − h2 (x + ct) + 2 2 x+ct 1 + [k1 (ξ) − k2 (ξ)] dξ . 2c x−ct !b !b Taking the modulus and since | a f dξ| ≤ a |f | dξ we have u1 (x, t) − u2 (x, t) =

|u1 (x, t) − u2 (x, t)| ≤

|h1 (x − ct) − h2 (x − ct)| 2 1 |h1 (x + ct) − h2 (x + ct)| + + 2 2c

Using (3.7.10)2 1 2c

x+ct

|k1 (ξ) − k2 (ξ)| dξ ≤ x−ct

x+ct

|k1 (ξ) − k2 (ξ)| dξ . x−ct

1 δ{x + ct − (x − ct)} = δt 2c

and thus |u1 (x, t) − u2 (x, t)| ≤ ε + δt . For t ﬁxed if h1 and h2 as well as k1 and k2 , are only “slightly” distinct, i.e., if ε and δ are “small”, the solution u2 approaches u1 as close as desired. In the case of non homogeneous equation 2 ∂2u 2∂ u − c = f (x, t) (3.7.11) ∂t2 ∂x2 we try to ﬁnd a solution of the form u = u1 + u2 with u1 a solution of homogeneous equation

∂ 2 u1 ∂ 2 u1 − c2 =0 2 ∂t ∂x2 with initial data u1 (x, 0) = h(x), ∂u1 /∂t(x, 0) = k(x) and u2 a solution of the equation 2 ∂ 2 u2 2 ∂ u2 − c = f (x, t) ∂t2 ∂x2

(3.7.12)

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

The Propagation of Longitudinal Stress Waves

dynamic

159

C

dt =

dx/

dx/

dt =

c

t

−c

D t

0

x

A

B

x

c(t − t ) Fig. 3.7.2

Domain of integration.

with initial data u2 (x, 0) = 0 ,

∂u2 (x, 0) = 0 . ∂t

Integrate now (3.7.12) in the domain D: 2 2 ∂ u2 2 ∂ u2 dxdt = −c f (x, t) dxdt ∂t2 ∂x2 D D

(3.7.13)

(3.7.14)

and using the Green’s formula ∂Q ∂P − dxdy = − P dx + Qdy ∂y ∂x D ∂D the formula (3.7.14) becomes ∂u2 ∂u2 dx + c2 dt = f (x, t) dxdt . − ∂x ∂D ∂t D Since along BC we have dx = −cdt, along CA we have dx = −cdt, and along AB we have dt = 0, this integral becomes ∂u2 ∂u2 ∂u2 ∂u2 ∂u2 ∂u2 dt + dx − dt + dx − dx + c2 dt c c ∂t ∂x ∂t ∂x ∂t ∂x BC CA AB = f (x, t) dxdt . D

Since in the brackets there are total diﬀerentials, the third term is zero from (3.7.13), and the fourth is zero on AB, we obtain cdu2 − cdu2 = f (x, t) dxdt BC

CA

D

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

160

dynamic

Dynamic Plasticity

t

x−

ct =

co n

st.

ξ B x 0 + η , t0 + c

•

t0

A(x0 + ξ , t0 + η )

η

x+

C ( x0 − ξ , t0 − η )

ct =

co n

ξ

ξ

ξ D x0 − cη , t 0 − c

0

x

x0 Fig. 3.7.3

st.

Four arbitrary characteristic lines.

or by integration

cu2 (C) − cu2 (B) − cu2 (A) + cu2 (C) =

f (x, t) dxdt D

or since the second and third terms are zero according to (3.7.13), ¯ 1 t x+c(t−t) u2 (C) = u2 (x, t) = f (¯ x, t¯) d¯ xdt¯. 2c 0 x−c(t−t¯) Thus the general solution is: u(x, t) =

1 h(x − ct) + h(x + ct) + 2 2c

x+ct

k(ξ) dξ + x−ct

1 2c

t

x+c(t−t¯)

f (¯ x, t¯) d¯ xdt¯. 0

x−c(t−t¯)

This solution depends on the Cauchy data on AB, and on the values of f (x, t) in the internal points of the triangle D. Let us discuss now the boundary conditions and mixed boundary value problem. The mixed boundary value problem is composed from: boundary conditions for x=a

and t ≥ 0

x=b

and t ≥ 0

and the initial conditions for a ≤ x ≤ b, t = 0. Let us consider four arbitrary characteristic lines from x − ct = const. and x + ct = const. (Fig. 3.7.3). The coordinates of B are: x + ct = x0 + ξ + c(t0 + η) x − ct = x0 − ξ − c(t0 − η) .

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

The Propagation of Longitudinal Stress Waves

dynamic

161

t B A C

D

ct = x−

0

Domain where the solution of the Cauchy problem is known x

0 initial condition on x ≥ 0, t = 0 given Fig. 3.7.4

Solution in B is known if given on A, D and C.

From here we have by adding: xB = x0 + ηc, tB = t0 + ξ/c. The coordinates from D are from: x − ct = x0 + ξ − c(t0 + η) x + ct = x0 − ξ + c(t0 − η) . From here we again ﬁnd: xD = x0 − cη, tD = t0 − ξ/c. From the general solution u(x, t) = f (x − ct) + g(x + ct) we obtain u(A) = f (D) + g(B) , u(C) = f (B) + g(D) . From here by adding: u(A) + u(C) = u(D) + u(B) . Thus if u is prescribed in A, D and C it follows in B. Thus the solution in any B can be obtained if prescribed by Cauchy data along the line x − ct = 0 and known in C by boundary conditions. The solution is unique in D and the relation is also linear. Let us consider now the reﬂection from a ﬁxed end. We have to ﬁnd out how the solution is extended by reﬂection. We consider the initial conditions ∂u (x, 0) = k1 (x) , ∂t and the boundary condition x = 0, t ≥ 0 : u(x, t) = 0. The solution in D is x+ct 1 h(x − ct) + h(x + ct) + u(x, t) = k(s) ds . 2 2c x−ct x ≥ 0,

t = 0 : u(x, 0) = h1 (x) ,

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

162

dynamic

Dynamic Plasticity

t t

t

D1 D

0

x Fig. 3.7.5

x0 − ct

x0

x0 + ct

−ct

0

+ct

Various domains for reﬂection of waves.

Let us ﬁnd the solution in D1 . For x = 0 from u(x, t) = f (x − ct) + g(x + ct) and u(0, t) = 0 we get f (−ct) + g(ct) = 0 or f (−x) = −g(x) with x arbitrary argument. From the general expressions x 1 1 1 f (x) = h(x) − k(ξ) dξ − [g(x0 ) − f (x0 )] , 2 2c x0 2 x 1 1 1 k(ξ) dξ + [g(x0 ) − f (x0 )] , g(x) = h(x) + 2 2c x0 2 we put x0 = 0 (see Fig. 3.7.5), we have: x 1 1 1 k(ξ) dξ − [g(0) − f (0)] , f (x) = h(x) − 2 2c 0 2 x 1 1 1 g(x) = h(x) − k(ξ) dξ + [g(0) − f (0)] . 2 2c 0 2 We replace here x by −x, h by h1 , k by k1 and we have x 1 1 1 k1 (−ξ) dξ − [g(0) − f (0)] . f (−x) = h1 (−x) + 2 2c 0 2 From the condition f (−x) = −g(x) follows: x 1 1 1 − h1 (−x) + k1 (−ξ) dξ − [g(0) − f (0)] 2 2c 0 2 x 1 1 1 = − h1 (x) − k1 (ξ) dξ − [g(0) − f (0)] . 2 2c 0 2 This relation is satisﬁed for any x if h1 (−x) = −h1 (x)

and k1 (−x) = −k1 (x) .

Thus the problem of a ﬁxed end u(0, t) = 0 for x = 0 in a mixed problem, is equivalent with the Cauchy problem for the whole line −∞ < x < +∞ with the odd functions h1 and k1 . . . . Therefore & −∞ < x < +∞ ∂u (x, 0) = k(x) : u(x, 0) = h(x) , ∂t t=0

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

dynamic

The Propagation of Longitudinal Stress Waves

t

163

x=

ct

Q

ct

t

x=

P

x

0 Fig. 3.7.6

x

0

The two domains where the above formula applies.

with h(x) =

h1 (x) −h1 (x)

for x ≥ 0 for x < 0 ,

k1 (x) =

k1 (x) −k1 (x)

for x ≥ 0 for x < 0 .

We can prove also the converse: if the initial data along the line −∞ < x < +∞ and t = 0 are odd with respect to the origin h1 (x) = −h1 (x) ,

k1 (−x) = −k1 (x) ,

then the solution of the wave equation is zero at that point (ﬁxed point). For the proof we start from the solution 1 +ct h1 (−ct) + h1 (ct) + k(s) ds = 0 . u(0, t) = 2 2c −ct Therefore the solution of the mixed problem in x ≥ 0, t ≥ 0 is x+ct h(x − ct) + h(x + ct) 1 + k(s) ds 2 2c x−ct u(x, t) = x+ct −h(ct − x) + h(x + ct) 1 + k(s) ds 2 2c −x+ct

for x > ct ,

for x < ct .

The last relation is obtained from the ﬁrst by replacing h(x − ct) by −h(ct − x), and k(x − ct) by −k(ct − k). The two relations are applied in the regions shown in Fig. 3.7.6. The two formulae given above are applied in the two regions shown in this ﬁgure. Let us study now the stress at a ﬁxed end of an elastic bar. On the direct waves u1 = f1 (x − ct) the stress is σ1 = E

∂u1 ∂u1 = −ρc , ∂x ∂t

while on the inverse waves u2 = f2 (x + ct) the stress is σ2 = E

∂u2 ∂u2 = ρc . ∂x ∂t

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

164

dynamic

Dynamic Plasticity

The total stress is

∂u2 ∂u1 + = ρc2 [f1 (x − ct) + f2 (x + ct)] , σ = σ1 + σ2 = ρc − ∂t ∂t while the total displacement is u = f1 (x − ct) + f2 (x + ct) from where for a ﬁxed x = 0 we have f1 (−ct) + f2 (ct) = 0, or f1 (−z) = −f2 (z). Thus at a ﬁxed end of the bar σ|x=0 = (σ1 + σ2 )|x=0 = 2f2 E . We arrive at an important conclusion: the stress is doubled due to reﬂection. If the incident wave reaching the ﬁxed end is still elastic, after reﬂection it may be nearly 2σY . So that an elastic wave at reﬂection may become a plastic wave. Now let us look at the conditions which exist at the free end. Let us consider the equation 2 ∂2u 2∂ u = c ∂t2 ∂x2

with the initial conditions & t=0 0 ≤ x < +∞

: u(x, 0) = h1 (x) ,

∂u (x, 0) = k1 (x) ∂t

and the boundary conditions at the free end x = 0: & t>0 ∂u (0, t) = 0 . : ∂x x=0

(3.7.15)

(3.7.16)

Let us show that the mixed problem with a free end ∂u/∂x(0, t) = 0 is equivalent with the Cauchy problem on the entire x-axis with initial conditions for displacement and velocities even. For the proof from u(x, t) = f (x − ct) + g(x + ct) follows ∂u/∂x(0, t) = f (−ct) + g (ct) = 0, i.e., f (−x) = −g (x) . From

x 1 1 1 f (−x) = h1 (−x) + k1 (−s) ds − [g(0) − f (0)] , 2 2c 0 2 x 1 1 1 g(x) = h1 (x) + k1 (s) ds + [g(0) − f (0)] , 2 2c 0 2

follows f (−x) = g (x) =

1 1 h (−x) − k1 (−x) , 2 1 2c 1 1 h1 (x) + k1 (x) , 2 2c

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

dynamic

The Propagation of Longitudinal Stress Waves

165

from where 1 1 h1 (−x) − k1 (−x) = −h1 (−x) − k1 (x) c c i.e., h1 (−x) = −h1 (x) ,

k1 (−x) = k1 (x) .

Since the derivative of an even function h1 (x) = h1 (−x) is an odd function h1 (x) = −h1 (−x) we have h1 (x) = h1 (−x) . Therefore the mixed problem for a free end is equivalent with the Cauchy problem on the entire axis with the conditions h1 (x) for x > 0 , h(x) = & u(x, 0) = h(x) h1 (−x) for x < 0 , −∞ < x < +∞ with ∂u t=0 (x, 0) = k(x) k1 (x) for x > 0 , ∂t k(x) = k (−x) for x < 0 . 1 Let us prove the converse. If the Cauchy conditions on −∞ < x < +∞ are even h1 (x) = h1 (−x), k1 (x) = k1 (−x) then ∂u/∂x(0, t) = 0. From the solution 1 x+ct h(x − ct) + h(x + ct) + u(x, t) = k(s) ds 2 2c x−ct follows for x = 0: ∂u h (−ct) + h (ct) 1 (0, t) = + [k1 (ct) − k1 (−ct)] = 0 ∂x 2 2c since h1 (−ct) = h1 (ct). The solution for the mixed problem for x > 0, t > 0 is: u(x, t) h(x − ct) + h(x + ct) 1 x+ct + k(s) ds 2 2c x−ct = x+ct ct−x 1 h(ct − x) + h(x + ct) + k(s) ds + k(s) ds 2 2c 0 0

for x > ct ,

for x < ct ,

which satisﬁes the initial conditions (3.7.15) and the boundary conditions (3.7.16). Let us examine the displacement at the free end of an elastic bar. We have on the direct waves u1 = f1 (x − ct) and the stress ∂u1 ∂u1 = −ρc ∂x ∂t and on the inverse waves u2 = f2 (x + ct) with the stress σ1 = E

σ2 = E

∂u2 ∂u2 = ρc . ∂x ∂t

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

166

Dynamic Plasticity

The total stress is

∂u1 ∂u2 + = ρc2 [f1 (x − ct) + f2 (x + ct)] σ = σ1 + σ2 = ρc − ∂t ∂t

and the total displacement is u = f1 (x − ct) + f2 (x + ct). If the end x = 0 is free, we have σ = 0 or f1 (−ct) + f2 (ct) = 0. That means f1 (−ct) = f2 (ct) . The total displacement is u|x=0 = (u1 + u2 )x=0 = 2f2 (ct) . That means that at a free end the displacement is doubled. Because for the stress we have σ1 = −σ2 a compressive wave is reﬂected as a tensile wave at the free end (or the reverse). If the mechanical proprieties are distinct in tension and in compression, that may make a diﬀerence. Bibliography Bell J. F., 1968, The Physics of Large Deformation of Crystalline Solids, Springer-Verlag, Berlin. Bell J. F., 1973, The experimental foundations of solid mechanics, in Handbook der Physic, Springer-Verlag, Berlin. Bodner S. R. and Clifton R. J., 1967, Experimental investigation of elastic-plastic pulse propagation in aluminum rods, J. Appl. Mech. Trans. ASME 34, 1, 91–99. Chen S. R., Maudlin P. J. and Gray III G. T., 1999, Constitutive behavior of model FCC, BCC, and HCP metals: experiments, modeling and validation, in Constitutive and Damage Modeling of Inelastic Deformation and Phase Transformation, Khan A. S. (ed.), NEAT Press, 623–626. Chou P. C. and Hopkins A. K., (eds.) 1973, Dynamic response of materials to intense impulsive loading, Air Force Materials Laboratory, 555 pp. Clifton R. J. and Bodner S. R., 1966, An analysis of longitudinal elastic-plastic pulse propagation, J. Appl. Mech. Trans. ASME 33, 2, 248–255. Cristescu N., 1957, On propagation of waves in rubber, Prikl. Mat. Meh. 21, 795 800 (in Russian). Cristescu N., 1967, Dynamic Plasticity, John Wiley & Sons, Inc., New York. Cristescu N., Dynamic plasticity, Appl. Mech. Rev. 21, 7, 659–668. Cristescu N. and Bell J. F., 1970, On unloading in the symmetrical impact of two aluminum bars, In: Inelastic Behavior of Solids, McGraw Hill Book Co., 1970, 397–419. Cristescu N., 1970, The unloading in symmetric longitudinal impact of two elastic-plastic bars, Int. J. Mech. Sci. 12, 6, 723–738. De Juhasz K. J., 1949a, Graphical analysis of impact of bars stresses above the elastic range. Part. I, J. Franklin Inst. 248, 15–48. De Juhasz K. J., 1949b, Graphical analysis of impact of bars stressed above the elastic range. Part. II, J. Franklin Inst. 248, 113–142.

dynamic

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

The Propagation of Longitudinal Stress Waves

dynamic

167

Francis P. H., 1966, Wave propagation in thin rods with quiescent temperature gradients, J. Appl. Mech. 33, 3, 702–704. Huﬃngton N. J., (ed.) 1965, Behaviour of materials under dynamic loading, Behavior of Materials under Dynamic Loading at the Winter Annual Meeting of the ASME, Chicago, Illinois, 1965, 187 pp. Jones S. E., Gillis P. P. and Foster J. C. Jr., 1987, On the equation of motion of the undeformed section of a Taylor Impact specimen, J. Appl. Phys. 61, 2, 499–502. Kanel G. I., 1999, Dynamic strength of materials, Fatigue Fract. Engng. Mater. Struct. 22, 1011–1019. K´ arm` an Th. and Duwez P., 1950, The propagation of plastic deformation in solids, J. Appl. Phys. 27, Ser E, 107–110. Kawata K. and Shioiri J., (eds.) 1978, High Velocity Deformation of Solids Symposium Tokyo/Japan, 1977, Springer Verlag, 452 pp. Kenning M. J., 1974, Uniqueness of uniaxial elastic-plastic interface motions, J. Mech. Phis. Solids 22, 437–456. Kinslow R., (ed.) 1970, High-Velocity Impact Phenomena, Academic Press, 579 pp. Kolsky H., 1953, Stress Waves in Solids, Clarendon Press, Oxford. Kolsky H., 1969, Production of tensile shock waves in stretched natural rubber, Nature 224, 5226, 1301. Lagoudas D. C., Ravi-Chandar K., Sarh K. and Popov P., 2003, Dynamic loading of polycrystalline shape memory alloy rods, Mech. Materials 35, 689–716. Lee L. H. N. and Chi-Mou Ni, 1973, A minimum principle in dynamics of elastic plastic continua at ﬁnite deformation, Archives of Mechanics 25, 3, 457–468. Lee L. H. N., 1974, Dynamic plasticity, Nuclear Eng. and Design 27, 386–397. Lenski V. S., 1949a, On the elastic-plastic shock of a bar on a rigid wall, Prikl. Mat. Meh. 12, 165–170 (in Russian). Lush P. A., 1991, Comparison between analytical and numerical calculations of liquid impact on elastic-plastic solid, J. Mech. Phys. Solids 39, 1, 145–155. Magness L. S. Jr., 1994, High strain rate deformation behaviors of kinetic energy penetrator materials during ballistic impact, Mech. of Materials 17, 147–154. Miklowitz J., (ed.) 1969, Wave propagation in solids, ASME Winter Annual Meeting, Los Alamos, California, 1969, 183 pp. Mines R. A. W., 2004, A one-dimensional stress wave analysis of a lightweight composite armour, Comp. Structures 64, 55–62. Misra J. C., Kar S. B. and Samanta S. C., 1987, Distribution of stresses in a heated nonhomogeneous rod, S. M. Archives 12/2, 97–111. Nemat-Nasser S., Li Y. F. and Isaacs J. B., 1994, Experimental/computational evaluation of ﬂow stress at high strain rates with application to adiabatic shear banding, Mec. Mater. 17, 111–134. Nonaka T., Clifton R. J. and Okazaki T., 1996, Longitudinal elastic waves in columns due to earthquake motion, Int. J. Impact. Engng. 18, 7–8, 889–898. Nowacki W. K., 1978, Problems of Wave Propagation in the Theory of Plasticity, Mir, Moscow. Ponomarev S. D., Biderman V. L., Likharev K. K., Makushin V. M., Malinin N. N. and Feodos’ev V. I., 1959, Resistence calculus in construction of machines, Mashigiz, Moscow, Tom III, 553–580 (in Russian). Raniecki B., 1971, The inﬂuence of dynamical thermal expansion on the propagation of plane elastic-plastic stress waves, Quart. Appl. Math. 29, 2, 277–290. Raiser G. F., Wise J. L., Clifton R. J., Grady D. E. and Cox D. E., 1994, Plate impact response of ceramics and glasses, J. Appl. Phys. 75, 8, 3862–3869.

January 12, 2007

168

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Dynamic Plasticity

Rakhmatulin H. A. and Demianov Yu. A., 1961, Strength under Impulsive Momentary Loads, Moscow (in Russian). Rakhmatulin H. A., 1945, On the propagation of unloading waves, Prikl. Mat. Meh. 9, 1, 91–100 (in Russian). Shim V. P. W., Yuan J. and Lee S.-H., 2001, A technique for rapid two-stage dynamic tensile loading of polymers, Experimental Mechanics 41, 1, 122–127. Santosham T. V. and Ramsey H., 1970, Small plastic strain wave propagation in prestressed soft copper rods, Int. J. Mech. Sci. 12, 5, 447–457. Shapiro G. S., 1946, Longitudinal vibration of bars, Prikl. Mat. Meh. 10, 597–616 (in Russian). Swegle J. W. and Ting T. C. T., 1982, Plastic wave propagation in a circular cylindrical rod, J. Appl. Mech. Trans. ASME 49, 253–256. Taylor G. I., 1946, The testing of materials at high rates of loading, J. Inst. Civil Engrs. 8, 486–519. Taylor G. I., 1958a, The use of ﬂat-ended projectiles for determining dynamic yield stress, Proc. Roy. Soc. Ser. A 194, 289–289. Taylor G. I., 1958b, The formation and enlargement of circular hole in a thin, plastic sheet, Quart. J. Mech. Appl. Math. 1, 103–124. Teng X., Wierzbicki T., Hiermaier S. and Rohr I., 2005, Numerical prediction of fracture in the Taylor test, Int. J. Solids Structures 42, 2929–2948. Tjavaras A. A. and Triantafyllou M. S., 1996, Shock waves in curved synthetic cables, J. Enge. Mech. 122, 4, 308–315. Varley E., (ed.) 1976, Propagation of shock waves in solids, The Applied Mechanics Conference, Salt Lake City, Utah, 1976.

dynamic

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Chapter 4

Rate Inﬂuence

4.1

Experimental Results

The rate inﬂuence seems to be the central problem of dynamic plasticity. It has been known for many years that during dynamic testing, solids behave in a more or less diﬀerent way than in static tests. Many theoretical and experimental papers have been devoted to this problem. Let us consider the problem shortly. We discuss the main conclusion resulting from the experiments that have been performed. Details concerning the experimental techniques will not be given here. We shall see however, that in some experimental papers the wave propagation phenomena were disregarded, although the rate of loading was high. This can be done only if the specimen is very short. The old tests are discussed in detail by Cristescu [1967], Cambell [1970], Cristescu and Suliciu [1982] and Goldsmith [2001], and will not be mentioned here any more. Only a few tests will be revealed. Strain rates ranging between 10−5 sec−1 and 10−3 sec−1 are termed static tests. Tests in which the rates of strain range between 10−2 sec−2 and 102 sec−1 can be termed intermediate tests (these are the rates of strains usually met in various metal working processes, for instance), while the tests producing rates of strains above 102 sec−1 (and certainly of the order of magnitude of 103 sec−1 and higher) can be called dynamic in the sense that as a rule in such tests the inertia forces, the propagation of waves etc. must be considered in the analyses. Sometimes the inertia forces are considered in the analysis when rates of strain of approximately 1 sec−1 are reached. A review is presented by Klepaczko [1998] on recent progress in shear testing of materials at high and very high (up to 106 s−1 ) strain rates. The classiﬁcation of various testing machines according to the kind of test performed, i.e., tension, compression, bending, combined loading etc., is not important for the approach followed here. Kinematic and dynamic jump conditions are also given. A theory of rate-type materials for one-dimensional case is due to Suliciu [1974]. He introduces diﬀerent classes of regulated functions and introduces the concept of wave propagation for the frame of regulated functions. The simplest diagnostic test is the uniaxial compression or tension test of a cylindrical specimen. For the description of the technical aspects of this kind of 169

dynamic

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

170

Dynamic Plasticity

experiments see for instance Ponomarev et al. [1956], Ilyushin and Lenskii [1959], Dally and Riley [1965], Bell [1973], Gupta [1976], etc. Basically there are two kinds of testing machines. With the so called “hard” machines the variation in time of the length of the specimen can be prescribed, while the response of the material is known by registering the force necessary to produce this deformation. Other kind of machines called “soft” can prescribe the stress applied to the specimen (by a weight attached directly or not to the specimen), while the response of the material is observed by measuring the elongation of the specimen. Both kinds of testing machines provide some stress–strain diagrams. The experiments made by Kolsky [1949] with copper and lead showed that the dynamic elastic modulus does not diﬀer sensibly from the static one (Fig. 4.1.1),

Fig. 4.1.1

Static and dynamic stress–strain curves for copper.

Fig. 4.1.2

Stress–strain curves for pure aluminum.

dynamic

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Rate Inﬂuence

Fig. 4.1.3

dynamic

171

Stress–strain curves for schist.

but that the whole dynamic stress–strain curve is higher that the static curve. The strain increases even when the stress is falling, and it follows that the dynamic constitutive equation for copper is time-dependent. The static stress–strain curve does not seem to be rate dependent. In Fig. 4.1.2 are given the stress–strain curves for pure aluminum as obtained with various rates of strains by Hauser et al. [1960] (reproduced here from Thomsen et al. [1968]). If the rates of strains are high (over 102 sec−1 , say), the inertia forces cannot be neglected and the wave propagation phenomena must be considered in the analysis of the experiment. For rocks the inﬂuence of the strain rate on both loading and unloading is ˙ = shown in Fig. 4.1.3 for two loading rates |σ| ˙ = 300 kgf cm−2 min−1 and |σ| −2 −1 1.33 kgf cm min both in loading and unloading. Thus the stress–strain curve is non-linear during loading and unloading. One can see also the important hysteresis loops during unloading and the fact that the whole curve is inﬂuenced by the loading rate. In Fig. 4.1.4 we give the variation in time of the strain and of the surface angle for copper (Bell [1968]) for an impact velocity V0 = 1200 cm/sec, measured at 5.1 cm from the impacted end. For high impact velocity the strain is higher, and that can not be explained by the classical theory. Another parameter which can be measured at the impacted end of the bar is the stress. Generally the stress can be measured with the help of piezoelectric crystal wafers placed at the impacted face. Filbey [1961] has used an X-cut quartz crystal wafer 2.12 cm in diameter and 0.25 mm thick. A typical result for two

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

172

Dynamic Plasticity

Fig. 4.1.4

Variation of strain and surface angle in time for copper.

Fig. 4.1.5

Peak stress at impacted end.

dynamic

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

Rate Inﬂuence

dynamic

173

experiments with symmetric impact is given in Fig. 4.1.5 (Filbey [1961]) who used the impact velocity V0 = 7100 cm/sec. The decrease is in microseconds to become nearly constant for a relatively long period of time (Fig. 4.1.6) (Filbey [1961]). The medium value of the peak stress is 71043 N cm−2 . The stress “plateau” which is reached after several microseconds is at the level 13160 N cm−2 . The decrease of the stress which follows afterwards is due to the unloading. Another experiment which played an important role in the development of the theory was the following one carried out by Bell [1951]. A medium carbon steel

Fig. 4.1.6

Fig. 4.1.7

Stress plateau.

General strain rate eﬀects on mortar strength.

January 12, 2007

174

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Dynamic Plasticity

long bar (about 183 cm in length and consisting of portions 0.64 or 0.35 cm in diameter) was subjected to a static extension. A dynamic loading was superposed. The experimental results obtained by Bell have shown that the ﬁrst waves which propagate in the bar are propagating with the bar velocity c0 . Similar tests were done afterwards by several authors. Similar dynamic loading tests followed by a dynamic reloading have been done by Alter and Curtis [1956] on lead specimens and afterwards by Bell and Stein [1962] on aluminum. The ﬁrst waves were propagating with the bar velocity. Similar tests in which the hitter was a composed bar made from two distinct materials (possessing distinct densities) have been carried out by other authors. The general trend in the unconﬁned tests of cementations material data is a very slight increase in strength from a low strain rate of 1.0 × 10−7 /s up to a strain rate of approximately 1.0/s for tensile strength properties, 10/s for shear strength properties and 100/s for compressive strength properties. Above these

Fig. 4.1.8 Typical stress–strain curves for polycarbonate at 23◦ C for strain rates of (a) 0.000368 s−1 , (b) 8.43 s−1 , and 6000 s−1 ; and measured 8% ﬂow stress as a function of logarithmic strain rate for polycarbonate at 23◦ C (specimen thickness: 4.4 mm, • 1.5 mm).

dynamic

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

Rate Inﬂuence

Fig. 4.1.9

Tree axial curves for granite (Maranini and Yamaguchi [2001]).

dynamic

175

January 12, 2007

176

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Dynamic Plasticity

critical strain rates a rather abrupt increase in strength occurs with a slope of (log10 strength/log10 strain rate) of approximately one-third. Representative strain rate eﬀects on unconﬁned strength properties reported by Schmidt and Ross [1999] are given in Fig. 4.1.7. See also the paper of Bertholf and Karnes [1975] on the same subject. Very high strain-rate response of a NiTi shape-memory alloy vas studied by Nemat-Nasser et al. [2005]. They adopt a split Hopkinson bar test to get such high strain rates of about 10,000/s. The result obtained is an increase of the true stress at high strain rates. The assumption of uniform stress and strain distribution within a split Hopkinson pressure bar specimen is assumed incorrect at high impact velocities (Dioh et al. [1995]), and that the propagation of plastic wave fronts within the split-Hopkinson-pressure-bar are responsible for the dependence of ﬂow stress measurements on specimen thickness at high strain rates. The same topic is used in Dioh et al. [1993]; they make tests studying the thickness of the specimens in the split Hopkinson pressure bar experiments. Various thermoplastics have been studied. For instance in Fig. 4.1.8 is showing some of the results. The “high” strain rates is completely above the other. Also in the lower ﬁgure one can see that the thick specimens are above the small one, at least for higher strain rates. Some other curves for granite measured in three axial stresses are shown in Fig. 4.1.9, from Maranini and Yamaguchi [2001]. The small original plateau is creep in a few minutes done before an unloading is performed to measure the elastic parameters (see Ch. 2). But changing the conﬁning pressure changes the whole stress–strain curve. Also, the volumetric stress–strain curves are shoving ﬁrst compression and afterwards dilatation. The compression is trying to disappear as the conﬁning pressure is increased signiﬁcantly, but not the creep by dilatancy. Similar results are mentioned by very many authors.

4.2

The Constitutive Equation

Many authors have proposed various constitutive equations in order to describe the mechanical properties of materials that exhibit the rate eﬀect. All have started from the assumption, suggested by experimental evidence, that, even while the stress is being continuously increased, there is no longer a one-to-one correspondence between stress and strain as prescribed by a ﬁnite stress–strain relation. The ﬁrst was Ludwik [1909] and then Prandtl [1928] who observed that for a ﬁxed plastic strain the corresponding stress is higher, the greater the average rate of strain at which the experiment is performed. Ludwik postulated the following logarithmic equation σ = σ1 + σ0 ln

ε˙P ε˙P 0

.

dynamic

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

Rate Inﬂuence

Fig. 4.2.1

dynamic

177

Inﬂuence of the rate of strain on the stress–strain curve.

Where σ1 , σ0 and ε˙P 0 are material constants. Here σ1 is the yield stress correspondP ing to the strain rate ε˙P 0 (Fig. 4.2.1). If the strain rate is greater than ε˙0 , the stress corresponding to a certain plastic strain is greater, σ0 is the measure of this increment. The reference conﬁguration for such constitutive equation is the actual one, since the strain is not present. Many simple models describing the rate eﬀect were inspired by this formula. If the elastic part of the strain can be neglected with respect to the plastic one, then the simplest of these models can be written as σ−σ Y if σ > σY , 3η ε˙ = 0 if 0 ≤ σ ≤ σY , where η is the viscosity coeﬃcient. This model can be called Bingham model (Bingham [1922]). In it ε˙ depends on the overstress. This model was used for various pastes, dough, vaseline, paints, mud etc., but also for various solid bodies as metals, rocks etc. The coeﬃcient η can be found experimentally in the following way. From here we obtain 3η =

σ2 − σ1 . ε˙2 − ε˙1

Generally, for most solid bodies η is decreasing with increasing ε, ˙ and therefore it is only within certain ranges of variation that η can be considered to be constant. If the material is work-hardening, and if the conventional quasi-static relation is σ = f (ε), then Malvern [1951a, 1951b] proposed the use of the expression: σ = f (ε) + a ln(1 + bε˙P ) .

January 12, 2007

10:41

178

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

dynamic

Dynamic Plasticity

Here a and b are material constants. Solving this equation with respect to the rate of strain, we can write this relation as: 1 σ − f (ε) exp −1 . (4.2.1) ε˙P = b a The reference conﬁguration is now the initial one. This equation suggest a generalization in the sense that the plastic rate of strain must be a function of the overstress σ − f (ε), that is, of the diﬀerence between the dynamic and the actual static plastic strain. Thus E ε˙P = F (σ − f (ε)) . We can write now

σ − f (ε) 3η ε˙ = 0

(4.2.2)

if σ > f (ε) , if 0 < σ ≤ f (ε) ,

where σ = f (ε) is the work-hardening condition. To give some values for η from creep curves of rock-salt (see Baroncea et al. [1977]) η is of the order 1015 Nm−2 sec (Poise). For schist it is 1012 Poise while for other rocks it may be higher (1017 – 1018 Poise for argillaceous schist, see Vyalov [1978]). For ice from 1010 to 1015 Poise. For quasistatic deformations (ε˙ ≈ 1 sec−1 ) for mild steel (Cristescu [1977]) η is of the order of magnitude of 107 Nm−2 sec, but for faster deformation (ε˙ ≈ 100 sec−1 ) it is of the order 106 Nm−2 sec. For even very high rate of strains (ε˙ > 103 sec−1 ) Cambell [1973] gives for various metals values of the order 103 Poise. The values given above are only illustrative. Since in most cases the elastic part of the strain is connected with the stress by the Hooke’s law EεE = σ , the full constitutive equation can be written in the form E ε˙ = σ˙ + F (σ − f (ε)) . With F (z) satisfying the properties F (z) > 0 if z > 0 , F (z) = 0 if z ≤ 0 . This property is related to the loading/unloading criteria. More generally, the plastic rate of strain can be considered a function of the stress and strain E ε˙P = g(σ, ε) , and it yields the constitutive equation E ε˙ = σ˙ + g(σ, ε) . This form of the constitutive equation has been used by Malvern [1951a, 1951b].

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Rate Inﬂuence

dynamic

179

Various form of such constitutive equation was used by very many authors. Sokolovski [1948a, 1948b] used it for perfectly plastic materials with g(σ, ε) = kF (|σ| − σY ) , where σY is the static yield stress. Ting and Symonds [1964] have used the expression q σ g(σ) = D −1 σY with D and q material constants, speciﬁc for the material considered. Gilman [1960] suggested g(σ) = ε˙0 exp(−A/σ) , where ε˙0 and A are material constants. Some generalizations are due to Perzina [1963] α N ) σ g(σ) = Aα exp −1 −1 , σY α=1 g(σ) =

N ) α=1

Bα

σ −1 σy

α ,

etc.

All the functions and constants which occur in various expressions of the function g are, sometimes, time and temperature dependent. One can compute the rate of strain locally, the averaging is not possible. The elastic constants are independent on the rate of strain. The reference conﬁguration is always the actual one. The basic idea of the constitutive equations given above is that the plastic rate of strain is a function only of the dynamic overstress. This leads to the conclusion that in the plastic range the stress–strain curves for various constant rates of plastic straining are parallel curves. As will be shown later on (see B´eda [1962a]) these curves are not always parallel. Thus, instead of (4.2.3) one must look for a quasi-linear constitutive equation of the form ∂ε ∂σ = ϕ(σ, ε) + ψ(σ, ε) (4.2.3) ∂t ∂t for both plastics (Cristescu [1964]), and for metals (Cristescu [1963, 1966]). Variants have been used by many authors. Suliciu [1966] have shown when the constitutive equation (4.2.3) can be written in the form σ = H(ε, t) . In (4.2.3) ϕ(σ, ε) which can also possibly depend on time, is the measure of the instantaneous response of the material to an increase of stress, while ψ(σ, ε) which can also possibly depend explicitly on time, will be the measure of the non-instantaneous response of the material. It will be assumed that ϕ > 0.

January 12, 2007

180

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

dynamic

Dynamic Plasticity

Of course, ϕ and ψ may also comprise various characteristic constants of the material (yield stress, viscosity coeﬃcient, etc.) which are to a great extent temperature dependent. In order to solve the problem of propagation of longitudinal waves in thin bars, a solution must be obtained for the following ﬁrst order quasi-linear system, containing three unknown functions σ, v and ε ∂ε ∂σ = ϕ(σ, ε) + ψ(σ, ε) , ∂t ∂t ∂v 1 ∂σ = , ∂t ρ ∂ε

(4.2.4)

∂v ∂ε = . ∂x ∂t The second equation is the equation of motion and the third one the compatibility equation; v is the particle velocity, and ρ is the constant density. The system (4.2.4) possesses three families of characteristic curves dx/dt = ±c(σ, ε) = ± ϕ(σ, ε)/ρ , (4.2.5) and dx = 0 .

(4.2.6)

Along the curves (4.2.5) the diﬀerential relations dσ = ±ρc(σ, ε) dv + ψ(σ, ε) dt

(4.2.7)

are satisﬁed while along the lines (4.2.6) are satisﬁed the relations dσ = ϕ(σ, ε) dε + ψ(σ, ε) dt .

(4.2.8)

Thus the system (4.2.4) is totally hyperbolic. Instead of integrating the system (4.2.4) it is possibly to integrate the equivalent diﬀerential relations (4.2.7) and (4.2.8) along the characteristic curves (4.2.5) and (4.2.6) respectively. The upper and lower signs correspond to each other. In the problem considered a perturbation produced at the end of the bar will propagate along the bar by waves whose velocity is c(σ, ε). There will be some stationary discontinuities [Eq. (4.2.6)]. In order to analyze such phenomena in detail, the dynamic and kinematics compatibility conditions must be taken into account. If [F ] is used to denote the jump of a certain function F across a wave front the compatibility conditions are ∂ε ∂σ ∂σ ∂σ =ϕ , dx + dt = 0 , ∂t ∂t ∂x ∂t 1 ∂σ ∂v ∂ε ∂ε (4.2.9) = , dx + dt = 0 , ∂t ρ ∂x ∂x ∂t ∂v ∂ε ∂v ∂v = , dx + dt = 0 . ∂x ∂t ∂x ∂t

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

Rate Inﬂuence

dynamic

181

The left three relations are obtained from Eqs. (4.2.4). The remaining three relations express the condition that the interior diﬀerentials dσ, dε and dv are continuous across a wave front. From Eq. (4.2.9) it follows that across any line (4.2.5), the derivatives of σ, ε and v are discontinuous while across a line (4.2.6) all the derivatives in the system (4.2.4) are continuous except the derivatives ∂ε/∂x which may be discontinuous. It should be noted that the function ϕ(σ, ε), corresponding to the instantaneous response of the material, is the only function involved in the expressions for the velocity of propagation and the dynamic compatibility conditions. The function ψ(σ, ε) describing the non-instantaneous response or time eﬀects is only involved in the diﬀerential relations (4.2.6) and (4.2.7). Depending on the explicit expression of the function ϕ(σ, ε), the velocity c(σ, ε) can increase or decrease when the stress is varying. For the integration method, we assume the bar to be of length l and at time t = 0 the ends of the bar are at x = 0 and x = l. The boundary conditions must be formulated as follows: at x = 0

and t > 0 ,

we know either v(0, t) or σ(0, t) .

(4.2.10)

and t > 0 ,

we know either v(l, t) or σ(l, t) .

(4.2.11)

Similarly: at x = l

The initial conditions are: at t = 0 and 0 ≤ x ≤ l

we know v(x, 0), σ(x, 0) and ε(x, 0) .

(4.2.12)

If the bar is initially at rest or moving rigidly then the functions prescribed by the conditions (4.2.12) are known along the characteristic line of positive slope passing through x = 0 and along the characteristic line of negative slope passing through x = l, i.e., along the ﬁrst wave fronts which propagate in the bar. Otherwise one must ﬁrst solve a Cauchy initial value problem, and then pass to the Goursat problem in the corners. If the striking body moves with respect to the material points of the bar, then a mixed boundary value problem must be solved in a domain with a ﬂoating boundary. That was the case with the initial tests done in dynamic plasticity. In this case the impacting body must move along the bar with a velocity smaller than the velocity of the waves. 4.3

Instantaneous Plastic Response

In the previous section it was assumed that during the entire process of elasticviscoplastic deformation a single constitutive equation written in quasi-linear diﬀerential form could be used. This procedure can generally be used for plastics, certain soils or rocks, rubbers, certain metals, etc. However, in some problems for

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

182

Dynamic Plasticity

Fig. 4.3.1

Stress–strain relationship for ψ = 0.

some materials, especially for the majority of metals, the total strain is always composed of two components: the elastic reversible component and the plastic irreversible one (Fig. 4.3.1), with the total strain bigger than 0.2% say: (4.3.1) ε = εE + εP E where ε = σ/E. Both components increase during the loading of a work-hardening material, but each of them corresponds to diﬀerent physical phenomenon and is therefore related to the stress by diﬀerent constitutive equations, though of course these two phenomena are very tightly interconnected. It should also be noted that the plastic part of the strain is in fact a visco-plastic component. Thus, there is no longer any question of a one-to-one correspondence between stress and strain, even in the loading process. The stress–strain relation is certainly not unique, since it depends on the loading rate. Thus, in this case the plastic part of the strain has a more general meaning than in classic inviscid plasticity theory. The exact deﬁnition, of the elastic component of the strain, can only be given when unloading is deﬁned. Let us now examine the constitutive equation for elastic-plastic work-hardening materials (Cristescu [1963]). If, at a point A in the plastic region (Fig. 4.3.1) the stress is increased by an amount ∆σ, this impulse will propagate in the bar and produce an increase ∆εE of the elastic part of the strain and an increase ∆εP of the plastic part of the strain. The former will be related to the stress increment by Hooke’s law, which will be written in a diﬀerential form

dynamic

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

dynamic

Rate Inﬂuence

183

∂σ/∂t = E(∂εE /∂t) .

(4.3.2)

The plastic component of the strain increment is generally related to the stress increment by a quasi-linear diﬀerential relation of the form ∂εP ∂σ = ϕ(σ, ε) + ψ(σ, ε) , (4.3.3) ∂t ∂t where the functions ϕ and ψ may depend on some other constants describing the mechanical properties of the material (yield limit, viscosity coeﬃcient, workhardening modulus, etc.). We assume that ϕ > 0. If the material is in elastic state, only elastic waves will propagate with the velocity (4.3.4) cE = E/ρ . If the material is plastic/rigid only constitutive equation (4.3.3) is added to the equation of motion. In this case, only pure plastic waves will propagate, the velocity of their fronts being (4.3.5) cP = ϕ(σ, ε)/ρ . If however, the material is elastic-plastic, the following system of equations will govern the motion ∂σ ∂εE −E = 0, ∂t ∂t ∂εP ∂σ − ϕ(σ, ε) = ψ(σ, ε) , ∂t ∂t

(4.3.6)

∂v ∂εE ∂εP − − = 0, ∂x ∂t ∂t ∂v ∂σ − = 0. ∂t ∂x The characteristic curves of the system are dx/dt = ±c(σ, ε) = ± ϕE/ρ(ϕ + E) , ρ

(4.3.7)

and dx = 0

(twice) .

(4.3.8)

Along the characteristics (4.3.7) the diﬀerential relations dσ = ±ρc{±(ψ/ϕ)} cdt + dv

(4.3.9)

are satisﬁed, while along the lines (4.3.8) are satisﬁed the relations dσ = EdεE , dσ = ϕ(σ, ε) dεP + ψ(σ, ε) dt .

(4.3.10)

The upper and lower signs in (4.3.7) and (4.3.10) correspond to each other.

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

184

dynamic

Dynamic Plasticity

Fig. 4.3.2

A dynamic stress–strain curve showing the “overstress”.

Three separate propagation velocities play a part in this problem: cE , cP and the velocity c of the elastic-plastic waves. These three velocities are clearly related as follows: 1 1 1 = 2 + 2 . c2 cE cP

(4.3.11)

This formula can also be written in the form c cP = . 1 − c2 /c2E

(4.3.12)

Thus, the velocity of the elastic waves cE can be considered as a “limiting velocity” for the elastic-plastic waves. It is the highest possible velocity of propagation in the material considered and an invariant of the wave propagation phenomenon. From (4.3.12) it follows immediately that cP ∼ = c when c cE . This formula can be used to ﬁnd cP , if c and cE are obtained by measurements. Generally we have c E > cP ≥ c . The equality cP = c holds when the material is plastic/rigid and work-hardening. In this case c2 = E1 (σ, ε)/ρ, where E1 (σ, ε) is the variable work-hardening modulus. A dynamic stress–strain curve showing the possible variations during tests is shown in Fig. 4.3.2. The overstress is something composed of several components. Interesting information can be obtained from the dynamic and kinematics compatibility conditions

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

Rate Inﬂuence

E ∂ε ∂σ −E = ∂t ∂t P ∂ε ∂σ −ϕ = ∂t ∂t E P ∂ε ∂ε ∂v − − = ∂x ∂t ∂t ∂σ ∂v − = ρ ∂t ∂x

185

0, 0, 0, 0,

∂σ ∂σ dx + dt ∂x ∂t E E ∂ε ∂ε dx + dt ∂x ∂t P P ∂ε ∂ε dx + dt ∂x ∂t ∂v ∂v dx + dt ∂x ∂t

dynamic

= 0, = 0, (4.3.13) = 0, = 0.

From (4.3.13) it follows that across the characteristic lines (4.3.7) all the derivatives involved in the system (4.3.13) are discontinuous. Thus (4.3.7) are wave fronts which aﬀect all the unknown functions and certainly both parts εE and εP of the strain. Across the lines (4.3.8) all the derivatives except for the derivatives ∂εE /∂x and ∂εP /∂x are continuous. From (4.3.13) we may easily obtain: c2E [∂εE /∂t] = c2P [∂εP /∂t] .

(4.3.14)

This is the relation between the jump of the derivatives of the two components of the strain, and the velocities of propagation cE and cP . Since in the majority of cases, c2E c2P , it follows that [∂εE /∂t] [∂εP /∂t], and thus in many cases, if the material is in an elastic-plastic state and the work-hardening modulus is much smaller than the elastic modulus, the elastic part of the discontinuity carried by the elastic-plastic wave, can be neglected in comparison with the plastic part. Since cE = const., all the considerations concerning the relation (4.3.14) depend only on the function ϕ(σ, ε). We shall now discuss the special case when ψ = 0. In this case the diﬀerential relations (4.3.9) reduce to the well-known relations dσ = ±ρ cdv , while from (4.3.10) it follows that EdεE = ϕ dεP . Since in general E ϕ, it again follows that dεE dεP along (4.3.8). This relation or its equivalent dε = (1 + ϕ/E) dεP represents the relation between the increments of the components of the strain in the case ψ = 0. If ψ = 0 the relation between the components of the strain along (4.3.8) is more complicated and follows directly from (4.3.10) ψ ϕ P dε + dt . dε = 1 + E E

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

186

Dynamic Plasticity

This relation can also be used to examine cases when certain components or the time inﬂuence can be neglected. It may be obtained directly from the ﬁrst two relations (4.3.6) by eliminating ∂σ/∂t. The conclusions are the following. If the constitutive (4.3.2) and (4.3.3) are used, then both the elastic and plastic components of the strain propagate by the same type of wave with the velocity (4.3.7). However both components also possess stationary discontinuities. It should be remembered that the plastic constitutive equation (4.3.3) involves both instantaneous and non-instantaneous plastic response terms. A similar theory for elastic-plastic-viscoplastic stress waves was developed also by Tanimoto [1994]. The endochronic theory of plasticity to show the eﬀect of the strain rate on the inelastic behavior of structural steel under cyclic loading condition is formulated by Chang et al. [1989]. From the endochronic theory (Valanis [1972]) one is taking dζ 2 = Pijkl dεpij dεpkl − g 2 dt2 . By using a 4th order isotropic tensor for P the previous relation can be written f 2 dZ 2 = h2 dεpij dεpkl − g 2 dt2 , and this equation can by written as g 2 dt2 = F 2 f 2 dZ 2 in which

F =

h2

− α )(σ − α ) (σij ij ij ij − 1. (s0y f )2

The viscoplastic ﬂow condition, equivalent to the overstress of viscoplasticity is (σij − αij )(σij − αij ) h2 −1 > 0. 0 2 (sy f ) All the other not explained notations are constants. The authors are also making some comparison of the analytical solutions and the experimental results. The same problem was considered experimentally by Zhao [1997]. The classical split Hopkinson pressure bar tests are used, together with the yield stress dependency on strain rate and temperature ε˙ Q σY = A ln + T ε˙0 RT where A, Q, R are constant coeﬃcients and T is the absolute temperature. Sets of tests of 230 s−1 to 1650 s−1 were considered for specimens of diameter 10 mm and length 10 mm. The results are shown in Fig. 4.3.3. The aluminum 1100-0 was tested by Pao and Gilat [1989]. They were tested for the plastic strain rate sensitivity with temperature as ∗ τ − τ ∗ ) σij v (¯ H0 sinh ε˙P = 2η exp − ij kT kT τ¯

dynamic

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Rate Inﬂuence

dynamic

187

Fig. 4.3.3 Comparison between stress–strain curves derived from real tests and those from simulated tests.

were H0 , η, v ∗ , and τ ∗ are determined from results of tests in which the material is deformed at various constant strain rates and temperatures. At T = 0, τ¯ = τ ∗ + H0 /v ∗ . Other values of material constants are given. They have used the same boundary conditions as given below and the results are given in Fig. 4.3.4. Comparison with the tests of Bell is done on three distances from the impacted end. The comparison seems good. The existence and properties of the free energy function compatible with the second law of thermodynamics in one-dimensional rate-type semilinear viscoelasticity is analyzed by Faciu and Mihailescu-Suliciu [1987]. Necessary and suﬃcient conditions are given such that a free energy as a function of strain and stress exists and is unique, that it is non-negative function and possesses a monotony property with respect to the equilibrium curve. A bound in energy for the smooth solutions of certain initial and boundary value problems with respect to the input data is established when the equilibrium curve is a non-monotonic curve. Bounds in energy for the smooth solutions of initial and boundary value problems for semi-linear hyperbolic systems were given by Fˇaciu and Simion [2000]. They prove that the integral energy identities for smooth solutions are still valid for weak solutions. Energy estimates of the weak solutions of the same problems are given. The way weak and strong discontinuities in the input data aﬀect the regularity of the total energy of the solution is discussed. The uniqueness of the weak solutions is derived.

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

188

Dynamic Plasticity

Fig. 4.3.4

Variation of strain with time at three indicated distances.

A nonhomogeneous and nonautonomous 2 × 2 quasilinear system of ﬁrst order describing rate-type materials is considered by Manganaro and Valenti [1993] within the framework of similarity reduction procedures. The constitutive equation is of the form ∂ε ∂v = φ(v, ε) + ψ(v, ε) . ∂t ∂t Classes of exact similarity solutions to the governing model as well as functional forms for the material response function involved have been determined. Reduction to linear form have been carried out for diﬀerent forms of constitutive laws. In another article by Menganaro and Meleshko [2002], the method of diﬀerential constrains is applied for systems written in Riemann variables. Generalized simple waves are considered. This class of solutions can be obtained by integrating a system of ordinary diﬀerential equations. The above rate-type models is one of the systems studied.

dynamic

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Rate Inﬂuence

dynamic

189

A constitutive law of the form ˙ + G(σ, ε(u), β) σ˙ = Eε(u) where E is a fourth order tensor, and β is the damage ﬁeld was considered by Chau et al. [2002]. When β = 1 the material is undamaged, while the value β = 0 indicates the stage of complete damage. The mechanical damage of the material, caused by excessive stress or strain, is described by a damage function whose evolution is modeled by an inclusion of parabolic type. The authors provide a variation formulation for the mechanical problem and sketch a proof of the existence of a unique weak solution to the model. They introduce and study a fully discrete scheme for the numerical solutions of the problem. An optimal order error estimate is derived for the approximate solutions under suitable solution regularity. Numerical examples are presented to show the performance of the method. The contact problems considered by Fern´ andez et al. [2003] involve the large class of elastic-viscoplastic materials. They focus on the ﬁnite element approximations which involve nonmatching meshes on the contact part. Such a conﬁguration in which the nodes inherited from the discretizations of the bodies may not coincide arises in computational situations when the diﬀerent bodies are independently meshed and/or there is an initial distance between the bodies and/or an evolution process is considered. The ﬁrst aim of the authors is to study the convergence of ﬁnite element methods and then to carry out the numerical experiments associated with the theoretical studies. A simply non-linear anelastic model describing the acceleration of the relaxation process in the presence of vibrations was considered by Dr˘ag˘anescu and C˘ap˘ aln˘ a¸san [2003]. An analytic variational iteration method is used in order to study the relaxation process. Also a method of identiﬁcation of the parameters of the system from the experimental data is given.

4.4

Numerical Examples

In the numerical examples of the rate-type constitutive equations under consideration were used in the form 1 + χΦ(σ, ε) σ˙ + Ψ(σ, ε) , (4.4.1) ε˙ = E with χ=

0

if σ ≤ f (ε) or σ˙ < 0 ,

1

if σ = f (ε) and σ˙ > 0 .

(4.4.2)

The coeﬃcient χ is used so that the constitutive equation is used during loading and unloading.

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

190

dynamic

Dynamic Plasticity

The characteristic lines are dx E = ±c(σ) = , dt ρ(1 + EΦ)

(4.4.3)

dx = 0 , the diﬀerential relations satisﬁed along them dσ = ±ρcdv − ρc2 Ψ(σ, ε) , dσ = EdεE ,

(4.4.4)

dεP = Φ(σ, ε) dσ + Ψ(σ, ε) dt . The coeﬃcient function Ψ(σ, ε) describing the non-instantaneous response was assumed to depend linearly on the overstress (Cristescu [1972a, 1972b], Cristescu and Cristescu [1973]): k(ε) [σ − f (ε)] if σ > f (ε) and ε ≥ σ , E E (4.4.5) Ψ(σ, ε) = 0 if σ ≤ f (ε) . For the relaxation boundary we write f (ε) =

if ε ≤ εY ,

σY 1/α

β(ε + ε0 )

(4.4.6)

if ε > εY

or some variants of this law. The examples given are for aluminum (1100◦F aluminum annealed for two hours at 590◦ C and then furnace cooled — see Bell [1968]). For this material the relations σ = Eε 1/α

σ = β(ε + ε0 )

if

σ ≤ σY ,

if

σ > σY

were used, where E = 7038000 N/cm2 and ρ0 = 2.7 g/cm3 , and therefore c0 = 5080 ms−1 . For the other constants, the following numerical values were used (Cristescu and Bell [1970] and Cristescu [1972b]): for the quasi-static stress–strain curve, 8 2 2 σY0 = 703.80 N/cm , β = 22908.0 N/cm , α = ; 3 for the dynamic stress–strain curve, 2

σY1 = 212.18 N/cm ,

2

β = 38640.0 N/cm ,

α = 2;

for the translated dynamic stress–strain curve, 2

σY2 = 759.00 N/cm ,

2

β = 38640.0 N/cm ,

α = 2,

ε0 = 0.000278 .

The true yield stress for the aluminum under consideration is in fact, and the stress– strain curve is obtained from the dynamic one by a translation along the strain axis (this deﬁnes ε0 ). The stress–strain curve obtained by this procedure is quite close to the dynamic one.

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Rate Inﬂuence

dynamic

191

The expression for k is an expression showing a small value for small strains but becomes greater, nearly constant, for higher values. Thus * ε + (4.4.7) k(ε) = k0 1 − exp − ε¯ with k0 and ε¯ material constants. Various variants of this constitutive law were used. Concerning the slope of the instantaneous curve we assume that it lies between the elastic slope and that of the relaxation boundary E≥

1 > f (ε) . Φ(σ, ε) + 1/E

(4.4.8)

Further Φ(σ, ε) was chosen to match a certain set of experimental data. Two forms were used. Starting from a cubic equation we have used Φ(ε) = χ

3[ε − εY − ε∗ + (a/3E)3/2 ]2/3 1 − , a E

where √ a=m+n ε with m, n material constants and ε∗ is a threshold strain. Some other value is # $ 3 E γ σ 2 √ 3 Φ(σ, ε) = χ −1 E p+q ε E where p, q and γ are material constants. It is quite diﬃcult to determine the velocity of propagation experimentally, and thus Φ. The numerical examples are for the impact of two bars, the “hitter” and the “specimen”. For the specimen we have t = 0,

0<x≤l:σ=ε=v=0

for the initial conditions. For the boundary conditions the end of the bar x = l is assumed free t ≥ 0,

x = l : σ = 0.

At t = 0 the bar is impacted at the end x = 0 by another bar identical with the specimen. Thus, for the hitter we have t = 0,

−l ≤ x < 0 : σ = ε = 0 ,

v=V .

Thus for t = 0 the end x = 0 of the specimen is subjected to a sudden jump. This jump was handled in two ways. First, it was assumed that the impact velocity is fast but smoothly transferred to the end of the specimen. A convenient very short time interval 0 ≤ t < tm was chosen, in which this smooth increase of velocity at the impacted end of the specimen takes place from zero up to vmax . For simplicity, it

January 12, 2007

10:41

192

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Dynamic Plasticity

Fig. 4.4.1

Variation of the strain at various sections along the bar, and time of contact.

was assumed in the program that the velocity at the end of the specimen increases according to a linear law. Thus, the ﬁrst kind of boundary conditions were t 0 ≤ t < tm : v = vmax , t m x=0 t ≤t≤T :v =v , m c H S Tc < t : σS = 0 , where tm is a conveniently chosen time interval (in most examples given here tm = 0.5 µs) and vmax = V /2. Tc is a computed time, called time of contact. In the time interval tm ≤ t ≤ Tc the ends x = 0 of the two bars are moving together. σS is the specimen stress which is computed as is Tc . Several examples have been computed. In Fig. 4.4.1 is given the variation of the strain at various sections along the bar. Also have been given also the time of contact and a classical solution. One can see that the rate type solutions are quite correct. In Fig. 4.4.2 is given the variation of the stress at the impacted end. After a peak, follows a plateau. Again the experimental data are quite well reproduced. The decrease of the stress is due to unloading. In Fig. 4.4.3 is shown the variation of the deformation at the 9D, i.e., close to the free end, while in Fig. 4.4.4 is given the variation of the displacement in time at various cross-sections. From the above one can see that a plateau for strains can be predicted for a ﬁnite distance (Suliciu [1972]). Daimaruya and Naitoh [1983] have also considered

dynamic

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

Rate Inﬂuence

Fig. 4.4.2

Variation of the stress at the impacted end.

Fig. 4.4.3

Variation of the strain in time at 9D.

dynamic

193

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

194

Dynamic Plasticity

Fig. 4.4.4

Comparison of the displacement-time curves.

the plateau problem; they have shown numerically taking the model (4.2.2) for hardened aluminum f (ε) = 6.89(20 − 0.01/ε) MPa, with the values of the constants E = 68.8 GPa, ρ = 2.67 × 103 kg/m3 , k = 106 sec−1 and impact velocity V = 15 m/sec, that a plateau of uniform strain adjacent to the impact end can exist. For larger value of k, the plateau will be shorter. Various variants of the constitutive equation as well as examples are considered by Cristescu and Suliciu [1982]. For instance ˙ + G(σ, ε(u), β) σ˙ = Eε(u) where β is a function which satisﬁes an ordinary diﬀerential equation as β˙ = ϕ(σ, ε(u), β) , (see Ionescu and Sofonea [1993], Fern´andez [2004]). Some other authors (Luo et al. [2003]) have used the same model to introduce the isothermal rheological forming of high-strength alloying parts with complicated curved surface. They have used various speeds and found that for the lower forming velocity (v = 0.022 mm/s) the non-uniformity of temperature ﬁeld is smaller than at higher speeds.

4.5

Other Papers

A ﬁrst study about the eﬀect of temperature gradients on the propagation of elastoplastic waves is due to Francis and Lindholm [1968]. It is question of the propagation

dynamic

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Rate Inﬂuence

dynamic

195

of an extensional elastoplastic wave through a long thin bar heated at the end to produce a continuously decreasing temperature proﬁle. The temperature distribution is approximated as an exponential function. Analytical solutions are obtained by Shaw and Cozzarelli [1971] for stress, velocity, and strain at the wave front in a suddenly loaded semi-inﬁnite rod of a material with a linear instantaneous response and nonlinear inelastic response. The material properties are assumed to depend on position directly or through a dependence on a prescribed non-uniform temperature ﬁeld. Detailed solutions are obtained for two examples, a nonlinear viscoelastic material with temperature dependent parameters and a rate-sensitive plastic material which may have temperature dependent parameters and yield point. The dynamic mechanical behavior of titanium in shear was studied by Lawson and Nicholas [1972]. They have used a constitutive equation of the form ∂τ ∂γ = + g(τ, γ) . ∂t ∂t They found that the torsional plastic waves in pure titanium can be predicted from the rate-dependent theory of plastic wave propagation. The excellent agreement between theoretical and experimental results for stresses at the end of a long tube subjected to a torsional pulse demonstrates the consistency of the entire testing procedure. The problem of impact on a nonlinear viscoelastic rod of ﬁnite length is considered by Mortell and Seimour [1972]. They have considered a constitutive law of the form G

σ˙ = φ(ε)ε˙ + ψ(σ, ε) . It is shown that, in the high frequency or geometrical acoustics limit, the disturbance in the rod may be represented as the superposition of two modulated simple waves traveling in opposite directions which do not interact in the body of the material. A comparison with the experiments is done by Kuriyama and Kawata [1973]. They consider three types of constitutive equation; that is, the Karman-type theory, the Malvern-type theory, and the Cristescu-type theory. The constitutive equation is written E ε˙ − σ˙ = h(σ, ε) . They ﬁnd that the front of the stress wave travels always with the elastic-wave velocity and the plateau of the uniform plastic strain remains in the neighborhood of the impact end. They ﬁnd that the Johnston–Gilman-type of constitutive equation is matching better. Suliciu et al. [1973] have developed a class of general solutions for wave propagation in a rate-type material. These solutions, obtained by invoking equation splitting, demonstrate elastic-like behavior for the kinematics variables u and ε although the material is inelastic. This observation serves as a warning to those carrying out dynamic experiments involving only axial loadings. Measurements of

January 12, 2007

196

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Dynamic Plasticity

strain and velocity may not reveal the true characteristics of materials. An extended solution for transverse motion is presented and experiments involving transverse deﬂection are highly recommended because these results do provide information about σ and therefore the rate dependencies. A one-dimensional problem has been considered by Nicholson and Phillips [1978]. They have considered elastic/viscoplastic/plastic materials of the form σ˙ σ σ˙ + + η σ − σ0 − k ε − ε˙ = E0 Ep E0 where σ0 are the quasi-static yield stress and all the other are constants. Various variants of the constitutive equation are considered for stress impact and velocity impact. Then the Laplace transform is used, and near the impact end the solution is obtained in terms of some special functions. For an elastic/viscoplastic material, a region of uniform strain arises at the impact end more rapidly for velocity impact than for stress impact. Also for an elastic/viscoplastic/plastic material, the plastic strain makes no contribution at the impact end for velocity impact, but it does for stress impact. For aluminum and copper rods, for a wide range of striking velocities and rods lengths, the general applicability of one-dimensional non-viscous dynamic plasticity theory is conﬁrmed (Dawson [1972]). A model of the kind used in this chapter vas proposed by Suliciu [1981] to describe the Savart–Masson eﬀect by a rate-type constitutive equation. The viscosity coeﬃcient has strong variations in some regions of the stress–strain plane that lie above the equilibrium curve σ = f (ε). Cernocky [1982] has considered four constitutive equations of viscoplasticity and made a comparison between them. Each theory is ﬁtted to the same stress– strain data, and both analytical and numerical methods are employed to highlight similarities and diﬀerences between their predictions. Diﬀerent manifestations of strain-rate and stress-rate history eﬀects predicted by the theories are compared, and the theories are shown to share a signiﬁcant qualitative bias between responses to stress and strain-controlled loading. Some dynamic tests on aluminum titanium and steel were done by Nicholas [1981]. He has found a rate sensitivity of 10 to 102 s−1 . In another papers Nicholas et al. [1987a, b] a ﬁnite diﬀerence computer code is used to numerically simulate uniaxial strain waves generated from plate impact experiments. The incremental ﬂow law of Bodner and Partom and the Perzyna law are compared with experiments. Numerical computations using a ﬁnite diﬀerence computer code illustrate that the decay of the amplitude of the propagating precursor elastic wave is a consequence of material strain-rate dependence. The possibility of describing rubber-like materials by means of a rate-type viscoelastic constitutive equation is due to Mihailescu-Suliciu and Suliciu [1987]. The problem of generation of one-dimensional tensile shock waves in rubber-like materials is studied numerically and compared to the exact elastic nonlinear solution and the steady wave solution. It is shown that a rate-type semilinear visco-elastic

dynamic

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Rate Inﬂuence

dynamic

197

model can describe the steepening of the wave during its propagation and a “thickness” of the wave is naturally incorporated. An energetic criterion for the numerical stability is also introduced. An experimental technique is described by Chhabildas and Swegle [1989] which uses anisotropic crystals to generate dynamic pressure-shear loading in materials. The coupled longitudinal and shear motion generated upon planar impact of anisotropic crystal can be transmitted into a specimen bonded to the rear surface of crystal, and monitored using velocity interferometer techniques. In a paper by Li and Clifton [1981] one is presenting stress–strain curves for aluminum sandwiched between hard steel plates. The shear strain rates go up to and sustain these rates for a duration of 10−6 s. These stress–strain curves are much higher than the classical ones. Damage is considered by Ziegler [1992] to be a time-variant imperfection of the yielding material, analogously to the growth of porosity of a voided material with given initial porosity. Also plastic strain is a distortion of the perfect elastic background structure. The internal variable approach is transformed into a numerical routine of computational dynamic viscoplasticity. Starting from the phenomena not well described as the increase of stress with strain rate, the propagation speed of the stress wave corresponding to a large strain is slow, and others, Tanimoto et al. [1993] try to explain it by introducing an elasticplastic-viscoplastic constitutive equation of the form ρ

∂σ ∂v = , ∂t ∂x ∂v ∂ε = , ∂x ∂t k2 k1 ∂σ 1 2 σE 2 σ + − 1 + − 1 σ, ∂ε E 3ζ σ ∂t 3η σS = ∂t 1 ∂σ , E ∂t

σ > σS σ ≤ σS ,

with the various constants given as: E = 103.5 GPa, σS = 102.4 MPa, ζ = 11.77 MPa, η = 1.177 × 103 Pa s, k1 = 0.85, k2 = 5.4, ρ = 8.391 × 10−9 kgr/mm3 . The approach is also numerical, as given above. Several ﬁgures are given to show the eﬀect. We give only two. In Fig. 4.5.1 is given the variation of stress in the distance from the impact end. In Fig. 4.5.2 is given the variation of strain with distance from the impacted end. Close to the impacted end the strain is constant (plateau) and this value is increasing in time. That is not in agreement with the tests, but the authors are trying to ﬁnd various arguments. An approach is developed to generate exact solutions to a hyperbolic model of the form ut + vx = 0 ,

vt + h(v)ux = f (v)

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

198

Dynamic Plasticity

Fig. 4.5.1

Stress-distance relationship.

Fig. 4.5.2

Strain-distance relationship.

by Fusco and Manganaro [1994a]. The leading idea of the analysis which is carried on herein is to require the model in point to be considered with a pair of additional equations deﬁning Riemann invariants-like quantities along the characteristic curves. Hence, classes of model constitutive laws allowing a reduction procedure to hold are characterized. Later on, a nonhomogeneous system of partial diﬀerential equations of ﬁrst order involving two dependent and two independent variables is considered also by Fusco and Manganaro [1994b]. The same authors (Fusco and Manganaro [1996]) consider the system ut − vx = 0 ,

εt − u x = 0 ,

vt − φ(t, ε, v)ux = ψ(t, ε, v)

for which solutions are given. The same kind of equations vas also considered by Tabov [1996]. He obtains easy to verify criterion for the existence of such solutions and clearly stated conditions on the initial data providing the existence and uniqueness of the solutions. The system vt − σx = 0 ,

σt − φ(t, σ)vx = ψ(t, σ)

is proposing to be reduced to linear form 2 × 2 non-homogeneous and nonautonomous ﬁrst order quasi-linear systems by Curr`o and Valenti [1996]. The system

dynamic

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Rate Inﬂuence

dynamic

199

through the use of a variable transformation is reduced to a homogeneous and an autonomous form which can be linearized by means of hodograph transformation. A general algorithm of implicit stress integration in viscoplasticity is presented by Kojic [1996]. The algorithm is ﬁrst applied to isotropic metals obeying the von Mises yield condition with mixed hardening and then to orthotropic metals. A theory of viscoplasticity bounded between two distinct rate-independent generalized plasticity models was considered by Auricchio [1997]. Main features of the model are the following: (1) it approaches the two rate-independent generalized plasticity models for the case of fast and slow loading conditions, respectively; (2) it properly describes loading-unloading-reloading conditions for any loading rate; (3) it reproduces the experimentally observed diﬀerence between the dynamic and the static yielding conditions. One has in mind metals, polymers, geomaterials, and shape-memory alloys. Both the time-continuous and the time-discrete version of the model are discussed. Several examples are given. The main objective of the paper by Lodygowski and Perzina [1997] is the investigation of adiabatic shear band localized fracture phenomenon in inelastic solids during dynamic loading processes. This kind of fracture can occur as a result of an adiabatic shear band localization generally attributed to a plastic instability implied by micro-damage and thermal softening during dynamic plastic ﬂow processes. A review is presented by Klepaczko [1998] on recent progress in shear testing of materials at high and very high strain rates. Some experimental technique are discussed which allow for materials testing in shear up to 106 1/s. More information is provided on experimental techniques based on the Modiﬁed Double Shear specimen loaded by direct impact. This technique has been applied so far to test a variety of materials, including construction, armor and inoxidable steels, and also aluminum alloys. The double shear conﬁguration has also been applied to test sheet metals, mostly used in the automotive industry, in a wide range of strain rates. A new experimental conﬁguration which can be applied for experimental studies of adiabatic shear propagation and high speed machining is discussed. One is also showing that for steel at lower impact velocities, the energy to the ﬁnal localization increases up to 681 MJ/m3 ; however, at impact velocities higher than 100 m/s, the energy drops considerably, to the value of ∼ 8.0 MJ/m3 . Thus, the energy drop is slightly less than a hundred times. Results of pressure-shear plate impact experiments on an alumina ceramic (AD85) containing a signiﬁcant amount of an oxide glass phase were done by Sundaram and Clifton [1998]. Under high strain-rate loading, the ceramic (porosity of approximately 9%) shows low shear strength and a strong strain softening behavior. The material is modeled as an elastic-visco-plastic solid. The collapse of the voids causes a strong hydrostatic relaxation which brings down the pressure. A ﬁnite element technique is presented by Yokoyama [2001] for the analysis of one-dimensional torsional plastic waves in thin-walled tube. Three diﬀerent nonlinear constitutive relations deduced from elementary mechanical models are used

January 12, 2007

200

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Dynamic Plasticity

to describe the shear stress–strain characteristics of the tube material at high rates of strain (103 s−1 ). It is question of elasto-plastic model of Karman-Duwez, the elasto-viscoplastic model of Sokolovsky–Malvern and the elasto-viscoplastic-plastic model of Cristescu–Lubliner. The resulting incremental equations of torsional motion for the tube are solved by applying a direct numerical integration technique in conjunction with the constitutive relations. A comparison with experimental results shows that the strain-rate dependent solutions show a better agreement with the experimental results than the strain-rate independent solutions. The superplastic deformation and cavitations damage characteristics of a modiﬁed aluminum alloy are investigated at a temperature from 500 to 550◦ C by Khaleel et al. [2001]. The experimental program consists of uniaxial tension tests and digital image analysis for measuring cavitations. The experiments reveal that evolution of damage is due to both nucleation and growth of voids. A viscoplastic model for describing deformation and damage in this alloy is developed based on a continuum mechanics framework. The model includes the eﬀect of strain hardening, strain rate sensitivity, dynamic and static recovery, and nucleation and growth of voids. Altenhof and Ames [2002] study the strain rate eﬀects for aluminum and magnesium steering wheel armatures when they are subjected to dynamic impact tests. Two geometrically diﬀerent steering wheel armatures, a three spoke proprietary aluminum alloy armature and a four spoke magnesium alloy armature, underwent experimental impact testing. The strain rates are not very high: 17 s−1 for aluminum and 46 s−1 for magnesium armature. Stress–strain response under constant and variable strain-rate is studied for selected models of inelastic behavior by Lubarda et al. [2003]. The derived closedform solutions for uniaxial loading enable simple evaluation of the strain-rate eﬀects on the material response. Various one-dimensional models have been written. In the case of parabolic hardening, the ﬂow stress is related to the plastic strain εp εp p σ−Y) p 2− p σ = Y + (ˆ εˆ εˆ where Y is the initial yield stress, and εˆp is the plastic strain at the apex of the plastic stress–strain curve with the stress σ p . For the hyperbolic type of hardening we have Yˆ − Y . σ p = Yˆ − 1 + εp /ˆ εp For viscoelastic-plastic model, the stress is Eε , σ = σ ∗ 1 − exp − ∗ σ

ε=−

σ σ∗ ln 1 − ∗ . E σ

In Fig. 4.5.3 are given three curves corresponding to this case. Here σ ∗ = η ε˙ with η the viscosity coeﬃcient. In a similar way one has considered several curves including the viscoelastic-elastoplastic model.

dynamic

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Rate Inﬂuence

dynamic

201

Fig. 4.5.3 The stress–strain curves for viscoelastic-plastic model in the case of parabolic hardening.

The split Hopkinson pressure bar, or Kolsky’s apparatus was re-analyzed by Zhao and Gary [1996] and by Zhao [2003]. The same system of equation 1 ∂σ ∂ε = ∂t E ∂t

if σ ≤ σs ,

1 ∂σ ∂ε = + g(σ, ε) ∂t E ∂t

if σ > σs

is used with g(σ, ε) =

(1 + Et /E) σ − σs − Et ε . η

He is proposing to calculate directly the dispersive relation for the wave dispersion corrections and to use the elastic simulation to determine more accurately correspondence between the wave beginnings. A method to increase measuring duration is proposed. An identiﬁcation technique, especially for non-metallic materials, based on an inverse calculation method is also presented. The Kolsky torsion bar was used by Hu and Feng [2004] to study the behavior of polymer melts at high shear rates from 102 s−1 to 104 s−1 and temperature up to 300◦C. To give an example on Fig. 4.5.4 is given one case considered. The important inﬂuence of the strain rate is evident. Constitutive modeling of the high strain rate behavior of interstitial-free steel was considered by Uenishi and Teodosiu [2004]. The strain rates are quite high of 1000 s−1 . To have an idea, we reproduce in Fig. 4.5.5 several curves from that paper. In order to simulate the high strain rate tensile test, and that of temperature, the Johnson–Cook model is used m T − Troom ε¯˙ 1− σ ¯ (¯ ε, ε¯˙, T ) = (A + B ε¯n ) 1 + C ln ε˙0 Tref − Troom

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

202

Dynamic Plasticity

Fig. 4.5.4

Shear stress proﬁles for various shear rates and 190◦ C initial temperature.

where σ ¯ , ε¯ and ε¯˙ are the equivalent tensile stress, the equivalent tensile strain and the equivalent tensile strain rate, respectively. The ﬁrst term represents the work hardening behavior at the reference strain rate ε˙0 and at the room temperature. The second and third terms express the eﬀects of strain rate and temperature, respectively. The parameters A, B, n, C and m are material parameters and T denotes the absolute temperature. Troom and Tref are the absolute room temperature and melting temperature of the material, in the case 293 and 1809 K, respectively. A FE analysis has been made under the assumption that the process is adiabatic. Stoﬀel [2004] [2005] has considered an evolution of plastic zones in dynamically loaded plates using diﬀerent elastic-viscoplastic laws. He has used the Chaboche [1989] low developed for non-linear hardening σij − Xij 3 p˙ , − X ) 2 IIσ (σrs rs n IIσ (σij − Xij )−R−k p˙ = , K

ε˙pij =

2 X˙ ij = aε˙pij − sXij p˙ ; 3

R˙ = b1 (b2 − R) p˙

with the abbreviations εpij , p, σij , Xij , R denoting the plastic strain tensor, equivalent plastic strain, second Piola–Kirchhoﬀ stress tensor, backstress tensor and isotropic hardening. The yield limit k and the material parameters a, s, b1 , b2 ,

dynamic

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Rate Inﬂuence

dynamic

203

Fig. 4.5.5 Stress–strain curves of an IF steel at diﬀerent strain rates, including strain rate jump tests: (1) monotonic tensile test at 1000 s−1 ; (2) tensile test at 1000 s−1 after a tensile pre-strain of 8% at 0.001 s−1 ; (3) after a tensile pre-strain of 16% at 0.001 s−1 ; (4) monotonic tensile test at 0.001 s−1 .

n, K must be obtained from tension tests. A separation of isotropic and kinematic hardening was not possible so that in the Chaboche model kinematic hardening is assumed. Another model considered is the Tanimura [1979] one, which can be expressed as σij 3 ε˙pij = rp˙ ) , 2 IIσ (σij p˙ = e (1/

√

−S0 3)II (σ )−τ ∗ σ ij

with the material parameters S0 , r, τ ∗ to be determined from uni-axial tension tests. This is an overstress model without hardening. The third model is the Bodner–Partom [1975] model. This is a model disregarding the yield stress. The model is σij 3 , ε˙pij = p˙ ) 2 IIσ (σrs 2 − 1 ( R+D )2n n+1 n p˙ = √ D0 e 2 IIσ (σrs ) , 3 σij p , R˙ = m1 (R1 − R)σij ε˙ij , D = Xij IIσ (σrs ) σij 3 p D1 − X X˙ ij = m2 ij σkl ε˙kl , ) 2 IIσ (σrs

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

204

Dynamic Plasticity

Fig. 4.5.6

Conical shape of the plate.

where the material parameters n, D0 , D1 , R1 , m1 , and m2 have to be identiﬁed from tension tests. These three models are applied by Stoﬀel for the motion of a thin (thickness 2 mm) circular membrane of 138 mm and 553 mm. The motion of such a plate at various times is shown in Fig. 4.5.6. Trying to describe the motion of such plates the author was obliged to consider the elastic material properties in the simulations. Using the Chaboche model elastic, hardening and viscous material properties can be separated from each other. This allows in the material parameter identiﬁcation procedure a precise adaptation of the viscoplastic law to the uni-axial tension tests. In the Bodner–Partom model elastic properties are not assumed and hardening as well as viscous behaviors are combined with each other. In the Tanimura model the hardening is neglected. With this described advantage in the case of the elasticviscoplastic Chaboche model simulations using this law lead to the most precise results. A novel technique for time-resolved detection and tracking of interfacial and matrix fracture in layered materials is due to Minnaar and Zhou [2004]. The measurements at multiple locations allow the speeds at which interfacial crack front or matrix cracking/delamination front propagates to be determined. The results show that the speed of delamination or the speed of matrix cracking/delamination increases linearly with impact velocity. In another paper Colak [2004] consider small strain, isotropic, viscoplasticity theory based on overstress, modiﬁed to model the complex cyclic hardening behavior under proportional and non-proportional loading. The theory is without yield

dynamic

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

Rate Inﬂuence

dynamic

205

surface and no loading/unloading conditions. The theory consists of two tensors valued state variables, which are in equilibrium stress and the kinematic stress, and a scalar isotropic stress with a ﬂow law. The propagation of stress pulses is studied by Ostoja-Starzewski [1995] in one-dimensional piecewise constant microstructure of grains with power-law elastic response, having randomness present in constitutive moduli and grain lengths. A study is conducted of the sensitivity of loading and unloading shock waves. The ﬂow law is (see Krempl [1998], development of viscoplasticity theory based on overstress Krempl [1988], S¨ ut¸cu ¨ and Krempel [1989]): ε˙ = ε˙ E + ε˙ P =

1 + v 3 σ − g σ˙ + E 2 Ek[Γ]

where g is the deviatoric part of the equilibrium stress G, Γ2 =

3 (σ − g) : (σ − g) 2

and the viscosity function k = k1

Γ 1+ k2

−k3

with k1 , k2 and k3 material constants. The equilibrium stress is introduced to represent the defect structure of the material. The growth law for the equilibrium stress consists of elastic, inelastic, dynamic recovery term and kinematic hardening contributions: Ψ[Γ] ˙ σ − g Γ g − f Ψ[Γ] σ˙ + − + 1− f g˙ = E k k A E where Ψ is the shape function which aﬀects the transition between initial quasi elastic behavior and inelastic ﬂow. It is related as C2 − C1 Ψ[Γ] = C1 + exp[C3 Γ] where C1 , C2 and C3 are material constants. The positive, decreasing shape function Ψ is bounded by 1 > Ψ[Γ]/E > Et /E. The growth laws for the kinematic stress f is given by Et (σ − g) f˙ = E k[Γ] where Et is the tangent modulus at the maximum inelastic strain. The state variable A, with the dimension of stress, grows according to 2 ˙ p˙ A = Ac [Af − A] 3 where Ac and Af are material constants. The equivalent inelastic strain rate p˙ is √ p˙ = ε˙P : ε˙P .

January 12, 2007

206

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Dynamic Plasticity

Fig. 4.5.7 Uniaxial dual-amplitude step-up test using modiﬁed viscoplasticity. Further hardening is observed after the increase in strain amplitude. The strain rate is ε˙ = 1 × 10−5 s−1 .

Since an extra hardening is observed and that is rate independent, one is using the Krempel [1998] constitutive equation. Also to include the strain amplitude eﬀect as well as the loading path eﬀect, the non-proportionality measure deﬁned by Tanaka [1994] is used. The forth order tensor C˙ ijkl = cc (uij ukl − Cijkl ) p˙ ˙ and the non-proportionality with cc a material constant, is introduced. u = ε˙ P /p, measure is Cijkl Cijkl − uij Cklij Cklmn umn . Φ= Cprst Cprst The center of inelastic strain range, Y is modeled by Tanaka [1994], ˙ = ry (εP − Y) p˙ Y where ry is a material constant. The size of the memory surface q is q = |εP − Y| where | | indicates magnitude. The theory was applied to various loadings. For instance, for uniaxial dual amplitude step-up test is shown in Fig. 4.5.7. The mathematical study of the problem of unilateral contact between an elasticviscoplastic body and a rigid frictionless foundation is due to Sofonea [1997]. The constitutive law is σ˙ = E ε˙ + G(σ, ε)

dynamic

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Rate Inﬂuence

where E and G are constitutive functions. For −k1 F1 (σ − f (ε)) G(σ, ε) = 0 k2 F2 (g(ε) − σ)

dynamic

207

G one is using if σ > f (ε) if g(ε) ≤ σ ≤ f (ε) if σ < g(ε)

where k1 , k2 > 0 are viscosity constants and F1 , F2 are increasing functions with F1 (0) = F2 (0) = 0. The variation formulation of the problem is given and the existence and uniqueness result for the displacement and stress ﬁeld is obtained. A ﬁxed point method was used in order to obtain the existence and uniqueness of the solution. The continuous dependence of the solution with respect to the input data as well as the stability result is then analyzed. Matos and Dodds [2002] have considered the initiation of brittle fracture triggered by a transgranular cleavage mechanism typical of that exhibited by ferritic steels operating in the ductile-to-brittle transition region. The plastic strain is of the form γ q q D − 1 >1 σ σ e e vp ε˙ = q 0 ≤1 σe where D and γ denote material parameters, q denotes the rate-dependent uniaxial tensile stress and σe denotes the static uniaxial tensile stress.

Fig. 4.5.8 Stress–strain curves of samples cut from an HSLA-65 plate at indicated directions and locations.

January 12, 2007

208

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Dynamic Plasticity

Fig. 4.5.9 Comparison of PB-model predictions with experimental results at a strain rate of 3000/s and indicated initial temperatures.

A paper in which one is discussing the Hopkinson technique for the dynamic recovery experiments is due to Nemat-Nasser et al. [1991]. In a recent paper NematNaser and Guo [2005] study the thermomechanical response of high-strength lowalloy steel (HSLA-65) in uniaxial compression tests. True strains exceeding 60% are achieved in these tests, over the range of strain rates from 10−3 /s to about 8500/s, and at initial temperatures from 77 to 1000 K. To show the inﬂuence of the strain rate is given the Fig. 4.5.8. Even the elastic parameters seem to be inﬂuenced. They apply the Johnson–Cook model and their own (PB-model). For their own model, it is for T ≤ Tc : 1/2 &3/2 γ ˙ τ = 760γ 0.15 + 1450 1 − −10.6 × 10−5 T ln 4 × 108 !γ where T = T0 + 0.267 0 τ dγ and for T > Tc we have τ = 760γ 0.15 where −1 γ˙ −5 . Tc = −10.16 × 10 ln 4 × 108 Figure 4.5.9 is showing the theory adapted to the experimental data. The compressive stress–strain behavior of a NiTi shape memory alloy has been determinated by Chen et al. [2001], over strain rates of 10−3 –7.5 × 102 s−1 . A split Hopkinson pressure bar with a pulse shaping technique was used to perform valid dynamic tests. Experimental results show that, the plateau stress of the shape memory alloy is strain rate dependent. The material is returning to its original length upon unloading.

dynamic

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Rate Inﬂuence

dynamic

209

Forrestal et al. [2003] present a Hopkinson bar technique to evaluate the performance of accelerometers that measure large amplitude pulses, such as those experienced during projectile penetration tests. An aluminum striker bar impacts a thin Plexiglas or copper disk placed on the impact surface of an aluminum incident bar. The Plexiglas or copper disk pulse shaper produces a nondispersive stress wave that propagates in the aluminum incident bar and eventually interacts with a tungsten disk at the end of the bar. A quartz stress gage is placed between the aluminum bar and tungsten disk, and an accelerometer is mounted to the free end of the tungsten disk. An analytical model shows that the rise time of the incident stress pulse in the aluminum bar is long enough and the tungsten disk length is short enough that the response of the tungsten disk can be accurately approximated as rigid-body motion. They measure stress at the aluminum bar-tungsten disk interface with the quartz gage and they calculate rigid-body acceleration of the tungsten disk from Newtonian’s Second Law and the stress gage data. In addition they measure strain-time at two locations on the aluminum incident bar to show that the incident strain pulse is nondispersive and they calculate rigid-body acceleration of the tungsten disk from a model that uses this strain-time data. Thus, they can compare accelerations measured with the accelerometer and accelerations calculated with models that use stress gage and strain gage measurements. They show that all three acceleration-time pulses are in very close agreement for acceleration amplitudes to about 20,000 G. In a recent paper G´ omez-del R´ıo et al. [2005] have tested dynamic tensile composites at law temperature using split Hopkinson pressure bar. The temperature is 20 and −60◦ C. The results of the dynamic tests showed little inﬂuence of temperature and strain rate on the tensile strength of a unidirectional laminate loaded in the ﬁber direction; in contrast, the strength increases appreciably in the transverse direction at low temperature and high strain rate. Regarding strain rate, a slight increase in tensile strength was observed under dynamic loading. In another paper M¨ uller et al.[2002] have a repetitive thermodynamics on viscoplastic body, since moulding plastic deformation is accompanied by heating. They have three such loadings. They show that the deformation in time, and temperature, is tending towards a single loading. In the paper by Tsai and Prakash [2005] is studied the normal plate impact experiments on 2-D layered material targets to understand the role of material architecture and material inelasticity in governing the elastic precursor decay and late-time wave dispersion. In order to understand the eﬀects of layer thickness and the distance of wave propagation on elastic precursor decay and latetime dispersion several targets with various layer and target thicknesses are employed. Moreover, in order to understand the eﬀects of material inelasticity both elastic-elastic and elastic-viscoelastic bilaminates are utilized. The results of the study indicate that the structure of acceleration waves is strongly inﬂuenced by impedance mismatch of the layers constituting the laminates, density of interfaces,

January 12, 2007

210

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Dynamic Plasticity

distance of wave propagation, and material inelasticity. The speed of elastic precursor is independent of the impedance mismatch of the individual laminae constituting the bilaminates and is equal to the average wave speed within the bilaminates. The speed of the late-time dispersion wave is observed to decrease with an increase in impedance mismatch; however, it is found to be independent of the density of interfaces, i.e., the number of layers in a given thickness laminate. The decay of the elastic precursor is observed to increase with an increase in impedance mismatch, the density of interfaces, and the distance of wave propagation. The rise-time of the late-time dispersion wave increases with an increase in impedance mismatch; however, it is observed to decrease with an increase in the density of interfaces. The frequency of oscillations of the late-time dispersive wave is observed to decrease with an increase in impedance mismatch; however, it is observed to increase with an increase in the density of interfaces. A model is presented by Ubachs et al. [2005] to describe the mechanical behavior of microstructure dependent materials. The model describes the microstructure evolution using a phase ﬁeld approach and employs a constitutive model dependent on the phase ﬁeld to account for the underlying microstructure. It has been demonstrated by applying it to eutectic tin-led solder, a material whose mechanical characteristics are strongly inﬂuenced by its continuously evolving microstructure. For the constitutive behavior the elasto-viscoplastic Perzyna model has been adopted. The Perzyna model allows the use of diﬀerent hardening functions, which makes it suitable for a large variety of materials. It is coupled to the phase ﬁeld model through the model parameters which are taken dependent on the mass fraction ﬁeld resulting from the solution of the phase ﬁeld equations. In this way the microstructure is accounted for using a continuum mechanics approach. Mixed-mode open-notch ﬂexure, anti-symmetric loaded end-notched ﬂexure and center-notched ﬂexure specimens were used to investigate dynamic mixed I/II mode delamination fracture using a fracturing split Hopkinson pressure bar by Wosu et al. [2005]. An expression for dynamic energy release rate is formulated and evaluated. The experimental results show that dynamic delamination increases linearly with mode mixing. In several papers by Krempl and Ho [2001], Ho and Krempl [2001], [2002] is developed a complicated theory based on overstress, to describe the rate sensitivities inside and outside the dynamic strain aging regime. The compressible and incompressible, isotropic, small strain viscoplasticity theory based on overstress is given. An experimental paper by Bourne [2006], is devoted to the plate impact to load in uniaxial strain and to show that a lower threshold exists for the propagation of fracture from the impact face. This is 4GPa in soda-lime glass. The velocity of impact is 1.5–2.5 km/s.

dynamic

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Rate Inﬂuence

dynamic

211

Bibliography Altenhof W. and Ames W., 2002, Strain rate eﬀects for aluminum and magnesium alloys in ﬁnite element simulations of steering wheel armature impact tests, Fatigue Fract. Engng. Mater. Struct. 25, 1149–1156. Alter B. E. K. and Curtis C. W., 1956, Eﬀect of strain rate on the propagation of a plastic strain pulse along a lead bar, J. Appl. Phys. 27, 1079–1085. Auricchio F., 1997, A viscoplastic constitutive equation bounded between two generalized plasticity models, Int. J. Plasticity 13, 8–9, 697–721. Baroncea A., Cristescu and Glodeanu E., 1977, A model for the description of the deformation of rocksalt, St. Cerc. Mec. Appl. 36, 1, 31–40 (in Roumanian). B´eda G., 1962a, Acta. Tech. Acad. Sci. Hung. 38, 161–187. Bell J. F., 1951, Propagation of plastic waves in prestressed bars, U.S. Navy Tech. Rep. No. 5, Baltimore, The Johns Hopkins University. Bell J. F., 1968, The phisics of large deformation of crystalline solids, Springer Tracts in Natural Philosophy, Vol. 14, Springer-Verlag, Berlin. Bell J. F., 1973, The experimental foundations of solid mechanics, in Hadbuch der Physik (ed. S. Flugge), Vol. Via/1, Springer-Verlag, Berlin. Bell J. F. and Stein A., 1962, The incremental loading wave in the pre-stressed plastic ﬁeld, J. M´ecan. 1, 4, 395–412. Bertholf L. D. and Karnes C. H., 1975, Two-dimensional analysis of the split Hopkinson pressure bar system, J. Mech. Phys. Solids 23, 1–19. Bingham E. C., 1922, Fluidity and Plasticity, McGraw-Hill, New York. Bodner S. R. and Partom Y., 1975, Constitutive equations for elasto-viscoplastic strainhardening materials, ASME J. Appl. Mech. 42, 385–389. Bourne N. K., 2006, On the impact and penetration of soda-lime glass, Int. J. Imp. Engineering (in press). Campbell J. D., 1970, Dynamic Plasticity of Metals, Springer Verlag, 92 pp. Campbell J. D., 1973, Dynamic plasticity-macroscopic and microscopic aspects, Materials Science and Engineering 12, 1, 3–21. Cernocky E. P., 1982, An examination of four viscoplastic constitutive theories in uniaxial monotonic loading, Int. J. Solids Structures 18, 11, 989–1005. Chaboche J. L., 1989, Constitutive equations for cyclic plasticity and cyclic viscoplasticity, Int. J. Plasticity 5, 247–302. Chang K. C., Sugiura K. and Lee G. C., 1989, Rate-dependent material model for structural steel, J. of Engeenering Mach. 115, 3, 465–474. Chau O., Fern´ andez-Garc´ıa J. R., Han W. and Sofonea M., 2002, A frictionless contact problem for elastic-viscoplastic materials with normal compliance and damage, Com. Met. Appl. Mech. Engi. 191, 44, 5007–5026. Chen W. W., Wu Q. P., Kang J. H. and Winfree N. A., 2001, Compressive superelastic behaviour of a NiTi shape memory alloy at strain rates of 0.001–750 s−1 , Int. J. Solids Struct. 38, 8989–8998. Chhabildas L. C. and Swegle J. W., 1989, Dynamic pressure-shear loading of using anisotropic crystals, J. Appl. Phys. 51, 9, 4799–4807. Colak O. U., 2004, A viscoplasticity theory appied to proportional and non proportional cyclic loading at small strains, Int. J. Plasticity 20, 1387–1401. Cristescu C. and Cristescu N. D., 1973, A numerical method to describe unloading in dynamic plasticity, 2nd Int. Conf. on “Structural Mechanics in Reactor Technology”, Berlin. L 4/8, 1–14.

January 12, 2007

212

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Dynamic Plasticity

Cristescu N. D., 1963, On the propagation of elastic-plastic waves in metallic rods, Bull. Acad. Polon. Sci. 11, 129–133. Cristescu N. D., 1964, Some problems in the mechanics of extensible strings, in: Kolsky H. and Prager W. (eds.), Symp. IUTAM Stress Waves in Anelastic Solids, Providence, 1963 (Springer Verlag, Berlin–G¨ ottingen–Heidelberg) 118–132. Cristescu N. D., 1966, About the propagation of elastic/plastic waves in thin rods, in: Dynamics of Mashines, Proc. Conf. Liblice-Praga, 1963, 87–96. Cristescu N. D., 1967, Dynamic Plasticity, North Holland Pub., Amsterdam. Cristescu N. D., 1972a, Rate-Type Constitutive Equations in Dynamic Plasticity, Noordhof International Publishing, Leyden, 287–310. Cristescu N. D., 1972b, A procedure for determining the constitutive equations for materials exhibiting both time-dependent and time-independent plasticity, Int. J. Solids Structures 8, 511–531. Cristescu N. D., 1977, Speed inﬂuence in wire drawing, Rev. Roumaine de M´ ecanique Appliqu´ee 22, 3, 391–399. Cristescu N. D. and Bell J. F., 1970, On unloading in the symmetrical impact of two aluminum bars, in: In Elastic Behaviour of Solids, Kannienen M. F., Adler W. F., Rosenﬁeld A. R. and Jaﬀee R. I. (eds.), McGraw Hill, New York, 397–421. Cristescu N. D. and Suliciu I., 1982, Viscoplasticity, Martinus Nijhoﬀ Pub.,307 pp. Curr` o C. and Valenti G., 1996, A linearization procedure for quasi-linear non homogeneous and non-autonomous ﬁrst-order systems, Int. J. Non-Linear Mechanics 31, 3, 377–386. Daimaruya M. and Naitoh M., 1983, On the existence of a strain plateau in the strain-rate dependent theory of Malvern for plastic wave propagation, J. Appl. Mech., Trans. ASME 50, 3, 678–679. Dally J. W. and Riley W. F., 1965, Experimental Stress Analysis, McGraw Hill, New York. Dawson T. H., 1972, On the applicability of one-dimensional non-viscous dynamic plasticity theory, Int. J. Mech. Sci. 14, 43–48. Dioh N. N., Leevers P. S. and Williams J. G., 1993, Thickness eﬀects in split Hopkinson pressure bar tests, Polymer 34, 20, 4230–4234. Dioh N. N., Ivankovic A., Leevers P. S. and Williams J. G., 1995, Stress wave propagation eﬀects in split Hopkinson pressure bar tests, Proc. Roy. Soc. London 449, 187–204. Drˇ agˇ anescu Gh. E. and Cˇ apˇ alnˇ aa¸san V., 2003, Nonlinear relaxation phenomena in polycristalline solids, Int. J. Nonlinear Sci. Num. Sci. 4, 219–225. Fˇ aciu C. and Mihailescu-Suliciu M., 1987, The energy in one-dimensional rate-type semilinear viscoelastcity, Int. J. Solids Sructures 23, 11, 1505–1520. Faciu C. and Simion N., 2000, Energy estimates and uniqueness of the weak solutions of initial-boundary value problems for semilinear hyperbolic systems, Z. Angev. Math. Phys. 51, 792–805. Fern´ andez J. R., Hild P. and Via˜ no J. M., 2003, Numerical approximation of the elasticviscoplastic contact problem with non-matching meshes, Numer. Math. 94, 501–522. Fern´ andez L. R., 2004, Numerical analysis of a contact problem between two elastic viscoplastic bodies with hardening and nonmatching meshes, Finite Elements in Analysis and Design 40, 771–791. Filbey G. L., 1961, Intensive Plastic Waves Ph.D. dissertation, The Johns Hopkins University, Baltimore. Forrestal M. J., Togami T. C., Baker W. E. and Frew D. J., 2003, Performance evaluation of accelerometers used for penetration experiments, Experimental Mechanics 43, 1, 90–96. Francis P. H. and Lindholm U. S., 1968, Eﬀect of temperature gradients on the propagation of elastoplastic waves, J. Appl. Mech. Trans. ASME 35, 3, 441–448.

dynamic

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Rate Inﬂuence

dynamic

213

Fusco D. and Manganaro N., 1994a, Riemann invariants-like solutions for a class of rate-type materials, Acta Mechanica 105, 23–32. Fusco D. and Manganaro N., 1994b, A method for determining exact solutions to a class of nonlinear models based on introduction of diﬀerential constrains, J. Math. Phys. 35, 7, 3659–3669. Fusco D. and Manganaro N., 1996, A method for ﬁnding exact solutions to hyperbolic systems of ﬁrst-order PDEs, IMA J. Appl. Math. 57, 3, 223–242. Gilman J. J., 1960, Physical nature of plastic ﬂow and fracture, in: Lee E. H. and Symonds P. S. (eds.), Plasticity, Proc. Second. Symp. on Naval Structural Mechanics, Providence, 1960 (Pergamon Press, New York–Oxford–London–Paris) 44–99. Goldsmith W., 2001, Impact, the Theory and Physical Behavior of Colliding Solids, Dover, N.Y. G´ omez-del R´ıo T., Barbero E., Zaera R. and Navarro C., 2005, Dynamic tensile behaviour at low temperature of CFRP using a split Hopkinson pressure bar, Composites Science and Technology 65, 61–71. Gupta Y. M., 1976, Shear measurements in shock-loaded solids, Appl. Phys. Lett. 29, 11, 694–697. Hauser F. E., Simmons J. A. and Dorn J. E., 1961, Strain rate eﬀects in plastic wave propagation, in: Shewmon P. G. and Zackay V. F. (eds.), Response of Metals to High Velocity Deformation, Proc. Conf. Colorado (Interscience Publ., New York, London) 93–110. Ho K. and Krempl E., 2001, The modeling of unusual rate sensitivities inside and outside the dynamic strain aging regime, Trans. ASME, J. Engng. Mat. Tech. 123, 28–35. Ho K. and Krempl E., 2002, Extension of the viscoplasticity theory based on overstress (VBO) to capture non-standard rate dependence in soils, Int. J. Plasticity 18, 851–872. Hu Y. and Feng R., 2004, On the use of a Kolsky torsion bar to study the transient largestrain response of polymer melts at high shear rates J. Appl. Mech. 71, 441–449. Ilyushin A. A. and Lenskii V. S., 1959, Strength of Materials, Fizmatghiz, Moscow (in Russian). Ionescu I. and Sofonea M., 1993, Functional and Numerical Methods in Viscoplasticity, Oxford University Press, Oxford, 265 pp. Khaleel M. A., Zbib H. M. and Nyberg E. A., 2001, Constitutive modeling of deformation and damage in superplastic materials, Int. J. Impact Engn. 17, 277–296. Klepaczko J. R., 1998, Remarks on impact shearing, J. Mech. Phis. Solids 46, 10, 2139–2153. Kojic M., 1996, The Governing Parameter Method for implicit integration of viscoplastic constitutive relations for isotropic and orthotropic metals, Computational Mechanics 19, 49–57. Kolsky H., 1949, An investigation of the mechanical properties of materials at very high rates of loading, Proc. Phys. Soc. B 62, 676–700. Krempl E., 1988, Phenomenological modeling of viscoplasticity, Revue Phys. Appl. Phisics Abstracts 23, 331–338. Krempl E., 1998, Creep-Plasticity Interaction. Lecture Notes. CISM No. 187, Udine, Italy, p. 74. Krempl E. and Ho K., 2001, Inelastic Compressible and Incompressible, Isotropic, Small Strain Viscoplasticity Theory Based on Overstress (VBO), Lemaitre Handbook of Materials Behaviour Models, Sec. 5.6, 336–348. Kuriyama S. and Kawata K., 1973, Propagation of stress wave with plastic deformation in metal obeying the constitutive equation of the Johnston–Gilman type, J. Appl. Phys. 44, 8, 3445–3454.

January 12, 2007

214

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Dynamic Plasticity

Lawson J. E. and Nicholas T., 1972, The dynamic mechanical behavior of titanium in shear, J. Mech. Phys. Solids 20, 65–76. Li C. H. and Clifton R. J., 1982, Dynamic stress–strain curves at plastic shear strain rate, in Shock Waves in Condensed Matter — 1981, Nellis W. J., Seaman L. and Graham R. A. (eds.), American Institute of Physics, New York, 360–366. Lodygowski T. and Perzyna P., 1997, Numerical modeling of localized fracture of inelastic solids in dynamic loading processes, Int. J. Numer. Meth. Engng. 40, 4137–4158. Lubarda V. A., Benson D. J. and Meyers M. A., 2003, Strain-rate eﬀects in rheological models of inelastic response, Int. J. Plasticity 19, 8, 1097–1118. ¨ Ludwik P., 1909, Uber den Einﬂuss der Deformationsgeschwindigkeit bei bleibenden Deformationen mit besonderer Ber¨ ucksichtigung der Nachwirkungserscheinungen, Physik. Zeitschrift 10, 411–417. Luo Y., Mori T., Li S. and Luo S., 2003, Isothermal rheological forming of high strength alloying part with complicated curved surface, Materials Sci. Forum 437 438, 337–340. Malvern L. E., 1951a, Plastic wave propagation in a bar of metal exhibiting a strain rate eﬀect, Quart. Appl. Math. 8, 4, 405–411. Malvern L. E., 1951b, The propagation of longitudinal waves of plastic deformation in a bar of material exhibiting a strain rate eﬀect, J. Appl. Mech. 18, 2, 203–208. Manganaro N. and Valenti G., 1993, Group analysis and linearization procedure for a nonautonomous model describing rate-type materials, J. Math. Phys. 34, 4, 1360–1369. Manganaro N. and Meleshko S., 2002, Reduction procedure and generalized simple waves for systhems written in Riemann variables, Nonlinear Dynamics, 30, 87–102. Maranini E. and Yamaguchi T., 2001, A non-associated viscoplastic model for the behavior of granite in triaxial compression, Mech. of Mater. 33, 5, 283–293. Matos C. G. and Dodds R. H. Jr., 2002, Probabilistic modeling of weld fracture in steel frame connections Part II: seismic loading, Engineering Structures 24, 687–705. Mihailescu-Suliciu M. and Suliciu I., 1987, On tensile shock waves in rubber-like materials, J. Appl. Mech. 54, 498–502. Minnaar K. and Zhou M., 2004, A novel technique for time-resolved detection and tracking of interfacial and matrix fracture in layered materials, J. Mech. Phys. Solids 52, 2771–2799. Mortell M. and Seymour B. R., 1973, Pulse propagation in nonlinear viscoelastic rod of ﬁnite length, SIAM J. Appl. Math. 22, 2, 209–224. M¨ uller I., Sahota H.-S. and Villaggio P., 2002, On the thermodynamics of repetitive visco-plastic moulding, Z. Angew. Math. Phys. 53, 1139–1149. Nemat-Nasser S., Isaacs J. B. and Starrett J. E., 1991, Hopkinson techniques for dynamic recovery experiments, Proc. R. Soc. Lond. A 435, 371–391. Nemat-Nasser S., Choi J. Y., Guo W. G. and Isaacs J. B., 2005, Very high strain-rate response of a NiTi shape-memory alloy, Mechanics of Materials 37, 287–289. Nemat-Nasser S. and Guo W. G., 2005, Thermomechanical response of HSLA-65 steel plates: experiments and modeling, Mechanics of Materials 37, 379–405. Nicholas T., 1981, Tensile testing of materials at high rates of strain, Experimental Mechanics 21, 5, 177–185. Nicholas T., Rajendran A. M. and Grove D. J., 1987a, Analytical modeling of precursor decay in strain-rate dependent materials, Int. J. Solids Struct. 12, 1601–1614. Nicholas T., Rajendran A. M. and Grove D. J., 1987b, An oﬀset yield criterion from precursor decay analysis, Acta Mechanica 69, 1–4, 205–218.

dynamic

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Rate Inﬂuence

dynamic

215

Nicholson D. W. and Phillips A., 1978, On the impact end in logitudinal dynamic plastic wave propagation, Acta Mechanica 29, 75–92. Ostoja-Starzewski M., 1995, Wavefront propagation in a class of random microstructuresII, Non-linear elastic grains, Int. J. Non-Linear Mechanics 30, 6, 771–781. Pao Y. H. and Gilat A., 1989, Modeling 1100-0 aluminum over a wide range of temperatures and strain rates, Int. J. Plasticity 5, 183–196. Perzina P., 1963, The study of the dynamical behaviour of rate sensitive plastic materials, Arch. Mech. Stos. 15, 113–130. Ponomarev S. D., Biderman V. L., Likharev K. K., Makushin V. M., Malinin N. N. and Feodos’ev V. I., 1956, Resistance calculus in construction of machines, Mashigiz Moscow, Tom III, 553–580 (in Russian). Prandtl L., 1928, Ein Gedankenmodell zur kinematischen Theorie der festen K¨orper, Z. Angew. Math. Mech. 8, 85–106. Schmidt M. L. and Ross C. A., 1999, Shear strength of concrete under dynamic loads, ASME Pressure Vessel and Piping Conf. Boston, MS, August 1999. Shaw R. P. and Cozzarelli F. A., 1971, Wave-front stress relaxation in a one dimensional nonlinear inelastic material with temperature and position dependent properties, J. Appl. Mech. 38, 1, 47–50. Sofonea M., 1997, On a contact problem for elastic-viscoplastic bodies, Nonlinear Analysis, Theory, Methods & Applications 29, 9, 1037–1050. Sokolovskii V. V., 1948a, Propagation of elastic-visco-plastic waves in bars, Docl. Akad. Nauk SSSR 60, 5, 775–778 (in Russian). Sokolovskii V. V., 1948b, Propagation of elastic-visco-plastic waves in bars, Pricl. Mat. Meh. 12, 3, 261–280 (in Russian). Stoﬀel M., 2004, Evolution of plastic zones in dynamically loaded plates using diﬀerent elastic-viscoplastic laws, Int. J. Solids and Structures 41, 6813–6830. Stoﬀel M., 2005, Sensitivity of simultaneous depending on material parameter variations, Mech. Res. Com. 32, 332–336. Suliciu I., 1966, private comunication. Suliciu I., 1972, Additional coments on Suliciu, Malvern and Cristescu’s paper. “Remarks concerning the “plateau” in dynamic plasticity”, Archives of Mechanics 27, 4, 665–667. Suliciu I., 1974, Classes of discontinuous motions in elastic and rate-type materials, Arch. Mech. Stos. 26, 4, 675–699. Suliciu I., 1981, On the Savart–Masson eﬀect, J. Appl. Mech. Trans. ASME 48, 426–428. Suliciu I., Lee S. Y. and Ames W. F., 1973, Nonlinear traveling waves for a class of rate-type materials, J. Math. Anal. Appl. 42, 2, 313–322. Sundaram S. and Clifton R. J., 1998, The inﬂuence of a glassy phase on the high strain rate response of a ceramic, Mechanics of Materials 29, 233–251. S¨ ut¸cu ¨ M. and Krempel E., 1989, A stability analysis of the uniaxial viscoplasticity theory based on overstress, Computational Mechanics 4, 401–408. Tabov I., 1996, Riemann invariants for a class of partial diﬀerential systems, Diﬀerential Equations 32, 11, 1550–1553. Tanaka E., 1994, A nonproportionality parameter and a cyclic viscoplastic constitutive model taking into account amplitude dependencies and memory eﬀects of isotropic harden, European J. of Mechanics 13, 2, 155–173. Tanimoto N., 1994, One-dimensional propagation speed of an elastic-plastic viscoplastic stress wave, Nuclear Eng. and Design 150, 2–3, 275–280. Tanimoto N., Fukuoka H. and Fujita K., 1993, One-dimensional numerical analysis of a bar subjected to longitudinal impulsive loading, ISME International Journal, Series A, 36, 2, 137–145.

January 12, 2007

216

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Dynamic Plasticity

Tanimura S., 1979, A practical constitutive equation covering a wide range of strain rates, Int. J. Eng. Sci. 17, 997–1004. Thomsen E. G., Yang C. T. and Kobayashi S., 1968, Mechanics of Plastic Deformation in Metal Processing, Macmillan Co., London. Ting T. C. T. and Symonds P. S., 1964, Longitudinal impact on visco-plastic rods linear stress–strain rate law, J. Appl. Mech. 31, Ser. E, 199–207. Tsai L. and Prakash V., 2005, Structure of weak shock waves in 2-D layered material systems, Int. J. Solids Struct. 42, 724–750. Ubachs R. L. J. M., Schreurs P. J. G. and Geers M. G. D., 2005, Phase ﬁeld dependent viscoplastic behaviour of solder alloys, Int. J. Solids Sructures 42, 2533–2558. Uenishi A. and Teodosiu C., 2004, Constitutive modeling of the high strain rate behaviour of interstitial-free steel, Int. J. Plasticity 20, 915–936. Valanis K. C., 1972, Irreversible thermodinamics of continuous media, Internal Variable Theory, CISM Courses and Lectures No. 77, International Centre for Mechanical Sciences, Springer, Wien. Vyalov S. S., 1978, Rheological foundations for soil mechanics, Vysh. Shkola, Moscow (in Russian). Wosu S. N., Hui D. and Dutta P. K., 2005, Dynamic mixed-mode I/II delamination fracture and energy release rate of unidirectional graphite/epoxy composites, Eng. Fracture Mech. 72, 1531–1558. Yokoyama T., 2001, Finite element computation of torsional plastic waves in a thin walled tube, Archive of Applied Mechanics 71, 6–7, 359–370. Zhao H., 1997, A study of specimen thickness eﬀects in the impact tests on polymers by numeric simulations, Polymer 39, 5, 1103–1106. Zhao H., 2003, Material behaviour characterization using SHPB techniques, tests and simulations, Computers & Structures 81, 12, 1301–1310. Zhao H. and Gary G., 1996, On the use of SHPB techniques to determine the dynamic behavior of materials in the range of small strains, Int. J. Solids Structures 33, 23, 3363–3375. Ziegler F., 1992, Developments in structural dynamic viscoplasticity including ductile damage, ZAMM 72, 4, T5–T15.

dynamic

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

Chapter 5

Mechanics of Extensible Strings

5.1

Introduction

The problem was considered for a long time. But generally only static problems or problems involving nearly quasi static conditions were studied (various cables existing in applications). Rubber cables or synthetic strings are elongating very much when impacted, even with quite small forces. But in some modern textile machines the speed of operation is quite high (knitting, weaving, sewing, carding machines). Also in elastic cables used to break airplanes on ships, the speed is quite high. In dynamic problems the cables are inﬂuenced what concerns the yield limit, the work-hardening modulus, the breaking stress and the elastic modulus. Impact velocities of the order of some hundred meters per second or even a few kilometers per second, when the component of the impact velocity ranges between the velocities of propagation of transverse and longitudinal waves, occur less often in practice and lead to diﬃcult mathematical problems, as will be pointed out below. One must also take into account that textile materials cannot resist transverse impacts if the latter exceed a certain limit; for each textile yarn there is a certain limiting transverse impact velocity which at once breaks the string at the point of impact. These limiting velocities, generally, of the order of many hundred meters per second. From the mechanical point of view, that is the simplest problem in which two kind of waves propagate and reﬂect together, inﬂuencing one another at every moment. This motion can be studied both experimentally and theoretically, because both kinds of wave can be observed experimentally during their propagation. The problem can be studied experimentally very well, for the two waves propagating and inﬂuencing each other. On the other hand, the mechanics of strings closely resembles many other problems of dynamic plasticity from the mechanical and mathematical points of view. We are not giving here a complete literature. The beginning of the literature is given in Cristescu [1967]. Some other papers are mentioned in the exposure. The equations of motion of a string in plane motion are written by Rakhmatulin 217

dynamic

January 12, 2007

10:41

218

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Dynamic Plasticity

Fig. 5.1.1

Typical conﬁguration of a yarn specimen after transverse impact.

and Shapiro [1955] in order to determine the dynamic relation between stress and strain for strings. The impact of strings by punctual bodies of ﬁnite mass, when the velocity of impact is variable, was studied by Rakhmatulin [1951] and Riabova [1953], and by some other authors. In the paper by Smith et al. [1956] a textile yarn segment about half a meter long is clamped at each end and impacted transversely at midpoint with a velocity of about 70 m/sec. The stress–strain curve for this yarn is obtained by measuring a high speed photographic record of the motion of the yarn. A typical conﬁguration of the yarn specimen after transverse impact is indicated in Fig. 5.1.1. It is assumed that the transverse waves always propagate more slowly and in fact are reduced to a single shock wave which modiﬁes the shape of the yarn. By measuring the lengths deﬁned in Fig. 5.1.1 on the frames of the photograph record, the average strain as deﬁned by L1 + L2 − L ε¯ = L is used. This manner of deﬁning strain as an average strain, in the presence of wave propagation, is certainly a restrictive one. By measuring also the velocity of propagation of the transverse wave, dynamic stress–strain curves are obtained for high-tenacity nylon, fortisan, and ﬁberglass. The stress–strain curves for nylon obtained by Smith et al. [1956] are reproduced in Fig. 5.1.2 for various strain rate. The important conclusion is that for such materials the increasing rate of strain tends to steepen the slope of the stress–strain curve at the origin. A theory of these phenomena, assuming the yarn to be inﬁnitely long, has been developed by Smith et al. [1958], and Smith et al. [1960]. The velocities of impact range between 1400 m/sec for undrawn nylon to 5000 m/sec for high tenacity rayon and glass-ﬁber. In Fig. 5.1.3 is given the stress–strain curves for acetate yarns as obtained by Smith et al. [1961]. All these yarns show an appreciable rate inﬂuence. The most strongly

dynamic

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Mechanics of Extensible Strings

Fig. 5.1.2

Fig. 5.1.3

Stress–strain curves for Nylon.

Stress–strain curves for braided silk.

dynamic

219

January 12, 2007

220

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Dynamic Plasticity

Fig. 5.1.4 Stress–strain curves for kapron for the following strain rates: (1) 1.2 × 10−3 sec−1 , (2) 1.2 × (10−2 sec−1 , 3) 1.2 × 10−1 sec−1 , (4) (280 sec−1 .

inﬂuenced factor is the yield stress, but generally the whole stress–strain curve is rate dependent. Another experimental technique that of impacting yarns with riﬂe bullets, was developed by Smith et al. [1963]. The transverse velocity of impact is now bigger: up to 700 m/sec. The eﬀect of air drag on the motion of yarn is also analyzed by Smith et al. [1964]. In another paper Fenstermaker and Smith [1965] have described experiments in which transversely impacted ﬁlaments are observed by ﬂash photography. Polyester yarns are used. The strain distribution is obtained at various times after impact and at various impact velocities. These experiments revealed important time eﬀects (creep and relaxation eﬀects) within 50 sec after impact. See also the papers of Smith and Fenstermaker [1967], Smith et al. [1965]. Longitudinal impact with a bullet were performed by Lewis [1957]; the velocity of the bullet is 170 m/sec. Similar experiments are reported by Victorov et al. [1966] for kapron and other yarns, tested at room temperature for rate of strain ranging between 10−3 and 102 sec−1 . An increase of the rate of strain raises the stress–strain curve appreciably.

dynamic

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Mechanics of Extensible Strings

dynamic

221

Some other authors have also reported results on transverse impact of yarns by bullets. But impact grater than 460 m/sec produce a sudden rupture of the yarn and generally all yarns are strongly rate dependent.

5.2

Equations of Motion

In order to obtain the equations of motion (Cristescu [1967]) of an extensible string moving in three-dimensional space, we use a curvilinear coordinate s taken along the string and starting from an arbitrary coordinate origin. This Eulerian coordinate is sometimes called the “laboratory” coordinate or the “actual” coordinate, corresponding to the deformed string at the actual moment t. The tension or total force in the string is denoted by T. It is a variable factor, both along the string and in time. In extensible, perfectly ﬂexible strings, the tension in every point is always directed along the tangent to the string, which will be represented below as a line. Consider a portion of the string comprised between the curvilinear coordinates s1 and s2 (Fig. 5.2.1). This portion of the string will be subjected now only to the tension, but possibly also, to various external forces (X, Y, Z), which are proportional to the length of the portion of the string considered. For this portion we can write " " s2 s2 ∂x "" ∂2x ∂x "" − T + Xds = ρ ds T ∂s "s2 ∂s "s1 ∂t2 s1 s1 and two similar equations for y and z. Here ρ is the density of the string, which is function of the two variables s and t. The projection of T on the three considered axes are T (∂x/∂s), T (∂y/∂s) and T (∂z/∂s), T being the modulus of T. The previous equation can be written in the form

Fig. 5.2.1

Element of a string.

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

222

dynamic

Dynamic Plasticity

s2

s1

∂ ∂s

∂x ∂2x T + X − ρ 2 ds = 0 ∂s ∂t

or taking into account that s1 and s2 are arbitrary ∂x ∂2x ∂ T +X =ρ 2 , ∂s ∂s ∂t

(5.2.1)

and two similar equations for y and z. It is easy to replace the curvilinear coordinate s by a Lagrangean coordinate s0 . The unknown function x, y, z will depend on the variable s0 through the intermediary of s, and also on the time t: x(s(s0 ), t) etc. Thus for a ﬁxed value of t, the formulae ∂x ∂x ds = , etc. ∂s0 ∂s ds0 will apply. The strain of the string is deﬁned by 2 2 2 ∂x ∂y ∂z ds − ds0 = + + −1. ε= ds0 ∂s0 ∂s0 ∂s0

(5.2.2)

(5.2.3)

The last expression is obtained using the formulae (5.2.2). Thus these formulae can be written ∂x ∂x , = (1 + ε) ∂s0 ∂s

∂y ∂y , = (1 + ε) ∂s0 ∂s

∂z ∂z . = (1 + ε) ∂s0 ∂s

(5.2.4)

From the law of conservation of mass, it follows that ρ ds = ρ0 ds0 where ρ0 is the density of the string in the initial non-deformed state. Thus, the relation between the actual density ρ and the initial one ρ0 is ρ0 = ρ(1 + ε) .

(5.2.5)

Taking into account the relation ds = (1 + ε) ds0

(5.2.6)

as well as (5.2.4) and (5.2.5), the equations of motion (5.2.1) can be written as ∂2x T ∂x ∂ − ρ0 2 + (1 + ε)X = 0 (5.2.7) ∂s0 1 + ε ∂s0 ∂t with two similar equations for y and z. To these equations must be added the constitutive equation.

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

Mechanics of Extensible Strings

5.3

dynamic

223

The Finite Constitutive Equation: Basic Formulae

The constitutive equation used most in dynamic problems is the ﬁnite constitutive equation, of the form T = T (ε) .

(5.3.1)

This function is generally a monotonic (sometimes strictly monotonic) increasing function. Taking into account (5.3.1) together with the system (5.2.7) and the relation obtained from (5.2.3) by diﬀerentiating with respect to s0 , we obtain xs0

∂xs0 ∂ys0 ∂zs0 ∂ε + ys0 + zs0 − (1 + ε) = 0, ∂s0 ∂s0 ∂s0 ∂s0

T ∂xs0 ∂xt (1 + ε)dT /dε − T ∂ε + xs0 − ρ0 + (1 + ε)X = 0 , 1 + ε ∂s0 ∂t (1 + ε)2 ∂s0

(5.3.2)

with two similar relations for y and z. For the sake of simplicity the notations xs0 = ∂x/∂s0 , xt = ∂x/∂t, etc. has been used. In order to ﬁnd the type of the system, let us ﬁnd the type of the characteristic lines. For this purpose, the relations dxs0 =

∂xs0 ∂xs0 dt , ds0 + ∂s0 ∂t

dxt =

∂xt ∂xt dt , ds0 + ∂s0 ∂t

(5.3.3)

and similar ones for y and z, will be combined with (5.3.2). The system (5.3.2) contains four equations with four unknown functions x, y, z, and ε, and two independent variables s0 and t. It is clear that the strain ε can be eliminated using (5.2.3). However, to facilitate subsequent mechanical interpretation it is more advantageous to retain ε as an unknown function. The ten relations (5.3.2), (5.3.3) contain ten derivatives of the form ∂xs0 /∂s, ∂xs0 /∂t, etc. By solving with respect to these derivatives we obtain ∂ε ξxs0 + ηys0 + ζzs0 , = ∂s0 (1 + ε)[ρ0 (ds0 /dt)2 − dT /dε] ∂xs0 (1 + ε)3 [dT /dε − ρ0 (ds0 /dt)2 ]ξ =− ∂s0 (1 + ε)3 [ρ0 (ds0 /dt)2 − T /(1 + ε)][ρ0 (ds0 /dt)2 − dT /dε] +

(5.3.4)

xs0 [(1 + ε)dT /dε − T ](ξxs0 + ηys0 + ζzs0 ) , (1 + ε)3 [ρ0 (ds/dt)2 − T /(1 + ε)][ρ0 (ds0 /dt)2 − dT /dε]

and similar expressions for the other second order derivatives which occur in (5.3.2). In (5.3.4) the notations

January 12, 2007

224

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

dynamic

Dynamic Plasticity

ds0 1 − dxt + (1 + ε)X , ξ = ρ0 dxs0 dt dt ds0 1 η = ρ0 dys0 − dyt + (1 + ε)Y , dt dt ds0 1 ζ = ρ0 dzs0 − dzt + (1 + ε)Z dt dt

(5.3.5)

have been used. From (5.3.4) it follows (Cristescu [1954]) that the system (5.3.2) is totally hyperbolic since it has four distinct families of characteristic curves. Two of them are deﬁned by the diﬀerential relations 1/2 ds0 T =± , (5.3.6) dt ρ0 (1 + ε) while the other two by the relations 1/2 ds0 1 dT =± . (5.3.7) dt ρ0 dε Thus all the characteristic lines are generally curved lines whose slope depends on T and ε. From the mechanical point of view, the characteristics lines represent wave fronts. There will be two kinds of waves: the characteristic lines (5.3.6) represent wave fronts which propagate with the velocity 1/2 T , (5.3.8) cI (ε) = ρ0 (1 + ε) while the characteristic lines (5.3.7) represent wave fronts which propagate with a velocity 1/2 1 dT . (5.3.9) cII (ε) = ρ0 dε If (5.3.6) is taken into account, it follows from (5.3.4) (Cristescu [1960, 1961]) that the following diﬀerential relations 1 xs0 (±cI (ε) dε − dv) , dxt = ±cI (ε) dxs0 + [(1 + ε)X − xs0 F ] dt − ρ0 1+ε (5.3.10) and four similar relations for y and z, are satisﬁed on these lines. Along the characteristics (5.3.7) are satisﬁed the diﬀerential relations 1+ε F dt = 0 . (5.3.11) ±cII (ε) dε − dv + ρ0 Here the notations 1 (xs dxt + ys0 dyt + zs0 dzt ) , dv = 1+ε 0 (5.3.12) 1 (Xxs0 + Y ys0 + Zzs0 ) F = 1+ε

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Mechanics of Extensible Strings

dynamic

225

have been used, where v is the projection on the tangent to the string of the velocity of the corresponding particle of the string. The diﬀerential dv is computed along a non-speciﬁed characteristic line. F is the projection on the tangent to the string of the external forces which act on the portion of the string considered, of unit length. The upper and lower signs in (5.3.6) and (5.3.10) and in (5.3.7) and (5.3.11) correspond to each other. Let us write the “jump conditions”, by denoting by [A] the jump of the function A across a characteristic line. Writing the relations (5.3.3) for either side of a characteristic line, and taking into account that the diﬀerentials dxs0 , dxt , etc. are computed along a characteristic line and are in fact “interior derivatives” which are continuous across such a line, we obtain for the kinematics compatibility conditions: ∂xs0 ds0 ∂xs ∂xt ds0 ∂xt + = 0, + =0 (5.3.13) ∂s0 dt ∂t ∂s0 dt ∂t with four similar relations for y and z. In (5.3.13) the rate ds0 /dt must be replaced by one of the two expressions given by (5.3.6) or (5.3.7), depending of the characteristic line considered. If the equations of motion (5.3.2) are written for either side of a characteristic line and the diﬀerence is taken, and if (5.3.13) is also taken into account, we obtain ∂xs0 ∂ys0 ∂zs0 ∂ε + ys0 + zs0 − (1 + ε) = 0, xs0 ∂s0 ∂s0 ∂s0 ∂s0 (5.3.14) 2 & T ∂xs0 ds0 (1 + ε)dT /dε − T ∂ε − ρ0 + = 0, xs0 1+ε dt ∂s0 (1 + ε)2 ∂s0 with two other relations for y and z. These are the dynamic compatibility equations (Cristescu [1954]). In order to see what happens on each characteristic line, we combine (5.3.6) and (5.3.14), to get ∂xs0 ∂ys0 ∂zs0 ∂ε + ys0 + zs0 = 0 and = 0. (5.3.15) xs0 ∂s0 ∂s0 ∂s0 ∂s0 Similarly, from (5.3.7) and (5.3.14) [taking into account also (5.2.2) and (5.2.3)] we obtain: ∂xs0 /∂s0 ∂ys0 /∂s0 ∂zs0 /∂s0 ∂ε . (5.3.16) = = = xs ys zs ∂s0 From (5.3.15) follows that the waves which propagate with the velocity (5.3.8) are transverse waves which aﬀect only the shape of the string but do not aﬀect the longitudinal strain (because [∂ε/∂s0 ] = 0). The waves which propagate with the velocity (5.3.9) are longitudinal waves which produce only propagable elongations of the string, but do not change its shape. The jumps [∂xs0 /∂s0 ], etc. of the second derivatives of the coordinates are simply the projections on the coordinate axes of the discontinuity of ∂ε/∂s0; the relation

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

226

dynamic

Dynamic Plasticity

∂xs0 ∂s0

2

+

∂ys0 ∂s0

2

+

∂zs0 ∂s0

2

=

∂ε ∂s0

2

is also satisﬁed. Thus the projection of the discontinuity on the tangent to the string will propagate through longitudinal waves while the orthogonal component of this discontinuity will propagate through transverse waves. Both types of waves inﬂuence one another. The equation of motion of strings considered to be made of a phase-transforming material like a shape-memory alloy, was done by Purohit and Bhattacharya [2003]. They study the phase boundaries, the driving force acting on them and the kinetic relation governing their propagation. The paper presents also a numerical method for studying general initial and boundary value problems in strings. 5.4

The Order of Propagation of Waves

The order of propagation depends on the initial and boundary conditions, as well on the constitutive equation. Suppose that, at the end of the string, the strain increases monotonically and that at each moment of time both types of waves are generated. The order of propagation of waves in the string will be examined for a material whose constitutive equation is represented in Fig. 5.4.1 (Cristescu [1954, 1958]). Such constitutive equation does not correspond to any speciﬁc material and has been selected only by way of example. From (5.3.8) and (5.3.9) it follows that cI < cII for those tension and strain states which are represented by points on the segments OA or BC. In this case the transverse waves propagate more slowly than the longitudinal ones. On the segments AB and CD the inequality cI > cII holds and in this case the transverse waves propagate faster than the longitudinal waves. Finally there are certain points A, B, C on the diagram, and sometimes even certain segments on this diagram, where the diﬀerential relation (1 + ε)

dT =T dε

(5.4.1)

is satisﬁed. In these points, or portions of the diagram, cI = cII and hence both waves generated at the end of the string propagate with the same velocity. The relation (5.4.1) is satisﬁed over an entire portion of the tension–strain diagram for synthetic strings (Miklowitz [1947], Marshall and Thomson [1954]). Generally cI = cII and we will consider this case. If the slope of the diagram is zero in some portions (for example A B ) then for the corresponding states of tension and strain the propagation of longitudinal waves is no longer possible, and cII = 0. If at a certain moment, the tension at the end of the string begins to increase once more (for instance starting at the point

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Mechanics of Extensible Strings

dynamic

227

Fig. 5.4.1 Typical tension–strain curve. At points A, B, C the velocities of propagation of transverse and longitudinal waves are equal.

B ) the longitudinal waves can propagate again. The case when the longitudinal waves propagate ﬁrst and the transverse ones (which do not produce elongations) later, is the simplest case and has bee studied by many authors (see Rahmatulin and Demianov [1961]). All these authors considered strings which were initially rectilinear and in which the two types of waves propagate successively in distinct portions of the string. 5.5

Boundary and Initial Conditions

We shell now formulate the boundary and initial conditions for a general threedimensional motion of the extensible string (Cristescu [1964]). One can formulate the boundary conditions for ﬁxed or moving points of the string. For instance in problems concerning the impact of strings by moving bodies, the body which strikes the string can contact the same material point of the string permanently or can move along it (ﬂoating boundary). Thus both stationary and moving boundaries have to be considered. The initial conditions can also be formulated in various manners. In the case of a Cauchy problem, for t = 0 and 0 ≤ s0 ≤ l the following functions must be prescribed ε(s0 , 0), v(s0 , 0), x(s0 , 0), . . . , xs0 (s0 , 0), . . . , xt (s0 , 0), . . . ,

(5.5.1)

where l is the initial length of the string. Thus, at the initial moment, the position of the string, the velocity of each of its points, and the strain distribution along the string must be known. It is assumed that the functions (5.5.1) possess continuous ﬁrst order derivatives. In this case (Courant [1962] Ch. V), within a certain band

January 12, 2007

228

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

dynamic

Dynamic Plasticity

0 ≤ t ≤ h, the system (5.3.2) possesses a unique solution with continuous derivatives, provided that h is suﬃciently small and the coeﬃcients in (5.3.2) as well as the data are Lipschitz-continuous. The solution can be further extended for t > h as long as the continuity conditions, which must be satisﬁed by the coeﬃcients, hold. Not all the functions in (5.5.1) can be prescribed arbitrarily since these functions must satisfy certain compatibility conditions, the equations given in the previous paragraphs. If the boundary conditions always aﬀect the same material points of the string (stationary boundaries) the boundary conditions have to be prescribed in the s0 Ot plane along the straight lines s0 = 0 and s0 = l. If the bodies which strike the string, or move its ends, move along the string, then the boundary conditions must be prescribed along ﬂoating boundaries. Such a problems arises for instance, if a string is wrapped around a bobbin. Another example is the safety cables used in the Saturn V rockets which have sent people to the Moon. It is known that in this case, in order to avoid the danger of ﬁre, a cable was attached to the rocket, close to the top (about 100 m), and the other end was attached to a pole on the ground. On this cable was attached a cable, isolated against ﬁre. When testing the system, one has observed that when the cage was going down, that the cable is almost able to wrap up around the pulley. In other words, when going down, the pulley was approaching the velocity of the transverse waves traveling in the cable. In all those cases the motion along the string of the impacting body is smaller than the velocity of propagation of the transverse cI or longitudinal waves. Thus, in most cases, a mixed boundary problem must be solved. If the striking body moves along the string with a velocity higher than cII or cI then certain discontinuities of the shape or of the strain of the string propagate, and these would soon produce an entanglement or rupture of the string. The elastic string. If the string is elastic, the constitutive equation (5.3.1) becomes T = Eε ,

(5.5.2)

where E is an elastic constant. The velocities of propagation of the two waves are (Cristescu [1951]) 1/2 1/2 Eε E cI (ε) = and cII = . (5.5.3) ρ0 (1 + ε) ρ0 Thus, the longitudinal waves propagate with a constant velocity. The equality (5.4.1) is impossible and hence the two waves always propagate with distinct velocities. For each ε, cII > cI (ε). The linear work-hardening string. In this case the constitutive equation (5.3.1) consists of two relations T = Eε if T ≤ TY , (5.5.4) T = TY + E1 (ε − εY ) if T ≥ TY ,

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

Mechanics of Extensible Strings

dynamic

229

where TY is the yield tension of the material considered and E1 is the constant workhardening modulus. If the tension does not exceeds the yield tension the situation coincides with that described above. If T > TY the velocities of propagation become 1/2 1/2 TY + E1 (ε − εY ) E1 cI (ε) = and cII = . (5.5.5) ρ0 (1 + ε) ρ0 It should be noted that in the neighborhood of the yield point, the velocity cI varies continuously with ε, while cII suﬀers a jump from cII = (E/ρ0 )1/2 for T < TY , to cII = (E1 /ρ0 )1/2 for T > TY . Generally cII is smaller in the plastic domain than in the elastic one and is a constant throughout this ﬁrst domain. Depending on the sizes of E1 and TY , three possibilities arise E1

TY 1 + εY

and cII > cI .

(5.5.6)

All of these possibilities are encountered in practice. The last of them leads to certain diﬃculties since, in this case, longitudinal shock waves can appear. The second case has already been discussed above; it corresponds to the case when both types of waves propagate with the same velocity, when the characteristic curves (5.3.6) and (5.3.7) coincide and the last three equations of the system (5.3.2) reduce to ∂xs0 ∂xt + (1 + ε)X = 0 , − ρ0 E1 ∂s0 ∂t with similar equations for y and z. Through the intermediary of ε, this system of equations becomes a system of three partially coupled diﬀerential equations. If external forces are absent the three equations are no longer partially coupled and each of them can be integrated separately. Inextensible strings. Another possible case is that of a string which has suﬀered a former deformation. The strain is then generally distributed non-homogeneously along the string but remains constant in time in each section of the string. In this case the system (5.3.2) reduces to three semi-linear non-coupled equations Φ(s0 )

∂2x ∂2x ∂x dΦ(s0 ) − ρ + + (1 + ε(s0 ))X(s0 , t) = 0 , 0 2 2 ∂s0 ∂t ∂s0 ds0

with two similar ones for y and z. Here Φ(s0 ) = T (ε)/(1 + ε) is a known function of s0 . The integration of such equations do not entail special diﬃculties. If the strain is uniformly distributed along the string ε = const., and the equation reduces to an equation with constant coeﬃcients

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

230

Dynamic Plasticity

c2I

∂2x ∂2x 1 + ε − 2 + X(s0 , t) = 0 , ∂s20 ∂t ρ0

with two others for y and z. Here cI and ε are constants. The string behaves as an inextensible string which may possibly undergo appreciable transverse motions. 5.6

Numerical Examples

The numerical examples are obtained with integration along the four characteristic lines. Details are given in Cristescu [1967] and will not be given here. Examples are given for semi-inﬁnite string, for ﬁnite string, for ﬁnite elastic string. For the extensible cable used to break high speed moving bodies when at the impacted end we have M dV = ATdt where V is the velocity of the body, A is the area of the transverse section of the string and T is the stress at the end of the string (see Fig. 5.6.1):

Fig. 5.6.1

Impact of a rectilinear cable with a fast moving body.

The shape of the cable is shown in Fig. 5.6.2. Were given also vertical velocity, horizontal velocity, strain distribution, longitudinal velocity, and variation of strain along the ﬁrst transverse wave front and the length of the cable at various times.

Fig. 5.6.2

Shape of the cable at various times.

dynamic

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

Mechanics of Extensible Strings

dynamic

231

Fig. 5.6.3 Motion of two bodies connected by an extensible cable; Schematic representation of two positions of the system.

Fig. 5.6.4

Successive positions of the system for the case M ∗ = 2M .

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

232

dynamic

Dynamic Plasticity

The motion of two bodies connected by an extensible cable was also considered. The mass of the two bodies were M ∗ = 2M or 2M ∗ = M (Fig. 5.6.3). The successive positions of the system for the case M ∗ = 2M are given in Fig. 5.6.4. Were also given the strain proﬁle at various time, the characteristic ﬁeld showing the propagation of the ﬁrst longitudinal and the ﬁrst transverse wave fronts in the cable and several reﬂections from the two ends of the cable, the equalization of the vertical velocities of the two bodies, the strain proﬁles at various times and the variation of the length of the cable. 5.7

Rate Inﬂuence

Finite constitutive equations cannot be used to describe the mechanical properties of synthetic strings for which the rate inﬂuence is very large. Thus, in many cases, various classes of diﬀerential constitutive equations, which can be applied to different kinds of materials, must be considered. Some such diﬀerential constitutive equations will be analyzed below in connection with the problem of rapid motion of extensible strings (Cristescu [1965]). The ﬁrst constitutive equation which will be considered is that which is quasilinear both in the rate of strain and in the rate of tension: ∂T ∂ε = g(T, ε) + f (T, ε) , (5.7.1) ∂t ∂t where the functions f and g may possibly depend explicitly on s0 , t, as well as on various characteristic constants (yield tension, etc.). The function g(T, ε) describes the instantaneous response properties of the material, at a certain increment of the tension, while the function f (T, ε) describes the non-instantaneous response properties. Relations of the type (5.7.1) can be used both for loading processes and for non-linear unloading processes. Various special cases of the relation (5.7.1) will be considered below. The constitutive equation must be supplemented by the equations xs0

∂xs0 ∂ys0 ∂zs0 ∂ε + ys0 + zs0 − (1 + ε) = 0, ∂s0 ∂s0 ∂s0 ∂s0

∂xt T ∂xs0 xs0 ∂T xs0 T ∂ε + − ρ0 − + (1 + ε)X = 0 , 1 + ε ∂s0 ∂t 1 + ε ∂s0 (1 + ε)2 ∂s0

(5.7.2)

with two other ones for y and z. (5.7.1) and (5.7.2) represent the system of equations that describes the motion of a string which satisﬁes a constitutive equation of the type (5.7.1). This time, there is one more unknown function T , so that there is now ﬁve unknown quantities i.e. x, y, z, ε and T . In order to ﬁnd the type of this system (5.7.1) and (5.7.2) will be combined with the six equations (5.3.3) as well as the relations dε =

∂ε ∂ε dt , ds0 + ∂s0 ∂t

dT =

∂T ∂T dt . ds0 + ∂s0 ∂t

(5.7.3)

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Mechanics of Extensible Strings

dynamic

233

Taken together, these relations form a system of ten equations with ten unknown derivatives ∂xs0 /∂s0 , ∂xt /∂t, ∂ys0 /∂s0 , ∂yt /∂t, ∂zs0 /∂s0 , ∂zt /∂t, ∂ε/∂s0 , ∂ε/∂t, ∂T /∂s0 and ∂T /∂t. By solving this system with respect to these derivatives, we obtain: ∂ε f dt + gdT + (1 + ε)F gds0 − ρ0 g(ds0 /dt) dv = ∂t [1 − ρ0 g(ds0 /dt)2 ] dv ∂ε −(f dt + gdT − dε) + ρ0 g[dv − (ds0 /dt)dε] − ((1 + ε)/ρ0 )gF ds0 = ∂s0 [1 − ρ0 g(ds0 /dt)2 ] ds0 ∂T −[ρ0 (ds0 /dt)2 f + 1] dT − (1 + ε)F ds0 + ρ0 (ds0 /dt) dv = , ∂t [1 − ρ0 g(ds0 /dt)2 ] dt ∂xs0 [T /(1 + ε) − ρ0 (ds0 /dt)2 ](f dt + gdT − dε)xs0 = ∂s0 −(1 + ε)[T /(1 + ε) − ρ0 (ds0 /dt)2 ][1 − ρ0 g(ds0 /dt)2 ] ds0

(5.7.4)

+

(1 + ε)[1 − ρ0 g(ds0 /dt)2 ][(1 + ε)Xdt − ρ0 dxt + ρ0 (ds0 /dt) dxs0 ] ds0 /dt −(1 + ε)[T /(1 + ε) − ρ0 (ds0 /dt)2 ][1 − ρ0 g(ds0 /dt)2 ] ds0

−

xs0 [1 − T g/(1 + ε)][(1 + ε)F dt − ρ0 (dv − (ds0 /dt) dε)] ds0 /dt , −(1 + ε)[T /(1 + ε) − ρ0 (ds0 /dt)2 ][1 − ρ0 g(ds0 /dt)2 ] ds0

and similarly for the other six derivatives. Thus, in the case of the constitutive equation (5.7.1) the equations of motion of the problem possess ﬁve families of characteristic lines 2 ds 1 T = c2I (T, ε) , = (5.7.5) dt ρ0 1 + ε

ds0 dt

2 =

1 = c2II (T, ε) , ρ0 g

s0 = const.

(5.7.6) (5.7.7)

Along these characteristic lines the following diﬀerential relations ρ0 dxt = ±ρ0 cI dxs0 + (1 + ε)Xdt −

xs0 {(1 − ε)F dt − ρ0 (dv ∓ cI dε)} , 1+ε

± cII (f dt + gdT ) +

1+ε F dt − dv = 0 , ρ0

dε = gdT + f dt ,

(5.7.8) (5.7.9) (5.7.10)

are satisﬁed respectively. Thus there are two types of propagable waves, whose velocities of propagation are functions of both tension and strain. There are also stationary (non propagable) discontinuities (5.7.7). Certain information concerning the nature of the waves which appear in this case can be obtained from the dynamic and kinematics compatibility conditions which are

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

234

dynamic

Dynamic Plasticity

∂xs0 ∂ys0 ∂zs0 ∂ε + ys0 + zs0 − (1 + ε) = 0, xs0 ∂s0 ∂s0 ∂s0 ∂s0 2 & T ∂T ∂xs0 ds0 xs0 xs0 T ∂ε − ρ0 + − = 0, 1+ε dt ∂s0 1 + ε ∂s0 (1 + ε)2 ∂s0 .................. ∂ε ∂T −g = 0, ∂t ∂t −

∂xs0 ∂s0

ds0 dt

2

+

∂xt = 0, ∂t

.................. ∂ε ∂ε dt + ds0 = 0 , ∂t ∂s0

∂T ∂T dt + ds0 = 0 , ∂t ∂s0 (5.7.11)

and four equations for y and z. The ﬁrst ﬁve relations (5.7.11) are the dynamic compatibility equations while last ﬁve are the kinematics compatibility conditions. In (5.7.11) and in the following formulae, the square brackets are used to denote the jump of a certain function across a wave front. Across the characteristic lines (5.7.5), it follows from the second, third and fourth relation (5.7.11) that ∂ε T ∂T = . ∂s0 1 + ε ∂s0 From this relation, and taking into account the other relations (5.7.11) as well, it follows that across a line (5.7.5) ∂ε ∂ε ∂T ∂T = = 0, (5.7.12) = = ∂s0 ∂s0 ∂t ∂t if the relation cI = cII is satisﬁed. Moreover, from the ﬁrst relation (5.7.11), we obtain ∂xs0 ∂ys0 ∂zs0 + ys0 + zs0 = 0. (5.7.13) xs0 ∂s0 ∂s0 ∂s0 Thus from (5.7.12) and (5.7.13) it follows that (5.7.5) are transverse wave fronts which aﬀect only the shape of the string but not the tension nor the longitudinal strain. Both the equation (5.7.5) of the characteristic curves and the diﬀerential relations (5.7.8) satisﬁed on these characteristics formally coincide with those corresponding to the ﬁnite constitutive equation.

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

dynamic

Mechanics of Extensible Strings

235

If one takes into account (5.7.6), it follows from (5.7.11) that across a characteristic of this family the relations 1 ∂xs0 1 ∂ys0 1 ∂zs0 ∂ε = = = (5.7.14) xs0 ∂s0 ys0 ∂s0 zs0 ∂s0 ∂s0 are satisﬁed if cI = cII . Thus the discontinuities of the derivatives of the coordinates are directed along the tangent to the string. From (5.7.14) one obtains conclusions similar to those of (5.3.16) in the case of the ﬁnite constitutive equation. Thus, (5.7.6) represent longitudinal wave fronts which aﬀect the strain and tension but not the shape of the string. The diﬀerential relations (5.7.9) are diﬀerent from those corresponding to the ﬁnite constitutive equation. The characteristics (5.7.12) represent stationary discontinuities. Across such a line, all the derivatives with respect to the variable t (the interior derivatives) are continuous. From the second relation (5.7.11), it follows that: xs0 ∂T xs0 ∂ε ∂xs0 =− + , (5.7.15) ∂s0 T ∂s0 1 + ε ∂s0 with two similar relations for y and z. Introducing this relation into the ﬁrst relation (5.7.11), we obtain [∂T /∂s0 ] = 0, so that the derivatives of the tension are continuous across a line ds0 = 0. It follows that (5.7.15) reduces to (5.7.14) and therefore that the stationary discontinuities aﬀect only the strain. We can consider some special cases. The ﬁrst one is if the form ∂ε ∂T =E − G(T, ε) , ∂t ∂t

(5.7.16)

where the function G(T, ε) is often taken to depend linearly on the overstress G(T, ε) = k[σ − F (ε)] .

(5.7.17)

In (5.7.17) k is a speciﬁc constant of the material while σ = F (ε) is the static constitutive equation of the material considered. Constitutive equation of the form (5.7.16) corresponds to materials whose instantaneous response to a tension increment is purely elastic. A second special case of the constitutive equation (5.7.1) is the constitutive equation ∂ε = f (T, ε) , ∂t

(5.7.18)

which corresponds to materials which do not possess an instantaneous response to an increment of the tension. This case leads to very interesting mathematical problems. The particular case of the Voigt model has been mentioned by Cristescu [1952] while for a general discussion of a constitutive equation of the form T = T (ε, ε) ˙

(5.7.19)

January 12, 2007

236

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

dynamic

Dynamic Plasticity

the reader is referred to Cristescu [1957]. Combining the equations of motion with (5.7.18), one obtains the complete system describing the motion. The characteristics of the system are 2 ds0 1 T = c2 (T, ε) , = (5.7.20) dt ρ0 1 + ε dt = 0 ,

(5.7.21)

ds0 = 0 .

(5.7.22)

It should be noted that the two distinct characteristic lines (5.7.6) in the present special case are superposed and coincide with the family of straight linear dt = 0. The characteristics (6.7.5), which are transverse wave fronts, exist in this particular case too, as for the constitutive equation (5.7.1). Thus the system is of an intermediary type. The inﬂuence of the temperature inﬂuence has been considered by Manacorda [1958]. Let us denote by θ(s0 , t) the actual temperature of the points of the string, by θe the actual external temperature and by θ∗ the initial uniform temperature of both string and external media. We shell also use the notation π = θ − θ∗ and πe = θe − θ∗ . The equations of motion, also take into account the force due to the resistance of the medium in which the string moves. This is of the form −R(x2t + yt2 + zt2 )v with R ≥ 0 (this force is directed along the velocity of the point, but in the opposite sense). Thus ∂ ∂xt T ∂x = + (1 + ε)(X − Rxt ) (5.7.23) ρ0 ∂t ∂s0 1 + ε ∂s0 and two similar expressions for y and z. Attaching the Fourier law and the constitutive law of the form ˙ π) . T = T (s0 , ε, ε,

(5.7.24)

Manacorda showed that across the transverse wave fronts (5.3.6) the second order derivatives of the strain as well as those of the temperature do not suﬀer a jump. Thus, the transverse waves do not directly inﬂuence the strain and temperature variation. The inﬂuence of temperature on the dynamics of extensible strings which move in a resistive medium has also been considered by Dinca [1967], who ﬁrst considered a constitutive equation of the form T = T (ε, π) .

(5.7.25)

The system is of hyperbolic-parabolic type. Dinca [1967] has used also instead of the Fourier law the law proposed by Kaliski [1965] and the system again becomes hyperbolic.

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

Mechanics of Extensible Strings

5.8

dynamic

237

Shock Waves

In the previous sections the integration schemes have been given for cases when only ordinary waves propagate in the string. Thus at the end of the string, for t = 0, the values of the stress and of the particle velocity, prescribed according to boundary and initial conditions, must coincide. In some particular motions of the string, one should consider the possibility that shock waves might appear. Two types of shock waves can occur, i.e. longitudinal shock waves which are propagable discontinuities of ε, T and v, and transverse shock waves which are propagable discontinuities of the slope of the string. We shall examine the propagation of shock waves in strings which can move in space (Cristescu et al. [1966]). As before, it will be assumed that the strings are perfectly ﬂexible, although to neglect the rigidity of the string when considering transverse shock waves is a fairly rash assumption. The propagation of shock waves in various particular cases, when the string moves in a single plane, has been studied by Rakhmatulin (see Rakhmatulin and Dmianov [1961]), P´er`es [1953] Ch. XII, Craggs [1954], and Pavlenko [1959]. The conditions satisﬁed across a shock wave front can be obtained from the conditions of continuity of coordinates, from the conditions of conservations of mass and conservation of momentum. If c is used to denote the velocity of propagation of the shock wave, it follows from the conditions of continuity of coordinates that [xt ] + c[(1 + ε)xs ] = 0 ,

(5.8.1)

with two similar conditions for y and z. These are the kinematics compatibility conditions. The vector form of this relation is [v] + c[(1 + ε)τ ] = 0 .

(5.8.1a)

We shall denote by “+” the value of a certain function after the shock wave front has passed, and by “−” the value of the same function before this event. The law of conservation of mass can be written as follows ρ0 ds0 = ρ− ds− = ρ+ ds+ .

(5.8.2)

Sometimes it is useful to write this relation in the form ρ0 = ρ− (1 + ε− ) = ρ+ (1 + ε+ ) .

(5.8.3)

Considering the element of the string which is traversed by the shock wave front in time dt, and writing for this element, of mass ρ0 ds0 , the conditions of conservation of momentum yields: − − − + + ρ− (1 + ε− )c(x+ t − xt ) = T xs − T xs .

(5.8.4)

The relation (5.8.1) can be written − − − + + x+ t − xt = c{(1 + ε )xs − (1 + ε )xs } .

(5.8.5)

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

238

dynamic

Dynamic Plasticity

Introducing (5.8.5) into (5.8.4) we obtain − − + + − − ρ0 c2 {(1 + ε+ )x+ s − (1 + ε )xs } = T xs − T xs ,

or 2 − − − {ρ0 c2 {(1 + ε+ ) − T + }x+ s = {ρ0 c (1 + ε ) − T }xs ,

(5.8.6)

and similar relations for y and z. The relations (5.8.6) link the values of various functions before and after the shock wave front has passed. They involve both the functions which describe the longitudinal motion of the string, and those which refer to the transverse motion. By squaring the relations (5.8.6), summing, and taking into account that xs , ys , zs are direction cosines which cannot be simultaneously zero, we obtain ρ0 c2 {(1 + ε+ ) − T + = ρ0 c2 (1 + ε− ) − T − ,

(5.8.7)

which yields the velocity of propagation: c2II =

[T ] . ρ0 [ε]

(5.8.8)

The formula (5.8.7) was derived by P´er`es [1953] Ch. XI, and by Pavlenko [1959] for the case of plane motion; it can be used to calculate the velocity of propagation of longitudinal shock waves. This velocity is generally variable and does not coincide with the velocity of propagation of smooth waves. However, this coincidence occurs if the slope is constant on the portion of the tension–strain curve considered (elastic, linear work-hardening, etc.). If the curvature of the tension–strain curve and the jumps [T ] and [ε] are not too big, the velocity furnished by (5.8.8) does not diﬀer greatly from the velocity of propagation of longitudinal smooth waves c2II = (1/ρ0 )(dT /dε). If one introduces (5.8.7) into (5.8.6) it follows that [xs ] = [ys ] = [zs ] = 0 .

(5.8.9)

In this case, and taking (5.8.3) into account, the two kinds of relation (5.8.1) and (5.8.4) reduce to a single type of relation [xt ] = −cII [ε]xs .

(5.8.10)

Thus the shock waves which propagate with the velocity (5.8.8) are longitudinal waves which do not change the shape of the string, while the jump of the material velocity is directed along the tangent to the string. The component of this velocity which is normal to the string remains continuous. The conclusions developed from (5.8.7) hold only if both terms in (5.8.7) are diﬀerent from zero. Let us consider the case when both these terms are zero. This yields a velocity of propagation c furnished by c2 =

T− T+ − T− T+ = = . + − ρ0 (1 + ε ) ρ0 (1 + ε ) ρ0 (ε+ − ε− )

(5.8.11)

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Mechanics of Extensible Strings

dynamic

239

Fig. 5.8.1 The ﬁrst special case when longitudinal and transverse shock waves propagate with the same velocity.

These are shock waves which produce discontinuities for all the unknown functions involved in the problem, i.e. [ε] = 0, [T ] = 0, [xs ] = 0, [ys ] = 0, [zs ] = 0, [xt ] = 0, [yt ] = 0, [zt ] = 0. This case has been discussed by Pavlenco [1959]. Let us examine in what circumstances such waves are possible. A ﬁrst case when such waves may arise is that shown in Fig. 5.8.1, when a whole portion of the stress–strain curve is a segment of the straight line passing trough the point (−1, 0), and the jump of the tension is comprised in this segment. A second possible case has been represented in Fig. 5.8.2, which is selfexplanatory; this case is certainly not a stable one. From these special cases, one can conclude that a shock wave which simultaneously carries discontinuities for both strain and slope, occurs seldom (for very special constitutive equations and loading laws). A third case when (5.8.11) holds is the case when [ε] = 0

so that [T ] = 0 .

In this case the formula (5.8.11) can be written T . c2I = ρ0 (1 + ε)

(5.8.12)

(5.8.13)

Introducing (5.8.12) into (5.8.1) [or into (5.8.4)] it follows that [xt ] + cI (1 + ε)[xs ] = 0 .

(5.8.14)

These are transverse shock waves. Their velocity of propagation (5.8.13) always coincides with the velocity of propagation of smooth transverse waves (5.3.8). For the elastic strings the formula (5.8.13) was given by Cristescu [1951] and for the general extensible strings by P´er`es [1953] Ch. XI #19. Taking into account that the case of simultaneous propagation of discontinuities of strain and slope occurs only very seldom, in the special cases mentioned in

January 12, 2007

10:41

240

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Dynamic Plasticity

Fig. 5.8.2 The second special case (unstable) when longitudinal and transverse shock waves propagate with the same velocity.

Figs. 5.8.1 and 5.8.2, one can conclude that a shock produced at a point of the string will generally propagate by means of two kinds of shock waves, one transverse and the other longitudinal. The discontinuities of the velocity prescribed by the boundary conditions produce a jump of the strain [formula (5.8.19)] which propagates by means of a longitudinal shock wave, and a jump of slope [formula (5.8.14)] which propagates by means of a transverse shock wave. These waves propagate with the velocities (5.8.8) and (5.8.13) respectively.

5.9

Other Papers

The equations of the elastic strings were considered by many other authors. Disturbances produced by the motion of a driver which is rigidly bonded to the edge of a plate are used by Parker and Varley [1968], to motivate parameter expansion technique which, when applied to the equations of ﬁnite elasticity, generate approximating equations which describe law-frequency deﬂection and stretching waves traveling along stretched elastic plates and rods in the limit when bending forces are negligible compared with membrane forces. The structure of the boundary layer at the driven edge and shock layers, where the low-frequency or ﬁlament approximations are locally invalid, are also discussed. The low-frequency equations are used to discuss the interaction between progressing ﬁnite amplitude deﬂection and stretch waves in the limit when the stretch rate is small compared with the angular speed of the plate. The disturbance is locally that of a pure deﬂection simple wave whose amplitude and frequency are modulated by slow variations in the stretch. As the stretch increases the frequency increases while the amplitude

dynamic

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Mechanics of Extensible Strings

dynamic

241

decreases. The stretch wave is also modiﬁed by deﬂection of the plate: the speeds of wavelets carrying constant values of stretch are always less than their values in the pure stretch simple wave. Also, Parker [1970] considers the motion of a plane non-linearly elastic string. It is shown that extensional signals passing through a non-uniform disturbance are not carried along exact characteristics, but are carried at a considerable slower speed, even though the governing equations are non-dispersive. The impact of composites impacted with a body will not be discussed here. We mention only the damage observed in composites, as one is impacting them, the successive impact of various laminas, and the successive damage produced (Cristescu et al. [1975]). That was continued by several other papers as for instance Papanicolaou et al. [1998], Navarro [1998] and Kook et al. [2000]. In these papers the ﬁgures are very close to those from impacted strings. The Riemann and Goursat step data problems for extensible strings have been considered by Mihailescu and Suliciu [1975a, b]. They consider longitudinal discontinuities, for which [λ] = 0, [τ ] = 0, U = λτ (|τ |) = 1, and therefore [U] = [λ]τ ,

[V] + c[λ]τ = 0 ,

c2 =

[T ] , ρ[λ]

and transversal discontinuities, for which [λ] = 0, [τ ] = 0, therefore [U] = λ[τ ] ,

[V] + cλ[τ ] = 0 ,

They write the system to be solved as ∂ T ∂V U −ρ = 0, ∂r λ ∂t T = f (ε) ≥ 0 ,

c2 =

T . ρλ

∂U ∂V − =0 ∂t ∂r

λ = |U| ≥ 1 ,

ε=λ−1

with f (0) = 0 f (ε) > 0

for ε ≥ 0 ,

f (ε) < 0 where U = ∂x/∂r, V = ∂x/∂t, ρ = const. > 0 and x is a function. In order to ensure unique solutions for the problems considered in the paper, one is adopting the following principle. A shock discontinuity is possible only when a rarefaction fan is not possible (Suliciu [1973]). The Goursat problem in strains is solved as well as the problem in velocities and the Riemann problem. The transient response of an impulsively loaded plastic string on a plastic foundation was considered by Mihailescu-Suliciu et al. [1996]. The last authors consider the problem of an impulsive loading of a long rigid-plastic string resting on a rigid-plastic foundation. A closed form solution is obtained by disregarding the longitudinal motion and

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

242

Dynamic Plasticity

Fig. 5.9.1

Final string shape for diﬀerent I0 .

considering an arbitrary large transversal motion. Expressions for the ﬁnal shape of the string are derived in terms of magnitude of the applied impulse. It is found that the stress and the foundation reaction force are not uniquely determined, while the shape of the string is. The ﬁnal shape of the string is given in Fig. 5.9.1. Here w is a dimensionless displacement, ζ a dimensionless variable and I0 an impulse. A continuous initial or initial-boundary value problem for an elastic visco-plastic string on an elastic viscoplastic foundation is formulated by Suliciu [1996]. An energy identity/inequality is deduced. Bounds in energy of the solutions are derived and the stress deviation of the viscoplastic model from the plastic one is estimated. As a farther limiting case similar results are derived for the rigid perfect plastic case. In the paper by Jang et al. [1990] the response of advanced composites to low-velocity projectile loading was investigated. The impact failure mechanisms of composites containing various ﬁbers with diﬀerent strength and ductility were studied by a combination of static indentation testing, instrumented falling dart impact testing, acoustic emission monitoring, and scanning electron microscopy. The composites containing ﬁbers with both high strength and high ductility demonstrate a superior impact resistance as compared to those containing ﬁbers with high strength (graphite ﬁbers) or high ductility (nylon) but not both. Upon impact loading, the composites containing polyethylene ﬁbers usually exhibited a great degree of plastic deformation and some level of delamination. The paper by Wang and Vu-Khanh [1991] reports both experimental and numerical investigations on delamination mechanisms in [05 , 905 , 05 ] carbon ﬁber/poly laminate subjected to low-velocity impact. It was found that these

dynamic

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Mechanics of Extensible Strings

dynamic

243

composites exhibits the same damage mechanisms as epoxy-based composites, but superior delamination resistance. Thick glass-ﬁbre-reinforced laminates of various dimensions have been subjected to low-velocity impact with a ﬂat-ended impactor by Zhou [1995]. Post-impact examination of damage is carried out by visual inspection, diametric crosssectioning, and ultrasonic C-scanning. A number of damage mechanisms have been observed, and their inﬂuence on impact behavior is found to be generally dependent on the impact force or incident kinetic energy level. By replacing the ﬁrst-order law of motion (velocity given) with a second-order law (acceleration given), dynamics of e.g. ﬂexible and rigid elastic strings is described by Uby [1996] in a similar manner. A system of nine coupled partial diﬀerential equations results, but on eliminating longitudinal motion, a smaller system is obtained. Classic vibration equations are recovered as special cases. The free surface spalling phenomena is 2D carbon/carbon and carbon-polyimide laminates was studied by Gupta et al. [1996] by subjecting them to laser-produced nano-second rise-time compressive stress pulses. The compression pulse travels through the laminate normal to the plies and, upon reﬂection into a tension pulse from the sample’s front surface, leads to ﬁber/matrix debondings either in the bundles within a ply or at the interplay interface. Additional information on the attenuation and the dispersion characteristics associated with the propagation of such stress pulses was also obtained for both types of composite microstructures. High speed cine techniques have been used by Gellert et al. [1998] to examine the perforation of thin targets constructed of glass ﬁber reinforced plastic, Spectra and Kevlar composites as well as nylon and Kevlar fabrics. From the ﬁlm record the kinetic, strain and (for the composites only) delamination/surface energy terms were evaluated for the rear layer of material. Simple models for the deformation of the panels were used to compare these energies, summed for all layers, with the projectile energy loss. All the energy terms are shown to be signiﬁcant. The work highlights many of the features which need to be accounted for in modeling ballistic perforation of fabric and ﬁber reinforced composite materials. Karbhari and Rydin [1999] have shown that resin transfer molded composites exhibit impact induced damage mechanisms and sequences diﬀerent from those shown by laminated composites due to diﬀerences in layering and compaction of reinforcement. In addition to the classical modes of damage, mechanisms such as inter-bundle, inter-bundle and void pocket cracking are also seen. In a paper denoted to the Riemann problem, Hanche-Olsen et al. [2002] presents the problem of Riemann for an elastic string with a linear Hooke’s law. They are showing that the Riemann problem has a unique solution. A weak solution of the nonstrictly hyperbolic conservation law when the total variation of the initial data is suﬃciently small is due to Reiﬀ [2002], which examined an elastic string of inﬁnite length in three-dimensional space, restricted to possess non-simple eigenvalues of constant multiplicity.

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

244

Dynamic Plasticity

Fig. 5.9.2

Traveling wave in a whipped string with a phase boundary.

The paper of Purohit and Bhattacharya [2003] presents a theory to describe the dynamical behavior of a string made of a phase-transforming material like a shape-memory alloy. The study of phase boundaries, the driving force acting on them and the kinetic relation governing their propagation is of central concern. The paper proposes a qualitative experimental test of the notion of a kinetic relation, as well as a simple experimental method for measuring it quantitatively. It presents a numerical method for studying initial and boundary value problems in strings, and concludes by exploring the use of phase transforming strings to generate motion at very small scales. Figure 5.9.2 is showing one example of traveling waves in a whipped string; the grid size is 1.25 × 10−3 in this calculation. The string is ﬁxed at the right end, initially stretched horizontally and then whipped or impacted at the left end x = 0 with the following velocity: y˙ 1 = 0 and y˙ 2 = 100.0 m/s , y˙ 2 = −100.0 m/s , y˙ 2 = 0.0 ,

0 ≤ t < 1.6 × 10−4 , 1.6 × 10−4 ≤ t < 3.2 × 10−4 ,

3.2 × 10−4 ≤ t < 1.2 × 10−3 .

The traveling wave propagating through the length of the string is discernible. The breakdown of classical solutions of the planar motion of an elastic string was studied by Manfrin [2004]. The string is inﬁnite in length and having a planar motion, in the absence of external forces. One assumes strict hyperbolicity in the sense

dynamic

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Mechanics of Extensible Strings

T (r) >

dynamic

245

T (r) >0 r

for any r > 1. A novel experimental technique is developed by Minnaar and Zhou [2004] for time-resolved detection and tracking of damage in the forms of delamination and matrix cracking in layered materials such as composite laminates. The technique is non-contact in nature and uses dual or quadruple laser interferometers for high temporal resolution. Simultaneous measurements of diﬀerential displacement and velocity at individual locations are obtained to analyze the initiation and progression of interfacial fracture and/or matrix cracking/delamination in a polymer matrix composite system reinforced by graphite ﬁbers. The measurements at multiple locations allow the speeds or matrix cracking/delamination front propagates to be determined. The results show that the speed of delamination or the speed of matrix cracking/delamination increases linearly with impact velocity. An analytical model for studying the material failure in shear hinges formed during the dynamic plastic response of a circular plate under projectile impact is due to Chen et al. [2005]. Analytic solutions for the ballistic perforation performance of a fully clamped plate struck by a blunt projectile are obtained. It takes into account both the global response (plate bending) and the localized shear. Based on the estimations of the shear strain and the size of shear hinge, condition for the initiation of an adiabatic shear band is formulated. The eﬀectiveness of the present model is demonstrated by reasonable agreement between the theoretical predictions and the available experimental data for the perforation of steel plates. In another paper (Stoﬀel [2006]) an explanation for the development of conical shapes in the case of shock wave loaded plated is proposed based on the wave propagation phenomena. Impact damage processes in composite sheet and sandwich honeycomb materials, impacted with an impactor of 5 kg from a drop hight of 1 m, with a velocity of 4,4 m s−1 , was done by Dear et al. [2006]. Experiments were conducted on aluminum plates of 1 mm thickness by using a gas gun and projectiles with blunt and hemispherical noses (Gupta et al. [2006]). Ballistic limit velocity was found to be higher for hemispherical projectiles than for blunt projectiles. The ballistic impact of woven fabric was done by Naik et al. [2006]. Using the analytical formulation, ballistc limit, contact duration at ballistic limit, surface radious of the cone formed and the radious of the damaged zone have been predicted for typical woven fabric composites. The numerical results of ballistic impact and perforation of woven aramid fabric are presented by Tan et al. [2006]. The crimp is introduced in several ways. Inﬂuence of boundary conditions on the ballistc performance of high-strength fabric target were considered by Zeng et al. [2006]. Targets that are unclamped on two edges can absorb more impact energy than those with all four sides clamped. It

January 12, 2007

10:41

246

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Dynamic Plasticity

also observed that slippage at clamped edges contributes to higher energy absorption. The impact velocity is less than 500 m/s. In another paper (Tan and Ching [2006]) a FE model of woven fabric that reﬂects the orthotropic properties of the fabric, the viscoelastic nature of the yarns, the crimping of the yarns, the sliding contact betveen yarns and yarn breakage using an assembly of viscoelastic bar elements.

Bibliography Chen X. W., Li Q. M. and Fan S. C., 2005, Initiation of adiabatic shear failure in a clamped circular plate, Int. J. Impact Engn. 31, 877–893. Courant R., 1962, Methods of Mathematical Physics, Vol. II, Partial Diﬀerential Equations, Interscience Publi., New York. Craggs J., 1954, Wave motion in plastic-elastic strings, J. Mech. Phis. Solids 2, 4, 115–124. Cristescu N., 1951, Discontinuities in the motion of perfectly ﬂexible elastic strings, Commun. Acad. Rep. Populare Romane 1, 439–445. Cristescu N., 1952, Discontinuities in the motion of visco-elastic, perfectly ﬂexible strings, Rev. Univ. C.I. Parhon Politeh. Bucuresti, Ser. Stiint. Nat. 1, 68–81. Cristescu N., 1954, About the loading and unloading waves which can appear in the motion of elastic or plastic ﬂexible strings, Prikl. Mat. Meh. 18, 3, 257–264 (in Russian). Cristescu N., 1957, On the propagation of waves in rubber, Prikl. Mat. Meh. 21, 6, 797–800 (in Russian). Cristescu N., 1958, Dynamic problems in the theory of plasticity, Editura Tehnica (in Rumanian). Cristescu N., 1960, Elastic-plastic waves in strings, Arch. Mech. Stos. 12, 597–615. Cristescu N., 1961, Spatial motions of elastic-plastic strings, J. Mech. Phys. Solids 9, 165–178. Cristescu N., 1964, Some problems of the mechanics of extensible strings, Symp. IUTAM Stress Waves in Anelastic Solids, Providence, 1963 (Springer-Verlag, Berlin–G¨ otthingen–Heidelberg) 118–132. Cristescu N., 1965, Loading/unloading criteria for rate sensitive materials, Arch. Mech. Stos. 17, 291–305. Cristescu N., 1967, Dynamic Plasticity, North-Holland Pub. Comp., 614 pp. Cristescu N., Dinca G. and Suliciu I., 1966, On the propagation of shock waves in extensible strings, Analele Univ. Bucuresti, Ser. Stiint. Nat., Mat.-Mec. 15, 65–73. Cristescu N., Malvern L. E. and Sierakowski R. L., 1975, in Foreign Object Impact Damage to Composites, ASTM STP 568, American Society for Testing and Materials, pp. 159–172. Dear J. P., Lee H. and Brown S. A., 2006, Impact damage processes in composite sheet and sandwich honeycomb materials, Int. J. Impact Engineerig (in print). Dinca G., 1967, Some remarks about the thermodynamics of extensible strings, Studii Cercetari Matematice 19, 659–680. Fenstermaker C. A. and Smith J. C., 1965, Appl. Polymer Symposia 1, 125–146. Gellert E. P., Pattie S. D. and Woodward R. L., 1998, Energy transfer in ballistic perforation of ﬁber reinforced composites, J. Materials Sci. 33, 1845–1850. Gupta N. K., Iqbal M. A. and Sekhon G. S., 2006, Experimental and numerical studies on the behavior of thin aluminum plates subjected to impact by blunt- and hemisphericsal-nosed projectiles, Int. J. Imp. Engineering (in press).

dynamic

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Mechanics of Extensible Strings

dynamic

247

Gupta V., Pronin A. and Anand K., 1996, Mechanisms and quantiﬁcation of spalling failure in laminated composites under shock loading, J. Composite Mat. 30, 6, 722–747. Hanche-Olsen H., Holden H. and Risebro N. H., 2002, The Riemann problem for an elastic string with a linear Hooke’s law, Quart. Appl. Math. 60, 4, 695–705. Jang B. Z., Chen L. C., Hwang L. R., Hawkes J. E. and Zee R. H., 1990, The response of ﬁbrous composites to impact loading, Polymer Composites 11, 3, 144–157. Karbhari V. M. and Rydin R. W., 1999, Impact characterization of RTM composites II: Damage mechanisms and damage, J. Materials Sci. 34, 5641–5648. Kaliski S., 1965, Wave equation of thermoelasticity, Bull. Acad. Polon. Sci., Ser. Sci. Tech. 13, 211–219. Kook J. S., Yang I. Y. and Adachi T., 2000, Characteristics of delamination in graphite/epoxy laminates under static and impact loads, Key Engng. Materials 183 187, 731–736. Lewis G. M., 1957, Proc. Conf. Prop. Mater. At High Rates of Strain (Inst. Mech. Engrs., London) 190–194. Manacorda T., 1958, Riv. Mat. Univ. Parma 9, 13–19. Manfrin R., 2004, On the breakdown of classical solutions of the planar motion of an elastic string, Bull. Sci. Math. 128, 253–263. Marshall I. and Thomson A. B., 1954, The cold drawing of high polimers, Proc. Roy. Soc. A 221, 541–557. Mihailescu M. and Suliciu I., 1975a, Riemann and Goursat step data problems for extensible strings, J. Math. Anal. Appl. 52, 10–24. Mihailescu M. and Suliciu I., 1975b, Riemann and Goursat step data problems for extensible strings with non-convex stress–strain relation, Rev. Roumaine Math. Pures. Appl. 20, 551–559. Mihailescu-Suliciu M., Suliciu I., Wierzbicki T. and Fatt Hoo M. S., 1996, Transient response of an impulsively loaded plastic string on a plastic foundation, Quart. Appl. Math. 54, 2, 327–343. Miklowitz J., 1947, The initiation and propagation of the plastic zone along a tension specimen of nylon, J. Colloid Sci. 2, 193–215. Minnaar K. and Zhou M., 2004, A novel technique for time-resolved detection and tracking of interfacial and matrix fracture in layered materials, J. Mech. Phys. Solids 52, 2771–2799. Naik N. K., Shrirao P. and Reddy B. C. K., 2006, Ballistic impact behaviour of woven fabric composites: Formulation, Int. J. Impact Engineering (in press). Navarro C., 1998, Simpliﬁed modelling of of the ballistic behaviour of fabrics and ﬁbre reinforced polymeric matrix composites, Key Engin. Mat. 141 143, 383–400. Papanicolaou G. C., Blanas A. M., Pournaras A. V. and Stavropoulos C. D., 1998, Impact damage and residual strength of FRP composites, Key Engin. Mat. 141 143, 127–148. Parker D. F., 1970, Interacting waves in long stretched elastic strings, J. Mech. Phis. Solids 18, 331–342. Parker D. F. and Varley E., 1968, Interaction of ﬁnite amplitude deﬂection and stretching waves in elastic membranes and strings, Quart. Journ. Mech. and Applied Math. 21, Pt.3, 329–352. Pavlenko A. L., 1959, On the propagation of perturbations in a ﬂexible string, Izv. Akad. Nauk. SSSR, Otd. Tekhn. Nauk, Mekhn. Mashinostr. 4, 112–122. P´er`es J., 1953, M´ecanique G´en´erale, Masson, Paris. Purohit P. K. and Bhattacharya K., 2003, Dynamics of strings made of phase transforming materials, J. Mech. Phis. Solids 51, 3, 393–424.

January 12, 2007

248

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Dynamic Plasticity

Rakhmatulin H. A., 1951, Transverse shock with variable velocity on a ﬂexible string, Uch. Zap. Mosk. Univ. 4, 5, 154. Rakhmatulin H. A. and Shapiro G. S., 1955, Propagation of perturbations in non linear-elastic and nonelastic media, Izv. Akad. Nauk SSSR, Otd. Fekhn. Nauk 2, 68–89. Rahmatulin H. A. and Demianov Yu. A., 1961, Strength under intensive momentary loads, Moscow (in Russian). Reiﬀ A. M., 2002, Existence of weak solutions to the elastic string equations in three dimensions, Quart. Appl. Math. 60, 3, 401–424. Riabova E. H., 1953, Transverse shock with variable velocity on a ﬂexible string, Vestn. Mosk. Univ. 10, 85–91. Smith J. C., Blandford J. M. and Schiefer H. F., 1960, Stress–strain relationship of yarns subjected to rapid impact loading: 6. Velocities of strain waves resulting from impact, Textile Res. J. 30, 10, 752–769. Smith J. C., Crackin F. L. Mc and Schiefer H. F., 1958, Stress–strain relationship in yarns subjected to rapid impact loading: 5. Wave propagation in long textile yarns impacted transversely, J. Res. Nat. Std. 60, 5, 517–534. Smith J. C., Crackin F. L. Mc, Schiefer H. F., Sione W. K. and Towne K. M., 1956, Stress–strain relationship in yarns subjected to rapid impact loading: 4. Transverse impact tests, J. Res. Nat. Bur. Std. 57, 2, 83–89. Smith J. C. and Fenstermaker C. A., 1967, Strain-wave propagation in strips of natural rubber subjected to high-velocity transverse impact, J. Appl. Phys. 38, 11, 4218–4224. Smith J. C., Fenstermaker C. A. and Shouse P. J., 1964, Experimental determination of air drag on textile yarn struck transversely by high-velocity projectile, J. Res. Nat. Bur. Std. C 68, 177–181. Smith J. C., Fenstermaker C. A. and Shouse P. J., 1965, Stress–strain relationships in yarns subjected to rapid impact loading. 11. Strain distribution resulting from riﬂe bullet impact, Textile Res. J. 35, 743. Smith J. C., Fenstermaker C. A. and Shouse P. J., 1963, Experimental determination of air drag on textile yarn struck transversly by high-velocity projectile, Textile Res. J. 33, 919–934. Smith J. C., Shouse P. J., Blandford J. M. and Towne K. M., 1961, Textile Res. J. 31, 721–734. Stoﬀel M., 2006, Shape forming of shock wave loaded viscoplastic plates, Mec. Res. Comm. 33, 35–41. Suliciu I., 1973, Motions with discontinuit´es in solides — Nonlinear models, Stud. Cerc. Mat. 25, 53–170 (in Rumanian). Suliciu I., 1996, An energetic characterization of the constitutive equations for plastic strings on plastic foundations, Constitutive Relation in High/Very High Strain Rates, IUTAM Symposium, Noda, Japan, Oct. 16–19, 1995. Spriger Vlg. Tan V. B. C. and Ching T. W., 2006, Computational simulation of fabric armour subjected to ballistic impacts, Int. J. Impact Engineering (in press). Tan V. B. C., Shim V. P. W. and Zeng X., 2006, Modelling crimp in woven fabrics subjected to ballistic impact, Int. J. Impact Engineering (in print). Uby L., 1996, Strings, rods, vortices and wave equations, Proc. R. Soc. Lond. 452, 1531–1543. Victorov V. V., Dobrovolsckii I. P., Cristrescu N., Kovalenco T. S., Stepanov P. D. and Shapiro G. S., 1966, Study of some dynamic properties of some polymers, Proc. Symp. on the Prop. of Elastic-plastic Waves in Cont. Med., Baku, 1964, 103–108.

dynamic

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Mechanics of Extensible Strings

dynamic

249

Wang H. and Vu-Khanh T., 1991, Impact-induced delamination in [05 , 905 , 05 ] carbon ﬁber/polyetheretherketone composite laminates, Polymer Eng. Sci. 31, 18, 1301–1309. Zeng X. S., Shim V. P. W. and Tan V. B. C., 2006, Inﬂuence of boundary conditions on the ballistic performance of high-strength fabric targets, Int. J. Impact Engineering (in press). Zhou G., 1995, Damage mechanisms in composite laminates impacted by a ﬂat-ended impactor, Composites Sci. Tech. 54, 267–273.

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

This page intentionally left blank

dynamic

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

dynamic

Chapter 6

Flow of a Bigham Fluid

This chapter is devoted to the motion of a Bingham body through various devices; through a tube with or without friction at the wall, ﬂow in a viscosimeter, ﬂow in the ﬁeld of natural slopes, etc. Plastic ﬂow through conical converging dies will not be described (Cristescu [1975] [1976], Fu and Loo [1995]). For general concept on strain rate intensity factor see Aleksandrov et al. [2003].

6.1

Flow of a Bingham Fluid Through a Tube

We consider a tube of length l and of radius R (Buckingham [1921]). We work in cylindrical coordinates. At z = 0 we have (Fig. 6.1.1) σ = −p

(6.1.1)

that is a pressure is applied.

r

v(r)

2r0

R

z

0

l Fig. 6.1.1

The ﬂow in a tube.

251

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

252

dynamic

Dynamic Plasticity

We assume “telescopic ﬂow” i.e., vr = vθ = 0 ,

vz = v = f (r) .

(6.1.2)

The rate of deformation tensor in cylindrical coordinates are Drr

Drz

1 ∂vθ ∂vr vr ∂vz 1 , Dθθ = + , Dzz = , Dθz = = ∂r r r ∂θ ∂z 2 ∂vz vθ 1 ∂vr 1 ∂vr 1 ∂vθ + , Drθ = − + . = 2 ∂z ∂r 2 ∂r r r ∂θ

∂vθ 1 ∂vz + r ∂θ ∂z

,

From here for our problem we have Drr = Dθθ = Dzz = Dθz = Drθ = 0 ,

Drz =

1 f (r) . 2

(6.1.3)

The constitutive equation for a Bingham (viscoplastic/rigid) ﬂuid is: σij = σδij + kij + 2ηDij

(6.1.4)

with the plastic part Dij = 2λkij

if

kij kij = 2k 2 .

(6.1.5)

If only kij kij < 2k 2

we have Dij = 0 .

From (6.1.3) and (6.1.5) we obtain Drz = 2λkrz

2 and krz = k 2 = τY2 .

(6.1.6)

Thus for the only non zero component: krz = kzr = τY (sign Drz ), all other kij = 0 .

(6.1.7)

We observe now that f < 0 or (∂vz /∂r) < 0 since vz decreases with increasing r. = 0, besides Drz and σrz . We Therefore sign Drz = −1. Since all Dij = 0 all σij have thus σrr = σθθ = σzz = σ ,

σθz = σrθ = 0 ,

σrz = σzr = −τY + ηf (r) .

(6.1.8)

The equations of motion in cylindrical coordinates are: 1 ∂σrθ ∂σzr σrr − σθθ ∂σrr + + + + ρ(br − ar ) = 0 , ∂r r ∂θ ∂z r 1 ∂σθθ ∂σzθ 2σrθ ∂σrθ + + + + ρ(bθ − aθ ) = 0 , ∂r r ∂θ ∂z r 1 ∂σzθ ∂σzz σrz ∂σrz + + + + ρ(bz − az ) = 0 . ∂r r ∂θ ∂z r

(6.1.9)

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

Flow of a Bigham Fluid

dynamic

253

Introducing (6.1.8) in (6.1.9)1 and (6.1.9)2 , and by disregarding the body forces and the accelerations, we have: ∂σ ∂σrr =0⇒ = 0, ∂r ∂r

⇒ σ(z) ∂σ ∂σθθ =0⇒ = 0, ∂θ ∂θ thus σ depends on z alone. Introducing (6.1.8) in (6.1.9)3 we obtain: dσ τY f = −η f + + , dz r r

(6.1.10)

(6.1.11)

where σ depends on z alone and f depends on r alone. This by integrating with respect to z we get τY f + z+C (6.1.12) σ = −η f + r r with the boundary conditions at the end of the tube (independent on r, thus constant in the hole cross section): z = 0 : σ = σ0 ⇒ C = σ0 z = l : σl = 0 .

(6.1.13)

Thus for z = l, from (6.1.12), by integration with respect to r, we obtain: −ηf r + τY r +

σ0 r2 + C1 = 0 l 2

(6.1.14)

or C1 σ0 r + . l 2 r Comparing now this equation with the last (6.1.8) we get: ηf = τY +

C1 σ0 r + . l 2 r From the shearing ﬂow symmetry it follows that for σrz =

r = 0,

(6.1.15)

(6.1.16)

∂v = 0 ⇒ f = 0 ⇒ Drz |r=0 = 0 ⇒ σrz |r=0 . ∂r

Thus, around r = 0 exists a cylinder of radius r0 , where kij kij < 2k 2 , i.e., is rigid and for r = r0 : σrz = −τY

(6.1.17)

the condition kij kij = 2k 2 is just satisﬁed. Introducing (6.1.17) in (6.1.16) for r = r0 we have −τY =

C1 σ0 r0 + . l 2 r0

(6.1.18)

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

254

dynamic

Dynamic Plasticity

From the global equilibrium condition of rigid cylinder of radius r0 (the inner core): πr02 σ0 = −τY (2πr0 )l or r0 σ0 . (6.1.19) τY = − 2l Introducing (6.1.19) in (6.1.18) we get C1 = 0. Returning to (6.1.15) by integration: σ0 −ηv + τY r + r2 + C2 = 0 . (6.1.20) 4l Flow with wall adherence. We assume now that the material adheres on the wall, i.e., r = R : v = 0.

(6.1.21)

By introducing (6.1.21) in (6.1.20) we obtain τY R + (σ0 /4l)R2 = −C2 and from (6.1.20): σ0 ηv = τY (r − R) + (r2 − R2 ) . (6.1.22) 4l If we put here v = 0 we get for r two solutions r1 = R ,

r2 = −R + 2r0 .

The second solution is impossible, since we must have r0 > R. The velocity of the rigid internal nucleus is obtained from (6.1.22) for r = r0 : σ0 (r0 − R)2 . v0 = − (6.1.23) 4lη The radius of the nucleus is [from (6.1.19)]: r0 = −

2lτY 2lτY = σ0 ∆p

with

σ0 < 0 .

(6.1.24)

If τY → 0 from (6.1.20) follows r0 → 0 and (6.1.22) becomes a parabolic distribution of velocities of a viscous ﬂuid, i.e., for ﬁxed l and ∆p, r0 is a measure of “plasticity”. Some conclusions: • r0 increases with l; when r0 increases towards R, l increases towards lMAX = (R∆p/2τY ), and from (6.1.23) v0 → 0. • r0 increases with τY (decrease of temperature, decrease of humidity, irradiation, etc.) when τY increases its maximal value is τYMAX = (R∆p/2l), from (6.1.24) r0 → R, and from (6.1.23) v0 → 0. • r0 decreases with the increasing σ0 , i.e., the inner core radius decreases with increasing pressure. If σ0 ⇒ r0 , i.e., σ0 towards σ0min = −2lτY /R and from (6.1.24) r0 → R and from (6.1.23) v0 → 0. • The maximum value of r0 is R = (2lτY /∆p), when the whole body becomes rigid and from (6.1.23) v = 0 since the ﬂuid adhere on the wall and v0 → 0. • Flow is possible only if r0 < R or (2lτY /∆p) < R or ∆p > (2lτY /R) is the limit pressure diﬀerence for the ﬂow to take place.

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

dynamic

Flow of a Bigham Fluid

255

• ∆p must be bigger if: the tube is longer (bigger l) τY is bigger (lower temperature or dryer paste) smaller R If the ﬂuid does not adhere to the wall, i.e., the slip is possible, see below. Volume ﬂux. The volume ﬂux of the ﬂuid comprised between r0 and R is: 2 2 2 4 4 − R σ0 R − r0 + σ0 R − r0 R 4l 2 4l 4 dQ1 2π = v2πr dr = dt η r0 R3 − r03 R2 − r02 −τY R − 2 3

(6.1.25)

with v from (6.1.22), or

r 3 r 2 dQ1 πσ0 R4 4 r0 5 r0 4 0 0 =− 1− − . +4 −2 dt 8ηl 3R 3 R R R

(6.1.26)

The volume ﬂux Q2 of the portion which remain rigid is [with v from (6.1.23)]: r0 r0 2πσ0 πσ0 dQ2 2 v2πr dr = − r dr = − = (r0 − R) (r0 − R)2 r02 . dt 4lη 4lη 0 0 (6.1.27) If at t = 0, Q = 0, the total volume ﬂux is Q = Q1 + Q2 , and 4 r0 Q πσ0 R4 1 r0 4 1− =− + t 8lη 3R 3 R

(6.1.28)

and with r0 from (6.1.24):

# 4 $ Q πσ0 R4 4 2 lτY 1 2lτY =− 1+ + t 8lη 3 R σ0 3 Rσ0

or

# 2 $ 2 Q πσ0 R4 2 2lτY 2lτY 1 2lτY =− 1− 1+ + t 8lη 3 Rσ0 3 Rσ0 Rσ0

(6.1.29)

(6.1.30)

which is the formula of Buckingham [1921]–Reiner [1926]. For τY = 0 this formula reduces to the one for viscous ﬂuids. If we introduce variables which do not depend on the tube dimensions V = (6.1.30) is written V =

4 Q/t , R3 π

P =−

Rσ0 2l

2 τY 1 τY 2 τY 2 P 1− + 1− η 3 P 3 P P

(6.1.31)

(6.1.32)

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

256

dynamic

Dynamic Plasticity

Ne wt on V

=P /η

V

B 0

a gh in

m

P

τY

Fig. 6.1.2

The diﬀerence between the two formulas.

for τY → 0 we obtain the solution for Newtonian viscosity V =

P η

or

Q πR4 σ0 = t 8ηl

i.e., the Hagen–Poiseuille formula (Fig. 6.1.2). Flow with friction at the wall. Viscous friction. For a general Bingham material, the fact that for r0 → R the ﬂow is no more possible is a restriction which we have to remove. Generally, when r0 increases, v0 decreases. This could be accepted up to a certain limit. Let us assume that for r0 → R : v → vf

(6.1.33)

where vf would be a limit velocity due to friction between the Bingham body and the wall. In this case, by replacing (6.1.22) by (6.1.33) we get η(v − vf ) = τY (r − R) +

σ0 2 (r − R2 ) . 4l

(6.1.34)

An estimation of the friction shearing stress τf can be obtained by assuming r0 = R and considering the motion of the material as a rigid body: πR2 σ0 = 2πRlτf or τf =

Rσ0 . 2l

(6.1.35)

Let us further assume that the friction takes place in a “boundary layer” of thickness h, and that the property of this boundary layer can be approximated by a Newtonian linear viscous ﬂow σ = 2µD, where µ is a viscosity coeﬃcient for the boundary layer. For the σrz = τf component we get ∂vf vf vf ≈ (6.1.36) τf = µ h ∂r h

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

Flow of a Bigham Fluid

Fig. 6.1.3

dynamic

257

The ﬂow of a Bingham body with adherence at the wall.

where h is the thickness of the boundary layer (assumed to be 10−n cm, with n = 3 or 4, say). Combining (6.1.36) and (6.1.35): vf =

Rσ0 h 2lµ

(6.1.37)

which is to be introduced in (6.1.34). Examples are given in Fig. 6.1.3 for v = 0 at r = R and in Fig. 6.1.4 for v = vf at r = R. The examples are computed for R = 2 cm, l = 20 cm, τY = 20 kPa, h = 10−2 cm, σ0 = 1 Mpa, µ = 0.01 kPa s and η = 1 s−1 . Viscoplastic friction. Any other friction law could be considered, for instance the friction law proposed for metal plasticity (Cristescu [1975]) (6.1.38) τ = m IIσ where m is a “friction factor” 0 ≤ m ≤ 1, with m = 1 corresponding to adherence and m = 0 for no friction. For Bingham model this law becomes: τ = m(τY + 2η IID ) . (6.1.39)

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

258

dynamic

Dynamic Plasticity

Fig. 6.1.4

The ﬂow of a Bingham body with friction at the wall.

For our case we have τ = m(−τY + 2ηDrz ) . Thus the slide takes place when Drz at the wall reaches the value 1 1 σ0 σ0 τY + r , σrz = r, Drz = f (r) = 2 2η 2l 2l and at the wall the law (6.1.40) becomes: σ0 τ = m R = mσrz |R . 2l Thus the sliding starts when the applied pressure reaches the " " 2l τ 2l = σrz "" σ0 = mR R R

(6.1.40)

(6.1.41)

(6.1.42)

(6.1.43)

and, again: τ = mσrz |R .

(6.1.44)

Thus, more pressure is needed if the contact surface ﬂuid/tube is longer, if the tube is thinner, and if m is bigger.

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

Flow of a Bigham Fluid

Fig. 6.1.5

dynamic

259

Motion in the case of a viscoplastic friction.

In the case when a viscous layer does not exist any more, and r0 = R, σrz |R = (σ0 /2l)R, and σrz |R increases with σ0 . When σ0 reaches a certain limit, satisfying (6.1.44) the plug moves. Figure 6.1.5 is an example.

6.2

Flow of a Bingham Fluid Between Two Circular Concentric Cylinders (Reiner [1960])

Let us consider two circular concentric cylinders of height h. The inner one has the radius Ri and is either kept ﬁxed and a torque M is measured, or is rotating with angular velocity ω˙ i . The external cylinder, of radius Re > Ri is either rotating with the angular velocity ω˙ e or is ﬁxed. Let us consider the stationary motion of a ﬂuid between these two cylinders (Fig. 6.2.1). This is a typical motion taking place in viscometers. If ω˙ i = 0 the viscometer is of Couette–Hatschek type. If ω˙ e = 0 we get the principle of the Searle viscometer. The ﬁxed cylinder (or mobile) can be used also for the measurement of the torque induced by the rotating ﬂuid.

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

260

dynamic

Dynamic Plasticity

h

Ri

Re

r1

ω e

Fig. 6.2.1

Flow of Bingham body between two cylinders.

We use cylindrical spatial coordinates r, θ, z. We assume the ﬂow ﬁeld of the form vr = vz = 0 ,

vθ = v = f (r) .

(6.2.1)

The components of the rate of deformation tensor in cylindrical coordinates become in this case vθ 1 f 1 ∂vθ − = f − , Drθ = 2 ∂r r 2 r Drr = Dθθ = Dzz = Drz = Dθz = 0 .

(6.2.2)

Since every single particle is in motion v = f = rω(r) ˙

(6.2.3)

where the angular velocity ω˙ depends on r. The rate of deformation becomes r dω˙ . 2 dr The Newtonian viscous ﬂuid is the ﬁrst case to consider. Drθ =

σrθ = ηr

dω˙ dr

(6.2.4)

(6.2.5)

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

Flow of a Bigham Fluid

dynamic

261

and σrr = σθθ = σzz = −p and σzθ = σzr = 0 .

(6.2.6)

The equilibrium equations becomes for this case (disregarding the body forces and the accelerations): ∂p 1 ∂σrθ − + = 0, ∂r r ∂θ ∂σrθ 1 ∂p 2σrθ − + = 0, ∂r r ∂θ r ∂p = 0. (6.2.7) ∂z Taking into account that the problem is with axial symmetry (∂/∂θ = 0) it follows that p = const. (the atmospheric pressure). From (6.2.7)2 follows C1 σrθ = 2 (6.2.8) r and with (6.2.5): dω˙ C1 η = 2 (6.2.9) dr r i.e., C1 (6.2.10) η ω˙ = 2 + C2 . 2r The two constants are determined from the boundary conditions: −

t>0

r = Ri : ω˙ = ω˙ i ,

Thus

C1 = 2η(ω˙ e − ω˙ i )

C2 = 2η

(6.2.11)

r = Re : ω˙ = ω˙ e . 1 1 − 2 Ri2 Re

−1

ω˙ e Re2 − ω˙ i Ri2 . Re2 − Ri2

(6.2.12)

Introducing in (6.2.10) we get: ω˙ =

ω˙ i Ri2 (Re2 /r2 − 1) − ω˙ e Re2 (Ri2 /r2 − 1) Re2 − Ri2

while the tangential stress follows from (6.2.8): 2η ω˙ e − ω˙ i . σrθ = 2 r 1/Ri2 − 1/Re2

(6.2.13)

(6.2.14)

The torque exerted on a cylindrical surface of radius r and of height h can be estimated as M = σrθ (2πrh) r

(6.2.15)

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

262

dynamic

Dynamic Plasticity

i.e., with (6.2.14): M = 4ηπh

ω˙ e − ω˙ i . 1/Ri2 − 1/Re2

Thus the torque is independent on r. In the particular case when the internal cylinder is ﬁxed: ω˙ i = 0 , ω˙ = ω˙ e

Re2 (1 − Ri2 /r2 ) , Re2 − Ri2

M = 4ηπh

1/Ri2

ω˙ e . − 1/Re2

(6.2.16)

The torque is measured either on the internal (ﬁxed) cylinder, or on the external one. In the particular case when the external cylinder is ﬁxed; ω˙ e = 0 , ω˙ = ω˙ i

Ri2 (Re2 /r2 − 1) , Re2 − Ri2

M = 4ηπh

−ω˙ i . − 1/Re2

1/Ri2

(6.2.17)

The Bingham ﬂuid. The constitutive equation is now: dω˙ dr

for σrθ > τY ,

ω˙ = const. = 0

for σrθ ≤ τY .

σrθ = τY + ηr

(6.2.18)

The other stress components satisfy (6.2.6) with p = const. From (6.2.7)2 follows again (6.2.8) and therefore with (6.2.18): dω˙ C1 τY +η = 3 , r dr r

(6.2.19)

or after integration C1 − τY ln r + C2 . (6.2.20) 2r2 Let us assume now that the internal cylinder is ﬁxed and the other one rotates with the angular velocity ω˙ e prescribed. Thus for η ω˙ = −

t>0

r = Ri : ω˙ i = 0 , r = Re : ω˙ = ω˙ e .

From (6.2.21)1 and (6.2.20) follows C2 =

C1 + τY ln Ri 2Ri2

(6.2.21)

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Flow of a Bigham Fluid

and (6.2.20) becomes C1 η ω˙ = 2

1 1 − 2 Ri2 r

− τY ln

dynamic

263

r . Ri

(6.2.22)

The constant C1 can be determined if the torque M is measured on one of the cylinders. We have M , (6.2.23) 2πh where h is the height of the portion of the cylinder in contact with the ﬂuid. Thus (6.2.22) becomes, if M is known, 1 1 r M − τY ln − (6.2.24) η ω˙ = 4πh Ri2 r2 Ri C1 =

and for the outer cylinder: M η ω˙ e = 4πh

1 1 − 2 Ri2 Re

− τY ln

Re Ri

(6.2.25)

which is the formula due to Reiner and Riwlin [1927]. In the particular case τY → 0 we obtain again (6.2.17)3 for the viscous ﬂuid. From (6.2.15) follows that for a constant value of M , the tangential stress σrθ is bigger when r is smaller. On the other hand the ﬂow takes place only if σrθ > τY , i.e., [from (6.2.15)]: M > M0 = τY 2πRi2 h .

(6.2.26)

M < M0

(6.2.27)

If

the Bingham ﬂuid is stressed, but no ﬂow is possible. If however (6.2.26) is satisﬁed, then a portion of the material in the neighborhood of the inner cylinder is ﬂowing. If the value of the measured moment is M1 , the radius r1 of the portion of the material which is in motion can be obtained from (6.2.15) for σrθ = τY : M1 r1 = . (6.2.28) 2πhτY The condition that the whole material in Ri ≤ r ≤ Re be in motion (i.e., r1 = Re ) is M ≥ Me = 2πRe2 hτY .

(6.2.29)

If M1 and r1 are measured (6.2.28) can be used to determine τY . Afterwards from (6.2.25) follows η. If the material comprised between r1 ≤ r < Re rotates as a rigid, the formula (6.2.24) becomes 1 M1 1 r1 − τY ln − (6.2.30) η ω˙ 1 = 2 2 4πh Ri r1 Ri

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

264

dynamic

Dynamic Plasticity

4πhη τ Y Re ln 1/Ri2 − 1/Re2 η Ri

4ηπ

M=

M=

Ne wto

nia

Bin gha m

e

n fl uid h ω& e 1/R 2 i − 1/R 2

4π 1/R 2 hη i − 1/R 2 ω&1 + τ Y e η ln Re Ri

ω1

0 No flow

= M0 increa sin g r1

Me

M Ri < r < Re

r1 = Re

r1 = Ri

Ri < r < r1 − viscoplastic ri < r < Re − rigid Fig. 6.2.2

The relationship between M and ω. ˙

and for the torque M1 =

4πhη 1/Ri2 − 1/r12

r1 τY ln ω˙ 1 + . η Ri

(6.2.31)

In Fig. 6.2.2 is showing the diﬀerent relations between M and ω˙ which results from the formulae. 4πhη τY Re ln 1/Ri2 − 1/Re2 η Ri is a measure of the Bingham eﬀect. It is sometimes convenient to introduce dimensionless variables, independent on the geometry of the apparatus V =2

ω˙ i , 1 − Ri2 /Re2

P =

M . 2Ri2 πh

With these variables one can rewrite (6.2.24) to become P τY ln(Ri /Re )2 V = 1− . η P 1 − (Ri /Re )2

(6.2.32)

(6.2.33)

The relationship P ∼ V deﬁnes the properties of the material called consistency.

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Flow of a Bigham Fluid

dynamic

265

Re

δ Ri r1

ω e Viscoplastic fluid

ω w

Rigid Boundary layer Fig. 6.2.3

The motion with a boundary layer.

For τY → 0 the model becomes a viscous ﬂuid. For η → 0 the model becomes a perfectly plastic one. Boundary layer. Static/dynamic dry friction. As the torque or ω˙ e is increased, there is a limit value of r1 when the powder (the Bingham body) in contact with the wall, will slip (Fig. 6.2.3). This will happen when the shear transmitted to the cylindrical surface of radius r1 equals or surpasses the frictional shearing force exerted on the cylinder of radius Re : 2πr1 hτY = 2πRe hτf , where τf is the frictional shearing stress. Thus (see Fig. 6.2.4) r1 τY = Re τf .

(6.2.34)

So long as τf >

r1 τY Re

(6.2.35)

the ﬂuid will adhere to the wall. If however, when r1 is increasing towards r1f r1f τY τf ≤ (6.2.36) Re the rigid portion of the ﬂuid of thickness Re − r1f will slip along the wall. Let us assume that in a very thin layer of thickness δ (see Fig. 6.2.3) the friction law can be described by a relationship of the form (6.2.37) τf = m(τY − 2n IID )

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

266

dynamic

Dynamic Plasticity

ω

increase during dynamic friction

start of dynamic friction

ω e − ω w

end of dynamic friction initiation

M0

Ms Me

M

∆M Fig. 6.2.4

Explanation of the text.

where m is a “friction factor” with 0 ≤ m ≤ 1, IID is the second invariant of the rate of deformation tensor of the material in the boundary layer, and n is a “dynamic friction factor” expressing a measure between the “static” and “dynamic” frictions. If no slip takes place then IID = 0 and the “static” friction law is τf = mτY .

(6.2.38)

The value m = 0 corresponds to perfect lubrication, when τf = 0. From (6.2.34) follows r1 = 0 and therefore the whole volume of ﬂuid comprised between Ri ≤ r ≤ Re is not moving at all and remain rigid. For m = 1 we get the other extreme case; again from (6.2.34) follows r1 = Re , i.e., when ω˙ (or M ) increases it is ultimately possible that the thickness of the rigid layer be reduced to zero thickness, when M → Me (Fig. 6.2.5). In the general case the law (6.2.37) will be used to describe the friction when the slip takes place. Since in IID a single nonzero component is involved r dω˙ (6.2.39) 2 dr we will write this component for the thin layer of thickness δ as nonzero component is involved Re ω˙ w − ω˙ e (6.2.40) Drθ ∼ = 2 δ where ω˙ w is the angular velocity of the external viscometer cylinder, ω˙ e is the “external” angular velocity of the layer r = Re after sliding (Fig. 6.2.6). The Drθ =

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

Flow of a Bigham Fluid

dynamic

267

Rigid Viscoplastic Ri

ω1

Re r1

τY

τ f > τY Fig. 6.2.5

Velocity proﬁle for r1 < Re .

Viscoplastic

Ri Re

Fig. 6.2.6

Velocity proﬁle for r1 = Re .

friction law (6.2.37) becomes

ω˙ w − ω˙ e τf = m τY − nRe δ

from where follows

(6.2.41)

δ . (6.2.42) m nRe Here since during dynamic friction τf < mτY follows that ω˙ e < ω˙ w . δ depends on the material and ﬂuid/viscometer interface, and n is the measure of the diﬀerence ω˙ e = ω˙ w +

τ

f

− τY

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

268

Dynamic Plasticity

ω w

Rigid Viscoplastic

ω e

Ri

Re

r1 τY

τf Fig. 6.2.7

Velocity proﬁle for the case of sliding with dry dynamic friction.

between static and dynamic frictions. In the case of “static” friction, when (6.2.38) holds, from (6.2.42) follows ω˙ e = ω˙ w . (6.2.42) is giving the value of ω˙ e to be introduced in the boundary condition (6.2.21). The quantity δ τ f (6.2.43) ∆ω˙ = ω˙ e − ω˙ w = − τY m nRe is the sudden decrease of ω˙ e and as such produces a sudden decrease ∆M of M [see (6.2.31)]. From the value Ms reached just before slip have started, M decreases to Ms − ∆M during slip. The jump decrease of M produces a jump decrease of r1 [see (6.2.28)], i.e., a sudden increase of the thickness of the rigid portion of the ﬂuid (Fig. 6.2.7). If ω˙ or M are further increased, r1 will continue to increase again. If ∆M is measured, one can determine ∆ω˙ and thus δ/n, assuming that m is determined by other experimental procedures. If δ is obtained by physical considerations, n follows. Generally we need the ratio δ/n, only. 6.3

A Model for Slow Motion of Natural Slopes (Cristescu et al. [2002])

Introduction. Gravitational creep ﬂow, in the sense of deformation in time along a slope under gravitational forces, is often encountered in nature. Examples include: submarine landslides, debris ﬂow, coal slurries, drilling mud, etc. Bedrock landslides have long been recognized as signiﬁcant geomorphic processes in mountainous topography.

dynamic

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Flow of a Bigham Fluid

dynamic

269

Some landslides are deep-seated and involve long-term displacement at low strain rates. Landslide velocities extend from millimeters per year, to hundreds of kilometers per hour. Conventional stability analysis, which treats the geologic material in the slope as a rigid perfectly plastic body, may provide information on the safety factor of stable mass of soil. To describe this a variety of nonlinear viscous models have been considered. To overcome some of limitations of the viscous ﬂow models, Desai et al. [1995] developed an elasto-viscoplastic model. Based on ﬁeld observations, it was assumed that a shear zone exists up to a certain depth, while the bottom layer under the shear zone remains rigid and at rest. It was supposed that in the shear zone the material obeys an associated viscoplastic constitutive equation while the inﬂuence between the rigid bottom and the shearing zone was described by a non associated viscoplastic constitutive equation. The postulated thickness of each of these zones was based on ﬁeld observations. The “interface” model developed by Desai et al. [1995] was further reﬁned by Samtani et al. [1996]; ﬁnite element implementation of the interface element was described along with veriﬁcation of the model with respect to the ﬁeld behavior of a creeping natural slope. The model parameters are determined from laboratory tests. Below is presented a new model describing gravitational motion along a slope. First, an analysis of gravitational consolidation is performed using an elasticviscoplastic constitutive equation for dry sand (Cristescu [1991]). Based on this analysis, it can be concluded that the assumption of a linear variation of density with depth applies. This hypothesis is supported by most experimental data (see for example Desai et al. [1995]). Next, a non homogeneous Bingham model, with yield stress depending on the current density, is considered for the geologic material in the slope. Although the density could be considered to be linearly dependent on depth, it is shown that a linear variation of the yield stress with depth is physically unacceptable. Here we give a procedure for the determination of all of the material parameters involved in the proposed model from in situ measurements. More speciﬁcally, we use only density measurements and measured displacement of the upper boundary of the shear zone corresponding to any time interval ∆t, with all of the other available inclinometer records being further used for validation purposes. Formulation of the problem. A granular material deposited on an inclined slope compacts slowly in time due to its own weight. The geometry of the natural slope and the related coordinate system is shown in Fig. 6.3.1. θ is the slope angle, the x-axis along the slope direction, y-axis normal to the x-axis and situated in the slope plane. The compaction characteristic can be described with a non associated viscoplastic constitutive equation of the form (see Ch. 2): W (t) ∂F 1 1− (6.3.1) D= 2η H(σ) ∂σ

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

270

Dynamic Plasticity

Fig. 6.3.1

Schematic ﬂow along a slope.

where D is the irreversible strain rate tensor, H(σ) is the yield function, F (σ) is !t the viscoplastic potential, σ is the Cauchy stress tensor, W (t) = t0 σ · Ddt is the irreversible stress work per unit volume, which is used here as an internal state variable, η is a viscosity coeﬃcient and the bracket A denotes the positive part of function A, i.e., A = A if A > 0 and A = 0 if A ≤ 0. If we assume that the gravitational stress state to which the granular material is subjected on the slope is essentially constant in time, Eq. (6.3.1) can be easily integrated to give the variation in time of the volumetric strain εv as 1 − W (t0 )/H(σ) ∂F/∂σ 1 ∂F t0 − t 1 − exp (6.3.2) εV (t) = ·σ (1/H) (∂F/∂σ) · σ H ∂σ 2η where t0 is an initial reference time, t is the current time, and σ is the mean stress. Since the density is related to the volumetric strain through ρ(t0 ) (6.3.3) ρ(t) = 1 − εV (t) we can determine at each depth the variation with time of the density. However, to obtain the density variation from Eq. (6.3.3), we need to estimate the stress distribution within the layer of bulk material. Consider a layer of material of constant depth h deposited horizontally (θ = 0 in Fig. 6.3.1). At an arbitrary depth y, the vertical stress is y ρ(t)gdy = −ρ(t0 )g(h − y) − ph (6.3.4) σyy (t) = h

where ph stands for the pressure exerted at the top surface y = h. For bodies of large lateral extent, assuming a plane strain state, Hooke’s law and isotropy, give the other stress components v σyy σxx = σzz = (6.3.5) 1−v

dynamic

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Flow of a Bigham Fluid

dynamic

271

where v is the Poisson’s ratio. The stress given by Eq. (6.3.5) correspond to t = t0 in Eq. (6.3.2) [i.e., the initial data for the viscoplastic Eq. (6.3.1)]. Next we give an example of application of Eqs. (6.3.2)–(6.3.5) for dry sand. The explicit expressions of the yield function, H, and viscoplastic potential, F , used in Eq. (6.3.2) are for dry sand. The material parameters involved in the expressions of these constitutive functions were determined from triaxial compression data reported in Hettler et al. [1984]. From Eq. (6.3.2) it follows that the density at any depth is an increasing function of time and tends asymptotically towards a limit value, say ρ(∞). Figure 6.3.2 shows the variation of the bottom density with time for h = 6 m, v = 0.36, and η = 20 Poise. Figure 6.3.3 shows the plot of the ultimate limit values of the density versus the depth y corresponding to v = 0.3. A linear law of variation of the limit density ρ(∞) with depth approximates the data well ρ h − ρ0 y + ρ0 (6.3.6) ρ= h where ρ0 = ρ(0) is the density at the bottom, y = 0 after compaction and ρh = ρ(h) is the density at the top, y = h. To capture the inﬂuence of the compaction history on the creep ﬂow of the material deposited on the slope, a non homogeneous Bingham model is proposed. if IIσ ≤ k 2 (ρ) 0 (6.3.7) D= k(ρ) 1 √ 1− σ if IIσ > k 2 (ρ) 2η(ρ) IIσ where D is the irreversible strain rate tensor, Dij = 1/2(vi,j + vj,i ), v the the σij is velocity ﬁeld, σ = σ − 1/3(trσ)1 is the stress deviator, and IIσ = (1/2)σij the second invariant of the stress deviator.

Fig. 6.3.2

Evolution in time of the bottom. Density as predicted by (6.3.3).

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

272

dynamic

Dynamic Plasticity

Fig. 6.3.3 Variation of the ultimate density (i.e., density at t → ∞) with depth as predicted by Eq. (6.3.3) (η = 20 Poise, h = 6 m).

In this model both the yield stress k(ρ) and the viscosity coeﬃcient η(ρ) are considered to be functions of the actual density; k is given in stress units and η in Poise. We make the usual kinematics assumption that the particles move in the slope direction (see Fig. 6.3.1) with a velocity depending on depth only, i.e., vx = V (y) , hence, the strain rate tensor is

vy = 0 ,

vz = 0

0 0. 0

0 1 ∂V D= 1 2 ∂y 0

1 0 0

(6.3.8)

(6.3.9)

We assume also that the depth, h, of the stratum is constant. Using Eqs. (6.3.9) and (6.3.7), we obtain (stresses are negative in compression) the following: σxx = σyy = σzz − p and σxz = σyz = 0

(6.3.10)

where −p is the mean pressure. Substituting Eq. (6.3.10) in Cauchy equilibrium equations we ﬁnd −

∂p ∂σxy + + ρg sin θ = 0 , ∂x ∂y

−

∂p ∂σxy + − ρg sin θ = 0 , ∂y ∂x ∂p = 0. ∂z

(6.3.11)

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

Flow of a Bigham Fluid

Fig. 6.3.4

dynamic

273

Variation of shearing stress with depth.

In the proposed constitutive Eq. (6.3.7), the yield stress is a function of the actual density. Since the density varies with depth, we further assume that the yield stress is a function of depth only. Thus the model exhibits transverse isotropy, i.e., the material is isotropic in any plane, y = constant (the group of symmetry of the material consists of all of the rotations about the y direction). Because the yield limit is assumed to depend solely on depth, it follows that the shear stress σxy is a function of y only. Hence, y ρ(y) dy (6.3.12) p(y) = −g cos θ h

and the shear stress is

y

σxy = −g sin θ

ρ(y) dy .

(6.3.13)

h

For the speciﬁc law of linear variation of ρ with depth, Eq. (6.3.6), and the boundary condition σxy |y=h = 0, we further obtain (ρh − ρ0 )(h + y) . (6.3.14) σxy = g sin θ (h − y) ρ0 + 2h Figure 6.3.4 shows the variation of σxy with depth corresponding to θ = 20◦ , h = 6 m, ρ0 = 1.4 g/cm3 , and ρh = 1.002 g/cm3 . The minimum value of σxy is reached at a point that is outside the interval 0 ≤ y ≤ h, while the maximum value is reached at the bottom ρ 0 − ρh hg sin θ . (6.3.15) σxy (0) = 2

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

274

dynamic

Dynamic Plasticity

This value is an increasing function of the stratum thickness h, and of the stratum slope θ. Similarly, we obtain ρ h − ρ0 2 (h − y 2 ) + ρ0 (h − y) . (6.3.16) p(y) = g cos θ 2h Its maximum value is reached at the bottom: ρ 0 + ρh gh cos θ . p(0) = 2 We note that p is a decreasing function of θ. Incipient shear ﬂow. According to the constitutive law Eq. (6.3.7), ﬂow takes place if and only if σxy (y) > k(y) i.e., when the shear stress surpasses the yield limit. The threshold condition for the ﬂow initiation is therefore σxy (y) = k(y). While most data support a linear variation of density with depth [see Eq. (6.3.6)], a linear variation of the yield stress with depth is physically unacceptable. A rigorous proof of this statement is presented in the next section. For the time being, we will postulate a power law variation of the yield stress with depth y n + kh (6.3.17) k(y) = (k0 − kh ) 1 − h where k0 = k(0) is the yield stress at the bottom, kh = k(h) the yield stress at the top, and n > 1 is a material constant. As an illustration of the capabilities of the model, in the following we describe the theoretical pattern of movements corresponding to n = 2 in the power law Eq. (6.3.17). The condition for ﬂow initiation σxy (y) = k(y) is G kh − k0 2 2 (ρ0 − ρh ) + (k y y + − k ) − Gρ 0 h 0 2h h2 h 1 + Gh(ρ0 + ρh ) − k0 = 0 2

(6.3.18)

where G = g sin θ. The case (G/2h)(ρ0 − ρh ) − (kh − k0 )/h2 = 0 corresponding to an overall depth of the moving slope given by h = 2(kh − k0 )/G(ρ0 − ρh ) is physically unacceptable and will not be considered. For h < 2(kh − k0 )/G(ρ0 − ρh ), the discriminant of Eq. (6.3.18), considered as a second order polynomial in y, is 1 ∆ = 2 [h2 G2 ρ2h + 2hG(ρ0 − ρh )kh + 4kh (kh − k0 )] . (6.3.19) h For h = const., the discriminant of ∆(θ) = 0, as a second order polynomial in h is ∆1 = 4kh h2 [kh (ρ0 − ρh )2 + 4(k0 − kh )ρ2h ] .

(6.3.20)

Since ρ0 ≥ ρh and k0 ≥ kh , it follows that ∆1 ≥ 0 and that the equation ∆(θ) = 0 has only one positive root. Furthermore, the equation ∆(θ) = 0 has a solution in (0, π/2) if and only if: h > H, where −(ρ0 − ρh )kh + kh [kh (ρ0 − ρh )2 + 4ρ2h (k0 − kh )] . (6.3.21) H= gρ2h

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

Flow of a Bigham Fluid

dynamic

275

In conclusion, if h < H, then σxy (y) < k(y) for any y ∈ [0, h], i.e., no shear ﬂow is possible. If h > H then: • Incipient shearing motion initiates at the depth hY I =

gρ0 sin θi − (2/h)(k0 − kh ) 2[((ρ0 − ρh )/2h) g sin θi − (k0 − kh )/h2 ]

where θi is the unique solution in (0, π/2) of the equation ∆(θ) = 0; σxy (y) < k(y) for any y = hY I ; the top stratum 0 < y < hY I is a rigid plug in motion, while the bottom stratum is rigid and at rest. • For slope inclination, θ > θi , ∆(θ > 0), Eq. (6.3.18) has two distinct solutions hY B and hY T . In this case, σxy (y) > k(y) for hY B < y < hY T and σxy (y) < k(y) otherwise. The pattern of movement of the slope is as depicted in Fig. 6.3.1. There is a shear zone hY B < y < hY T , its lower and upper boundaries being the solutions of Eq. (6.3.18), i.e., √ −ρ0 g sin θ + (2/h)(k0 − kh ) − ∆ , hY B = 2[((ρ0 − ρh )/2h)g sin θ − (k0 − kh )/h2 ] √ −ρ0 g sin θ + (2/h)(k0 − kh ) + ∆ . (6.3.22) hY T = 2[((ρ0 − ρh )/2h)g sin θ − (k0 − kh )/h2 ] As an example, Figs. 6.3.5(a)–6.3.5(c) show the variation of the shear stress σxy (y) and of the yield limit k(y) with depth corresponding to a slope inclination θ = θi /2, θ = θi and θ = 1.2θi , respectively; h = 20 m, k0 = 48 kPa, kh = 8 kPa, ρ0 = 1.3 g/cm3 , and ρh = 1.2 g/cm3 . For this set of values of the constitutive parameters: θi = 8.4◦ . The thickness of the top rigid stratum depends strongly on the magnitude of the yield stress kh . If kh is very small, the thickness of this stratum becomes very small (i.e., if kh → 0 then hY T → 0). The top rigid stratum hY T ≤ y ≤ h moves with the velocity v(hY T ) of the layer y = hY T (“plug ﬂow”), while the bottom rigid stratum 0 ≤ y ≤ hY B is at rest. The case when this bottom layer may slide along the bottom bedrock will be discussed in the section “Slip with friction at the bottom”. Note that from Eq. (6.3.18) it follows that there is an inclination, θ = θC , such that the lower boundary of the shearing zone coincides with the bottom layer y = 0, sin θC =

k0 ((ρh + ρ0 )/2)gh

(6.3.23)

the upper boundary y = hY T of the shearing zone being k0 ρh . hY T = 2h 1 − 2k0 ρh − kh (ρ0 + ρh ) Let us brieﬂy analyze some limit cases. If the yield stress at the bottom of the stratum is excessively high, then the incipient shear ﬂow takes place at the free surface. Indeed, if in Eq. (6.3.22) k0 → ∞ then hY i → h. Note that if the ﬂow condition σxy (y) = k(y) is satisﬁed at y = h, i.e., motion starts at the free surface,

January 12, 2007

276

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Dynamic Plasticity

(a)

(b) Fig. 6.3.5 Variation of the shear stress σxy and yield stress k (n = 2) with depth for diﬀerent slope inclination θ: (a) θ < θi , the yield condition is not satisﬁed; no shear or rigid motion is possible. (b) θ = θi , shear is possible at depth y = hY I ; the layer hY I < y < h is in a rigid body motion. (c) θ > θi , in the layer hY B < y < hY I , |σxy (y)| > k(y) so the material is shearing; for y > hY B the material is at rest.

dynamic

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Flow of a Bigham Fluid

dynamic

277

(c) Fig. 6.3.5

(Continued ).

then the yield stress at the free surface approaches zero and the material is free ﬂowing. Generally, even after ﬂow has initiated, the material will further compact if the stress to which it is subjected is below the compressibility/dilatancy boundary of the material. Compaction results in an increase of the yield limit, which causes a decrease in the displacement rate to extremely low values. Conversely, a decrease in yield stress and an increase in the unit weight of the soil may be caused, for instance, by heavy rainfalls or sudden snow melting, water-level change, volcanic eruption, or earthquake shaking. This in turn, results in a higher displacement rate. Another possible trigger of shear ﬂow may be an additional pressure added in a short time interval to the top boundary of the stratum (a thick layer of snow, for instance), which will raise the curve σxy = σxy (y) is such that it will intersect k = k(y). In our analysis, we have assumed that the depth h of the stratum is constant and θ is steadily increased. However, a similar solution can be obtained if the inclination θ of the slope is constant, and the thickness h is steadily increased. Determination of k(y). Several methods can be used to determine k. A procedure based on in situ measurements will be given in the section “Example of slow motion of a natural slope”.

January 12, 2007

278

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Dynamic Plasticity

Fig. 6.3.6 Floating boundaries between the rigid and viscoplastic domains when the slope θ ranges from θi (slope angle corresponding to incipient shear ﬂow) to θC (corresponding to viscoplastic motion up to the bottom of stratum).

In the following, we present an inverse method based on laboratory measurements of the motion of the stratum for diﬀerent chute inclinations θ. Speciﬁcally, the necessary data are: • the measured value of the depth hY i , where the shear motion initiates and the corresponding inclination θi ; • hYB and hY T for successive increasing values of θ (θ > θi ), [see Eq. (6.3.22)]. Obviously, the slope of σxy as well as the locations of the vertical lines y = hYB (θ) and y = hY T (θ) (see Fig. 6.3.6) is changing with increasing θ; and • the critical value θC (or of hY T ) corresponding to the case when the whole stratum is in motion [see Eq. (6.3.23)]. Using the measured values of hYB (θ) and hY T (θ), respectively, we then compute σxy (hYB (θ)) and σxy (hY T (θ)) to get k(hYB ) and k(hY T ), respectively. These data points are then used to approximate k(y). Once k(y) is determined, the evolution in time of the boundaries between the domains of rigid motion and of viscoplastic deformation corresponding to a given law of variation of the chute angle with time can be obtained using Eqs. (6.3.22) and (6.3.23). As an example, Fig. 6.3.6 shows the variation with θ of the upper rigid-viscoplastic boundary hY T (θ) and lower rigid-viscoplastic boundary hYB (θ) for θ ∈ (θi , θC ) and the following set of values of the constitutive parameters: k0 = 48 kPa, kh = 8 kPa, n = 2, ρ0 = 1.3 g/cm3 ,

dynamic

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Flow of a Bigham Fluid

dynamic

279

Fig. 6.3.7 Variation of the shear stress σxy and yield stress k(y) for three values of the exponent n [see Eq. (6.3.17)]; only n > 1 is physically possible.

ρh = 1.2 g/cm3 . The initial common point of these boundaries is at h = hY I and θ = θi , hY T (θ) is an increasing function (i.e., the thickness of the rigid stratum is decreasing) while hYB (θ) is a decreasing function (i.e., the thickness of the lower rigid stratum decreases). Note that the stress distribution σxy (y) given by Eq. (6.3.14) is general and does not involve any constitutive assumptions. We have postulated a power law variation (n > 1) of the yield stress k(y) with depth [see Eq. (6.3.17)]. In the following we show that a linear variation (n = 1) or n < 1 is physically unacceptable. Indeed, for the non homogeneous Bingham material Dxy is proportional to the overstress σxy − k and thus reaches a maximum value at a location that corresponds to a maximum in overstress. If a linear dependence is assumed (see Fig. 6.3.7, case n = 1) then for h = const., and θ gradually increased, σxy (y) intersects k(y) always at y = 0. Thus, shear ﬂow would always initiate at the bottom. Though this is a possible particular case, generally it is expected that incipient shear ﬂow would start at some other depth, mainly if h were very large. The same arguments hold against the choice of a power law variation with n < 1 (see Fig. 6.3.7). Only for n > 1 (see Fig. 6.3.7), incipient shear ﬂow can start anywhere between 0 and h. Generally, the yield stress may depend on other parameters such as humidity, temperature, and particle size. Here we assume that all of these parameters inﬂuence ρ, which in turn aﬀects k.

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

280

dynamic

Dynamic Plasticity

Velocity ﬁeld. According to the proposed model Eq. (6.3.7), in the shear zone (IIσ > k 2 ), 2η(y)Dxy = [σxy − k(y)](sign σxy )

(6.3.24)

and since from Eq. (6.3.14) we have sign σxy = +1, we obtain Dxy =

1 [σxy (y) − k(y)] 2η(y)

Dxy = 0 for 0 ≤ y ≤ hYB

for hYB < y < hY T , (6.3.25) and hY T ≤ y ≤ h ,

σxy (y) − k(y) being the “overstress”. Substituting Eqs. (6.3.9), (6.3.14), (6.3.15) in (6.3.17) we obtain 1 ρ h − ρ0 2 k0 − kh dV 2 n = g sin θ (h − y ) + ρ0 (h − y) − (h − y) − kh . dy η 2h hn (6.3.26) For simplicity, we assume that the viscosity η is constant. If there is no slip at the bottom, i.e., V (hYB ) = 0, then after integration we obtain the velocity ﬁeld in the viscoplastic zone hYB < y < hY T 1 2 1 1 3 ρ h − ρ0 2 g sin θ h y − y + ρ0 hy − y V (y) = η 2h 3 2 k0 − kh n+1 (h − y) − kh y + C (6.3.27) + (n + 1)hn where

1 3 1 2 ρ h − ρ0 2 g sin θ h hYB − hYB + ρ0 hhYB − hYB 2h 3 2 k0 − kh (h − hYB )n+1 − kh hYB . + (n + 1)hn

1 C=− η

For the particular case when hYB = 0, C = −(1/η)((k0 − kh )/(n + 1))h. As an example Fig. 6.3.8 shows the velocity proﬁle Eq. (6.3.27) after ∆t = 100 days for: θ = 10.81◦ , h = 20 m, k0 = 48 kPa, kh = 8 kPa, ρ0 = 1.3 g/cm3 , ρh = 1.2 g/cm3 , and η = 1.48 × 106 Poise. The bottom layer 0 ≤ y ≤ hYB of the granular material remains rigid and at rest (V = 0). The top layer hY T ≤ y ≤ hYB moves as a rigid with the velocity V (hY T ) of the layer y = hY T . Note that if velocity data are available and if no slip takes place at the bottom, η can be estimated from Eq. (6.3.27). Both the exponent n in the expression of k(y) and the viscosity coeﬃcient η inﬂuence the velocity proﬁles. Setting θ = 10.81◦ , h = 20 m, k0 = 48 kPa, kh = 8 kPa, 3

3

ρ0 = 1.3 g/cm , ρh = 1.2 g/cm , n = 2, η = 1.48 × 106 Poise,

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

Flow of a Bigham Fluid

dynamic

281

Fig. 6.3.8 Computed velocity proﬁle corresponding to θ = 10.81◦ ; viscoplastic ﬂow develops in the layer hYB < y < hY T (hYB = 6.32 m, hY T = 13.9 m).

Fig. 6.3.9

Inﬂuence of the parameter n on the velocity proﬁle.

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

282

dynamic

Dynamic Plasticity

for the lower η we obtain a larger shear deformation zone, a thinner rigid layer, and more severe displacements (see Fig. 6.3.8). Figure 6.3.9 shows the inﬂuence of n when all of the other constitutive parameters are ﬁxed (same numerical values as in the previous example). Using Eq. (6.3.27) we can also compute the total volume of granular material moving down the slope. The total volume of granular material moving down between hYB ≤ y ≤ hY T in a width interval ∆z in the z-direction and in a unit time interval (the ﬂux) is hY T QS = ∆z u(y) dy (6.3.28) hY B

to which we have to add the material that is in rigid body motion in the zone hY T ≤ y ≤ h, i.e., h QT = ∆z u(hY T ) dy = (∆z)u(hY T )(h − hT ) . (6.3.29) hY T

Thus, for a unit width interval in the z-direction (∆z = 1), and n = 2, we obtain "hT 2 2 " ρ h − ρ0 y4 y3 y 2y " g sin θ h − + ρ − h 0 " h 2 12 2 6 1 " QS = " + C y|hhTY " η 2 + k0 − kh (y − h)4 − kh y "" 12h2 2 hY 2 2 ρ h − ρ0 h4T h3T hT 2 hT g sin θ h − + ρ0 h − h 2 12 2 6 1 + ChT = η 2 + k0 − kh (hT − h)4 − kh hT 12h2 2 2 2 ρ h − ρ0 hY h4Y h3Y 2 hY g sin θ h + ρ0 h − − h 2 12 2 6 1 − ChY . − η 2 + k0 − kh (hY − h)4 − kh hY 12h2 2 (6.3.30) Slip with friction at the bottom. In the following, we further examine how frictional eﬀects at the interface inﬂuence the pattern of movement. Most authors consider Coulomb friction at the interface, τ = µσn .

(6.3.31)

According to Eq. (6.3.31), the tangential stress τ , at any point, is proportional to the normal pressure σn , and is directed opposite to the relative motion between the soil and the bedrock. The coeﬃcient of friction µ is taken as a constant for a given soil and is considered to be independent of the velocity. It is worthwhile

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Flow of a Bigham Fluid

dynamic

283

to note that Coulomb’s law describes correctly the mechanics of friction between two rigid bodies. To accurately reproduce friction between a rigid body and a deformable body, diﬀerent friction law should be considered. To describe friction between a rigid and a perfectly plastic body, the following law was proposed on a great number of tests (Levanov et al. [1976]): σ τ (6.3.32) = ks 1 − exp a τY σY where a < 0, 0 ≤ ks ≤ 1, and τY and σY are the yield stress in simple shear and uniaxial compression, respectively. Generally, ks characterize the rugosity of the hard surface and ranges from 0 to 1. The limit ks = 1 corresponds to very high rugosity when no slip is possible, and a viscoplastic deformation takes place up to the rigid surface. The limit value ks = 0 corresponds to ideal smooth contact and “perfect” lubrication, when sliding is taking place at the smallest applied shearing stress. Note that for normal pressures much lower than σY , the law Eq. (6.3.32) reduces to Coulomb’s law Eq. (6.3.31), while for high pressures (generally for σ > σY ) when the material is fully plastic Eq. (6.3.32) reduces to τ = mτY

(6.3.33)

with m constant, i.e., a constant shear stress is assumed at the interface, irrespective of the normal pressure. Since the maximum shear a material can withstand according to the von Mises yield criterion is τY , it follows that 0 ≤ m ≤ 1: (i) for no friction, m = 0; (ii) for the case of complete adherence to the wall (no slip), m = 1, the material in contact with the wall is deforming plastic. The friction law Eq. (6.3.33) is widely used in plastic forming of metals to describe friction between the die (rigid body) and deforming material (Avitzur [1968]). A generalization of the friction law Eq. (6.3.33) to the case of contact between a rigid body and a viscoplastic material was proposed by Cristescu [1975] (6.3.34) τ = m IIσ where IIσ is the second invariant of the stress deviator. In the case where the viscoplastic material is of Bingham type, the friction law Eq. (6.3.34) becomes (6.3.35) τ = m(k + 2η IID ) where k is the yield stress of the material, η is the viscosity, IID is the second invariant of the stretching tensor D and 0 ≤ m ≤ 1. In the following, we consider friction law Eq. (6.3.35) between the material in the slope and the bedrock (assumed to be a rigid body). This law reproduces the fact that the frictional shear stress is identical with the shearing yield stress. Let as assume that the maximum shear stress that the bottom surface, y = 0 can hold without relative motion is mk0 , m < 1, then σxy |y=0 = mk0 is ﬁrst reached at θ = θs 2mk0 (6.3.36) sin θs = (ρ0 + ρh )hg

January 12, 2007

284

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Dynamic Plasticity

Fig. 6.3.10 The angle at which sliding initiates and the extent of the shear zone for diﬀerent friction conditions at the interface y = 0.

[see Eq. (6.3.15)] and the thickness of the rigid plug sliding along the bottom surface, y = 0 is hYB (θs ) [see Eq. (6.3.22)]. In conclusion, if the friction law Eq. (6.3.35) is assumed at the interface and θ ≥ θs , then there will be a rigid plug at the bottom (see Fig. 6.3.10), i.e., the viscoplastic deformation zone cannot extend to the bottom. If m → 1 (very rough bottom surface) it follows that the sliding velocity Vs → 0 and the zone of viscoplastic ﬂow extends to the bottom. In the case where θ is ﬁxed and h is steadily increased, the depth at which sliding starts is hs =

2mk0 . (ρ0 + ρh )g sin θ

Similar arguments hold, if somewhere in the stratum 0 ≤ y ≤ h there exists a weaker plane y = ys along which the maximum shear stress is much smaller than in the neighborhood layers. In other words, there exists a plane y = ys of yield stress k(ys ) smaller than that of the stress above it. As an example, see the case study reported by Alonso et al. [1993] where a thin marl layer has weaker shear properties than all of the other materials in the moving stratum. Example of slow motion of a natural slope. Laboratory experiments are far from being representative of long-term in situ behaviors. Hence, we propose a procedure for the identiﬁcation of the model parameters based on in situ measurements: density measurements and inclinometer recordings.

dynamic

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

Flow of a Bigham Fluid

dynamic

285

The coeﬃcients of the proposed model are: the viscosity η, the densities ρ0 and ρh , as well as the parameters involved in the law of variation of the yield stress with depth: k0 , kh and n. From measurements of the density of the slope material at the surface and at two other depths we can estimate ρh and the slope of the density line. One inclinometer record gives the values of the upper limit, hY T , the lower limit of the shear zone hYB and h (the extent of the domain of interest). Given the slope angle θ, ρ0 , and ρh from Eq. (6.3.14), we calculate σxy (hY T ) and σxy (hYB ). Since the yield condition is satisﬁed at hY T and hYB , it follows that k(hY T ) = σxy (hY T ) and k(hYB ) = σxy (hYB ). Next, using Eq. (6.3.17) we calculate ln[(kh − k(hYB ))/(kh − kY T )] , n= ln[(h − hYB )/(h − hY T )] k(hYB ) − k(hY T ) , (1 − (k(hYB )/h)n − (1 − (k(hY T )/h)n n k(hYB ) − (k0 − kh ) 1 − . h

k0 = kh + kh = kYB

(6.3.37)

Further, the measured displacement of the upper boundary of the stress zone, u(hY T ), corresponding to any time interval ∆t, permits the determination of the viscosity coeﬃcient η. Indeed, assuming V (hYB ) = 0 (i.e., the strata below the shear zone are at rest) from Eq. (6.3.27) we obtain ρ h − ρ0 2 1 3 3 h (hY T − hYB ) − (hY T − hYB ) 2h 3 g sin θ − h ) h(h Y T YB ∆t η= +ρ 0 1 u(hY T ) 2 2 (h − − h ) YT YB 2 k0 − kh n+1 n+1 + [(h − hY T ) − (h − hYB ) ] − kh (hY T − hYB ) (n + 1)hn (6.3.38) with u(hY T ) the measured displacement of the upper boundary of the shear zone. Hence, all of the material parameters are obtained from exact formulae. In the following, we apply the proposed model to the description of the slow movement of a natural slope, the Villarbeney landslide in Switzerland (data after Samtani et al. [1996]). Creep ﬂow data over one year were recorded at two locations E1 and E2 about 250 m apart. At both locations it was observed that there is a top layer, which is moving essentially as a rigid body. Under this layer, another layer exists where shearing ﬂow takes place. At even deeper layers no motion was recorded. Taking the origin of the y axis at the bottom.

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

286

dynamic

Dynamic Plasticity Table 6.3.1 Model parameter n at location E1 . kh (kPa) 10 20

n 1.14 1.31

30

1.55

42.5

2

At location E1 hY T (= 6m) ≤ y ≤ h(= 18m)

top layer in rigid motion

hYB (= 1m) ≤ y ≤ hY T (= 6m)

slow creep shearing takes place

0 ≤ y ≤ hYB (= 1m)

rigid at rest.

(6.3.39)

At location E2 hY T (= 2m) ≤ y ≤ h(= 8m)

top layer in rigid motion

hYB (= 0.5m) ≤ y ≤ hY T (= 2m)

slow creep shearing takes place

0 ≤ y ≤ hYB (= 0.5m)

rigid at rest.

(6.3.40)

At the location of borehole E1 , the base slope angle is θ = 14◦ , while at location E2 , the base slope angle is θ = 17◦ . Samtani et al. [1996] also give an empirical linear law for the variation with depth of the unit weight of the form γ(h − y) = γh + ζ(h − y)

(6.3.41)

where γ(h − y) is the unit weight at the depth h − y below the surface, γh is the unit weight at the surface, and ζ is a material parameter. At borehole E1 , γh = 21.85 kN/m3 and ζ = 0.0024 kN/m4 , while at borehole E2 : γ = 21.6 kN/m3 and ζ = 0.024 kN/m4 . The data thus support the linear law of variation of density with depth Eq. (6.3.6) that we have obtained using the constitutive Eq. (6.3.2). Using Eqs. (6.3.39) and (6.3.41), we obtain k(hYB ) = 90.637 kPa and k(hY T ) = 63.824 kPa at E1 , and k(hYB ) = 47.989 kPa and k(hY T ) = 38.281 kPa at E2 . The exponent n and k0 in the power law variation of yield stress with depth can be estimated using Eq. (6.3.37). However, the ground yield stress kh at both locations was not available. As an example in Table 6.3.1, we give the values of this experiment corresponding to several values of the ground yield stress kh . We assume kh = 30 kPa at location E1 and using Eq. (6.3.37) we obtain n = 1.55. Next, we calculate the viscosity coeﬃcient η using Eq. (6.3.38) and the measured displacement of the upper boundary of the shear zone u(hY T ) = 17.5 mm corresponding to ∆t = 100 days. We obtain η = 1.523 × 109 Poise. All of the other available inclinometer records at location E1 are further used for validation purposes. Figures 6.3.11(a)–6.3.11(d) show a comparison between the data (symbols) and the predicted displacement proﬁles (lines) at location E1 corresponding to time intervals 148, 196, 260, and

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Flow of a Bigham Fluid

dynamic

287

Fig. 6.3.11 Villaberney landslide. Experimental displacement proﬁles (symbols) and model predictions (dashed lines) at location E1 after a period of: ∆t = 148, 196, 260 and 356 days. The displacement after ∆t = 100 days, which was used for the determination of the model parameters, is not shown.

356 days. At location E2 we assume that kh = 22 kPa, and to calculate η we use the measured displacement of the upper boundary of the shear zone, u(hY T ) = 6.3 mm, corresponding to ∆t = 100 days. The obtained values are: η = 3.852×108 Poise and n = 2. The model predictions versus the data, which was not used for identiﬁcation

January 12, 2007

288

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Dynamic Plasticity

Fig. 6.3.12 Villaberney landslide. Experimental displacement proﬁles (symbols) and model predictions (dashed lines) at location E2 after a period of: ∆t = 148, 196, 260 and 356 days. The displacement proﬁle after ∆t = 100 days, which was used for the determination of the model, is not given.

of the model parameters (readings at ∆t = 148, 196, 260 and 365 days), are shown in Figs. 6.3.12(a)–6.3.12(d). The model predictions seem reasonable; however for an accurate determination of the exponent n, we would have needed the value of the yield stress kh at the surface.

dynamic

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Flow of a Bigham Fluid

dynamic

289

Conclusion. The non homogeneous Bingham model proposed accounts for the eﬀect of gravitational consolidation on the material response and allows for a variation of density and yield stress with depth. A criterion for shear ﬂow initiation is formulated and the ensuing motion is described. Generally, at a certain depth there is a shear region; the top layer above it is in rigid motion (unless the cohesion is zero). The layer below the shear region is either rigid and at rest or in rigid body motion (plug sliding along the bedrock). Velocity proﬁles for several slip conditions at the interface with the bedrock are given. A procedure for determining the constitutive parameters using only the measured displacement of the upper boundary of the shear zone, u(hY T ), corresponding to any time interval ∆t, and density measurements was given. Finally, the model was used to predict the observed ﬁeld behavior of the natural slope from the Villarbeney landslide in Switzerland, and Fosso San Martino (inclinometers readings after Bertini et al. [1984]) (Cazacu and Cristescu [2000]). Let as note that records of a single inclinometer were used for the determination of the model, whereas all the other available records were utilized to test the predictive capabilities of the model. Laboratory tests have been undertaken by Petley and Allison [1997] to elucidate the behavior of deep-seated landslides. In deep-seated failures deformation has been reported at depths of up to 250 m. In the movement zone, owing to the weight of the overburden and the surrounding stress environment, conventional soil mechanics cannot be used to explain eﬀectively associations between the landslip activity and the deformation mechanisms operating within the mowing mass. A number of tests were undertaken, the most signiﬁcant focusing on the transition between ductile and brittle behavior. The results presented in this paper identify a transitional phase of behavior in which creep-like movement will manifest itself at the base of a deep-seated landslide as growth of microcracks. In the Mount Stuart batholith, Washington, Paterson and Miller [1998] have examined magmatic fabrics patterns around stopped blocks in tonalite located near the pluton roof and completed 1:1 scale, three-dimensional mapping of fabric patterns around stopped blocks in diorite located ≈ 1000 m below the roof. There are many places in the world where we have a sliding of several millimeters in 100 days, say. They are producing a recurrent instability phenomenon. Slow motion develops along a deep-seated sliding surface, involving a volume of rock between 22 and 35 million cubic meters. For instance, at Rosone in Italy, such a slide was studied by Forlati et al. [2001]. This rock slope is aﬀected by recurrent instability phenomena. The slow movement develops along a deep-seated sliding surface, involving a volume of rock between 22 and 35 million cubic meters. A series of non-linear, time dependent analyses has been carried out through the ﬁnite element method. A visco-plastic constitutive law, allowing for strain softening eﬀects.

January 12, 2007

10:41

290

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Dynamic Plasticity

The ﬂow of a Bingham ﬂuid taking into account inhomogeneous yield limit of the ﬂuid was considered by Hild et al. [2002]. After setting the general three dimensional problem, the blocking property is introduced. Then they focus on necessary and suﬃcient conditions such that blocking of ﬂuid occurs. The anti-plane ﬂow in two dimensional and one dimensional cases is considered. More ﬁne properties dealing with local stagnant regions as well as local regions where the ﬂuid behaves like a rigid body are obtained in dimension one. Some other ˙ n were variants of Bingham bodies including non-linear Bingham as τ = τy + K(γ) considered by Talmon and Huisman [2005] to describe the ﬂow of drilling ﬂuids.

6.4

How to Measure the Viscosity and Yield Stress

Introduction. There are many apparatuses used today to measure the viscosity of ﬂuids and/or yield stress. Their principles and theories are presented in many books, as for instance in Bird et al. [1987]. Generally all these devices need a signiﬁcant volume of liquid in order to determine its viscosity. However, for some applications like biomedical, ﬂuid supply can be extremely limited. For that reason, we have recently developed a falling cylinder viscometer that requires only a tiny amount of ﬂuid (about 20 µl) in order to measure viscosity. This viscometer is based on a falling ball viscometer of Tran-Son-Tay et al. [1988]. The advantage of falling cylinder versus the falling ball is that the generated shear rate is better deﬁned. Falling cylinder viscometers have been used for over 75 years, but remarkably the problem of a cylinder of ﬁnite length falling inside a cylindrical tube has not been solved yet in simple closed form solution, involving a magnetic ﬁeld as well. It appears that Pochettino [1914] was the ﬁrst to study experimentally the passage from “solid state” to the “ﬂuid state” using a method of falling cylinder in order to study the mechanical properties of tar. Bridgman [1926] used a falling cylinder to determine the “relative viscosities” of ﬂuids subjected to high pressures. He devised the apparatus and analyzed the various possible experimental errors, mainly related to the “inertia eﬀect”, i.e., the time needed for the cylinder to reach a steady-state falling velocity. His apparatus did not give the absolute viscosity, but only the relative viscosity. The relative viscosities for a variety of ﬂuids, for several temperatures and pressures were determined. It was found that viscosity increases with pressure. Using a falling cylinder type viscometer, viscosities of methane and propane at low temperatures and high pressures were determined by Huang et al. [1966], and viscosities of methane, ethane, propane and n-butane by Swift et al. [1960]. A theoretical analysis of the laminar ﬂuid in the annulus of a falling cylinder viscometer was made by Lohrenz et al. [1960]. The falling cylinder viscometer was analyzed by Ashare et al. [1965] for both Newtonian and non-Newtonian ﬂuids; approximate expression for axial

dynamic

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Flow of a Bigham Fluid

dynamic

291

non-Newtonian ﬂow in the annuli was developed. They assumed that, since annular slit is small, it can be regarded as a plane slit. A theoretical analysis for the falling cylinder viscometer for Bingham ﬂuid and power law model, is due to Eichstadt and Swift [1966], while the inﬂuence of the eccentricity on the terminal velocity of the cylinder was considered by Chen et al. [1968]. A falling magnetic stainless steel slug was developed by Mc Duﬃe and Barr [1969] to measure viscosities between 1 and 104 P at pressure up to 3500 Kg/cm2 and temperature between −60◦ and 100◦ C. The motion of the slug was determined with a diﬀerential transformer that moved along the tube. An automatic falling cylinder viscometer for high pressures was also developed by Irving and Barlow [1971]; the sinker was either a solid cylinder or one with a central hole, and the fall time is detected inductively by a series of coils along the viscometer tube. Viscosity in the range 0.01–3000 P was determined. Another kind of falling coaxial cylinder viscometer for lower viscosity ﬂuids as paints, was constructed by Chee et al. [1976], where a weighted rod is falling into a closed-end concentric cylinder. A laser Doppler technique was used to measure the velocity of a falling-slug in a high pressure viscometer by Dandridge and Jackson [1981]; the viscosities of two polyisobutenes have been determined as function of pressure. Viscosities in excess of 107 Pa s have been determined by this method. An improved version of the viscometer was presented by Chan and Jackson [1985]. Measurements of the relative viscosity of aqueous solutions for various temperatures and pressures up to 120 MPa are due to Tanaka et al. [1988]; they found that viscosity increases almost linearly with pressure. Tanaka et al. [1994] later used a laser beam that passed through a pair of sapphire windows to a phototransistor to determine the falling time of the cylinder. A special designed falling cylinder viscometer was used by Kiran and Sen [1992] to measure high-pressure viscosities in the 10 to 70 MPa range and temperatures from 310 to 450 K, of n-butane, n-pentane, n-hexane and n-octane (see also Kiran and Sen [1995]). Kiran and Gokmenoglu [1995] also published viscosity values for Polyethylene solutions subjected to high pressures. Chen and Swift [1972] analyzed the “entrance” and “exit” eﬀects in a falling cylinder viscometer for creeping and non-creeping ﬂow, giving a numerical correction for incompressible Newtonian ﬂuid. End eﬀects occurring in the falling cylinder viscometer were also analyzed by Wehbeh and Hussey [1993]; experimental data for closed and open tubes were also presented. A theoretical and experimental study allowing for the prediction of end eﬀects is due to Gui and Irvine [1994]; the ﬂow ﬁeld is obtained numerically (see also Gui and Irvine [1996]). A superposition technique was utilized by Park and Irvine [1995] to account for the end eﬀects of a ﬂat ends falling cylinder viscometer; the technique is applicable for Newtonian ﬂuids. Park and Irvine [1997] also gave a method to simultaneously determine the density and viscosity of the liquid by using needles of three distinct densities. The derivation of the “exact” solution for the motion of a liquid ﬂowing past a falling cylinder with a frontal spherical end was analyzed by Borisov [1998] with some assumptions concerning the front shape of the cylinder and liquid velocity. The ﬁnite element

January 12, 2007

292

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Dynamic Plasticity

study of a uniform ﬂow past a needle in a cylindrical tube for materials having diﬀerent constitutive equations is due to Phan-Thien et al. [1993]. In the chapter we present a simple theory of the ﬂow of a viscous ﬂuid in a falling cylinder viscometer according to Cristescu et al. [2002], and Cristescu [2005]. The velocity proﬁle is obtained in ﬁnite form for both open tube and closed tube. Also in ﬁnite form is obtained a formula for the determination of the viscosity coeﬃcient. These formulae contain also a term describing the inﬂuence of a magnetic ﬁeld on the motion of the falling cylinder and of the ﬂuid. How this term is used in viscosity measurements will be described in future papers. Since all the obtained formulae are in ﬁnite form, a parametric study (determination of the inﬂuence of various factors involved) of the ﬂuid ﬂow in the falling cylinder viscometer can be done quite easily. The comparison of the determination of the viscosity parameter according to the present theory with viscosity determined with a cone-plate viscometer is quite good. Microrheometer. The most common viscometers and rheometers presently in use are those based on the measurement of stress on a ﬁxed surface while a parallel or opposing surface is moved with a known applied strain rate. However, as already mentioned, these devices require fairly large sample volumes. Often it is diﬃcult, if not impossible, to collect large volumes of samples for testing. In response to this chalange, Tran-Son-Tay et al. [1988] developed an acoustically tracked falling ball

Fig. 6.4.1 Schematic of Microrheometer (a-sample tube, b-cylinder, c-piezoelectric crystal, d-ultrasound transducer, e-water jacket, f-electromagnet).

dynamic

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Flow of a Bigham Fluid

dynamic

293

rheometer (Microrheometer). The Microrheometer (Fig. 6.4.1) is a unique device that was designed to measure the viscosity and viscoelasticity of small samples of biological ﬂuids by using a spherical steel ball that is concentrically located in a small cylindrical tube with a volume of about 20 µl. The ball falls either under the force of gravity or is levitated and oscillated with a force produced by a magnetic ﬁeld. The position of the ball is tracked by ultrasonic pulse-echo method. Furthermore, the small volume permits accurate temperature control and rapid temperature changes to be eﬀected in the sample under study. Modiﬁcations have been made to the original setup so that a constant shear rate will be exhibited across the ﬂuid, that is, a falling cylinder is used in place of a ball. A 20 µl sample is loaded, by retrograde injection, into a disposable glass tube with an inner diameter of 1.6 mm and a height of 10 mm. Once loaded, the tube is centered inside a cylindrical, Plexiglas, water-jacket chamber. The ultrasonic transducer is housed at the bottom center of the Plexiglas chamber. An O-ring forms a watertight seal with the base of the sample tube and with the transducer. A plastic cap is screwed into place at the top of the chamber and provides a seal that completely protects the sample. A schematic of the Microrheometer is given in Fig. 6.4.1. The exact size of the tube and falling cylinder are given in Fig. 6.4.2. One can see that the falling cylinder is very large, as compared with the tube. That is very important for the approach. A small electromagnet coupled with a micromanipulator is used to position and drop a 1.215 mm diameter cylinder in the center of the tube, where the strongest echo occurs. The pulse-echo mode is used to locate and track the falling cylinder. A single sound pulse is transmitted into the ﬂuid medium by pulsing an ultrasound

Fig. 6.4.2 The dimensions of the falling cylinder and tube; CD-cylinder diameter 1.215 mm, CHcylinder height 4.90 mm, TID-tube inner diameter 1.61 mm, TOD-tube outer diameter 2.21 mm, IH-tube height 10.0 mm.

January 12, 2007

294

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Dynamic Plasticity

transducer that also acts as a receiver. Any returning echoes from the cylinder cause a voltage rise across the transducer that is ampliﬁed by the ultrasonic pulse/receiver unit. The time for the sound waves to travel to and back from the cylinder, and the speed of sound in the ﬂuid are measured. From that information, the distance between the transducer and the cylinder, i.e., the location of the falling cylinder is determined. Two types of measurements can be performed with our Microrheometer: (1) a speed-of-sound evaluation, and (2) a steady-state viscosity. The parameters of interest are c, the local speed of sound in the medium and η, the bulk suspension viscosity. In order to measure the speed of sound in the ﬂuid, the instrument needs to be calibrated. To accomplish this, the sample chamber is ﬁrst ﬁlled to the top with distilled water and then capped with a glass cover slip to assure a ﬁxed sample height h. Once the chamber height is determined, the water is removed and replaced by the ﬂuid sample. The local speed of sound in the medium c, is then determined. The ﬂuid viscosity is determined from the speed of sedimentation of the falling cylinder. Details of the theory, including the use of a magnetic force to pull on the

Fig. 6.4.3 Main bang in the large signal on the left, the echo of the cylinder is the smaller signal on the right (at 3).

dynamic

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Flow of a Bigham Fluid

dynamic

295

Fig. 6.4.4 Falling of the cylinder with constant velocities (on 3). The measurements starts at point 1 and end at 3, where the cylinder reaches the bottom.

Fig. 6.4.5 Three approaches of the theory: falling in an inﬁnite tube, moving up or down under a pressure gradient, and falling in a closed tube.

cylinder, are provided in the following section. The main bang followed by the pulse reﬂected from the top of the cylinder is shown in Fig. 6.4.3. The time for the sound waves to travel to and back from the cylinder, and the speed of sound in the ﬂuid is measured. That is shown also in Fig. 6.4.4 where is shown that on the portion considered, the reading is quite linear. That is shown in Fig. 6.4.5. That is why the theory is based on three successive approaches. First we study the ﬂow in an inﬁnite open tube (see the ﬁrst Fig. 6.4.5). Then is studied the ﬂow in an inﬁnite tube under a pressure gradient (second Fig. 6.4.5). Finally at the end we study the ﬂow in a ﬁnite tube, having in mind that a part of the ﬂuid is ﬂowing up while some is ﬂowing down with the cylinder (last Fig. 6.4.5). Theory. In what follows we use cylindrical coordinates (see Fig. 6.4.6) and the notation shown in this ﬁgure. We use: ρc -cylinder density, ρ-ﬂuid density, v1 -velocity of the cylinder.

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

296

dynamic

Dynamic Plasticity

Fig. 6.4.6

Schematic of the falling cylinder viscometer and notations used.

Assumptions made are: A1. The ﬂow is laminar and telescopic; the velocity components are vr = vθ = 0 , vz = v = f (r) with r = x2 + y 2 . A2. The boundary conditions at the cylinder wall:

(6.4.1)

r = R1 : v(R1 ) = −v1

(6.4.2)

t ≥ 0,

i.e. the ﬂuid adders to the cylinder wall. A3. The boundary condition at the tube wall t ≥ 0,

r = R2 : v(R2 ) = 0

i.e., the ﬂuid adheres to the tube wall.

(6.4.3)

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

Flow of a Bigham Fluid

dynamic

297

A4. The ﬂuid is a Newtonian viscous ﬂuid Tij = 2ηDij

(6.4.4)

where Tij is the Cauchy stress deviator, and η is the viscosity coeﬃcient, which may depend on z, if the ﬂuid is non-homogeneous. Taking into account (6.4.1) the only non-zero strain rate is Drz =

1 f (r) 2

(6.4.5)

and from (6.4.4) we get for the stresses Trr = Tθθ = Tzz = σ ,

Tθz = Tθr = 0 ,

Trz = η(z)f (r) .

(6.4.6)

Since v is varying with r and assuming that this variation is of the kind shown in Fig. 6.4.6, we expect for Trz : positive if R1 < r < r0 ∂v (6.4.7) Trz = η(z) negative if r0 < r < R2 ∂r 0 for r = r0 if at r = r0 the velocity reaches a maximum and the stress Trz is zero. From the equilibrium equations written in cylindrical coordinates, since the problem is with cylindrical symmetry, follows for our case ∂σ ∂σ = = 0, ∂r ∂θ

∂Trz ∂σ Trz + + + ρbz = 0 ∂r ∂z r

(6.4.8)

where bz is the body force component. Thus σ(z) depends on z alone, and from the last equation (6.4.8) and (6.4.6) we get dσ d(rf ) + + ρbz r = 0 . (6.4.9) η dr dz Integrating once with respect to r, we get r C1 dσ + ρbz + . Trz = − dz 2 r Integrating a second time with respect to r we obtain 2 dσ r ηf + + ρbz = C1 ln r + C2 . dz 4

(6.4.10)

(6.4.11)

The integration constants can be determined from the boundary conditions A2 and A3 ηv1 + (dσ/dz + ρbz )(R22 − R12 )/4 , ln(R2 /R1 ) 2 ηv1 + (dσ/dz + ρbz )(R22 − R12 )/4 R2 dσ C2 = + ρbz − ln R2 . dz 4 ln(R2 /R1 ) C1 =

(6.4.12)

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

298

dynamic

Dynamic Plasticity

Thus the velocity distribution is obtained as 2 2 1 r R2 − r2 R2 − R12 dσ dσ + ρbz + ηv1 + + ρbz ln ηv = dz 4 ln(R2 /R1 ) dz 4 R2 (6.4.13) if the viscosity coeﬃcient is known and dσ/dz is the pressure gradient along the tube. Let us write now a global equilibrium condition for the cylinder: the projections on the z-axis of all forces acting on the cylinder are zero; i.e., gravitational force + buoyancy force + shearing force on the cylinder wall = 0. Thus R1 g(ρc − ρ + m) (6.4.14) 2 with m the “local density” of the magnetic force. With (6.4.9) this relation becomes 2 R 2 R2 R22 − R12 R1 R2 dσ + ρbz ln + 1 ln − [g(ρc − ρ + m)] ηv1 = dz 2 R1 4 2 R1 Trz |R1 =

(6.4.15) which is a relation between ηv1 , (dσ/dz) + ρbz and m. We can examine now the velocity proﬁle for open tube. First let us consider an open vertical tube (or an “inﬁnite” tube) in which can move a heavy cylinder

1.0E-03

Velocity of Fluid (m/s)

8.0E-04

6.0E-04

4.0E-04

2.0E-04

0.0E+00 5.1E-04 R1

5.6E-04

6.1E-04

6.6E-04

Radius (m)

7.1E-04

7.6E-04

8.1E-04 R2

Fig. 6.4.7 Velocity of the ﬂuid moving upward under the pressure gradient (6.4.16) which keeps the cylinder stationary.

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Flow of a Bigham Fluid

dynamic

299

and a pressure gradient exists. Let us assign various values to the pressure gradient dσ/dz in order to ﬁnd out the various possible velocity proﬁles. Example 1. From (3.14) follows that if the pressure gradient satisﬁes the relation dσ −(R12 /2) ln(R2 /R1 )[g(ρc − ρ + m)] + ρbz = dz (R12 /2) ln(R2 /R1 ) − (R22 − R12 )/4 the cylinder is stationary (v1 = 0). In other words under this pressure gradient the shearing forces of the ﬂuid ﬂowing upwards will keep stationary the cylinder. Figure 6.4.7 shows an example computed for η = 0.1014 N s/m2 (101.4 P) and dσ + ρbz = 9.36 × 104 Pa m−1 . dz The velocity distribution shown was obtained with (6.4.12).

(6.4.16)

Example 2. If the pressure gradient is greater than that obtained from (3.16), the shearing force of the ﬂuid ﬂowing up is able to move upwards the cylinder. In order to give an example, Fig. 6.4.8 is showing the velocity proﬁle of the ﬂuid for (dσ/dz) + ρbz = 1.2 × 105 Pa × m−1 . If this term reaches the value 1 × 106 Pa × m−1 the velocity of the ﬂuid in contact with the cylinder is equal with that of the cylinder itself. This case can be obtained from (3.12) by putting the condition that the maximum velocity of the ﬂuid be reached for r = R1 . Example 3. This example considers the most common case when term (dσ/dz) + ρbz has a smaller value than that obtained from (3.15). Figure 6.4.9 shows an example obtained with the value (dσ/dz) + ρbz = 8.0 × 104 Pa m−1 and same η as before. In this case most of the ﬂuid is moving upwards, but a thin layer of ﬂuids neighboring the cylinder, the ﬂuid is moving downwards. In the present example |v1 | = 0.000528 m/s (down) is obtained from (6.4.14). Example 4. The last example corresponds to very small values for (dσ/dz) + ρbz . Let us consider the case when the pressure gradient is zero dσ/dz = 0. Introducing this value in (6.4.14) together with ρg = 9.807 × 103 (kg/m2 s2 ) and same value for η as above, we get v1 = −0.00363 m/s (down). The velocity proﬁle follows from (6.4.12). This time the falling cylinder induces into the ﬂuid a shearing stress which will put it to ﬂow downwards (see Fig. 6.4.10). The velocity of the ﬂuid in contact with the tube is certainly zero. Velocity proﬁle for closed tube. Let us consider now the case when the bottom of the tube is closed and the pressure gradient is generated by the falling cylinder. We can write down the condition that the volume of the ﬂuid displaced by the falling cylinder is equal to the volume of the ﬂuid ﬂowing (up and down) between the cylinder and the tube: R2 v2πr dr = v1 πR12 . (6.4.17) R1

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

300

dynamic

Dynamic Plasticity

Fluid Velocity (m/s)

1.6E-03

1.2E-03

8.0E-04

4.0E-04

0.0E+00 5.1E-04 R1

5.6E-04

6.1E-04

6.6E-04

7.1E-04

7.6E-04

Radius (m)

8.1E-04 R2

(a)

4.0E-02

Fluid Velocity (m/s)

3.0E-02

2.0E-02

1.0E-02

0.0E+00 5.1E-04 R1

5.6E-04

6.1E-04

6.6E-04

Radius (m)

7.1E-04

7.6E-04

8.1E-04 R2

(b) Fig. 6.4.8 Velocity proﬁle from the ﬂuid ﬂowing upwards under a pressure gradient greater than (6.4.16); the ﬂuid pushing the cylinder upwards: (a) the pressure gradient slightly bigger than (6.4.17); (b) pressure gradient bigger than (6.4.16) when the velocity of the cylinder is equal with the maximum velocity of the ﬂuid (and a small plateau exists).

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

dynamic

Flow of a Bigham Fluid

301

Fluid Velocity (m/s)

6.7E-04

2.7E-04

-1.3E-04

-5.3E-04 5.1E-04

5.6E-04

6.1E-04

R1

6.6E-04

7.1E-04

7.6E-04

8.1E-04 R2

Radius (m)

Fig. 6.4.9 Under a small pressure gradient, part of the ﬂuid is moving up, but part is moving down with the falling cylinder.

Fluid Velocity (m/s)

-7.0E-04

-1.7E-03

-2.7E-03

-3.7E-03 5.1E-04 R1

Fig. 6.4.10 zero).

5.6E-04

6.1E-04

6.6E-04

Radius (m)

7.1E-04

7.6E-04

8.1E-04 R2

The velocity proﬁle in the ﬂuid generated by the falling cylinder (pressure gradient is

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

302

dynamic

Dynamic Plasticity

Fig. 6.4.11

Schematic of the ﬂuid ﬂow in the case of closed tube.

Introducing here v(= f ) from (6.4.11) we get 3 dσ r 2 R2 + ρbz + C1 r ln r + C2 r dr = v1 R12 − η R1 dz 4

(6.4.18)

with the values of C1 and C2 from (3.14) and the notations R22 − R12 1 1 ln R2 ln R1 R24 − R14 2 2 + R2 − − R1 − Σ=− 16 4 ln(R2 /R1 ) 2 4 2 4 (R22 − R12 )2 R22 R22 − R12 − ln R2 4 2 8 ln(R2 /R1 ) 1 1 ln R2 ln R1 1 R22 − − R12 − V =− ln(R2 /R1 ) 2 4 2 4 +

+

R2 ln R2 R22 − R12 + 1 ln(R2 /R1 ) 2 2

(6.4.19)

we ﬁnally obtain dσ V + ρbz = η|v1 | dz Σ

(6.4.20)

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

Flow of a Bigham Fluid

dynamic

303

which established another relationship between η v1 and (dσ/dz) + ρbz , obtained from a kinematic assumption. However, the term η v1 as obtained from (6.4.20) and from (6.4.15) must be equal. From this condition follows (R12 /2) ln(R2 /R1 )[g(ρc − ρ + m)] dσ + ρbz = . dz V /Σ − (R12 /2) ln(R2 /R1 ) + (R22 − R12 )/4

(6.4.21)

This relation determines (dσ/dz) + ρbz . The magnetic force is involved as a “local density”, i.e., if pushing down it is equivalent with a heavier cylinder. After calibration, this observation will be used to speed up some tests with very viscous ﬂuids, and using the very same magnetic cylinder. Introducing this value into (6.4.20) we obtain a formula for the determination of the viscosity coeﬃcient η: dσ Σ + ρbz . (6.4.22) η= V |v1 | dz We can consider the expression α=

(R12 /2)g ln(R2 /R1 ) Σ β 2 V Σ/V − (R1 /2) ln(R2 /R1 ) + (R22 − R12 )/4

(6.4.23)

to be a viscometer constant. We have introduced β as a correction parameter, mainly because the cylindrical magnet has sometimes no perfect cylindrical shape, and also to take into account the end eﬀects. Thus the formula for the determination of the viscosity coeﬃcient (6.4.22) writes η=α

ρc − ρ + m . |v1 |

(6.4.24)

Shearing stress distribution. The shearing stress distribution in the layer of ﬂuid is obtained from (6.4.10) with (6.4.12), as r ηv1 + ((dσ/dz) + ρbz )(R22 − R12 )/4 1 dσ + ρbz + . (6.4.25) Trz = − dz 2 ln(R2 /R1 ) r The stress becomes zero there where the ﬂuid velocity is maximum; Trz = 0 or v = vmax for r = r0 . That is obtained from 1 r0 dσ + ρbz + C1 = 0 − dz 2 r0 i.e.,

r0 =

2C1 (dσ/dz) + ρbz

(6.4.26)

which determines r0 . From the numerical examples given in this paper one can see that r0 depends strongly on the pressure gradient. Example 5. In order to check the prediction of the above formulae, we have performed experiments with a variety of standardized ﬂuids available in our laboratory.

January 12, 2007

304

10:41

Fluid

Number of Falling Cylinder samples

Average Falling Cylinder Velocity (m/s)

Average Viscosity as determined from the Theory (cp)

Standard deviation of Theoretical Value

Accuracy % (theoretical value-Brookﬁeld value)/Brookﬁeld value)

Variability % (standard deviation/ Measured value)

1

1005

16

5.25E-04

1067

87

6.169154229

8.153701968

2 3

3085 9549

17 37

1.71E-04 6.05E-05

3274 9442

241 1564

6.126418152 −1.120536182

7.361026268 16.56428723

Dynamic Plasticity

Viscosity as measured on the Brookﬁeld (cp)

Summary statistics of all samples computed both experimentally and theoretically.

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Table 6.4.1

dynamic

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

Flow of a Bigham Fluid

dynamic

305

The tests were done with a custom made falling cylinder viscometer. The viscometer data are: R1 = 0.000505 m (cylinder radius) R2 = 0.000805 m (container inner radius) 3

ρc = 7228 kg/m (cylinder density) ρf = 1000 kg/m3 (ﬂuid density) . A sample of standard 1000 cP calibration ﬂuid was measured to verify its viscosity using a cone-plate viscometer (Brookﬁeld, MA). We have tested 17 samples of this calibration ﬂuid and determined a coeﬃcient of viscosity µ = 1067 ± 87 cP compared with 1005 cP as determined by the cone-plate viscometer. The experimental viscosity coeﬃcient is 6.17% higher than the cone-plate value. Though the matching is quite good, the existing diﬀerence may be due either to the disregarding in the theory of the end eﬀects, or/and to the non-perfect cylindrical shape of the falling cylinder. However, for all practical measurements of viscosities, the accuracy is quite good. The data for all sample ﬂuids is summarized in Table 6.4.1. In order to make another check of the prediction of the above formulae, we use the experimental data given by Park and Irvine [1997] for the Canon S-60 standard

0.01 0.005 0

Fluid velocity (m/s)

-0.005 -0.01

-0.015 -0.02 -0.025

R1 -0.03 2

R2 4

6

Radius (m) Fig. 6.4.12

8 -3

x 10

Velocity proﬁle obtained for v1 = 0.02903 m/s.

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

306

Dynamic Plasticity

0.02 0.01 0

Fluid velocity (m/s)

-0.01 -0.02 -0.03 -0.04 -0.05 -0.06 2

R2

R1 4

6

Radius (m) Fig. 6.4.13

8 -3

x 10

Velocity proﬁle for v1 = 0.05251 m/s.

ﬂuid. The tests done for the falling needle viscometer are: R1 = 1.99 × 10−3 m (needle diameter); R2 = 9.525 × 10−3 m (container diameter); L = 10.2 cm (needle length); ρ = 0.8589 × 103 kg/m3 (ﬂuid density). For the needle density ρc = 1.1019 × 103 kg/m3 the terminal falling velocity recorded was v1 = 0.02903 m/s. We have determined a coeﬃcient of viscosity η = 115 cP as compared with 101.4 cP given in the Cannon speciﬁcations. It is 13% higher. The ﬂow of the ﬂuid is shown in Fig. 6.4.12. For the needle density ρc = 1.2998 kg/m3 the terminal falling velocity was found v1 = 0.05251 m/s. The determined viscosity coeﬃcients is η = 116 cP to be compared with 101.4 cP. The velocity proﬁle is shown in Fig. 6.4.13. Thus the determined viscosity coeﬃcients are about 14% higher than the Cannon speciﬁcation value. Conclusion. A simple theory is presented in which the solution of the ﬂow of a viscous ﬂuid in a falling cylinder viscometer is expressed in a closed form. The formula giving the viscosity of the ﬂuid is also obtained in ﬁnite form. Since all the formulae are obtained in ﬁnite forms, one can easily study the inﬂuence of all parameters involved [as densities (maybe variable), geometry of cylinder-tube, pressure gradient,

dynamic

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

dynamic

Flow of a Bigham Fluid

307

magnetic force, etc.] on the cylinder-ﬂuid motion. The comparison of the viscosity coeﬃcients, as determined by our experiments with the falling cylinder microrheometer and using the present theory, and as determined with a classical coneplate viscometers is quite good. It is important to note that the formulae for velocity, stress, viscosity, etc. contain a term that describes the inﬂuence of a magnetic ﬁeld on the motion of the cylinder and thus on the ﬂow of the ﬂuid. However, the inﬂuence and use of a magnetic ﬁeld in viscometer studies will be treated in a future paper. An extension of the analysis to nonhomogeneous ﬂuids, viscoplastic materials, and to the case when the ﬂuid slides along the tube and/or cylinder is to be considered in the future. Further developments. An extension of the theory for Non-Newtonian ﬂuids was done by Tigoiu and Cipu [2005]. They have in mind that some biological ﬂuids are of this kind. The velocity, in physical cylindrical components is: vr = 0 ,

vθ = 0 ,

vz = V1 f (r) ,

r ∈ [R1 , R2 ] .

(6.4.27)

The corresponding boundary conditions on both the falling cylinder and the pipe are vz (R1 ) = −V1 ,

vz (R2 ) = 0 .

(6.4.28)

It is well known that the velocity ﬁeld (6.4.27) is associated to a viscometric motion and therefore Cauchy’s stress tensor is given by ˜ 1 , A2 ) . T(x, t) = −pI + T(A

(6.4.29)

Here p is the pressure ﬁeld, I is the identity tensor, A1 , A2 are the ﬁrst two Rivlin– ˜ should be given in explicit forms in Ericksen tensors. The eﬀective stress tensor T next sections. After some calculi we obtain from (6.4.27) (A1 )rz = V1 f , (A2 )rr = 2V12 f 2 , (A1 A2 + A2 A1 )rz = 2V13 f 3 ,

(6.4.30)

A3 = 0 and all other components of A1 , A2 are null. We pass to non-dimensional variables and functions by z = H z¯ ,

r = R1 r¯ ,

f = f¯ ,

p = p0 p¯ ,

σz = ρ1 g¯ σz

and T˜ = T0 T¯ (6.4.31)

where we denote T0 ≡ η0 (V1 /R1 ). Here η0 is a characteristic shear viscosity. We remark that the velocity ﬁeld (6.4.28) satisﬁes the continuity equation and then the ﬂow problem can be written, after using (6.4.31), as

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

308

dynamic

Dynamic Plasticity

h (r) =

1 1 d ˜ (rTrr (r)) , Re r dr

1 d (rTrz (r)) = Re σz , r dr R2 f (1) = −1 , f = 0, R1

(6.4.32)

where Re ≡ (ρ1 gR12 /η0 V1 ) is a modiﬁed Reynolds number, described by means of characteristic quantities of our problem (ρ1 being the ﬂuid mass density) and where we have suppressed the overlines. For this end we remark that (∂p/∂θ) = 0. At this level of generality, the arguments are given by (6.4.29), (6.4.30) and Wang’s representation theorem for isotropic functions. Consequently p = C0 z + h(r). In (6.4.32) we have denoted σz = (p0 /ρ1 gH)(∂p/∂z) + 1 the “modiﬁed pressure gradient”. We remark that equation (6.4.32)1 leads to the determination of the pressure ﬁeld, once the eﬀective stress tensor components are known. The above mentioned components will be determined after solving the boundary value problem (6.4.32)2 –(6.4.32)3 . For this, a ﬁrst integral is simply obtained from (6.4.32) and leads to the determination of the shear stress component which, in dimensional variables, is 1 V1 C1 1 ∂p C1 η0 = + ρ1 g r + η0 V1 . (6.4.33) T˜rz (r) = σz r + 2 r 2 ∂z r The dimensional constant C1 will be independently determined for each investigated model. We remark here that the necessary condition of having a constant velocity (for the falling cylinder) is given by the global equilibrium of forces acting on the cylinder (gravitational force, buoyancy force, shearing force and magnetic force). Some elementary calculi lead to the following formula (ρc being the mass density of the falling cylinder) 1 T˜rz (R1 ) = (ρc − ρ1 + fm ) gR1 . 2

(6.4.34)

Employing (6.4.33) and (6.4.34) we obtain η0 V1 =

1 (ρc − ρ1 + fm ) g − σz } R12 . 2C1

(6.4.35)

This formula is a compatibility condition between the geometry, material and ﬂow parameter (connecting V1 , fm , η0 and σz ) and which leads to the determination of the necessary magnetic ﬁeld density fm . We remind, that the shear viscosity η on viscometric ﬂows is given by η(k) =

τ (k) , k

(6.4.36)

where k stands for the shear rate and τ (k) for the shear stress. Formula (6.4.36) is the support for the T0 expression in (6.4.31).

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

Flow of a Bigham Fluid

dynamic

309

The Third Grade Fluid Case. For the third grade ﬂuid we employ the eﬀective ˜ and constitutive restrictions as obtained in Tigoiu [1987] stress tensor T ˜ 1 , A2 , A3 ) = µA1 + α1 (A2 − A21 ) + β1 A3 T(A + β2 (A1 A2 + A2 A1 ) + β3 (trA21 )A1 , µ ≥ 0,

β1 < 0 ,

(6.4.37)

β1 + 2(β2 + β3 ) ≥ 0 ,

where µ, α1 and βi , i = 1, 2, 3 are constant constitutive moduli. Use of (6.4.37) in ﬂow equation (6.4.32)2 leads, after a ﬁrst integration, to the following non-dimensional problem f + βf 3 =

1 1 Reσz r + C1 , 2 r

f (1) = −1 ,

f (R2 /R1 ) = 0 ,

(6.4.38)

where the left term in equation (6.4.37)1 is the non-dimensional shear component of Cauchy’s stress tensor. We see that this problem has a unique solution 3 3 1 4 4 2+ 2+ + C + C C − C , (6.4.39) f (r) = 27β 27β (2β)1/3 where C ≡ C(r) ≡ ar +

C1 , r

a≡

1 Reσz 2

and β ≡

2(β2 + β3 ) 2 V1 . µR12

We remark here that, the normal force acting on the outer cylinder is given, in non-dimensional form, by Trr (R2 /R1 , z) = −Re p(R2 /R1 , z) + αf 2 (R2 /R1 ) .

(6.4.40)

The explicit formula for Trr is obtained if we introduce p(r, z) = C0 z + h(r) where h(r) is obtained from h (r) =

α 1 ∂ (rf 2 (r)) Re r ∂r

(6.4.41)

and (6.4.39). In formulae (6.4.40), (6.4.41) α stands for the non-dimensional constitutive moduli α1 , α ≡ (α1 V1 /µR1 ). The solution f (r) is ﬁnally obtained from (6.4.39) + (6.4.38)2 , after applying a shooting method (for determination of the constant C1 ), by numerical integration. The results are plotted. The Second Order Fluid Case. We consider now a falling cylinder viscometer ﬁlled with a second order ﬂuid with the shear viscosity depending on the shear rate. The corresponding constitutive law for the eﬀective stress is given by ˜ 1 , A2 ) = η(tr A21 )A1 + α1 (A2 − A21 ) , T(A

(6.4.42)

January 12, 2007

310

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Dynamic Plasticity

where we generally suppose that η is a positive, bounded and decreasing C 2 function (deﬁned on a compact set of positive numbers). For the numerical application we consider ' 2 &( 1 2 2 log(f ) + 1.7897 . η(trA1 ) = η0 exp −A(ln 10) 2 Here η0 = 102.8 Pa s is supposed to be the zero shear rate viscosity. Equation (6.4.32)1 is now given in dimensional form by 1 ∂ (rf 2 (r)) . h (r) = V12 α1 (6.4.43) r ∂r After obtaining f from the corresponding boundary value problem for (6.4.32)2 – (6.4.32)3 , the pressure ﬁeld will be determined from (6.4.43). We consider, as in the previous section, the non-dimensional ﬂow problem ∂ σ ¯z [rη(tr A21 )f (r)] = r , f (1) = −1 ; f (R2 /R1 ) = 0 . (6.4.44) ∂r Wi In (6.4.44) we denote with W i the corresponding Weissenberg number given by W i = (V1 η0 /ρ1 gR12 ). Similar to the third grade ﬂuid case, a ﬁrst integral is obtained from (6.4.44)1 as: σz C1 Trz (r) ≡ η(tr A21 )f (r) = r+ . (6.4.45) Wi r With the above mentioned properties for η, we can easily see that the equation η(X 2 )X − g(r) = 0

(6.4.46) ¯ has a unique solution X = X(r). Consequently we can uniquely express from (6.4.45) the derivative of f as a continuously diﬀerentiable function of r. Finally it results that the considered problem (6.4.44) has a unique twice continuously diﬀerentiable solution. To obtain the ﬁnal solution we will numerically solve the problem (6.4.44) for the mentioned solution of a polyisobutylene in decline. Closed Domain Case. In this section we consider the case of a third grade ﬂuid model. However, in the case of a linear viscous ﬂuid the velocity ﬁeld is analytically obtained. In almost all other cases we can not expect any analytical solutions. In order to put into evidence end eﬀects (i.e., in a closed pipe), we simulate such eﬀects by a kind of “volumetric ﬂow rate” equilibrium. The result leads to the determination of a modiﬁed pressure gradient σz necessary for the above mentioned equilibrium. With this σz the characteristics of the velocity ﬁeld (as solution of the new boundary value problem) are diﬀerent from those of the velocity ﬁeld which has been obtained in previous section. In order to do this, we write the balance of the volume of ﬂuid (per unit time) pushed downwards by the falling cylinder with the volume of ﬂuid (per unit time) ﬂowing upwards and downwards between the pipe and the cylinder. Therefore we have R2 rf (r) dr . πR12 V1 = 2πV1 R1

dynamic

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Flow of a Bigham Fluid

dynamic

311

Fig. 6.4.14 Velocity ﬁelds for a closed domain for diﬀerent values of computed apparent modiﬁed pressure gradient σz .

For a third grade ﬂuid, the obtained values for σz (corresponding to V1 = 0.00007 m s−1 , 0.000528 m s−1 and 0.00363 m s−1 , respectively) are |σz | = 90.91, 685.5 and 4713.5, respectively. The corresponding graphics for the velocity ﬁelds are shown in Fig. 6.4.14. In all graphics it is put into evidence a domain in neighborhood of the pipe in which an inverse ﬂow occurs. The three domains have practically similar dimensions, that is the point of cut oﬀ with the axe vz = 0 is almost the same in the three cases. However, the dimension of the domain is diﬀerent from the case of a linear viscous ﬂuid.

Bibliography Aleksandrov S. E., Goldshtein R. V. and Lyamina E. A., 2003, Developing the concept of the strain rate intensity factor in plasticity theory, Doklady Physics 48, 3, 131–133. Alonso E. E., Gens A. and Lloret A., 1953, The landslide of Cortes de Pallas, Spain, G´eotechnique 43, 507–521. Ashare E., Bird R. B. and Lescarboura J. A., 1965, Falling cylinder viscometer for non Newtonian ﬂuids, AIChE Jour. 11, 5, 910–916. Avitzur B., 1968, Metal Forming: Processes and Analysis, Mc Graw Hill, New York. Bertini T., Cugusi F., D’Elia B. and Rossi-Doria M., 1984, Climatic conditions and slow movements of colluvial covers in Central Italy, Proc. IV Int. Symp. on Landslaides, Toronto, Vol. I, 367–376.

January 12, 2007

312

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Dynamic Plasticity

Bird B. R., Armstrong R. C. and Hassager O., 1987, Dynamics of Polymeric Liquids, Wiley, New York. Borisov V. B., 1998, The equation for a falling-cylinder viscometer, High Temperature 36, 2, 293–298. Bridgman P. W., 1926, The eﬀect of pressure on the viscosity of forty-three pure liquids, Proc. Amer. Acad. Arts Sci. 61, 56, 57–99. Buckingham E., 1921, On plastic ﬂow through capillary tubes, Proc Amer. Soc. Testing Materials 117, 1154–1161. Cazacu O. and Cristescu N., 2000, Constitutive model and analysis of creep ﬂow of natural slopes, Rev. italiana di geotecnica 3, Luglio-Settembre, 44–54. Chan R. K. Y. and Jackson D. A., 1985, An automated falling-cylinder high pressure Laser-Doppler viscometer, J. Phys. E: Sci. Instrum. 18, 510–515. Chee K. K., Sato K. and Rudin A., 1976, Falling coaxial cylinder viscometer for polymer solutions, Journal of Applied Polymer Science 20, 1467–1474. Chen M. C. S., Lescarboura J. A. and Swift G. W., 1968, The eﬀect of eccentricity on the terminal velocity of the cylinder in a falling cylinder viscometer, AIChE Journal 14, No. 1, 123–127. Chen M. C. S. and Swift G. W., 1972, Analysis of entrance and exit eﬀects in a falling cylinder viscometer, AIChE Journal 18, No. 1, 146–149. Cristescu N., 1975, Plastic ﬂow through conical converging dies using a viscoplastic constitutive equation, Int. J. Mech. Sci. 17, 425–433. Cristescu N., 1976, Drawing through conical dies. An analysis compared with experiments, Int. J. Mech. Sci. 18, 1, 45–49. Cristescu N., 1991, Nonassociated elastic/viscoplastic constitutive equations for sand, Int. J. Plasticity 7, 41–64. Cristescu N. D., 2005, Theory of Falling Cylinder Viscometers (in print). Cristescu N. D., Conrad B. P. and Tran-Son-Tay R., 2002, A closed form solution for falling cylinder viscometers, Int. J. Engn. Sci. 40, 605–620. Cristescu N. D., Cazacu O. and Cristescu C., 2002, A model for slow motion of natural slopes, Canadian Geotech. Journal 39, 4, 924–937. Dandridge A. and Jackson D. A., 1981, Measurements of viscosity under pressure: a new method, J. Phys. D: Appl. Phys. 14, 829–831. Desai C. S., Samtani N. C. and Vulliet L., 1995, Constitutive modeling and analysis of creeping slopes, J. of Geotehnical Eng., ASCE 121, 43–56. Mc Duﬃe G. E. and Barr T., 1969, Pressure viscometer for viscosities between 1 and 104 P, The Review of Scientiﬁc Instruments 40, No. 5, 653–655. Eichstadt F. J. and Swift G. W., 1966, Theoretical analysis of the falling cylinder viscometer for power law and Bingham plastic ﬂuids AIChE Journal 6, 1179–1183. Forlati F., Gioda G. and Scavia C., 2001, Finite element analysis of a deep-seated slope deformation, Rock Mech. and Rock Engineering 34, 2, 135–159. Fu M. and Loo Z. J., 1995, J. Materials Proc. Tech. 55, 442–447. Gui F. and Irvine T. F. Jr., 1994, Theoretical and experimental study of the falling cylinder viscometer, Int. J. Heat Mass Transfer. 37, 1, 41–50. Gui F. and Irvine T. F. Jr., 1996, An absolute falling tube viscometer, Experimental Thermal and Fluid Science 12, 325–337. Hettler A., Gudehus G. and Vardoulakis I., 1984, Stress–strain behaviour of sand in triaxial tests, in Results of the International Workshop on Constitutive Relations for Soils, Grenoble, France, September 1982, Gudehus G., Darve F. and Vardulakis I. (eds.), A.A. Balkema, Rotterdam, The Nederlands, 55–66.

dynamic

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Flow of a Bigham Fluid

dynamic

313

Hild P., Ionescu I. R., Lachand-Robert T. and Ro¸sca I., 2002, The blocking of an inhomogeneous Bingham ﬂuid. Applications to landslides, Mat. Modelling and Num. Anal. 36, 6, 1013–1026. Huang E. T. S., Swift G. W. and Kurata F., 1966, Viscosities of methane and propane at low temperatures and high pressures, AIChE. 12, 5, 932–936. Irving J. B. and Barlow A. J., 1971, An automatic high pressure viscometer, Journal of Physics E: Scientiﬁc Instruments 4, 232–236. Kiran E. and Sen Y. L., 1992, High-pressure viscosity and density of n-alkanes, International Journal of Thermophysics 13, No. 3, 411–442. Kiran E. and Sen Y. L., 1995, Viscosity of polymer solutions in near-critical and supercritical ﬂuids. Ch. 9 in Viscosity of Polymer Solutions in Fluids, Kiran E. and Brennecke J. F. (eds.), ACS Symposium Series 514, Am. Ch. Soc. 1993, 104–120. Kiran E. and Gokmenoglu Z., 1995, High-pressure viscosity and density of polyethylene solutions in n-pentane, Journal of Applied Polymer Science 58, 2307–2324. Levanov A. N., Kolmogorov V. L., Burkin S. P., Katak B. R., Ashpur Iu. V. and Spasskii Iu. M., 1976, Contact Friction in the Metal Working Processes, Metallurgia Publisher, Moscow (in Russian). Lohrenz J., Swift G. W. and Kurata F., 1960, An experimentally veriﬁed theoretical study of the falling cylinder viscometer, AIChE Journ. 6, 4, 547–550. Park N. A. and Irvine T. F. Jr., 1995, Falling cylinder viscometer end correction factor, Rev. Sci. Instrum. 66, 3982–3984. Park N. A. and Irvine T. F. Jr., 1997, Liquid density measurements using the falling needle viscometer, Int. Comm. Heat Mass Transfer. 42, 3, 303–312. Paterson S. R. and Miller R. B., 1998, Stoped blocks in plutons: paleo-plumb bobs, viscometers, or chronometers? J. of Structural Geology 20, 9/10, 1261–1272. Petley D. N. and Allison R. J., 1997, The mechanics of deep-seated landslides, Earth Surface Processes and Landforms 22, 747–758. Phan-Thien N., Jin H. and Zheng R., 1993, On the ﬂow past a needle in a cylindrical tube, Journal of Non-Newtonian Fluid Mechanics 47, 137–155. Pochettino A., 1914, Su le propriet` a dei corpi plastici, Il Nuovo Cimento 8, 6th Ser., 77–108. ¨ Reiner M. and Riwlin R., 1927, Uber die Str¨ omung einer elastichen Fl¨ ussigkeit im Couette Apparat, Kolloid. Z. 43, 1–5. ¨ Reiner M., 1926, Uber die Str¨ omung einer elastichen Fl¨ ussigkeit durch eine Kapillare, Kolloid Z. 39, 80–87. Reiner M., 1960, Deformation, Strain and Flow, Wiley-Interscience, New York. Samtani N. C., Desai C. S. and Vulliet L., 1996, An interface model to describe viscoplastic behavior, Int. Jour. of Numerical and Analyt. Meth. in Geomech. 20, 4, 231–252. Swift G. W., Lohrenz J. and Kurata F., 1966, Liquid viscosities above the normal boiling point for methane, ethane, propane, and n-butane, AIChE Jour. 6, 3, 415–419. Talmon A. M. and Huisman M., 2005, Fall velocity of particles in shear ﬂow of drilling ﬂuids, Tunnelling and Underground Space Technology 20, 2, 193–201. Tanaka Y., Ohta K., Kybota H. and Makita T., 1988, Viscosity of aqueous solutious of 1, 2-ethanediol and 1,2-propanediol under high pressures, International Journal of Thermophysics 9, 4, 511–523. Tanaka Y., Xiao Y. F., Matsuo S. and Makita T., 1994, Density, viscosity and dielectric constant of HCFC-225ca and HCFC-225cb at temperatures from 293 to 323 K and pressures up to 80 Mpa, Fluid Phase Equilibria 97, 155–165. Tigoiu V., 1987, Wave propagation and thermodynamics for third grade ﬂuids, St. Cerc. Mat. 29, 4, 279–347.

January 12, 2007

314

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Dynamic Plasticity

Tigoiu V. and Cipu C., 2005, Non-Newtonian ﬂuid ﬂows in a falling cylinder viscometer, trends in applications of mathematics to mechanics, Wang Y. and Hutter K. (eds.), Proc. Of the XIVth Int. Simp. on Trends in Appl. of Math. to Mech., Seeheim, Germany, 22–28 Aug., 2004, Shaker Verlag. Tran-Son-Tay R., Beaty B. B., Acker D. N. and Horchmuth R. M., 1988, Rev. Sci. Instrum. 59, 1399–1404. Wehbeh E. G., Ui T. J. and Hussey R. G., 1993, End eﬀects for the falling cylinder viscometer, Phys. Fluids A 5, 1, 25–33.

dynamic

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

Chapter 7

Axi-Symmetrical Problems

7.1

Introduction

In previous sections we have considered cases when the boundary and initial conditions conform to the assumption that only a single component of stress and a single component of velocity occur. Sometimes, in these cases, a constitutive equation is not used at all and the procedure is somehow similar to that used in some static problems, i.e., the equation of motion and continuity condition are only combined with a yield condition but not a constitutive equation. Using this procedure a suﬃcient number of equations is obtained for the number of unknown quantities required. Sometimes else, a constitutive equation is used, but this is in fact a onedimensional stress–strain relation, and therefore as a rule, the methods used do not greatly diﬀer from those used for the study of the propagation of longitudinal waves in thin bars. In all the cases examined the propagation of a single type of wave has been considered if the equation of motion is of the hyperbolic type. Otherwise, propagation is assumed to occur by diﬀusion according to an equation of parabolic type. First let as present shortly the static, plane stress, problem (Sokolovski [1969]) when at the oriﬁce one is given a pressure. For a Mises type of yield condition 1 1 2 2 (σ − σx σy + σy2 ) + σxy = k 2 = σY2 3 x 3 the problem is hyperbolic close to the oriﬁce, but elliptic at farther distances Fig. 7.1.1. √ The characteristics are logarithmic spiral lines. The ﬁgure corresponds to p = 3k when b ≈ 5.13a. On this circle the problem is parabolic. For greater distances the problem is elliptic. For the Tresca condition, written in cylindrical coordinates σθ + σr = 2k the characteristics are logarithmic spirals up to b = a exp(p/2k), where p is the applied pressure at the oriﬁce. The Fig. 7.1.2 is obtained for p = 2k when the logarithmic spirals are until the circle r = b is reached. Further on the problem we have a single family of straight lines, the problem being parabolic. 315

dynamic

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

316

Dynamic Plasticity

Fig. 7.1.1

The characteristics for the plane stress problem satisfying a Mises condition.

Fig. 7.1.2

The characteristics for the Tresca condition.

dynamic

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Axi-Symmetrical Problems

dynamic

317

The simple problem of enlargement of circular holes in thin inﬁnite plate taking into account variations in geometry, material properties, and loading conditions, was considered by several authors. Upadhyay and Stokes [1977] have used for that a Ramberg–Osgood constitutive equation: n ' ˙ ( II II T 2n + 1 T Tij T˙ij = 2Ge˙ ij − 2 2 k IIT combined with a Mises yield condition. As remarked by Bernstein and Shokooh [1980], when subjected to creep test, aluminum exhibits characteristics which are analogous to those of thermorheologically simple material in the sense that, on a plot of logarithm of creep function versus logarithm of time, the curves corresponding to diﬀerent stresses have the same shape so that they all could be shifted to form a master curve. Based on this observation and in analogy with the idea of time-temperature superposition, a theory for viscoelastic materials is developed in which the natural time appearing explicitly in the argument of relaxation or creep function is replaced by a suitable scalar-valued function of stress tensor. A comparison between the Perzyna viscoplastic model and the Consistency viscoplastic model is due to Heeres et al. [2002]. If, in the problem considered, there occur two or three components of velocity and therefore several components of stress and strain, and the problem is dynamic, one is obliged to consider a complete constitutive equation. Several types of constitutive equations are used in theory of plasticity. This set of constitutive equations can be divided into several group, each group of constitutive equations is characterized by certain dynamic properties. In problems in which several components of velocity, stress and strain are involved, several kind of plastic waves are present. Thus, depending on the theory of plasticity used, the plastic waves are coupled (Cristescu [1956], [1967], Nowachi [1974]). The coupling of plastic waves was ﬁrst discussed many years ago. Some authors have used for this purpose constitutive equations written in ﬁnite form. First were discussed axi-symmetrical problems. That will be discussed also below. In order to analyze such problems, without overcomplicating the writing, we analyze a case in which the whole problem depends only on a single spatial coordinate, although many components of stress and strain are involved. 7.2

Enlargement of a Circular Oriﬁce

The simplest possible case is the one in which two velocity components are involved. It is assumed that along a cylindrical hole of radius r = R the radius is enlarged and rotated. Thus the radius is enlarged (velocity u) and rotated (velocity v) (see Fig. 7.2.1). It is question of sudden motion, so that the inertia forces are involved. From all the stresses involved we assume that σr , σθ , and σrθ are diﬀerent of zero, but σz = σrz = σθz = 0. There are two velocity components distinct of zero; the radial one u, and the circumferential one v.

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

318

dynamic

Dynamic Plasticity

σθ

σ rθ

0

σr

r v

r

u

Fig. 7.2.1

Enlargement of a circular hole in a plate.

We apply the Hencky–Nadai constitutive equation. For our case we have: S S σr = εr and σθ = εθ . E E The strain components are: ∂u u 1 ∂v v , εθ = , εrθ = − . (7.2.1) εr = ∂r r 2 ∂r r If we assume incompressibility we have: εr + εθ + εz = 0 , from where we obtain εz if the other two components are known. The Hencky–Nadai constitutive equation is for our case: ∂u u ∂v v S S 2 + , σrθ = − , σr = E ∂r r 2E ∂r r where E 2 = IIε = ε2r + ε2θ + εr εθ + ε2rθ ,

(7.2.2)

(7.2.3)

(7.2.4)

and the work-hardening law is written: S = F (E) .

(7.2.5)

The equation of motion, with Xr and Xθ the two body forces per unit volume are: σr − σθ ∂ 2 u ∂σr = + Xr , ρ 2 − ∂t ∂r r ρ

2σrθ ∂ 2 v ∂σrθ = + Xθ . − 2 ∂t ∂r r

(7.2.6)

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

dynamic

Axi-Symmetrical Problems

319

Introducing here (7.2.3) we get: ρ

∂ 2u ∂2v ∂2u − L − P = Φ, ∂t2 ∂r2 ∂r2

(7.2.7)

∂ 2u ∂2v ∂2v ρ 2 −P 2 −M 2 = Ψ, ∂t ∂r ∂r where L= M = P =

ES − S 2S + (2εr + εθ )2 , E 2E 3 ES − S 2 S + εrθ , 2E 2E 3

(7.2.8)

ES − S (2εr + εθ )εrθ , 2E 3

and Φ=

ES − S S εr − εθ + (2εr + εθ )[(εr − εθ )(2εθ + εr ) − 2ε2rθ ] + Xr , E r 2E 3 r

2S ES − S εrθ + εrθ [(εr − εθ )(2εθ + εr ) − 2ε2rθ ] + Xθ . Er 2E 3 r There are two waves propagating with the velocities: & c21 M + L ± (M − L)2 + 4P 2 . = 2ρ c22 Ψ=

(7.2.9)

Both are real (the expressions at the right hand side are positive). Also, c21 > c22 .

(7.2.10)

The diﬀerential relations satisﬁed on the characteristic lines are: {Φ(M − ρc2 ) − ΨP } dt − ρ(M − ρc2 )(cdur − dut ) − ρP (cdvr − dvt ) = 0 (7.2.11) where c is either c1 or c2 , and we denote ur = (∂u/∂r), etc. Let us write now the jump conditions. First the kinematics jump conditions are 2 2 ∂ u ∂ u dr = 0 , dt + ∂t2 ∂r∂t 2 2 ∂ u ∂ u dt + dr = 0 . ∂r∂t ∂r2 From here we obtain easy the kinematics jump conditions, for u and v are similar: 2 2 ∂ u ∂ u 2 (dt) − (dr)2 = 0 , 2 ∂t ∂r2 2 2 ∂ v ∂ v 2 (dt) (dr)2 = 0 . − (7.2.12) 2 ∂t ∂r2

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

320

dynamic

Dynamic Plasticity

The dynamic jump conditions are [from (7.2.7)]: 2 2 2 ∂ u ∂ v ∂ u −L −P = 0, ρ ∂t2 ∂r2 ∂r2 2 2 2 ∂ u ∂ v ∂ v − P − M = 0. ρ 2 2 ∂t ∂r ∂r2 From (7.2.12) and (7.2.13) we get easily 2 2 2 ∂ v ∂ u ∂ u 2 ρc − L −P = 0, 2 2 ∂r ∂r ∂r2 2 2 2 ∂ v ∂ v ∂ u 2 ρc − P −M = 0, 2 2 ∂r ∂r ∂r2 or we can write also:

2 ∂ v ∂2u −P = 0, (ρc − L) 2 ∂r ∂r2 2 2 ∂ u ∂ v − P = 0. (ρc2 − M ) 2 ∂r ∂r2

(7.2.13)

(7.2.14)

2

(7.2.15)

These relations are valid for both waves; we have to precise only the velocity. It is easy to show by direct computation that P ρc22 − L = − . ρc21 − L P

(7.2.16)

From (7.2.16) and (7.2.15) we get [∂ 2 u/∂r2 ]1 [∂ 2 v/∂r2 ]2 P ρc22 − L = − , = = − [∂ 2 v/∂r2 ]1 ρc21 − L [∂ 2 u/∂r2 ]2 P or,

∂2u ∂r2

1

∂ 2u ∂r2

∂2v + ∂r2 2

1

∂2v ∂r2

(7.2.17)

= 0.

(7.2.18)

2

Thus at each point the jumps are orthogonal. Both waves are coupled, i.e., they are both dilatational and shearing [see (7.2.11), (7.2.15), (7.2.17)]. Both involve the stresses σr and σrθ and also both components of the velocity u and v. From (7.2.15), if the ratio between jumps is eliminated, it follows P M − ρc2 . = 2 L − ρc P

(7.2.19)

If M > L from (7.2.19) we have (P/(ρc2 − L)) > 1, or from (7.2.17) we obtain [∂ 2 u/∂r2 ]1 > [∂ 2 v/∂r2 ]1 that is the wave “one” is mainly a dilatational one. If M < L from (7.2.19) follows (P/(ρc2 − L)) < 1, and from (7.2.17) we obtain [∂ 2 u/∂r2 ]1 < [∂ 2 v/∂r2 ]1 that is the wave “one” is primarily a shearing wave. If M ∼ = L, then both waves are equally dilatant and shearing.

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

dynamic

Axi-Symmetrical Problems

321

The coupling coeﬃcient is P , that is if P = 0 an uncoupling takes place. That can happen if: • εrθ = 0 or v = 0. The wave “one” is pure dilatational and the only propagable, with the velocity: 1 3S 2 S ∗ c1 = ε + ρ 2E 3 θ 2E 2 which becomes smaller i.e., c∗1 < c1 . • u = 0, i.e., εr = εθ = 0; the only wave which exists is the wave “two” which becomes pure shearing. For the velocity of propagation we have: c∗2 =

S 2ρε2rθ

and we have c∗2 > c1 . Therefore we have c2 < c∗2 < c∗1 < c1 . • The third case is the elastic body, i.e., ES − S = 0. The coupling factor is P . If it is present one has coupling. And we have to integrate two equations separately, as if they are not inﬂuencing each other. If it is question what is coupling the waves it is the work hardening condition (7.2.5).

7.3

Thin Wall Tube

Let us consider now the problem of a thin wall tube, loaded at one of its end by tension and torque. Thus we have two loadings, and we expect a combined load. The boundary conditions are: at x = 0 a combined loading at x = l0 the end is ﬁxed . We are using cylindrical coordinates x, r, and θ, and the displacements are u, v and w = 0. Thus the velocity components are ut , vt , and 0. The stress components

v u

l0 Fig. 7.3.1

Thin wall tube subjected to tension and torque.

x

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

322

dynamic

Dynamic Plasticity

are σr , σrθ , and σrx are assumed to be small, at least compared with σxx = σ and σθx = τ , which are dominant. We assume also axial-symmetry thus (∂/∂θ) = 0. The equations of motion are: ∂σ ∂ut + Fx = ρ , ∂x ∂t

(7.3.1) ∂vt ∂τ + Fθ = ρ , ∂x ∂t where Fx and Fθ are the corresponding body forces, and ρ is the constant density. The strains are: ∂w w ∂u εrr = = 0, εθθ = = 0, εxx = = ε, ∂r r ∂x v 1 ∂v 1 ∂u ∂w 1 ∂v = γ , εrx = + = 0 , εrθ = − = 0. εθx = 2 ∂x 2 ∂r ∂x 2 ∂r r (7.3.2) We use also the noticing 1 σ2 σ : σ = + τ2 . (7.3.3) 2 3 We introduce now the constitutive equations. We introduce one in very general form and we particularize it later on. Thus, assuming small strains, IIσ =

ε˙ = ε˙ E + ε˙ P .

(7.3.4)

For the elastic we assume the Hooke’s law:

2Gε˙ E = σ˙ , σ˙ m = 3K ε˙m .

(7.3.5)

The plastic part of the strain rate, satisfy a general constitutive equation of the form: ε˙ P = Aσ˙ + B where A is a fourth order tensor and B a second order tensor. For our case we have ε˙P ˙ xx + ϕ12 σ˙ θx + ψ1 , xx = ϕ11 σ ˙ xx + ϕ22 σ˙ θx + ψ2 . ε˙P θx = ϕ21 σ

Introducing here the Hooke’s law, these equations becomes: ∂ut 1 2 = ϕ11 + σ˙ + ϕ12 τ˙ + ψ1 , ∂x 3 E ∂vt 4 1 = ϕ21 σ˙ + 2ϕ22 + τ˙ + 2ψ2 , ∂x 3 G

(7.3.6)

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

Axi-Symmetrical Problems

dynamic

323

where σ 9KG , and σm = . 3K + G 3 In order to simplify the problem, we introduce the new notation: 1 1 1 2ϕ11 + + , α12 = ϕ12 , β1 = ψ1 , α11 = 3 G 3K E=

4 1 ϕ21 , α22 = 2ϕ22 + , 3 G with whom the constitutive equation becomes: α21 =

β2 = 2ψ2 ,

∂ut = α11 σ˙ + α12 τ˙ + β1 , ∂x ∂vt = α21 σ˙ + α22 τ˙ + β2 . (7.3.7) ∂x This is the general form of the constitutive equation. Until now we have not said what is α11 , . . . . . . etc. In order to make a discussion we consider now several particular cases. P1. Elastic. In the elastic case, we have: ϕ11 = ϕ12 = ϕ21 = ϕ22 = ψ1 = ψ2 = 0 . The constitutive equation becomes: ∂vt ∂ut = σ˙ , G = τ˙ . ∂x ∂x The two equations are completely separated and we have two kinds of waves which propagate independently. E

P2. Rate semi linear (the constitutive equation is of Malvern type). For such equations we have: ϕ11 = ϕ12 = ϕ21 = ϕ22 = 0 . The constitutive equation can be written: k σ˙ 1 1− √ σ, ε˙ = + E 3η IIσ 1 k τ˙ + 1− √ τ, γ˙ = 2G 2η IIσ

(7.3.8)

where k is the yield stress, assumed constant or not, and η is a viscosity coeﬃcient, assumed also possibly variable. P3. Piece-wise work-hardening (separated for the two components). In this case we have ϕ12 = ϕ21 = 0 .

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

324

dynamic

Dynamic Plasticity

The constitutive equations are:

1 2 σ˙ + ψ1 , ϕ11 + 3 E ∂vt 1 = 2ϕ22 + τ˙ + ψ2 . ∂x G

∂ut = ∂x

(7.3.9)

P4. The Prandtl–Reuss constitutive equation. In this case we have: ψ1 = ψ2 = 0 . The constitutive equation is in general: σ˙ ij 2G σij σij , H σmn σmn . σij σij = H σkl dεP kl 2Gε˙ij = σ˙ ij +

and

This constitutive equation particularized for the problem is: 2 1 4 1 1 2 σ σ˙ + στ τ˙ , ε˙ = + E 27 H IIσ 3 H IIσ 1 2 1 1 2 + γ˙ = τ˙ . στ σ ˙ + τ 9 H IIσ 2G H IIσ

(7.3.10)

P5. Rate quasi-linear. In this case, assuming that the strains are small, we have to start with:

P VP ε˙ij = ε˙E , ij + ε˙ij + ε˙ij σ˙ ij 1 k F (IIσ ) + 1− √ σij + σ σ˙ σij , ε˙ij = 2G 2η 2IIσ kl kl IIσ

and for the work-hardening:

P ε˙ij = F (IIσ )σkl σ˙ kl . σij

For the problem considered this law is reduced to 4 F (IIσ ) 2 k 2 F (IIσ ) 1 1 + 1− √ σ, σ σ˙ + στ τ˙ + ε˙ = E 27 IIσ 3 IIσ 3η IIσ 2 F (IIσ ) F (IIσ ) 2 k 1 1 γ˙ = + 1− √ τ. στ σ˙ + τ τ˙ + 9 IIσ 2G IIσ 2η IIσ

(7.3.11)

From here for F = 0 we obtain the rate semi linear constitutive equation, while if η → ∞ we obtain the classic plasticity theory. The velocity of propagation for P5 and P4 are variable and equal to: & c2T L α11 + α22 ± (α11 − α22 )2 + 4α12 α21 (7.3.12) = 2ρ(α11 α22 − α12 α21 ) c2LT

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

dynamic

Axi-Symmetrical Problems

325

and cT L > cLT . For the particular case P3 we have: c2L3 =

1 , ρα11

and c2T 3 =

1 , ρα22

and these velocities are also variable. For the particular cases P1 and P2 the velocities are constant and equal to: c2L1 = c2L2 =

E , ρ

c2T 1 = c2T 2 =

G . ρ

Let us consider two particular cases. If everywhere we have vt = 0, then considering again the initial equations (with ϕ12 = 0) we have a single kind of longitudinal wave which propagates with the velocity c2L0 =

3E 1 , ρ 2Eϕ11 + 3

which for the special cases P1 and P2 reduce to the elastic bar velocity. In a similar case if ut = 0 the only existing wave is the one propagating with the velocity c2T 0 =

1 G ρ 2Gϕ22 + 1

which are shearing waves and the formula is reduced to that from elastic waves in the case ϕ22 = 0. Let us consider now the diﬀerential relations along the characteristics. We have for the general case: ∓ρc(1 − ρα22 c2 ) dut ∓ ρ2 α12 c3 dvt + (1 − ρα22 c2 ) dσ + ρα12 c2 dτ + {ρβ1 c2 (1 − ρα22 c2 ) + β2 α12 ρ2 c4 ∓ (1 − ρα22 c2 ) Fx ∓ ρc3 α12 Fθ } dt = 0 . (7.3.13) Here we have to replace c by one of the four expressions (7.3.12). For the particular case P3 the diﬀerential relations are: ∓ρcL3 dut + dσ + (ρβ1 c2L3 ∓ cL3 Fx ) dt = 0 , ∓ρcT 3 dvt + dτ + (ρβ2 c2T 3 ∓ cT 3 Fθ ) dt = 0 .

(7.3.14)

For the particular case P2 they are: ( ' E Fx dt = 0 , ∓ ρEdut + dσ + β1 E ∓ ρ ∓ ρGdvt + dτ +

' β2 G ∓

G Fθ ρ

( dt = 0 .

(7.3.15)

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

326

dynamic

Dynamic Plasticity

For the particular case P1 they are: ∓ ρEdut + dσ ∓

∓

E Fx dt = 0 , ρ G Fθ dt = 0 . ρ

ρGdvt + dτ ∓

(7.3.16)

Let us write now the coupling jump conditions. We have from the constitutive equations (the brackets stand for the “jumps” of the function considered): ∂σ ∂τ ∂ut = α11 + α12 , ∂x ∂t ∂t

∂vt ∂σ ∂τ = α21 + α22 . ∂x ∂t ∂t

From the equation of motion we get: ∂σ ∂ut = , ρ ∂t ∂x Finally, we have also the relation ∂ψ ∂ψ = −c , ∂t ∂x From here we obtain:

ρ

∂vt ∂τ = . ∂t ∂x

for ψ = ut , vt , σ, τ .

∂ut 2 2 ∂vt (1 − ρα11 c ) = ρα12 c , ∂x ∂x ∂vt 2 2 ∂ut (1 − ρα22 c ) = ρα21 c . ∂x ∂x

From all those relations we conclude that α12 and α21 are the coeﬃcients that couple the wave. They are introduced by the yield condition, which are relating all stresses in a single condition. Thus we have:

P5

&

instantaneous response

non-instantaneous response

α12 = 0 ← coupling

← coupling

α21 = 0 ← P3 α =0← 12 ← P2 α 21 = 0 ← P1 P4

coupling

← no coupling

partially coupling or uncoupling ← coupling uncoupled

← coupling

uncoupled

← no coupling

A combined tension–torsion impact testing apparatus and an experimental study in the incremental wave propagation is due to Tanimura [1978]. The apparatus can realize a tension–torsion loading. To obtain a practical form of the general equation, the methods to examine the existence of the instantaneous plastic property and to

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Axi-Symmetrical Problems

dynamic

327

obtain directly the coeﬃcients of the general equation, through the experiments in which the incremental torsional impact or the incremental combined impact is applied to the tubular specimens, have been presented. By a special mechanism for clamping and quick releasing of the input bar, a combined impulse could be generated easily with a short rise time. Through an experiment in which the torsional incremental impact was applied to the tubular specimens of commercial pure aluminum and copper, it could be observed that the incremental wave velocity, just after passing through the partial unloading, was clearly smaller than the elastic wave velocity. A general study is given by Ting [1970] of plane and cylindrical wave propagation of combined stress in an elastic-plastic medium. The relations between the stresses on both sides of an elastic-plastic boundary are derived. Also presented are the restrictions on the speed of an elastic-plastic boundary. The combined longitudinal and torsional plastic waves in thin-walled tube of rate-independent isotropic workhardening material are used by Ting [1973] to illustrate the problems involved when the speeds are equal. Plastic wave speeds in materials whose elastic response is linear and isotropic while the plastic ﬂow is incompressible and isotropically workhardening are obtained also by Ting [1977]. One of the three plastic wave speeds is identical to the elastic shear wave speed regardless of the form of the yield condition. The other two plastic wave speeds are determined for materials obeying the von Mises yield condition. See also Mandel [1974]. The propagation of waves in thin tubes, subjected to longitudinal and torsional loading, was also considered by Myers and Eisenberg [1974], [1975]. They ﬁnd that the fast and slow wave speeds are 1/2 1/2 1 1 {b + (b2 − 4aA4 )1/2 } {b − (b2 + 4aA4 )1/2 } , cs = cf = 2aρ 2aρ for a constitutive equation sij 3 s, ∆)s¯˙ ] ε˙P ij = [φ(¯ 2 s¯ % s¯ 3 2 P s¯ = sij sij , ∆ = . ε˙P ij ε˙ ij dt + 2 3 E All the other coeﬃcients are variable. Integration along characteristics is also done, for solutions with or without radial inertia. The thin-walled tube was considered also by Yokoyama [2001]. He has considered various models to describe the propagation only of simple torsional waves in tubes. These were elasto-plastic, elasto-viscoplastic and elasto-viscoplastic-plastic with linear work-hardening. The constitutive equation is of the form 1 k 1 + G H τ˙ + G τ − g(γp ) τ˙ > 0 , h γ˙ = τ ˙ k + τ − g(γ ) τ˙ < 0 . p G G

January 12, 2007

328

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Dynamic Plasticity

with Hh = dh(γp )/dγp and the function h(γp ) denotes the limiting maximum dynamic shear stress-plastic shear strain curve. When τ˙ → ∞ from the ﬁrst equation we have G (γ < γY ) 1 dτ = = dγ 1/G + 1/Hh Ht (γ ≥ γY ) which is the instantaneous response curve. The integration is numerical using ﬁnite element formulation. Then one compares the velocity of propagation of the shearing strain with the tests of Yew and Richardson [1969]. One is not ﬁnding a good coincidence, since none of the considered theories, considered by the author, could predict that plastic shear strains along the axis of the thin-walled tube decrease with increasing distance from the impacted end. However one is ﬁnding that the rate dependent models give an overall better agreement with the experimental data than the rate-independent models. The smaller plastic strains are propagated with higher velocity in the torsional wave-propagation experiments than predicted by the rate-independent plastic wave theory, whereas the situation is reversed for larger plastic strains. Assuming a one-dimensional rate independent theory of combined longitudinal and torsional plastic wave propagation in thin-walled tube, restrictions are obtained on the possible speeds of elastic-plastic boundaries by Clifton [1968]. A laser-induced deformation modes in thin metal targets is considered by O’Keefe et al. [1973]. An analogy with dilatational and transverse plastic waves in a thin membrane is considered. Some experimental data are due to Hsu and Clifton [1974a] for longitudinal plastic waves propagating in thin-walled tubes of alpha-titanium. Strain-time proﬁles recorded in these experiments show evidence of (i) stress levels considerably above quasistatic values at the same strain, (ii) decay of the amplitude of the elastic precursor, and (iii) variation with distance of propagation of the speed at which a given level of strain propagates. These features of the strain-time proﬁles are interpreted as indicating that a strain-rate dependent theory is necessary to describe the observed wave phenomena. Numerical solutions based on such a theory agree reasonably well with experimental results. In another paper Hsu and Clifton [1974b] present experiments in which combined longitudinal and torsional plastic waves are generated in thin-walled tubes of alpha-titanium by subjecting pre-torque tubes to longitudinal impact. Longitudinal and torsional strain-time proﬁles are recorded at several stations along the specimen. These strain-time proﬁles exhibit features which cannot be explained within the framework of a strain-rate independent theory. The latter theory requires the wave generated under the loading employed to consist of, successively, a fast simple wave, an intermediate constant state region, a slow simple wave, and a ﬁnal constant-state region. The experiments, done by the authors, show no evidence of an intermediate constant-state region; furthermore, a ﬁnal constant-state region is not observed even though the latest times of observation are greater than the time at which, according to a strain-rate independent

dynamic

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

Axi-Symmetrical Problems

dynamic

329

theory, a constant strain-rate region is expected. Straightforward generalization of the rate-dependent theory to allow for combined stress state leads to a theory which predicts the observed strain-time proﬁles with good accuracy. The theory applied by the authors is τ˙ ∂ τ¯ ∂ τ¯ σ˙ + Φ(¯ τ , γ¯ p ) , γ˙ = + Φ(¯ τ , γ¯ p ) , ε˙ = E ∂σ G ∂τ which are giving such results. In another paper Abou-Sayed and Clifton [1976] consider the oblique impact of fused-silica target plates by A1 6061-T6 projectile plates. The equations of motion are ∂σ ∂u ∂v ∂τ = ρ0 , = ρ0 . ∂X ∂t ∂X ∂t The present analysis of the propagating waves in the fused-silica plates indicates that the main features of the normal velocity proﬁles at the free surface will be the same as for the case of uniaxial strain. The predicted velocity-time proﬁle and the rise time for the normal velocity agree closely with those measured experimentally. The predicted eﬀect of the combined loading on the normal component of the particle velocity is a shift in the ﬁnal plateau value due to the interaction between the longitudinal wave reﬂected from the free surface and the on-coming shear wave. The eﬀect of this interaction propagates back towards the free surface at the longitudinal wave speed so that the disturbance reaches the rear surface, before the arrival of the shear wave front. The shear wave front propagating in the shear-strain-free compressed region of the specimen remains non-dispersive. The initial jump in the transverse acceleration maintains its strength as it propagates inside the body. A numerical solution is presented by Abou-Sayed and Clifton [1977a] for the case of symmetric impact of two skewed plates, modeled to represent 6061-T6 Aluminum. One is considering a Perzina [1966] type of constitutive equation ε˙ij =

1+v v ∂f σ˙ ij − δij σ˙ kk + Φ(¯ τ , γ¯ p ) . E E ∂σij

The main features of the solution are, except near the impact face, the same as in previous solutions based on a rate-independent theory. Free-surface velocity-time proﬁles are obtained for the target rear surface. Results are reported by Abou-Sayed and Clifton [1977b] for experiments employing two types of oblique-plate-impact conﬁgurations. One, a symmetric conﬁguration, uses 6061-T6 Aluminum plates for both targets and projectiles. The second, an asymmetric conﬁguration, uses a 6061-T6 Aluminum projectile and a fused silica target. The experimental results are compared to analytical solutions based on an elastic-viscoplastic model for the aluminum alloy and a hyperelastic model for fused silica. The normal velocity-time proﬁle for the symmetric conﬁguration shows close agreement with the predicted one. The plastic deformation of circular membranes of strain-rate dependent, work-hardening metal is analyzed based on the strain increment theory by

January 12, 2007

330

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Dynamic Plasticity

Tobe et al. [1979]. Numerical solutions for aluminum membranes are obtained under various types of loading as well as impulsive pressure, pulses caused by underwater wire explosions. When the duration of the loading pulse is less than one-third of the time required to ﬁnish the deformation of the membrane, the deﬂection of a deformed membrane depends almost only on the impulse of the loading pulse and the instantaneous proﬁle of the membrane is found to be trapezoidal during deformation. The relation between impulse of loading and deﬂection is calculated and illustrated. The neglect of strain-rate dependency of material leads to a notable underestimation of the forming limit. In a paper written by Kim and Clifton [1980] one is using the plate impact experiment to study the material behavior at high strain rates. The results show that the transverse velocity proﬁle is clearly more sensitive to the constitutive relations than is the longitudinal velocity proﬁle. In addition, the transverse velocity proﬁle gives the relatively long time history of the ﬂow characteristics of solids, whereas the longitudinal one does not because the plastic strain rate decreases as the stress state becomes more nearly that of hydrostatic pressure. Improved agreement between theoretical predictions and results of pressure shear impact experiments appears to require improved constitutive models for plastic ﬂow. Comparisons presented here suggest that models are required which characterize plastic ﬂow characteristics accurately along loading trajectories with sharp changes in direction. The computed transverse velocity-time proﬁles have regions of steeper slope than observed in the experiments. This discrepancy appears to be mainly due to the inadequacy of the assumption of isotropic hardening and the yield function. Comparison of the various strain-time proﬁles reveals qualitative agreement in the main features, but with several characteristic diﬀerences (G¨ uldenpfennig and Clifton [1980]). First, the solution based on self-consistent slip models does not show a constant state region between the fast and slow simple waves. Such intermediate constant states regions are predicted by theories based on smooth yield surfaces, but are not observed in experiments. Second, the decrease in shear strain in early part of the wave proﬁle is greater for the self-consistent slip models than for the experiments or for the predictions of an isotropic work-hardening, smooth yield surface model. Third, for small strains, the slip-models with independent and latent hardening predict the experimental results appreciably better than either of the other models. Fourth, all models predict the late-arriving, large amplitude strains would arrive earlier than observed in the experiments. In a paper written by Chhabilidas and Swegle [1980] an experimental technique is described which uses anisotropic crystals to generate dynamic pressure-shear loading in materials. The technique has been successfully used to detect a 0.2 GPa shear wave in 6061-T6 aluminum at 0.7 GPa longitudinal stress. A viscoplastic constitutive equation of Bingham type was used by Tayal and Natarajan [1981] together with ﬁnite element method to analyze the extrusion of rate sensitive aluminum through a conical die, extrusion of superplastic alloy

dynamic

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Axi-Symmetrical Problems

dynamic

331

through a tube of uniform diameter under complete sticking conditions and extrusion of a Pb-Sn eutectic alloy through a conical die. The results are compared with experimentally measured values. A good agreement is found. Gilat and Clifton [1985] compared experimental results with predictions based on elastic/viscoplastic models of the form τ , γ¯ p ) ε˙vp ij = Φ(¯

∂f . ∂σij

The eﬀective shear stress τ¯ was taken to have the value of the plastic potential f . Two ﬂow potentials were used: 1/2 1 σ σ , f (σij ) = 2 ij ij 1/2 1 (σ − αij )(σij − αij ) f (σij , αij ) = , 2 ij where αij denotes the coordinates of the center of a yield surface that translates in ˙ γ p )nij where nij = ∂f /∂σij = (σij − αij )/2¯ τ is the direction according to α˙ ij = µ(¯ determined by unloading at various stages of, for example, a simple shear experiment in order to determine the extent of the elastic region. The plastic strain rate function Φ(¯ τ , γ¯ p ) characterizes the material’s response in simple shear. Its value during such an experiment is equal to the current value of the plastic shear strain rate. The yield surfaces are 1 (σ σ ) = k 2 (¯ γ p) for isotropic hardening , 2 ij ij 1 (σ − αij )(σij − αij ) = k02 for kinematic hardening , 2 ij where k(¯ γ p ) is the quasi-static ﬂow stress in pure shear at a plastic shear strain γ¯ p , and k0 is the initial yield stress in shear. For these models the transverse velocity predicted at the free surface is less for kinematic hardening than for isotropic hardening; such a diﬀerence was observed in all symmetric impact experiments. Better determination of Φ(¯ τ , γ¯ p ) especially for the small plastic strains that occur in symmetric impact experiments, would be helpful. The ﬂow stress increases strongly with increasing plastic strain rate at strain rates above 104 s−1 . Hydrostatic pressure up to 2 GPa appears to have no signiﬁcant eﬀect on plastic ﬂow in 6061-T6 aluminum and at most a minor eﬀect on plastic ﬂow in alpha titanium. In plate impact experiments, the elastic precursor is attenuated as it propagates through the shocked specimen due to plastic straining at the shock front. However, the plastic strain rates (Meir and Clifton [1986]) required to explain the observed precursor decay are much higher than the strain rates that are predicted for known initial dislocation densities in the unshocked specimen, regarded as homogeneous. When dislocation generation at the surfaces is included in the computations, the calculated precursor amplitudes are comparable with measurements only for thin

January 12, 2007

10:41

332

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Dynamic Plasticity

(3 mm) specimens. When subgrain boundaries are included as additional sources for dislocation generation, the computed velocity-time proﬁles at 3 and 6.6 mm are in good agreement with measured proﬁles. An analysis is presented by Klopp and Clifton [1990] concerning the eﬀect of the inclination of the waves due to the tilt, on the calculation of stress, strain, and strain rate in the specimen. The errors seem to be small. Frutschy and Clifton [1997] present some modiﬁed pressure-shear plate impact experiment to test materials at high temperatures (up to 700◦ C). The high strain rate experiment is up to 106 s−1 . In another paper Frutschy and Clifton [1998] present the dynamic response of copper at strain rates of 105 –106 s−1 and temperatures up to 700◦ C. They show that the ﬂow stress increases with increasing strain rate, and decreases with increasing temperature. They compare the experiment with some popular models, but they show that the models do not predict the softening that is observed at large strains.

7.4 7.4.1

Wire Drawing Introduction

The processes of metal extrusion or drawing have been considered within the framework of classical time-independent plasticity theory (see Avitzur [1968]). The theory considered here is to describe the inﬂuence of the speed of the process (of the order of 100 m/s) on all the other involved parameters (Cristescu [1975], [1976]). We consider mainly wires which are very thin, less than 0.5 mm in diameter. Let us assume that the main mechanical properties of the material can be described with a viscoplastic constitutive equation. Since the elastic part of the strain will be neglected the simplest possible model is a Bingham-type constitutive equation of the form σm 1 1− √ √ σij (7.4.1) Dij = 2η 3 IIσ where σm is the mean yield stress which depends on reduction and is an approximation of the isotropic work-hardening law σ ¯ = f (¯ ε) of the material, and is the positive part. Thus the model is viscoplastic rigid. A second assumption is that the circular conical die remains rigid during plastic ﬂow and that in the domain where plastic ﬂow takes place (domain II) the process is axi-symmetric. Assuming volume incompressibility the following velocity ﬁeld components in spherical co-ordinate r, θ, ϕ can be obtained cos θ 2 , vθ = vϕ = 0 , (7.4.2) v = vr = −vf rf r2 in the domain II deﬁned by r0 ≤ r ≤ rf , 0 ≤ θ ≤ α, 0 ≤ ϕ ≤ 2π. According to (7.4.2) the material particles are moving radially towards the apex 0. Since in the domain I (for r > r0 ) the whole rod is moving as a rigid body with the absolute

dynamic

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Axi-Symmetrical Problems

Fig. 7.4.1

dynamic

333

Geometry of wire drawing.

velocity v0 and since in the domain III the rod is moving again as a rigid body with the absolute velocity vf , the spherical surfaces r = r0 and r = rf are discontinuity surfaces for the velocity ﬁeld. Along the surface Γ2 (r = r0 ) the tangential discontinuity of the velocity ﬁeld is obtained from (7.4.2) as ∆v = −v0 sin θ along r = r0 ,

0≤θ≤α

(7.4.3)

while along the surface Γ1 (r = rf ) the tangential discontinuity of the velocity is ∆v = −vf sin θ along r = rf ,

0 ≤ θ ≤ α.

(7.4.4)

Another evident formulae is R . (7.4.5) sin α From (7.4.2) the following components of the rate of strain result, in spherical coordinates, cos θ cos θ ∂v v v = 2vf rf2 3 , Dθθ = = −vf rf2 3 , Dϕϕ = , Drr = ∂r r r r r (7.4.6) sin θ 1 1 ∂v Drθ = = vf rf2 3 , Drϕ = Dθϕ = 0 2r ∂θ 2 r and obviously v0 R02 = vf Rf2 ,

r=

Drr + Dθθ + Dϕϕ = 0 .

(7.4.7)

Therefore, according to the kinematical velocity ﬁeld chosen, plastic deformation takes place in region II only, while regions I and III remain rigid. Dissipation is

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

334

dynamic

Dynamic Plasticity

calculated in region II, and dissipation due to the velocity discontinuity along Γ1 and Γ2 , while along Γ3 the dissipation is produced by the friction existing there. Γ5 is stress free. The surface Γ6 (x = r0 ) at the entrance and Γ4 (x = r0 cos α) at the exit of the die are used for the computation of the balance of forces. The semiangle of the die is denoted by α, the drawing stress by σf and a possible back-stress by σb . 7.4.2

Basic Equations

For the problem under consideration, taking into account the spherical symmetry and (7.4.6), the constitutive equation can be written as σm 2 1 1− √ √ (σrr − σθθ ) , Drr = 2η 3 IIσ 3 σm 1 1 1− √ √ (σθθ − σrr ) , Dθθ = 2η 3 3 IIσ σm 1 1− √ √ σrθ . (7.4.8) Drθ = 2η 3 IIσ The second invariant of the stress deviator is 1 2 IIσ = (σrr − σθθ )2 + σrθ . (7.4.9) 3 Using (7.4.6) and (7.4.8) the expression for this invariant can be written as vf rf2 σm IIσ = √ + 3 η 11 cos2 θ + 1 . (7.4.10) r 3 Another group of equations are the equilibrium equations. Since we have σrϕ = σθϕ = 0, σθθ = σϕϕ and since the problem is axially symmetric with respect to ϕ, the set of equilibrium equations reduces to two 1 ∂σrθ 2(σrr − σθθ ) + σrθ cot gθ ∂σrr + + = 0, ∂r r ∂θ r ∂σrθ 1 ∂σθθ 3σrθ + + = 0. ∂r r ∂θ r From (7.4.6), (7.4.8)3 and (7.4.10) we get σrθ = √

σm sin θ sin θ √ + ηvf rf2 3 r 11 cos2 θ + 1 3

(7.4.11)

(7.4.12)

which satisﬁes the requirement that σrθ = 0 for θ = 0. Introducing (7.4.12) in (7.4.11)2 a diﬀerential equation is obtained, which after integration yields # $ √ 3σm 1 2 ln cos θ + σθθ = √ (7.4.13) + cos θ + C(r) 11 11 where C is a undetermined function depending on r alone.

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

dynamic

Axi-Symmetrical Problems

335

Any one from the two equations (7.4.8) taken together with (7.4.6), (7.4.10) and (7.4.13) now yields $ # √ 3σm 1 + C(r) ln cos θ + cos2 θ + σrr = √ 11 11 √ + 2 3σm √

cos θ cos θ + 6vf rf2 η 3 . (7.4.14) 2 r 11 cos θ + 1 To determine the function C for θ = 0, we obtain 4 1 σm 168 C(r) = − vf rf2 η 3 − √ ln r + C1 (7.4.15) 3 r 3 123/2 where C1 is an integration constant, which is determined from the condition r = r0 ,

θ = 0 we have σrr = σxb .

Thus it is found for C1 , $ # √ 2 3σm 14 vf rf η σm 1 − ln 1 + 1 + + √ 4.04145 ln r0 − σm , C1 = σxb − √ 11 3 r03 11 3 and for σθθ we get $ # √ vf rf2 η 4 3σm 1 14 2 σθθ = √ − ln cos θ + cos θ + + 3 11 3 r3 r0 11 $ # √ 3σm r0 1 σm − σm ln 1 + 1 + + √ 4.04145 ln + σxb − √ r 11 3 11

(7.4.16)

and a similar procedure can be used to determine σrr . This is an approximate value since we have not taken into account the friction. We have to compute now the stress power per unit volume 2σm IID + 4ηIID , (7.4.17) σij Dij = √ 3 where 1 1 2 2 2 2 2 2 IID = Dij Dij = (Drr + Dθθ + Dϕϕ ) + Drθ + Dθϕ + Dϕr . (7.4.18) 2 2 Using (7.4.6) in (7.4.17) and (7.4.18) we get v 2 r4 η 2σm vf rf2 2 θ + 1 + f f (11 cos2 θ + 1) . 11 cos σij Dij = √ r6 3 2r3 After integrating over the volume of zone II, and using (7.4.5): ˙ = 2πσm vf Rf2 ln R0 f (α) + 2 πvf2 Rf η W Rf 3 sin α # $ 3 Rf 11 × 1− 1 − cos α + (1 − cos3 α) , R0 3

(7.4.19)

January 12, 2007

10:41

336

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

dynamic

Dynamic Plasticity

where

# $ √ 11 1 1 1 1 + ln cos α + cos2 α + (cos α) cos2 α + −f (α) = √ 11 11 11 2 3 sin2 α # $& 12 12 1 − ln 1 + . (7.4.20) − 11 11 11

The ﬁrst term is the time independent while the second term in (7.4.19) corresponds to the time dependent term. 7.4.3

Friction Laws

We ﬁrst consider a Coulomb friction law τ = µσθθ .

(7.4.21)

Here µ is the constant friction coeﬃcient and σθθ is the stress normal to the die surface. Since the velocity along the surface is cos α v = −vf rf2 2 r the rate of the work done by the stress vector on conical die surface Γ3 (r0 ≥ r ≥ rf , θ = α) is rf cos α ˙ σθθ vf rf2 2 2πr sin α dr . WΓ3 = −µ r r0 Introducing here (7.4.16) and after some algebra, we get # 3 $ 2 σm R 4 sin α R0 f 2 ˙ Γ3 = −2µπvf R cot α √ v 1 − − η 2.0207 ln W f f 9 Rf R0 Rf 3 ( #√ ' 2 3σm 14 1 sin α Rf 2 √ − vf η ln cos α + cos α + + σxb 11 3 R0 R0 11 ( $& ' √ 3σm 1 − σm . (7.4.22) ln 1 + 1 + − √ 11 11

Rf + ln R0

Another law in metal plasticity is that the modulus of shearing stress due to √ friction is proportional to the yield stress τY = σY / 3. For viscoplastic materials this law is generalized as (7.4.23) τ = m IIσ where m is a constant friction coeﬃcient and 0 ≤ m ≤ 1. m = 0 means no friction, while m = 1 means adherence on the wall. Using (7.4.10) (7.4.23) can be written $ # vf rf2 σm (7.4.24) τ = m √ + 3 η 11 cos2 α + 1 . r 3

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

Axi-Symmetrical Problems

dynamic

337

With this law the rate of work done on the conical die surface is # $& 3 cos α η sin α σ R v R m f f f ˙ Γ3 = 2πmvf R2 √ ln + 11 cos2 α + 1 −1 . W f sin α 3Rf R0 3 R0 (7.4.25) Let us observe that both expressions are variable depending on vf , η and α. The dependency on r is distinct; in the law (7.4.21) it decreases with decreasing r, while in the law (7.4.23) it increases with increasing r. We assume all the other parameters to stay constants. 7.4.4

Drawing Stress

We apply now the theorem of powder expanded, extended to the volume V of the viscoplastic domain. We have σij Dij dV + σi [vi ] dS + σi [vi ] dS = σi vi dS , (7.4.26) Γ1

V

Γ2

∂V

where σi is the component of the stress vector on Γ1 , Γ2 or ∂V while [v] is the jump of the particle velocity at the crossing of the surface Γ1 or of the surface Γ2 . The term on the right-hand side of (7.4.26) represents the rate of work done by the stress vector on the surface bounding the volume V . This term can be decomposed into ﬁve parts. On the plane Γ6 where x = r0 we have ˙ Γ6 = −πR02 v0 σxb , W

(7.4.27)

˙ Γ4 = πR2 vf σxf . W f

(7.4.28)

while on Γ4 where x = rf ,

Along Γ5 the rate of work is zero since this surface is stress free. Along the surfaces where a friction law exists the integral is already computed. Let us consider now the last term from right. The velocity discontinuity is [v] = v0 sin θ. The surface element is dA = rj2 sin θ dθ dϕ . Thus

σi [vi ] dA =

Γ2

α

σi τi sin2 θ dθ

2πv0 r02

(7.4.29)

0

where τi is the vector tangent to Γ2 in the meridian plane. From the global condition of equilibrium of the forces which act on the domain I of the bar we have dA = 0 −πσ0 R02 + σ0∗ Γ2

we determine σ0∗ =

σ0 σ0 R02 = (1 + cos α) . − cos α) 2

2r02 (1

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

338

dynamic

Dynamic Plasticity

Introducing this value in (7.4.29) we get 2 σi [vi ] dA = −(1 + cos α)πv0 r0 σ0 Γ2

or

σi [vi ] dA = − Γ2

α

sin3 θ dθ

0

− cos α + 1/3 cos3 α + 2/3 πv0 R02 σ0 . 1 − cos α

Similar for the surface Γ4 we get 1 2 3 σi [vi ] dA = πvf rf σf (1 + cos α) (1 − cos α) + (1 − cos α) . 3 Γ4

(7.4.30)

(7.4.31)

Combining all these formulae, for the second friction law, we have − cos2 α + (1/3) cos3 α + 2/3 sin2 α σf σb 1 + 2 = σm 2 cos α − cos2 α − (2/3) cos3 α − 1/3 σm sin2 α # 3 $ 1 Rf 11 2 ηvf R0 1− 1 − cos α + (1 − cos3 α) + + 2f (α) ln Rf 3 σm Rf sin α R0 3 # 3 $&& R0 ηvf sin α R 2 f √ + 11 cos2 α + 1 1 − + √ mctgα ln Rf σm Rf R0 3 3 +

2 L σY m 3 Rf σm

(7.4.32)

where

' ( √ 11 1 1 1 1 + ln cos α + cos2 α + −f (α) = √ (cos α) cos2 α + 11 11 11 2 3 sin2 α −

' (& 12 12 1 − ln 1 + . 11 11 11

and N=

ηvf σm Rf

(7.4.33)

is a “speed eﬀectiveness parameter” expressing the inﬂuence of the speed on the energy dissipated in the domain of viscoplastic deformation. Further the term containing the factor m expresses the energy dissipation due to friction; in this term a component due to the speed inﬂuence is also present. The ﬁnal term in Eq. (7.4.32) is due to the friction along the die land of length L. In the same equation the dissipation term due to the presence of discontinuity surfaces Γ1 and Γ2 is also involved, but not additively. Since the rates of deformation involved in viscoplastic deformation in region II are very high, the resultant heating was also considered (Cristescu [1980]), in order

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Axi-Symmetrical Problems

dynamic

339

to be able to choose the values of the various constants from the constitutive equation correctly. It was assumed that the heating is adiabatic, that is " dT "" ρc " = σij Dij dV (7.4.34) dt med V where c is the speciﬁc heat (assumed constant), T is the temperature and dT /dt|med is the mean temperature gradient over the volume V , deﬁned by " dT dT "" 1 dV. = " dt V dt med

V

On the right-hand side of (7.4.34) is the stress power over the volume V , which is given by the above formula. This equation becomes # 3 $ R N R 2 0 f " 2f (α) ln 1− + 2 " R σ πv dT " f f m Rf 3 sin α R0 . = " dt med V ρc 11 3 × 1 − cos α + (1 − cos α) 3 This equation was used to estimate the mean rise of temperature due to fast viscoplastic deformation. For steel wire and R0 = 0.5 mm, vf = 1 m/s, α = 6◦ , η = 0.34 Nmm−2 s, ρc = 3.60 Nmm−2 (◦ C)−1 , r% = 20%, an approximate mean temperature rise of ∆Tmed = 84.0◦ C (28.2◦ C due to plastic deformation and 55.8◦ C due to the speed eﬀect), is obtained, estimating that the particles cross region II in a time interval less than 5 × 10−4 s. For vf = 50 m/s and η = 0.023 Nmm−2 s, the mean temperature rise due to viscolastic deformation is ∆Tmed = 121◦ C (29.6◦ C due to plastic deformation and the remaining due to the speed eﬀect). Another estimation of temperature rise was done by integrating numerically the equation (7.4.34). This is no more done since the temperature rise is less than 150◦ C at the most and thus do not change the constants of the materials signiﬁcantly. 7.4.5

Comparison with Experimental Data

We have chosen the experimental data by Wistreich [1955] for copper wires with Rf = 1.27 mm and mean yield stress of σY = 349.7 MN/m2 have been drawn at a speed of vf = 33 mm/sec, the friction coeﬃcient is µ = 0.025. The viscosity coeﬃcient for copper was taken from Lindholm and Bessey [1969] η = 2.78 MN/m−2 from where N = 0.2069. For these values of the constants, the results shown in Fig. 7.4.2 were obtained. For various reductions in area deﬁned by # 2 $ Rf r% = 100 1 − R0 the variation of the drawing stress with semi-cone angle α is plotted. The discrepancy with experimental data existing for α relatively big and/or r small is due to the bulging phenomenon.

January 12, 2007

10:41

340

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Dynamic Plasticity

Fig. 7.4.2 Variation of drawing stress with semi-cone angle for various reductions in area: comparison between theory and experiment.

Fig. 7.4.3

Total drawing force for various reductions and area and three semi-cone angles.

dynamic

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Axi-Symmetrical Problems

dynamic

341

Fig. 7.4.4 Variation of relative drawing stress and optimum die angle with the speed eﬀectiveness parameter N , for diﬀerent degrees of reduction.

Another comparison with experimental data has been done for the total drawing force as measured by Wistreich for semi-cone die angles equal to: 2.29◦ , 8.02◦ and 15.47◦. These experimental results are shown in Fig. 7.4.3 together with the theory. For mild steel Manjoine (see Lindholm and Bessey [1969]) and Cristescu [1977] give D ≈ 10−1 –1 s−1 , η ≈ 104 kNm−2 s, for D ≈ 1–10 s−1 , η ≈ 1700 kNm−2 s, for D ≈ 10–102 s−1 , η ≈ 200 kNm−2 s, and for D ≈ 102 –103 s−1 , η ≈ 24 kNm−2 s. For higher rates of deformation Campbell [1973] suggests η ≈ 2 kNm−2 s and it is varying very little. Let us observe that an increase of vf does not imply an increase on N , since η may decrease signiﬁcantly with the increase of vf . In the example given below, σb = 0 and L = 0, the consideration of these two parameters can be done very easily. In Fig. 7.4.4 are given for three reductions, the optimum relative drawing stress for diﬀerent values of N (full lines). From this ﬁgure it can be seen that the drawing stress increases with reduction and become large for very thin wires. A comparison with the experiments was done also by Cristescu [1977] for copper of diameter wires 2R0 = 0.94 mm and steel wires of 2R0 = 1.02 mm, tested slowly.

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

342

Dynamic Plasticity

Fig. 7.4.5

Drawing forces for copper wires.

For the die semi-angle α = 8◦ , the length of the land L = 0.5 mm, friction coeﬃcient on the land m = 0.08, friction on the conical surface µ = 0.09, and viscosity of the copper η = 2.94 Nmm−2 s. Figure 7.4.5 shows some results for α = 8◦ (smaller ﬁgures) and α = 7◦ . That is because α = 8◦ is closer to the optimum die angle. The lines are the theoretical ones. The ﬁgure corresponds to L = 0.5 mm, µ = 0.06, m = 0.08, and η = 2.94 Nmm−2 s. Similar results for steel wires. 7.4.6

Other Papers

A visio-plastic method, for big deformations, was developed by Dahan and Le Nevez [1983]. First some extrusion pieces are obtained and measured. Then by a ﬁnite diﬀerence one is obtaining for a rigid work-hardening and isotropic material, the stress deviator and the strain. Also a Bingham model was used by Ionescu and Vernescu [1988], to describe numerically the wire drawing. The friction conditions are of two types: a Coulomb friction law and a viscoplastic one. The drawing speeds is low, with the viscosity coeﬃcient 2.94 Ns/mm2 .

dynamic

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

Axi-Symmetrical Problems

dynamic

343

The same theory was presented in a book devoted to “Mathematical Models in Working Metals” by Camenschi and S ¸ andru [2003]. The book contains much more than drawing of bars but this theory is presented. In reality the book presents some papers published since 1978. For instance the drawing of bars with asymptotic developments was ﬁrs published in Camenschi et al. [1979] for a friction law of the form (7.4.23) and in Camenschi et al. [1983] for a Coulomb friction law. Concerning the drawing theory one is assuming N < 1, that is slow processes. The solution is obtained for the incompressibility condition by introducing the ﬂow function ψ = ψ(r, θ) = R22 vf ψ 0 (r0 , θ), and vr0 = − where the upper index ments one is writing

0

r02

∂ψ 0 1 , sin θ ∂θ

vθ0 = −

r0

1 ∂ψ 0 sin θ ∂r0

is for dimensionless magnitudes. For asymptotic develop-

ψ 0 (r0 , θ) = ψ00 (θ) + N ψ10 (r0 , θ) + O(N 2 ) , p0 (r0 , θ) = p00 (r0 , θ) + N p01 (r0 , θ) + O(N 2 ) . and the solution is obtained in dimension quantities with a formula for the stress as well. One is obtaining the drawing force as # $ 3 R1 R23 2 |σf | 1 − 3 F (α, m) + N ln =√ G(α, m) σY R1 R2 3N where one have used the friction law (7.4.23) and m , γ= √ 1 − m2 α sin2k−1 θdθ % Ik = , 0 1 − sin2 θ(λ1 − λ2 sin2 θ)

k = 1, 2, 3

√ 3γ( 3 sin 2α − 3γ cos 2α + 2γ) √ , λ1 = sin2 α( 3 cos α + 3γ sin α)2 6γ 2 √ , sin α( 3 cos α + 2γ sin α)2 √ (cos3 α/2)(2γ + 3 sin 2α) √ F (α, m) = , γ(sin α/2)(1 + 2 cos α) + 3 cos α cos(α/2) √ (m/3) cos α sin2 α − sin α(γ sin α − (2/ 3) cos α)I1 √ G(α, m) = (1 − cos α)[sin 2α − (γ/ 3)(1 − cos α)(1 + 2 cos α)] √ √ (γ( 3 sin 2α + 6γ cos 2α − 4γ)I2 + 4γ 2 I3 )/( 3 sin 2α + 6γ sin2 α) √ − . (1 − cos α)[sin 2α − (γ/ 3)(1 − cos α)(1 + 2 cos α)] λ2 =

2

January 12, 2007

344

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Dynamic Plasticity

The authors have determined also several optimum angles for the drawing, depending on friction, reduction and N . They have also considered a Coulomb friction law in Camenschi et al. [1983]. The same authors, S¸andru and Camenschi [1979] have considered the rolling of a material, by assuming that the rolls can be approximated by two straight lines. They apply an asymptotic series development. The kinetic and dynamic eﬀects, on the upper bound loads in metal forming processes, are due to Tirosh and Kobayashi [1976]. It is question of forging, extrusion and piercing. The same kind of approach was applied for rolling of viscoplastic materials (Tirosh et al. [1985]). Since the arc of contact area is practically small (α ≈ 5 deg) and the thickness of the sheet is small with respect to the roller diameter, the authors replace the arc of the contact area by a straight line. The strains are σm σrr − σθθ 1 1− √ √ , Drr = 2η 2 3 IIσ σm 1 1− √ √ τrθ , Drθ = 2η 3 IIσ and repeat the theorem of powder expansion and also with the same friction laws. The comparison with the tests seems good. Comparisons with experiments and with FEM are done. For instance in Fig. 7.4.6 a comparison with the data by Shida and Awazuhara [1973] and the FEM method by Li and Kobayashi [1982] are done. In another paper by Iddan and Tirosh [1996] one renounces at this assumption. The dynamic fracture by spallation in metals was considered by Gilman and Tuler [1970]. The stress state associated with plane strain is described, and the eﬀect of the initial conditions and the time dependent conditions of the material on spallation is discussed. Fu and Luo [1995] consider the rigid-viscoplastic FEM to analyze the viscoplastic forming process. The general rigid-viscolastic FEM formulation is given and speciﬁc formulations of isothermal forging processes and superplastics forming are listed also. As an application, the combined extension process of pure lead, which is strain-rate sensitive at room temperature, is analyzed. The simulated results reveal the variation of the forming load with the stroke and its dependence on conditions. On the basis of the metal ﬂow patterns deﬁned by the rigid-viscoplastic ﬁniteelement method, the change of the position of the neutral layer is given and it is found that the occurrence of folding at the ﬂange may be attributed mainly to an abnormal ﬂow pattern. Moreover, the calculated results bring to light the rule of deformation distribution and its dependence on strain rate. Alexandrov and Alexandrova [2000], assuming a rigid viscoplastic material model, show that the velocity ﬁelds adjacent to the surfaces of maximum friction must satisfy sticking conditions. This means that the stress boundary conditions, the maximum friction law, may be replaced by the velocity boundary condition.

dynamic

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Axi-Symmetrical Problems

Fig. 7.4.6 for steel.

dynamic

345

Comparisons between measured, predicted, and computed roll force versus reduction

For planar ﬂows, they show that plastic deformation in the vicinity of maximum friction surfaces is possible. The metal forming processes of aluminum-alloy wheel forging at elevated temperature are analyzed by the ﬁnite element method by Kim et al. [2002]. A coupled thermo-mechanical model for the analysis of plasic deformation and heat transfer is adapted in the ﬁnite element formulation. The rolling problem is not mentioned in the present book. We would like to mention the paper by Angelov [2004] in which a variational analysis of a rigidplastic rolling problem was considered. The material is rigid-plastic, strain-rate sensitive and incompressible. A nonlinear friction law is considered.

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

346

7.5 7.5.1

Dynamic Plasticity

Floating Plug Formulation of the Problem

In the present text the geometry of the ﬂoating plug is studied in order to optimize the tube drawing process, i.e., in order to increase the drawing speed, to increase the reduction per pass, to reduce the consumption of energy used, etc. For this purpose the theory of fast tube drawing with ﬂoating plug is formulated and a formula is given expressing the drawing stress as function of various parameters involved in the drawing process (drawing speed, semi-cone die angle α, tube geometry, mechanical properties of the material, friction coeﬃcients and plug geometry). Some data, mainly of experimental character and of industrial practice can be found in Bisk and Shveikin [1963] and Perlin [1957]. From the experiments described in these books it results that when the drawing speed is increased from 20 m/min to 60 m/min the drawing force increases several times (two or even three times). The signiﬁcant inﬂuence of the speed on the wire drawing process was mentioned. Since the rates of strains are higher than 102 s−1 , one has to describe theoretically this process with a viscoplastic constitutive equation (Cleja and Cristescu [1979]). Due to the geometrical symmetry of the die, plug and of the tube the problem can be considered to be axisymmetrical. For this reason the geometry of the deformation process was represented in Fig. 7.5.1 in a symmetry plane. The tube of initial thickness R1 − R3 enter in the die with the speed v0 and leaves it with the speed vf . The thickness of the tube at the exit is R2 −R4 . Three domains can be distinguished: in domains I and III the material is assumed rigid, while in domain II the viscoplastic deformation takes place and a Bingham type of constitutive equation

Fig. 7.5.1

Geometry of ﬂoating plug.

dynamic

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

Axi-Symmetrical Problems

dynamic

347

σm 1− √ √ σij (7.5.1) 3 IIσ is satisﬁed. Here again σm is the “mean” yield stress, i.e., the area under the universal stress–strain curve divided by the equivalent strain, while 1 Dij = 2η

Z =

Z

if Z > 0

0

if Z ≤ 0 .

(7.5.2)

It is assumed that the domains previously mentioned are separated by the discontinuity surfaces Γ1 and Γ2 . Generally it is assumed that one of the two curves Γ1 or Γ2 has a prescribed shape and the second one is then determined accordingly. In what follows Γ2 is taken as an arc of a circle of radius r2 . It will be assumed that in the domain II the material ﬂows radially towards the pole 0 situated at the distance x from the symmetry axis; in what follows x is to be determined. Here we will determine the semi-angle γ of the ﬂoating plug. From the point of view of the optimization of the drawing process, this angle is a fundamental parameter of the geometry of the ﬂoating plug. Let V be the domain ﬁlled up with the viscoplastic material and Γ = Γσ ∪ Γv = ∂V , where Γσ is the portion of the boundary where the stress vector is prescribed and Γv the one on which the velocity ﬁeld is prescribed. Let v be a kinematic admissible ﬁeld (i.e., div v = 0 in V and v|Γv = v0 ). We denote by D the set of kinematic admissible ﬁelds on V . Then the functional 2 ) 1 σm σ ij Dij + √ IID dV + [t · v] dσ J(v) = 2 3 V j=1 Γj

X · v dV −

−

t · v dσ

(7.5.3)

Γσ

V

is minimized. Here [f ] = f + − f − is the jump of f at the crossing of the considered surface. Let Dγ ⊂ D0 be a family of kinematic admissible ﬁelds depending on a parameter γ. The kinematic ﬁeld which corresponds to that value of γ for which J(v) on Dγ is minimum will be determined. 7.5.2

Kinematics of the Deformation Process

From r2 sin α = R2 − x ,

r2 sin γ = R4 − x

(7.5.4)

the following expression for x x= and for r2

R2 sin γ − R4 sin α sin γ − sin α

(7.5.5)

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

348

dynamic

Dynamic Plasticity

r2 =

R2 − R4 R2 − x = sin α sin α − sin γ

(7.5.6)

are obtained. The relation between the velocities v0 at the entrance and vf at the exit is obtained as R2 − R42 vf . (7.5.7) v0 = 22 R1 − R32 Writing now the condition of equal rates of ﬂow for a circular annulus comprised at the entrance between radii r1 (θ) sin θ + x and R3 and at the exit between r2 sin θ + x and R4 , the equation of the discontinuity surface Γ1 & 2 − R2 1 R 1 3 r1 (θ) = [(r2 sin θ + x)2 − R42 ] 2 + R32 − x (7.5.8) sin θ R2 − R42 is obtained. Here r1 (θ) can be either a decreasing or increasing function of θ. In order to determine a kinematic admissible velocity ﬁeld we introduce the curvilinear coordinates θ, r, ϕ by X = (r sin θ + x) cos ϕ ,

Y = (r sin θ + x) sin ϕ ,

Z = −r cos θ

(7.5.9)

where X, Y, Z are the Cartesian coordinates of a point P belonging to the domain II, the OZ axis is the symmetry axis, and θ ∈ [γ, α], r ∈ [r2 , r1 [θ]], ϕ ∈ [0, 2π] (see Fig. 7.5.1 which corresponds to ϕ = 0). Denoting by vr , vθ and vϕ the components of the particle velocity in the curvilinear coordinates chosen, and taking into account that due to symmetry vθ = vϕ = 0, from the incompressibility condition, we get C(θ) vr = r(r sin θ + x) where the function C(θ) is determined from the continuity of the normal component of the velocity at the crossing of the surface Γ2 , i.e., for r = r2 : vr = vf cos θ. The following velocity ﬁeld is thus found r2 (r2 sin θ + x) vr = vf cos θ , θ ∈ (γ, α) , r ∈ (r2 , r1 (θ)) r(r sin θ + x) vθ = vϕ = 0 .

(7.5.10)

The components of the rate of strain are Drr = −vf r2 (r2 sin θ + x) cos θ

2r sin θ + x , [r(r sin θ + x)]2

Dθθ = vf r2

r2 sin θ + x cos θ , r2 (r sin θ + x)

Dϕϕ = vf r2

r2 sin θ + x cos θ sin θ , r(r sin θ + x)2

Dθr = −vf r2

r(r2 sin θ + x) + x2 sin θ − xr2 cos 2θ , 2r2 (r sin θ + x)2

Dθϕ = Dϕr = 0 .

(7.5.11)

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

dynamic

Axi-Symmetrical Problems

With these formulas the second invariant of the rate of strain tensor is 2 vf r2 (Ar2 + Br + C) , 2IID = Dij Dij = 2 r (r sin θ + x)2

349

(7.5.12)

where 1 A = 6 cos2 θ sin2 θ(r2 sin θ + x)2 + (r2 sin3 θ + x)2 , 2 B = 6x sin θ cos2 θ(r2 sin θ + x)2 + x(r2 sin3 θ + x)(x sin θ − r2 cos 2θ) , x2 [x sin θ − r2 cos 2θ]2 . (7.5.13) 2 With the help of the invariant IIε for the Bingham model the stress power can be expressed as 2σm σij Dij = √ IID + 4IID , (7.5.14) 3 C = 2x2 cos2 θ(r2 sin θ + x)2 +

where σij are the stress components. For the whole volume V of the domain II deﬁned by θ ∈ (γ, α), r ∈ (r2 , r1 (θ)), ϕ ∈ [0, 2π], using (7.5.12)–(7.5.14) we get 4πσm σij Dij dv = √ vf r2 I1 (γ, α; r2 , r1 (θ)) + 4πη(vf r2 )2 I2 (γ, α; r2 , r1 (θ)) , 6 V (7.5.15) where the following notations

α

r1 (θ)

I1 (γ, α) = γ

and

r2

α

r1 (θ)

I2 (γ, α) = γ

r2

√ Ar2 + Br + C drdθ r(r sin θ + x) Ar2 + Br + c drdθ r3 (r sin θ + x)3

(7.5.16)

(7.5.17)

were used, together with the Jacobian of (7.5.9). 7.5.3

Friction Forces

Friction forces are involved at the interfaces between the tube and die and between the tube and the plug. On the conical surface of the plug it will be assumed that the friction between the rigid surface of the plug and the viscoplastic body, can be described by |tτ | = m IIσ = k + 2η IID . (7.5.18) The friction force T2 between the tube and the plug land at exit, Γ9 (see Fig. 7.5.1) has the direction k and the modulus |T2 | = 2πm2 τ2 lR4

(7.5.19)

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

350

dynamic

Dynamic Plasticity

where m2 is the friction factor, τ2 is the actual shearing yield stress of the tube at the exit while l is the length of the plug land at the exit. The resultant of the normal forces on the conical portion of the ﬂoating plug (θ = γ) has the modulus r1 (γ)−ε Tθθ |θ=γ (r sin γ + x) dr , (7.5.20) Nγ = 2π r2

Tθθ being the normal component on the conical portion of the plug. The contact between the tube and the plug, on the conical portion, is expressed by a relationship between r2 and r1 (γ) − ε with a = ε sin γ, representing the clearance between the maximum diameter of the plug and the inside diameter of the tube at entrance. The magnitude of Tθθ will be obtained assuming that the friction law (7.5.18) is giving the same tangential stress with the one given by a law of Coulomb type |tτ | = µ|Tθθ |, µ being the corresponding friction factor. Thus µTθθ = m4 IIσ . (7.5.21) This suggestion is done by the computations done at the bar. On the conical portion of the plug the modulus of the friction force is r1 (γ)−ε Tγ = 2πm4 IIσ |θ=γ (r sin γ + x) dr . (7.5.22) r2

The equilibrium condition of all the forces which act on the ﬂoating plug is Nγ + T2 + Tγ = 0

(7.5.23)

since the cylindrical portion of the plug, of radius R3 , is not in contact with the interior of the tube. Projecting now (7.5.18) on the symmetry axes of the plug and using (7.5.19), (7.5.20) and (7.5.22), we obtain the following equation which determine m4 τ2−1 sin γ − cos γ I3 (γ; r2 , r1 (γ) − ε) (7.5.24) l= m2 R4 µ with the notation

I3 (γ; r2 , r1 (γ) − ε) =

r1 (γ)−ε

IIσ |θ=γ (r sin γ + x) dr

r2

=

1 k sin γ[(r1 (γ) − ε)2 − r22 ] + xk(r1 (γ) − ε − r2 ) 2 r1 (γ)−ε + 2η IID |θ=γ (r sin γ + x) dr . (7.5.25) r2

In the next paragraph we ﬁrst determine the value of γ which minimize the functional J(v) and which is used to determine the length l of the cylindrical part of the plug.

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

Axi-Symmetrical Problems

7.5.4

dynamic

351

Determination of the Shape of the Floating Plug

For the problem considered here the functional J(v) on Uad (γ) becomes a function of γ j(γ) = 2πvf

√ 1 π(R12 − R32 ) σ0 (R22 − R42 ) − I5 + 2kr2 I1 (γ, α) 2 A(S1 )

+ km3 r2 R2 ln + ηvf r22

r1 (α) r1 (γ) − ε cos α + km4 r2 R4 ln cos γ r2 r2

*√ 2m3 R2 I4 (α, r2 , r1 (α)) cos α

+ √ + 2m4 R4 I4 (γ, r2 , r1 (γ) − ε) + I2 (γα) + m2 τ2 lR4 + m1 τ1 LR2

(7.5.26)

with the notations Ij introduced by the formulae (7.5.16) and (7.5.17) and A(S1 ) is the area of the surface S1 . Proof. For the computation of J(v) on Uad (γ) we use the formula divσ + ρb = 0 and we observe that the integrals on the volume are computed by (7.5.15)–(7.5.17), with the remark that I2 is now multiply with 1/2. The surfaces Sj involved, correspond to the values j = 3, 5–12, while the surfaces Sk , correspond to the value k = 1, 4. S2 is not involved in the computation of J(v) since on this surface the stress vector is not known. On the surface S3 — since Γ3 is a ﬂow line — the speed has the tangential component equal to vr , and the modulus of the tangential vector of the stress is given by (7.5.18). Thus r1 (α) t · v dA = −2πm3 vr IIσ |θ=α (r sin α + x) dr . (7.5.27) S3

r2

With (7.5.10) this relation becomes t · v dA = −2πm3 vf r2 R2 I6 (α; r2 , r1 (α)) cos α

(7.5.28)

S3

with the notation

r1 (α)

I6 (α; r2 , r1 (α)) = r2

IIσ |θ=α dr . r

(7.5.29)

Using now (7.5.18), (7.5.29) is now written I6 (α; r2 , r1 (α)) = k ln

r1 (α) √ + 2ηvf r2 I4 (α; r2 , r1 (α)) r2

(7.5.30)

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

352

dynamic

Dynamic Plasticity

where

r1 (α)

I4 (α; r2 , r1 (α)) = r2

√ " Ar2 + Br + C "" dr . r3 (r sin θ + x) "θ=α

(7.5.31)

In a similar way we compute the integral on S4 which becomes r1 (α)−ε t · v dA = −2πm4 vr IIσ |θ=γ (r sin α + x) dr S4

r2

= −2πm4 vf r2 R4 I6 (γ; r2 , r1 (γ) − ε) cos γ

(7.5.32)

while I6 is computed with (7.5.29)–(7.5.31), with the integral limits taken correspondingly. The surface S4 is a surface of discontinuity for the vector ﬁeld, [v]|S4 = −v. The integral S6 is t · v dA = −πv0 σ0 (R12 − R32 ) . (7.5.33) S6

The integral S1 will be computed from the term [v] · t, where t is the stress vector which act on this surface. In the symmetry plane considered, the tangent and normal unit vectors on S1 , deﬁned by the equation r = r1 (θ), deﬁned by (7.5.8), are 1 [(−r1 cos θ + r1 sin θ)k + (r1 sin θ + r1 cos θ)i] τ = 2 r1 + (r1 )2 1 [−(r1 sin θ + r1 cos θ)k + (r1 sin θ − r1 cos θ)i] . (7.5.34) n= 2 r1 + (r1 )2 The tangential components of the velocity are: v0 vτ+ = v0 · τ = (r1 sin θ − r1 cos θ) (r1 )2 + r12 vr r vτ− = vr · τ = (vr cos θ k − vr sin θ i) · τ = − 1 2 . (r1 )2 + r1

(7.5.35)

The normal component of the velocity is continuous at the crossing of S1 , and is vn = v0 · n = −v0

r1 sin θ + r1 cos θ . (r1 )2 + r12

(7.5.36)

The traction vector which act on the surface S1 (as a part of the boundary of III, thus of normal n) is determined from a mean formula, obtained from the equilibrium forces which act on the domain III: −π(R12 − R32 )σ0 k + σ0∗ A(S1 )k = 0 .

(7.5.37)

For the computation of the area A(S1 ) we take care of the element of the surface: % (7.5.38) dA = (r1 sin θ + x) (r1 )2 + r12 dθdϕ

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

dynamic

Axi-Symmetrical Problems

with r = r1 (θ) given by (7.5.8) and thus α % (r1 sin θ + x) (r1 )2 + r12 dθ . A(S1 ) = 2π

353

(7.5.39)

γ

From (7.5.37) and (7.5.39) we obtain: π(R12 − R32 ) σ0 . σ0∗ = A(S1 ) The stress vector on the surface S1 is given by the formula: t = t(x, n) = −σ0∗ k .

(7.5.40)

(7.5.41)

Thus from (7.5.35), (7.5.40), (7.5.41) and (7.5.34) we ﬁnd: α v0 (r1 sin θ − r1 cos θ) + vr r1 π(R12 − R32 ) σ0 2π [v] · t dA = A(S1 ) (r1 )2 + r12 S1 γ × (−r1 cos θ + r1 sin θ)(r1 sin θ + x) dθ .

(7.5.42)

We introduce notation: the v0 α vr (r1 sin θ − r1 cos θ)(r1 sin θ + x) (r1 sin θ − r1 cos θ) + r1 dθ I5 = vf γ v0 (r1 )2 + r12 (7.5.43) and the relation (7.5.42) becomes: π(R12 − R32 ) 2πσ0 vf I5 . t · [v] dA = − (7.5.44) A(S1 ) S1 On the surfaces S9 and S11 , taking into account the friction forces on the plug, we have: t · v dA = −2πm2 τ2 vf lR4 ,

S9

(7.5.45) t · v dA = −2πm1 τ1 vf LR2 ,

S11

where τj (with j = 1, 2) are the plasticity limits at shearing, corresponding to the surfaces, and l the cylindrical lengths of the plug at the exit is given by (7.5.24). The integral S4 is computed with (7.5.32): t · [v] dA = − t · v dA . (7.5.46) S4

S4

Introducing the integrals already computed we get: √ π(R12 − R32 ) J(v) = 2 2πkvf r2 I1 (γ, α) + 2πη(vf r2 )2 I2 (γ, α) − 2πσ0 vf I5 A(S1 ) r1 (α) √ + 2ηvf r2 I4 (α, r2 , r1 (α)) + 2πm3 vf r2 R2 cos α k ln r2 r1 (γ) − ε √ + 2πm4 vf r2 R4 cos γ k ln + 2ηvf r2 I4 (γ, r2 , r1 (γ) − ε) r2 + πv0 σ0 (R12 − R32 )

(7.5.47)

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

354

dynamic

Dynamic Plasticity

which will be denoted by j(γ) and which by minimization will determine a value which will be denoted γ ∗ = γopt ; because the value of the functional J(v) computed on real ﬁelds towards the pole O, in the plane of symmetry, (in the deforming ﬁeld) becomes a function of γ. The shape of the plug is given by the value γopt and the lengths l computed from (7.5.24), for this value of γ. With these values of γ and l we will compute the drawing force. 7.5.5

The Drawing Force

The drawing stress will be determined from the theorem of powder expanded applied to the domain V bounded by the boundaries S3 –S13 and which contains the discontinuity surfaces S1 and S2 : σ · D dx + V

2 ) k=1

Sk

t · [v] dA =

t · v dA ,

(7.5.48)

∂V

,13 (with ∂V = j=3 Sj ). In this formula ε˙ will be computed with the kinematics admissible ﬁeld (7.5.10) using γ = γopt , while the stress ﬁeld σ must be considered a static admissible ﬁeld (i.e., satisfying the equilibrium equations and the boundary conditions). Since we were unable to ﬁnd such a ﬁeld, we compute the power σ · D with the formula (7.5.15) with D found previously. Therefore we found the approximate values for the velocity by a minimization procedure. The integral on the volume from (7.5.48) is given by (7.5.15). The integral on S2 is computed with a similar procedure with the one which was used to get (7.5.43) and (7.5.44). The unit vectors on the tangent and normal at Γ2 are τ = sin θ k + cos θ i and n = − cos θ k + sin θ i and therefore vτ+ = 0 ,

vr− = vf k · τ = vf sin θ .

(7.5.49)

The stress vector on S2 will be computed from a global condition of equilibrium of the forces which act on the rigid domain III of the tube: dA k , (7.5.50) 0 = −2π(m1 τ1 LR2 + m2 τ2 lR4 ) + πσf (R22 − R42 ) − σf∗ S2

since we assume that σf∗ k is a mean stress on the surface. With the expression dA = r2 (r2 sin θ + x) dθdϕ of the element of the surface S2 , with (7.5.49) and (7.5.50), the integral on S2 is computed from "α " x sin 2θ cos3 θ " + θ− t · [v] dA = −2πr2 vf σf∗ r2 − cos θ + " 3 2 2 S2 γ

(7.5.51)

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

dynamic

Axi-Symmetrical Problems

355

or if we replace σf∗ from (7.5.50)

# cos3 θ πvf r2 − cos θ + t · [v] dA = r2 (cos γ − cos α) + x(α − γ) 3 S2 x + 2

$""α sin 2θ " θ− " [2(τ1 m1 LR2 + m2 τ2 lR4 ) − σf (R22 − R42 )] . " 2 γ

(7.5.52) The integrals on the surfaces S9 and S11 are computed in (7.5.45) taking into account the friction forces between the tube at exit and the plug. The integral on S13 is t · v dA = πvf σf (R22 − R42 ) . (7.5.53) S13

Introducing now in (7.5.48) the formulae (7.5.15), (7.5.44), (7.5.52), (7.5.28)– (7.5.33), (7.5.45) and (7.5.53) and taking into account the integrals on Sj with j = 5, 7, 8, 10, 12 are zero, we obtain: √ π(R12 − R32 ) 2kr2 I1 (γ, α) + 2ηvf r22 I2 (γ, α) − σ0 I5 A(S1 ) m1 τ1 LR2 + m2 τ2 lR4 + (1/2)σf (R22 − R42 ) r2 (cos γ − cos α) + x(α − γ) "α " x sin 2θ cos3 θ " + θ− × r2 − cos θ + " 3 2 2 γ +

= −m3 r2 R2 cos αI6 (α, r2 , r1 (α)) − m4 r2 R4 cos γI6 (γ, r2 , r1 (γ) − ε) −

v0 σ0 2 σf 2 (R2 − R42 ) . (R1 − R32 ) − m2 τ2 lR4 − m1 τ1 LR2 + 2vf 2

(7.5.54)

We use now (7.5.26) and (7.5.30), and grouping the terms which contain vf we obtain from (7.5.54) the following expression for the drawing force σf =

τ2 m2 lR4 + m1 τ1 LR2 R22 − R42 + x + 2

# "α cos3 θ "" R22 − R42 r2 − cos θ + " 2[r2 (cos γ − cos α) + x(γ − α)] 3 γ &−1 "α $ " " sin 2θ "" R22 − R42 min J(v) 2 " θ− + + ηv r I (γ, α) . f 2 2 " " 2 2 2πvf γ=γ ∗ γ (7.5.55)

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

356

dynamic

Dynamic Plasticity

In this formula, the terms which contains vf will describe the speed inﬂuence on the drawing force. We note that all the integrals I1 , I2 , I4 , I5 do not depend on vf . At the end, we will make precise how to make these computations, which are involved in the drawing force σf [the formula (7.5.55) as well as in J(v) — the formula (7.5.47)]. Let cos2 θ 2 2 2 2 (7.5.56) δ = x cos θ(r2 sin θ + x) 2 sin θ + 2 √ √ √ √ Ax + δ Ax + δ , x2 = (7.5.57) x1 = sin θ sin θ and the variable t: √ t = Ar2 + Br + C − Ar . (7.5.58) Then for I1 (γ, α) we obtain the formula: I1 (γ − α) " √ " √ √ "( " " α '√ √ " t − x1 " "r1 (θ) C "" t − C "" A δ " " √ "− ln " ln |2 At − B| − ln " dθ = " t + C " sin θ x x sin θ " t − x2 " "r2 γ (7.5.59) while for I2 (γ, α) — formula (7.5.17) — follows: " " α# " b " r e "− − a ln "" I2 (γ − α) = " r sin θ + x r sin θ(r sin θ + x) γ 1 − 2

c f + 2 r sin θ(r sin θ + x)2

$""r1 (θ) " dθ " "

(7.5.60)

r2

where

3B sin θ 6C sin2 θ + A− , x x2 C 3C sin θ 1 , c= 3, b= 3 B− x x x 2B sin θ 3C sin2 θ sin θ − −A + , e= 2 x x x2 B sin θ C sin2 θ sin θ −A + − . f = x x x2 The integral (7.5.31) for θ ∈ [γ, α] is computed according to: " " ' " t − √C " b1 b2 c1 " " √ "− √ − √ − √ I4 (θ, r2 , r1 (θ)) = a1 ln " "t + C " t − C t+ C (t − C)2 (" " " "r1 (θ) " t − x1 " f c2 f 1 2 "− " √ − + e1 ln "" − t − x2 " t − x1 t − x2 "r2 (t + C)2 a=

1 x3

(7.5.61)

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

Axi-Symmetrical Problems

where

B sin θ 3C sin θ B2 − + A− , 8C x x2 √ √ (B − 2 AC) B − 2 AC − 8C sin θ/x

dynamic

357

1 a1 = √ Cx2 b1 =

8Cx2 √ √ (B + 2 AC)(B + 2 AC − 8C sin θ/x) , b2 = 8Cx2

,

(x21 − C) sin2 θ (x22 − C) sin2 θ , f = , 2 2x4 2x4 √ (B − 2 AC)2 √ , c1 = a Cx2 ' √ ( √ sin θ (x21 − C) sin2 θ 3 δ √ , − A+ e1 = 3 − x x 2x δ √ (B + 2 AC)2 √ c2 = . 8 Cx2

f1 =

The integral I3 (γ, r2 , r1 (γ) − ε) — the formula (7.5.25) — needs the following computation: r1 (γ)−ε IID |θ=γ (r sin γ + x) dr r2

√ " Ar2 + Br + C "" = dr r2 (r sin γ + x) "θ=γ r2 " # √ " √ 1 B − 2C sin γ "" t − C "" B − 2 AC √ √ "− √ = ln " 2 " " 2x 2x C t+ C t− C √ √ " $"r (θ)−ε " " " δ "" t − x1 "" "" 1 1 B + 2 AC " √ + 2 ln " . − " " " 2x x t − x2 t+ C θ=γ r2

r1 (γ)−ε

(7.5.62) The integral I5 , given by formula (7.5.43), which is involved in the computation of the functional is computed numerically. The same with the integrals with respect to θ, from the relations (7.5.59) and (7.5.60), one compute them numerically. 7.5.6

Numerical Examples

In order to show how the previously established formula can be used several numerical examples will be given. In choosing the constants involved in the constitutive equation, some experimental data obtained for mild steel was used. For this

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

358

dynamic

Dynamic Plasticity

material some mechanical properties which can be described by a Bingham model were already given previously. We stress however, that the numerical examples given here have a qualitative character only. Drawing stress. Several reductions in area were considered. By deﬁnition the reduction in area is R2 − R42 (7.5.63) r% = 100 1 − 22 R1 − R32 while λ=

1 R12 − R32 = R22 − R42 1 − r/100

(7.5.64)

is called the coeﬃcient of extension. In order to give more general examples, the inﬂuence of the speed will be described with the parameter ηvf which is called “speed factor”, or by the dimensionless number ηvf (7.5.65) N= σY 0 R1 which is called the “parameter of speed inﬂuence”. Here σY 0 is the initial limit of plasticity. For big speeds, η decreases very little. We remind that in order to establish from one dimensional test a relation between η and the speed, we deﬁne a mean value for the strain rate √ 3πvf 2r2 1 √ I1 (γ, α) IID dV = (7.5.66) Dm = V V V 6 extended over the whole viscoplastic domain of volume V estimated by 3 r12 − r22 r1 − r23 (cos γ − cos α) − x(α − γ) V = 2π 3 2

(7.5.67)

where r1 is a mean value r1 (mean) = (1/2)(r1 (α)+r1 (γ)). The term from the square bracket from (7.5.66) is computed numerically. The formula (7.5.67) introduces √ ¯ = 2Dm / 3 was used as the mean errors in the estimation of Dm of 1%. Then D equivalent speed of deformation. The coeﬃcient of viscosity in the Bingham model was chosen from the experi¯ From the mental data which correspond to the speed of deformation D1 = D. experimental data of Manjoine [1944] and Cristescu [1977] was establish the empi¯ in s−1 . ¯ + 0.000204, with η in kgf mm−2 s and D rical formula η = (0.74/D) Another parameter involved in the theory of tube drawing is the reduction in diameter deﬁned by the ratio R3 /R4 . The thickness of the wall is expressed by R3 /R1 . Thus in order to characterize the geometry of the tube drawing we use: • the reduction in area r% or λ; • the reduction in diameter expressed by R3 /R4 ; • the reduction of the wall thickness expressed by R3 /R1 .

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Axi-Symmetrical Problems

dynamic

359

In all examples given below the radius R4 was maintained constant and all the other radius were varied in order to obtain various reductions in areas, various reduction in diameter and various wall thicknesses. Most computations were done for the angle α = 12◦ , but other cases were also considered. Concerning the free surface a, in most of the cases it was taken a = 0.5 mm, and sometimes a = 1 mm. Generally this free surface must be small, and for tubes with thin walls and carefully prepared drawing, a can be chosen smaller than 0.5 mm. In the following examples several values for the friction factor m were considered. In the computation of the land l according to the formula (7.5.24) the friction coeﬃcient µ is also involved. After choosing m, the value for µ was obtained from the empirical formula µ = (3/4)m, which was obtained for drawing of wires. The optimum γ angle. We observe also that J(v) increases faster when γ increases than when γ decreases. That suggests for the practice the idea that the ﬂoating plug is to be computed for higher speeds and that will be good for smaller speeds as well. In Fig. 7.5.2 is given a ﬁgure showing the contribution of various terms in the minimum of the functional. The ﬁrst curve is the friction ﬂoating plug-tube, the second the friction matrix-tube and the third the internal dissipation. The inﬂuence of the speed and of the friction factors on the value of the functional. One can see a signiﬁcant inﬂuence on the functional of the speed and of the friction factors (Fig. 7.5.3).

Fig. 7.5.2

Contribution of various terms contained in the functional for α = 13◦ .

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

360

Dynamic Plasticity

Fig. 7.5.3

Speed inﬂuence and friction inﬂuence on the functional J(v).

Fig. 7.5.4

Inﬂuence of the die angle on the drawing stress.

dynamic

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

Axi-Symmetrical Problems

dynamic

361

The inﬂuence of the die angle. The inﬂuence of the die angle on the drawing stress and corresponding plug angle is shown on Fig. 7.5.4 for two sets of friction factors and three sets of velocity factors. One can see that the increase of the drawing stress with speed is more signiﬁcant at small die angles. On the same ﬁgure by dotted or interrupted lines are given the values of the plug angle corresponding to various frictions, speeds and die angles. When the die angle is increased, the corresponding plug angle must also be increased. The diﬀerence α − γ increases slightly when α increases. The drawing stress is decreasing when the die angle is increasing. The optimum angle γ decreases with the increase of the speed. That is more important at small speeds. For higher speeds this decrease is smaller. Our solution does not allow a too much increase of α, since in this case we have some other phenomena (Bramley and Smith [1976]). The shape of the ﬂoating plug is deﬁned essentially by the angle γ and the length l of the land. While γ is uniquely deﬁned, l is not. Here the maximum value for l was computed, that is the value which would keep the ﬂoating plug in its most advanced position there where the whole conical surface of the plug is in contact with the inner surface of the tube. For practical purposes l is to be reduced with one third or even with one half of this computed length. Figure 7.5.5 gives the values of γ and l for various die angles and three drawing speeds. It is shown that l

Fig. 7.5.5

Computation of γ and l, for three drawing speeds.

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

362

Dynamic Plasticity

increases with α, but decreases when the drawing speed is increased. For a certain high speed and/or certain small α, l can decrease even to zero, i.e., the ﬂoating plug can be kept in equilibrium without any cylindrical land. A further increase of the drawing speed or a further decrease of the die angle is certainly impossible since the plug cannot be maintained in equilibrium any more. There are also some other limit drawing regimes which may occur when the drawing stress equals the current yield stress of the material; these limit drawing regimes can also be found quite easily using the main formula (7.5.55) with the condition σf < σY . Thus another limitation for the drawing speed and die angle is found. It is also found that if the friction coeﬃcient is higher, then the angle γ is only slightly reduced but l is reduced signiﬁcantly. The inﬂuence of the tube geometry on the drawing process with ﬂoating plug can be considered easily using formulas (7.5.47), (7.5.24) and (7.5.55). One of the geometrical parameters of signiﬁcance for the tube drawing is the wall thickness expressed by the ratio R3 /R1 . Generally, when the wall thickness decreases stress increases (more signiﬁcantly at high reductions in area and high drawing speeds) (Fig. 7.5.6), the plug angle increases and l also increases (Figs. 7.5.7 and 7.5.8).

Fig. 7.5.6

Variation of wall thickness for various speeds.

dynamic

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Axi-Symmetrical Problems

Fig. 7.5.7

dynamic

363

Variation of plug angle and of length l.

Another important drawing parameter is the diameter reduction expressed by the ratio R3 /R4 . Generally an increase of this ratio decreases γ, increases l maximal, increase σf , etc. Signiﬁcant diameter reductions are impossible with thin wall tubes, high reductions in area or high drawing speeds. All these limit drawing regimes can be easily computed. The clearance a, is of less importance in the whole process. Certainly an increase of a, decreases the drawing stress and therefore allows an increase of the drawing speed. Conclusions. The most important conclusions are: (1) The drawing stress for tube drawing with ﬂoating plug is obtained from formula (7.5.55). It gives the drawing stress as function of the drawing speed, die angle, tube geometry, and mechanical properties of the material, friction coeﬃcients and plug geometry. (2) The optimum geometry of the ﬂoating plug is obtained for various drawing conditions. (3) The optimum semi-cone plug angle is decreasing with decreasing semi-cone die angle, increasing speed, increasing friction, increasing tube wall thickness, increasing diameter reduction.

January 12, 2007

364

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Dynamic Plasticity

Fig. 7.5.8 Nomogram for the computation of ﬂoating plugs for drawing of small tubes. There are three programs: initial diameter × initial thickness of the wall → ﬁnal diameter × the ﬁnal thickness of the wall. Various angles α and various drawing stress are given.

(4) The plug land is increasing with α. Also l is increasing when the friction decreases and when the speed decreases. The plug land increases signiﬁcantly with the increase of the diameter reduction, and increases when the wall thickness is decreasing. (5) There are limit drawing regimes which cannot be surpassed; these correspond to cases when the drawing stress reaches the actual yield stress of the tube or when the plug land decreases to zero. Another theory of drawing with ﬂoating plug is due to S ¸ andru and Camenschi [1988] (see also Ioan and Ioan [1999]). They are assuming again slow processes so that N < 1, and asymptotic developments follows. The drawing stress is

dynamic

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

Axi-Symmetrical Problems

dynamic

365

σf R22 2 R2 LmL 2 √ = √ + σY N 3(R22 − R42 )(R12 − R32 ) 3 R22 − R42 $ # R2 (R22 − R12 ) R2 (R32 − R22 ) + R1 (R12 − R32 ) F (α) + F (γ) × R1 R3 A R32 (R12 − R22 ) G(α, γ) + √ −√ 2 2 2 2 2 3(R2 − R4 )(R1 − R3 ) 3(R1 − R32 )(R22 − R42 ) R1 R3 + R32 (R22 − R12 ) ln × R12 (R32 − R22 ) ln R2 R1 were all the constants are determined from other equations. Here u(θ) = a + bp(θ) + q(θ) , A + Bp(θ) + Dq(θ) + K1 (θ)p(θ) + K2 (θ)q(θ) , 6 α 9 K1 (θ) = − f (t)q(t) sin t dt , 16 γ α 9 f (t)p(t) sin t dt , K2 (θ) = 16 γ v(θ) =

1 + cos 2θ , 3 1 θ q(θ) = + cos 2θ ln tan − (1 − 3 cos θ)(1 + cos θ) , 3 2

p(θ) =

F (α) = [2a sin α − u (α) cos α] sin2 α , F (γ) = [2a sin γ − u (γ) cos γ] sin2 γ , G(α, γ) = mα cot α + mγ cot γ − 4[v(α) − v(γ)] − v (α) cot α + v (γ) cot γ tan α/2 + [A cos γ + v (γ) sin γ + mγ sin γ] ln tan γ/2 # α u (t) α −2 dt + 6 ln tan 2 3u2 (t) + u2 (t)/4 γ × γ

α

u(t) sin t

dt − 3u2 (t) + u2 (t)/4

γ

α

$ u(t) sin t ln(tan t/2) dt . 3u2 (t) + u2 (t)/4

Several examples are given for the determination of the drawing stress and all the other unknown quantities.

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

366

7.6 7.6.1

Dynamic Plasticity

Extrusion Formulation of the Problem

Let us consider now a mathematical model for hot tube extrusion, taking into account the inﬂuence of the working speed, when melted glass is used as a lubricant. We consider the problem of being stationary and isothermal. The working speed is considered variable during the process but for a certain magnitude of this velocity it is assumed that it is maintained constant for certain time interval so that during this time the process is considered “stationary”. Therefore, the variation of the working speed is described by a set of stationary cases (Cleja-Tigoiu and Cristescu [1985]). The extrusion problem considered with classical plasticity theory was considered by many authors. We mention here only Avitzur [1968], Blazynski [1976], Maneghin et al. [1980], Medvedev et al. [1980], Hartley [1971], etc. to mention just a few. The cylindrical billet of annular cross-section with outer radius R1 , inner radius R3 and length l is pushed out from a cylindrical container using a ram which is moving with the speed v0 (Fig. 7.6.1). In the interior of the billet a cylindrical plug of radius R3 and moving together with the ram is used to control the ﬁnal inner radius of the tube. In front of the billet, between the billet and container, is placed a glass ring which at the beginning of the process melts and forms a dead zone which during the extrusion process is an extrusion of the die. All other surfaces of the billet are also glass lubricated. As is well known, glass lubrication allows higher working speeds and therefore high rates of deformation are involved (of the order of 102 s−1 ). Due to the symmetry of the process the considered problem is axial symmetric and the geometry of the process is shown in Fig. 7.6.1 (not to

Fig. 7.6.1

Geometry of extrusion process.

dynamic

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Axi-Symmetrical Problems

dynamic

367

scale). The mathematical problem reduces to the determination of the velocity ﬁeld v and the stress ﬁeld σ, smooth in V , which must satisfy the equilibrium condition, incompressibility condition and a constitutive equation of Bingham type: k 1 1− √ σ (7.6.1) divσ = 0 , div v = 0 , D = 2η IIσ where the same notation as given previously are used. η is the viscosity coeﬃcient and k is the mean yield stress in pure shear, both η and k being temperature dependent. A prime denotes “deviator”. Boundary conditions, which will be given below, have also to be satisﬁed. The kinematic velocity ﬁeld is obtained from the following assumptions. There are two subdomains I and III, of V where the material is assumed to be in a rigid state and moving with velocity v0 k and vf k, respectively. Thus the incompressibility condition yields the following relationship between v0 and vf : vf (R22 − R32 ) = v0 (R12 − R32 ) .

(7.6.2)

Further it is assumed that in the domain II viscoplastic deformation takes place. In the interior of V the velocity ﬁeld is assumed to be smooth. Thus the surfaces S0 and Sf (the rigid-viscoplastic interfaces) are continuity surfaces for the velocity ﬁeld. We assume also that the melted glass forms a dead zone, the billet-melted glass interface surface, denoted by S4 , is a ﬂow surface (ﬂow line tube) which can be considered to be a surface of velocity discontinuity. The shape of this surface changes during the extrusion process. Finally we assume that the plug-billet interface S3 is also a ﬂow surface. On these surfaces friction takes place which will be described by the law: (7.6.3) |tτ | = m IIσ where tτ is the friction stress and 0 ≤ m ≤ 1 is the constant friction factor. On the surfaces Sj (j = 5, . . . , 8) there is a friction between the rigid material and rigid tool surface, while the velocities on S1 and S2 are known and related by Eq. (7.6.2). To solve the problem the velocity ﬁeld and the ram pressure have to be determined. The velocity ﬁeld is chosen from the range of kinematically admissible velocity ﬁelds as being the one for which the functional J(v) related to the Bingham model takes the smallest value. Starting from the equation of the ﬂow lines in V a smooth kinematic admissible velocity ﬁeld is derived which satisﬁes the incompressibility condition, and takes given values on S1 and S2 . This velocity ﬁeld depends on the functions g0 and gf which are involved in the deﬁnition of the surfaces S0 and Sf . The velocity ﬁeld which approximates the real one corresponds to the values g0∗ and gf∗ for which J(v), considered a functional of g0 and gf , takes the smallest value. The ram pressure is obtained from the theorem of power expanded written for the approximate velocity ﬁeld previously determined. The approximate velocity

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

368

dynamic

Dynamic Plasticity

ﬁeld and the ram pressure can be determined numerically only. Since signiﬁcant computing time is involved, several simplifying assumptions concerning the shape of the surfaces S0 and Sf will be made. Thus the functional J(v) is transformed into a real function depending on a certain number of real parameters. The inﬂuence of the working speed on the process (ram pressure, dead zone shape, etc.) is obtained numerically for cases suggested by practical applications, assuming that the mechanical properties of the material, the lubrication conditions and the geometry of the process (i.e., Ri ) are known. 7.6.2

Kinematics of the Process

Due to the axial symmetry of the problem, cylindrical coordinates (r, θ, z) will be used. The equation of the ﬂow surfaces are r = G(z, α)

(7.6.4)

with α ∈ [R3 , R2 ]. The cylindrical surfaces r = α are the ﬂow surfaces in domain III. Let us assume that the surfaces S0 and Sf of equations surfaces are z = Γ0 (r) ,

z = Γf (r)

(7.6.5)

have unique intersections with the ﬂow surfaces α = const. for any α ∈ [R3 , R2 ]. It follows that the equations of these surfaces can be written as function of r = f0 (α) ,

r = ff (α)

(7.6.6)

where f0 yields from the incompressibility condition written in the form v0 [f02 (α) − R32 ] = vf (α2 − R32 ) or

f0 (α) =

R12 − R32 2 (α − R32 ) + R32 R22 − R32

(7.6.7) 1/2 (7.6.8)

if Eq. (7.6.2) is also used. From Eqs. (7.6.5) and (7.6.6) the equations of the surfaces S0 and Sf can be written as z = Γ0 (f0 (α)) ≡ g0 (α) ,

z = Γf (α) ≡ gf (α) .

Thus the equations of the ﬂow surface are f0 (α) , r = G(z, α) ≡ F (z, α) , α,

(7.6.9)

z ≤ g0 (α) g0 (α) ≤ z ≤ gf (α)

(7.6.10)

z ≥ gf (α) ,

for α ∈ [R3 , R2 ]. Since the velocity ﬁeld is smooth in V , the derivative of the function F (z, α), with respect to z must satisfy the conditions lim Fz (z, α) = 0 ,

lim Fz (z, α) = 0 .

z g0 (α)

z gf (α)

(7.6.11)

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

dynamic

Axi-Symmetrical Problems

369

Fα (z, α)Fz (z, α) = 0

(7.6.12)

It will be assumed also that in the interior of II and that it is ﬁnite. Since the inner cylindrical surface of the tube is α = R3 we have F (z, R3 ) = R3

(7.6.13)

for any z ∈ [g0 (α), gf (α)]. From (7.6.12) we conclude that through any point P of II passes a unique ﬂow line. Therefore, the family β = const. of orthogonal lines to the ﬂow lines exists; their equation in the plane (z, r) is Φ(z, r) = β ,

(7.6.14)

with β a real number belonging to a certain interval. The orthogonally condition of the curves (7.6.10) and (7.6.14) is Φz = Fz Φr .

(7.6.15)

Since Φr (z, α) = 0 in II, (7.6.14) can be solved, with respect to r. From (7.6.10) and (7.6.14) written as f1 (z, r; α, β) = r − F (z, α) = 0 ,

(7.6.16)

f2 (z, r; α, β) = Φ(z, α) − β

and using the theorem of implicit functions we get the nonsingular mapping r = u(α, β) ,

z = v(α, β)

(7.6.17)

because 1 + Fz2 Fz is ﬁnite and non-zero in the interior of II. Further the formulae Fα Fα Fz ∂z ∂r = =− , , ∂α 1 + Fz2 ∂α 1 + Fz2 ∆ = Φr

(7.6.18)

(7.6.19)

∂r Fz2 ∂z Fz = , = , ∂β Φr (1 + Fz2 ) ∂β Φr (1 + Fz2 ) yield from Eqs. (7.6.16) and (7.6.17). Thus x = u(α, β) cos θ ,

y = u(α, β) sin θ ,

z = v(α, β)

(7.6.20)

deﬁne a nonsingular mapping from (x, y, z) → (q = α, q = θ, q = β), since the Jacobian " " " ∂z ∂r ∂z ∂r "" √ − (7.6.21) g ≡ r "" ∂α ∂β ∂β ∂α " 1

computed with Eq. (7.6.19)

is non-zero.

" " F (z, α) "" Fα Fz "" √ g= 1 + Fz2 " Φr "

2

3

(7.6.22)

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

370

dynamic

Dynamic Plasticity

In the new system of coordinates the incompressibility condition is 3 1 ) ∂ √ i ( gv ) = 0 div v = √ g i=1 ∂q i

(7.6.23)

with v i the contravariant components of the velocity. Since q 1 = α = const. are ﬂow lines it yields v = v β eβ

(no summation)

with eβ directed along the ﬂow lines in the ﬂow sense. From Eqs. (7.6.23) and (7.6.24) and the axial symmetry we get √ β gv = C(α) .

(7.6.24)

(7.6.25)

The function C(α) is determined from the condition lim r=F (z,α) zg0 (α)

v(r, z) = v0 k .

Thus the kinematic velocity ﬁeld considered is C(α) ∂r ∂z eβ ir + k , v = C(α) √ = √ g g ∂β ∂β

(7.6.26)

(7.6.27)

where ir and k are unit vectors (see Fig. 7.6.1). By inverting the relations (7.6.17) and using (7.6.21) we get r ∂z ∂α = √ , ∂r g ∂β

∂α r ∂r = −√ . ∂z g ∂β

(7.6.28)

From (7.6.27) and (7.6.24) the components of the kinematic velocity ﬁeld in the cylindrical coordinates are ∂α ∂α 1 1 vr = − C(α) , vθ = 0 , vz = C(α) , (7.6.29) r ∂z r ∂r where α is considered to be a function of z and r according to Eq. (7.6.10): α = H(z, r)

(7.6.30)

so that r = F (z, H(z, r)). To get the explicit expression of C(α) involved in Eqs. (7.6.26) and (7.6.27) the following limits are necessary: from (7.6.19)1 and (7.6.11)1 yields ∂r = Fα (g0 (α), α) , r=F (z,α) ∂α

∂z = 0; r=F (z,α) ∂α

zg0 (α)

zg0 (α)

lim

lim

(7.6.31)

from (7.6.19)2 , (7.6.22) and (7.6.11)1 we have lim sign(Φr Fz )r=F (z,α) 1 ∂z zg0 (α) = lim √ g ∂β F (g0 (α), α)|Fα (g0 (α), α)| r=F (z,α) zg0 (α)

(7.6.32)

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

dynamic

Axi-Symmetrical Problems

371

1 ∂r = 0. √ g ∂β r=F (z,α)

(7.6.33)

and lim

zg0 (α)

Thus C(α) = v0 F (g0 (α), α)|Fα (g0 (α), α)| .

(7.6.34)

Using (7.6.34) in (7.6.29) and (7.6.10) the kinematic velocity ﬁeld expressed as a function of z, r is vr = −v0 f0 (α)|Fα (g0 (α), α)| vz = v0 f0 (α)|Fα (g0 (α), α)|

1 ∂α , r ∂z

∂α , ∂r

(7.6.35)

vθ = 0 , with α = H(z, r). By diﬀerentiation of Eq. (7.6.10) ∂α 1 = , ∂r Fα (z, α)

∂α Fz (z, α) = , ∂z Fα (z, α)

(7.6.36)

is obtained. From (7.6.36), (7.6.35) and (7.6.10), another form of the velocity ﬁeld, this time as function of z and α, can be obtained vr =

v0 f0 (α) |Fα (g0 (α), α)| Fz (z, α) , F (z, α) Fα (z, α)

vz =

v0 f0 (α) |Fα (g0 (α), α)| , F (z, α) Fα (z, α)

(7.6.37)

vθ = 0 . The previous formulae will be written in a particular form for the case when the ﬂow lines are sinusoidal lines, deﬁned by r = F (z, α) = A(α){sin[a(α)z + b(α)] + 1} + α ,

(7.6.38)

with 1 [f0 (α) − α] , 2 where a(α) and b(α) are determined by (7.6.11) as A(α) =

a(α) =

π , gf (α) − g0 (α)

b(α) =

π gf (α) − 3g0 (α) . 2 gf (α) − g0 (α)

(7.6.39)

(7.6.40)

Condition (7.6.13) is satisﬁed since (7.6.8) yields A(R3 ) = 0. Formulae (7.6.38) to (7.6.40) yield vf α . (7.6.41) F (g0 (α), α) = f0 (α) ≡ v0 f0 (α)

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

372

dynamic

Dynamic Plasticity

In this particular case the velocity ﬁeld is written as α ∂α α ∂α , vz = vf , vθ = 0 , (7.6.42) r ∂z r ∂r with α = H(z, r) obtained from Eq. (7.6.39) by inversion, with respect to α. In what follows we will need the expression of the second invariant IID in cylindrical coordinates, which, using the incompressibility condition, becomes vr = −vf

2 2 2 IID = Drr + Dθθ + Drz + Drr Dθθ .

(7.6.43)

The components of the rate of deformation tensor corresponding to the ﬁeld (7.6.42) are α ∂α α ∂ 2 α 1 ∂α − 2 + , Drr = −vf r ∂r r ∂z r ∂r∂z α ∂α , r2 ∂z & 2 2 ∂α ∂2α 1 vf ∂2α ∂α α ∂α −α 2 . =− +α 2 − + 2 r ∂z ∂z ∂r r ∂r ∂r

Dθθ = −vf Drz

(7.6.44)

In forming the partial derivatives of the function α = H(z, r), (7.6.38) is used. Thus the second invariant IID can be considered either as a function of z and r if α = H(z, r) is used, or a function of z and α if r is represented by F (z, α). The latter version will be used further on. 7.6.3

The Approximate Velocity Field

The functional attached to the Bingham model, for the case considered here is ) ) IID dV + 2k IID dV − t · v dσ + t · [v] dσ , J(v) = 2η V

V

j

Sj

i

Si

(7.6.45) where Sj with j = 2 and 5–8 are the surfaces on which the velocity is prescribed and Si with i = 3, 4 are the discontinuity surfaces for the velocity ﬁeld and on which it is assumed that the stress vector t is known. The approximate velocity ﬁeld for the extrusion problem is determined by minimizing on the kinematical velocity ﬁeld (7.6.42) using (7.6.38) to form the appropriate expression of J(v) [in the sense that in this functional on surfaces S4 and S3 the stress vector is replaced by Eq. (7.6.3)]. On the family of kinematic admissible velocity ﬁelds J becomes a functional of g0 and gf . The values g0∗ and gf∗ for which J takes the smallest value deﬁne the approximate solution of the problem. The geometry of the viscoplastic domain is known if the surfaces S4 , S0 and Sf are known. The volume integrals from (7.6.45) are calculated with (7.6.43) and (7.6.44) by assuming that IID depends on α and z alone. Passing from the variables (z, r, θ) to (z, α, θ) with r = F (z, α), we obtain for instance for the ﬁrst integral

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

dynamic

Axi-Symmetrical Problems

R2

gf (α)

IID dV = 2π V

IID (z, α)F (z, α)|Fα (z, α)| dzdα . R3

373

(7.6.46)

g0 (α)

On the boundaries S3 and S4 the tangential component of the stress vector, according to (7.6.3) is given by (7.6.47) |tτ | = mi IIσ = mi 2η( IID + k) , where mi (i = 3, 4) is the constant friction factor on the corresponding surface. The equation of the surface S4 deﬁned by α = R2 is x = F (z, R2 ) cos θ , y = F (z, R2 ) sin θ ,

(7.6.48)

z = z, with θ ∈ [0, 2π] and z ∈ [g0 (R2 ), gf (R2 )]. The element of area is dσ = F (z, R2 ) 1 + Fz2 (z, R2 ) dθdz . The velocity ﬁeld is tangent to the surface S4 and from (7.6.42) yields 2 2 R2 ∂α ∂α + , |vτ | = vf F (z, R2 ) ∂r ∂z

(7.6.49)

(7.6.50)

where ∂α/∂r and ∂α/∂z are computed with (7.6.36). Thus from (7.6.47)–(7.6.49), the integral on S4 is obtained with gf (R2 ) 1 + Fz2 (z, R2 ) dz . t · v dσ = −2πm4 vf R2 (2η IID (z, R2 ) + k) |Fα (z, R2 )| S4 g0 (R2 ) (7.6.51) On the cylindrical surface S3 (α = R3 ) the velocity is tangent to the surface and from (7.6.42), (7.6.36) and (7.6,13) we get the relative velocity between the billet and the plug: v0 1 − k. (7.6.52) v3 = vf Fα (z, R3 ) vf The integral over S3 is computed with (7.6.47) and (7.6.52) as gf (R3 ) t · v dσ = −2πm3 R3 (2η IID (z, R3 ) + k)|v3 | dz . S3

(7.6.53)

g0 (R3 )

The integral over S2 is zero since this surface is stress free. On the surface Sj with j = 5–8 friction between rigid tool walls and billet takes place and is prescribed by the law |tτ | = mj τj

(no summation) ,

(7.6.54)

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

374

dynamic

Dynamic Plasticity

where τj is the constant shearing yield stress of the material along the wall Sj . The law (7.6.54) is a particular version of (7.6.3). Denoting by Lj the length of the cylindrical surfaces Sj , the integrals over these surfaces are t · v dσ = −2πm5 L5 τ5 R1 v0 , S5

t · v dσ = −2πm7 L7 τ7 R2 vf ,

(7.6.55)

S7

t · v dσ = −2πm8 L8 τ8 R3 |vf − v0 | , S8

while the integral on S6 is zero. With the expression of all these integrals, the functional which has to be minimized, with respect to g0 and gf becomes R2 gf (α) (ηIID + k IID )F (z, α)|Fα (z, α)| dzdα J(v) = 4π R3

g0 (α)

+ 2πm5 L5 τ5 R1 v0 + 2πm7 L7 τ7 R2 vf + 2πm8 L8 τ8 R3 |vf − v0 | " " gf (R3 ) " 1 v0 " + 2πm3 R3 vf − "" dz (2η IID (z, R3 ) + k) "" Fα (z, R3 ) vf g0 (R3 )

gf (R2 )

+ 2πm4 R2 vf

(2η

IID (z, R2 ) + k)

g0 (R2 )

1 + Fz2 (z, R2 ) dz , |Fα (z, R2 )|

(7.6.56)

where F (z, α) given by (7.6.38) depends on g0 and gf . 7.6.4

The Extrusion Pressure

The extrusion pressure is determined from the theorem of power expanded σ · D dV = t · v dσ (7.6.57) V

S

with S=

8 -

Sj

j=1

and in which the internal dissipation and those on various surfaces are computed for the approximate velocity ﬁeld already determined. The dissipation on the surface S1 is t · v dσ = π(R12 − R32 )v0 p (7.6.58) S1

in which p is the extrusion pressure.

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

dynamic

Axi-Symmetrical Problems

375

For the Bingham model (7.6.1) the stress power is σij Dij dV = 4η IID dV + 2k IID dV V

V

(7.6.59)

V

with the volume integrals calculated according to the same procedure as for (7.6.46). Taking into account in (7.6.57) the integral on S1 as given by (7.6.58), the integral on S4 and S5 furnished by (7.6.51) to (7.6.53), the integrals on S5 , S7 and S8 given by (7.6.55) (the integrals on S2 and S6 are zero) we get the ram pressure 1 1 p= 2 2 R1 − R3 πv0

σ · D dV + 2m3 R3

V gf∗ (R2 )

gf∗ (R3 )

g0∗ (R3 )

(2η

IID (z, R3 ) + k)|v3 | dz

1 + Fz2 (z, R2 ) dz |Fα (z, R2 )| g0∗ (R2 ) vf vf + 2m5 L5 τ5 R1 + 2m7 L7 τ7 R2 + 2m8 L8 τ8 R3 −1 . v0 v0 + 2m4 R2

vf v0

(2η

IID (z, R2 ) + k)

(7.6.60)

In this formula g0∗ and gf∗ are the functions which deﬁne the surfaces S0 and Sf . From (7.6.60) the ram pressure can be determined if either the velocity of the ram or the velocity vf at the exit of the container is known. The value of the extrusion pressure depends on the parameters deﬁning the geometry (Rj , g0∗ and gf∗ ), on the mechanical properties of the billet (η and k), on the friction factors (mi ) on various interface surfaces, and certainly on v0 or vf . The mechanical parameters and the friction conditions are strongly temperature dependent. 7.6.5

Numerical Examples

In order to determine numerically the ram pressure and the inﬂuence of the working velocity on this pressure, we have to ﬁnd ﬁrst g0∗ and gf∗ . Since signiﬁcant computing time is necessary in order to ﬁnd g0∗ and gf∗ by minimizing the functional J, simplifying assumptions concerning the shape of these surfaces are necessary. These simpliﬁcations, suggested by experimental evidence, must keep the formulae involved in the problem as simple as possible. In a ﬁrst particular case the surfaces S0 and Sf are assumed to be conical, i.e., straight lines in the symmetry plane. These straight lines pass trough the points Q(0, R2 ) and P (−L, R1 ), respectively r − R1 = m0 (z − L) r − R2 = mf z .

(7.6.61)

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

376

dynamic

Dynamic Plasticity

If m0 and mf are ﬁnite, (7.6.61) and (7.6.6) yield α − R2 ≡ gf (α) = z mf f0 (α) − R1 + m0 L ≡ g0 (α) = z . (7.6.62) m0 With these expressions for g0 and gf the functional J becomes a function of the real parameters γ0 , γf and L. These parameters may vary in the intervals R1 R2 , π , γf ∈ arctan ,π , (7.6.63) L ∈ (0, l) , γ0 ∈ arctan L0 L0 where l is the initial length of the billet, m0 = tan γ0 and mf = tan γf . Another case in which simpliﬁcations are possible is the one in which it is assumed that gf (α) − g0 (α) = L .

(7.6.64)

Equations (7.6.40), (7.6.41) and (7.6.64) then yield π 2g0 (α) π 1− a= , b= L 2 L in which the function g0 and the real parameter L are arbitrary. In another particular case we can assume that g0 and gf are chosen so that the surfaces S0 and Sf are circles in the plane of symmetry: for instance circles with centers at the points C0 (Z0 , R0 ) and Cf (Zf , Rf ) and passing through P and Q, respectively. Then we have % z = Z0 − ρ20 − [f0 (α) − R0 ]2 ≡ g0 (α) z = Zf −

% (R2 − Rf )2 + Zf2 − (α − Rf )2 ≡ gf (α) .

(7.6.65)

In this case the real parameters on which the function J depends are R0 , Z0 , ρ0 , Rf and Zf . Some combinations of the particular cases given above can be imagined. The mechanical properties of the billet at high temperatures are described by choosing appropriate values for the viscosity coeﬃcient η and the mean yield stress k. In the numerical examples we have taken into account the dependence of η on the mean rate of deformation Dm deﬁned by 2 2 1 ¯ D = √ Dm = √ IID dV , (7.6.66) 3 3V V ¯ is computed for each particular where V is the volume of the viscoplastic domain. D ¯ case of extrusion considered. From the graphical plot of the function η = η(D) obtained from experimental data, the corresponding value of the viscosity coeﬃcient is obtained.

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Axi-Symmetrical Problems

dynamic

377

For high temperatures the value of k was determined from uniaxial experiments. The geometry of the extrusion process will be characterized by the reduction in area R2 − R32 (7.6.67) r% = 100 1 − 22 R1 − R32 and the geometry of the billet. In the numerical examples given below the data for steel AISI 304 as given by Polukhin et al. [1976] have been used. Thus for the temperature range of 1100– √ ◦ −2 1200 C, the mean yield stress is k = 3.5 kgf mm and σY f = 3τ7 = 8 kgf mm−2 . For the working speed v0 ranging between 200 mm s−1 and 400 mm s−1 and ¯ takes values between 38.12 s−1 and 58.40 s−1 . reductions of 96.14% and of 97%, D The corresponding values for η are 2.2 × 106 Poise and 1.5 × 106 Poise. For the reduction mentioned, the radii Ri are: R1 = 74 mm, R2 = 28.5 mm, R3 = 25 mm and R1 = 74 mm, R2 = 23.5 mm, R3 = 20 mm, respectively. On the billet-plug and billet-container interfaces, the lubricant used is powdered glass, which at high pressure and temperature melts forming a thin ﬁlm with the thickness of a few microns (5–17 µm). On the surface S4 the interface between the melted glass and the billet, the friction factor is very small. From the experimental data by Maneghin et al. [1980] the friction factor at all surfaces lubricated by melted glass was taken m = 0.02 and in one single case m = 0.04. For the particular shape of the surfaces S0 and Sf described by formulae (7.6.62) the numerical values of the parameters γ0 , γf and L for which the functional J(v) — now a function J(L, γ0 , γf ) of real variables — takes a minimal value, have been determined. This is done for various prescribed values of v0 , various geometries of the billet and product, prescribed mechanical properties of the metal and those of the lubricant, by a trial and error procedure. Then the value of L for which the function J(L, γ0 , γf ) has a minimum is found. With this value of L, the parameter γ0 is varied and its value which minimizes J is found. We return now and with this new value of γ0 kept constant vary again L, etc. After several iterations the parameter γf is varied also. The ﬁnal values of the tree parameters obtained by this trial and error procedure are denoted by (L∗ , γ0∗ , γf∗ ). We start with prescribed values of γ0 and γf in the neighborhood of 90◦ . On Fig. 7.6.2 for v0 = 300 mm s−1 is shown the dependence of J(L, γ0∗ , γf∗ ) on L for ﬁxed values of γ0∗ and γf∗ . The dependence of J(L∗ , γ0 , γf∗ ) on γ0 is shown on Fig. 7.6.3 while that of J(L∗ , γ0∗ , γf∗ ) on γf is on Fig. 7.6.4. If the reduction in area is increased by a few per cent the minimum value of J increases. The values of γ0∗ and γf∗ do not change signiﬁcantly but the value of L∗ increases when reduction is increased. With an increase of the friction factor, the minimum value of J increases, L∗ slightly increases but γ0∗ and γf∗ are practically the same. For each ﬁxed value of v0 , geometry conditions, mechanical proprieties and lubrication conditions, using the determined values of L∗ , γ0∗ , γf∗ , the ram pressure is

January 12, 2007

378

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Dynamic Plasticity

Fig. 7.6.2 Dependence of functional J on the length L for various reductions and friction factors, showing the minimum.

Fig. 7.6.3 Dependence of functional J on angle γ0 , for various reductions and friction factors, showing the minimum.

dynamic

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Axi-Symmetrical Problems

Fig. 7.6.4

dynamic

379

Dependence of functional J on the angle γf ; the minimum is close to 90◦ .

Fig. 7.6.5 The inﬂuence of working speed on the length L of the viscoplastic domain and on the extrusion pressure.

obtained from formula (7.6.60). On Fig. 7.6.5 is shown the working speed inﬂuence on the extrusion pressure: the extrusion pressure increasing with increasing v0 . The inﬂuence of v0 on L∗ is also shown on this ﬁgure: L∗ increases signiﬁcantly with v0 . The signiﬁcant increase of L∗ with v0 is accompanied by an increase of the volume Vg of the melted glass. It has been shown that the geometry of the viscoplastic domain, and therefore of the melted glass, is strongly dependent on the working speed. During the extrusion process, the melted glass is a self-adjusting die. A control volume of the melted glass during extrusion may ensure the optimal working conditions.

January 12, 2007

10:41

380

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Dynamic Plasticity

Bibliography Abou-Sayed A. S. and Clifton R. J., 1976, Pressure shear waves in fused silica, J. Appl. Phys. 47, 5, 1762–1770. Abou-Sayed A. S. and Clifton R. J., 1977a, Analysis of combined pressure-shear waves in an elastc/viscoplastic material, J. Appl. Mech. Trans. ASME 44, 79–84. Abou-Sayed A. S. and Clifton R. J., 1977b, Pressure-shear waves in 6061-T6 aluminum due to oblique-plate-impact, J. Appl. Mech. Trans. ASME 44, 1, 85–88. Alexandrov S. and Alexandrova N., 2000, On the maximum friction law in viscoplasticity, Mech. Time-Dependent Materias 4, 99–104. Angelov T. A., 2004, Variational analysis of a rigid-plastic roling problem, Int. J. Engng. Sci. 42, 1779–1792. Avitzur B., 1968, Metal Forming: Processes and Analysis, McGraw-Hill, New York. Bernstein B. and Shokooh A., 1980, J. Rheology 24, 2, 189–211. Bisk M. B. and Shveikin V. V., 1963, Tube drawing with ﬂoating plugs, Metalurgya, Moscow (in Russian). Blazynski T. Z., 1976, Metal Forming. Tool Proﬁles and Flow, Macmillan, London. Bramley A. N. and Smith D. J., 1976, Metals Technology, 322. Camenschi G. and S ¸ andru N., 2003, Mathematical Models in Metal Working, Bucharest, 188 pp. (in Roumanian). Camenschi G., Cristescu N. and S ¸ andru N., 1979, High speed wire drawing, Archives of Mechanics 31, 5. Camenschi G., Cristescu N. and S ¸ andru N., 1983, Developments of high speed viscoplastic ﬂow through conical converging dies, Trans. ASME, J. Appl. Mech. 50. Campbell J. D., 1973, Dynamic plasticity — macroscopic and microscopic aspects, Materials Science and Engineering 12, 1, 3–21. Chhabildas L. C. and Swegle J. W., 1980, Dynamic pressure-shear loading of materials using anisotropic crystals, J. Appl. Phys. 51, 9, 4799–4807. Cleja S. and Cristescu N., 1979, Inﬂuence of the drawing speed on the optimum shape of the ﬂoating plug, Rev. Roum. Sci.-Mec. Appl. 24, 3, 357–377. Cleja-Tigoiu S. and Cristescu N., 1985, A ﬂow analysis of rigid-viscoplastic body through annular oriﬁce, Int. J. Mech. Sci. 27, 5, 291–301. Clifton R. J., 1968, Elastic-plastic boundaries in combined longitudinal and torsional plastic wave propagation, J. Appl. Mech. Trans. ASME 35, 4, 782–786. Cristescu N., 1956, Some remarks concerning the case of plane axial symmetrical deformation in dynamic problems of plasticity, Comm. Acad. Rep. Pop. Rom. 6, 19–28 (in Romanian). Cristescu N., 1967, Dynamic Plasticity, North-Holland Pub. Co., 614 pp. Cristescu N., 1975, Plastic ﬂow through conical converging dies, using a viscoplastic constitutive equation, Int. J. Mech. Sci. 17, 425–433. Cristescu N., 1976, Drawing through conical dies — an analysis compared with experiments, Int. J. Mech. Sci. 18, 45–49. Cristescu N., 1977, Speed inﬂuence in wire drawing, Rev. Roum. Sci. Techn. Mec. Appl. 22, 3, 391–399. Cristescu N., 1980, On the optimum die angle in fast wire drawing, J. Mech. Working Tech. 3, 275–287. Dahan N. and Le Nevez P., 1983, M´ethode de calcul des grandes d´eformations plastiques et endommagement dans les pi`eces extrudees, M´emoire et Etudes Scientiﬁques Revue de M´etallurgie 80, 10, 557–566.

dynamic

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Axi-Symmetrical Problems

dynamic

381

Frutschy K. J. and Clifton R. J., 1997, High-temperature pressure-shear plate impact experiments using pure tungsten carbide impactors, Experimental Mechanics 38, 2, 116–125. Frutschy K. J. and Clifton R. J., 1998, High-temperature pressure-shear plate impact experiments on OFHC copper, J. Mech. Phys. Solids 46, 19, 1723–1743. Fu M. and Luo Z. J., 1995, The simulation of the viscoplastic forming process by the ﬁnite element method, J. Materials Process. Tech. 55, 442–447. Gilat A. and Clifton R. J., 1985, Pressure-shear waves in 6061-T6 aluminum and alpha titanium, J. Mech. Phys. Solids 33, 3, 263–284. Gilman J. J. and Tuler F. R., 1970, Dynamic fracture by spallation in metals, Int. J. Fracture Mech. 6, 2, 169–182. G¨ uldenpfennig J. and Clifton R. J., 1980, Plastic waves of combined stress based on self consistent slip models, J. Mech. Phys. Solids 28, 3–4, 201–219. Hartley C., 1971, Int. J. Mech. Sci. 17, 651–663. Heeres O. M., Suiker A. S. J. and de Borst R., 2002, A comparison between the Perzyna viscoplastic model and the Consistency viscoplastic model, Europ. J. Mech. A/Solids 21, 1–12. Hsu J. C. C. and Clifton R. J., 1974a, Plastic waves in a rate sensitive material-I. Waves of uniaxial stress, J. Mech. Phys. Solids 22, 233–253. Hsu J. C. C. and Clifton R. J., 1974b, Plastic waves in a rate sensitive material-II. Waves of combined stress, J. Mech. Phys. Solids 22, 255–266. Ioan S. and Ioan R., 1999, A mathematical model of bimetallic tube drawing with ﬂoating plug, Rev. Roum. Sci. Tech.-Mec. Appl. 44, 1, 49–72. Iddan D. and Tirosh J., 1996, Analysis of high-speed rolling with inertia and rate eﬀects, J. Appl. Mech. Trans. ASME 63, 27–37. Ionescu I. R. and Vernescu B., 1988, A numerical method for viscoplastic problem. An application to wire drawing, Int. J. Engng. Sci. 26, 6, 627–633. O’Keefe J. D., Skeen C. H. and York C. M., 1973, Laser-induced deformation modes in thin metal targets, J. Appl. Phys. 44, 10, 4622–4626. Kim K. S. and Clifton R. J., 1980, Pressure-shear impact of 6061-T6 aluminum, J. Appl. Mech. 47, 1, 11–16. Kim Y. H., Ryou T. K., Choi H. J. and Hwang B. B., 2002, An analysis of the forging processes for 6061 aluminum-alloy wheels, J. Materials Process. Tech. 123, 279–276. Klopp R. W. and Clifton R. J., 1990, Analysis of tilt in the high-strain-rate pressure-shear plate impact experiment, J. Appl. Phys. 67, 11, 7171–7173. Li G. J. and Kobayashi S., 1982, Rigid-plastic ﬁnite-element analysis of plane-strain roling, ASME, J. Eng. for Industry 104, 1, 55–64. Lindholm U. S. and Bessey R. L., 1969, A survey of rate dependent strength properties of metals, Rept. AFML-TR-69-119. Mandel J., 1974, Introduction a la mecanique des milieux continues deformables, PWN, Warszawa. Maneghin I. V., Pritomanov A. E., Shpittel T. and Knauschner A., 1980, Hot extrusion of tubes and proﬁles, Metallurgya, Moscow (in Russian). Manjoine M. J., 1944, The inﬂuence of rate of strain and temperature on yield stresses in mild steel, J. Appl. Mech. 66, A-211. Medvedev M. I., Laskutov P. A. and Ratner A. G., 1980, Metallurgya, Moscow (in Russian). Meir G. and Clifton R. J., 1986, Eﬀects of dislocation generation at sursaces and subgrain boundaries on precursor decay in high-purity LiF., J. Appl. Phys. 59, 1, 124–148.

January 12, 2007

382

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Dynamic Plasticity

Myers C. D. and Eisenberg M. A., 1974, The eﬀect of radial inertia on combined plastic stress wave propagation in thin-walled tubes, J. Appl. Mech. Trans. ASME 41, 3, 619–624. Myers C. D. and Eisenberg M. A., 1975, The eﬀect of radial inertia on the plastic stress wave speeds in thin-walled tubes under combined stress, Acta Mechanica 22, 163–170. Nowachi W. K., 1974, Stress Waves in Non-Elasic Solids, Pergamon Press, Oxford. Perlin I. A., 1957, Drawing Theory, Metalurghizdat (in Russian). Perzina P., 1966, Fundamental problems in viscoplasticity, Advances in Appied Mechanics, Academic Press, New York, 9, 243–377. Polukhin P. I., Gun G. Y. and Galkin A. M., 1976, Plastic deformation strength of metals and alloys, Reference Book, Metallurgya, Moscow (in Russian). S ¸ andru N. and Camenschi G., 1979, Viscoplastic ﬂow through inclined planes with applications to the strip drawing, Lett. Appl. Engng. Sci. 17, 773–784. S ¸ andru N. and Camenschi G., 1988, Mathematical model of the tube drawing with ﬂoating plug, Int. J. Engng. Sci. 26, 6, 567–585. Shida S. and Awazuhara H., 1973, J. Japan Soc. Tech. Plasticity 14, 267–272. Sokolovski V. V., 1969, Theory of plasticity, Iz. Vashaia Skola (in Russian). Tanimura S., Igaki H., Majima H. and Tada M., 1978, Combined tension–torsion impact testing apparatus and an experimenal study in the incremental wave propagation, Bulletin of the JSME 21, 160, 1455–1461. Tayal A. K. and Natarajan R., 1981, Extrusion of rate-sensitive materials using a viscoplastic constitutive equation and the ﬁnite element method, Int. J. Mech. Sci. 23, 89–98. Ting T. C. T., 1970, Elastic-plastic boundaries in the propagation of plane and cylindrical waves of combined stress, Quart. Appl. Math. 27, 4, 441–449. Ting T. C. T., 1973, On wave propagation problems in which cf = cs = c2 occurs, Quart. Appl. Math. 31, 3, 275–286. Ting T. C. T., 1977, Plastic wave speeds in isotropically work-hardening materials, J. Appl. Mech. Trans. ASME 44, 1, 68–72. Tirosh J. and Kobayeski S., 1976, Kinetic and dynamic eﬀects on the upper-bound loads in metal-forming processes, J. Appl. Mech. Trans. ASME 43, 2, 314–318. Tirosh J., Iddan D. and Pawelski O., 1985, The mechanics of high-speed rolling of viscoplastic materials, J. Appl. Mech. Trans. ASME 52, 309–318. Tobe T., Kato M. and Obara H., 1979, Metal forming by underwater wire explosion 1. An analysis of plastic deformation of circular membranes under impulsive loading, Bulletin JSME 22, 164, 271–278. Upadhyay P. C. and Stokes V. K., 1977, On the dynamic expansion of a circular hole in an inﬁnite plate, J. Appl. Mech. Trans. ASME 44, 577–582. Wistreich J. G., 1955, Proc. Inst. Mech. Engng. London 169, 654. Yew C. H. and Richardson H. A. Jr., 1969, Strain-rate eﬀect and incremental plastic wave in copper, Exp. Mech. 9, 8, 366–373. Yokoyama T., 2001, Finite element computation of torsional plastic waves in a thin walled tube, Archive of Appl. Mech. 71, 6–7, 359–370.

dynamic

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

Chapter 8

Plastic Waves. Perforation

8.1

Introduction

Problems of plastic waves were considered by a lot of authors from variety points of view. Some restrictive relations for possible constitutive equations are due to B´eda [1997]. Problems of plastic waves, problems of perforation etc. were considered; for a review of the subject see Davids [1960], Shewmon and Zackay [1961], Kolsky and Prager [1964], Cristescu [1967], Campbell [1972], Burke and Weiss [1971], Ezra [1973], Rinehart [1975], Cristescu et al. [2003], Zukas [2004] and the papers Backman and Goldsmith [1978], Zhu et al. [1992], Fomin and Kiselev [1997], Cheeseman and Bogetti [2003]. Chernyshov [1966] has shown that the structure of shock waves is practically the same as for gases. A suﬃcient condition is established by Lee [1975] for uniqueness of the dynamic path of an elastic-plastic body subject to prescribed kinematic boundary conditions on a part of the surface and prescribed time-dependent Lagrangian tractions on the remainder. The problems considered until now are of some importance for civil engineering, mechanical engineering, seismology, military applications, etc. The history of soil history is older than that of theory of plasticity. In the last times the theory of plasticity has developed faster, since the experimental facts are easier than in the soils or rock mechanics. Also it is more diﬃcult to interpret the results of soil and rock mechanics. While the plastic deformation in metallic bodies is studied in more than half a century, the experiments with soils and rock mechanics are done only in the last decades. The physics is also quite complex: the soils is considered a continuous medium where solid bodies, ﬂuids and gas are mixed together in a complex manner in what is called a three-phase medium. Sometimes one of these tree medium is absent and the body becomes a two-phase medium. If α1 , α2 , α3 denote the relative proportions by volume of gas, liquid and solid constituents of the soil, so that α1 + α2 + α3 = 1 , (8.1.1) 3 and if ρ1 , ρ2 and ρ3 are the corresponding densities (in g/cm ), the density ρ of the soil considered as a three-phase medium will be ρ = α1 ρ1 + α2 ρ2 + α3 ρ3 . (8.1.2) 383

dynamic

January 12, 2007

10:41

384

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

dynamic

Dynamic Plasticity

The density of air is ρ1 = 1.2 × 10−3 g/cm3 of water ρ2 = 1 g/cm3 , while for the solid an average value ρ3 = 2.65 g/cm3 is used. One is introducing also the concept of porosity as the ratio between the volume of the pores and that of the soil itself. Various constitutive equations have been established for soils and rocks (see Ch. 2). Sometimes Eulerian methods were used since “big” strains are involved. In hydrostatic tests the compressibility of the soil is considered. The compaction property is highly dependent on the water content of the body and is diﬀerent under dynamic and static loadings. In static experiments it is the solid skeleton of the body that generally supports most of the pressure if the sample is drained, because there is suﬃcient time for the water to drain away from the pores during the experiment. In dynamic experiments the situation is quite diﬀerent. The mixture of water and air, if the sample is drained, there is not suﬃcient time for the water to escape during a dynamic experiment. In dynamic loading experiments it is the water–air mixture that supports most of the applied pressure. However if the water–air mixtures, the total volume of air is larger than that of the water, then the mixture is much more compressible than the solid skeleton: in these cases the skeleton supports most of the pressure. For very high pressures however, skeleton compressibility plays an important role in the overall compressibility of the body. 8.2

Various Theories

In the previous sections we have discussed the laws of variation of the volume as well as various possible critical stress conditions. In the present section we present several old stress–strain relations which have played a role in the development of the theory. They are very similar to the classic theories of plasticity. S. S. Grigorian [1959, 1960b, 1967] assumes that the Prandtl–Reuss theory can be used to describe the mechanical properties of soft soils. If vi are the velocity components, and 1 ∂vi ∂vj (8.2.1) + Dij = 2 ∂xj ∂xi are the components of the rate of strain, and xi are the Cartesian coordinates, then the constitutive equations are ˜ dσ ij + λσij , dt where the derivatives are taken in the sense of Jauman ˜ ∂σij dσ ∂σij ij = + vk − Ωik σjk − Ωjk σik , dt dt ∂xk = 2GDij

(8.2.2)

(8.2.3)

and 2Ωij =

∂vi ∂vj − . ∂xj ∂xi

(8.2.4)

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

Plastic Waves. Perforation

dynamic

385

The factor λ in (8.2.2) plays the same role as in classical plasticity theory. The elastic behavior of the material corresponds to λ = 0, and the plastic state to λ > 0. This factor can be expressed in terms of invariants following the usual and summation, we obtain procedure: by multiplying (8.2.2) by σij 4GW ≡ 2Gσij Dij = σij

˜ dσ ij + λσij σij . dt

(8.2.5)

Since IIσ = F (p) and σij

˜ dσ dIIσ ij = , dt dt

it follows from (8.2.5) that λ=

4GW − F (p)(∂p/∂t + vi ∂p/∂xi ) . 2F (p)

(8.2.6)

This formula is used only if

4GW > F (p)

∂p ∂p + vi ∂t ∂xi

,

otherwise λ = 0. To the constitutive equation one is adding the equation of motion and the continuity equation. The Prandtl–Reuss constitutive equation is proposed for dynamic problems for soils since soils being dispersed media, there is not a single reference conﬁguration for them. The system of equation was analyzed also from the thermodynamic point of view. There are three functions (Grigorian [1960a]) to be determined from tests: p = f (ρ, ρm , H) ,

Hσ = F (p, H) ,

G = G(ρm , H) .

(8.2.7)

Here H is the humidity, i.e., the ratio between the volume of the water and that of the mineral particles, per unit mass of soil. Since in dynamic problems there is no time for water to drain away from the pores dH/dt = 0. If H = Hmax , that is the soil is fully saturated, in dynamic experiments such soils behave as barotropic liquids. Thus for small or moderate values of H the soil is irreversible compressible. The other functions involved in (8.2.7) are determined as usual for compressible materials. The Coulomb ﬂow rule was used by Chadwick et al. [1964], as associated ﬂow rule. They have assumed that the soil obeys Hooke’s law within the elastic range and the Coulomb’s criterion and the associated ﬂow rule during yielding under the restriction of perfectly plastic ﬂow. According to the rule mentioned, if f (σij ) = 0 denotes the yield function and the elastic domain corresponds to f < 0, then the plastic part of the rate of strain is furnished by ∂f ε˙pij = λ˙ , ∂σij

(8.2.8)

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

386

dynamic

Dynamic Plasticity

˙ where λ(x, t) is a scalar function satisfying the condition λ ≥ 0. The elastic strain rates satisfy a Hookean law. The authors consider only spherical-symmetry problems and therefore spherical polar coordinates r, θ, ϕ are used. The principal components of the stress are σr , σθ and σϕ . If ∂v v , ε˙θ = ε˙ϕ = ∂r r are the components of the strain rate then the associated ﬂow rule is ∂f ∂f ∂f ε˙pr = λ˙ , ε˙pθ = λ˙ , ε˙pϕ = λ˙ , ∂σr ∂σθ ∂σϕ ε˙r =

(8.2.9)

(8.2.10)

where f is one of the six expressions involved in the Coulomb yield condition. At singular points the generalized ﬂow rule proposed by Koiter [1953] and Prager [1953] is used. The “plastic gas” model was considered by Rakhmatulin and Stepanova [1958]. It was used for soils in one-dimensional problems. By deﬁnition a “plastic gas” is a continuous body whose density changes during loading (increasing pressure) according to a prescribed law, while during unloading (decreasing pressure) the density remains constant and equal to the maximum density reached during loading. On repeated loading the density does not change as long as the pressure does not exceed the value reached previously. This model was proposed for the use in problems in which high pressures are involved. Since experiments have shown that for such pressures the temperature rise is negligible, temperature changes are generally disregarded. Very many problems have been solved using the model mentioned above (Rakhmatulin et al. [1964]). Let us see what Sagomonian [1961] has to say about this problem. The problem is one-dimensional and cylindrically symmetrical. In cylindrical Lagrange coordinates r and θ, the equation of motion and the equation of mass conservation are ∂2u ∂σr ∂ + (σr − σθ ) (r + u) , ρ0 r 2 = (r + u) ∂t ∂r ∂r 1 ∂ ρ0 (r + u)2 = r. 2 ∂r ρ Assuming that σr = σθ = −p, the ﬁrst equation becomes

(8.2.11)

r + u ∂p ∂2u . (8.2.12) =− ∂t2 r ∂r The problems to be solved are the following. An inﬁnitely long cylindrical explosive of initial radius r0 is exploded in an inﬁnite medium. It is assumed that the explosion products expand as a polytrophic gas whose adiabatic exponent is γ. Since in most cases the maximum pressure is reached just behind the shock wave front, Sagomonian assumes that the density of the plastic gas changes only on the front (in the transition zone). Thus, behind the shock wave front the density is a function only of r, and the motion is that of a non-homogeneous incompressible medium. ρ0

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

Plastic Waves. Perforation

To the equation (8.2.11) one attaches the law of soil compressibility 1 ρ0 (σr + σθ + σz ) = F 1 − , 3 ρ

dynamic

387

(8.2.13)

and the Coulomb condition is written in the form σr − σθ = −τ0 + µ(σr + σθ )

(8.2.14)

with τ0 = 2k cos ϕ and µ = sin ϕ and assuming that σr > σθ . The ﬁrst case considered is µ = 0, i.e., the case of frictionless soils. The Eq. (8.2.11) becomes ∂ ∂2u ∂σr − τ0 (r + u) , = (r + u) ∂t2 ∂r ∂r or, by formal integration with respect to r, r∗ r ∂2u σr (r, t) = ρ0 dr + τ0 {ln(r + u) − ln R} − pk (t) . 2 r0 r + u ∂t ρ0 r

(8.2.15)

(8.2.16)

Here r0 is the radius of the charge hole at the moment of explosion, pk (t) is the pressure at r = r0 , while the radius of the hole at a certain moment is R(t) = r0 + u(r0 , t). The relation (8.2.16) holds for all points between the hole and the shock wave front. Thus denoting by an asterisk the values of any function on this front, we have r∗ r ∂2u ∗ dr + τ0 {ln r∗ − ln R} − pk (t) . (8.2.17) σr = ρ0 2 r0 r + u ∂t From (8.2.16) and (8.2.17), it follows that r∗ r ∂2u ∗ σr − σr = −ρ0 dr − τ0 {ln r∗ − ln(r + u)} . 2 r0 r + u ∂t

(8.2.18)

If, in (8.2.14) µ = 0, then the ﬁrst equation (8.2.11) becomes (r + u)

∂ ∂2u τ0 ∂ ∂σr + v (r + u)σr = ρ0 r 2 + (r + u) , ∂r ∂r ∂t 1 + µ ∂r

(8.2.19)

with v = 2µ/(1 + µ). By multiplying both sides of (8.2.19) by (r + u)v−1 and integrating with respect to r, we obtain r ∂2u v (r + u) σr (r, t) = ρ0 (r + u)v−1 r 2 dr ∂t r0 +

τ0 1 [(r + u)v − Rv ] − Rv pk (t) . 1+µv

Hence, on the shock wave front we have r∗ ∂2u τ0 1 ∗v (r − Rv ) − Rv pk (t) . (r + u)v−1 r 2 dr + r∗v σr∗ = ρ0 ∂t 1+µv r0

(8.2.20)

(8.2.21)

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

388

dynamic

Dynamic Plasticity

Thus, from the last two formulae it follows that r∗ ∂2u v ∗v ∗ (r + u) σr − r σr = −p0 (r + u)v−1 2 rdr ∂t r τ0 {r∗v − (r + u)v } . v(1 + µ)

−

For cohesionless soils (τ0 = 0) this formula becomes r∗ ∂2u v ∗v ∗ (r + u) σr − r σr = −ρ0 (r + u)v−1 r 2 dr . ∂t r

(8.2.22)

(8.2.23)

As has already been mentioned, it is assumed that the density change occurs only in the transition zone, and therefore, that behind the shock wave front, the density is a function only of the Lagrangiann coordinate r. Thus, from the second equation (8.2.11), by integration with respect to r, it follows that (r + u)2 = 2ψ(r) + ϕ(t) with

r

ψ(r) = r0

ρ0 r¯d¯ r. ρ(¯ r)

(8.2.24)

The arbitrary function ϕ(t) is determined by the boundary conditions r = r0 : ψ(r0 ) = 0 ,

ϕ(t) = {r0 + u(r0 , t)}2 = R2 (t)

so that (r + u)2 = 2ψ(r) + R2 (t)

(8.2.25)

r∗2 = 2ψ(r∗ ) + R2 (t) .

(8.2.26)

or, on the shock wave front

From (8.2.25), we obtain the velocity and acceleration as RR˙ ∂u = , ∂t 2ψ(r) + R2 ¨ ˙ 2 ∂2u R˙ 2 + RR (RR) = − . ∂t2 [2ψ(r) + R2 ]3/2 2ψ(r) + R2

(8.2.27)

Across the shock wave front the jump conditions ρ0 D = ρ(D − u˙ ∗ ) ,

ρ0 Du˙ ∗ = −σr∗ − pa

are satisﬁed. In these conditions, D is the velocity of the displacement of the wave, u˙ ∗ the material velocity just behind the shock front, and pa is the pressure ahead of the shock wave. We therefore obtain dψ 1 ρ0 u˙ ∗2 u˙ ∗ ρ0 ∗ ∗ + pa , D = , b(r ) = = . −σr = 1 − b(r∗ ) 1 − b(r∗ ) ρ(r∗ ) dr r r=r∗ (8.2.28)

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

dynamic

Plastic Waves. Perforation

389

Introducing (8.2.25)–(8.2.28) into (8.2.18), (8.2.22) and (8.2.23), we obtain r∗ r∗ rdr rdr ¨ + R˙ 2 )ρ0 ˙ 2 ρ0 −σr (r, t) = (RR − (R R) 2 2ψ + R (2ψ + R2 )2 r r +

˙ 2 ρ0 (RR) r∗ + pa , + τ ln 0 1 − b r∗2 r+u

¨ + R˙ 2 )ρ0 −(r + u) σr = (RR

r∗

v

r

r

∗

˙ 2 ρ0 − (RR) r

rdr (2ψ + R2 )1−(v/2)

˙ 2 rdr ρ0 (RR) + ∗ 2 2−(v/2) 1 − b (r )2−v (2ψ + R )

τ0 (r∗v − (r + u)v ) + pa r∗v , + v(1 + µ) ¨ + R˙ 2 )ρ0 −(r + u)v σr = (RR r

˙ 2 ρ0 − (RR) r

+

r

∗

(8.2.29)

r∗

(8.2.30)

rdr (2ψ + R2 )1−(v/2)

rdr (2ψ + R2 )2−(v/2)

˙ 2 ρ0 (RR) + pa r∗v . ∗ 1 − b (r )2−v

(8.2.31)

From the relations (8.2.27)–(8.2.31) it follows that all the quantities required to describe the motion can be expressed by two functions, i.e., a function only of the Lagrangean coordinate ψ(r) and another one function only of time R(t). A ﬁrst solution is obtained, assuming that behind the shock wave front the density is a constant ρ1 and that ρ0 /ρ1 = b1 .

(8.2.32)

From (8.2.24) and (8.2.6) it then follows that ψ(r) =

1 b1 (r2 − r02 ) , 2

r∗2 =

R2 (t) − b1 r02 . 1 − b1

(8.2.33)

With this expression for ψ(r), one can compute the integrals in (8.2.29)–(8.2.31) and thus express the solution in terms of the function R(t) and its ﬁrst two derivatives. The case when the density is not constant behind the shock wave front has also been considered by an iterative method. In the same paper by Sagomonian [1961], solutions for the cases of polar symmetry and of the propagation of plane waves were also given. Many other problems were solved using the previously mentioned model for the soils concerned. For instance, the penetration of sharp, rotationally symmetrical bodies into the ground was examined by Rachmatulin et al. [1964] in Ch. IV, where a bibliography of the problem is also given.

January 12, 2007

390

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Dynamic Plasticity

The propagation of spherical collapsing waves which propagate in an elasticbrittle material was studied by Aliev [1963]. The same problem for an elastic-plastic medium, which is incompressible both during loading and unloading and satisﬁes a Tresca yield condition during loading, was considered by Shemiankin [1961]. In another paper, Medvedeva and Shemiankin [1961] have examined the propagation of spherical waves in a medium satisfying a Coulomb yield condition, for a compaction law written in the form n ρ0 , −σ = K 1 − ρ where K and n are positive constants. The model is applied to various rocks. The locking medium was considered by many authors. The main idea is: once the density of the medium reaches a certain limit value, characteristic of the medium, no further density increase is possible. During unloading, the density remains constant and equal to the limiting density. There has also been proposed a model known as an ideal locking medium, which is deﬁned by most authors as follows. The material, of a certain initial density, does not at ﬁrst oﬀer any resistance to compression, but once the limiting density ρ∗ is reached, this remains constant during any subsequent motion and Coulomb’s yield condition is satisﬁed. In a certain sense, the ideal locking medium is a model corresponding to the perfectly plastic/rigid model of plasticity theory. It seems that the idea of locking medium was ﬁrst used in the paper by Ishlinskii et al. [1954] and Salvadori et al. [1955]. These authors start from the experimental observation that if a cylindrical hole some ten meters deep and of diameter 10 to 15 cm is made in a soil (of clay type) and if an explosion is produced in this hole, the density of the soil to a distance of 1 m around the hole increases considerably (approximately 30 per cent). This experiment is described mathematically. Ishlinskii [1954] established the equations of plane motion of certain materials like sand. He made four hypothesis: the medium is non-elastic and incompressible, the stress do not depend on the rate of strain, the directions of principal axes of stresses coincide at each point with the directions of the principal axes of strain, the state of stress satisﬁes the same yield condition as in the static case. The propagation of spherical shock waves in sandy type medium was considered by Kompaneets [1956]. He assumed that initially the medium is of density ρ0 and has a small resistance to shear. When reaching the density ρ1 , the medium becomes incompressible and plastic, and satisﬁes a plasticity condition of the Coulomb form σr − σθ = k + m(σr + σθ + σϕ ) . He also assumes that shock waves are produced by an explosion detonated in a small sphere. Andriankin and Koryavov [1959] consider that the soil compaction along the shock wave front is not constant. They assumed that the compaction produced by the shock wave front depends on the amplitude of the wave; a power law of compaction of the form

dynamic

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Plastic Waves. Perforation

dynamic

391

p = p0 β 1−n εn , is proposed. Here n and β are constants, p0 is the pressure ahead of the wave front and ε = 1 − ρ0 /ρ. A viscous model for plug formation in plates is due to Pytel and Davids [1963]. The paper presents the analysis of a viscous model for the study of impact of plates by projectiles under conditions which would lead to failure of the plate by the formation of a plug. The impact is represented by a velocity uniformly distributed over a circular area on the plate surface. Only the vertical shearing stress is considered and it is assumed to depend only on the radial coordinate. The stress, velocity and displacement proﬁles are calculated for the viscous model. The calculated displacement proﬁles are compared with experimental proﬁles. Spherical elastic-plastic boundaries due to loading were considered by Srinivasan and Ting [1974]. They have considered spherical waves in an elastic-plastic, isotropically work-hardening medium generated by radial stress uniformly applied at a spherical cavity. The radial stress and its time derivative at the cavity may be discontinuous at time t0 . If the applied radial stress is continuous while its time derivative is not, the discontinuity propagates into r > r0 along the characteristics and/or the elastic-plastic boundaries. If the applied radial stress itself is discontinuous, the discontinuity may propagate into r > r0 in the form of a shock wave, or a centered simple-wave, or a combination of both. In any case, the solutions in the neighborhood of (r0 , t0 ) are obtained for all possible combinations of discontinuous loadings applied at r = r0 . This is a systematic study on the nature of the solution near (r0 , t0 ) where the applied load is discontinuous. Solutions for specials materials, such as linearly work-hardening or ideally-plastic ones, and for special applied loadings at the cavity obtained by other workers, in which the nature of the solutions near (r0 , t0 ) are assumed a priori rather than determined, are compared with the results obtained here. Wave propagation in elastic circular membrane is considered by Hutton and Counts [1974]. One is starting from the problem given in Cristescu [1967] Ch. 5. The equations of motion for meridian line of the membrane are ∂2η ξη σ1 ∂η p ∂ω ∂ σ2 − (1 + ε1 ) ξ + η0 2 = η ∂τ p0 ∂η0 ∂η0 1 + ε1 p0 ∂η0 p0 p ∂η ∂ ∂2ω ξ σ1 ∂ω − −η0 2 = η ∂τ p0 ∂η0 ∂η0 1 + ε1 p0 ∂η0 where η and η0 are the actual and initial radial coordinates, ω is the axial coordinate, ε1 , ε2 , ε3 are the meridional, circumferential, normal strains, and σ1 , σ2 , σ3 are the corresponding stress components, p/p0 is the ratio of instantaneous pressure to maximum pressure, τ is the nondimensional time, and ξ = 1 + ε2 . The totally hyperbolic equations are integrated along characteristics. Strain and inertia waves propagate with constant velocities during elastic deformation.

January 12, 2007

392

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Dynamic Plasticity

The buckling problem. Dynamic axisymmetric buckling of circular cylindrical shells struck axially by a mass is studied by Karagiozova and Jones [2000] in order to clarify the initiation of buckling and to prove some insight into the buckling mechanism as a transient process. It is assumed that the material is elastic-plastic with linear strain hardening and displaying the Bauschinger eﬀect. The deformation process is analyzed by a numerical simulation using a discrete model. It is found that the development of the buckling shape depends strongly on the inertia properties of the striker and on the geometry of the shell. A new concept is presented by Karagiozova and Jones [2001], [2002] for the dynamic elastic-plastic axisymmetric buckling of circular cylindrical shells under axial impact. The phenomena of dynamic plastic buckling and dynamic progressive buckling are analyzed from the viewpoint of stress wave propagation resulting from an axial impact. The conditions for the development of dynamic plastic buckling are obtained. It is concluded that shells made of strain rate insensitive materials can respond either by dynamic plastic buckling or dynamic progressive buckling, depending on the inertia properties of the shell, while those shells made of strain rate sensitive materials respond always by dynamic progressive buckling. It is shown that the prediction for the peak load depends on the particular yield criterion used in the analysis. The speeds of the stress waves that can propagate in an elastic-plastic medium with isotropic linear strain hardening in a plane stress state are obtained by Karagiozova [2004] to analyze the inﬂuence of the transient deformation process on the initiation of buckling in square tubes under axial impact. The kinematic conditions across a surface of discontinuity were employed to obtain the stress wave propagation speeds for an initial condition. It is shown that the plastic wave speeds depend on the stress state and on the direction of wave propagation. The material hardening properties have a stronger eﬀect on the speed of the slow plastic wave, while the shear stress aﬀects both the speeds of the fast and slow plastic waves. The magnitude of the instantaneously applied in-plane load at t = 0, which results from an impact in the direction “one”, is obtained as a function of the initial velocity when using the diﬀerential relationship along the characteristics. A general non-dimensional formula based on the dynamic cavity-expansion model is proposed buy Chen and Li [2002] to predict penetration depth into several mediums subjected to a normal impact of a non-deformable projectile. The proposed formula depends on two dimensionless numbers and shows good agreement with penetration tests on metal, concrete and soil for a range of nose shapes and impact velocities. The validity of the formula requires that the penetration depth is larger than the projectile diameter and the projectile nose length while projectile remains rigid without noticeable deformation and damage. A theoretical investigation of plane waves in granular soils is presented by Osinov [1998]. Dynamic equations are derived with the use of the hypoplasticity theory for granular materials. For numerical calculations the material parameters of Karlsruhe sand are used. Wave speeds slopes of characteristics of dynamic equations are calculated for various stresses and densities.

dynamic

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Plastic Waves. Perforation

8.3

dynamic

393

Perforation with Symmetries

For perforation ﬁrst to be seen is the paper by Backman and Goldsmith [1978]. This big paper presents the problem until 1978, characteristics of the projectile and the targets, semi-inﬁnite targets, thin plate penetration and perforation, and thick plates. The problem was considered also by Demiray and Eringen [1978]. By means of a nonlocal viscous ﬂuid model, an investigation is carried out of the problem of penetration of a cylindrical projectile into a plate leading to a failure of the plate by a plug formation. The eﬀect of impact is represented by a uniform initial velocity distribution over a circular region on the surface of the plate. The behavior of this plate material is assumed to be viscous and spatially nonlocal, and only the eﬀects of vertical shearing stress are considered. The expression of stress, velocity and displacement are obtained and the calculated displacement proﬁles are compared with some existing experimental proﬁles. The problem of impact of a liquid cylinder on an elastic-plastic solid was considered by Lush [1991]. He has modiﬁed the model to incorporate the unloading of the plastic wave which is produced by multiple reﬂections of the elastic release wave. In general the agreement between penetration rate, contact pressure and depth of penetration is good. Afterwards, the ballistic strengths of composites are considered mainly in Cheeseman and Bogetti [2003]. First is described a single ﬁber subjected to transverse impact (see Ch. 5). Then is described the mechanisms inﬂuencing ballistic performance. The ﬁbers are Kevlar or Spectra laminates which are impacted with impact velocities up to 1000 m/s. If the cover factors of the fabrics are from 0.6 to 0.95 they are eﬀective in ballistic applications. The crimp that is the undulation on the yarns due to their interlacing in the woven structure is also discussed. Generally is discussed all the factors which have collaboration in the perforation. An oblique penetration was considered by Macek and Duﬀey [2000]. A spherical cavity expansion is assumed with the local velocity normal equal to the penetrator surface VN (see Fig. 8.3.1). Incompressible kinematics is also assumed. The incompressible condition is r∗3 − ri∗3 = r3 − ri3 ,

(8.3.1)

where ∗ refer to the deformed conﬁguration, the other radii to the undeformed conﬁguration. The subscript i refer to the inner surface of the ith layer. The radial displacement is ur = r∗ − r = (ri∗3 + r3 − ri3 )1/3 − r .

(8.3.2)

The radial velocity distribution is obtained from (8.3.2) Vr =

ri∗2 Vi , r∗2

(8.3.3)

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

394

dynamic

Dynamic Plasticity

Fig. 8.3.1

Spherical cavity expansion idealization.

with V the velocity. The radial acceleration is determined by diﬀerentiation: ∗ 2 ∗3 ri ˙ i + 2ri∗ Vi2 1 − ri . (8.3.4) V ar = r∗ r∗2 r∗5 The corresponding spherically symmetric strain ﬁeld as a result of incompressibility is obtained from (8.3.2): εθ =

r∗ r∗ ur = − 1 = ∗3 −1, ∗3 r r (r − ri + ri3 )1/3

(r∗3 − ri∗3 + ri3 )2/3 dur = −1. dr r∗2 The approximated eﬀective strain ﬁeld is εr =

εθ − εr =

R3 r∗3 − r3 r∗3 − r3 = ∗2 ∗3 i ∗3 i 3 1/3 ≈ i ∗3 i . 3 r r r (r − ri + ri )

(8.3.5)

(8.3.6)

(8.3.7)

For a Hooke’s material with spherically symmetry and incompressible, the eﬀective stress is 2 (8.3.8) σe = σθ − σr = E(εθ − εr ) . 3 If the material has yielded and a Mohr–Coulomb yield criterion with damage is used then Y0 (8.3.9) Y = σθ − σr = Y0 + λP , P ≥ − , εθ ≤ εut , λ Y = σθ − σr = λD P ,

εθ > εut ,

(8.3.10)

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Plastic Waves. Perforation

dynamic

395

where εut is the tensile failure strain, P is the pressure, Y0 is the yield stress at zero pressure, λ is the Mohr–Coulomb slope, and λD denotes the slope after failure. The equilibrium equation in the deformed conﬁguration is dσr 2 + ∗ (σr − σθ ) = ρar = ρV˙ r . dr∗ r Combining (8.3.4) and (8.3.11) ∗ 2 dσr 1 2 ri ri∗3 ∗ ˙ . + (σ − σ ) = ρ + 2ρr − V r θ i 1 dr∗ r∗ r∗ r∗2 r∗5

(8.3.11)

(8.3.12)

The governing equation for an elastic sub-layer is found from (8.3.7), (8.3.8) and (8.3.12): ∗ 2 dσr 1 4E ri ri∗3 ∗ 2 ˙ =ρ ∗ − ∗5 + ∗4 (ri∗3 − ri3 ) . (8.3.13) Vi + 2ρri Vi ∗ ∗2 dr r r r 3r The eﬀective stress is 2 ri∗3 − ri3 E . (8.3.14) 3 r∗3 Integrating (8.3.13) with σr = σr0 at r∗ = r0∗ on the outer surface layer, ∗ 1 ri 1 ri∗3 ri∗3 ri∗ ∗ ˙ + ρr − + − − σr (r∗ ) = σr0 + 2ρri∗ Vi2 V i i r0∗ r∗ 4r∗4 4r0∗4 r0∗ r∗ ri3 ri∗3 4E ri∗3 1 − . (8.3.15) − + 9 r0∗3 r∗3 ri∗3 σe =

Putting r¯ = ri∗ /r∗ and r¯0 = ri∗ /r0∗ this equation becomes r¯4 − r¯04 + ρri∗ V˙ i (¯ σr (¯ r ) = σr0 + 2ρVi2 r¯0 − r¯ + r0 − r¯) 4 ri3 4E 3 3 (¯ r − r¯ ) 1 − ∗3 . + 9 0 ri

(8.3.16)

The equivalent pressure is σr + 2σθ . (8.3.17) 3 Using (8.3.7), (8.3.8), (8.3.16) in (8.3.17) the pressure for an elastic layer is ri3 4 P (¯ r ) = −σr − E r¯3 1 − ∗3 9 ri r¯4 − r¯04 + ρri∗ V˙ i (¯ r0 − r¯) = − σr0 + 2ρVi2 r¯0 − r¯ + 4 ri3 4E r¯03 1 − ∗3 . (8.3.18) − 9 ri P (¯ r) = −

The radial stress distribution and pressure depend also on the acceleration term.

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

396

dynamic

Dynamic Plasticity

For a plastic sub-layer the eﬀective stress σe can be written using (8.3.8), (8.3.9), and (8.3.17) as α σe = σθ − σr = Y0 + λP = Y0 − ασr , (8.3.19) λ where α = 3λ/(3 + 2λ). From (8.3.19) we get also α 2 Y0 + σr . (8.3.20) P =− λ 3 Using (8.3.19) in (8.3.12) we get for the plastic sub-layer: ∗ 2 dσr 1 2αY0 2α ri ri∗3 ∗ 2 ˙ + + σ = ρ + 2ρr V − . V r i i i dr∗ r∗ r∗ r∗2 r∗5 λr∗

(8.3.21)

Multiplying with the integrating factor r2α we get: ∗2α−1 r∗3 r∗2α−4 ρr∗2 V˙ i ∗2α−1 Y0 ∗2α r − i + i r σr r∗2α = 2ρRVi2 + r +K. 2α − 1 2α − 4 2α − 1 λ (8.3.22) Applying the boundary condition σr = σrx at the elastic-plastic boundary r∗ = rx∗ we get: # ∗ 2α $ ∗ 2α ri∗3 Y0 rx rx 1 ∗ 2 1− − + σ + 2ρr V σr (r) = rx i i λ r∗ r∗ r∗ (2α − 1) r∗4 (2α − 4) − 2ρri∗ Vi2

rx∗ r∗

2α

ri∗3 ρri∗2 V˙ i 1 1 rx∗2α−1 − + . − ∗2α rx∗ (2α − 1) rx∗4 (2α − 4) 2α − 1 r∗ r (8.3.23)

By non-dimensionalizing the radius r¯x = ri∗ /rx∗ we obtain # 2α $ 2α r¯ r¯ Y0 1− + r) = σrx σr (¯ λ r¯x r¯x

r /¯ rx )2α r /¯ rx )2α r¯4 − r¯x4 (¯ r¯ − r¯x (¯ − 2α − 1 2α − 4 # $ 2α r¯ ρri∗ V˙ i r¯ − r¯x . + 2α − 1 r¯x

+ 2ρVi2

(8.3.24)

Three possible stress states are possible: elastic σe < Y0 + λP , plastic σe = Y0 + λP or pressure-failed P < −Y0 /λ. To determine if the material yields ﬁrst or pressurefails ﬁrst, the expanded radius at which yielding occurs Ry can be compared to the expanded radius at which failure occurs Rf . Setting (8.2.14) equal to the yield stress produces 3 Ry 2 σe = E = Y0 + λP . (8.3.25) 3 r∗

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

dynamic

Plastic Waves. Perforation

397

Using (8.3.18) in (8.3.25) yields Ry3 =

9(Y0 − λσr )r∗3 . (6 + 4λ)E

(8.3.26)

The failure radius Rf is found by setting the pressure given by (8.3.18) equal to the failure pressure: P = −σr −

4ERf3 Y0 =− . ∗3 9r λ

(8.3.27)

Solving for Rf3 : 9r∗3 (Y0 − λσr ) . (8.3.28) 4λE From (8.3.26) and (8.3.28) the material will yield before pressure-failing Ry3 < Rf3 if 1 1 < (8.3.29) 6 + 4λ 4λ because σr < 0. Any real Mohr–Coulomb material 0 < λ < ∞ will yield before pressure-failing. The materials will not pressure-fail after yielding if Y0 α 2 Y0 + σr > − (8.3.30) P =− λ 3 λ or if Y σr < . (8.3.31) λ Since σr < 0 pressure-failure cannot occur. The elastic-plastic interface r¯x is found from the condition that the eﬀective stress σe in the elastic region equals the current yield stress, Y = Y0 + λP . From (8.3.14) and (8.3.18) # 2 3 ri3 r¯x4 − r¯04 2 E r¯ 1 − ∗3 = Y0 + λP = Y0 + λ − σr0 + 2ρVi r¯0 − r¯x + 3 x ri 4 Rf3 =

+ ρri∗ V˙ i (¯ r0

$ ri3 4E r¯03 1 − ∗3 . − r¯x ) − 9 r1

(8.3.32)

Simplifying (8.3.32) we ﬁnd the following equation for r¯x : C1 where

r¯x4 − C¯1 r¯x + C2 r¯x3 − C3 = 0 , 4

(8.3.33)

ri3 2 , C2 = E 1 − ∗3 , C1 = 3 ri 4 ri3 r¯0 4λE r¯03 − r¯0 − λρri∗ V˙ i r¯0 − 1 − ∗3 . C3 = Y0 − λσr0 + 2λρVi2 4 9 ri 2λρVi2

C¯1 = 2λρVi2 + λρri∗ V˙ i ,

Equation (8.3.33) is solved by Newton iteration for 0 < r¯x < 1.

January 12, 2007

398

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

dynamic

Dynamic Plasticity

Further is described a damaged sub-layer, damage-undamaged interface location, stress-based failure, multilayer systems, etc. A comparison with the experiments (data by Longcope and Forrestal [1983]): 162 kg penetrator, 1.56 m long, 0.156 m diameter ogival nose shape (6.0 caliber radius head), impact velocity 520 m/s, impact angle 90◦ , angle of attack of 0◦ , ρ = 1.62×10−9 Mg/mm3 , E = 3.192×103 MPa, Y = 10.0 MPa, λ = 1.00, λd = 1.00. The comparison is very good. Some other comparisons with experimental data are also given. Another spherical cavity-expansion and comparison with experiment is due to Forrestal and Tzou [1997]. A spherically symmetric cavity is expanded from zero initial radius at constant velocity V . For slow enough V , there are three regions of response: an elastic region, a region with radial cracks (the material reaches its tensile strength), and a plastic region (the material reaches its shear strength). The plastic region is bounded by r = V t and r = ct, the cracked region is bounded by r = ct and r = c1 t, and the elastic region is bounded by r = c1 t and r = cd t where r is the radial Eulerian coordinate, t is time and c, c1 , and cd are velocities. In the plastic region a linear pressure-volumetric strain relation and a Mohr–Coulomb yield criterion are satisﬁed: pK(1 − ρ0 /ρ) = Kη p = (σr + σθ + σφ )/3 ; σr − σθ = λp + τ ;

σθ = σφ

(8.3.34)

τ = [(3 − λ)/3]Y

with Y the uniaxial compressive strength, and σr and σθ are the Cauchy stress, positive in compression. In the cracked region σθ = 0. For the elastic incompressible material we have: ∂v 2v ∂σr 2 ∂v ∂v + = 0, + (σr − σθ ) = −ρ0 +v (8.3.35) ∂r r ∂r r ∂t ∂r with v the particle velocity. From (8.3.34) and (8.3.35) we have ∂σr αλσr ατ ∂v ∂v + + = −ρ0 +v ∂r r r ∂t ∂r

(8.3.36)

where α = 6/(3 + 2λ). With dimensionless variables S = σr /τ , U = v/c, ε = V /c and the similarity transformation ξ = r/ct where c is he elastic-plastic interface velocity we have: 2U dS αλS α ρ 0 c2 dU dU dU + = 0, + =− + ξ −U . (8.3.37) dξ ξ dξ ξ ξ τ dξ dξ The boundary condition at the cavity surface is U (ξ = ε) = ε and (8.3.37a) is U = ε3 /ξ 2 . Introducing in (8.3.37b) and multiplying with ξ αλ , we get: d αλ 2ρ0 c2 ε3 αλ−2 2ρ0 c2 ε6 αλ−5 (ξ S) = −αξ αλ−1 − ξ ξ + dξ τ τ

(8.3.38)

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

Plastic Waves. Perforation

dynamic

399

which can be integrated 2ρ0 c2 ε3 1 2ρ0 c2 ε6 1 1 − + + Cξ −αλ (8.3.39) λ τ (αλ − 1) ξ τ (αλ4) ξ 4 where C is the integration constant. Particle velocity is obtained by diﬀerentiating displacement: S=−

3τ 2 3ρ0 c2 , U= + . 3 3ξ Eξ 2Eξ 2 At the elastic and plastic interface the Hugoniot jump conditions hold: S=

ρ2 (v2 − c) = ρ1 (v1 − c) ,

σ2 + ρ2 v2 (v2 − c) = σ1 + ρ1 v1 (v1 − c)

(8.3.40)

(8.3.41)

where 1 and 2 represent the quantities in elastic and plastic regions. For incompressible material ρ1 = ρ2 = ρ0 and radial stress and particle velocity are continuous. From (8.3.41b) we get for 1/3 3τ V = ξ=1:ε= c 2E and 2 −αλ 1 2ρ0 V 2 ε4 ε − + S= ξ − αλ λ τ (1 − αλ)ξ (4 − αλ)ξ 4 2ε3 2ε6 ρ0 c2 3τ + − ξ −αλ . + τ E αλ − 1 αλ − 4 Or the radial stress at the cavity surface: ρ0 V 2 6 2αλ 1−αλ 2 −αλ 1 2ε4αλ ε − ε S(ε) = − + + αλ λ τ (1 − αλ)(4 − αλ) 1 − αλ 4 − αλ (8.3.42) In the elastic-cracked-plastic response σθ = σφ = 0 and the radial stress is ε3 ε6 3 + 2λ −αλ 1 2ρ0 c2 ξ − − − S= λ(3 − λ) λ τ (αλ − 1)ξ (αλ − 4)ξ 4 2ρ0 c2 ε3 ε6 ξ −αλ . (8.3.43) + − τ αλ − 1 αλ − 4 For a compressible target the equations are: ∂σr 2v ∂ρ ∂ρ 2(σr − σθ ) ∂v ∂v ∂v =− , ρ + +v + = −ρ +v ∂r r ∂t ∂r ∂r r ∂t ∂r (8.3.44) Eliminating σθ and ρ we get 2v α ∂σr ∂v ∂σr + =− +v , ∂r r 2K(1 − η) ∂t ∂r ∂σr αλσr ατ ρ0 ∂v ∂v + + =− +v ∂r r r 1 − η ∂t ∂r

(8.3.45)

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

400

dynamic

Dynamic Plasticity

where 6 , α= 3 + 2λ

ατ η= 2K

σr 2 − τ 3

.

Introducing the dimensionless variables S = σr /τ, U = v/c, ε = V /c, β = c/cp , β1 = c1 /cp , βε = V /cp , c2p = K/ρ0 , ξ = r/ct the system of equations becomes dU 2U/ξ + (τ α2 /2Kξ)[(ξ − U )/(1 − η)](λS + 1) = , dξ (αβ 2 /2)[(ξ − U )/(1 − η)]2 − 1 dS α/ξ + αλS/ξ + (2β 2 KU/τ ξ)[(ξ − U )/(1 − η)] = dξ (αβ 2 /2)[(ξ − U )/(1 − η)]2 − 1

(8.3.46)

which are to be solved with the Runge–Kutta method. The radial stress and particle velocity are continuous at the elastic-plastic interface. Thus at ξ = 1 we have S1 = S 2 =

2[(1 − 2v)(1 + γβ) + (1 + v)(γβ)2 ] , 3(1 − 2v)(1 + γβ) − 2λ(1 + v)(γβ)2

3τ (1 + v)(1 − 2v)(1 + γβ) , E[3(1 − 2v)(1 + γβ) − 2λ(1 + v)(γβ)2 ] 2 cp 1+v E(1 − v) γ2 = , c2d = = cd 3(1 − v) (1 + v)(1 − 2v)ρ0

U1 = U2 =

(8.3.47)

with S2 and U2 known, one can calculate the dimensionless radial stress and particle velocity in the plastic region. Further the elastic-cracked-plastic response is calculated and a cavity-expansion numerical results is given for K = 6.7 GPa, Y = 130 MPa, λ = 0.67, E = 11.3 GPa, v = 0.22, f = 13 NPa, ρ0 = 2260 kg/m3 . The penetration equations and comparison with data are reasonable. Dynamic cavity expansion of ceramic materials when subjected to cavity expansion at constant velocity was considered by Satapathy and Bless [2000], Satapathy [2001]. All ﬁve zones are considered: cavity, comminuted zone, radially cracked zone, elastic zone and undisturbed zone (Fig. 8.3.2). For spherical symmetry the conservation equations for mass and momentum in Eulerian coordinates are: 1 ∂ ∂ρ + 2 (ρr2 v) = 0 , ∂t r ∂r σr − σθ ∂σr +2 = −ρ ∂r r The stresses are positive in compression.

∂v ∂v +v ∂t ∂r

.

(8.3.48)

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

Plastic Waves. Perforation

Fig. 8.3.2

dynamic

401

Dynamic response regions in a spherical cavity.

In the elastic region due to spherical symmetry the stresses are ∂u u E (1 − v) + 2v , σr = − (1 + v)(1 − 2v) ∂r r ∂u u E σθ = − v + . (1 + v)(1 − 2v) ∂r r

(8.3.49)

Since the particle velocity is negligible in the elastic region, it is ignored and the equation to be integrated is ∂ 2 u 2 ∂u 2u 1 ∂2u − + = , ∂r2 r ∂r r2 Ce2 ∂t2 where Ce is the dilatational elastic wave seed, and with ξ1 = r/Cc t and u¯1 = u/Cc t this equation becomes 2 ¯ u ¯ d2 u 2 d¯ 2¯ u 2 2d u + − = α ξ , 2 2 dξ1 ξ1 dξ1 ξ1 dξ12

(8.3.50)

with α = Cc /Ce . Forrestal and Luk [1988] have shown that this equation has the solution 1 − 3α2 ξ12 , u ¯ = Aαξ1 − B 3α2 ξ12 where A and B are constants of integration, with 3 α2 (1 − v) 2σf B = − A, A = . 2 ρ0 Cc2 2v(α3 − 1) + 2α3 − 3α2 + 1 In the cracked region only radial stresses are transmitted ∂σr 2σr ∂2u + = −ρ 2 . ∂r r ∂t

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

402

dynamic

Dynamic Plasticity

Since σr = −E

∂u , ∂r

and ξ2 =

r , Cpt

u ¯2 =

u , Cp t

this equation becomes ¯2 u2 d2 u ¯2 d2 u 2 d¯ + = β 2 ξ22 2 , 2 dξ2 ξ2 dξ2 dξ2

Cp β= , Ccr

Ccr =

E ρ

with the following solution u ¯2 = −c1

1 + β 2 ξ22 + c2 ξ2

and c1 =

Y − 1)

E(β 2

,

c2 =

(1 − v)(2α3 − 3α2 + 1) σf γ Y β2γ2 + 1 + . 2 2 γE β − 1 ρ0 Ce 2v(α3 − 1) + 2α3 − 3α2 + 1

For the passage to the next domain the conditions ρ1 (v1 − C) = ρ2 (v2 − C) ,

σ2 − σ1 = ρ1 (C − v1 )(v2 − v1 )

are used. Denoting the volumetric strain in the elastic side η=

α2 (α − 1)(1 − v) ρ0 6σf P =1− =− 2 3 , K ρ ρCe 2α (1 + v) − 3α2 + 1 − 2v

the following relation between α and β is obtained # 2 $ ρ0 Cc − V1 2 2 + σ1 β 2 γ 2 − γ 2 Y (1 − β γ ) 1 − 3K 1 − η1 γ2 =

=

α Ce β Ccr

2

Y (1 − β 2 γ 2 )[1 −

ρ0 Cc −V1 2 3K ( 1−η1 ) ]

+ σ1 β 2 γ 2 − η1 β 2 γ 2 ρ0 [(Ce − V1 )/(1 − η)]2

σ1 − η1 ρ0 [(Ce − V1 )/(1 − η1 )]2

.

The product βγ is function of α only. One assumes that the shear strength increases linearly with the conﬁning pressure σr + 2σθ σr − σθ = λ1 . 2 3 Using this equation in the equation of motion (8.3.48)2 we obtain ∂σr σr ∂v ∂v + 2α ¯ = −ρ +v , (8.3.51) ∂r r ∂t ∂r where α ¯ = 6λ1 /(3 + 4λ1 ). Using the similarity transformation v r u , u ¯3 = and U = , ξ3 = Vt Vt V in the comminuted region, (8.3.51) becomes

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

Plastic Waves. Perforation

dynamic

403

σr dσr dU + 2α ¯ = −ρV 2 (U − ξ3 ) . (8.3.52) dξ3 ξ3 dξ3 One is disregarding dilatancy and compaction and from the mass conservation D1 v= 2 , r where D1 is the constant of integration. This is in non-dimensional quantities 1 (8.3.53) U= 2. ξ3 Inserting it in the Eq. (8.3.52) and integrating, we get 2 D2 ρV 2 2 2α−4 ¯ 2α−1 ¯ ξ ξ + 2α¯ , + σr = − 2α¯ − ξ3 2α ¯−1 3 2α ¯−1 3 ξ3 where D2 is the integration constant. The density for this region is the same as that at the cracked-comminuted boundary ρ = ρ0 /(1 − Y /3K). Denoting the pressure at the cavity surface by Pc , the stress required to maintain the constant cavity expansion velocity is: " 2α−4 ¯ " 2δ 2α−1 3 δ ¯ − + . (8.3.54) Pc ≡ σr "" = Y δ 2α¯ + ρ0 V 2−α ¯ 1 − 2α ¯ (1 − 2α ¯ )(2 − α ¯) ξ3 =1

The quantity δ is related to α and β by 1 . 3[c2 − c1 (1 + β 2 )] The equation in the saturated region becomes dσr dU 4τ + = −ρV 2 (U − ξ3 ) . dξ3 ξ3 dξ3 Integrating this equation with (8.3.53) yields 1 2τ ρV 2 4 Pc = + 4τ ln δ1 + 3+ 4 − . α ¯ 2 δ1 δ1 The application is for the alumina ceramic Coors AD995, for which we have E = 373.14 GPa, K = 231.8 GPa, ρ = 3890 kg/m, and the quasi-static compressive strength Y = 2.62 GPa, and the tensile strength σf = 0.262 GPa. The tungsten projectile for impact velocities up to 3.5 km/s are shown in Fig. 8.3.3. A dynamic spherical cavity expansion in a pressure sensitive elastoplastic medium was considered also by Durban and Masri [2004]. The material behavior is described by the hypoelastic model of the Drucker–Prager material with a nonassociated ﬂow rule, with arbitrary strain-hardening. Simple analytical solutions are given for the fully incompressible elastic/perfectly plastic material with a nonassociated ﬂow rule. A numerical analysis is given for the fully incompressible strain-hardening solid with a non-associated ﬂow rule. In another paper by Gao et al. [2004] one considers the same problem and comparison with experiments, perforation of concrete. The following nine assumptions are given and argued. The medium of concrete can be considered as ideal ﬂuid for high-velocity impact, where the shear modulus is zero, which can satisfy δ3 =

January 12, 2007

10:41

404

Fig. 8.3.3 levels.

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Dynamic Plasticity

Cavity expansion pressure versus penetration velocity for diﬀerent shear-saturation

the needs of engineering analysis for the case of high-velocity and high-pressure. To be compared with the compressive strength, the tensile strength is very little. For high-velocity and high-pressure impacting, the tensile strength can be neglected. During the impact or penetration, the elastic ultimate stress of concrete can be neglected while the wave velocity of elastic stress is very high. There is an ultimate density for concrete during the impact pressing, to which the density of concrete medium can not be increased again for further compressing. A series of experiments had proved that the ultimate density had almost no changes for the higher pressure. During the compressing until ultimate density, the concrete medium subjects to ideal plastic deformation. There is no change of stress. In this process, the air voids are gradually compressed out of the concrete. The wave velocity of stress is zero. The region of medium response will expand in the external normal direction of the projectile surface. In the compressed region, the density and volume of the concrete material have not any more changes. Therefore, the stress wave is constant-volume wave. The thermal conduction can be neglected during impacting. The projectile is non-deformable. The dynamic penetration of the projectile is studied by writing the mass conservation, the momentum conservation and the energy conservation. One is studying the penetration equation and the scabbing produced. The criteria for scabbing is σ ∗ − σ ≥ σs where σ ∗ is the front peak value of the attenuation stress wave, σ is the compressing stress where crack is caused and σs is the tensile stress of concrete. For a parabola nose projectile and concrete with density of ρ = 2400 kg/m3 , with ultimate (the highest) density of ρ∗ = 2640 kg/m3 , the compressive strength

dynamic

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Plastic Waves. Perforation

Fig. 8.3.4

dynamic

405

The measurement and calculation deceleration curves of a projectile in the second test.

σc = 3.0 × 107 N/m2 , mass of the projectile mp = 7.63 kg, the moment of inertia Jp = 0.162 kg/m2 , the friction coeﬃcient µf = 0.1 and the thickness of one target plate is 0.3 m. The plates were 1 m apart and the striking velocity of the projectile is 532 m/s in the ﬁrst series of test and 580 m/s in the second. One has measured the deceleration curve and also the scabbing. The case of three cement plates is shown in Fig. 8.3.4. A new constitutive model for cold compaction of metal powders is developed by Gu et al. [2001]. The plastic ﬂow of metal powders at the macroscopic level is assumed to be representable as a combination of a distortion mechanism, and a consolidation mechanism. For the distortion mechanism the model employs a pressure-sensitive, Mohr–Coulomb type yield condition, and a new physically based non-associated ﬂow rule. For the consolidation mechanism the model employs a smooth yield function which has a quarter-elliptical shape in the mean-normal pressure and the equivalent shear stress plane, together with an associated ﬂow rule. The constitutive model has been implemented in a ﬁnite element program. The material parameters in the constitutive model have been calibrated for MH-100 iron powder by ﬁtting the model to reproduce data from true triaxial compression experiments, torsion ring-shear experiments, and simple compression experiments. The predictive capability of the constitutive model and computational procedure is checked by simulating two simple powder forming processes: (i) a uniaxial strain compression of a cylindrical sample, and (ii) forming of a conical shaped-charge liner. In both cases the predicted load-displacement curves and density variations in the compacted specimens are shown to compare well with corresponding experimental measurements.

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

406

Dynamic Plasticity

The transverse cracks in glass/epoxy cross-ply laminates impacted by projectiles was considered by Takeda et al. [1981]. They started from the glass/epoxy cross-ply laminates impacted by cylindrical projectiles with diﬀerent impactor nose shapes and lengths, a sequential delamination mechanism is dominant, initiated by a generator strip, of with approximately equal to the impactor diameter, cut from the ﬁrst lamina by two through-the-thickness cracks parallel to the ﬁbers of the ﬁrst lamina Cristescu et al. [1975]. They have continued the tests and the impactor velocity for the development of the transverse cracks appears to be independent of the impactor type and to be about 23 m sec−1 . Above this threshold velocity, the mean transverse crack distance decreases sharply as the impactor velocity increases. The curves are eventually ﬂattened out at higher velocities. Another paper about damage of composites is due to Nemes and Sp´eciel [1995]. The problem is mathematically well-posed wave propagation problem, with an unique and stable solution. A big new paper, devoted to a new membrane model for ballistic impact response and V50 performance of multi-play ﬁbrous systems was written by Phoenix and Porwal [2003]. They started with Rakhmatulin and Dem’yanov [1961] equations * u +⊕ 1 ∂2u 1 ∂ (ε = r cos γ) − (8.3.55) t a0 ∂t2 r ∂r r2 and 1 ∂2v 1 ∂ (εt r sin γ) =− (8.3.56) 2 a0 ∂t r ∂r where a0 is reduced to a0 = E/ρ, the symbol [ ]⊕ means the quantity is kept only if positive, and 2 2 ∂u ∂v 1+ + −1 εt = ∂r ∂r is the strain. These equations are discussed and integrated. Ultimately one expresses the threshold projectile velocity V50 above which the membrane fails by perforation 50% of the time, in terms of Cunniﬀ’s dimensionless scaling parameters √ 3 2 3/4 V50 / Ω = 21/3 ε1/12 y max (1 + θ Γ0 )/Kmax where Kmax is accurately represented by 4θ2 Γ0 2 (ψ − 1) Kmax ≈ exp − 3(1 + θ2 Γ0 ) max

1/3 × ψmax

ψmax /εy max (ψmax − 1) ln[1 + ψmax /εy max (ψmax − 1)]

and ψmax ≈

(1 + θ2 Γ0 )/(2θ2 Γ0 )

&2/3

dynamic

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Plastic Waves. Perforation

with

dynamic

407

√ 3 Ω a normalizing velocity and Ω is expressed in yarn (ﬁber) properties as % Ω = (1/2)(σy max εy max /ρy ) Ey /ρy .

The comparison with Kevlar 29, Kevlar KM2, PBO and Spectra 1000 are good. For Kevlar 29, we have σy max ≈ 2.9 GPa, εy max ≈√ 0.034, Ey ≈ 74 GPa, ρy = 3 1440 kg/m3 and producing the normalizing velocity Ω ≈ 624 m/s.. Warren et al. [2004], document the results of a combined experimental, analytical, and computational research program that investigates the penetration of steel projectiles into limestone targets at oblique angles. The striking velocities were 0.4 to 1.3 km/s. In several papers, one have studied the eﬀect of preliminary strain hardening on the ﬂow stress of titanium and a titanium alloy during shock compression by Razoreniv et al. [2005]. The eﬀect of preliminary strain hardening of titanium and a titanium alloy on their mechanical properties under quasi-static and highrate (> 105 s−1 ) loading is studied. Preliminary hardening is accomplished using equal-channel angular pressing and shock waves. High-rate deformation is attained via shock-wave loading of samples. The experimental results show that structural defects weaken the dependence of the yield strength on the strain rate. The diﬀerence in the rate dependence can be so high that the eﬀect of these defects on the ﬂow stress can change sign when going from quasi-static to high-rate loading. The ﬂyer plates were launched at velocities of 0.1–1.23 km/s.

8.4

Modeling of the Taylor Cylinder Impact Test. Anisotropy

The anisotropy of the impact bar was also considered, starting from a simpliﬁed description of the Taylor impacting bar. One has considered the simpliﬁed theory by Hawkyard et al. [1968], Hawkyard [1969], Hutchings [1979] and Jones et al. [1987]. The projectile is deformed by the impact and, from geometrical measurements made before and after impact, the yield stress of the specimen is deduced. Copper and mild steel were ﬁrst considered at various temperatures. The proﬁles predicted of the specimen, after the tests, were afterwards approximated in various ways. A comparison with the measured shape of the specimen after the test is afterwards done. Polymers were also considered with projectiles measured before and after impact. New equation was developed. But again with a schematic illustration of the projectile. In another paper Jones et al. [1991] a simple theoretical analysis of the old problem is presented. The analysis is more complete, but retains the mathematical simplicity of the earlier versions. The major thrust is to separate the material response into two phases. The ﬁrst phase is dominated by strain rate eﬀects and has a variable plastic wave speed. The second phase is dominated by strain hardening eﬀects and has a constant plastic wave speed. Estimates for dynamic yield stress, strain, strain-rate, and plastic wave speed during both phases

January 12, 2007

408

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Dynamic Plasticity

are given. In the paper an example of a cooper specimen impacting a steel anvil with an initial speed of 187 m/s, is given. Experimental techniques are described and illustrated by Nemat-Nasser et al. [1994] for direct measurement of temperature, strain-rate, and strain eﬀects on the ﬂow stress of metals over a broad range of strains and strain rates. Taylor anvil tests are performed, accompanied by high-speed photographic recording of the deformation, and the results are compared with those obtained by ﬁnite-element simulations, leading to ﬁne tuning of parameters in the material’s ﬂow stress. Constitutive models and solution algorithms for anisotropic elastoplastic material strength are developed by Maudlin and Schiferl [1996] for use in the high-rate explicit multi-dimensional continuum mechanics codes. The constitutive modeling is posed in an unrotated material frame using the polar decomposition theorem. Continuous quadratic and discontinuous piecewise yield functions obtained from polycrystal simulations for metallic hexagonal-close-paked and cubic crystal structures are utilized. Associative ﬂow formulations incorporating these yield functions are solved using various solution algorithms; explicit, semi-explicit and geometric normal return schemes are assessed for stability, accuracy and eﬃciency. Isotropic scaling (hardening) of the anisotropic yield surface shapes is included in the modeling. An explosive forming application involving large strain was selected to investigate the eﬀect of using anisotropic materials. Axisymmetric two-dimensional forming simulations were performed for both crystal structures producing resultant formed shapes that are unique to the material’s initial yield anisotropy, and are distinct from isotropic results. Initial axisymetric geometry of a simple explosive forming problem for titanium simulated with the EPIC code, is given. In another paper a new one-dimensional simpliﬁed analysis of the Taylor impact test is presented by Jones et al. [1996]. This analysis diﬀers from any previously presented in that the wave mechanics are separated from the calculation of dynamic stress. The new results utilize post test measurements to estimate key parameters in the plastic wave propagation. However, these measurements are incorporated into the analysis in a very unconventional way. A comparison with continuum code calculations shows very good agreement has been achieved. Simple conservation relationships (jump conditions) in conjunction with postulated material constitutive behavior are applied by Maudlin et al. [1997] to steady plastic strain waves propagating in problems of uniaxial stress and Taylor Cylinder Impact. These problems are simulated with a two-dimensional Lagrangian continuum mechanics code for the purpose of numerically validating the jump relationships as an accurate analytical representation of plastic wave propagation. The constitutive behavior used in this eﬀort assumes isotropy and models the thermodynamic response with a Mie-Grunisen Equation-of-State and the mechanical response with the rate-dependent Johnson-Cook and MTS ﬂow stress models. The jump relationships successfully replicate the results produced by continuum code simulations of plastic wave propagation and provide a methodology for constructing mechanical constitutive models from experimental plastic wave speed information.

dynamic

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Plastic Waves. Perforation

dynamic

409

Comparison are also presented between experimental speeds from Taylor Cylinder Impact tests with jump relationships and continuum code predictions, indicating that the above mentioned ﬂow stress models may not accurately capture plastic wave propagation speeds in annealed and hardened copper. Taylor cylinder impact testing is used by Maudlin et al. [1999] to validate anisotropic elastoplastic constitutive modeling by comparing polycrystal-computed yield-surface shapes (topography) with measured shapes from post-test Taylor specimens and quasi-static compression specimens. Measured yield-surface shapes are extracted from the experimental post-test geometries using classical r-value deﬁnitions modiﬁed for arbitrary stress state and specimen orientation. Rolled tantalum (body-centered-cubic metal) plate and clock-rolled zirconium (hexagonalclose-packed metal) plate are both investigated. The results indicate that an assumption of topography invariance with respect to strain rate is well justiﬁed for tantalum. However, a strong sensitivity of topography with respect to strain rate for zirconium was observed, implying that some accounting for a deformation mechanism rate dependence associated with lower-symmetry materials should be included in the constitutive modeling. Discussion of the importance of this rate dependence and texture evolution in formulating constitutive models appropriate for ﬁnite-element model applications is provided. In another paper by Maudlin et al. [1999] Taylor impact tests using specimens cut from a rolled plate of tantalum were conducted. The tantalum was experimentally characterized in terms of ﬂow stress and crystallographic texture. A piece-wise yield surface was interrogated from an orientation distribution function corresponding to this texture assuming two slip system modes, in conjunction with an elastic stiﬀness tensor computed from the same orientation distribution function and single crystal elastic properties. This constitutive information was used in a code of a Taylor impact test. A forged and round-rolled pure tantalum bar stock was observed by Maudlin et al. [2003] to exhibit large asymmetry in bulk plastic ﬂow response when subjected to large strain Taylor cylinder impact testing. This low-symmetry behavior was analyzed experimentally investigating both the initial stock and the impactdeformed material via x-ray crystallographic texture measurements and automated electron back-scatter diﬀraction scans to establish spatial micro structural uniformity. Polycrystal simulations based upon the 110 measured duplex texture and experimentally inferred deformation mechanisms were performed to project discrete yield surface shapes. Subsequent least squares ﬁtting and eigensystem analysis of the resulting quadratic forth-order tensors revealed strong normal/shear coupling in the yield surface shape. This mixed-mode coupling produces a shearing deformation in the 1–2 impact plane of a Taylor specimen whose axis is coincident with the compressive 3-axis. The resultant deformation generates an unusual rectangular-shaped impact footprint that is conﬁrmed by ﬁnite-element calculations compared to experimental post-test geometries.

January 12, 2007

410

8.5

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Dynamic Plasticity

Analysis of the Steady-State Flow of a Compressible Viscoplastic Medium Over a Wedge (Cazacu et al. [2006])

Penetration mechanics has a long and rich history. Information concerning the stress-time response in the target during penetration is lacking. A comprehensive review of empirical equations for maximum penetration depth in rock, concrete, soil, ice, and marine sediments can be found in Batra [1987], Heuze [1990], Zukas et al. [1990], etc. The maximum penetration depth is expressed as a function of initial impact velocity, penetrator cross-sectional area, penetrator weight, and/or nose geometry. However, in these equations the only target material properties considered are the initial density and unconﬁned strength. A large number of semi-analytical models where penetration is idealized as uniform expansion of a spherical or cylindrical cavity into a semi-inﬁnite target have been proposed. These cavity expansion analyses provide the radial stress at the cavity surface as a function of the cavity velocity and acceleration. This radial stress is considered to be the load on the penetrator and subsequently used in conjunction with equations of motion to calculate the maximum depth of penetration. As emphasized in recent contributions, good agreement between model and data could be expected only if the compressibility and rate sensitivity of the target material are accounted for. In the present section (Cazacu et al. [2006]) I present a new model for calculating the resistance to penetration into geological or geologically derived materials. In the analyses it is assumed that the rate of penetration and all ﬂow ﬁelds are steady as seen from the tip of the penetrator. This hypothesis is supported by penetration tests into cementitious materials (grout, concrete) for impact velocities below 1000 m/s. The shear response of the target material is modeled by a modiﬁed Bingham type viscoplastic equation proposed by Cazacu and Cristescu [2000], Cristescu et al. [2002]. The rationale for adopting such a model is that it accounts for both strain rate and compaction eﬀects on yielding, which are key properties of any porous/brittle material. In the law-pressure regime, a non-linear pressurevolume relationship is considered. Based on experimental observations which show that in the high-pressure regime a very large increase in pressure is necessary to produce even a very small change in density, the hypothesis of a “locking medium” is adopted: the density cannot exceed a critical value. The penetrator is wedgeshaped with high length-over-diameter ratio. Contact between the projectile nose and target is considered to be of Coulomb type with constant friction coeﬃcient, whereas the frictional contact between the remainder of the projectile and target is considered to be slip-rate dependent. Resistance to penetration is calculated for diﬀerent interface conditions between the target and wedge. It is shown that for low to intermediate impact velocities, accounting for friction alters the optimal wedge geometry for penetration performance by blunting the nose. Furthermore, the higher the velocity, the greater the inﬂuence of the nose geometry (wedge semi-angle) on penetration.

dynamic

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Plastic Waves. Perforation

dynamic

411

The deviatoric response of the target material is modeled by a non-homogeneous Bingham type rigid/viscoplastic equation: if IIS ≤ k 2 (ρ) , 0 D = (8.5.1) 1 k(ρ) 1− √ s if IIS > k 2 (ρ) , 2η IIs with the Macauley bracket. The inﬂuence of the degree of compaction on the behavior is modeled through the dependence of the yield limit in shear, k, on the current density ρ. Thus, for stress states satisfying IIS ≤ k 2 (ρ) the model response is rigid, otherwise the model response is viscoplastic. A power law variation of the yield limit with the current density is assumed n ρ0 , (8.5.2) k(ρ) = k0 + β 1 − ρ where ρ0 and k0 = k(ρ0 ) are the density and yield stress of the undeformed medium, respectively, while n and β are material constants. The yield stress k is given in stress units and η in Poise. The stress-volume relationship adopted reﬂects the following experimental observations (see Schmidt [2003]): • in the low to moderate pressure regime, most cementitious materials show a highly non-linear mean stress-volumetric strain response, the reversible decrease in volume being very small, • in the high-pressure regime, a very large increase in pressure is necessary in order to produce even a very small change in volume. Thus, the hypothesis of a “locking medium” applies, i.e., the density cannot exceed a critical value. This critical density, called locking density, is the density at which no volume change occurs under hydrostatic conditions. It will be denoted by ρ∗ and the pressure level at which this density is ﬁrst reached, called locking pressure, is denoted by p∗ . Hence, ρ = ρ0 for p > p∗ while for ρ ≤ ρ∗ , the pressure vs. density relationship p = p(ρ) is assumed to be of the form m ρ p(ρ) = p∗ (8.5.3) ρ∗ where m is a material constant. The relationships (8.5.1)–(8.5.3) could be inverted, to give: k(ρ) p(ρ)I + 2η + √ D for D = 0 , IID σ= (8.5.4) p(ρ)I for D = 0 . Note that the model accounts for both rate dependency and compaction eﬀects on yielding, which are key properties of any cementations or geologic materials. Generally post-test observations of penetration experiments in geologic or cementations materials (grout, concrete) indicate that there are four stages of the

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

412

dynamic

Dynamic Plasticity

Fig. 8.5.1

Schematic of the ﬂow over the wedge.

penetration event. The ﬁrst stage corresponds to nose penetration when the target material is restrained from large movements; the second stage corresponds to chipping and cratering at the point of impact; the third stage occurs when the projectile is fully embedded and the pusher plate hits the target and strips oﬀ while the forth stage occurs when the full length of the projectile is in the penetration channel or tunnel created by the penetrator. The analyses presented here concerns the steady-state ﬂow of the target material over a projectile fully embedded in the target (i.e., forth stage of penetration). The penetrator is considered to be rigid and wedge-shaped. Post-test observations indicate that for impact velocities up to 1000 m/s, penetration paths are relatively straight and stable with regard to the original shotline. Thus, we can assume that the problem is axi-symmetric with respect to the wedge centerline. Let us denote by D = D0 ∪ Dvisco ∪ Df the domain occupied by the penetrator and the target material around it (see Fig. 8.5.1). The lateral extent of this domain is F × R, where R is the wedge semi-height and F is a number estimated from post-test observations. In the domains D0 and Df (i.e., in front of and behind the penetrator), it is assumed that the target material is in rigid body motion while in the domain Dvisco the material undergoes viscoplastic deformation. We further suppose that in Dvisco the ﬂow lines are centered at a certain pole O. Hence, the viscoplastic domain Dvisco is bounded by the nose surface, Γ1 , MP, and the two surfaces S0 and Sf . The surface Sf is of radius OP ≡ rf = (R/sin α)F , while the surface S0 is of radius OM ≡ r0 (R/sin α)(1 + F ) (see Fig. 8.5.1). We assume that there exists velocity discontinuities tangent to the surfaces S0 and Sf , while the components of velocity normal to these surfaces are continuous. Since across S0 ] · n = 0 , [V (8.5.5) with n the outward normal unit vector, it follows that in the viscoplastic domain, Dvisco , the only non-zero velocity component is the radial component, Vr = V cos θ ,

0≤θ≤α

(8.5.6)

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

dynamic

Plastic Waves. Perforation

413

and consequently the only non-zero components of the rate of deformation are Dθθ =

V cos θ r

and Drθ = −

V sin θ 2r

(8.5.7)

The continuity equation reduces to: ∂ (rρ) = 0 . (8.5.8) ∂r Since ρ = ρ0 on S0 , in the viscoplastic domain, r0 (8.5.9) ρ = ρ0 . r Obviously, the compaction law (8.5.9) could also be obtained by imposing that the velocity be the same in the domains D0 and Df (debit compatibility). In the following, we estimate the resistance to penetration based on energy considerations. The wedge semi-angle that minimizes the resistance to penetration is then determined for diﬀerent interface conditions between the wedge and the target. Along the surface of the wedge signiﬁcant friction arises. The mechanics of friction at high sliding speeds is very complex. Much of the work reported is at lower speeds or pressures than those occurring during a penetration event. In view of this, in our analysis we assume that Coulomb friction law applies along Γ1 , the surface area of contact between the nose of the rigid projectile and the target, i.e. τ = µσn ,

(8.5.10)

where τ is the shear stress in the deformed material, µ is a friction coeﬃcient taken as constant, and σn is the normal pressure between the nose and the target material. In plastic forming of metals, when one body is fully plastic and the other is rigid, it is often assumed a friction law of the form (see Avitzur [1968]): √ (8.5.11) τ = µr σY / 3 , where τ is the shear stress in the deformed material, µr is a friction coeﬃcient taken constant and σY is the yield limit of the material. In general, 0 ≤ µr ≤ 1, the case µr = 0 corresponds to “no friction”, while µr = 1 corresponds to adherence of the plastic body to the rigid die wall. Hence, according to the friction law (8.5.11) irrespective of the normal pressure between the two bodies, the shear stress is constant. The density of the target material behind the penetrator is: ρ = ρf √ where ρf = ρ|r=rf while the state of stress is such that IIS = k(ρf ) (i.e., on the yield surface) (see Cristescu [1975]). Thus, it can be assumed that the contact between the rigid penetrator and the compacted material behind the penetrator is described by a law similar to (8.5.11), i.e. τ = µr k(ρf ) .

(8.5.12)

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

414

dynamic

Dynamic Plasticity

The theorem of power expanded is used to compute the resistance to penetration. In the domains D0 and Df no deformation occurs and therefore no internal power dissipation is involved. In the viscoplastic domain, the stress power per unit volume, σ : D can be expressed as (8.5.13) σ : D = σij Dij = 4ηIID + 2k(ρ) IID + p · tr D . Using the work-hardening law (8.5.2) in conjunction with the radial compaction law (8.5.8), we obtain n V 3 + cos2 θ V 2 3 + cos2 θ r + k0 + β 1 − σ:D=η 2 r 3 r0 r 3 m ρ0 r0 m V cos θ . (8.5.14) + p∗ ρ r r Integrating over Dvisco , we arrive at: r0 α ˙ σ : D dV = (σ : D) rdθdr , W = Dvisco

rf

0

or

2 ˙ = η V (7α + sin α cos α) ln r0 W 6 rf # n+1 $ rf r0 V 1− + √ F (α) k0 (r0 − rf ) + β n+1 r0 3 $ m # m−1 V sin α ρ0 r0 r0 −1 (8.5.15) + p∗ m − 1 ρ∗ rf !α√ where F (α) = 0 3 + cos2 θdθ. The surfaces S0 and Sf are surfaces of velocity ˙ !discontinuity. The ! power dissipated at the crossing of these surfaces is: WS0 ,Sf = t · [v ]dA + t · [v ] dA, where t is the stress vector while [v ] is the jump in S0 Sf velocity across the respective surface. Since the magnitude of the tangential jump is V sin θ, we obtain: α ˙ σrθ V sin θr0 dθ t · [v ] dA = WS0 = 0

S0

√ ηV (α − sin α cos α) − r0 k0 V 3F1 (α) , 2 α = −σrθ V sin θrf dθ t · [v ] dA = 2

=− ˙S W f

0

S0

n √ rf ηV (α − sin α · cos α) + k0 + β 1 − V 3F1 (α) 2 r0 2

= where

F1 (α) = 0

α

sin2 θ √ dθ . 3 + cos2 θ

(8.5.16)

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

Plastic Waves. Perforation

dynamic

415

Assuming Coulomb friction [see (8.5.10)] along Γ1 , the surface area of contact between the nose of the rigid projectile and the target, the dissipation due to friction is: rf ˙ (V cos α · σθθ |θ=α ) dr WΓ1 = µ r0

4 V cos α + η ln = µV cos α 3 #

r0 × k0 (r0 − rf ) + β n+1 p∗ + µV cos α m−1

ρ0 ρ∗

r0 rf

+

cos α 4 √ 3 3 + cos2 α

n+1 $ & rf 1− r0 #

r0

r0 rf

m−1

$ −1 .

(8.5.17)

Assuming that the friction law (8.5.11) applies along Γ2 , the surface area of contact between the penetrator and the compacted target material behind it (see Fig. 8.5.1), then ˙ k(ρf )V ds = µr k(ρf )V L , (8.5.18) WΓ2 = µr Γ2

where L is the length of the shank. Next, the resistance to penetration can be computed from energy balance. Consider the control volume V = D0 ∪ Dvisco ∪ Df i.e., in the domain comprised between the planes x = 0 and x = OS and y = 0 and y = F · R, (see Fig. 8.5.1). At steady state, the stress power theorem writes: ˙ S0 + W ˙S +W ˙ Γ1 + W ˙ Γ2 σ : D dV + W f Dvisco

(σb V − σf V ) dA .

=

(8.5.19)

∂V

In (8.5.19), σb denotes the magnitude of the stress vector acting along the direction of the velocity on the boundary of the domain D0 (i.e., in front of the penetrator) while σf is the magnitude of the stress vector acting on the boundary of Df . We may assume that σf = k(ρf ), where ρf is the density of the compacted target material behind the penetrator. Substituting (8.5.14) to (8.5.18) into (8.5.19), we obtain the expression of σb , the resistance to penetration, as: σb =

1 ˙ +W ˙ S0 + W ˙S +W ˙ Γ1 + W ˙ Γ2 + k(ρf )V F R) . (W f V (F + 1)R

(8.5.20)

To illustrate the predictive capabilities of the model, we will apply it to concrete for impact velocities of 300 m/s to 1000 m/s. In an attempt to study the inﬂuence of the frictional contact at the penetrator/target interface on the resistence to penetration for various impact velocities, the friction coeﬃcient µ between the tip of the projectile and target was varied between 0.001 and 0.2. The coeﬃcient of friction

January 12, 2007

416

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Dynamic Plasticity

between the body of the wedge and the target was set to µr = 0.6. The target material parameters involved in Eqs. (8.5.1)–(8.5.3) were assigned numerical values for conctrete material of initial density ρ0 = 2 g/cm3 and unconﬁned compressive strength is of 42.2 MPa. This implies that the pressure range of interest varies from tents of Mega-Pascals (MPa) to the order of a Giga-Pascal (GPa) for a case involving a high-strength steel penetrator. Thus, to characterize the behaviour of the concrete material for pressures representative for the in situ material, quasi-static compression tests were conducted for conﬁning pressures in the range 0–450 MPa using a standard fully automated MTS testing machine at a strain rate of approximately 0.77 · 10−6 /s. To better characterize the time and history eﬀects on the behaviour of the material, in each quasi-static test the loading path considered of several loadingcreep-unloading-reloading cycles. As already mentioned, before passing from loading to unloading, the load was held constant for 10–20 minutes in order to separate viscous eﬀects from unloading. As an example, in Figs. 8.5.2(a) and (b) are shown the results of a tests under σ3 = 200 MPa conﬁnement. The variation of the axial strain rate, ε˙1 with time during the third creep cycle is presented in Fig. 8.5.3 showing that within the load was held constant until the time rate of change of the axial strain approached zero. Note that hysteresis eﬀects were very much reduced thus allowing a rather accurate determination of the elastic parameters from the slopes of the unloading curves. No Hugoniot shock test data were available for

Fig. 8.5.2 Cyclic quasi-static test results under σ3 = 200 MPa: (a) principal stress diﬀerence versus axial strain; (b) principal stress diﬀerence versus radial strain.

dynamic

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Plastic Waves. Perforation

Fig. 8.5.3 pressure.

dynamic

417

Axial strain rate versus time during this 3rd creep cycle under σ3 = 300 MPa conﬁning

this material. Thus, the licking pressure was considered to be p∗ = 0.5 GPa, a value which is based on post-test data on cementious materials. The corresponding locking density ρ∗ is estimated using the relationship 1 ρ∗ = ρ0 1 − εfV where εfV = 0.068 corresponds to the volumetric deformation at failure under conﬁnement 450 MPa. For sake of simplicity, we assume a quadratic dependence of pressure on density [i.e., we set m = 2 in (8.5.3)]. We take the yield limit of the undisturbed medium k(ρ0 ) to be equal to the unconﬁned yield limit, i.e., k(ρ0 ) = 10 MPa. One of the challenges associated with modeling penetration is that the only information that could be gathered during penetration concerns the projectile trajectory and deceleration. To date, there is no in-target instrumentation for measuring deformation during penetration, there is no data from which the yield limit k(ρf ) may be inferred. Thus, we will assume that k(ρf ) = F F · k(ρ0 ), F F being a parameter, which depends on the impact velocity. Setting n = 2 in the law of variation of k(ρ), we estimate the parameter β as k(ρ0 )(F F − 1) . β= (1 − ρ0 /ρf )2 The wedge dimensions are set at: R = 6.35 mm, L = 89 mm. As an example, in Fig. 8.5.4 is shown (σb /p∗ ), the resistance to penetration normalized by the locking pressure, versus the projectile semi-angle α for an impact

January 12, 2007

418

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Dynamic Plasticity

Fig. 8.5.4 Resistance to penetration σb normalized by the locking pressure p∗ as a function of projectile semi-angle α for diﬀerent values of the friction coeﬃcient between the target and the wedge tip; impact velocity V = 300 m/s.

velocity V = 300 m/s. Calculations were done for 4 diﬀerent values of the coeﬃcient of friction between the wedge tip and target material. The yield stress of the compacted target k(ρf ) was considered to be 2.5 k(ρ0 ). Note that irrespective of the contact conditions between the wedge and target, there exists a critical angle for which the resistance to penetration is minimal. All the others parameters being kept the same, the more friction that is present, the blunter the nose required to achieve minimum resistance to penetration (of course, assuming that no erosion takes place and that the nose does not fail). This trend was observed for all impact velocities. The plots of the optimal wedge-angle vs. impact velocity for diﬀerent values of the friction coeﬃcient between the tip and target are presented in Fig. 8.5.5. Since compaction ratios were not available, in the calculations it was assumed that for an impact velocity of 1000 m/s k(ρf )/k(ρ0 ) is double than at 300 m/s impact velocity. The results indicate that at higher impact velocities a sharper nose is required for optimum performance. However, for modest friction (µ = 0.01), the sharpening is minimal. Figure 8.5.6 shows the resistance to penetration corresponding to optimum wedge angle versus the coeﬃcient µ between the wedge tip and target for diﬀerent impact velocities. Irrespective of the contact conditions, an increase in resistance to penetration occurs with increased impact velocity. In an attempt to study the inﬂuence of the frictional contact at the penetrator/target interface on the resistance to penetration for various impact velocities,

dynamic

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Plastic Waves. Perforation

dynamic

419

Fig. 8.5.5 Optimum projectile semi-angle versus impact velocity for various contact conditions between the wedge tip and viscoplastic target.

Fig. 8.5.6 Normalized resistance to penetration corresponding to the optimum projectile semiangle versus the coeﬃcient of friction between the wedge tip and viscoplastic target for various impact velocities.

January 12, 2007

10:41

420

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Dynamic Plasticity

the friction coeﬃcient µ between the tip of the projectile and target was varied between 0.001 and 0.2. The coeﬃcient of friction between the body of the wedge and the target was set to µr = 0.6. It was found that irrespective of the contact conditions between the penetrator and target, there exists a critical angle for which the resistance to penetration is minimal. All the other parameters being kept the same, the more friction that is present, the blunter the nose required to achieve minimum resistance to penetration (of course, assuming that no erosion takes place and that the nose does not fail). This trend was observed for all impact velocities in the range considered 300–1000 m/s. The resistance to penetration at optimal nose angle was found to be greater for higher impact velocity. An theory of optimal nose geometry for a rigid penetrator is due to Jones et al. [1998]. A net force on the nose of a rigid projectile normally penetrating a compliant target is given. The frictional eﬀects are neglected. A comparison of experimental results with simulations over a wide range of stiking velocities (less than 1000 m/s) is giving accurate prediction (Waren and Tabbara [2000]). Bibliography Aliev H. M., 1963, Dokl. Akad. Nauk. SSSR 151, 80–83 (in Russian). Andriankin E. I. and Koryavov V. P., 1959, Shock wave in a plastic medium of variable density, Dokl. Akad. Nauk. SSSR 128, 257–260 (in Russian). Avitzur B., 1968, Metal Forming: Processes and Analysis, Mc Graw Hill, New York. Backman M. E. and Goldsmith W., 1978, The mechanics of penetration of projectile into targets, Int. J. Engng. Sci. 16, 1–99. Batra R. C., 1987, Steady-state penetratration of viscoplastic targets, Int. J. Engng. Sci. 24, 9, 1131–1141. B´eda G., 1997, Constitutive equations and nonlinear waves, Nonlinear Analysis, Theory, Methods & Applications 30, 1, 397–407. Burke J. J. and Weiss V. (eds.), 1971, Shock Waves and the Mechanical Properties of Solids, Syracuse University Press, 417 pp. Campbell J. D. 1972, Dynamic Plasticity of Metals, Springer-Verlag, Wien, 92 pp. Cazacu O. and Cristescu N. D., 2000, Constitutive model and analysis of creep ﬂow of natural slopes, Italian Geo. Journal 34, 3, 44–54. Cazacu O., Ionescu I. R. and Perrot T., 2004, Penetration of a rigid body into a viscoplastic compressible ﬂuid, ECCOMAS 2004, Jyv¨ askyl¨ a, 24–28 July, 2004. Cazacu O., Cristescu N. D. and Schmidt M. J., 2006, Analysis of steady-state ﬂow of a compressible viscoplastic medium over a wedge, Int. J. Num. Anal. Meth. Geomechanics 30, 489–499. Chadwick P., Cox A. D. and Hopkins H. G., 1964, Phil. Trans. Roy. Soc. London A 256, 235–300. Cheeseman B. A. and Bogetti T. A., 2003, Ballistic impact into fabric and compliant composite laminates, Comp. Structures 61, 161–173. Chen X. W. and Li Q. M., 2002, Deep penetration of a non-deformable projectile with diﬀerent geometrical characteristics, Int. J. Impact Engng. 27, 619–637.

dynamic

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Plastic Waves. Perforation

dynamic

421

Chernyshov A. D., 1966, On the character of strong jumps in certain complex media, PMM J. Appl. Math. Mech. 30, 6, 1226–1232 (in Russian). Cristescu N., 1967, Dynamic Plasticity, North-Holland, 614 pp. Cristescu N., 1975, Plastic ﬂow through conical converging dies, using a viscoplastic constitutive equation, Int. J. Mech. Sci. 17, 425–433. Cristescu N., 1980, On the optimum die angle in fast wire drawing, J. Mech. Working Tech. 3, 275–287. Cristescu N. D., 2000, A model of stability of slopes, in Slope Stability 2000. Proceedinds of Sessions of Geo-Denver 2000, Griﬃths D. V., Fenton G. A. and Martin T. R. (eds.), Geotechnical Special Publication 101, 86–98. Cristescu N., Malvern L. E. and Sierakowski R. L., 1975, Failure mechanisms in composite plates impacted by blunt-ended penetrators, foreign object impact damage to composites, American Society for Testing and Materials, ASTM, STP 568, 159–172. Cristescu N. D., Craciun E. M. and So´ os E., 2003, Mechanics of Elastic Composites, Chapman & Hall/CRC, 682 pp. Cristescu N. D., Cazacu O. and Cristescu C., 2002, A model for slow motion of natural slopes, Canadian Geotechnical Journal 39, 4, 924–937. Davids N. (ed)., 1960, International Symposium on Stress Wave Propagation in Materials, Interscience Pub., 337 pp. Davids N. (ed)., 1969, Stress Wave Propagation in Materials, Intern. Sympo., Pennsylvania, Inter. Sci., New York–London. Demiray H. and Eringen A. C., 1978, A nonlocal model for plug formation in plates, Int. J. Engng. Sci. 16, 287–297. Durban D. and Masri R., 2004, Dynamic spherical cavity expansion in a pressure sensitive elastoplastic medium, Int. J. Solids Struct. 41, 5697–5716. Ezra A. A., 1973, Principles and Practice of Explosive Metalworking, Industrial Newspapers Limited, 270 pp. Fomin V. M. and Kiselev S. P., 1997, Elastic-Plastic Waves in Porous Materials, in High-Pressure Shock Compression of Solids IV, Davison L., Horie Y. and Shahinpoor M. (eds.), Springer, 205–232. Forrestal M. J. and Luk V. K., 1988, Dynamic spherical cavity-expansion in a compressible elastic-plastic solid, J. Appl. Mech. 55, 2, 275–279. Forrestal M. J. and Tzou D. Y., 1997, A spherical cavity-expansion penetration model for concrete targets, Int. J. Solids Struct. 34, 31–32, 4127–4146. Gao S., Jin L. and Liu H., 2004, Dynamic response of a projectile perforating multi-plate concrete targets, Int. J. Solids Struct. 41, 4927–4938. Grigorian S. S., 1959, On the general equations of the dynamics of soils, Dokl. Acad. Nauk. SSSR 124, 285–288 (in Russian). Grigorian S. S., 1960a, On the ﬁnal deﬁnition on the motion of soils, Prikl. Mat. Mech. 24, 651–662 (in Russian). Grigorian S. S., 1960b, On the fundamental representation of the dynamics of soils, Prikl. Mat. Mech. 24, 6, 1057–1072 (in Russian). Grigorian S. S., 1967, Some problems of mathematical theory of deformation and failure of solid soils, Prikl. Mat. Mech. 31, 643–669 (in Russian). Gu C., Kim M. and Anand L., 2001, Constitutive equations for metal powders: application to powder forming processes, Int. J. Plasticity 17, 147–209. Hawkyard J. B., 1969, A theory for the mushrooming of ﬂat-ended projectiles impinging on a ﬂat rigid anvil, using energy considerations, Int. J. Mech. Sci. 11, 313–333.

January 12, 2007

422

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Dynamic Plasticity

Hawkyard J. B., Eaton D. and Johnson W., 1968, The mean dynamic yield strength of cooper and low carbon steel at elevated temperatures from measurements of the “mushrooming” of ﬂat-ended projectiles, Int. J. Mech. Sci. 10, 929–948. Heuze F. E., 1990, An overview of projectile penetration into geological-materials, with emphasis on rocks, Int. J. Rock Mech. Min. Sci. 27, 1–14. Hutchings I. M., 1979, Estimation of yield stress in polymers at high strain-rates using G. I. Taylor’s impact technique, J. Mech. Phys. Solids 26, 289–301. Hutton D. V. and Counts J., 1974, Wave propagation in an elastic circular membrane subjected to impulsive pressure loading, J. Appl. Mech. Trans. ASME 41, 1, 290–291. Ishlinskii A. Yu., 1954, Ukr. Mat. Zh. 6, 430–441 (in Russian). Ishlinskii A. Yu., Zvolinskii N. V. and Stepanenko I. A., 1954, Dokl. Akad. Nauk. SSSR 95, 729–731 (in Russian). Johnson G. R. and Holmquist T. J., 1988, Evaluation of cylinder-impact test data for constitutive model constants, J. Appl. Phys. 64, 8, 3901–3910. Jones S. E., Gillis P. P. and Foster J. C. Jr., 1987, On the equation of motion of the undeformed section of a Taylor impact specimen, J. Appl. Phys. 61, 2, 499–502. Jones S. E., Gillis P. P., Foster J. C. Jr and Wilson L. L., 1990, A one-dimensional, two-phase ﬂow model for Taylor impact specimens, Trans. ASME, J. Engn. Mat. Tech. 113, 228–235. Jones S. E., Maudlin P. J. and Foster J. C. Jr, 1996, An engineering analysis of plastic wave propagation in the Taylor test, Int. J. Impact Engng. 19, 2, 95–106. Jones S. E., Rule W. K., Jerome D. M. and Klug R. T., 1998, On the optimal nose geometry for a rigid penetrator, Comp. Mech. 22, 413–417. Karagiozova D., 2004, Dynamic buckling of elastic-plastic square tubes under axial impact — I: stress wave propagation phenomenon, Int. J. Impact Engng. 30, 143–166. Karagiozova D. and Jones N., 2000, Dynamic elastic-plastic bucling of circular cylindrical shell under axial impact, Int. J. Solids Struct. 37, 2005–2034. Karagiozova D. and Jones N., 2001, Inﬂuence of stress waves on the dynamic progressive and dynamic plastic buckling of cylindrical shell, Int. J. Solids Struct. 38, 6723–6749. Karagiozova D. and Jones N., 2002, On dynamic buckling phenomena in axially loaded elastc-plastic cylindrical shells, Int. J. Non-Lin. Mech. 37, 1223–1238. Koiter W. T., 1953, Stress–strain relations, uniqueness and variational theorems for elastic-plastic materials with a singular yield surface, Quart. Appl. Math. 11, 350–354. Kolsky H. and Prager W., 1964, Stress Waves in Anelastic Solids, Springer-Verlag, 342 pp. Kompaneets A. S., 1956, Dokl. Akad. Nauk. SSSR 109, 49–52 (in Russian). Lee L. H. H., 1975, Bifurcation and uniqueness in dynamics of elastic-plastic continua, Int. J. Engng. Sci. 13, 1, 69–76. Longcope D. B. and Forrestal M. J., 1983, Penetration of targets describet by a Mohr Coulomb failure criterion with a tension cutoﬀ, J. Appl. Mech. 50, 327–333. Lush P. A., 1991, Comparison between analytical and numerical calculations of liquid impact on elastic-plastic solid, J. Mech. Phys. Solids 39, 1, 145–155. Macek R. W. and Duﬀey T. A., 2000, Finite cavity expansion method for near-surface eﬀects and layering during earth penetration, Int. J. Impact Engng. 24, 239–258. Maudlin P. J. and Schiferl S. K., 1996, Computational anisotropic plasticity for high-rate forming applications, Comput. Methods Appli. Mech. Engrg. 131, 1–30. Maudlin P. J., Foster J. C. Jr. and Jones S. E., 1997, A continuum mechanics code analysis of steady plastic wave propagation in the Taylor test, Int. J. Impact Engng. 19, 3, 231–256.

dynamic

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Plastic Waves. Perforation

dynamic

423

Maudlin P. J., Gray III G. T., Cady C. M. and Kaschner G. C., 1999, High-rate material modelling and validation using the Taylor cylinder impact test, Phil. Trans. R. Soc. Lond. A 357, 1707–1729. Maudlin P. J., Bingert J. F., House J. W. and Chen S. R., 1999, On the modeling of the Taylor cylinder impact test for orthotropic textured materials: experiments and simulations, Int. J. Plasticity 15, 139–166. Maudlin P. J., Bingert J. F. and Gray III G. T., 2003, Low-symmetry plastic deformation in BCC tantalum: experimental observations, modeling and simulations, Int. J. Plasticity 19, 483–515. Medvedeva N. S. and and Shemiankin E. I., 1961, J. Appl. Mech. Tech. Phys. 6, 78–87. Nemat-Nasser S., Li Y.-F. and Isaacs J. B., 1994, Experimental/computational evaluation of ﬂow stress at high strain rates with application to adiabatic shear banding, Mech. of Mat. 17, 111–134. Nemes J. A. and Sp´eciel E., 1995, Use of a rate-dependent continuum damage model to describe strain-softening in laminated composites, Comp. Structures 58, 6, 1083–1092. Osinov V. A., 1998, Theoretical investigation of large-amplitude waves in granular soils, Soil Dynamics Earthquake Engn. 17, 13–28. Phoenix S. L. and Porwal P. K., 2003, A new membrane model for the ballistic impact response and V50 performance of multi-play ﬁbrous systems, Int. J. Solids Struct. 40, 6723–6765. Prager W., 1953, On the use of singular yield conditions and associated ﬂow rules, J. Appl. Mech. 20, 3, 317–320. Pytel A. and Davids N., 1963, A viscous model for plug formation in plates, J. Franklin Inst.-Engineering Appl. Math. 276, 5, 394–406. Razorenov S. V., Savinykh A. S., Zaretsky E. B., Kanel G. I. and Kolobov Yu. R., 2005, Eﬀect of preliminary strain hardening on the ﬂow stress of titanium and titanium alloy during shock compression, Physics of the Solid State 47, 4, 663–669. Rakhmatulin Kh. A. and Dem’yanov Yu. A., 1961, Strength under High Transient Loads (English translation, Israel Program for Scientiﬁc Translations, 1966). Rakhmatulin H. A. and Stepanova L. I., 1958, On the propagation of explosion shock waves in sols, in: The Problems of Destruction of Rocks by Explosion (Moscow) 149–159 (in Russian). Rakhmatulin H. A., Sagomonian A. Yu. and Alekseev N. A., 1964, The Problems of Dynamics of Soils (Izv. MGU, Moscow) (in Russian). Rinehart J. S., 1975, Stress Transients in Solids, HyperDynamics, 230 pp. Sagomonian A. Yu., 1961, One-dimensional motion of soils with spherical, cylindrical and plane waves, in: Dynamics of Soils, No. 44 (Moscow), 43–87 (in Russian). Salvadori M. G., Skalak R. and Weidlinger R., 1955, Trans. N.Y. Acad. Sci. Ser. II 21, 427–434. Satapathy S., 2001, Dynamic spherical cavity expansion in brittle ceramics, Int. J. Solids Struct. 38, 5833–5845. Satapathy S. S. and Bless J. S., 2000, Cavity expansion resistance of brittle materials obeying a two-curve pressure-shear behavior, J. Appl. Phys. 88, 7, 4004–4012. Schmidt M. J., 2003, High Pressure and High Strain Rate Behaviour of Cementitious Materials: Experiments and Elastic/Viscoplastic Modeling, PhD dissertation, University of Florida. Schmidt M. J., Cazacu O., Ross C. A. and Cristescu N. D., 2001, Dynamic behaviour of mortar: experimental data and modeling, Proceedings of the 10th International Conference on Computer Methods and Advances in Geomechanics, Tucson, Arizona.

January 12, 2007

424

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Dynamic Plasticity

Shemiankin E. I., 1961, J. Prikl. Mech. Tech. Fiz. 5, 91–99 (in Russian). Shewmon P. G. and Zackay V. F., 1961, Response of Metals to High Velocity Deformation, Intersience Publishers, 491 pp. Srinivasan M. G. and Ting T. C. T., 1974, Initiation of spherical elastic-plastic boundaries due to loading at a spherical cavity, J. Mech. Phys. Solids 22, 415–435. Takeda N., Sierakowski R. L. and Malvern L. E., 1981, Transverse cracks in glass/epoxy laminates impacted by projectiles, J. Material Sci. 16, 7, 2008–20011. Warren T. L. and Tabbara M. R., 2000, Simulations of the penetration of 6061-T6511 aluminum targets by spherical-nosed VAR 4340 steel projectiles, Int. J. Solids Struct. 37, 4419–4435. Warren T. L., Hanchak S. J. and Poormon K. L., 2004. Penetration of limestone targets by ogive-nosed VAR 4340 steel projectiles at oblique angles: experiments and simulations, Int. J. Imp. Engineering 30, 1307–1331. Zhu G., Goldsmith W. and Dharan C. K. H., 1992, Penetration of laminated Kevlar by projectiles — I. Experimental investigation. Int. J. Solids Struct. 29, 4, 399–420. Zukas J. A., Nichols T., Greszczuk L. B. and Curran D. R., 1990, Impact Dynamics, Wiley, New York, 155–214. Zukas J. A., 2004, Introduction to Hydrocodes, Elsevier.

dynamic

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

Chapter 9

Hypervelocity Impact (Information)

9.1

Introduction

Several papers were published in the last years about hypervelocity impact. It seems that the beginning is a big paper by Al’tshuler [1965]; it is a review paper containing everything which was done up to this year (shock adiabats and their experimental registration, methods of obtaining semiempirical equation of state, shock adiabats, speed of sound and isentropic elasticity of shock-compressed bodies, on the composition of the earth’s core and the mantle, dynamic strength of materials, etc.). A paper by Alekseevskii [1966] is devoted to penetration of a rod with high velocity; the main ideas and schemes are given an example is computed for the velocity of 1470 m/s. Then is the paper by Tate [1967]. A modiﬁed hydrodynamic theory which takes some account of strength eﬀects is used to predict the deceleration of a long rod after striking a target. The results are then compared with experimental data from X-ray observation. The Bernoulli equation is used. The theory of long rod penetration as given in a previous paper is extended by Tate [1969] to take into account of the deformation of a soft rod against a rigid target and the penetration of a rigid projectile into a soft target. It is shown that it is theoretically possible to have a decrease in depth of penetration with increasing impact velocity, and a method for deducing the average radius of the hole is given. The Bernoulli equation is again given for materials which behave as a ﬂuid. A semi-inﬁnite solenoid in a uniform velocity ﬂow ﬁeld is used by Tate [1986], as a model for the quasisteady primary phase of long rod penetration. Assumptions: the materials to be incompressible, to obey a Mises yield criterion, when yielding the materials are perfectly plastic, the Levy–Mises ﬂow law applies, the materials are eitherelastic or plastic, a modiﬁed Bernoulli equation is established. In another paper Tate [1990] is proposing a segmented rod to explain penetration; the projectile is ﬁred up to 1800 m/s. Allen and Rogers [1961] study the penetration of metal rods into semi-inﬁnite metal targets. They have investigated experimentally at velocities up to 0.3 cm/µs. Results are compared with predictions from the hydrodynamic theory of jet penetration. Experimental results indicate that the eﬀective yield strength is relatively 425

dynamic

January 12, 2007

426

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Dynamic Plasticity

independent of the strength of the rod. The hydrodynamic theory of penetration was determined to be generally acceptable except where the density of the jet is much greater than that of the target. The impact ﬂash jet initiation phenomenology was considered by several authors. Shaped charge theory predicts that a jet will form when the impact angle between two colliding surfaces is greater than an initiation angle criterion which is a function of material properties and impact velocity. Because the eﬀective impact angle continuously sweeps over a range of values as a spherical particle impacts a ﬂat target, this jet initiation angle criterion is satisﬁed at some point during the penetration process. A simple model has been developed by Ang [1990] which predicts the jet initiation from either the target or the particle material. The hypervelocity impact of a projectile upon a thin metal plate and subsequent formation of back-surface debris is reviewed by Anderson et al. [1990]. At suﬃciently high impact velocities, roughly greater than 3.0 km/s, shock formation and interaction dominate and control the overall response of both the projectile and the target plate. The authors focus upon the importance of shock heating, melting, and vaporization in the application. They also assess the current status of computational modeling of this kind of impact event, speciﬁcally addressing recent work bearing on the sensitivity of such modeling to the equations of state and certain numerical issues. More accurate data in multi-dimensional experiments may be able to resolve the question of what are the major causes of diﬀerences between calculations and experiments. The theory is summarized and the origins of the target resistance term are examined by Anderson and Walker [1991]. Numerical simulations were performed of a tungsten-alloy, long-rod projectile into a semi-inﬁnite hardened steel target at three impact velocities suﬃciently high to result in projectile erosion (impact velocity apt to 1.5 km/s). The constitutive responses of the target and projectile were varied parametrically to assess the eﬀects of strain hardening, strain-rate hardening, and thermal softening on penetration response. The results of one of the numerical simulations were selected to compare and contrast in detail with the predictions of the Tate model. A computational study was performed by Anderson et al. [1993a] to quantify the eﬀects of strain rate on replica-model experiments of penetration and perforation. The impact of a tungsten-alloy, long-rod projectile into an armor steel target at 1.5 km/s was investigated. It was found that over a scale factor of 10, strain-rate eﬀects change the depth of penetration, for semi-inﬁnite targets, and the residual velocity and length of projectile, for ﬁnite-thickness targets, by an order of 5%. Although not modeled explicitly in the present study, the time-dependence of damage was examined. Damage accumulation is a strong function of absolute time, not scaled time. At homologous times, a smaller scale will have less accumulated damage than a larger scale; therefore, the smaller scale will appear stronger, particularly in situation where the detailes of damage evolution are important.

dynamic

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Hypervelocity Impact (Information)

dynamic

427

The penetration resistance of hard layers, such as ceramics and hardened steels, struck by high velocity long rod projectiles can be characterized by the depth of penetration tests (Bless and Anderson [1993]). The depth of penetration tests can be used to calculate average penetration resistance. The tests can also be used to compute diﬀerential eﬃciency. Implications for the eﬀectiveness of hypervelocity penetration (for 2–5 km/s) are that the optimum velocity for energy eﬃcient penetration will be much higher for hard materials than for conventional armor steel. Furthermore, ceramics will continue to substantially outperform armor steels, while high hardness steels will lose their relative advantages against long rod projectiles above 3 km/s. Numerical simulations are used by Anderson et al. [1993b] to examine long-rod penetration as a function of impact velocity. Similarities and diﬀerences between the penetration histories are analyzed, including penetration and tail velocities, penetration depths, crater radii, centerline interface pressures, and the extends of plastic ﬂow in the projectile and target. The Tate’s Bernoulli equation is used 1 1 ρp (v − u)2 + Yp = ρt u2 + Rt 2 2 where Yp is the ﬂow stress of the projectile, and Rt is deﬁned as the target resistance in the one-dimensional formulation, v is the projectile (tail) velocity, u is the penetration (interface) velocity. The one-dimensional modiﬁed Bernoulli theory is often used to examine long-rod penetration into semi-inﬁnite targets, and integral to the theory is a term that describes the resistance of the target to penetration. It is shown that the hydrodynamic theory gives smaller penetration velocities. The impact velocities are 1.5–4.5 km/s. One is also observing that the target resistance decreases with impact velocity, and it is shown that this is a consequence of both the residual phase of penetration and variations in the size of the plastic zone ﬁeld. Calculations of steel target penetration by L/D ≤ 1 tungsten and tungsten alloy projectiles have been extended to L/D = 1/32 over the velocity range 1.5 to 5 km/s by Orphal et al. [1993]. L is the projectile length and D the projectile diameter. The ratio of crater to projectile diameter tends to 1 as L/D decreases over this entire velocity range. For impact velocities of 1.5 and 3 km/s, penetration depth normalized by projectile length increases with decreasing projectile L/D up to a maximum value and then decreases for still lower L/D. Experiments at impact velocities of 2 and 3 km/s conﬁrm these results. For 5 km/s impact velocity, the calculations show P/L increasing (P depth of penetration) with decreasing projectile L/D over the entire range 1/32 ≤ L/D ≤ 1. Comparison with the experiments by Bjerke et al. [1992] is also done. Walker and Anderson [1995] found that in general the time histories of penetration predicted by the Tate model can be in good agreement with those computed from numerical simulations. However, discrepancies exist between the model and numerical simulations at the beginning and at the end of penetration. From insights provided by numerical simulations, assumptions are made concerning the velocity

January 12, 2007

428

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Dynamic Plasticity

and stress proﬁles in the projectile and the target. Using these assumptions, the time-dependent, cylindrically-symmetric, axial momentum equation is explicitly integrated along the centerline of the projectile and target to provide the equation of motion. The model requires the initial interface velocity — which can be found, for example, from the shock jump conditions — and material properties of the projectile and target to compute the time history of penetration. Agreement between the predictions of this one-dimensional, time-dependent penetration model is in good agreement with experimental results and numerical simulations. Analytic penetration modeling usually relies on either a momentum balance or an energy-rate balance to predict depth of penetration by a penetrator based on initial geometry and impact velocity. Based on the ﬂow ﬁeld and constitutive assumptions it is then possible to derive a momentum or an energy-rate balance. In another paper Walker et al. [1995] is presented the results of impact tests, as well as discusses the shaped charge design modiﬁcations for the nickel and molybdenum launchers. Radiographs are presented of impacting projectiles, as are post test photographs of various targets. The data are unique in that they represent low L/D projectile impacts into both monolithic blocks and spaced plates at velocities above 10 km/s. The aluminum projectiles are being launched at 11.25±0.20 km/s, the molybdenum projectiles at 11.72 ± 0.10 km/s, and the nickel projectiles at 10.81 ± 0.10 km/s. The impact data for aluminum agree well with trends seen at lower velocity light gas gun testing and scaled approaches. The paper by Walker [2001] examines the use of assumed ﬂow ﬁelds within a target created by impact and then examines the resulting predicted behavior based on either momentum conservation or energy conservation. It is shown that for the energy rate balance to work, the details of energy transfer mechanisms must be included in the model. In particular, how the projectile energy is initially transferred into target kinetic energy and elastic compression energy must be included. As impact velocity increases, more and more energy during the penetration event is temporarily deposited within the target as elastic compression and target kinetic energy. This energy will be dissipated by the target at a later time, but at the time of penetration it is this transfer of energy that deﬁnes the forces acting on the projectile. Thus, for an energy rate balance approach to successfully model penetration, it must include the transfer of energy into kinetic energy within the target and the storage of energy by elastic compression. Understanding the role of energy dissipation in the target clariﬁes the various terms in analytic models and identiﬁes their origin in terms of the fundamental physics. Understanding the modes of energy transfer also assists in understanding the hypervelocity result that penetration depth only slowly increases with increasing velocity even through the kinetic energy increases as the square of the velocity. At ordnance velocities (1.0–1.9), there is a pronounced decrease in penetration eﬃciency, as measured by P/L, when projectiles of larger L/D are used, as mentioned by Anderson et al. [1995b]. The inﬂuence of L/D on penetration is

dynamic

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Hypervelocity Impact (Information)

dynamic

429

refered to the L/D eﬀect. They numerically examine the L/D eﬀect at higher velocities, from 2.0 km/s to 4.5 km/s. It is found that as the velocities increases, there is a change in mechanism for the L/D eﬀect. At ordnance velocities the L/D eﬀect is mostly due to the decay in penetration velocity during the steady-state region of penetration. At higher velocities, the steady-state region of penetration shows no L/D dependence, and the L/D eﬀect is due primarily to the penetration of the residual rod at the end of the penetration event. This change in mechanism is related to the change in slope of the penetration-versus-impact velocity for eroding projectiles. Anderson et al. [1995a] study in a paper the penetration behavior of tungsten alloy, long-rod penetrators into high-hard steel, at two impact velocities 1.25 km/s and 1.70 km/s. The positions of the nose and tail of the projectile were measured by means of a 600 kV ﬂash X-ray system at diﬀerent times during penetration. The experiments were numerically simulated. The computational results are in very good agreement with the experimental position-time data. The computational results by Lawrence et al. [1995] are discussed and compared with new experimental observations obtained at an impact velocity of ∼ 10 km/s. In the experiment, the debris cloud was generated by the impact of a plate-shaped titanium projectile with a thin titanium shild. When 0.76 mm diameter tungsten rods impact AD995 Alumina at velocities up to 3.5 km/s, Subramanian and Bless [1995] show that penetration and consumption velocities are approximately linear functions of impact velocity. At 3.5 km/s, the penetration falls below the hydrodynamic limit by 15%. Neither the primary penetration nor the total penetration (i.e., ﬁnal depth of penetration) reached the limiting value of 2.23 suggested by hydrodynamic theory. The residual penetration, which is the diﬀerence between the total and primary penetration, was almost zero at 3 to 3.5 km/s. This suggests that the ceramic retains considerable strength ahead of the penetrator/target interface. Primary penetration approaches 75% of the hydrodynamic limit. A systematic study is decribed by Chhabildas et al. [1995], has led to the successful launch of thin ﬂier plates to velocities of 16 km/s. The energy required to launch a ﬂier plate to 16 km/s is approximately 10 to 15 times the energy required to melt and vaporize the plate. In the experiments by Brannon and Chhabildas [1995], a thin plate of zinc is impacted by a tantalum ﬂier plate at speeds ranging from 8 to 10.1 km/s, producing pressures from 3 Mbar to over 5,5 Mbar and temperatures as high as 39000 K. Such high pressures produce essentially full vaporization of the zinc. Trucano and Chhabildas [1995] used the Sandia Hypervelocity Launcher to get velocities in excess of 10 km/s. In the ﬁrst experiment the launch of an intact 0.33 gram titanium alloy chunk ﬂier to a velocity of 10.2 km/s. In a paper by Anderson et al. [1996a] one is considering the ballistic impact experiments which were performed on ceramic laminate targets at three scale sizes,

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

430

Dynamic Plasticity

normally 1/3, 1/6 and 1/12, to quantify the eﬀects of scale on various responses, in particular, the ballistic limit velocity. Some of the measured quantities showed little or no dependence on scale size, whereas other quantities, particularly the ballistic limit velocity, were found to vary with scale size. The impact velocities are up to 2.69 km/s. The ballistic limit velocity VBL is Vr =

0 ≤ Vs ≤ VBL

0, a(Vsp

−

p 1/p VBL )

,

Vs > VBL

where Vr , Vs and VBL are the residual, striking (impact), and limit velocities. In another paper by Orphal et al. [1996] a series of 26 terminal ballistics experiments was performed to measure the penetration of simple conﬁned aluminum nitride targets by a long tungsten rod. Impact velocities ranged from 1.5 to about 4.5 km/s. Penetrator diameter D was 0.762 mm. From the data u = dp/pt = speed of penetration into the target and vc = d(L − Lr )/dt = speed of “consumption” of the long rod were obtained. In a paper by Anderson et al. [1996], a common measure of penetration eﬃciency is given by the depth of penetration P into a semi-inﬁnite target normalized by the original length of the projectile L. It has been known for many years that P/L depends upon the aspect ratio L/D for projectiles with relatively small aspect ratios, e.g. 1 ≤ L/D ≤ 10. This inﬂuence of L/D on penetration is referred to as the L/D eﬀect. Although observed, the L/D eﬀect for large aspect ratio rods is not as well documented. Further, published penetration equations have not included the L/D eﬀect for high aspect ratio rods. The authors have compiled a large quantity of experimental data that permits the quantiﬁcation of the L/D eﬀect for projectiles with aspect ratios of 10 ≤ L/D ≤ 30. Numerical simulations reproduce the observed experimental behavior; thus, no new physics is required to explain the phenomenon. The numerical simulations allow investigation of the fundamental mechanics leading to a decrease in penetration eﬃciency with increasing aspect ratio. In a paper by Piekutowski et al. [1996] one is studying the perforation experiments of 26.3 mm thick aluminum plates and 12.9 mm diameter, 88.9 mm long, ogive-nose steel rods. For normal and oblique impacts with striking velocities between 280 and 860 m/s, one is measuring the residual velocities and displayed the perforation process with X-ray photographs. They have developed perforation equations that accurately predict the ballistic limit and residual velocities. Forty terminal ballistics experiments were performed by Orphal et al. [1997] to measure the penetration of simple conﬁned boron carbide targets by long tungsten roads. Impact velocities ranged from 1.5 to about 5.0 km/s. For tests with velocities 1.493 ≤ v ≤ 2.767 km/s, the penetrator diameter was 1.02 mm. For tests with impact velocities v ≥ 2.778 km/s the penetrator diameter was 0.762 mm. For tests in the velocity range 2.335 < v < 2.761 km/s both penetrator sizes were used. The penetration velocity u is found to depend linearly on the impact velocity u = 0.757v − 0.406.

dynamic

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Hypervelocity Impact (Information)

dynamic

431

The shock-wave compression of brittle solids was studied by Grady [1998]. Extensive experimental investigation in the form of large-amplitude, nonlinear wave-proﬁle measurements which manifest the shock strength and equation-of-state properties of brittle solids has been performed. The results of experiments performed to determine a complete set of independent elasic constants and the eﬀect of shock-induced shear strain on the delamination strength of a glass-ﬁber-reinforced plastic composite is due to Dandecar et al. [1998]. Two analytical models for the crater size generated by long-rod and thick-walled tube projectiles are presented by Lee and Bless [1998]. The ﬁrst is based on energy; in a steady-state penetration, the kinetic energy loss of a projectile is related to the total energy deposited in the target. This simple approach provides an upper bound for the crater size. The second approach is based on the observation that two mechanisms are involved in cavity growth due to long projectiles: ﬂow of projectile erosion products, which exerts radial stress on the target and opens a cavity, and radial momentum of the target as it ﬂows around the projectile nose. The speed of impact is less than 5 km/s. This analysis includes the centrifugal force exerted by the projectile, radial momentum of the target, and the strength of the target. Thus, it can estimate the extent of cavity growth due to projectile mushrooming, which cannot be predicted by other analyses. This model is shown to be in good agreement with experimental data. Yaw has been known to generally inﬂuence the penetration performance of long-rod projectiles. Experiments have shown that even small angles of yaw can signiﬁcantly degrade performance. The experiments by Bless et al. [1999] have shown that even small angles of yaw can signiﬁcantly degrade performance. The authors show that a critical feature of a yawed impact is the transverse load on the penetrator. Transverse loads tend to decrease the misalignment of rod axis and velocity vector. They use classical cavity expansion theory to quantify the impact transients and determine the magnitude of the transverse load. Then, a steady-state slot-cutting model is used to calculate the shape and orientation of a projectile that exits a ﬁnite plate. They found that this is contrary to the ﬁndings of some previous studies considered. The strength pf the projectile may be ignored compared to the inertial loads even at the relatively high impact velocities. The theory agrees well with reverse impact experimental data on ﬁnite plate. Two and three-dimensional numerical simulations have been conducted by Anderson et al. [1999b] to help better understand the penetration and perforation of chemical submunition targets by tungsten-alloy long-rod projectiles. In particular, the computational results are analyzed to assess modeling assumptions in the application of the modiﬁed Bernoulli model of Tate to this class of problems. For the study, the chemical submunitions were treated as long steel cylinders ﬁlled with water. Impacts near the submunitions ends were neglected. Many of the simulations conducted looked at rod penetration through two successive submunitions. For

January 12, 2007

432

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Dynamic Plasticity

purposes of the computational study, the cylinders were idealized as ﬂat plates. The study considered three impact obliquities (60◦ , 70◦ and 80◦ ) and two impact velocities (2.0 and 4.0 km/s). Penetration velocities, erosion rates, and the eﬀects of a ﬁnite projectile diameter were investigated as a function of obliquity and impact velocity. Experimental data by Anderson et al. [1999a] show that penetration velocities and instantaneous penetration eﬃciencies fall below that expected from hydrodynamic theory, even at impact velocities as high as 4.0 km/s. For steel rod impacting an aluminum target, the hydrodynamic penetration velocity is achieved only at impact velocity of about 4 km/s. Numerical simulations, using appropriate strength values, are in excellent agreement with the experimental data. Parametric studies demonstrate that both projectile and target strength have a measurable eﬀect even at such high impact velocities. The ballistic performance of 17 penetrator materials, representing 5 distinct steel alloys treated to various hardnesses along with one tungsten alloy, has been investigated by Anderson et al. [1999]. Residual length and velocities, as well as the ballistic limit velocities, were determined experimentally for each of the alloy types for length to diameter (L/D) ratio 10 projectiles against ﬁnite-thick armor steel targets. An equation for the residual velocity VR in terms of the impact velocity VP and ballistic limit is m 1/m VR VP =a −1 VBL VBL were VBL is the ballistic limit velocity, was used. The target thickness normalized by the projectile diameter (T/D) was 3.55. For some of the projectile types, a harder target, with the same thickness, was also used. It was found that the ballistic limit velocity decreases signiﬁcantly when the projectile hardness exceeds that of the target. Numerical simulations are used to investigate some of the observed trends. It is shown that the residual projectile length is sensitive to projectile hardness; the numerical simulations reproduce this experimental observation. The results of experiments showed that the residual velocity either increased or remained approximately constant as the projectile strength was increased. It is assumed that the plastic work per unit volume is approximately a constant, that is, there is a trade oﬀ between strength and ductility. An Eulerian wave code was used by Anderson et al. [1999d] to simulate the impact, penetration, and detonation of a 23-mm highexplosive projectile into a water-ﬁlled tank. The pressure-time response is compared with results from an experiment. Computed peak pressures and impulses compare well with the experimental values. Orphal and Anderson [1999] report a direct observation of the streamline reversal of eroded rod material proposed by Allen and Rogers [1991]. Allen and Rogers suggested that the turning of high-velocity long-rod penetrator material at the target interface could be viewed as a reversal of the direction of a streamline with

dynamic

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Hypervelocity Impact (Information)

dynamic

433

only a change of sign in the velocity. Allen and Rogers’ streamline reversal model has two important consequences. First the eroded debris has a speed of vd = 2u − v relative to the target, where v is the impact velocity and u is the speed of penetration of the rod relative to the target. Secondly, a consequence of this formula is that the length of the rod debris, is given by the diﬀerence in the initial length of the rod and the remaining length of the rod. Results of a time-resolved experiment for a tungsten penetrator into a polycarbonate target at 3.61 km/s and a corresponding numerical simulation are consistent with streamline reversal. Numerical simulations are then used in a parametric study to investigate the eﬀects of various density relations between penetrator and target materials. The dimensions of holes produced by the impact of aluminum spheres with various thicknesses and aluminum sheets are presented and analyzed by Piekutowski [1999]. The sphere diameters ranged from 3.18 mm to 19.05 mm and the bumper sheet thickness to projectile diameter ratio, ranged from 0.026 to 0.504 with the majority of the tests having this ratio of less than 0.234. Impact velocities ranged from 1.98 km/s to 7.23 km/s. As this ratio is increased the holes tended to be less circular. Piekutowski et al. [1999] performed a series of depth of penetration experiments using 7.11 mm diameter, 71.12 mm long ogive-nose steel projectiles and 254 mm diameter aluminum targets. The projectiles had a nominal mass of 0.021 kg and were launched with striking velocities between 0.5 and 3.0 km/s. Post test radiographs of the targets showed three diﬀerent regions of penetrator response as the striking velocity increased: (1) the projectiles remained rigid and visibly undeformed; (2) the projectiles deformed during penetration without nose erosion, deviated from the target centerline, and exited the side of the target of turned severely within the target; and (3) the projectiles eroded during penetration and lost mass. Similar experiments have been done with spherical nose steel projectiles by Forestal and Piekutowski [2000]. Goldsmith [1999] has published a very big review paper on the subject. Everything published until 1999 is mentioned: background and scope, oblique impact, yaw impact, impact with yaw and obliquity, moving targets, rotating penetrators, tumbling impact, impingement of jets or long rods with relative target motion, ricochet, and conclusions-status on non-standard projectile impact. He is also mentioning the rate of the impact velocities: subordnance v0 < 500 m/s, ordnance 500 < v0 < 1500 m/s, ultraordnace 1.5 < v0 < 3 km/s, and hypervelocity v0 > 3 km/s. The references are also quite big, starting with Euler and continuing to 367 references. See also Batra and Lin [1988]. Powder guns or a two-stage, light-gas launched the projectiles at normal impacts to striking velocities between 0.4 and 1.9 km/s, by Frew et al. [2000]. In addition, an analytical penetration equation that described the target resistance by its density and a strength parameter determined from depth of penetration versus striking velocity data, is also done.

January 12, 2007

10:41

434

9.2

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Dynamic Plasticity

Further Studies

The process of long-rod penetration into thick metallic targets is examined by Rosenberg and Dekel [2001] through a series of two-dimensional simulations. The aim of the research presented, is to uncover the inherent material similarities in this process. In particular, the search is for non-dimensional parameters which account for the depth of penetration, such as the density ratio, and the relative strengths of penetrator and target. The velocity of impact is less than 7 km/s. The simulation results are in accord with existing empirical data, shedding more light on the penetration process and emphasizing the diﬃculties in achieving an overall normalization procedure for this process. Target hole sizes and geometries were measured for a series of highly oblique hypervelocity impacts of steel spheres against thin laminated targets by Orphal and Anderson [2001]. The impact velocity was nominally 4.6 km/s for most of the experiments with a few tests conducted at 7.3 km/s. Impact obliquity ranged from 60◦ to 80◦ from the normal to the target plane. Projectiles were stainless steel spheres with masses of 222 g, 25 g, and 1 g. Targets were laminated MX-2600 silica phenolic bonded to a 2024-T3 substrate. Target thickness was varied to give thickness to projectile diameter 0.6 and 0.3 for each projectile. The normal penetration of a deformable projectile into an elastic-plastic target is considered by Roisman et al. [2001]. The force imposed on the projectile by the target is generally a complex function of the strength of the target material, the projectile velocity, its diameter and shape, as well as the instantaneous penetration depth. When this force exceeds a certain critical value the projectile begins to deform. At moderate to high values of the impact velocity, the projectile’s tip material ﬂows plastically with large deformations causing the formation of a mushroom-like conﬁguration. This process is accompanied by erosion of the projectile material. In the rear, elastic, part of the projectile the deformation remain small and the region can be approximated as a rigid body being decelerated by the projectile’s yield stress. The general model allows one to predict the penetration depth, the projectile’s eroded length and the crater diameter. It has been shown that in the limit of very high impact velocities the present model reduces to the well-known form of the hydrodynamic theory of shaped-charge jet. Also, a simpliﬁed asymptotic formula for the crater radius has been derived which includes the eﬀect of the target’s yield stress and compares well with experimental data for very high impact velocities. The paper by Lynch et al. [2001] presents scale size ﬁrings of two novel shape KE penetration into a steel/ceramic/steel target at four velocities between 1.8 and 2.9 km/s. The two novel shapes were a three piece segment rod and a telescopic rod/tube. Two unitary rod designs were also included in the assessment. All the penetrators had a similar mass of 60 grams. Test data against semi-inﬁnite rolled homogeneous armor was used to obtain the mass eﬀectiveness of the ceramic target

dynamic

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Hypervelocity Impact (Information)

dynamic

435

for each rod shape and velocity. The performance rankings of the penetrators against the ceramic target were found to be similar to those for semi-inﬁnite rolled homogeneous armor. Hydrocode analysis of the experiments gave some valuable insights into the penetration processes of the two novel penetrator designs. Predicted depth of penetration compared very well with experimental values, but enhancements to the physics of the ceramic model are needed in order to simulate cover plate eﬀects. Tests surpassing 11 km/s have been reported by Reinhart et al. [2001]. The temperature, and hence the density of the ﬂyer-plate is also well known prior to impact. In a paper by Hari Manoj Simha et al. [2002] is described the computational modeling of the penetration response of a high-putity ceramic, namely the AD99.5 alumina. This material is the most widely investigated ceramic, and extensive materials testing and ballistic data are available. The model development is based on constitutive relationships inferred from bar impact and plate impact data. A novel element removal scheme for ceramics is presented, and the code is then used to investigate the penetration response of AD-99.5 alumina in the depth of penetration and semi-inﬁnite conﬁgurations. The computations are found to be in excellent agreement with the experimental results. The impact velocities are smaller than 3.5 km/s. A pulse shaping techniques to obtain compressive stress–strain data for brittle materials with the split Hopkinson pressure bar apparatus is presented by Frew et al. [2002]. The conventional split Hopkinson pressure bar apparatus is modiﬁed by shaping the incident pulse such that the samples are in dynamic stress equilibrium and have nearly constant strain rate over most of the test duration. A thin disk of annealed or hard copper is placed on the impact surface of the incident bar in order to shape the incident pulse. Analytical models and data that show a wide variety of incident strain pulses are produced by varying the geometry of the copper disks and the length and striking velocity of the striker bar. A model that corrects for the added sabot mass and shows good agreement with experiments conducted with high-strength steel striker and incident bars is presented by Forrestal et al. [2002]. They point out that this added sabot mass eﬀect will be even more pronounced with titanium, aluminum or magnesium bars. In another paper Piekutowski [2003] study the impact tests using aluminum bumper sheets ranging from 0.076 mm to 4.80 mm thick and impact velocities ranging from 1.98 to 7.19 km/s used to determine the fragmentation initiation threshold for aluminum spheres impacting at hypervelocity. Tests using 0.53 mm and 12.70 mm diameter aluminum spheres indicated that the fragmentation initiation threshold velocity scaled with the bumper-thickness projectile diameter ratio. When a conventional split Hopkinson pressure bar is used to investigate the dynamic ﬂow behavior of ductile metals, Chen et al. [2003] observe that the results at small strain (ε

P LASTICITY

This page intentionally left blank

% : / " . * $

1 -"45*$*5: /%$SJTUFTDV 6OJWFSTJUZPG'MPSJEB 64"

World Scientiﬁc / & 8 + & 3 4 & : t - 0 / % 0 / t 4 * / ( " 1 0 3 & t # & * + * / ( t 4 ) " / ( ) " * t ) 0 / ( , 0 / ( t 5" * 1 & * t $ ) & / / " *

Published by World Scientific Publishing Co. Pte. Ltd. 5 Toh Tuck Link, Singapore 596224 USA office: 27 Warren Street, Suite 401-402, Hackensack, NJ 07601 UK office: 57 Shelton Street, Covent Garden, London WC2H 9HE

British Library Cataloguing-in-Publication Data A catalogue record for this book is available from the British Library.

DYNAMIC PLASTICITY Copyright © 2007 by World Scientific Publishing Co. Pte. Ltd. All rights reserved. This book, or parts thereof, may not be reproduced in any form or by any means, electronic or mechanical, including photocopying, recording or any information storage and retrieval system now known or to be invented, without written permission from the Publisher.

For photocopying of material in this volume, please pay a copying fee through the Copyright Clearance Center, Inc., 222 Rosewood Drive, Danvers, MA 01923, USA. In this case permission to photocopy is not required from the publisher.

ISBN-13 978-981-256-747-5 ISBN-10 981-256-747-X

Printed in Singapore.

YHwa - Dynamic Plasticity.pmd

1

12/26/2006, 11:42 AM

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

IN MEMORIAM I would like to mention, with all the sadness possible, the memory of my wife Cornelia, which disappeared meantime, and which helped me always so much.

v

dynamic

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

This page intentionally left blank

dynamic

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Preface

The present book is not simply a new addition of the book Dynamic Plasticity, initially published in 1967, a long time ago. Certainly this edition is not only a new version, containing the essential of the old book and what has been done meantime. Why again Dynamic Plasticity? Well because very many books published meantime on the subject are not mentioning the waves which are to be considered in Dynamic Plasticity. Also, generally, the plastic waves are slower than the elastic one. Thus, when considering a simple problem of propagation of waves in thin bars, for any loading at the end, the plastic waves are reached by the elastic ones, and will not propagate any more. Only a part of the bar is deforming plastically. Examples of this kind are very few. I thought that this new version is too restrictive for the today students which know little of static plasticity, diﬀerential equations, dynamic elastic–plastic properties, etc. Therefore, I thought to write a simpler book, containing the main concepts of dynamic plasticity, but also something else. Thus I thought that this new version would contain the elementary concepts of static plasticity, etc., which would be useful to give. Also it would be good to give other problems, not directly related to dynamic plasticity. Thus I started with some classical problems on static plasticity, but only the simplest things, so that the readers would afterwards understand also the dynamic problems. Also, since in dynamic problems the soils and rocks played a fundamental role, I thought to write a chapter on rocks and soils. Then were expressed several chapters about dynamic plasticity, as propagation of elastic–plastic waves in thin bars, the rate inﬂuence and the propagation of waves in ﬂexible strings. It is good to remember here that all problems related to dynamic problems, are to be considered using the mechanics of the wave propagation; without the wave propagation mechanics all results concerning constitutive equations, rate eﬀect, etc. are only informative. Such problems are mentioned however in the book. We have presented mainly the diﬀerent aspects on constitutive equations of materials, as resulting from dynamic problems. Rate eﬀects are considered in this way. They have been used by a variety of authors. The same with the mechanics of ﬂexible strings, presented afterwards. Not very many authors have considered till now the mechanics of deformable cables. vii

dynamic

January 12, 2007

viii

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Dynamic Plasticity

Therefore I thought to write a very simple book, which can be read by the students themselves, without any additional help. They can understand what “plasticity” is after all. Then several other problems have been presented. Not trying to remove the fundamentals, I have thought also to add some additional problems, which are in fact dynamic, though the inertia eﬀect is disregarded. They are the stationary problems, quite often met in many applications. It is question obviously, about problems involving Bingham bodies, as wire drawing, ﬂoating with working plug, extrusion, stability of natural inclined plane, etc. Further I have considered various problems of plastic waves, using various theories. Also the perforation problems, was presented, using various symmetry assumptions, or any other assumption made. The last chapter is on hypervelocity impact. To keep it simple, I have given only very few information about. Thus I wished to show what hypervelocity is and how is it considered now. Though the book is a very simple one, I wished to ask any author to disregard possible missing of some papers. All literature is certainly incomplete. One has done today much more than given here. It was impossible for me to mention “all” authors in this ﬁeld. N. D. Cristescu [email protected]ﬂ.edu

dynamic

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

dynamic

Contents

Preface

vii

Introduction 1 Diagnostic Tests . . . . . . . . . . . . . . . . . . . 2 Tests Performed at Long and Short Term Intervals 3 Long-Term Tests . . . . . . . . . . . . . . . . . . . 4 Temperature Inﬂuence . . . . . . . . . . . . . . . . 5 The Inﬂuence of the Hydrostatic Pressure . . . . . 6 Variation of Elastic Parameters with Plastic Strain

. . . . . . . . . . . . . . . . . . . . . . . . . (Metals)

. . . . . .

. . . . . .

. . . . . .

. . . . . .

1. Yield Conditions 1.1 1.2 1.3 1.4 1.5 1.6 1.7 1.8 1.9 1.10 1.11 1.12 1.13 1.14

15

Stresses . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Yield Conditions . . . . . . . . . . . . . . . . . . . . . . . . . . The Classical Constitutive Equation for Perfectly Plastic Materials . . . . . . . . . . . . . . . . . . . . . . . . . . Work-Hardening Materials . . . . . . . . . . . . . . . . . . . . . Isotropic Hardening . . . . . . . . . . . . . . . . . . . . . . . . The Universal Stress Strain Curve . . . . . . . . . . . . . . . . Constitutive Equation for Isotropic Work-Hardening Materials The Drucker’s Postulate . . . . . . . . . . . . . . . . . . . . . . Kinematical Work-Hardening . . . . . . . . . . . . . . . . . . . Further Developments . . . . . . . . . . . . . . . . . . . . . . . Experimental Tests . . . . . . . . . . . . . . . . . . . . . . . . . Viscoplasticity . . . . . . . . . . . . . . . . . . . . . . . . . . . Rate Type Constitutive Equations . . . . . . . . . . . . . . . . General Principles . . . . . . . . . . . . . . . . . . . . . . . . .

. . . .

15 19

. . . . . . . . . . . .

22 25 27 29 30 31 32 34 35 38 42 43

. . . . . . . . . . . .

2. Rocks and Soils 2.1 2.2

1 1 5 9 11 12 12

53

Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Experimental Foundation . . . . . . . . . . . . . . . . . . . . . . . ix

53 59

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

x

dynamic

Dynamic Plasticity

2.3 2.4 2.5 2.6

The Constitutive Equation Failure . . . . . . . . . . . . Examples . . . . . . . . . . Viscoelastic Model . . . . .

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

3. The Propagation of Longitudinal Stress Waves in Thin Bars 3.1 3.2 3.3 3.4 3.5 3.6 3.7

The Equation of Motion . . . . . . . . . . . . . . . . The Finite Constitutive Equation . . . . . . . . . . . The Unloading Problem . . . . . . . . . . . . . . . . Determination of the Loading/Unloading Boundary The Finite Bar . . . . . . . . . . . . . . . . . . . . . Examples . . . . . . . . . . . . . . . . . . . . . . . . The Elastic Solution . . . . . . . . . . . . . . . . . .

105 . . . . . . .

. . . . . . .

. . . . . . .

. . . . . . .

. . . . . . .

. . . . . . .

. . . . . . .

. . . . . . .

4. Rate Inﬂuence 4.1 4.2 4.3 4.4 4.5

Experimental Results . . . . . The Constitutive Equation . . Instantaneous Plastic Response Numerical Examples . . . . . . Other Papers . . . . . . . . . .

. . . . .

. . . . .

. . . . .

. . . . .

. . . . .

. . . . .

. . . . .

. . . . .

. . . . .

. . . . .

. . . . .

. . . . .

. . . . .

. . . . .

. . . . .

. . . . .

. . . . .

. . . . .

. . . . .

. . . . .

Introduction . . . . . . . . . . . . . . . . Equations of Motion . . . . . . . . . . . The Finite Constitutive Equation: Basic The Order of Propagation of Waves . . Boundary and Initial Conditions . . . . Numerical Examples . . . . . . . . . . . Rate Inﬂuence . . . . . . . . . . . . . . Shock Waves . . . . . . . . . . . . . . . Other Papers . . . . . . . . . . . . . . .

6.3 6.4

. . . . . . . . . . . . Formulae . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . .

. . . . . . . . .

. . . . . . . . .

. . . . . . . . .

. . . . . . . . .

Flow of a Bingham Fluid Through a Tube . . . . . . . . . . Flow of a Bingham Fluid Between Two Circular Concentric Cylinders (Reiner [1960]) . . . . . . . . . . . . . . . . . . . A Model for Slow Motion of Natural Slopes (Cristescu et al. [2002]) . . . . . . . . . . . . . . . . . . . . How to Measure the Viscosity and Yield Stress . . . . . . .

7. Axi-Symmetrical Problems 7.1

169 176 181 189 194 217

6. Flow of a Bigham Fluid 6.1 6.2

105 108 124 127 134 144 155 169

5. Mechanics of Extensible Strings 5.1 5.2 5.3 5.4 5.5 5.6 5.7 5.8 5.9

71 76 88 94

. . . . . . . . .

. . . . . . . . .

. . . . . . . . .

. . . . . . . . .

217 221 223 226 227 230 232 237 240 251

. . . . 251 . . . . 259 . . . . 268 . . . . 290 315

Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 315

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

dynamic

Contents

7.2 7.3 7.4

7.5

7.6

Enlargement of a Circular Oriﬁce . . . . . . . . . . Thin Wall Tube . . . . . . . . . . . . . . . . . . . . Wire Drawing . . . . . . . . . . . . . . . . . . . . . 7.4.1 Introduction . . . . . . . . . . . . . . . . . 7.4.2 Basic Equations . . . . . . . . . . . . . . . 7.4.3 Friction Laws . . . . . . . . . . . . . . . . 7.4.4 Drawing Stress . . . . . . . . . . . . . . . . 7.4.5 Comparison with Experimental Data . . . 7.4.6 Other Papers . . . . . . . . . . . . . . . . . Floating Plug . . . . . . . . . . . . . . . . . . . . . 7.5.1 Formulation of the Problem . . . . . . . . 7.5.2 Kinematics of the Deformation Process . . 7.5.3 Friction Forces . . . . . . . . . . . . . . . . 7.5.4 Determination of the Shape of the Floating 7.5.5 The Drawing Force . . . . . . . . . . . . . 7.5.6 Numerical Examples . . . . . . . . . . . . Extrusion . . . . . . . . . . . . . . . . . . . . . . . 7.6.1 Formulation of the Problem . . . . . . . . 7.6.2 Kinematics of the Process . . . . . . . . . 7.6.3 The Approximate Velocity Field . . . . . . 7.6.4 The Extrusion Pressure . . . . . . . . . . . 7.6.5 Numerical Examples . . . . . . . . . . . .

xi

. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Plug . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . . . . . . . .

8. Plastic Waves. Perforation 8.1 8.2 8.3 8.4 8.5

Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . Various Theories . . . . . . . . . . . . . . . . . . . . . . . Perforation with Symmetries . . . . . . . . . . . . . . . . Modeling of the Taylor Cylinder Impact Test. Anisotropy Analysis of the Steady-State Flow of a Compressible Viscoplastic Medium Over a Wedge (Cazacu et al. [2006])

9. Hypervelocity Impact (Information) 9.1 9.2

317 321 332 332 334 336 337 339 342 346 346 347 349 351 354 357 366 366 368 372 374 375 383

. . . .

. . . .

. . . .

. . . .

. . . .

383 384 393 407

. . . . . 410 425

Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 425 Further Studies . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 434

Author Index

447

Subject Index

457

This page intentionally left blank

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Introduction

Theory of Plasticity studies the distribution of stresses and particle velocities (or displacements) in a plastically (irreversible) deformed body, when are known the external factors which have acted upon him and the history of variation of these factors. The theory was applied to metals to describe working processes both at cold (drawing, rolling, etc.) and warm (extrusion, forging, etc.), to describe term behavior (high and law) involving also temperatures, to short term behavior, to describe impact, shocks, perforation, etc. It was applied to geomaterials, as soils, rocks, sands, clays, etc., with the description of civil engineering applications as tunnels, wells, excavations of all sorts, etc. It was applied to other materials as concrete, asphalt, ceramics, ice, powder-like materials, various pastes, slurries, etc. In the classical sense the Plasticity Theory is time independent. However a time dependent theory was also developed and called Viscoplasticity. Besides Rheology deals with any ﬂow or deformation in which time is the main parameter. From the point of view of formulation of problems, in plasticity one considers in some of the problems, as in elasticity, that the strains are small; whoever in some other problems the consideration of the problems are as in nonlinear ﬂuid mechanics when the strain are ﬁnite. 1

Diagnostic Tests

These are the slow tests in compression or in tension (ε˙ ≤ 10−2 s−1 , say) so as the strain is uniform along the specimen. We denote by σPK =

F A0

and by

σC =

F A

the Piola–Kirchhoﬀ and the Cauchy’s stresses. Here F is the total force applied axially to the specimen, and A the current area, and by A0 the initial area of the cross section of the specimen. We also denote by εH = ln

l l0

and by 1

εc =

l − l0 l0

dynamic

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

2

Dynamic Plasticity

Stress

Q

σY

σP

0

εP

R

εE Fig. 1

Strain

Typical diagram of a diagnostic test.

the Henchy’s strain or the Cauchy’s strain. Here again l is the length of the working area of the specimen, and l0 is the initial length of the same area. As a sign convention, σ > 0 in tension for metals, but it is a reverse convention for rocks and soils (see Fig. 1). σP is the proportionally limit of the specimen where we apply the Hooke’s law σ = Eε with E the Young’s modulus which is constant, and independent on the loading rate and on the loading history. Up to σP we apply the Hooke’s law in both loading und unloading. σY is a conventional or oﬀset yield limit . deﬁned by the permanent εY , generally 0.1% = 0.5% of the total strain. Essentially is that εY is deﬁned by a convention. Thus for ε < εY the unloading is perfectly elastic without hysteresis loop, as σ = σQ + E(ε − εQ ) . Thus we assume small strains and ε = εE + εP . In elasticity we apply the Hooke’s law written as σ = C[ε] or σij = Cijkl εkl where C is a fourth order tensor. We apply this law during loading and unloading and the natural reference conﬁguration is the stress-free strain-free state. If we introduce the two deviators by: tr σ tr ε l and ε = ε − l, σ = σ − 3 3 the Hooke’s law can be written σ = 2Gε

and tr σ = 3Ktr ε ,

dynamic

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

Introduction

dynamic

3

σ

ε

0 Fig. 2

Nonlinear elastic curve.

σ E

A

σ

∆σ

D

F

σ∗ 0

B

εP

Fig. 3

C

εE ∆ε P

ε

Stress work per unit volume.

where G and K are the two elastic constants. The above relations are applied for any elastic isotropic body. There are nonlinear elastic bodies as for instance rubber (see Fig. 2). The stress– strain curve is nonlinear but reversible. The unloading is according to some other law, exhibiting a signiﬁcant hysteresis loop. We cannot describe this behavior by the Hooke’s law but with a nonlinear law, giving a one-to-one correspondence. Since the material remembers his initial conﬁguration, the reference conﬁguration is the initial one. For dissipative materials as the plastic ones, we can deﬁne an irreversible stress work per unit volume by: T σ(t)ε˙P (t) dt . W (T ) = 0

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

4

Dynamic Plasticity

σ

σ∗

• •

•

•

• ε

0 Fig. 4

Lack of one-to-one correspondence.

σ

σY

0

ε

εY

Fig. 5

Linear work-hardening.

That is shown in Fig. 3; it is the total irreversible area under the curve. The remaining area is the potential energy of deformation reversible for the reversible elastic materials (conservative). In order to deﬁne work-hardening, we start with the Fig. 3. In a loading loop BAEDC producing the irreversible strain ∆εP and returning to the same stress σ ∗ , we deﬁne by: (σ − σ ∗ )∆εP > 0 irreversibility , ∆σ∆εP > 0 stability . These two conditions are known as the Drucker’s postulate and are used to deﬁne the plastic work-hardening. Another postulate is due to Iliushin’s; it says that the loading–unloading FAEDF must be positive. In plasticity there is no one-to-one stress–strain correspondence. That is very clear in Fig. 4. The loading history must be known; to a single stress correspond several strains. Plasticity starts with unloading, as compared with nonlinear elastic behavior; and with the plastic strains which can develop only if σ > σY . The linear work-hardening is deﬁned by two straight lines (Fig. 5): σ = Eε

if σ ≤ σY ,

σ = σY + E1 (ε − εY ) if σ ≥ σY . Here E1 is the constant work-hardening parameter, and E1 E.

dynamic

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Introduction

dynamic

5

σ B 2σ Y 2σ Y C 0

ε

K G M Fig. 6

Various hardening laws.

If the stress is increasing very slowly, in the so-called “soft” machines, one is observing some steps on the stress–strain curve. It is question of the so-called Savart–Masson eﬀect, later rediscovered by Portevin–Le Chatelier eﬀect. It was shown that this eﬀect can by described by a rate-type constitutive equation (Suliciu [1981]). The viscosity coeﬃcient has strong variation in some regions of the ε, σ plane that lie above the equilibrium curve. For most materials, if σ is on a plastic state, then −σ is also on the plastic state. As it is well known, there are a lot of materials which do not satisfy this condition. For rocks for instance, if σY t is the yield stress in tension, then σY c is in compression, and |σY c | |σY t |. That is also for concrete, cast iron, soils, glass, powders, etc. That is called Bauschinger eﬀect, discovered in 1886. In Fig. 6 it is along BCK, that is the segment 2σY stays more or less constant during loading. For metals the elastic domain has a constant size 2σY during loading. If during unloading we follow BCGM then the hardening is said to be isotropic. If during unloading we follow the path BCK we say that the hardening is kinematic. Generally, if the yield stress in one direction is diminished by a previous plastic deformation in the opposite direction we have a Bauschingr eﬀect. It introduces anisotropy, sough it can be removed by annealing at high temperature. If we do a loading in a single direction, we cannot distinguish between the two hardening.

2

Tests Performed at Long and Short Term Intervals

If dx is a material element in current conﬁguration, and dX in the initial conﬁg˙ uration, we call λ = dx/dX elongation. The rate of elongation is D = λ/λ (= ε˙ sometimes).

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

6

Dynamic Plasticity

σ

ε→

+∞

local increase of ε (dynamic ) ε2 > ε1 ε1 > ε0 ε0

&

ε→

−∞

σ = const. creep ε = const.

&

stress relaxation

ε

0 Fig. 7

Eﬀect of change of rate of elongation.

Table 1

Variation of ε. ˙

ε˙ < 10−20 s−1 10−8 s−1 ≥ ε˙ ≥ 10−12 s−1

slow tectonic motion, creep tests,

10−4 s−1 ≥ ε˙ ≥ 10−1 s−1

testing machines,

ε˙ 1 s−1 ε˙ 10 s−1

hammer drop, the strain is not uniform, wave propagation is needed,

ε˙ 102 s−1 ε˙ 104 s−1

metal drawing, air gun bullet, high speed impact, ballistics,

ε˙ 106 s−1 − 107 s−1

high speed drawing of very ﬁne wires, or very fast tests.

The change of rate of deformation is shown in Fig. 7. An increase of ε˙ is raising the curves. But this raise in technically limited by the machine we have. For an additional increase, we need dynamic curves, with an local increase ˙ This of ε. increase is done by elastic waves propagating with the velocity c0 = E/ρ. A table of approximate increase of ε˙ is given in Table 1. This is a very approximate table of variation of ε. ˙ For constant stress we have creep, but for constant strain we have stress relaxation. Any other intermediate variation of the strain rate is possible. For |ε| ˙ → ∞ we have very fast variation of the strain rate, impossible to realize practically. In order to have a representation we take into account that mainly the plastic properties are inﬂuenced by the change of the rate of strain (see Fig. 8). A relationship was proposed by Ludwik from 1909, and is of the kind shown on Fig. 8. Thus we have for a ﬁxed strain: σ = σY + σ0 ln

ε˙P ε˙P 0

and σ > σY > 0

dynamic

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

Introduction

dynamic

7

σ ε2 > ε1 ε1 > ε0

σY

0

Fig. 8

ε0

•

ε

Inﬂuence of the strain rate on the stress–strain curve.

with σ0 = constant. If the elastic strains are disregarded, the stress–strain curves are σ − σY if σ > σY , 3η ε˙ = 0 if 0 ≤ σ ≤ σY , where σ − σY is the overstress. σY is the yield stress for a conventional small ε˙0 obtained in very slow performed tests, when ﬂow starts being possible. η is a viscosity coeﬃcient; if two tests are performed with the strain rates ε˙1 and ε˙2 we have: σ2 − σ1 , 3η = ε˙2 − ε˙1 to determine η. If η is constant for any strain rates, the relation is linear, otherwise nonlinear. Since in this relation there is no strain, the reference conﬁguration is the actual one. For work-hardening materials (Malvern): σ − f (ε) if σ > f (ε) , 3η ε˙ = 0 if 0 ≤ σ ≤ f (ε) . The reference conﬁguration is the initial one or a relative one, corresponding to the state when the test started (for geomaterials, for instance). Let as give several examples. In Fig. 9 is given the stress–strain curves for schist. One can see that the inﬂuence of the strain rate is felt from the beginning. The hole curve is inﬂuenced, not only the plastic part. Also, the last points correspond to failure. Thus with an increase of loading rate the stress at failure is increased, while the strain at failure is decreased. Thus a theory of failure expressing in stresses only, would not work. In order to see that the inﬂuence of the strain rate is not always to be seen always on the stress–strain curves. In Fig. 10 are given the curves for granite, obtained in

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

8

Dynamic Plasticity

Fig. 9

Fig. 10

Stress–strain curves for schist.

Inﬂuence of the strain rate on granite.

triaxial tests (after Sano, Ito, Terada [1981]). One can see that the inﬂuence of the strain rate is practically zero on the axial stress strain curves. But the inﬂuence on the radial strain is remarkable on the other curves. Failure is the last point, but for the lowest radial curve is extended until −0.064, thus extending very much outside the ﬁgure. Concerning failure one can see that stress at failure is increased with the strain rate, while the strain is decreased. Thus failure would be impossible to describe with a condition written in stresses only.

dynamic

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Introduction

3

dynamic

9

Long-Term Tests

In order to ﬁnd out the principal properties of creep and relaxation, one is doing long-terms tests. If the stress applied is relative small, the creep is transient, i.e., stabilizing after a certain time. In Fig. 11 is shown the creep curves for schist. One can see that the ﬁrst curves correspond to transient creep only. The stresses are too small. The fact that the stresses are small, on the right side is given the ε˙ − t curves. The curves corresponding to the transient case come quite fast at the origin (ε˙ → 0). For higher stresses, we obtain a steady state creep, with ε˙ = const. That is obtained generally for σ ≥ 0.6σc , where σc is the short-term failure strengths. Temperature has a strong inﬂuence on creep. With increasing temperature the creep curves start at a lower stresses and extend very much. When the applied stress is still increased, we arrive at the tertiary creep, where ε¨ > 0. That means that soon failure will take place. From the right side of the diagram, the tertiary creep is not bringing the curves at zero. From the very many laws existing, the most known is the Norton law where ε˙ ∼ σ n . Generally we describe creep by ε˙ = f (σ, ε), the temperature being also inﬂuenced. For relaxation one is describing it with σ˙ = g(σ, ε), the temperature being again present. Jugging only from the creep curves, it is diﬃcult to see if they correspond to a viscoelastic model or to a viscoplastic one. The only things we can say is the diﬀerence in the history dependent principle. Figure 12 is showing the diﬀerence. If one is loading with the stress σ1 and then increase it to σ2 , or applied from the beginning the stress σ2 , we obtain the same thing (at left) if there are no internal changes, or obtain something diﬀerent (at right), with possibly internal changes. In the ﬁrst case the loading is history independent, while in the second we have a history dependency. The history dependency is probably viscoplastic.

Fig. 11

Creep curves for schist.

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

10

dynamic

Dynamic Plasticity

ε σ2

ε

σ2

σ2 σ2 σ1

σ1 t 0

t 0

Fig. 12

Fig. 13

Principle of history dependency.

The method used for the determination of the elastic parameters.

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Introduction

dynamic

11

Thus we have to consider plasticity only if: • • • • •

the stresses σ > σY , we obtain an irreversible strain, we have a history dependence, generally, we have a initial reference conﬁguration, generally, the deviator relationship (σ ∼ ε ) is distinct from the volumetric (tr σ ∼ tr ε).

Concerning the procedure used to measure the elastic parameters for various materials, for metals there are no problems. The problem is for the powder-like materials, or for rocks, for instance. The idea is that for such materials the hysteresis loop is quite important, so that if one is doing the unloading immediately, it is diﬃcult to determine the elastic parameters directly. Figure 13 (after a PhD of Niandou [1994]) is showing such a problem. If one is trying to determine the elastic parameters directly immediately after loading, one obtains the hysteresis loops shown. One has to wait after each re-loading a number of minutes during which the rock is creeping. On the last ﬁgure shown one can see that the rate of deformation is decreasing wary much. Thus after a period of time if one is doing the unloading, no hysteresis loops are observed any more. This method is to separate the rheological properties from the unloading. That is the method proposed for rocks since 1988 (Cristescu). It was applied to many other materials since that time.

4

Temperature Inﬂuence

A temperature increases will decrease: • • • •

the the the the

elastic parameters, yield stress, work-hardening modulus, ultimate strength.

It is important to mention here the Zener–Hollomon parameter for metals: ∆H , Z = ε˙ exp RT where ∆H is the activation energy which may depend on temperature, R is a universal gas constant and T the absolute temperature. For ε = const. the stress can be obtained from ∆H . σ = f (Z) = f ε˙ exp RT That is we can change the rate of strain or temperature according to this relation.

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

12

Dynamic Plasticity

Fig. 14

5

Triaxial stress–strain curves for alumina powder.

The Inﬂuence of the Hydrostatic Pressure

It was shown that with an increase of pressure: the yield stress slight increases, the ultimate strength increases, the elastic modules G and K increase (increase of wave velocities), the work-hardening modulus increase and the ductility increases signiﬁcantly. The last increase has lead to new methods of metal working, where an additional pressure was used. Generally, for metals the constitutive equations is written in deviators. The above is not true for: rocks, soils, wood, cast iron, powder like materials, granular like materials, etc. For all these materials the pressure plays an important role. In Fig. 14 is shown the stress–strain curves for alumina powder, obtained in triaxial tests. One can see that all curves, the axial, diameter, and volumetric curves, are strongly dependent on the pressure (written along the curves). 6

Variation of Elastic Parameters with Plastic Strain (Metals)

During plastic deformation the elastic parameters vary. That has a signiﬁcance for the expression of wave velocities (say). For cylindrical specimens subjected to uniaxial tests ε2 = ε3 = −νε1

dynamic

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Introduction

dynamic

13

with ν the Poisson’s ratio. For isotropic elastic materials 0 ≤ ν ≤ 0.5. If ν ≈ 0 no lateral strain is to be expected. For ν ≈ 0.5 we have an incompressible material ε11 + ε22 + ε33 = 0. For rubber ν = 0.47, steel 0.25 ≤ ν ≤ 0.30, aluminum 0.26 ≤ ν ≤ 0.36, cork ν = 0.00, polyethylene and paraﬃn ν ≈ 0.5. In the plastic domain for aluminum ν is very close to 0.5, thus shoving plastic incompressibility. Thus the variation of the volume is elastic only: σ = 3KεE and εP = 0. This result is true for metals, only. For rocks, granular materials, etc. it is not. Bibliography Niandou H., 1994, Th´ese de Doctorat, Lab. de M´ecanique de Lille URA 1441 CNRS. Sano O., Itˆ o I. and Terada M., 1981, Inﬂuence of strain rate on dilatancy and strength of oshima granite under uniaxial compression, J. Geophys. Res. 86, B10, 9299–9311. Suliciu I., 1981, On the Savart–Masson eﬀect, J. Applied Mech. 48, 426–428.

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

This page intentionally left blank

dynamic

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

dynamic

Chapter 1

Yield Conditions

1.1

Stresses

In order to understand well the problem we have to show several concepts which are helping. We choose an octhaedrical plane and its normal (see Fig. 1.1.1). For a point of stress (σ 1 , σ 2 , σ 3 ) we have the stress vector tn which must be projected on the hydrostatic line and on a normal to the hydrostatic line. Since σ1 0 0 tn = [n1 , n2 , n3 ] 0 σ2 (1.1.1) 0, 0

0

σ3

its components are i1 i2 i3 tn = n · T = σ1 √ + σ2 √ + σ3 √ 3 3 3 so that the projection of this vector on the hydrostatic line is σ2 σ3 σ1 + + = σ, tn · n = 3 3 3 where σ is the mean stress. The projection on the hydrostatic line is now

(1.1.2)

(1.1.3)

i2 i3 i1 (tn · n)n = σ √ + σ √ + σ √ 3 3 3 with absolute value |(tn · n)n| = |σ| . The projection normal to the octhaedrical line is tτ = tn − (tn · n)n σ σ σ σ2 σ3 σ1 i1 + √ − √ i2 + √ − √ i3 = √ −√ 3 3 3 3 3 3 1 = √ (σ1 i1 + σ2 i2 + σ3 i3 ) 3 15

(1.1.4)

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

16

dynamic

Dynamic Plasticity

Fig. 1.1.1

Octahedral plane and all other associated concepts.

with the absolute value

|tτ | = τoct =

2 IIσ . 3

(1.1.5)

We got thus the interpretation of Roˇs and Eichinger [1926]: the absolute value of the vector tensor normal to the linear hydrostatic axes is equal to the square root of the second invariant of the deviatoric stress tensor. For notation we give IIσ =

1 2 3 2 1 2 [(σ ) + (σ2 )2 + (σ3 )] = τoct ¯ = σ 2 1 2 3

(1.1.6)

= σij − σδij is the stress deviator. and σij Since the vector tτ in entirely in the octahedral plane, one can try to project it on various directions in this plane. Thus projecting on the π plane is giving (see Fig. 1.1.2): σ1 2 σ2 2 σ3 2 i1 + √ i2 + √ i3 . tn |π = √ 3 3 3 3 3 3

Now projecting on the σ 3 direction we have, σ2 2 1 σ3 2 σ1 2 1 +√ −√ tn · (−i3 ) = √ 3 32 3 32 3 3 1 = √ (σ1 + σ2 − 2σ3 ) 3 2 σ = − √3 . 2

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

Yield Conditions

dynamic

17

σ3'

π 2π 3

i3' 0 i'2

i1'

π 3

α ωσ

σ1'

σ2' tτ

Fig. 1.1.2

Octahedral plane with the assumption σ2 > σ1 > σ3 .

Thus we can write: σ tn · i2 = τoct cos α = √2 , 2 2π = tn · i3 = τoct cos α + 3 2π = tn · i1 = τoct cos α − 3

σ √3 , 2

(1.1.7)

σ1

√ , 2

σ1 σ2 σ3 = IIIσ . Taking into account that

2π 1 2π cos α − = cos 3α , cos α cos α + 3 3 4

we arrive at the relation

cos 3α =

3 IIσ

3

IIIσ , 2

(1.1.8)

α ∈ [0, π/3] deﬁnes the orientation in the octahedral plane of the stress vector t(x, n) and is the angle with ii corresponding to σi maximum. tτ is located between ii corresponding to σi maxim and ij corresponding to σj intermediate.

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

18

Dynamic Plasticity σ3 1 1 1 , , n 3 3 3

σ3′

σ2′

α τoct

P

σ σ1′

σ2

0

σ1

Fig. 1.1.3

Possible use of the invariants.

i3′ i3

arc cos

1 3

= 54 $73 n

0 Fig. 1.1.4

Projection on the octahedral plane.

If we write √ √ cos α σ2 / 2 = m, − 3 σ3 − σ1 sin α we obtain the Lode parameter, which is deﬁning the orientation in the octahedral plane.

dynamic

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

Yield Conditions

dynamic

19

From (1.1.7) we get:

3 τoct sin α − 2 σ2 − σ3 3 = τoct sin α + 2 2 σ3 − σ1 3 =− τoct sin α . 2 2 σ1 − σ2 = 2

π , 3 π , 3

(1.1.9)

Since we have chosen σ2 > σ1 > σ3 we have: σ1 − σ2 < 0

or

σ2 − σ3 > 0

or

σ3 − σ1 < 0

or

π π ≤ α ≤ 2π + , 3 3 π π − ≤α≤π− , 3 3

π+

0 ≤ α ≤ π.

Therefore we have 0 ≤ α ≤ π/3 which is satisfying all the inequalities. Since τmax = τ1 = (σ2 − σ3 )/2, we have: τmax π = sin α + 3 (3/2)τoct and since we have to choose only half of the interval 0 ≤ α ≤ π/6 to get diﬀerent values for the ratio, we get: √ 3 τmax ≤√ (0.866 =) ≤1 (1.1.10) 2 IIσ √ for α = π/6 and α = 0. The conclusion is that τmax and IIσ is quite close to each other. Thus a point of coordinates σ1 , σ2 , σ3 can be replaced by a point σ, τ, α, introducing the three invariants: the ﬁrst invariant of the stress, and the second and third invariants of the stress deviator (Fig. 1.1.3). We have still show howa quantity is projected on the octahedral plane. We have cos(i3 , i3 ) = 2/3, and just any quantity which is projected on the octahedral plane is to be multiplied by 2/3 (Fig. 1.1.4).

1.2

Yield Conditions

It is assumed that when deforming plastically all materials are satisfying a condition called yield condition. At least most metals satisfy this condition. The yield conditions satisfy a few general conditions. Let us describe them.

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

20

dynamic

Dynamic Plasticity

Assumption 1. We assume that for each material a yield function f (σ) exists so that: f (σ) < 0

or if f (σ) = 0 and ∂f σ˙ = 0 ∂σ ij

f (σ) = 0

and

∂f σ˙ ij < 0 the material is elastic ; ∂σij for loading in perfect plasticity ,

ij

∂f σ˙ ij > 0 ∂σij

for loading for work-hardening plasticity .

In order to give an example let us consider the yield criteria of von Mises which can be written f (σ) := IIσ − k 2 . Here k if it is constant the material is perfectly plastic; if however k is changing when the plastic deformation takes place, that is k(εP ), the material is work-hardening. Assumption 2. For metals the yield is independent of the spherical part of the stress. Thus f depends on the stress deviator f (σ). That means that the yield conditions are cylindrical in the stress space. Assumption 3. The material is initially isotropic. Therefore f (Iσ , IIσ , IIIσ ) = k 2 the yield function depends on invariants only. There are no preferred directions; f does not depend on the orientation of the principal axes. Taking into account the previous assumption, f depends on the deviator invariants: f (IIσ , IIIσ ) = k 2 .

(1.2.1)

Assumption 4. Since for most metals the curves σ–ε are symmetric with respect to the origin of axes, we must have f (σ) = f (−σ). Because IIσ = II(−σ ) the third deviator invariant must be involved in even powers. The Tresca [1868] Yield Condition. It is, in the octhaedrical plane, a regular hexagon as shown in Fig. 1.2.1. Thus the Tresca hexagon is deﬁne as τmax = k = const. It can be expressed in terms of invariants as described previously. Thus we can write (σ1 − σ2 ) = 4k 2 , σ1 σ2 + σ2 σ3 + σ3 σ1 = −IIσ , σ1 σ2 σ3 = IIIσ , σ1 + σ2 + σ3 = 0 . We can eliminate all the deviator stress components to get 2 27IIσ3 4 IIIσ2 3IIσ − − 1 − = 0, 64k 6 27 IIσ3 4k 2

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

Yield Conditions

dynamic

21

σ3' σ3 > σ1 > σ2

σ3 > σ2 > σ1 2 −σ

k =2

σ3 −

2 σ 3 Y

σ1 −

σ1'

σ

3

σ1 > σ2 > σ3 Fig. 1.2.1

Fig. 1.2.2

σ1

=2 k

σ2− σ1 = 2k

σ1 > σ3 > σ2

σ1− σ2 = 2k

σ3

0

π 3

=2 k

σ3 σ 2−

k =2

σ2 > σ3 > σ1

σ2'

σ2 > σ1 > σ3

The Tresca hexagon.

The plane Tresca hexagon.

which is due to Reuss. That is a complicated way of expressing the Tresca yield condition, so that today it is expressed also as τmax = k. For the plane problems it is expressed in a simpler way as in Fig. 1.2.2. For the Tresca condition the relationship between the yield stresses in shear and tension is 2τY = σY . The number 1/2 is a little too small, experimentally it is ranging somewhere between 0.55 and 0.6.

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

22

Dynamic Plasticity

The Mises [1913] Yield Condition. The von Mises yield condition is expressed as IIσ = k 2 , where IIσ = =

1 2 2 2 [(σ11 − σ22 )2 + (σ22 − σ33 )2 + (σ33 − σ11 )2 ] + σ12 + σ23 + σ31 6 1 2 [(σ ) + (σ2 )2 + (σ3 )2 ] . 2 1

The von Mises yield condition is represented in the three axial stress space as a circular cylinder shown in the last two ﬁgures. For the plane case it is an ellipse. For the von Mises yield condition the relationship between the yield stress in shear √ ∼ and tension is τY = σY / 3 = 0.557σY . That is a much better value. All the correspondences of the two yield condition and the tests are shoving a better ﬁtting of the von Mises than that of Tresca. Also, any generalization of this condition to for anisotropic materials is a combination of the two conditions.

1.3

The Classical Constitutive Equation for Perfectly Plastic Materials

Saint-Venant–Mises Constitutive Equation The ﬁrst law of plasticity is due to Barr´e de Saint-Venant [1870]. He has done several assumptions which have been inspired from metal working theories but the meaning of the plastic ﬂow was changed. They are: εE = 0

the elastic part of the strain rate is negligible

since εP V ≈ 0 plastic incompressibility is assumed, i.e., D = D , σ = λD as in Newtonian viscosity, but λ is variable, λ is determined from a plasticity condition; squaring the above law we have √ σ : σ 2 σ : σ = λ D : D or λ = √ D:D

and for a von Mises plasticity condition IIσ = k 2 = conts. for perfect plasticity: k λ= √ . IID Thus the constitutive equation is:

√

k σ = √ D IID IIσ < k

and tr D = 0 if IIσ = k 2

or IID = 0

for perfectly plastic , for rigid behavior .

The meaning of k follows from the yield conditions. For von Mises yield conditions

dynamic

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Yield Conditions

dynamic

23

1 1 2 2 2 2 2 2 σ : σ = (σ11 + σ22 + σ33 ) + σ12 + σ23 + σ31 = k2 2 2 2 if all σij = 0 besides σ12 = 0 we obtain σ12 = k 2 or, if the yield stress in pure shear is τ , τ = k.√ In uniaxial tensile tests σ11 = 0 all other σij = 0, we obtain Y 2 /3 = k 2 , or k = Y / 3, where Y is the yield stress in uniaxial tensile (or compressive) tests. Thus we arrive at the relation σY τY = √ , 3

for the yield stresses in pure shear and tensile, for the von Mises yield condition. The classical constitutive equation seems to be a non-Newtonian ﬂuid, but it is not, since it is time-independent (nonviscous). To show that we write the constitutive equation as D σ √ , = k IID and we change v with µv, with µ > 0, that is we change the time. We have D → µD, and IID → µ2 IID thus µ disappears from the constitutive equation. Thus the main properties of the constitutive equation are time independent, the reference conﬁguration is the present one (in the case we have no internal changes) D is involved as for ﬂuids; it is used when the plastic deformation are signiﬁcant, the elastic part of the strain rate are negligible, as in some metal working problems. The Prandtl–Reuss Constitutive Equation This is a constitutive equation developed by Prandtl [1924] for two-dimensional cases and extended by Reuss [1930] for the three-dimensional case. Assuming small deformations the constitutive equations are: ε˙ = ε˙ E + ε˙ P ,

ε˙ E =

1 σ˙ , 2G

tr σ˙ = 3K tr ε˙ ,

(1.3.1)

λ σ˙ , tr ε˙ P = 0 . 2G Thus the strain rates are additive, the reference conﬁguration is usually the initial one, G is the shearing modulus, and K is the bulk modulus with G = E/2(1 + v) and K = E/3(1 − 2v). From there one receive ε˙ P =

+ λσij . 2Gε˙ij = σ˙ ij

(1.3.2)

In (1.3.2) we have 10 variables, 3 velocities, 6 stresses and λ. If we assume the von Mises yield condition IIσ = k 2 , we obtain either σ˙ ij IIε˙ P + σij ε˙ij = 2G k

January 12, 2007

24

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

dynamic

Dynamic Plasticity

or ε˙ij =

˙P σ˙ ij W + σ 2G 2k 2 ij

˙ P = σij ε˙P the stress work per unit volume. with W ij With all these the Prandtl–Reuss constitutive materials is √ σ˙ ij IIε + σij ε˙ij = 2G k if IIσ = k 2 tr σ˙ = 3K tr ε˙ σ˙ ij if IIσ < k 2 ε˙ij = 2G tr σ˙ = 3K tr ε˙ if IIσ = k 2

equation for perfectly plastic

and σij σ˙ ij = 0 ,

(1.3.3) or and σij σ˙ ij < 0 .

σ˙ ij = 0 is called consistency condition. The reference conﬁguration The relation σij is either the actual one or the conﬁguration after unloading from current conﬁguration. Also, εE does not satisfy the Saint-Venant compatibility conditions, since there may be no single valued continuous displacement ﬁeld that would take the whole body from deformed conﬁguration to an unstressed conﬁguration. Thus ε˙ P is not explicitly integrable. It is easy to show that the Prandtl–Reuss constitutive equation is time-independent, i.e., they are nonviscous.

The Hencky Constitutive Equation This is a constitutive equation developed by H. Hencky [1924], tough A. Nadai [1923] has used it for torsion problems, and afterwards it was used by A. A. Iliushin [1961]. The main assumption is that one can write it as for Hooke law, but the “plastic” parameters are variable, not constant. Thus: σ = 2GP ε , σ = 3KP ε . But KP coincides with K because the volume behavior is elastic. So it is only G which can be written: √ IIσ S = , 2GP = √ E IIε if one uses the Sokolovsckii notation. Thus for work-hardening condition: S = F (E) , σ =

F (E) ε , E

σ = 3Kε ,

(1.3.4)

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Yield Conditions

dynamic

25

or, E = F −1 (S) , ε =

F −1 (S) σ , S

(1.3.5)

σ˙ for all cases . 3K One has to observe that this constitutive equation was extensively used because it is easily reversible; it is written in ﬁnite form and called constitutive equation of “plastic deformation”; it was used when the strain are increasing continuously; for proportional loading paths σ(X, t) = λ(t)σ 0 (X), the Prandtl–Reuss constitutive equation coincides with the Hencky (Iliushin [1961]); the reference conﬁguration is the initial one. We can think to another variant of the Hencky constitutive equation by assuming: ε˙ =

ε = ε E + εP , εE satisfy the Hooke constitutive equation, the plastic strain satisﬁes −1 1 F (S) − σ . εP = S 2G

(1.3.6)

If we diﬀerentiate the constitutive equation we can write: −1 F (S) d F −1 (S) σ˙ + σ for E = F −1 (S) and S˙ > 0 for loading , dt S S ε˙ = for unloading elastic ˙ σ for E = F −1 (S) and S˙ ≤ 0 or E < F −1 (S) 2G σ for all cases . ε˙ = 3K The Hencky’s constitutive equation is obviously time independent. 1.4

Work-Hardening Materials

We assume for work-hardening materials small strains so that ε = ε E + εP . The elastic rate of deformation components satisfy ε˙E ˙ kl . ij = Aijkl σ The yield function F exists which satisfy F (σij , εP kl , χ) = 0

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

26

Dynamic Plasticity

Fi = 0

∂Fi ∂σ kl Fj = 0 ∂F j ∂σ kl Fig. 1.4.1

The Koiter generalization.

P with F (0, εP ij , χ) < 0 at reference conﬁguration with εij and χ ﬁxed at a particle. χ is a scalar called work-hardening parameter. If F (σij , χ), i.e., εP ij is not explicitly involved the work-hardening is called isotropic. If however, F (σij , εP kl ) the work-hardening is inducing anisotropy. The plastic rate of deformation is given by: P F (σij , εkl , χ) < 0 or for ∂F 0 F (σij , εP σ˙ ij ≤ 0 . P kl , χ) = 0 and ε˙ij = ∂σij ∂F ˙ ij ) for F (σij , εP σ˙ ij > 0 . Bij (σkl , εP mn , χ, σ kl , χ) = 0 and ∂σij

The initial data are deﬁned by εP (0) = εP 0 , and χ(0) = χ0 , thus a reference conﬁguration in assumed, not necessarily the stress-free, strain-free conﬁguration. Since it is assumed that both at time t and t + ∆t the yield condition is satisﬁed during a loading, we have ∂F ∂F ∂F χ˙ = 0 , σ˙ ij + P ε˙P ij + ∂σij ∂χ ∂εij which shows that all the increments are not independent. This is the consistency condition. Because when approaching the yield condition by continuity, we must have: lim Bij (σkl , εP ˙ ij ) = 0 , mn , χ, σ ∂F σ˙ ij → 0 , ∂σij which is the continuity condition. That means that only the normal component of the increment of the stress tensor is giving a plastic increment of the strain ﬁeld. Thus we have ε˙P ˙ mn ) ij = λ(σkl , σ

∂F ∂σij

dynamic

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

Yield Conditions

dynamic

27

and we call the constitutive law associated to the yield condition. That is true for most metals, but not true for rocks or soils, for instance. For such materials we have to introduce a plastic potential following the idea of von Mises from 1928: ε˙ij = µ(σkl , σ˙ mn )

∂H , ∂σij

where H is the plastic potential. For such materials the constitutive equation is called nonassociated. There are yield conditions which have several constitutive equation meeting at a point. For instance the Tresca yield condition is of this kind (see Fig. 1.4.1). In this case we use the idea of Koiter [1953]: ε˙P ij = λk

∂Fk ∂σij

with the constants λk deﬁned by: ∂Fk σ˙ = 0 for perfect plasticity ∂σ ij λk > 0 if

Fk (σmn ) = 0 Fk (σmn ) < 0

λk = 0 if

Fk (σmn ) = 0

ij

and

∂Fk σ˙ ij > 0 for working-hardening ∂σij

or

∂Fk ∂σmn σ˙ mn < 0

for perfect plasticity

∂Fk σ˙ mn ≤ 0 ∂σmn

for working-hardening .

and

Thus, only at the corner are involved several values of λk .

1.5

Isotropic Hardening

For the isotropic hardening the yield condition is written F (σij , χ) : f (σij ) − H(χ), and in a speciﬁc form f (IIσ , IIIσ ) = H(χ). It is interesting to follow the way in which the work-hardening parameter is determined. It can be the irreversible stress work per unit volume (Fig. 1.5.1), i.e.,

t

χ(t) = W P (t) =

σij (X, s)ε˙P ij (X, s) ds 0

or

t χ(t) = 0

4 II P ds = 3 ε˙

t 0

t 2 P P dεij dεij ds = ε¯˙P (s) ds , 3 0

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

28

Dynamic Plasticity

σ3'

A

0

σ2'

σ1' Fig. 1.5.1

The isotropic hardening.

where ε¯˙P is not a derivative. In this case χ(t) is the history of the eﬀective plastic strain increment. However we can still consider by deﬁnition: 2 P P ε (t)εP χ(t) = ε¯ (t) = ij (t) 3 ij and the work-hardening parameter is equivalent to the plastic strain. For the von Mises yield condition written as: √ σ ¯ = 3k with σ ¯ the equivalent stress: 3 2 (σ1 + σ22 + σ32 )1/2 = 3IIσ σ ¯= 2 =

1/2 1 2 2 2 [(σ11 − σ22 ) + (σ22 − σ33 ) + · · · ] + 3(σ23 + · · · ) . 2

If only one component, say, σ11 = 0, and all the others σij = 0, then σ ¯ = |σ11 |. For such a component we write: σ ¯ (t) = F (W P (t)) , t P ¯ σ ¯ (t) = H ε˙ (s) ds , 0

σ ¯ (t) = G(¯ εP (t)) , which describe various possible variants of the isotropic work-hardening.

dynamic

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

Yield Conditions

29

σ1 = H σ1

dynamic

( ∫ ε ds ) P 1

σ

σ = H ( χ ( t )) ∆σ

σ1

t

W P (t ) = ∫0 σ 1

dl σ 12 (t ) − l0 2E

t

χ (t ) = ∫0 ε P ( s ) ds

0

∆χ

dl dσ 1 dW P = σ 1 − E l0

ε 1P

Fig. 1.6.1

1.6

The universal stress–strain curve.

The Universal Stress Strain Curve

If we do a single test we have σ ¯ = σ11 = σ1 (assume that σ11 is positive). If = εP the specimen is cylindrical, εP 2 3 , and if we assume plastic incompressibility P P ε1 = −2ε2 . Thus if we take all these into account we have (Fig. 1.6.1): 2 P P 2 1 P2 2 dεij dεij = dεP dε = ε˙P + 1 ds . 1 3 3 2 1 Thus if we are doing a single test we discover a three-dimensional law to be applied generaly. We have to apply the general law since the function H is already known. If the constitutive equation is ε˙P ij (t) = λ(t)σij (t) with λ ≥ 0, i.e., the principal directions of ε˙P ij and of σij coincide, then we have

˙ P (t) = σ W ¯ (t)ε¯˙P (t) . That is easy to show since

σij λσij

=

3 σ σ 2 ij ij

Thus the work-hardening law is

σ ¯ (t) = F 0

t

2 P P ¯ ε¯˙P . ε˙ ε˙ = σ 3 kl kl

¯˙ ds . σ ¯ (s)ε(s)

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

30

Dynamic Plasticity

We have the suggestion to write this law t P ¯ σ ¯ (t) = H ε˙ (s) ds 0

and it is easy to pass from one to the other. If the variation of the plastic strains is proportional, i.e., P εP ij (t, X) = h(t)εij0 (X)

at every particle X. Then dεP dh ij = εP ij0 dt dt i.e., dh . ε¯˙P = ε¯P 0 dt By integration with respect to time at a ﬁxed particle X with h(0) = 0, we get t ε¯˙P (s) ds = ε¯P 0 h(t) . 0

Generally a proportional variation of εP ij in every point of the body is not possible, but in very special designed laboratory test. The equality t ε¯˙P (s) ds = ε¯P (t) 0

do not hold for all practical cases. Thus the work-hardening condition σ ¯ (t) = G(¯ εP (t)) is generally not correct, though extensively used. It disregards the history dependence of the plastic deformation. This is a closed relation to nonlinear elasticity. 1.7

Constitutive Equation for Isotropic Work-Hardening Materials

From the work-hardening condition f (σij ) = F (χ) ,

we get the consistency condition ∂f ∂F λ ∂F χ˙ = σ σ . ˙ ij = σ ∂σij ∂χ ∂χ kl 2G kl If we solve with respect to λ and we introduce in the constitutive equation ε˙P ij =

λ σ . 2G ij

dynamic

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

Yield Conditions

We get ε˙P ij

1 = 2IIσij (∂F/∂χ)

dynamic

31

∂f ˙ kl σij . σ ∂σkl

Thus the general constitutive equation is σ˙ ij 1 + ε˙ij = 2G 2IIσ (∂F/∂χ)

∂f ˙ kl σij σ ∂σkl

with the bracket deﬁned by A if f (σij ) = F (χ) and A = ) = F (χ) and f (σij 0 if ) < F (χ) . f (σij

∂f ˙ ij > 0 σ ∂σij ∂f ˙ ij ≤ 0 or σ ∂σij

If we write the yield condition in the form F (σij , χ) := f (σij ) − H(χ) ,

then the constitutive equation is ε˙P ij =

)σ˙ kl

∂F (∂F/∂σkl (∂F/∂χ)(∂F/∂σmn )σmn ∂σij

with a similar deﬁnition of the bracket . 1.8

The Drucker’s Postulate

For stable work-hardening materials Drucker [1951] has established the following postulate. Assume that a stress–strain curve is built. It is showing as in the Fig. 1.8.1. We start from a stress σ0 . We load by producing also some plastic deformation ∆εP 1 . Then we unload, up to the initial stress σ0 . If the material is a stable work-hardening, then two conditions are to be satisﬁed: ε˙P ˙ ij ≥ 0 , ij σ 0 ε˙P ij (σij − σij ) ≥ 0 .

Thus the plastic work done by external agency during the application of an additional stress is positive and the net total work performed by the external agency during the cycle of adding and removing stress is non-negative. The Drucker’s postulate has signiﬁcant consequences for metal plasticity. Thus the yield condition must be convex, nowhere concave. That is shown in Fig. 1.8.2. Another similar postulate was invented by Iliushin, but it is connected to the strain concept. One is starting from a certain strain εij and one make a loading

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

32

Dynamic Plasticity

Fig. 1.8.1

The Drucker’s postulate.

F (σ ij , χ ) = 0

εijP

F (σ ij , χ ) = 0

σ ij0

σ ij

σ ij

σ ij0

Fig. 1.8.2

εij

Consequences of the Drucker’s postulate.

and unloading until one reaches the same strain (see Fig. 1.8.1). A weakened form of Iliushin’s postulate, which says that the changing rate of the stress work done along every standard strain cycle should be non-negative, whenever the incorporated plastic sub path tends to vanish, is due to Bruhns et al. [2005]. The Drucker’s postulate has been extensively considered in the literature. It is a nonenergetic and equivalent to associated ﬂow rule (see Stoughton and Yon [2005] for literature). 1.9

Kinematical Work-Hardening

Another work-hardening law is the kinematical work-hardening. It is shown in Fig. 1.9.1 for a plastic rigid model. The yield surface does not change shape; it translates in the stress space. The size of the elastic domain remains constant and

dynamic

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

Yield Conditions

dynamic

33

σ1

arc tan c1

σY

σ Y + c1ε 0' c1ε

0

σ Y − c1ε

−σY

Fig. 1.9.1

The work-hardening model.

F ( t + ∆t ) = 0

F (t ) = 0

M

σ ij cεijP

0' P

α ij

N

α ij

σ ij

0

σ ij Fig. 1.9.2

The kinematical work-hardening assumptions.

equal to 2σY (rigid). The origin translates with c1 ε in the case of linear workhardening/rigid model. c1 is a constant work-hardening modulus. This model is describing an idealized Bauschinger eﬀect. For the general three-dimensional case the initial surface is F (σij ) = 0. The translated surface is F (σij − αij ) = 0, where the coordinates of the new origin are αij . Some additional postulates are to be satisﬁed by αij in order to satisfy the history of the plastic deformation. It must satisfy the initial condition α = 0 if εP = 0. It is called sometimes “back stresses”.

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

34

Dynamic Plasticity

Prager [1959] postulated that the yield surface translates in the direction normal ∂F/∂σij at the current stress state σij in the nine-dimensional space, i.e., in the direction of PM. That is α˙ ij = cε˙P ij if we assume ε˙P ij ∼ ∂F/∂σij . Consideration in spaces with smaller dimensions than nine, may lead to mistakes since the normal may not remain normal. The constitutive equation is (Fig. 1.9.2) ∂F (σ − α) . ∂σ The scalar η is obtained from the consistency condition ˙ = η(σ, εP , σ) ˙ ˙ ε(σ, εP , σ)

∂F (σ − α) ˙ = 0, : (σ˙ − α) ∂σ where, if one takes into account the above relations we have ε˙P ij =

∂F (σkl − αkl ) (∂F (σkl − αkl )/∂σmn )σ˙ mn . c(∂F (σkl − αkl )/∂σgh )(∂F (σkl − αkl )/∂σgh ) ∂σij

If we make the assumption that the yield surface translates in the direction PN, i.e., ˙ = (σ − α)µ˙ , α where µ˙ > 0 is an additional unknown. It is a diﬃcult problem with this additional unknown. 1.10

Further Developments

Combined Isotropic and Kinematical Hardening. Some authors have combined the two models to get a combination in the form f (σ − α, χ) = 0 , where α and χ are the two work-hardening coeﬃcients, the kinematical and workhardening. As an example one can consider yield surfaces of the form f=

1 1 (σ − α)(σ − α) − σY2 = 0 . 2 3

Mr´ oz [1969] has introduced the multi-surface model to describe the cyclic eﬀect and the nonlinearity of stress–strain loops. There are several such surfaces fi (σ − α, χi ) = 0 ,

i = 1, 2, . . . , n .

Dafalias and Popov [1975] have reduced the number of surfaces at two, one corresponding to the conventional yield surface and the other is a bounding surface.

dynamic

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

Yield Conditions

dynamic

35

Thus the two surfaces are f = (σ − α)2 − σY2 = 0 ,

f ∗ = (σ ∗ − α∗ )2 − σY∗2 = 0 ,

with α and α∗ the two centers σY and σ ∗ their respective sizes. Valanis [1971] has proposed a new theory in which the present state of the material depends on the present values and the past history of observable variables. The theory is called endochronic and is expressed by z deP ρ(z − z ) dz , σ = 2G dz 0 where the yield surface is a derivable result of the theory. ρ(z) is a material function and z is the intrinsic time deﬁned by dz =

dζ , f (ζ)

where f (ζ) is the non-negative intrinsic time scale, with f (0) = 1 and ζ deﬁned by √ dζ = dεP dεP . Some other further developments will no more be cited. 1.11

Experimental Tests

Some authors have tested the yield surfaces in plasticity or the work-hardening surfaces. Thus Lode [1926] has tested the yield surfaces of Tresca and Mises. Some of his results are shown in Fig. 1.11.1. One can see that he found mostly the Mises yield condition to be satisﬁed. He has tried steel, copper and nickel, and he ﬁnd all to better satisfy the Mises condition. Also from the old results are to be mentioned the Taylor and Quinney [1931] results. They have tested copper, aluminum and mild steel. From their results we

Fig. 1.11.1

The Lode’s tests results.

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

36

Dynamic Plasticity

give here Fig. 1.11.2. As one can see according to Taylor and Quinney the Mises yield condition is in better agreement with the data, than the Tresca. From the old papers devoted to tests is also the paper of Roˇs and Eichinger [1929]. They have also compared the Tresca and Mises yield condition. Generally they ﬁnd the Mises yield condition in better agreement with experimental data. That is shown on Fig. 1.11.3 given below. From more recent papers in which the authors tried to compare the initial and subsequent yield surfaces in plasticity is the paper of Naghdi et al. [1958]. The initial surface is an ellipse, while the next ones, when only an shearing stress is applied, are deformed, trying to form an pointed corner at a thin walled tube (Fig. 1.11.4). Outer tests are reported by Phillips [1986]. Figure 1.11.5 is shoving some of his results, obtained at several temperatures shown. No lateral inﬂuence is shown but a signiﬁcant Bauschinger eﬀect is there. The surfaces are translated and deformed. The last authors are Williams and Svensson [1970] [1971]. In the ﬁrst paper they try to apply a tensile plastic strain to 1100-F aluminum. They found again a

Fig. 1.11.2

Experimental results of Taylor and Quinney [1931].

Fig. 1.11.3

Experiments of Roˇs and Eichinger [1929].

dynamic

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Yield Conditions

Fig. 1.11.4

The tests of Naghdi et al. [1958] for initial and subsequent yield loci.

Fig. 1.11.5

Second, third and fourth subsequent yield surfaces (Phillips [1986]).

dynamic

37

considerable Bauschinger eﬀect, but they found also a cross eﬀect. They found also corners in tension, as shown in Fig. 1.11.6. In another paper they apply a torsion plastic prestrain. This time they do not ﬁnd corners, but strong Bauschinger eﬀect is still there.

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

38

Dynamic Plasticity

Fig. 1.11.6

Comparison of initial and subsequent yield loci (Williams and Svensson [1970]).

Fig. 1.12.1

1.12

Tests done with various velocities.

Viscoplasticity

In all the constitutive equations of plasticity, they are time-independent. Thus several phenomena cannot be represented. For instance, if one is doing the same experiment with various speeds, one is obtaining distinct curves as a result (see Fig. 1.12.1). That cannot be described with a time-independent constitutive equation. Also, if we stop the test at a certain stress level, and we quip the stress constant, we observe a phenomena which is creep (Fig. 1.12.2). Also, if we quip the strain constant we observe that the stress relaxes. Any other behavior intermediate is possible. There are a number of materials which have such mechanical propriety which cannot be described: waxes, heavy oils, pastes, butter, creams, tooth pastes, etc. For such materials a new type of model was developed. It is called Bingham body.

dynamic

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

Yield Conditions

dynamic

39

σ creep

relaxation

ε 0 Fig. 1.12.2

Curves for creep or stress relaxation.

The assumptions for Bingham bodies are: Incompressibility, i.e., tr ε˙ = 0 . A viscoplastic function is deﬁned as g(σ ij ) :=

(1.12.1)

IIσ − k .

The constitutive equation is: 0 ε˙ij = 1 k √ 1 − σ˙ ij 2η IIσ

(1.12.2)

if IIσ ≤ k 2 if IIσ > k 2 .

(1.12.3)

Here k and η are two constants which characterize the model. They are absolute constants or relative constants, i.e., they may depend on the particle X. From (1.12.3) we get: σ = K + G ,

(1.12.4)

Gij = 2η ε˙ij

(1.12.5)

G is due to a Newtonian viscosity

with η a viscosity coeﬃcient. K is a plastic deviatory stress in the sense of Saint-Venant: f (K) : = IIK − k 2 ≤ 0 yield condition ε˙ij = 2λKij .

(1.12.6) (1.12.7)

We assume η > 0 and λ ≥ 0 with λ

= 0 if f (Kij ) < 0 > 0 if f (Kij ) = 0 .

(1.12.8)

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

40

dynamic

Dynamic Plasticity

II σ ′

overstress

II σ ′ = k 2

σ′

0 '

ε′ij

0

Rigid Viscoplastic

Fig. 1.12.3

The Bingham model.

From (1.12.7), (1.12.5) and (1.12.4) we get = (1 + 4ηλ)Kij σij

(1.12.9)

and for the invariants IIσ = (1 + 4ηλ)2 IIK .

(1.12.10)

If IIK < k 2 from these formulae follows λ = 0, and from (1.12.10) we have IIσ = IIK < k 2 . If IIK = k 2 from (1.12.8)2 and (1.12.10) follows √ IIσ 1 −1 > 0. (1.12.11) λ= 4η k From here we have IIσ > k 2 . Thus the constitutive equation is if IIσ < k 2 0 ε˙ij = 1 k 1− √ σ if IIσ > k 2 . 2η IIσ

(1.12.12)

The states IIσ = k 2 are not in the constitutive equation, so that strain rates for those states are not deﬁned. However, when IIσ k 2 , from (1.12.12) it follows. From here follows that if IIσ is increased the strain rate is also increasing. If IIσ is decreased, the strain rate is decreasing. If IIσ is decreased towards k 2 the strain rates decreases towards zero ε˙ij → 0. Thus we obtain the constitutive equation (1.12.3) (Fig. 1.12.3). If IIσ > k 2 from (1.12.12)2 we get 2 k (2η)2 IIε˙ = 1 − √ IIσ , IIσ

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Yield Conditions

and from here 2η

IIε˙ + k = IIσ .

dynamic

41

(1.12.13)

If IIσ < k 2 from (1.12.12)1 we have ε˙ij = 0 or IIε˙ = 0. (1.10.12) can be used to inverse the constitutive equation. We obtain √ undetermined with IIσ ≤ k for ε˙ij = 0 σij = (1.12.14) k ε˙ij for ε˙ij = 0 . 2η + √ IIε˙ Since in some of the problems one is giving the velocity (experimentally suggested) it is useful to get also the stress power. For ε˙ij = 0 from (1.10.14) we obtain ε˙ij = 2k IIε˙ + 4ηIIε˙ (1.12.15) σij and it is expressed in terms of kinematics variables only. Concerning the reference conﬁguration it is the actual one, since strain is not involved. If the model is used with variable k and η (nonhomogeneous) then the reference conﬁguration is the initial one. The generalization of this constitutive equation is presented in the next chapters. There are very many generalizations based on the concept of “overstress” due especially to Krempl and his collaborators (Krempl [1979]). For instance in the paper of Ho and Krempl [2000], the constitutive equation for small strain, for volume preserving inelastic deformation is 3 s−g 1+v 3 s−g 1+v s˙ + = s˙ + F [Γ] , e˙ = e˙ el + e˙ in = E 2 Ek[Γ] E 2 Γ where s and e are the deviator stress and strain tensors, respectively. The inelastic part of the ﬂow law can either be written using the decreasing, positive viscosity function k[Γ] with k[0] = 0 having the dimension of time, or in terms of the increasing, positive ﬂow function F [Γ] with F [0] = 0 having the dimension of 1/time. The overstress invariant is 3 tr ((s − g)(s − g)) Γ= 2 and g is the deviator of the equilibrium stress. The elastic volumetric relation augments the deviator law by 1 − 2v tr σ˙ . tr ε˙ = E The new growth law for the deviator state variable equilibrium stress g is s−g ψ[Γ] ˙ ψ[Γ] g−f s˙ + + 1− f. g˙ = − E p˙ E k[Γ] A + βΓ E For the deviator kinematics stress f we have ˆt s − g E f˙ = E k[Γ]

January 12, 2007

42

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

dynamic

Dynamic Plasticity

and ﬁnally a simple growth law for the secular isotropic stress is A˙ = Ac (Af − A)p˙ . The positive, decreasing shape function ψ[Γ] controls the transition from the initial quasi linear behavior to ﬁlly established ﬂow and is bounded by E > ψ[Γ] > Et where Et is the tangent modulus at the maximum strain of interest. It is related ˆt = Et (1 − (Et /E)). The ˆt by E to the tangent modulus based on inelastic strain E eﬀective inelastic strain rate is given by p˙ = Γ/(Ek[Γ]) = F [Γ]. The quantities Ac and Af are constants with no dimension and of the dimension of stress, respectively. Ac controls the speed with witch the ﬁnal value of A, i.e., Af , is reached. The model is slightly changed to describe various eﬀects, as: relaxation, the cyclic Swift eﬀect, the pre-necking and post-necking relaxation, creep, free-end torsion, rate-dependent deformation behavior of metals and solid polymers, high temperature applications, etc. 1.13

Rate Type Constitutive Equations

From now on, we will assume that always exists an instantaneous elastic response. It always exists for one-dimensional rate-type models, i.e., for any given state. If a jump in strain is produced, the stress also jumps and its jump is uniquely determined by the strain alone. For several components of stress it is no more so evident. We will assume however that the instantaneous response is path independent. From physical point of view one can accept this assumption, and from experimentally point of view one is not able to imagine tests which will contradict. The purpose of this section is (Suliciu [1989]), to examine the consistency of a simpliﬁed form of the instantaneous modules with the requirement of existence of instantaneous elastic response. The constitutive equation we deal with is of the form ˙ = ε(E, T)E ˙ + G(E, T, k) , T

ˆ k˙ = k(E, T, k) ,

(1.13.1)

where E and T are symmetric and objective strain and stress tensors conjugated with respect to the stress power w: w=

1 ˙ , T·E ρ0

(1.13.2)

where ρ0 is the mass density in the reference conﬁguration, and k is a isotropic workhardening parameter. T is the Cauchy stress tensor and E is the strain tensor. For a body modeled by constitutive equation (1.13.1), a process starting at a state (E0 , T0 , k0 ) ∈ D is a curve (E(t), T(t), k(t)) in D for t ∈ [0, t0 ), t0 ≥ 0 with E(0) = E0 , T(0) = T0 , k(0) = k0 which veriﬁes (1.13.1). One may term the set De from D where both G and kˆ vanish the equilibrium set of the model since a process starting at such a state, and generated by the

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Yield Conditions

dynamic

43

constant strain E(t) = E0 for all t ≥ 0 will be the constant process (E(t) = E0 , T(t) = T0 , k(t) = k0 ) for all t ≥ 0. Depending on the structure of the equilibrium set De we may classify the models described by the constitutive equation of the form (1.13.1) as viscoelastic or viscoplastic models. If the function G in (1.12.1) is independent of k and if there is a function of strain TR (E) for E in some strain domain DE ⊂ S such that (E, TR (E)) ∈ D for all E ∈ DE and G(E, T) = 0 if and only if T = TR (E) then the model may be called viscoelastic (the evolution equation for k may be disregarded). In other terms, the model is called viscoelastic if the equilibrium state of stress is determined by the state of strain alone. The model (1.13.1) may be called viscoplastic if the equilibrium set De contains an open set in D and De ⊂ D is a strict inclusion. The inﬂuence of the temperature in one-dimensional stress–strain curves are described by many authors. For stainless steel it is given in Xue et al. [2004] which wave used an explosion technique to study the thick-walled cylinder under highstrain deformation of ∼ 104 s−1 . The shear-band initiation and propagation were examined. Several grain size were considered. 1.14

General Principles

For the general principles, see Malvern [1969], Mase and Mase [1999] and Fung and Tong [2001]. Let us consider a volume V bounded by a ﬁxed surface S. Conservation of Mass. ! The mass is M = V ρ dV . The rate of increase of mass is (Fig. 1.14.1): ∂ρ ∂M = dV (1.14.1) ∂t V ∂t if no mass is created or destroyed inside. That ! ! must be equal to ! the rate of inﬂow ˆ dS = − V ∆ · (ρv) dV , the trough the surface which is S −ρvn dS = − S ρv · n last one is coming from the divergence theorem. Combining with (1.14.1) we have ∂ρ + ∆ · (ρv) dV = 0 . ∂t V Thus must be true for arbitrary V , thus ∂ρ + ∆ · (ρv) = 0 ∂t or, in rectangular Cartesian coordinates ∂ρ ∂(ρvi ) + = 0. ∂t ∂xi Since ∂ρ ∂vi ∂(ρvi ) = vi + ρ , ∂xi ∂xi ∂xi

(1.14.2)

(1.14.2a)

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

44

dynamic

Dynamic Plasticity

nˆ

v

P V dS

S

Fig. 1.14.1

The reference volume in space.

and from the material derivative ∂ρ ∂ρ dρ = + vi , dt ∂t ∂xi the above law is dρ ∂vi +ρ =0 dt ∂xi

(1.14.3)

or in vector form dρ + ρ div v = 0 . (1.14.3a) dt That is the continuity equation due to Euler in 1757. If the density of all the particles is constant, then div v = 0 ,

(1.14.4)

which is the condition of incompressibility. The continuity condition can be written in material form. If V is the volume of material at time t, and V0 the volume at the same material at time t0 , we have (Fig. 1.14.2) ρ(X, t0 ) dV0 = ρ(x, t) dV = ρ(x(X, t), t)|J| dV0 V0

V

V0

with |J| the absolute value of the Jacobian determinant " " ∂x ∂x " " ∂x " " " ∂X ∂Y ∂Z "" " " " ∂y ∂y " " ∂y J ≡" ". " ∂X ∂Y ∂Z "" " " " ∂z ∂z " " ∂z " " ∂X ∂Y ∂Z

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

Yield Conditions

dynamic

45

x = χ ( X , t ).

m0 V0

m

R

V

Fig. 1.14.2

The material form of continuity condition.

ρbdV

dV

tdS

V dS

S Fig. 1.14.3

The momentum balance.

! We have from conservation of mass V0 [ρ0 − ρ|J|] dV0 = 0. But for arbitrary volume V0 we have ρ|J| = ρ0 , and since at t = t0 we have no empty spaces, ρ = ρ0 > 0 it follows J = 1 and therefore J > 0 for t > t0 . Therefore we have ρJ = ρ0 .

(1.14.5)

This is also due to Euler in 1762. Equation of Motion. Let us consider a body V (see Fig. 1.14.3), which is a closed thermodynamic system, which is not exchanging matter. We postulate that d t dS + ρb dV = ρv dV , dt V S V

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

46

dynamic

Dynamic Plasticity

! ˆ · T, where (d/dt) is the material derivative of the integral. If we replace here t = n we have in Cartesian coordinates d Tji nj dS + ρbi dV = ρvi dV . dt v S V Using the divergence theorem to pass to a volume integral, and since ρ dV = const ., we can write dvi ∂Tji dV = 0 . + ρbi − ρ ∂xj dt V For an arbitrary V , ∂Tji dvi , + ρbi = ρ ∂xj dt

(1.14.6)

which are the equations of motion of Cauchy’s. In vector form, they can be written ∆ · T + ρb = ρ

dv dt

(1.14.6a)

independent of the system of coordinates. For the equilibrium problems we have ∆ · T + ρb = 0. Moment of Momentum Principle. The total moment of momentum is

(r × t) dS + S

(r × ρb) dV = V

d dt

(r × ρv) dV V

and in Cartesian components d ermn xm tn dS + ermn xm bn ρ dV = ermn xm vn ρ dV . dt V S V Here we take care that tn = Tjn nj , we use the divergence theorem

xm Tjn nj dS = S

V

∂(xm Tjn ) dV , ∂xj

and ρ dV = const., to obtain d(xm vn ) ∂(xm Tjn ) ρ dV . ermn + xm bn ρ dV = ermn ∂xj dt V V If we develop the derivatives ∂Tjn dvn dxm vn + xm dV . ermn xm + δmj Tjn + ρxm bn dV = ermn ∂xj dt dt V V

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

Yield Conditions

dynamic

47

Grouping now the terms we have dvn ∂Tjn + δmj Tjn dV = ermn xm + ρbn − ermn vm vn dV . ∂xj dt V V We ! take into account that ermn vm vn = 0 since vm vn is symmetric in mn, so that e T dV = 0, or of any V , ermn Tmn = 0. Thus for r = 1 we have T23 − T32 = V rmn mn 0, and so on. Thus the stress tensor is symmetric. Energy Balance. We chose again a closed thermodynamic system not exchanging mater with the surroundings. The work is on the system, not by the system. Power input is t · v dS + ρb · v dV . Pinput = S

In Cartesian coordinates

V

Pinput =

Tji nj vi dS +

S

ρbi vi dV V

∂vi ∂Tji vi dV = + ρbi + Tji ∂xj ∂xj V dvi = + Tji [Dij + Wij ] dV vi ρ dt V 1 d (vi vi ) ρ dV + = Tji Dij dV dt V 2 V d 1 = Tij Dij dV . ρvi vi dV + dt V 2 V In vector form we have Pinput =

d dt

V

1 ρv · v dV + T : D dV . 2 V

Thus the rate of work which is the power input is equal to the variation of the kinetic energy plus the total stress power. The heat input rate is ˆ dS + ρr dV , Qinput = − q · n S

V

where the ﬁrst integral is the heat ﬂux through the surface of contact S (q is the heat ﬂux vector), while the second is the distributed internal heat source of strength r per unit mass. The total energy E is E˙ total = K˙ + U˙ = Pinput + Qinput ,

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

48

dynamic

Dynamic Plasticity

where K is the kinetic energy and U the internal energy (elastic stored energy, and all other nonspeciﬁed energies). Thus we have dK d dK + + ρu dV = T : D dV dt dt V dt V ˆ dS + ρr dV . + − q·n S

V

Simplifying and transforming the surface integral in a volume integral, we have for arbitrary V in vector form and coordinate form: ρ

du = T : D + ρr − ∆ · q , dt

(1.14.7) du ρ = Tij Dij + ρr − qj,j , dt which is the energy equation due to Kirchhoﬀ in 1894. Here ρ du/dt is the rate of increase of the internal energy ρu per unit volume, ρr is the internal supply of heat per unit volume, and −qi,i the inﬂow per unit volume of heat through the boundaries of the element. In elasticity the heat transfer is insigniﬁcant. But in plasticity we have a heating due to the plastic deformation, a heating at the tectonic plates, volcanoes, etc. The Second Law of Thermodynamics. If we introduce the Piola–Kirchhoﬀ stress tensor 1 ˜ S = ρ−1 T(FT )−1 = S , (1.14.8) ρ0 the energy balance can be written ρe˙ − ρSij F˙ij +

∂qi = ρr . ∂xi

(1.14.9)

The entropy rate γ is deﬁned as ρr q + div , (1.14.10) θ θ where η = η(X, t) is the entropy per unit mass while θ = θ(X, t) > 0 is the absolute temperature. The second law of thermodynamics, or the Clausius–Duhem inequality (not used here), states that (Truesdell and Toupin [1960]) ργ = ρη˙ −

γ ≥ 0.

(1.14.11)

From (1.14.9), (1.14.10) and (1.14.11) follows γ = η˙ −

e˙ 1 ∂θ + θ−1 Sij F˙ij − 2 qi ≥ 0. θ ρθ ∂xi

If one introduces the free energy ψ = e − θη ,

(1.14.12)

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Yield Conditions

dynamic

49

then (1.14.12) can be expressed as θγ = −ψ˙ − η θ˙ + Sij F˙ij −

1 ∂θ qi ≥ 0. ρθ ∂xi

(1.14.13)

˜ given by (1.14.8), we can write the balance equations in initial Using the tensor S coordinates ρ0

∂vi ∂ S˜ij − = ρ0 b i , ∂t ∂Xj

(1.14.14)

∂ q˜i ∂e ∂Fij − S˜ij + ρ0 = ρ0 r , ∂t ∂t ∂Xi ˜ = JF−1 q (see Green and Rivlin [1964a,b]). with q A regular surface Σ with equation ϕ(X, t) = 0, is called an acceleration wave through the body if ϕ is continuous and their derivatives may have jump discontinuities across Σ, while being continuous at all points. The quantities U =−

∂ϕ/∂t , |Grad ϕ|

ni =

∂ϕ/∂Xi , |Grad ϕ|

(1.14.15)

are called the propagation speed and the direction of propagation of the acceleration wave, respectively. ˜ ψ, . . . cannot be independent; they have The jumps of the derivatives of v, F, θ, S, to satisfy three types of conditions. The geometric and kinematics compatibility conditions give those relations between the jumps of ∂v/∂t, ∂v/∂X, etc., that are due to the continuity of v or follow from the fact that v and F are the partial derivatives of the same vector function χ. These compatibility conditions can be written as ∂Fkl ∂Fkl ∂vk ∂vk = U 2 ak , = −U ak nl , = ak n l n j , = ∂t ∂Xj ∂Xl ∂t ∂θ ∂θ = −U v , = vnj , (1.14.16) ∂t ∂Xj # $ $ # ∂ S˜ij ∂ S˜ij = −U sij , = sij nk , etc. ∂t ∂Xk Here [f ] = f + − f − , f + being the limit value of f at a point on the surface Σ, reached from the positive side of the normal (n, −U ) to Σ at that point, and f − being the limit value of f at the same point but reached from the other side of the surface. The vector a = (a1 , a2 , a3 ) is called the mechanical amplitude of the wave, the scalar v is called the thermal amplitude of the wave and sij may be called the stress amplitude, etc.

January 12, 2007

10:41

50

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Dynamic Plasticity

The second group of restrictions imposed on the jumps comes from the balance equations. They are called dynamic compatibility equations and they are obtained from (1.14.14) as follows: one considers (1.14.14) on each side of the surface Σ and then, after taking limit values at a point on Σ, one calculates the diﬀerence between the two obtained relations. Since b and r are assumed continuous, one obtains the following homogeneous dynamic compatibility conditions. # ˜ $ ∂ Sij ∂vi − = 0, ρ0 ∂t ∂Xj (1.14.17) ∂ q ˜ ∂e ∂F ij j − S˜ij + = 0. ρ0 ∂t ∂t ∂Xj The third group of restrictions is imposed by the constitutive equations, i.e., ˜ η, ψ and q. These restricthose relations that must exist between F, θ, Grad θ, S, tions will be discussed in the other chapters. In case of an isolated discontinuity surface, the geometric-kinematic and dynamic compatibility conditions have been presented for the ﬁrst time by Hadamard [1903] for the general three-dimensional case. Bibliography Bruhns O. T., Xiao H. and Meyers A., 2005, A weakened form of Ilyushin’s postulate and the structure of self-consistent Eulerian ﬁnite elastoplasticity, Int. J. Plasticity 21, 199–219. Dafalias Y. F. and Popov E. P., 1976, Plastic internal variables formalism of cyclic plasticity, J. Appl. Mech. 43, 645–651. Drucker D. C., 1951, A more fundamental approach to plastic stress–strain relations, Proc. 1st U.S. Natl. Cogr. Appl. Mech., 487–491. Fung Y. C. and Tong P., 2001, Classical and Computational Solid Mechanics, World Scientiﬁc, 930 pp. Green A. E. and Rivlin R. S., 1964a, Simple force and stress multipoles, Arch. Rational Mech. Anal. 16, 5, 325–353. Green A. E. and Rivlin R. S., 1964b, Multipolar continuum mechanics, Arch. Rational Mech. Anal. 17, 2, 113–147. Hadamard J., 1903, Le¸cons sur la Propagation des Ondes et les Equations de l’Hydrodynamique, Herman, Paris. Hencky H., 1924, Zur Theorie plastischer Deformationen und der hierdurch hervorgerufenen Nachspannungen, Zeits. Angew. Math. U. Mech. 4, 323–334. Ho K. and Krempl E., 2000, Modeling of positive, negative and zero rate sensitivity by using the viscoplasticity theory based on overstress (VBO), Mech. Time-Dep. Materials 4, 21–42. Iliushin A. A., 1961, On the postulate of plasticity, Prikl. Mat. Mech. 25, 503. Koiter W. T., 1953, Stress–strain relations, uniqueness and variational theorems for elastic, plastic materials with a singular yield surface, Q. Appl. Math. 11, 350–354. Krempl E., 1979, Viscoplasticity based on total strain: The modeling of creep with special considerations of initial strain and aging, J. Eng. Mat. Tech. 101, 380–386.

dynamic

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Yield Conditions

dynamic

51

Lode W., 1926, Versuche uber den Einﬂuss der mittleren Hauptspannung auf das Fliessen der Metalle Eisen, Kupfer, und Nickel, Z. Physik 36, 913–939. Malvern L. E., 1969, Introduction to the Mechanics of a Continuous Medium, PrenticeHall, Inc., 713 pp. Mase G. Th. and Mase G. E., 1999, Continuum Mechanics for Engineers, CRC Press, 377 pp. Mises R. von, 1913, Mechanik der festen K¨ orper in plastisch deformable Zustand, Nachr. Akad. Wiss. G¨ ottingen Math.-Phis. K1 H.4, 582–592. Mr´ oz Z., 1969, An attempt to describe behaviour of metals under cyclic loads using a more general workhardening model, Acta. Mech. 7, 199–212. Nadai A., 1923, Der Beginn des Fliessvorganges in einem tortierten Stab, Zeits. Angew. Math. Mech. 3, 442–456. Naghdi P. M., Essenburg F. and Koﬀ. W., 1958, An experimental study of initial and subsequent yield surfaces in plasticity, J. Appl. Mech. 25, 201–209. Phillips A., 1986, A review of quasistatic experimental plasticity and viscoplasticity, Int. J. Plasticity 2, 315–328. Prager W., 1959, An Introduction to Plasticity, Addison-Westley Publishing Co. Prandtl L., 1924, Spannungsgsverteilung in plastischen Koerpern, Proc. 1st Int. Congr. Appl. Mech. (Delft), 43–54. Reuss E., 1930, Beruecksichtigung der elastischen Formaenderungen in der Plasizitaets theorie, Zeits. Angew. Math. U. Mech. 10, 266–274. Ros M. and Eichinger A., 1926, Proc. 2nd Int. Congr. Appl. Mech. (Z¨ urich), 315. Ros M. and Eichinger A., 1929, Metalle Diskussionsbericht No. 34 der Eidgenossen Materialprufungsanstalt, Zurich, 315. Saint-Venant, Barr´e de., 1870, M´emoire sur l’´etablissement des ´equations diﬀ´erentielles des mouvements int´erieure op´er´es das les corps solides ductiles au del` a des limite o` u l’´elasticit´e pourrait les ramener ` a leur premier ´etat, C. R. Ac. Sci. (Paris) 70, 473–480. Stoughton T. B. and Yon J. W., 2005, Review of Drucker’s postulate and the issue of plastic stability in metal forming, Int. J. Plasticity (in print). Suliciu I., 1989, Some remarks on the instantaneous response in rate-type viscoplasticity, Int. J. Plasticity 5, 173–181. Taylor G. I. and Quinney H., 1931, The plastic distortion of metals, Philos. Trans. Roy. Sos. London A 230, 323–362. Tresca H., 1868, Memoire sur l’ecoulment des corps solides, M´em. Sav. Acad. Sci. Paris, 733–799. Truesdell C. and Toupin E. R., 1960, The Classical Field Theories, Handbuch der Physik, Vol. III/1, Springer Verlag, Berlin. Valanis K. C., 1980, Fundamental consequences of a new intrinsic time measure plasticity as a limit of the endoshronic theory, Arch. Mech. 32, 171. Williams J. F. and Svensson N. L., 1970, Eﬀect of tensile prestrain on the yield locus of 1100-F Aluminium, J. Strain Analysis 5, 2, 128–139. Williams J. F. and Svensson N. L., 1971, Eﬀect of torsional prestrain on the yield locus of 1100-F Aluminium, J. Strain Analysis 6, 4, 263–272. Xue Q., Meyers M. A. and Nesterenco V. F., 2004, Self organization of shear bands in stainless steel, Mater. Sci. Eng. A 384, 35–46.

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

This page intentionally left blank

dynamic

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

dynamic

Chapter 2

Rocks and Soils

2.1

Introduction

The constitutive equation for rocks or soils is much more complicated. The reason is that the experimental results are much more involved. Even the elastic constants are no more what they were for metals, and the methods of ﬁnding them from tests are diﬀerent from what we know from metals. The yield conditions are diﬀerent. While for metals a cylindrical constitutive yield condition, independent of the mean stress is quite normal, such a yield condition for rocks is not acceptable. One has tried to introduce a yield condition depending also on mean stress and on the third deviator stresses F (Iσ , IIσ , θ) = 0 , where θ=

√ 3 3IIIσ 1 sin−1 3 3 2 IIσ

is the Lode angle. The most familiar are the Mohr–Coulomb and Drucker–Prager yield conditions. The ﬁrst condition is written τ = c − σ tan φ with 1√ σc σt c= 2

−1

and φ = sin

σc − σt σc + σt

with 0 ≤ φ

0, σ > 0. We write the displacement on one side and another side and because this displacement is the same (du)− = v − dt + ε− dx (du)+ = v + dt + ε+ dx or [v] = −c[ε] .

(3.5.2)

This is the kinematics condition. c X1

X2

+

ε + [ε ] v + [v ] Fig. 3.5.4

− Y (t )

ε v

Formation of shock waves.

→x

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

138

dynamic

Dynamic Plasticity

We write now the balance of linear momentum. We have d Y (t) d X2 ρv(X, t) dX + ρv(X, t) dX dt X1 dt Y (t)

X2

=

ρb(X, t) dX + σ(X2 , t) − σ(X1 , t)

X1

or making the derivatives Y (t) X2 ∂v(X, t) ∂v(X, t) dX − ρv − (Y (t), t)Y˙ (t) + dX ρ ρ ρv + (Y (t), t)Y˙ (t) + ∂t ∂t Y (t) X1

X2

=

ρb(X, t) dX + σ(X2 , t) − σ(X1 , t) .

X1

We introduce new notations when X1 → Y (t), X2 → Y (t) and v + (Y (t), t) = lim v(X, t) X → Y (t) X < Y (t) and the velocity of propagation c = Y˙ (t). With these notations we obtain cρ[v] = −[σ] which is the dynamic jump condition. We obtain also from here 1 [σ] c= ρ [ε]

(3.5.3)

(3.5.4)

for the velocity of propagation. It is certainly not independent and does not coincide with the velocity of the acceleration waves. We have a total of four unknown functions σ, ε, v, c but we have only three equations. Another condition is obtained from boundary conditions or some other condition which may result from the problem. This is a very simple theory, which replaces the diﬀerential relations with algebraic linear equations. It allows an elementary study of the interaction between elastic (loading and unloading) and plastic waves. It also allows a very simple description of reﬂection and refraction of waves. Reﬂection of waves. When waves are reﬂected from the end of the bar, many situations may arise, depending on whether the end of the bar is free, ﬁxed, or whether the bar continues with another bar, with diﬀerent material proprieties. If an impact is produced at one end x = −l of the bar, the ﬁrst wave to reach the other end x = 0 is always an elastic wave and σ = −ρc0 v. The displacement due to this elastic wave is u1 = f1 (c0 t − x) ,

(3.5.5)

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

The Propagation of Longitudinal Stress Waves

dynamic

139

where f1 is an arbitrary function to be determined by the initial conditions. The corresponding stress is σ1 = E(∂u1 /∂x) = −ρc0 (∂u1 /∂t)

(3.5.6)

for the inverse waves (propagating in the opposite direction) u2 = f2 (c0 t + x) ,

(3.5.7)

σ2 = E(∂u2 /∂x) = ρc0 (∂u2 /∂t) .

(3.5.8)

and

Let us consider the case when the end x = 0 of the bar is free. After the reﬂection of the elastic wave, the total stress will be σ = σ1 + σ2 = E{f2 (c0 t + x) − f1 (c0 t − x)} .

(3.5.9)

But at the end x = 0 the stress vanishes for all t f2 (c0 t) − f1 (c0 t) = 0 .

(3.5.10)

One can therefore conclude that f1 (z) = f2 (z) = f (z), and the displacement after reﬂection will be u = u1 + u2 = 2f (c0 t) .

(3.5.11)

Furthermore, due to reﬂection at the free end the displacement produced by the wave is doubled, as is also the velocity. With regard to stress, we have in this case σ1 = −σ2 , i.e., a compressive wave is reﬂected as a tensile one and vice versa. If we now assume that the second end of the bar is ﬁxed rigid, then the displacement of this end is zero for all t f1 (c0 t) + f2 (c0 t) = 0 , and therefore f1 (z) = −f2 (z), i.e., the displacement produced by the reﬂected wave is equal to that produced by the incident wave, but in the reverse direction. This stress σ = σ1 + σ2 = 2Ef2 (c0 t)

(3.5.12)

is doubled due to reﬂection from the ﬁxed end. For this reason, an elastic wave can be reﬂected a plastic one, if on reﬂection, the stress carried by the reﬂected wave exceeds the yield stress. If the bar is continued with another one, possessing diﬀerent mechanical properties the situation is more complicated: a reﬂected wave of intermediate intensity will propagate from the end of the bar, but at the same time a wave will also be reﬂected in the other medium (see Kolsky [1953]). The previous arguments are generally also valid for plastic waves. The ﬁnite bar. Many authors have considered the problem of normal impact of a ﬁnite bar against a rigid target. Let us examine the problem as done by Lenski [1949]. A bar of length l moves with velocity V from right to left (Fig. 3.5.4).

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

140

dynamic

Dynamic Plasticity

−εY

−ε

0

−σ Y −σ Fig. 3.5.5

Elastic linearly work-hardening plastic bar striking a rigid target.

x=

c1 t

t

x=

c 0t

σ =0 0

x Fig. 3.5.6

The ﬁrst waves to propagate in the bar.

At time t = 0 the bar strikes a rigid wall x = 0. It is assumed that the impact velocity is suﬃciently high to produce elastic-plastic strains and that the material of the bar is linear work-hardening. Due to the sudden impact and linear workhardening only shock waves are considered. Thus, after impact two shock waves, one elastic and one plastic will propagate. Their wave fronts delimitate three distinct regions in the bar. In the ﬁrst region (Fig. 3.5.6) ε0 = 0, v0 = −V , in the second region ε1 = −εY , σ1 = −EεY and v1 = −V + c0 εY . In the third region v2 = 0 and ε2 = (1/c1 )(c0 εY − V ) − εY ,

σ2 = (E1 − E)εY + E1 ε2 .

(3.5.13)

Therefore, for the plastic strains to appear, the velocity of impact must satisfy the condition V > c0 εY . After the time t = l/c0 the elastic wave front is reﬂected from the free end. Behind this front σ3 = ε3 = 0 ,

v3 = 2c0 εY − V .

(3.5.14)

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

dynamic

The Propagation of Longitudinal Stress Waves

141

σ t

ε2

4′′

ε 4′′

ε 4′

ε σ4

4′ 3

2 1

0

S Fig. 3.5.7

σ2

l

x

Stresses and strains during unloading after the ﬁrst reﬂexion.

When the wave fronts of the plastic and of the elastic unloading waves meet at the section S (Fig. 3.5.7) several situations are possible, depending on the magnitude of the velocity V . Let us consider ﬁrst the case when, after the two wave fronts have met, the plastic wave does not propagate any more. In this case the elastic waves will spread in both directions from S (Fig. 3.5.10). The leftward wave is always an elastic one. On both sides of the section S the particle velocities are equal to v4 = v4 , otherwise the bar will break. From the balance of the force it also follows that, σ4 = σ4 (the stresses are initial stresses). The strains in the two regions will be diﬀerent. In the region 4 the material is in an elastic state, the yield point was never reached, while in the region 4 the material is also in an elastic state, but is being unloaded after a plastic deformation. This situation is shown in Fig. 3.5.7. Thus the stress–strain relation that acts on the two sides of the section S is σ = Eε

and σ = σ2 + E(ε − ε2 ) . σ4

σ4 ,

v4

(3.5.15)

v4

From these relations and the conditions = = and the jump conditions, we obtain c 0 + c1 2c2 + c0 c1 − c21 ε4 = (c0 εY − V ) , ε4 = 0 (c0 εY − V ) , 2 2c0 2c20 c1 3c0 − c1 (c0 εY − V ) + V . 2c0 Thus the strain is discontinuous across the section S. This is a non-propagable discontinuity surface. If the plastic wave stops at S (Fig. 3.5.10), the strain for x > xS must be bigger than the strain corresponding to the yield stress ε4 > −εY . From this condition it follows that 2c0 ε Y c0 . V < 1+ c 0 + c1 v4 = v4 =

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

142

dynamic

Dynamic Plasticity

σ

t

ε2

ε5 σ5

5 4′′

ε

4′ 3

2 1 0 0

S Fig. 3.5.8

l

x

Possible separation from the wall at the ﬁrst reﬂection.

If we have also v4 = v4 > 0 when the elastic wave propagating to the left reaches the end of the bar, this end can possibly be pulled away from the wall (Fig. 3.5.8). If the separation takes place σ5 = 0 and c20 − c21 (c0 εY − V ) , v5 = 2c0 εY − V , c20 c1 where εP is the plastic strain. The plastic strain is constant in the part of the bar to the left of section S, whose length is ε5 = −εP =

xS = 2c1 l/(c0 + c1 ) . From here we obtain also the separation condition V < 2c0 εY . The time during which the bar is in contact with the wall is 2l/c0. After the separation the bar will have a sudden change of diameter. If the inequality 2c0 c0 ε Y 2c0 εY < V < 1 + c 0 + c1 is satisﬁed, then the elastic waves will again propagate from S in both directions, but the bar will continue to touch the wall for a little longer: 4l/(c0 + c1 ). Now the elastic wave propagating to the right is reﬂected and when it arrives at the impact end separation takes place. If ﬁnally the inequality 2c0 c0 ε Y V > 1+ c 0 + c1 holds, then ε4 < −εY and the plastic wave continues to propagate to the right from the section S (Fig. 3.5.10). There are two possibilities. Either the elastic wave which

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

dynamic

The Propagation of Longitudinal Stress Waves

143

σ ε2 ε6

t S1

S

σ3 E

C B

6 2

5

ε 4 = −ε Y

D

4

•

•

ε

σ 4 = −σ Y σ5 =σ6

A

σ2 1 0 x

Fig. 3.5.9

Characteristic ﬁeld for the case when two stationary discontinuities occur.

propagates to the left from S is reﬂected from the end x = 0 and then meets the plastic wave at S1 , which in the meantime continues to propagate. Or the elastic wave which propagates from S to the right and is reﬂected from the end x = l meets the plastic wave ﬁrst. That depends on the velocities of propagation of the elastic and plastic waves. In Fig. 3.5.9 the ﬁrst of these two possible cases is represented, when c0 /c1 > 4.236. Now the length of the plastically deformed portion of the bar, the abscissa of the section S1 , is xS1 = 2lc1 /(c0 + c1 ) . The magnitudes of the strain and velocity in regions 1, 2 and 3 coincide with those given in the previous example. In region 4, since ε = −εY , it follows that v4 = 3c0 εY − V . The stresses in regions 5 and 6 are equal and satisfy the relations: σ5 + σY = E(ε5 + εY ) and σ6 − σ2 = E(ε6 − ε2 ) . Using the momentum equation for shock waves together with the condition v6 = v5 and the previous relation we obtain (Fig. 3.5.10) ε5 =

3c20 − c21 V εY − , c1 (c0 + c1 ) c1 v5 = v6 =

ε6 =

c21 + c20 V εY − , c1 (c0 + c1 ) c1

2c0 c1 εY . c 0 + c1

Finally the bar will possess two stationary discontinuity fronts. If necessary the analysis can be continued in a similar way for greater impact velocities. Many such kinds of problems, described only by shock waves, can be found in the papers by De Juhasz [1949a], [1949b] and in the book by Rakhmatulin and Demianov [1961].

January 12, 2007

10:41

144

Dynamic Plasticity

Fig. 3.5.10

3.6

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Elastic linearly work-hardening plastic bar striking a rigid target.

Examples

The examples given are the impact of two identical aluminum 1100 bars (Cristescu and Bell [1970], Cristescu [1970]). The bars are 25 cm in length and one inch in diameter. The experimental results are due to J. F. Bell published in several papers and the books by Bell [1968, 1973]. Numerical integration method. The constitutive equation is written σ = F (ε) or in an inverse ε = F −1 (σ). F is a strictly increasing function. We consider σ and ε positive in compression. The density is ρ = 0.002757 g cm−4 sec2 . The plastic deformation is εP = F −1 (σ) − σ/E. The characteristics are

dynamic

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

The Propagation of Longitudinal Stress Waves

dynamic

145

dx = ±c = ± dt

E ρ(1 + Eϕ)

(3.6.1)

and dσ = ∓ρcdv .

(3.6.2)

The diﬀerential relations along the characteristics are: dx = 0 (twice)

(3.6.3)

and dεP = ϕdσ

(3.6.4)

EdεE = dσ . The constitutive equation is written as σ˙ 1 σ˙ −1 + χ (F (σ)) − σ˙ = + ϕ(σ)σ˙ ε˙ = E E E and χ=

1

if σ = σm (x)

0

if σ ≤ σY or σY < σ < σm (x) .

(3.6.5)

We introduce the dimensionless variables v kx σ , T = kt , X = . S= , V = E c0 c0 Now we choose the highest value of dx/dt in the whole ﬁeld, i.e., dx/dt = ±c0 or dX/dT = ±1 the bar velocity, with c0 = 5080 m/sec. The principle of the method is an integration along characteristic lines. We will not give details. The method is convergent since the monotone bounded sequence F (ε) < c(i) (σ, ε) ≤ c(i−1) (σ, ε) ≤ · · · ≤ c0 ρ is always satisﬁed. It is very rapid, since we do 2-3 iterations in one point. Initial and boundary conditions. The initial conditions are for the specimen (S): & t=0 :σ=ε=v=0 0≤x≤l and for the hitter (H): t=0

&

−l ≤ x ≤ 0

: σ = ε = 0,

v=V .

The boundary conditions are, if v(0, t) is prescribed: x = l,

t ≥ 0 : σ = 0,

x = −l ,

t ≥ 0 : σ = 0,

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

146

dynamic

Dynamic Plasticity

2l V 0 ≤ t ≤ t∗ = : vH = vS = vmax = c0 2 x=0

t∗ ≤ t < Tc : vH = −vS

or σH = σS = σmax ,

symmetry of motion ,

Tc ≤ t : σS = 0 .

Here Tc is the time of contact between the two bars. The boundary conditions can be prescribed for σ(0, t) if the stress is measured in a hard transmitter bar or with a piezocrystal, and v = −ϕ(σ). The initial conditions are formulated to make economy of computer time and to avoid the singular point O. The ﬁrst initial conditions are named S from shock. An initial shock wave is propagating and reﬂecting from the free end (see Fig. 3.6.1). Thus AR is a tensile unloading shock wave. For a constitutive equation of the form σ = βε1/2 we have along this line: 1 β2 ∗ t. x = −c0 (t − t ) and x = c(σ)t = ρ 2σ From here we get: t2 β2 2 ∗ 2ρc0 (t − t)2 2 3/2 2√ 2 1 2 σ vb (t) = + − σY σY 3β ρ ρc0 3β ρ

σb (t) =

(i)

where “b” stands for “before”. We now use the jump condition to pass at “after” the shock.

t

Tc t

V max

M A

V ! VY

V

0 , t

V max VY

0

Fig. 3.6.1

xM

xA

The initial condition S.

R

VY

l

x

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

dynamic

The Propagation of Longitudinal Stress Waves

147

We have: jump condition : σa − σb = −ρc0 (va − vb ) , after : −σa + ρc0 va = const. , in R : σb = σY = ρc0 vb , σa = 0 . From here we get: 1 σa − σb = − {2σY − (ρc0 vb − σb )} , 2 va = vb −

1 (σa − σb ) , ρc0

(ii)

σa P , εP a = εb . E Though along the line x = −c0 (t − t∗ ) for the data “after” we have: 0 ≤ x ≤ xM : σ = σmax = const. εE a =

xM ≤ x < xA : (i) , xA ≤ x ≤ l : (ii) . These are the initial data along the reﬂected shock wave. We have tested also a second type of initial data called L (linear). There are no shocks now and we have the boundary conditions: t 0 ≤ t ≤ tm = 20 µ sec : σ = σmax , tm x=0 tm ≤ t < Tc : vH = vS , Tc ≤ t : σS = 0 .

Tc

t

σm

ax

t*

σY

tm ty

σ (0, t )

σ max σ Y

σ=

0

x

0

Fig. 3.6.2

l The initial boundary conditions L.

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

148

dynamic

Dynamic Plasticity

Tc t A

V ! VY tm

V (o,t) V max V

0

Fig. 3.6.3

R

σ = σY xA

x

l

x

The initial data of a mixed type M.

Now we get along the line:

∗

x = −c0 (t − t )

and x =

1 β2 ρ 2σ

tm t− σ . σm

From here:

√ √ − 2ρc0 (t∗ − t) + 2ρc20 (t∗ − t)2 + 4β 2 (tm /σmax )t (i) σb = 2β(tm /σmax ) and a similar formula for vb . A mixed initial condition called M (mixed) has also been considered. It is a one dimensional simulation of the three dimensional wave initiations at the end of the bar: a sudden shock up to σ ¯ = 0.794σmax after which follows a linear variation up to σmax reached at tm = 40 µ sec. Thus t ¯+ (σm − σ ¯) , 0 ≤ t ≤ tm = 40 µ sec : σ = σ tm x=0 tm ≤ t < Tc : vH = vS , Tc ≤ t : σS = 0 . We have to ﬁnd x ¯ from

x=

1 β2 t and x = c0 (t∗ − t) . ρ 2¯ σ

We obtain x ¯=

c0 t∗ √ , 1 + c0 2ρ¯ σ /β

from where x ¯ = 2.64D < xA for V = 40 m/sec.

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

The Propagation of Longitudinal Stress Waves

For

dynamic

149

∗ x = c0 (t − t) 0≤x≤x ¯: 1 β2 x = ρ 2¯ σ

we have: √ √ σb = σa √ ¯ )[t − σ ¯ tm /(σmax − σ ¯ )]} −c0 2ρ(t∗ − t) + 2ρc20 (t∗ − t)2 + {4β 2 tm /(σmax − σ = 2βtm /(σmax − σ ¯) and a similar formula for va . In the interval where the reﬂected wave is still felt: x ¯ ≤ x ≤ l : σb =

t2 β2 2ρc20 (t∗ − t)2

if

σb > σa → (ii) ⇒ σa σb ≤ σa → (i) ⇒ σa .

Concerning the constitutive equation we have used three. First was used the dynamic curve σ = Eε ,

σ = σY 1 = 307.5 psi

σ = βε1/2 ,

σ ≥ σY 1 .

with β = 5.6 × 104 psi , E = 10.2 × 106 psi , c0 = 5080 m/sec , εY 1 = 0.00003014 . That was the fundamental constitutive equation. Since the yield stress was not correct, we have translated the parabola to get the correct yield stress. Thus σ = Eε ,

σ ≤ σY 2 = 1100 psi

σ = β(ε + ε0 )1/2 ,

σ ≥ σY 2

and εY 2 = 0.00010784, and ε0 = 0.0002779988 (the translation on horizontal). The quasi-static stress–strain curve is σ = 3.32 × 104 ε3/8 from where: σ = Eε ,

σ ≤ σY 0 = 1068.24 psi

σ = 3.32 × 104 ε3/8 ,

σ ≥ σY 0 .

In the examples σmax is given while vmax is computed. First comparison was for the time of contact Tc which is obtained by observing the interruption of the longitudinal beam of light from a source on one side of the impact faces before, during, and after collision, by means of a photomultiplier tube on the opposite side (Fig. 3.6.4).

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

150

Fig. 3.6.4

Dynamic Plasticity

Time of contact versus velocity; a comparison of theoretical and experimental data.

Fig. 3.6.5

Coeﬃcient of restitution versus impact velocity.

dynamic

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

The Propagation of Longitudinal Stress Waves

dynamic

151

A second comparison with the experimental data is the coeﬃcient of restitution deﬁned e = (2vf − V )/V with vf the ﬁnal velocity (travel time of the free end of specimen after separation) (Fig. 3.6.5). The characteristic planes for the impact for more than 34 m/sec are given in Fig. 3.6.6. L means “loading”, while U means “unloading”. The time of contact coincides with the experiment.

(a)

(b)

Fig. 3.6.6 (a) Characteristic plane for σY = σY 1 and V = 35.85 m/sec. (b) Characteristic plane for σY = σY 2 and V = 34.98 m/sec.

January 12, 2007

10:41

152

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Dynamic Plasticity

Fig. 3.6.7

A comparison of computed strain-time proﬁles with experimental data.

The best comparison with the experiment is on the graph of variation of strain at various cross sections. The graph given is only for the higher yield stress. All three theoretical solutions are shown. Also the time of contact is given (Fig. 3.6.7). The displacement variation is given in Fig. 3.6.8 for the two yield stresses and the three initial boundary conditions. The diameters where the variation is measured are shown. The variation of the stress at the impacted end is shown in Fig. 3.6.9. The initial rise of the stress at the impacted end is not given. The stress plateau is shown very clearly. One has compared also the cross section xA when the reﬂected shock wave is completely absorbed. Both theoretically and experimentally one have found xA between 4 and 5 diameters.

dynamic

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

The Propagation of Longitudinal Stress Waves

dynamic

153

Fig. 3.6.8 Computed displacement-time curves compared with experimental values obtained with an optical displacement technique.

The velocity of propagation is checked by Swegle and Ting [1982]. They have tested if the waves travel with the velocity predicted by the one-dimensional theory, although they have larger rise-times. That was what they have found. In a paper by Jones et al. [1987], a one-dimensional analysis is presented that leads to the appropriate equation of motion for the undeformed portion of a plastic, rigid rod after impact with a rigid anvil. This equation is used as a basis for deducing material properties of the rod material from post-test measurements. Data

January 12, 2007

154

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Dynamic Plasticity

Fig. 3.6.9 Variation of stress in time at the impact end of the bar. The experiment data were obtained with piezo crystal measurements. The dynamic overstress is not included in the present discussion.

for copper, for depleted uranium, for iron and steel are given for velocity surpassing 300 m/s. The impact of a solid cylinder (aluminum) by a compressible ﬂuid (water) is considered by Lush [1991]. The speeds of impact are 10, 100 and 350 m s−1 . The main modiﬁcation of the model is to incorporate the unloading of the plastic wave which is produced by the multiple reﬂections of the elastic release wave. In general the agreement between penetration, rate, contact pressure and depth of penetration is good.

dynamic

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

The Propagation of Longitudinal Stress Waves

dynamic

155

The formation, propagation, and reﬂection of shock waves is studied for synthetic curved cables by Tjavaras and Triantafyllou [1996]. First, analytical solutions are derived for weightless cables with nonlinear stress–strain relation, which are then compared with numerical solutions. For very small curvature the analytical and numerical solutions show that synthetic lines can form shock waves when loaded impulsively. The tension is ampliﬁed signiﬁcantly when a reﬂection occurs, pointing to a probable mechanism of failure. The examples are on Catenary. In another paper by Nonaka et al. [1996] the integration is done again, trying to explain some damage that appeared after earthquakes. One considers ﬁnite thin elastic bars and assumes that the second end is free, then ﬁxed, and in ﬁnal assuming that at the second end the rod is miss-matched impedance. The mechanical impedance is expressed by the change of the velocity by αρc with α > 0. For α very large one obtains various examples for steel: E = 206 GPa, ρ = 7850 kg/m3 , c = 5120 m/s. Several strengths measurements are presented by several papers by Kanel [1999]. The presented experimental data for engineering metals and alloys and for metals single crystals demonstrate the eﬀects of material grain structure and temperature on the resistance to high-rate rupture. Several ﬁgures are given, showing this inﬂuence. A technique for rapid two-stage dynamic tensile loading of polymers, based on a tensile Hopkinson bar apparatus, was developed by Shim et al. [2001]. In this technique, the initial incident wave and its reﬂection are used to load a specimen in quick succession. Consequently, the specimen is stressed, momentarily unloaded, and then reloaded until fracture. A procedure to obtain the associated stress–strain curves for such double-stage loading is formulated. This procedure is examined experimentally and analytically to substantiate their validity. To verify the proposed approach, a relatively rate-insensitive material was subjected to two-stage dynamic tension. The stress–strain curves obtained via the procedure established were compared with results from static loading. A ﬂat-nosed cylinder moving at a suﬃciently high impact velocity is assumed to fracture by Teng et al. [2005]. The fracture mechanism is investigated numerically using ABAQUS/Explicit. The impact velocity of the projectiles ranges from 240 m/s to 600 m/s. It is found that a more ductile cylinder tends to fail by petalling while a less ductile one by shear cracking.

3.7

The Elastic Solution

D’Alembert solution. For the progressive waves which translate in space we have the equation 2 ∂2u 2∂ u = c ∂t2 ∂x2

(3.7.1)

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

156

dynamic

Dynamic Plasticity

with c = const. If we change the variables α = x − ct ,

β = x + ct

where α, β are characteristic variables, we have ∂u ∂u ∂u ∂u ∂u ∂u = + , = −c +c ∂x ∂α ∂β ∂t ∂α ∂β ∂2u ∂2u ∂2u ∂2u + = + 2 ,··· . ∂x2 ∂α2 ∂α∂β ∂β 2 If we introduce in the equation we receive ∂2u =0 ∂α∂β from where we get the solution u = f (x − ct) + g(x + ct) which is the d’Alembert solution. It gives the general solution with f and g to be determined from initial data. u = f (x − ct) are the direct waves, propagating towards the right. Let us introduce a mobile system of coordinates, for an observer which translates with the speed ct. In the new system of coordinates x ¯ = x − ct, t¯ = t we have u(¯ x, t¯) = f (¯ x) i.e., the observer sees the same stationary wave. The Cauchy problem for the equation (3.7.1) with initial data: ∂u u(x, 0) = h(x) and (x, 0) = k(x) (3.7.2) ∂t with h of class C2 (h and ﬁrst two derivatives are continuous) and k of class C1 along −∞ < x < ∞ and the solution u = f (x − ct) + g(x + ct)

(3.7.3)

2

with f and g arbitrary and of class C . For t = 0 we have f (x) + g(x) = h(x) . By derivation of (3.7.3) ∂u (x, 0) = −cf (x) + cg (x) = k(x) . ∂t Integrating (3.7.5): 1 x −f (x) + g(x) = k(ξ) dξ + g(x0 ) − f (x0 ) . c x0 From (3.7.4) and (3.7.6) we obtain 1 1 f (x) = h(x) − 2 2c 1 1 g(x) = h(x) + 2 2c

x

x0

x

x0

(3.7.4)

(3.7.5)

(3.7.6)

1 k(ξ) dξ − [g(x0 ) − f (x0 )] 2 1 k(ξ) dξ + [g(x0 ) − f (x0 )] . 2

(3.7.7)

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

dynamic

The Propagation of Longitudinal Stress Waves

157

t

x0 − ct0

x0

ct =

xP

xP ct = x+

x−

x−

+ ct 0

ct = x

0

− ct

0

t = x0 x+c

0

domain of influence of P

Q ( x0 , t 0 )

t0

x0 + ct0

x

P domain of dependence of Q ( x0 , t0 )

domain of determin acy of the segment x 0 − ct0 ≤ x ≤ x0 ≤ ct0 Fig. 3.7.1

The various domains existing.

We replace x by x − ct in the ﬁrst relation and x by x + ct in the second, and by adding: u(x, t) = f (x − ct) + g(x + ct) 1 x−ct 1 x+ct 1 h(x − ct) + h(x + ct) − k(ξ) dξ + k(ξ) dξ . = 2 c x0 c x0 The last two terms can be written in the form: 1 h(x − ct) + h(x + ct) + u(x, t) = 2 2c

x+ct

k(ξ) dξ .

(3.7.8)

x−ct

The ﬁrst term corresponds to the solution with initial zero velocities (k(0) = 0) and the last term to the solution with initial zero displacements (h(0) = 0). The various domains which are involved in various problems and haw are they called are shown in Fig. 3.7.1. The prescribed data in P are not enough for the determination of the solution. One can put the problem if the solution is unique? Let us assume that u1 (x, t) and u2 (x, t) are two distinct solutions which satisfy the initial data (3.7.2). It follows that u = u1 − u2 is also a solution of (3.7.1) with the initial values u(x, 0) = 0

and

∂u (x, 0) = 0 ∂t

corresponding to h = k = 0. It follows from (3.7.8) that u(x, t) = 0 for any x and t ≥ 0. Thus u1 = u2 and the solution is unique. We have to study the dependence of the solution on the initial data. From (3.7.8) it follows that the solution u(x0 , t0 ) at Q(x0 , t0 ) depends on the Cauchy data along x0 − ct0 ≤ x ≤ x0 + ct0 and t = 0.

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

158

dynamic

Dynamic Plasticity

Let us show the continuous dependence of the solution (3.7.8) on the Cauchy data. Let us assume two sets of Cauchy data: u1 (x, 0) = h1 (x) , u2 (x, 0) = h2 (x) ,

∂u1 (x, 0) = k1 (x) ∂t ∂u2 (x, 0) = k2 (x) ∂t

(3.7.9)

and let us assume that |h1 (x) − h2 (x)| < ε ,

|k1 (x) − k2 (x)| < δ

(3.7.10)

for −∞ < x < ∞ and ε > 0, δ > 0 arbitrary. From (3.7.8) we have: h1 (x − ct) − h2 (x − ct) h1 (x + ct) − h2 (x + ct) + 2 2 x+ct 1 + [k1 (ξ) − k2 (ξ)] dξ . 2c x−ct !b !b Taking the modulus and since | a f dξ| ≤ a |f | dξ we have u1 (x, t) − u2 (x, t) =

|u1 (x, t) − u2 (x, t)| ≤

|h1 (x − ct) − h2 (x − ct)| 2 1 |h1 (x + ct) − h2 (x + ct)| + + 2 2c

Using (3.7.10)2 1 2c

x+ct

|k1 (ξ) − k2 (ξ)| dξ ≤ x−ct

x+ct

|k1 (ξ) − k2 (ξ)| dξ . x−ct

1 δ{x + ct − (x − ct)} = δt 2c

and thus |u1 (x, t) − u2 (x, t)| ≤ ε + δt . For t ﬁxed if h1 and h2 as well as k1 and k2 , are only “slightly” distinct, i.e., if ε and δ are “small”, the solution u2 approaches u1 as close as desired. In the case of non homogeneous equation 2 ∂2u 2∂ u − c = f (x, t) (3.7.11) ∂t2 ∂x2 we try to ﬁnd a solution of the form u = u1 + u2 with u1 a solution of homogeneous equation

∂ 2 u1 ∂ 2 u1 − c2 =0 2 ∂t ∂x2 with initial data u1 (x, 0) = h(x), ∂u1 /∂t(x, 0) = k(x) and u2 a solution of the equation 2 ∂ 2 u2 2 ∂ u2 − c = f (x, t) ∂t2 ∂x2

(3.7.12)

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

The Propagation of Longitudinal Stress Waves

dynamic

159

C

dt =

dx/

dx/

dt =

c

t

−c

D t

0

x

A

B

x

c(t − t ) Fig. 3.7.2

Domain of integration.

with initial data u2 (x, 0) = 0 ,

∂u2 (x, 0) = 0 . ∂t

Integrate now (3.7.12) in the domain D: 2 2 ∂ u2 2 ∂ u2 dxdt = −c f (x, t) dxdt ∂t2 ∂x2 D D

(3.7.13)

(3.7.14)

and using the Green’s formula ∂Q ∂P − dxdy = − P dx + Qdy ∂y ∂x D ∂D the formula (3.7.14) becomes ∂u2 ∂u2 dx + c2 dt = f (x, t) dxdt . − ∂x ∂D ∂t D Since along BC we have dx = −cdt, along CA we have dx = −cdt, and along AB we have dt = 0, this integral becomes ∂u2 ∂u2 ∂u2 ∂u2 ∂u2 ∂u2 dt + dx − dt + dx − dx + c2 dt c c ∂t ∂x ∂t ∂x ∂t ∂x BC CA AB = f (x, t) dxdt . D

Since in the brackets there are total diﬀerentials, the third term is zero from (3.7.13), and the fourth is zero on AB, we obtain cdu2 − cdu2 = f (x, t) dxdt BC

CA

D

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

160

dynamic

Dynamic Plasticity

t

x−

ct =

co n

st.

ξ B x 0 + η , t0 + c

•

t0

A(x0 + ξ , t0 + η )

η

x+

C ( x0 − ξ , t0 − η )

ct =

co n

ξ

ξ

ξ D x0 − cη , t 0 − c

0

x

x0 Fig. 3.7.3

st.

Four arbitrary characteristic lines.

or by integration

cu2 (C) − cu2 (B) − cu2 (A) + cu2 (C) =

f (x, t) dxdt D

or since the second and third terms are zero according to (3.7.13), ¯ 1 t x+c(t−t) u2 (C) = u2 (x, t) = f (¯ x, t¯) d¯ xdt¯. 2c 0 x−c(t−t¯) Thus the general solution is: u(x, t) =

1 h(x − ct) + h(x + ct) + 2 2c

x+ct

k(ξ) dξ + x−ct

1 2c

t

x+c(t−t¯)

f (¯ x, t¯) d¯ xdt¯. 0

x−c(t−t¯)

This solution depends on the Cauchy data on AB, and on the values of f (x, t) in the internal points of the triangle D. Let us discuss now the boundary conditions and mixed boundary value problem. The mixed boundary value problem is composed from: boundary conditions for x=a

and t ≥ 0

x=b

and t ≥ 0

and the initial conditions for a ≤ x ≤ b, t = 0. Let us consider four arbitrary characteristic lines from x − ct = const. and x + ct = const. (Fig. 3.7.3). The coordinates of B are: x + ct = x0 + ξ + c(t0 + η) x − ct = x0 − ξ − c(t0 − η) .

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

The Propagation of Longitudinal Stress Waves

dynamic

161

t B A C

D

ct = x−

0

Domain where the solution of the Cauchy problem is known x

0 initial condition on x ≥ 0, t = 0 given Fig. 3.7.4

Solution in B is known if given on A, D and C.

From here we have by adding: xB = x0 + ηc, tB = t0 + ξ/c. The coordinates from D are from: x − ct = x0 + ξ − c(t0 + η) x + ct = x0 − ξ + c(t0 − η) . From here we again ﬁnd: xD = x0 − cη, tD = t0 − ξ/c. From the general solution u(x, t) = f (x − ct) + g(x + ct) we obtain u(A) = f (D) + g(B) , u(C) = f (B) + g(D) . From here by adding: u(A) + u(C) = u(D) + u(B) . Thus if u is prescribed in A, D and C it follows in B. Thus the solution in any B can be obtained if prescribed by Cauchy data along the line x − ct = 0 and known in C by boundary conditions. The solution is unique in D and the relation is also linear. Let us consider now the reﬂection from a ﬁxed end. We have to ﬁnd out how the solution is extended by reﬂection. We consider the initial conditions ∂u (x, 0) = k1 (x) , ∂t and the boundary condition x = 0, t ≥ 0 : u(x, t) = 0. The solution in D is x+ct 1 h(x − ct) + h(x + ct) + u(x, t) = k(s) ds . 2 2c x−ct x ≥ 0,

t = 0 : u(x, 0) = h1 (x) ,

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

162

dynamic

Dynamic Plasticity

t t

t

D1 D

0

x Fig. 3.7.5

x0 − ct

x0

x0 + ct

−ct

0

+ct

Various domains for reﬂection of waves.

Let us ﬁnd the solution in D1 . For x = 0 from u(x, t) = f (x − ct) + g(x + ct) and u(0, t) = 0 we get f (−ct) + g(ct) = 0 or f (−x) = −g(x) with x arbitrary argument. From the general expressions x 1 1 1 f (x) = h(x) − k(ξ) dξ − [g(x0 ) − f (x0 )] , 2 2c x0 2 x 1 1 1 k(ξ) dξ + [g(x0 ) − f (x0 )] , g(x) = h(x) + 2 2c x0 2 we put x0 = 0 (see Fig. 3.7.5), we have: x 1 1 1 k(ξ) dξ − [g(0) − f (0)] , f (x) = h(x) − 2 2c 0 2 x 1 1 1 g(x) = h(x) − k(ξ) dξ + [g(0) − f (0)] . 2 2c 0 2 We replace here x by −x, h by h1 , k by k1 and we have x 1 1 1 k1 (−ξ) dξ − [g(0) − f (0)] . f (−x) = h1 (−x) + 2 2c 0 2 From the condition f (−x) = −g(x) follows: x 1 1 1 − h1 (−x) + k1 (−ξ) dξ − [g(0) − f (0)] 2 2c 0 2 x 1 1 1 = − h1 (x) − k1 (ξ) dξ − [g(0) − f (0)] . 2 2c 0 2 This relation is satisﬁed for any x if h1 (−x) = −h1 (x)

and k1 (−x) = −k1 (x) .

Thus the problem of a ﬁxed end u(0, t) = 0 for x = 0 in a mixed problem, is equivalent with the Cauchy problem for the whole line −∞ < x < +∞ with the odd functions h1 and k1 . . . . Therefore & −∞ < x < +∞ ∂u (x, 0) = k(x) : u(x, 0) = h(x) , ∂t t=0

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

dynamic

The Propagation of Longitudinal Stress Waves

t

163

x=

ct

Q

ct

t

x=

P

x

0 Fig. 3.7.6

x

0

The two domains where the above formula applies.

with h(x) =

h1 (x) −h1 (x)

for x ≥ 0 for x < 0 ,

k1 (x) =

k1 (x) −k1 (x)

for x ≥ 0 for x < 0 .

We can prove also the converse: if the initial data along the line −∞ < x < +∞ and t = 0 are odd with respect to the origin h1 (x) = −h1 (x) ,

k1 (−x) = −k1 (x) ,

then the solution of the wave equation is zero at that point (ﬁxed point). For the proof we start from the solution 1 +ct h1 (−ct) + h1 (ct) + k(s) ds = 0 . u(0, t) = 2 2c −ct Therefore the solution of the mixed problem in x ≥ 0, t ≥ 0 is x+ct h(x − ct) + h(x + ct) 1 + k(s) ds 2 2c x−ct u(x, t) = x+ct −h(ct − x) + h(x + ct) 1 + k(s) ds 2 2c −x+ct

for x > ct ,

for x < ct .

The last relation is obtained from the ﬁrst by replacing h(x − ct) by −h(ct − x), and k(x − ct) by −k(ct − k). The two relations are applied in the regions shown in Fig. 3.7.6. The two formulae given above are applied in the two regions shown in this ﬁgure. Let us study now the stress at a ﬁxed end of an elastic bar. On the direct waves u1 = f1 (x − ct) the stress is σ1 = E

∂u1 ∂u1 = −ρc , ∂x ∂t

while on the inverse waves u2 = f2 (x + ct) the stress is σ2 = E

∂u2 ∂u2 = ρc . ∂x ∂t

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

164

dynamic

Dynamic Plasticity

The total stress is

∂u2 ∂u1 + = ρc2 [f1 (x − ct) + f2 (x + ct)] , σ = σ1 + σ2 = ρc − ∂t ∂t while the total displacement is u = f1 (x − ct) + f2 (x + ct) from where for a ﬁxed x = 0 we have f1 (−ct) + f2 (ct) = 0, or f1 (−z) = −f2 (z). Thus at a ﬁxed end of the bar σ|x=0 = (σ1 + σ2 )|x=0 = 2f2 E . We arrive at an important conclusion: the stress is doubled due to reﬂection. If the incident wave reaching the ﬁxed end is still elastic, after reﬂection it may be nearly 2σY . So that an elastic wave at reﬂection may become a plastic wave. Now let us look at the conditions which exist at the free end. Let us consider the equation 2 ∂2u 2∂ u = c ∂t2 ∂x2

with the initial conditions & t=0 0 ≤ x < +∞

: u(x, 0) = h1 (x) ,

∂u (x, 0) = k1 (x) ∂t

and the boundary conditions at the free end x = 0: & t>0 ∂u (0, t) = 0 . : ∂x x=0

(3.7.15)

(3.7.16)

Let us show that the mixed problem with a free end ∂u/∂x(0, t) = 0 is equivalent with the Cauchy problem on the entire x-axis with initial conditions for displacement and velocities even. For the proof from u(x, t) = f (x − ct) + g(x + ct) follows ∂u/∂x(0, t) = f (−ct) + g (ct) = 0, i.e., f (−x) = −g (x) . From

x 1 1 1 f (−x) = h1 (−x) + k1 (−s) ds − [g(0) − f (0)] , 2 2c 0 2 x 1 1 1 g(x) = h1 (x) + k1 (s) ds + [g(0) − f (0)] , 2 2c 0 2

follows f (−x) = g (x) =

1 1 h (−x) − k1 (−x) , 2 1 2c 1 1 h1 (x) + k1 (x) , 2 2c

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

dynamic

The Propagation of Longitudinal Stress Waves

165

from where 1 1 h1 (−x) − k1 (−x) = −h1 (−x) − k1 (x) c c i.e., h1 (−x) = −h1 (x) ,

k1 (−x) = k1 (x) .

Since the derivative of an even function h1 (x) = h1 (−x) is an odd function h1 (x) = −h1 (−x) we have h1 (x) = h1 (−x) . Therefore the mixed problem for a free end is equivalent with the Cauchy problem on the entire axis with the conditions h1 (x) for x > 0 , h(x) = & u(x, 0) = h(x) h1 (−x) for x < 0 , −∞ < x < +∞ with ∂u t=0 (x, 0) = k(x) k1 (x) for x > 0 , ∂t k(x) = k (−x) for x < 0 . 1 Let us prove the converse. If the Cauchy conditions on −∞ < x < +∞ are even h1 (x) = h1 (−x), k1 (x) = k1 (−x) then ∂u/∂x(0, t) = 0. From the solution 1 x+ct h(x − ct) + h(x + ct) + u(x, t) = k(s) ds 2 2c x−ct follows for x = 0: ∂u h (−ct) + h (ct) 1 (0, t) = + [k1 (ct) − k1 (−ct)] = 0 ∂x 2 2c since h1 (−ct) = h1 (ct). The solution for the mixed problem for x > 0, t > 0 is: u(x, t) h(x − ct) + h(x + ct) 1 x+ct + k(s) ds 2 2c x−ct = x+ct ct−x 1 h(ct − x) + h(x + ct) + k(s) ds + k(s) ds 2 2c 0 0

for x > ct ,

for x < ct ,

which satisﬁes the initial conditions (3.7.15) and the boundary conditions (3.7.16). Let us examine the displacement at the free end of an elastic bar. We have on the direct waves u1 = f1 (x − ct) and the stress ∂u1 ∂u1 = −ρc ∂x ∂t and on the inverse waves u2 = f2 (x + ct) with the stress σ1 = E

σ2 = E

∂u2 ∂u2 = ρc . ∂x ∂t

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

166

Dynamic Plasticity

The total stress is

∂u1 ∂u2 + = ρc2 [f1 (x − ct) + f2 (x + ct)] σ = σ1 + σ2 = ρc − ∂t ∂t

and the total displacement is u = f1 (x − ct) + f2 (x + ct). If the end x = 0 is free, we have σ = 0 or f1 (−ct) + f2 (ct) = 0. That means f1 (−ct) = f2 (ct) . The total displacement is u|x=0 = (u1 + u2 )x=0 = 2f2 (ct) . That means that at a free end the displacement is doubled. Because for the stress we have σ1 = −σ2 a compressive wave is reﬂected as a tensile wave at the free end (or the reverse). If the mechanical proprieties are distinct in tension and in compression, that may make a diﬀerence. Bibliography Bell J. F., 1968, The Physics of Large Deformation of Crystalline Solids, Springer-Verlag, Berlin. Bell J. F., 1973, The experimental foundations of solid mechanics, in Handbook der Physic, Springer-Verlag, Berlin. Bodner S. R. and Clifton R. J., 1967, Experimental investigation of elastic-plastic pulse propagation in aluminum rods, J. Appl. Mech. Trans. ASME 34, 1, 91–99. Chen S. R., Maudlin P. J. and Gray III G. T., 1999, Constitutive behavior of model FCC, BCC, and HCP metals: experiments, modeling and validation, in Constitutive and Damage Modeling of Inelastic Deformation and Phase Transformation, Khan A. S. (ed.), NEAT Press, 623–626. Chou P. C. and Hopkins A. K., (eds.) 1973, Dynamic response of materials to intense impulsive loading, Air Force Materials Laboratory, 555 pp. Clifton R. J. and Bodner S. R., 1966, An analysis of longitudinal elastic-plastic pulse propagation, J. Appl. Mech. Trans. ASME 33, 2, 248–255. Cristescu N., 1957, On propagation of waves in rubber, Prikl. Mat. Meh. 21, 795 800 (in Russian). Cristescu N., 1967, Dynamic Plasticity, John Wiley & Sons, Inc., New York. Cristescu N., Dynamic plasticity, Appl. Mech. Rev. 21, 7, 659–668. Cristescu N. and Bell J. F., 1970, On unloading in the symmetrical impact of two aluminum bars, In: Inelastic Behavior of Solids, McGraw Hill Book Co., 1970, 397–419. Cristescu N., 1970, The unloading in symmetric longitudinal impact of two elastic-plastic bars, Int. J. Mech. Sci. 12, 6, 723–738. De Juhasz K. J., 1949a, Graphical analysis of impact of bars stresses above the elastic range. Part. I, J. Franklin Inst. 248, 15–48. De Juhasz K. J., 1949b, Graphical analysis of impact of bars stressed above the elastic range. Part. II, J. Franklin Inst. 248, 113–142.

dynamic

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

The Propagation of Longitudinal Stress Waves

dynamic

167

Francis P. H., 1966, Wave propagation in thin rods with quiescent temperature gradients, J. Appl. Mech. 33, 3, 702–704. Huﬃngton N. J., (ed.) 1965, Behaviour of materials under dynamic loading, Behavior of Materials under Dynamic Loading at the Winter Annual Meeting of the ASME, Chicago, Illinois, 1965, 187 pp. Jones S. E., Gillis P. P. and Foster J. C. Jr., 1987, On the equation of motion of the undeformed section of a Taylor Impact specimen, J. Appl. Phys. 61, 2, 499–502. Kanel G. I., 1999, Dynamic strength of materials, Fatigue Fract. Engng. Mater. Struct. 22, 1011–1019. K´ arm` an Th. and Duwez P., 1950, The propagation of plastic deformation in solids, J. Appl. Phys. 27, Ser E, 107–110. Kawata K. and Shioiri J., (eds.) 1978, High Velocity Deformation of Solids Symposium Tokyo/Japan, 1977, Springer Verlag, 452 pp. Kenning M. J., 1974, Uniqueness of uniaxial elastic-plastic interface motions, J. Mech. Phis. Solids 22, 437–456. Kinslow R., (ed.) 1970, High-Velocity Impact Phenomena, Academic Press, 579 pp. Kolsky H., 1953, Stress Waves in Solids, Clarendon Press, Oxford. Kolsky H., 1969, Production of tensile shock waves in stretched natural rubber, Nature 224, 5226, 1301. Lagoudas D. C., Ravi-Chandar K., Sarh K. and Popov P., 2003, Dynamic loading of polycrystalline shape memory alloy rods, Mech. Materials 35, 689–716. Lee L. H. N. and Chi-Mou Ni, 1973, A minimum principle in dynamics of elastic plastic continua at ﬁnite deformation, Archives of Mechanics 25, 3, 457–468. Lee L. H. N., 1974, Dynamic plasticity, Nuclear Eng. and Design 27, 386–397. Lenski V. S., 1949a, On the elastic-plastic shock of a bar on a rigid wall, Prikl. Mat. Meh. 12, 165–170 (in Russian). Lush P. A., 1991, Comparison between analytical and numerical calculations of liquid impact on elastic-plastic solid, J. Mech. Phys. Solids 39, 1, 145–155. Magness L. S. Jr., 1994, High strain rate deformation behaviors of kinetic energy penetrator materials during ballistic impact, Mech. of Materials 17, 147–154. Miklowitz J., (ed.) 1969, Wave propagation in solids, ASME Winter Annual Meeting, Los Alamos, California, 1969, 183 pp. Mines R. A. W., 2004, A one-dimensional stress wave analysis of a lightweight composite armour, Comp. Structures 64, 55–62. Misra J. C., Kar S. B. and Samanta S. C., 1987, Distribution of stresses in a heated nonhomogeneous rod, S. M. Archives 12/2, 97–111. Nemat-Nasser S., Li Y. F. and Isaacs J. B., 1994, Experimental/computational evaluation of ﬂow stress at high strain rates with application to adiabatic shear banding, Mec. Mater. 17, 111–134. Nonaka T., Clifton R. J. and Okazaki T., 1996, Longitudinal elastic waves in columns due to earthquake motion, Int. J. Impact. Engng. 18, 7–8, 889–898. Nowacki W. K., 1978, Problems of Wave Propagation in the Theory of Plasticity, Mir, Moscow. Ponomarev S. D., Biderman V. L., Likharev K. K., Makushin V. M., Malinin N. N. and Feodos’ev V. I., 1959, Resistence calculus in construction of machines, Mashigiz, Moscow, Tom III, 553–580 (in Russian). Raniecki B., 1971, The inﬂuence of dynamical thermal expansion on the propagation of plane elastic-plastic stress waves, Quart. Appl. Math. 29, 2, 277–290. Raiser G. F., Wise J. L., Clifton R. J., Grady D. E. and Cox D. E., 1994, Plate impact response of ceramics and glasses, J. Appl. Phys. 75, 8, 3862–3869.

January 12, 2007

168

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Dynamic Plasticity

Rakhmatulin H. A. and Demianov Yu. A., 1961, Strength under Impulsive Momentary Loads, Moscow (in Russian). Rakhmatulin H. A., 1945, On the propagation of unloading waves, Prikl. Mat. Meh. 9, 1, 91–100 (in Russian). Shim V. P. W., Yuan J. and Lee S.-H., 2001, A technique for rapid two-stage dynamic tensile loading of polymers, Experimental Mechanics 41, 1, 122–127. Santosham T. V. and Ramsey H., 1970, Small plastic strain wave propagation in prestressed soft copper rods, Int. J. Mech. Sci. 12, 5, 447–457. Shapiro G. S., 1946, Longitudinal vibration of bars, Prikl. Mat. Meh. 10, 597–616 (in Russian). Swegle J. W. and Ting T. C. T., 1982, Plastic wave propagation in a circular cylindrical rod, J. Appl. Mech. Trans. ASME 49, 253–256. Taylor G. I., 1946, The testing of materials at high rates of loading, J. Inst. Civil Engrs. 8, 486–519. Taylor G. I., 1958a, The use of ﬂat-ended projectiles for determining dynamic yield stress, Proc. Roy. Soc. Ser. A 194, 289–289. Taylor G. I., 1958b, The formation and enlargement of circular hole in a thin, plastic sheet, Quart. J. Mech. Appl. Math. 1, 103–124. Teng X., Wierzbicki T., Hiermaier S. and Rohr I., 2005, Numerical prediction of fracture in the Taylor test, Int. J. Solids Structures 42, 2929–2948. Tjavaras A. A. and Triantafyllou M. S., 1996, Shock waves in curved synthetic cables, J. Enge. Mech. 122, 4, 308–315. Varley E., (ed.) 1976, Propagation of shock waves in solids, The Applied Mechanics Conference, Salt Lake City, Utah, 1976.

dynamic

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Chapter 4

Rate Inﬂuence

4.1

Experimental Results

The rate inﬂuence seems to be the central problem of dynamic plasticity. It has been known for many years that during dynamic testing, solids behave in a more or less diﬀerent way than in static tests. Many theoretical and experimental papers have been devoted to this problem. Let us consider the problem shortly. We discuss the main conclusion resulting from the experiments that have been performed. Details concerning the experimental techniques will not be given here. We shall see however, that in some experimental papers the wave propagation phenomena were disregarded, although the rate of loading was high. This can be done only if the specimen is very short. The old tests are discussed in detail by Cristescu [1967], Cambell [1970], Cristescu and Suliciu [1982] and Goldsmith [2001], and will not be mentioned here any more. Only a few tests will be revealed. Strain rates ranging between 10−5 sec−1 and 10−3 sec−1 are termed static tests. Tests in which the rates of strain range between 10−2 sec−2 and 102 sec−1 can be termed intermediate tests (these are the rates of strains usually met in various metal working processes, for instance), while the tests producing rates of strains above 102 sec−1 (and certainly of the order of magnitude of 103 sec−1 and higher) can be called dynamic in the sense that as a rule in such tests the inertia forces, the propagation of waves etc. must be considered in the analyses. Sometimes the inertia forces are considered in the analysis when rates of strain of approximately 1 sec−1 are reached. A review is presented by Klepaczko [1998] on recent progress in shear testing of materials at high and very high (up to 106 s−1 ) strain rates. The classiﬁcation of various testing machines according to the kind of test performed, i.e., tension, compression, bending, combined loading etc., is not important for the approach followed here. Kinematic and dynamic jump conditions are also given. A theory of rate-type materials for one-dimensional case is due to Suliciu [1974]. He introduces diﬀerent classes of regulated functions and introduces the concept of wave propagation for the frame of regulated functions. The simplest diagnostic test is the uniaxial compression or tension test of a cylindrical specimen. For the description of the technical aspects of this kind of 169

dynamic

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

170

Dynamic Plasticity

experiments see for instance Ponomarev et al. [1956], Ilyushin and Lenskii [1959], Dally and Riley [1965], Bell [1973], Gupta [1976], etc. Basically there are two kinds of testing machines. With the so called “hard” machines the variation in time of the length of the specimen can be prescribed, while the response of the material is known by registering the force necessary to produce this deformation. Other kind of machines called “soft” can prescribe the stress applied to the specimen (by a weight attached directly or not to the specimen), while the response of the material is observed by measuring the elongation of the specimen. Both kinds of testing machines provide some stress–strain diagrams. The experiments made by Kolsky [1949] with copper and lead showed that the dynamic elastic modulus does not diﬀer sensibly from the static one (Fig. 4.1.1),

Fig. 4.1.1

Static and dynamic stress–strain curves for copper.

Fig. 4.1.2

Stress–strain curves for pure aluminum.

dynamic

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Rate Inﬂuence

Fig. 4.1.3

dynamic

171

Stress–strain curves for schist.

but that the whole dynamic stress–strain curve is higher that the static curve. The strain increases even when the stress is falling, and it follows that the dynamic constitutive equation for copper is time-dependent. The static stress–strain curve does not seem to be rate dependent. In Fig. 4.1.2 are given the stress–strain curves for pure aluminum as obtained with various rates of strains by Hauser et al. [1960] (reproduced here from Thomsen et al. [1968]). If the rates of strains are high (over 102 sec−1 , say), the inertia forces cannot be neglected and the wave propagation phenomena must be considered in the analysis of the experiment. For rocks the inﬂuence of the strain rate on both loading and unloading is ˙ = shown in Fig. 4.1.3 for two loading rates |σ| ˙ = 300 kgf cm−2 min−1 and |σ| −2 −1 1.33 kgf cm min both in loading and unloading. Thus the stress–strain curve is non-linear during loading and unloading. One can see also the important hysteresis loops during unloading and the fact that the whole curve is inﬂuenced by the loading rate. In Fig. 4.1.4 we give the variation in time of the strain and of the surface angle for copper (Bell [1968]) for an impact velocity V0 = 1200 cm/sec, measured at 5.1 cm from the impacted end. For high impact velocity the strain is higher, and that can not be explained by the classical theory. Another parameter which can be measured at the impacted end of the bar is the stress. Generally the stress can be measured with the help of piezoelectric crystal wafers placed at the impacted face. Filbey [1961] has used an X-cut quartz crystal wafer 2.12 cm in diameter and 0.25 mm thick. A typical result for two

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

172

Dynamic Plasticity

Fig. 4.1.4

Variation of strain and surface angle in time for copper.

Fig. 4.1.5

Peak stress at impacted end.

dynamic

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

Rate Inﬂuence

dynamic

173

experiments with symmetric impact is given in Fig. 4.1.5 (Filbey [1961]) who used the impact velocity V0 = 7100 cm/sec. The decrease is in microseconds to become nearly constant for a relatively long period of time (Fig. 4.1.6) (Filbey [1961]). The medium value of the peak stress is 71043 N cm−2 . The stress “plateau” which is reached after several microseconds is at the level 13160 N cm−2 . The decrease of the stress which follows afterwards is due to the unloading. Another experiment which played an important role in the development of the theory was the following one carried out by Bell [1951]. A medium carbon steel

Fig. 4.1.6

Fig. 4.1.7

Stress plateau.

General strain rate eﬀects on mortar strength.

January 12, 2007

174

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Dynamic Plasticity

long bar (about 183 cm in length and consisting of portions 0.64 or 0.35 cm in diameter) was subjected to a static extension. A dynamic loading was superposed. The experimental results obtained by Bell have shown that the ﬁrst waves which propagate in the bar are propagating with the bar velocity c0 . Similar tests were done afterwards by several authors. Similar dynamic loading tests followed by a dynamic reloading have been done by Alter and Curtis [1956] on lead specimens and afterwards by Bell and Stein [1962] on aluminum. The ﬁrst waves were propagating with the bar velocity. Similar tests in which the hitter was a composed bar made from two distinct materials (possessing distinct densities) have been carried out by other authors. The general trend in the unconﬁned tests of cementations material data is a very slight increase in strength from a low strain rate of 1.0 × 10−7 /s up to a strain rate of approximately 1.0/s for tensile strength properties, 10/s for shear strength properties and 100/s for compressive strength properties. Above these

Fig. 4.1.8 Typical stress–strain curves for polycarbonate at 23◦ C for strain rates of (a) 0.000368 s−1 , (b) 8.43 s−1 , and 6000 s−1 ; and measured 8% ﬂow stress as a function of logarithmic strain rate for polycarbonate at 23◦ C (specimen thickness: 4.4 mm, • 1.5 mm).

dynamic

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

Rate Inﬂuence

Fig. 4.1.9

Tree axial curves for granite (Maranini and Yamaguchi [2001]).

dynamic

175

January 12, 2007

176

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Dynamic Plasticity

critical strain rates a rather abrupt increase in strength occurs with a slope of (log10 strength/log10 strain rate) of approximately one-third. Representative strain rate eﬀects on unconﬁned strength properties reported by Schmidt and Ross [1999] are given in Fig. 4.1.7. See also the paper of Bertholf and Karnes [1975] on the same subject. Very high strain-rate response of a NiTi shape-memory alloy vas studied by Nemat-Nasser et al. [2005]. They adopt a split Hopkinson bar test to get such high strain rates of about 10,000/s. The result obtained is an increase of the true stress at high strain rates. The assumption of uniform stress and strain distribution within a split Hopkinson pressure bar specimen is assumed incorrect at high impact velocities (Dioh et al. [1995]), and that the propagation of plastic wave fronts within the split-Hopkinson-pressure-bar are responsible for the dependence of ﬂow stress measurements on specimen thickness at high strain rates. The same topic is used in Dioh et al. [1993]; they make tests studying the thickness of the specimens in the split Hopkinson pressure bar experiments. Various thermoplastics have been studied. For instance in Fig. 4.1.8 is showing some of the results. The “high” strain rates is completely above the other. Also in the lower ﬁgure one can see that the thick specimens are above the small one, at least for higher strain rates. Some other curves for granite measured in three axial stresses are shown in Fig. 4.1.9, from Maranini and Yamaguchi [2001]. The small original plateau is creep in a few minutes done before an unloading is performed to measure the elastic parameters (see Ch. 2). But changing the conﬁning pressure changes the whole stress–strain curve. Also, the volumetric stress–strain curves are shoving ﬁrst compression and afterwards dilatation. The compression is trying to disappear as the conﬁning pressure is increased signiﬁcantly, but not the creep by dilatancy. Similar results are mentioned by very many authors.

4.2

The Constitutive Equation

Many authors have proposed various constitutive equations in order to describe the mechanical properties of materials that exhibit the rate eﬀect. All have started from the assumption, suggested by experimental evidence, that, even while the stress is being continuously increased, there is no longer a one-to-one correspondence between stress and strain as prescribed by a ﬁnite stress–strain relation. The ﬁrst was Ludwik [1909] and then Prandtl [1928] who observed that for a ﬁxed plastic strain the corresponding stress is higher, the greater the average rate of strain at which the experiment is performed. Ludwik postulated the following logarithmic equation σ = σ1 + σ0 ln

ε˙P ε˙P 0

.

dynamic

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

Rate Inﬂuence

Fig. 4.2.1

dynamic

177

Inﬂuence of the rate of strain on the stress–strain curve.

Where σ1 , σ0 and ε˙P 0 are material constants. Here σ1 is the yield stress correspondP ing to the strain rate ε˙P 0 (Fig. 4.2.1). If the strain rate is greater than ε˙0 , the stress corresponding to a certain plastic strain is greater, σ0 is the measure of this increment. The reference conﬁguration for such constitutive equation is the actual one, since the strain is not present. Many simple models describing the rate eﬀect were inspired by this formula. If the elastic part of the strain can be neglected with respect to the plastic one, then the simplest of these models can be written as σ−σ Y if σ > σY , 3η ε˙ = 0 if 0 ≤ σ ≤ σY , where η is the viscosity coeﬃcient. This model can be called Bingham model (Bingham [1922]). In it ε˙ depends on the overstress. This model was used for various pastes, dough, vaseline, paints, mud etc., but also for various solid bodies as metals, rocks etc. The coeﬃcient η can be found experimentally in the following way. From here we obtain 3η =

σ2 − σ1 . ε˙2 − ε˙1

Generally, for most solid bodies η is decreasing with increasing ε, ˙ and therefore it is only within certain ranges of variation that η can be considered to be constant. If the material is work-hardening, and if the conventional quasi-static relation is σ = f (ε), then Malvern [1951a, 1951b] proposed the use of the expression: σ = f (ε) + a ln(1 + bε˙P ) .

January 12, 2007

10:41

178

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

dynamic

Dynamic Plasticity

Here a and b are material constants. Solving this equation with respect to the rate of strain, we can write this relation as: 1 σ − f (ε) exp −1 . (4.2.1) ε˙P = b a The reference conﬁguration is now the initial one. This equation suggest a generalization in the sense that the plastic rate of strain must be a function of the overstress σ − f (ε), that is, of the diﬀerence between the dynamic and the actual static plastic strain. Thus E ε˙P = F (σ − f (ε)) . We can write now

σ − f (ε) 3η ε˙ = 0

(4.2.2)

if σ > f (ε) , if 0 < σ ≤ f (ε) ,

where σ = f (ε) is the work-hardening condition. To give some values for η from creep curves of rock-salt (see Baroncea et al. [1977]) η is of the order 1015 Nm−2 sec (Poise). For schist it is 1012 Poise while for other rocks it may be higher (1017 – 1018 Poise for argillaceous schist, see Vyalov [1978]). For ice from 1010 to 1015 Poise. For quasistatic deformations (ε˙ ≈ 1 sec−1 ) for mild steel (Cristescu [1977]) η is of the order of magnitude of 107 Nm−2 sec, but for faster deformation (ε˙ ≈ 100 sec−1 ) it is of the order 106 Nm−2 sec. For even very high rate of strains (ε˙ > 103 sec−1 ) Cambell [1973] gives for various metals values of the order 103 Poise. The values given above are only illustrative. Since in most cases the elastic part of the strain is connected with the stress by the Hooke’s law EεE = σ , the full constitutive equation can be written in the form E ε˙ = σ˙ + F (σ − f (ε)) . With F (z) satisfying the properties F (z) > 0 if z > 0 , F (z) = 0 if z ≤ 0 . This property is related to the loading/unloading criteria. More generally, the plastic rate of strain can be considered a function of the stress and strain E ε˙P = g(σ, ε) , and it yields the constitutive equation E ε˙ = σ˙ + g(σ, ε) . This form of the constitutive equation has been used by Malvern [1951a, 1951b].

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Rate Inﬂuence

dynamic

179

Various form of such constitutive equation was used by very many authors. Sokolovski [1948a, 1948b] used it for perfectly plastic materials with g(σ, ε) = kF (|σ| − σY ) , where σY is the static yield stress. Ting and Symonds [1964] have used the expression q σ g(σ) = D −1 σY with D and q material constants, speciﬁc for the material considered. Gilman [1960] suggested g(σ) = ε˙0 exp(−A/σ) , where ε˙0 and A are material constants. Some generalizations are due to Perzina [1963] α N ) σ g(σ) = Aα exp −1 −1 , σY α=1 g(σ) =

N ) α=1

Bα

σ −1 σy

α ,

etc.

All the functions and constants which occur in various expressions of the function g are, sometimes, time and temperature dependent. One can compute the rate of strain locally, the averaging is not possible. The elastic constants are independent on the rate of strain. The reference conﬁguration is always the actual one. The basic idea of the constitutive equations given above is that the plastic rate of strain is a function only of the dynamic overstress. This leads to the conclusion that in the plastic range the stress–strain curves for various constant rates of plastic straining are parallel curves. As will be shown later on (see B´eda [1962a]) these curves are not always parallel. Thus, instead of (4.2.3) one must look for a quasi-linear constitutive equation of the form ∂ε ∂σ = ϕ(σ, ε) + ψ(σ, ε) (4.2.3) ∂t ∂t for both plastics (Cristescu [1964]), and for metals (Cristescu [1963, 1966]). Variants have been used by many authors. Suliciu [1966] have shown when the constitutive equation (4.2.3) can be written in the form σ = H(ε, t) . In (4.2.3) ϕ(σ, ε) which can also possibly depend on time, is the measure of the instantaneous response of the material to an increase of stress, while ψ(σ, ε) which can also possibly depend explicitly on time, will be the measure of the non-instantaneous response of the material. It will be assumed that ϕ > 0.

January 12, 2007

180

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

dynamic

Dynamic Plasticity

Of course, ϕ and ψ may also comprise various characteristic constants of the material (yield stress, viscosity coeﬃcient, etc.) which are to a great extent temperature dependent. In order to solve the problem of propagation of longitudinal waves in thin bars, a solution must be obtained for the following ﬁrst order quasi-linear system, containing three unknown functions σ, v and ε ∂ε ∂σ = ϕ(σ, ε) + ψ(σ, ε) , ∂t ∂t ∂v 1 ∂σ = , ∂t ρ ∂ε

(4.2.4)

∂v ∂ε = . ∂x ∂t The second equation is the equation of motion and the third one the compatibility equation; v is the particle velocity, and ρ is the constant density. The system (4.2.4) possesses three families of characteristic curves dx/dt = ±c(σ, ε) = ± ϕ(σ, ε)/ρ , (4.2.5) and dx = 0 .

(4.2.6)

Along the curves (4.2.5) the diﬀerential relations dσ = ±ρc(σ, ε) dv + ψ(σ, ε) dt

(4.2.7)

are satisﬁed while along the lines (4.2.6) are satisﬁed the relations dσ = ϕ(σ, ε) dε + ψ(σ, ε) dt .

(4.2.8)

Thus the system (4.2.4) is totally hyperbolic. Instead of integrating the system (4.2.4) it is possibly to integrate the equivalent diﬀerential relations (4.2.7) and (4.2.8) along the characteristic curves (4.2.5) and (4.2.6) respectively. The upper and lower signs correspond to each other. In the problem considered a perturbation produced at the end of the bar will propagate along the bar by waves whose velocity is c(σ, ε). There will be some stationary discontinuities [Eq. (4.2.6)]. In order to analyze such phenomena in detail, the dynamic and kinematics compatibility conditions must be taken into account. If [F ] is used to denote the jump of a certain function F across a wave front the compatibility conditions are ∂ε ∂σ ∂σ ∂σ =ϕ , dx + dt = 0 , ∂t ∂t ∂x ∂t 1 ∂σ ∂v ∂ε ∂ε (4.2.9) = , dx + dt = 0 , ∂t ρ ∂x ∂x ∂t ∂v ∂ε ∂v ∂v = , dx + dt = 0 . ∂x ∂t ∂x ∂t

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

Rate Inﬂuence

dynamic

181

The left three relations are obtained from Eqs. (4.2.4). The remaining three relations express the condition that the interior diﬀerentials dσ, dε and dv are continuous across a wave front. From Eq. (4.2.9) it follows that across any line (4.2.5), the derivatives of σ, ε and v are discontinuous while across a line (4.2.6) all the derivatives in the system (4.2.4) are continuous except the derivatives ∂ε/∂x which may be discontinuous. It should be noted that the function ϕ(σ, ε), corresponding to the instantaneous response of the material, is the only function involved in the expressions for the velocity of propagation and the dynamic compatibility conditions. The function ψ(σ, ε) describing the non-instantaneous response or time eﬀects is only involved in the diﬀerential relations (4.2.6) and (4.2.7). Depending on the explicit expression of the function ϕ(σ, ε), the velocity c(σ, ε) can increase or decrease when the stress is varying. For the integration method, we assume the bar to be of length l and at time t = 0 the ends of the bar are at x = 0 and x = l. The boundary conditions must be formulated as follows: at x = 0

and t > 0 ,

we know either v(0, t) or σ(0, t) .

(4.2.10)

and t > 0 ,

we know either v(l, t) or σ(l, t) .

(4.2.11)

Similarly: at x = l

The initial conditions are: at t = 0 and 0 ≤ x ≤ l

we know v(x, 0), σ(x, 0) and ε(x, 0) .

(4.2.12)

If the bar is initially at rest or moving rigidly then the functions prescribed by the conditions (4.2.12) are known along the characteristic line of positive slope passing through x = 0 and along the characteristic line of negative slope passing through x = l, i.e., along the ﬁrst wave fronts which propagate in the bar. Otherwise one must ﬁrst solve a Cauchy initial value problem, and then pass to the Goursat problem in the corners. If the striking body moves with respect to the material points of the bar, then a mixed boundary value problem must be solved in a domain with a ﬂoating boundary. That was the case with the initial tests done in dynamic plasticity. In this case the impacting body must move along the bar with a velocity smaller than the velocity of the waves. 4.3

Instantaneous Plastic Response

In the previous section it was assumed that during the entire process of elasticviscoplastic deformation a single constitutive equation written in quasi-linear diﬀerential form could be used. This procedure can generally be used for plastics, certain soils or rocks, rubbers, certain metals, etc. However, in some problems for

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

182

Dynamic Plasticity

Fig. 4.3.1

Stress–strain relationship for ψ = 0.

some materials, especially for the majority of metals, the total strain is always composed of two components: the elastic reversible component and the plastic irreversible one (Fig. 4.3.1), with the total strain bigger than 0.2% say: (4.3.1) ε = εE + εP E where ε = σ/E. Both components increase during the loading of a work-hardening material, but each of them corresponds to diﬀerent physical phenomenon and is therefore related to the stress by diﬀerent constitutive equations, though of course these two phenomena are very tightly interconnected. It should also be noted that the plastic part of the strain is in fact a visco-plastic component. Thus, there is no longer any question of a one-to-one correspondence between stress and strain, even in the loading process. The stress–strain relation is certainly not unique, since it depends on the loading rate. Thus, in this case the plastic part of the strain has a more general meaning than in classic inviscid plasticity theory. The exact deﬁnition, of the elastic component of the strain, can only be given when unloading is deﬁned. Let us now examine the constitutive equation for elastic-plastic work-hardening materials (Cristescu [1963]). If, at a point A in the plastic region (Fig. 4.3.1) the stress is increased by an amount ∆σ, this impulse will propagate in the bar and produce an increase ∆εE of the elastic part of the strain and an increase ∆εP of the plastic part of the strain. The former will be related to the stress increment by Hooke’s law, which will be written in a diﬀerential form

dynamic

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

dynamic

Rate Inﬂuence

183

∂σ/∂t = E(∂εE /∂t) .

(4.3.2)

The plastic component of the strain increment is generally related to the stress increment by a quasi-linear diﬀerential relation of the form ∂εP ∂σ = ϕ(σ, ε) + ψ(σ, ε) , (4.3.3) ∂t ∂t where the functions ϕ and ψ may depend on some other constants describing the mechanical properties of the material (yield limit, viscosity coeﬃcient, workhardening modulus, etc.). We assume that ϕ > 0. If the material is in elastic state, only elastic waves will propagate with the velocity (4.3.4) cE = E/ρ . If the material is plastic/rigid only constitutive equation (4.3.3) is added to the equation of motion. In this case, only pure plastic waves will propagate, the velocity of their fronts being (4.3.5) cP = ϕ(σ, ε)/ρ . If however, the material is elastic-plastic, the following system of equations will govern the motion ∂σ ∂εE −E = 0, ∂t ∂t ∂εP ∂σ − ϕ(σ, ε) = ψ(σ, ε) , ∂t ∂t

(4.3.6)

∂v ∂εE ∂εP − − = 0, ∂x ∂t ∂t ∂v ∂σ − = 0. ∂t ∂x The characteristic curves of the system are dx/dt = ±c(σ, ε) = ± ϕE/ρ(ϕ + E) , ρ

(4.3.7)

and dx = 0

(twice) .

(4.3.8)

Along the characteristics (4.3.7) the diﬀerential relations dσ = ±ρc{±(ψ/ϕ)} cdt + dv

(4.3.9)

are satisﬁed, while along the lines (4.3.8) are satisﬁed the relations dσ = EdεE , dσ = ϕ(σ, ε) dεP + ψ(σ, ε) dt .

(4.3.10)

The upper and lower signs in (4.3.7) and (4.3.10) correspond to each other.

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

184

dynamic

Dynamic Plasticity

Fig. 4.3.2

A dynamic stress–strain curve showing the “overstress”.

Three separate propagation velocities play a part in this problem: cE , cP and the velocity c of the elastic-plastic waves. These three velocities are clearly related as follows: 1 1 1 = 2 + 2 . c2 cE cP

(4.3.11)

This formula can also be written in the form c cP = . 1 − c2 /c2E

(4.3.12)

Thus, the velocity of the elastic waves cE can be considered as a “limiting velocity” for the elastic-plastic waves. It is the highest possible velocity of propagation in the material considered and an invariant of the wave propagation phenomenon. From (4.3.12) it follows immediately that cP ∼ = c when c cE . This formula can be used to ﬁnd cP , if c and cE are obtained by measurements. Generally we have c E > cP ≥ c . The equality cP = c holds when the material is plastic/rigid and work-hardening. In this case c2 = E1 (σ, ε)/ρ, where E1 (σ, ε) is the variable work-hardening modulus. A dynamic stress–strain curve showing the possible variations during tests is shown in Fig. 4.3.2. The overstress is something composed of several components. Interesting information can be obtained from the dynamic and kinematics compatibility conditions

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

Rate Inﬂuence

E ∂ε ∂σ −E = ∂t ∂t P ∂ε ∂σ −ϕ = ∂t ∂t E P ∂ε ∂ε ∂v − − = ∂x ∂t ∂t ∂σ ∂v − = ρ ∂t ∂x

185

0, 0, 0, 0,

∂σ ∂σ dx + dt ∂x ∂t E E ∂ε ∂ε dx + dt ∂x ∂t P P ∂ε ∂ε dx + dt ∂x ∂t ∂v ∂v dx + dt ∂x ∂t

dynamic

= 0, = 0, (4.3.13) = 0, = 0.

From (4.3.13) it follows that across the characteristic lines (4.3.7) all the derivatives involved in the system (4.3.13) are discontinuous. Thus (4.3.7) are wave fronts which aﬀect all the unknown functions and certainly both parts εE and εP of the strain. Across the lines (4.3.8) all the derivatives except for the derivatives ∂εE /∂x and ∂εP /∂x are continuous. From (4.3.13) we may easily obtain: c2E [∂εE /∂t] = c2P [∂εP /∂t] .

(4.3.14)

This is the relation between the jump of the derivatives of the two components of the strain, and the velocities of propagation cE and cP . Since in the majority of cases, c2E c2P , it follows that [∂εE /∂t] [∂εP /∂t], and thus in many cases, if the material is in an elastic-plastic state and the work-hardening modulus is much smaller than the elastic modulus, the elastic part of the discontinuity carried by the elastic-plastic wave, can be neglected in comparison with the plastic part. Since cE = const., all the considerations concerning the relation (4.3.14) depend only on the function ϕ(σ, ε). We shall now discuss the special case when ψ = 0. In this case the diﬀerential relations (4.3.9) reduce to the well-known relations dσ = ±ρ cdv , while from (4.3.10) it follows that EdεE = ϕ dεP . Since in general E ϕ, it again follows that dεE dεP along (4.3.8). This relation or its equivalent dε = (1 + ϕ/E) dεP represents the relation between the increments of the components of the strain in the case ψ = 0. If ψ = 0 the relation between the components of the strain along (4.3.8) is more complicated and follows directly from (4.3.10) ψ ϕ P dε + dt . dε = 1 + E E

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

186

Dynamic Plasticity

This relation can also be used to examine cases when certain components or the time inﬂuence can be neglected. It may be obtained directly from the ﬁrst two relations (4.3.6) by eliminating ∂σ/∂t. The conclusions are the following. If the constitutive (4.3.2) and (4.3.3) are used, then both the elastic and plastic components of the strain propagate by the same type of wave with the velocity (4.3.7). However both components also possess stationary discontinuities. It should be remembered that the plastic constitutive equation (4.3.3) involves both instantaneous and non-instantaneous plastic response terms. A similar theory for elastic-plastic-viscoplastic stress waves was developed also by Tanimoto [1994]. The endochronic theory of plasticity to show the eﬀect of the strain rate on the inelastic behavior of structural steel under cyclic loading condition is formulated by Chang et al. [1989]. From the endochronic theory (Valanis [1972]) one is taking dζ 2 = Pijkl dεpij dεpkl − g 2 dt2 . By using a 4th order isotropic tensor for P the previous relation can be written f 2 dZ 2 = h2 dεpij dεpkl − g 2 dt2 , and this equation can by written as g 2 dt2 = F 2 f 2 dZ 2 in which

F =

h2

− α )(σ − α ) (σij ij ij ij − 1. (s0y f )2

The viscoplastic ﬂow condition, equivalent to the overstress of viscoplasticity is (σij − αij )(σij − αij ) h2 −1 > 0. 0 2 (sy f ) All the other not explained notations are constants. The authors are also making some comparison of the analytical solutions and the experimental results. The same problem was considered experimentally by Zhao [1997]. The classical split Hopkinson pressure bar tests are used, together with the yield stress dependency on strain rate and temperature ε˙ Q σY = A ln + T ε˙0 RT where A, Q, R are constant coeﬃcients and T is the absolute temperature. Sets of tests of 230 s−1 to 1650 s−1 were considered for specimens of diameter 10 mm and length 10 mm. The results are shown in Fig. 4.3.3. The aluminum 1100-0 was tested by Pao and Gilat [1989]. They were tested for the plastic strain rate sensitivity with temperature as ∗ τ − τ ∗ ) σij v (¯ H0 sinh ε˙P = 2η exp − ij kT kT τ¯

dynamic

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Rate Inﬂuence

dynamic

187

Fig. 4.3.3 Comparison between stress–strain curves derived from real tests and those from simulated tests.

were H0 , η, v ∗ , and τ ∗ are determined from results of tests in which the material is deformed at various constant strain rates and temperatures. At T = 0, τ¯ = τ ∗ + H0 /v ∗ . Other values of material constants are given. They have used the same boundary conditions as given below and the results are given in Fig. 4.3.4. Comparison with the tests of Bell is done on three distances from the impacted end. The comparison seems good. The existence and properties of the free energy function compatible with the second law of thermodynamics in one-dimensional rate-type semilinear viscoelasticity is analyzed by Faciu and Mihailescu-Suliciu [1987]. Necessary and suﬃcient conditions are given such that a free energy as a function of strain and stress exists and is unique, that it is non-negative function and possesses a monotony property with respect to the equilibrium curve. A bound in energy for the smooth solutions of certain initial and boundary value problems with respect to the input data is established when the equilibrium curve is a non-monotonic curve. Bounds in energy for the smooth solutions of initial and boundary value problems for semi-linear hyperbolic systems were given by Fˇaciu and Simion [2000]. They prove that the integral energy identities for smooth solutions are still valid for weak solutions. Energy estimates of the weak solutions of the same problems are given. The way weak and strong discontinuities in the input data aﬀect the regularity of the total energy of the solution is discussed. The uniqueness of the weak solutions is derived.

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

188

Dynamic Plasticity

Fig. 4.3.4

Variation of strain with time at three indicated distances.

A nonhomogeneous and nonautonomous 2 × 2 quasilinear system of ﬁrst order describing rate-type materials is considered by Manganaro and Valenti [1993] within the framework of similarity reduction procedures. The constitutive equation is of the form ∂ε ∂v = φ(v, ε) + ψ(v, ε) . ∂t ∂t Classes of exact similarity solutions to the governing model as well as functional forms for the material response function involved have been determined. Reduction to linear form have been carried out for diﬀerent forms of constitutive laws. In another article by Menganaro and Meleshko [2002], the method of diﬀerential constrains is applied for systems written in Riemann variables. Generalized simple waves are considered. This class of solutions can be obtained by integrating a system of ordinary diﬀerential equations. The above rate-type models is one of the systems studied.

dynamic

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Rate Inﬂuence

dynamic

189

A constitutive law of the form ˙ + G(σ, ε(u), β) σ˙ = Eε(u) where E is a fourth order tensor, and β is the damage ﬁeld was considered by Chau et al. [2002]. When β = 1 the material is undamaged, while the value β = 0 indicates the stage of complete damage. The mechanical damage of the material, caused by excessive stress or strain, is described by a damage function whose evolution is modeled by an inclusion of parabolic type. The authors provide a variation formulation for the mechanical problem and sketch a proof of the existence of a unique weak solution to the model. They introduce and study a fully discrete scheme for the numerical solutions of the problem. An optimal order error estimate is derived for the approximate solutions under suitable solution regularity. Numerical examples are presented to show the performance of the method. The contact problems considered by Fern´ andez et al. [2003] involve the large class of elastic-viscoplastic materials. They focus on the ﬁnite element approximations which involve nonmatching meshes on the contact part. Such a conﬁguration in which the nodes inherited from the discretizations of the bodies may not coincide arises in computational situations when the diﬀerent bodies are independently meshed and/or there is an initial distance between the bodies and/or an evolution process is considered. The ﬁrst aim of the authors is to study the convergence of ﬁnite element methods and then to carry out the numerical experiments associated with the theoretical studies. A simply non-linear anelastic model describing the acceleration of the relaxation process in the presence of vibrations was considered by Dr˘ag˘anescu and C˘ap˘ aln˘ a¸san [2003]. An analytic variational iteration method is used in order to study the relaxation process. Also a method of identiﬁcation of the parameters of the system from the experimental data is given.

4.4

Numerical Examples

In the numerical examples of the rate-type constitutive equations under consideration were used in the form 1 + χΦ(σ, ε) σ˙ + Ψ(σ, ε) , (4.4.1) ε˙ = E with χ=

0

if σ ≤ f (ε) or σ˙ < 0 ,

1

if σ = f (ε) and σ˙ > 0 .

(4.4.2)

The coeﬃcient χ is used so that the constitutive equation is used during loading and unloading.

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

190

dynamic

Dynamic Plasticity

The characteristic lines are dx E = ±c(σ) = , dt ρ(1 + EΦ)

(4.4.3)

dx = 0 , the diﬀerential relations satisﬁed along them dσ = ±ρcdv − ρc2 Ψ(σ, ε) , dσ = EdεE ,

(4.4.4)

dεP = Φ(σ, ε) dσ + Ψ(σ, ε) dt . The coeﬃcient function Ψ(σ, ε) describing the non-instantaneous response was assumed to depend linearly on the overstress (Cristescu [1972a, 1972b], Cristescu and Cristescu [1973]): k(ε) [σ − f (ε)] if σ > f (ε) and ε ≥ σ , E E (4.4.5) Ψ(σ, ε) = 0 if σ ≤ f (ε) . For the relaxation boundary we write f (ε) =

if ε ≤ εY ,

σY 1/α

β(ε + ε0 )

(4.4.6)

if ε > εY

or some variants of this law. The examples given are for aluminum (1100◦F aluminum annealed for two hours at 590◦ C and then furnace cooled — see Bell [1968]). For this material the relations σ = Eε 1/α

σ = β(ε + ε0 )

if

σ ≤ σY ,

if

σ > σY

were used, where E = 7038000 N/cm2 and ρ0 = 2.7 g/cm3 , and therefore c0 = 5080 ms−1 . For the other constants, the following numerical values were used (Cristescu and Bell [1970] and Cristescu [1972b]): for the quasi-static stress–strain curve, 8 2 2 σY0 = 703.80 N/cm , β = 22908.0 N/cm , α = ; 3 for the dynamic stress–strain curve, 2

σY1 = 212.18 N/cm ,

2

β = 38640.0 N/cm ,

α = 2;

for the translated dynamic stress–strain curve, 2

σY2 = 759.00 N/cm ,

2

β = 38640.0 N/cm ,

α = 2,

ε0 = 0.000278 .

The true yield stress for the aluminum under consideration is in fact, and the stress– strain curve is obtained from the dynamic one by a translation along the strain axis (this deﬁnes ε0 ). The stress–strain curve obtained by this procedure is quite close to the dynamic one.

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Rate Inﬂuence

dynamic

191

The expression for k is an expression showing a small value for small strains but becomes greater, nearly constant, for higher values. Thus * ε + (4.4.7) k(ε) = k0 1 − exp − ε¯ with k0 and ε¯ material constants. Various variants of this constitutive law were used. Concerning the slope of the instantaneous curve we assume that it lies between the elastic slope and that of the relaxation boundary E≥

1 > f (ε) . Φ(σ, ε) + 1/E

(4.4.8)

Further Φ(σ, ε) was chosen to match a certain set of experimental data. Two forms were used. Starting from a cubic equation we have used Φ(ε) = χ

3[ε − εY − ε∗ + (a/3E)3/2 ]2/3 1 − , a E

where √ a=m+n ε with m, n material constants and ε∗ is a threshold strain. Some other value is # $ 3 E γ σ 2 √ 3 Φ(σ, ε) = χ −1 E p+q ε E where p, q and γ are material constants. It is quite diﬃcult to determine the velocity of propagation experimentally, and thus Φ. The numerical examples are for the impact of two bars, the “hitter” and the “specimen”. For the specimen we have t = 0,

0<x≤l:σ=ε=v=0

for the initial conditions. For the boundary conditions the end of the bar x = l is assumed free t ≥ 0,

x = l : σ = 0.

At t = 0 the bar is impacted at the end x = 0 by another bar identical with the specimen. Thus, for the hitter we have t = 0,

−l ≤ x < 0 : σ = ε = 0 ,

v=V .

Thus for t = 0 the end x = 0 of the specimen is subjected to a sudden jump. This jump was handled in two ways. First, it was assumed that the impact velocity is fast but smoothly transferred to the end of the specimen. A convenient very short time interval 0 ≤ t < tm was chosen, in which this smooth increase of velocity at the impacted end of the specimen takes place from zero up to vmax . For simplicity, it

January 12, 2007

10:41

192

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Dynamic Plasticity

Fig. 4.4.1

Variation of the strain at various sections along the bar, and time of contact.

was assumed in the program that the velocity at the end of the specimen increases according to a linear law. Thus, the ﬁrst kind of boundary conditions were t 0 ≤ t < tm : v = vmax , t m x=0 t ≤t≤T :v =v , m c H S Tc < t : σS = 0 , where tm is a conveniently chosen time interval (in most examples given here tm = 0.5 µs) and vmax = V /2. Tc is a computed time, called time of contact. In the time interval tm ≤ t ≤ Tc the ends x = 0 of the two bars are moving together. σS is the specimen stress which is computed as is Tc . Several examples have been computed. In Fig. 4.4.1 is given the variation of the strain at various sections along the bar. Also have been given also the time of contact and a classical solution. One can see that the rate type solutions are quite correct. In Fig. 4.4.2 is given the variation of the stress at the impacted end. After a peak, follows a plateau. Again the experimental data are quite well reproduced. The decrease of the stress is due to unloading. In Fig. 4.4.3 is shown the variation of the deformation at the 9D, i.e., close to the free end, while in Fig. 4.4.4 is given the variation of the displacement in time at various cross-sections. From the above one can see that a plateau for strains can be predicted for a ﬁnite distance (Suliciu [1972]). Daimaruya and Naitoh [1983] have also considered

dynamic

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

Rate Inﬂuence

Fig. 4.4.2

Variation of the stress at the impacted end.

Fig. 4.4.3

Variation of the strain in time at 9D.

dynamic

193

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

194

Dynamic Plasticity

Fig. 4.4.4

Comparison of the displacement-time curves.

the plateau problem; they have shown numerically taking the model (4.2.2) for hardened aluminum f (ε) = 6.89(20 − 0.01/ε) MPa, with the values of the constants E = 68.8 GPa, ρ = 2.67 × 103 kg/m3 , k = 106 sec−1 and impact velocity V = 15 m/sec, that a plateau of uniform strain adjacent to the impact end can exist. For larger value of k, the plateau will be shorter. Various variants of the constitutive equation as well as examples are considered by Cristescu and Suliciu [1982]. For instance ˙ + G(σ, ε(u), β) σ˙ = Eε(u) where β is a function which satisﬁes an ordinary diﬀerential equation as β˙ = ϕ(σ, ε(u), β) , (see Ionescu and Sofonea [1993], Fern´andez [2004]). Some other authors (Luo et al. [2003]) have used the same model to introduce the isothermal rheological forming of high-strength alloying parts with complicated curved surface. They have used various speeds and found that for the lower forming velocity (v = 0.022 mm/s) the non-uniformity of temperature ﬁeld is smaller than at higher speeds.

4.5

Other Papers

A ﬁrst study about the eﬀect of temperature gradients on the propagation of elastoplastic waves is due to Francis and Lindholm [1968]. It is question of the propagation

dynamic

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Rate Inﬂuence

dynamic

195

of an extensional elastoplastic wave through a long thin bar heated at the end to produce a continuously decreasing temperature proﬁle. The temperature distribution is approximated as an exponential function. Analytical solutions are obtained by Shaw and Cozzarelli [1971] for stress, velocity, and strain at the wave front in a suddenly loaded semi-inﬁnite rod of a material with a linear instantaneous response and nonlinear inelastic response. The material properties are assumed to depend on position directly or through a dependence on a prescribed non-uniform temperature ﬁeld. Detailed solutions are obtained for two examples, a nonlinear viscoelastic material with temperature dependent parameters and a rate-sensitive plastic material which may have temperature dependent parameters and yield point. The dynamic mechanical behavior of titanium in shear was studied by Lawson and Nicholas [1972]. They have used a constitutive equation of the form ∂τ ∂γ = + g(τ, γ) . ∂t ∂t They found that the torsional plastic waves in pure titanium can be predicted from the rate-dependent theory of plastic wave propagation. The excellent agreement between theoretical and experimental results for stresses at the end of a long tube subjected to a torsional pulse demonstrates the consistency of the entire testing procedure. The problem of impact on a nonlinear viscoelastic rod of ﬁnite length is considered by Mortell and Seimour [1972]. They have considered a constitutive law of the form G

σ˙ = φ(ε)ε˙ + ψ(σ, ε) . It is shown that, in the high frequency or geometrical acoustics limit, the disturbance in the rod may be represented as the superposition of two modulated simple waves traveling in opposite directions which do not interact in the body of the material. A comparison with the experiments is done by Kuriyama and Kawata [1973]. They consider three types of constitutive equation; that is, the Karman-type theory, the Malvern-type theory, and the Cristescu-type theory. The constitutive equation is written E ε˙ − σ˙ = h(σ, ε) . They ﬁnd that the front of the stress wave travels always with the elastic-wave velocity and the plateau of the uniform plastic strain remains in the neighborhood of the impact end. They ﬁnd that the Johnston–Gilman-type of constitutive equation is matching better. Suliciu et al. [1973] have developed a class of general solutions for wave propagation in a rate-type material. These solutions, obtained by invoking equation splitting, demonstrate elastic-like behavior for the kinematics variables u and ε although the material is inelastic. This observation serves as a warning to those carrying out dynamic experiments involving only axial loadings. Measurements of

January 12, 2007

196

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Dynamic Plasticity

strain and velocity may not reveal the true characteristics of materials. An extended solution for transverse motion is presented and experiments involving transverse deﬂection are highly recommended because these results do provide information about σ and therefore the rate dependencies. A one-dimensional problem has been considered by Nicholson and Phillips [1978]. They have considered elastic/viscoplastic/plastic materials of the form σ˙ σ σ˙ + + η σ − σ0 − k ε − ε˙ = E0 Ep E0 where σ0 are the quasi-static yield stress and all the other are constants. Various variants of the constitutive equation are considered for stress impact and velocity impact. Then the Laplace transform is used, and near the impact end the solution is obtained in terms of some special functions. For an elastic/viscoplastic material, a region of uniform strain arises at the impact end more rapidly for velocity impact than for stress impact. Also for an elastic/viscoplastic/plastic material, the plastic strain makes no contribution at the impact end for velocity impact, but it does for stress impact. For aluminum and copper rods, for a wide range of striking velocities and rods lengths, the general applicability of one-dimensional non-viscous dynamic plasticity theory is conﬁrmed (Dawson [1972]). A model of the kind used in this chapter vas proposed by Suliciu [1981] to describe the Savart–Masson eﬀect by a rate-type constitutive equation. The viscosity coeﬃcient has strong variations in some regions of the stress–strain plane that lie above the equilibrium curve σ = f (ε). Cernocky [1982] has considered four constitutive equations of viscoplasticity and made a comparison between them. Each theory is ﬁtted to the same stress– strain data, and both analytical and numerical methods are employed to highlight similarities and diﬀerences between their predictions. Diﬀerent manifestations of strain-rate and stress-rate history eﬀects predicted by the theories are compared, and the theories are shown to share a signiﬁcant qualitative bias between responses to stress and strain-controlled loading. Some dynamic tests on aluminum titanium and steel were done by Nicholas [1981]. He has found a rate sensitivity of 10 to 102 s−1 . In another papers Nicholas et al. [1987a, b] a ﬁnite diﬀerence computer code is used to numerically simulate uniaxial strain waves generated from plate impact experiments. The incremental ﬂow law of Bodner and Partom and the Perzyna law are compared with experiments. Numerical computations using a ﬁnite diﬀerence computer code illustrate that the decay of the amplitude of the propagating precursor elastic wave is a consequence of material strain-rate dependence. The possibility of describing rubber-like materials by means of a rate-type viscoelastic constitutive equation is due to Mihailescu-Suliciu and Suliciu [1987]. The problem of generation of one-dimensional tensile shock waves in rubber-like materials is studied numerically and compared to the exact elastic nonlinear solution and the steady wave solution. It is shown that a rate-type semilinear visco-elastic

dynamic

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Rate Inﬂuence

dynamic

197

model can describe the steepening of the wave during its propagation and a “thickness” of the wave is naturally incorporated. An energetic criterion for the numerical stability is also introduced. An experimental technique is described by Chhabildas and Swegle [1989] which uses anisotropic crystals to generate dynamic pressure-shear loading in materials. The coupled longitudinal and shear motion generated upon planar impact of anisotropic crystal can be transmitted into a specimen bonded to the rear surface of crystal, and monitored using velocity interferometer techniques. In a paper by Li and Clifton [1981] one is presenting stress–strain curves for aluminum sandwiched between hard steel plates. The shear strain rates go up to and sustain these rates for a duration of 10−6 s. These stress–strain curves are much higher than the classical ones. Damage is considered by Ziegler [1992] to be a time-variant imperfection of the yielding material, analogously to the growth of porosity of a voided material with given initial porosity. Also plastic strain is a distortion of the perfect elastic background structure. The internal variable approach is transformed into a numerical routine of computational dynamic viscoplasticity. Starting from the phenomena not well described as the increase of stress with strain rate, the propagation speed of the stress wave corresponding to a large strain is slow, and others, Tanimoto et al. [1993] try to explain it by introducing an elasticplastic-viscoplastic constitutive equation of the form ρ

∂σ ∂v = , ∂t ∂x ∂v ∂ε = , ∂x ∂t k2 k1 ∂σ 1 2 σE 2 σ + − 1 + − 1 σ, ∂ε E 3ζ σ ∂t 3η σS = ∂t 1 ∂σ , E ∂t

σ > σS σ ≤ σS ,

with the various constants given as: E = 103.5 GPa, σS = 102.4 MPa, ζ = 11.77 MPa, η = 1.177 × 103 Pa s, k1 = 0.85, k2 = 5.4, ρ = 8.391 × 10−9 kgr/mm3 . The approach is also numerical, as given above. Several ﬁgures are given to show the eﬀect. We give only two. In Fig. 4.5.1 is given the variation of stress in the distance from the impact end. In Fig. 4.5.2 is given the variation of strain with distance from the impacted end. Close to the impacted end the strain is constant (plateau) and this value is increasing in time. That is not in agreement with the tests, but the authors are trying to ﬁnd various arguments. An approach is developed to generate exact solutions to a hyperbolic model of the form ut + vx = 0 ,

vt + h(v)ux = f (v)

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

198

Dynamic Plasticity

Fig. 4.5.1

Stress-distance relationship.

Fig. 4.5.2

Strain-distance relationship.

by Fusco and Manganaro [1994a]. The leading idea of the analysis which is carried on herein is to require the model in point to be considered with a pair of additional equations deﬁning Riemann invariants-like quantities along the characteristic curves. Hence, classes of model constitutive laws allowing a reduction procedure to hold are characterized. Later on, a nonhomogeneous system of partial diﬀerential equations of ﬁrst order involving two dependent and two independent variables is considered also by Fusco and Manganaro [1994b]. The same authors (Fusco and Manganaro [1996]) consider the system ut − vx = 0 ,

εt − u x = 0 ,

vt − φ(t, ε, v)ux = ψ(t, ε, v)

for which solutions are given. The same kind of equations vas also considered by Tabov [1996]. He obtains easy to verify criterion for the existence of such solutions and clearly stated conditions on the initial data providing the existence and uniqueness of the solutions. The system vt − σx = 0 ,

σt − φ(t, σ)vx = ψ(t, σ)

is proposing to be reduced to linear form 2 × 2 non-homogeneous and nonautonomous ﬁrst order quasi-linear systems by Curr`o and Valenti [1996]. The system

dynamic

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Rate Inﬂuence

dynamic

199

through the use of a variable transformation is reduced to a homogeneous and an autonomous form which can be linearized by means of hodograph transformation. A general algorithm of implicit stress integration in viscoplasticity is presented by Kojic [1996]. The algorithm is ﬁrst applied to isotropic metals obeying the von Mises yield condition with mixed hardening and then to orthotropic metals. A theory of viscoplasticity bounded between two distinct rate-independent generalized plasticity models was considered by Auricchio [1997]. Main features of the model are the following: (1) it approaches the two rate-independent generalized plasticity models for the case of fast and slow loading conditions, respectively; (2) it properly describes loading-unloading-reloading conditions for any loading rate; (3) it reproduces the experimentally observed diﬀerence between the dynamic and the static yielding conditions. One has in mind metals, polymers, geomaterials, and shape-memory alloys. Both the time-continuous and the time-discrete version of the model are discussed. Several examples are given. The main objective of the paper by Lodygowski and Perzina [1997] is the investigation of adiabatic shear band localized fracture phenomenon in inelastic solids during dynamic loading processes. This kind of fracture can occur as a result of an adiabatic shear band localization generally attributed to a plastic instability implied by micro-damage and thermal softening during dynamic plastic ﬂow processes. A review is presented by Klepaczko [1998] on recent progress in shear testing of materials at high and very high strain rates. Some experimental technique are discussed which allow for materials testing in shear up to 106 1/s. More information is provided on experimental techniques based on the Modiﬁed Double Shear specimen loaded by direct impact. This technique has been applied so far to test a variety of materials, including construction, armor and inoxidable steels, and also aluminum alloys. The double shear conﬁguration has also been applied to test sheet metals, mostly used in the automotive industry, in a wide range of strain rates. A new experimental conﬁguration which can be applied for experimental studies of adiabatic shear propagation and high speed machining is discussed. One is also showing that for steel at lower impact velocities, the energy to the ﬁnal localization increases up to 681 MJ/m3 ; however, at impact velocities higher than 100 m/s, the energy drops considerably, to the value of ∼ 8.0 MJ/m3 . Thus, the energy drop is slightly less than a hundred times. Results of pressure-shear plate impact experiments on an alumina ceramic (AD85) containing a signiﬁcant amount of an oxide glass phase were done by Sundaram and Clifton [1998]. Under high strain-rate loading, the ceramic (porosity of approximately 9%) shows low shear strength and a strong strain softening behavior. The material is modeled as an elastic-visco-plastic solid. The collapse of the voids causes a strong hydrostatic relaxation which brings down the pressure. A ﬁnite element technique is presented by Yokoyama [2001] for the analysis of one-dimensional torsional plastic waves in thin-walled tube. Three diﬀerent nonlinear constitutive relations deduced from elementary mechanical models are used

January 12, 2007

200

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Dynamic Plasticity

to describe the shear stress–strain characteristics of the tube material at high rates of strain (103 s−1 ). It is question of elasto-plastic model of Karman-Duwez, the elasto-viscoplastic model of Sokolovsky–Malvern and the elasto-viscoplastic-plastic model of Cristescu–Lubliner. The resulting incremental equations of torsional motion for the tube are solved by applying a direct numerical integration technique in conjunction with the constitutive relations. A comparison with experimental results shows that the strain-rate dependent solutions show a better agreement with the experimental results than the strain-rate independent solutions. The superplastic deformation and cavitations damage characteristics of a modiﬁed aluminum alloy are investigated at a temperature from 500 to 550◦ C by Khaleel et al. [2001]. The experimental program consists of uniaxial tension tests and digital image analysis for measuring cavitations. The experiments reveal that evolution of damage is due to both nucleation and growth of voids. A viscoplastic model for describing deformation and damage in this alloy is developed based on a continuum mechanics framework. The model includes the eﬀect of strain hardening, strain rate sensitivity, dynamic and static recovery, and nucleation and growth of voids. Altenhof and Ames [2002] study the strain rate eﬀects for aluminum and magnesium steering wheel armatures when they are subjected to dynamic impact tests. Two geometrically diﬀerent steering wheel armatures, a three spoke proprietary aluminum alloy armature and a four spoke magnesium alloy armature, underwent experimental impact testing. The strain rates are not very high: 17 s−1 for aluminum and 46 s−1 for magnesium armature. Stress–strain response under constant and variable strain-rate is studied for selected models of inelastic behavior by Lubarda et al. [2003]. The derived closedform solutions for uniaxial loading enable simple evaluation of the strain-rate eﬀects on the material response. Various one-dimensional models have been written. In the case of parabolic hardening, the ﬂow stress is related to the plastic strain εp εp p σ−Y) p 2− p σ = Y + (ˆ εˆ εˆ where Y is the initial yield stress, and εˆp is the plastic strain at the apex of the plastic stress–strain curve with the stress σ p . For the hyperbolic type of hardening we have Yˆ − Y . σ p = Yˆ − 1 + εp /ˆ εp For viscoelastic-plastic model, the stress is Eε , σ = σ ∗ 1 − exp − ∗ σ

ε=−

σ σ∗ ln 1 − ∗ . E σ

In Fig. 4.5.3 are given three curves corresponding to this case. Here σ ∗ = η ε˙ with η the viscosity coeﬃcient. In a similar way one has considered several curves including the viscoelastic-elastoplastic model.

dynamic

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Rate Inﬂuence

dynamic

201

Fig. 4.5.3 The stress–strain curves for viscoelastic-plastic model in the case of parabolic hardening.

The split Hopkinson pressure bar, or Kolsky’s apparatus was re-analyzed by Zhao and Gary [1996] and by Zhao [2003]. The same system of equation 1 ∂σ ∂ε = ∂t E ∂t

if σ ≤ σs ,

1 ∂σ ∂ε = + g(σ, ε) ∂t E ∂t

if σ > σs

is used with g(σ, ε) =

(1 + Et /E) σ − σs − Et ε . η

He is proposing to calculate directly the dispersive relation for the wave dispersion corrections and to use the elastic simulation to determine more accurately correspondence between the wave beginnings. A method to increase measuring duration is proposed. An identiﬁcation technique, especially for non-metallic materials, based on an inverse calculation method is also presented. The Kolsky torsion bar was used by Hu and Feng [2004] to study the behavior of polymer melts at high shear rates from 102 s−1 to 104 s−1 and temperature up to 300◦C. To give an example on Fig. 4.5.4 is given one case considered. The important inﬂuence of the strain rate is evident. Constitutive modeling of the high strain rate behavior of interstitial-free steel was considered by Uenishi and Teodosiu [2004]. The strain rates are quite high of 1000 s−1 . To have an idea, we reproduce in Fig. 4.5.5 several curves from that paper. In order to simulate the high strain rate tensile test, and that of temperature, the Johnson–Cook model is used m T − Troom ε¯˙ 1− σ ¯ (¯ ε, ε¯˙, T ) = (A + B ε¯n ) 1 + C ln ε˙0 Tref − Troom

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

202

Dynamic Plasticity

Fig. 4.5.4

Shear stress proﬁles for various shear rates and 190◦ C initial temperature.

where σ ¯ , ε¯ and ε¯˙ are the equivalent tensile stress, the equivalent tensile strain and the equivalent tensile strain rate, respectively. The ﬁrst term represents the work hardening behavior at the reference strain rate ε˙0 and at the room temperature. The second and third terms express the eﬀects of strain rate and temperature, respectively. The parameters A, B, n, C and m are material parameters and T denotes the absolute temperature. Troom and Tref are the absolute room temperature and melting temperature of the material, in the case 293 and 1809 K, respectively. A FE analysis has been made under the assumption that the process is adiabatic. Stoﬀel [2004] [2005] has considered an evolution of plastic zones in dynamically loaded plates using diﬀerent elastic-viscoplastic laws. He has used the Chaboche [1989] low developed for non-linear hardening σij − Xij 3 p˙ , − X ) 2 IIσ (σrs rs n IIσ (σij − Xij )−R−k p˙ = , K

ε˙pij =

2 X˙ ij = aε˙pij − sXij p˙ ; 3

R˙ = b1 (b2 − R) p˙

with the abbreviations εpij , p, σij , Xij , R denoting the plastic strain tensor, equivalent plastic strain, second Piola–Kirchhoﬀ stress tensor, backstress tensor and isotropic hardening. The yield limit k and the material parameters a, s, b1 , b2 ,

dynamic

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Rate Inﬂuence

dynamic

203

Fig. 4.5.5 Stress–strain curves of an IF steel at diﬀerent strain rates, including strain rate jump tests: (1) monotonic tensile test at 1000 s−1 ; (2) tensile test at 1000 s−1 after a tensile pre-strain of 8% at 0.001 s−1 ; (3) after a tensile pre-strain of 16% at 0.001 s−1 ; (4) monotonic tensile test at 0.001 s−1 .

n, K must be obtained from tension tests. A separation of isotropic and kinematic hardening was not possible so that in the Chaboche model kinematic hardening is assumed. Another model considered is the Tanimura [1979] one, which can be expressed as σij 3 ε˙pij = rp˙ ) , 2 IIσ (σij p˙ = e (1/

√

−S0 3)II (σ )−τ ∗ σ ij

with the material parameters S0 , r, τ ∗ to be determined from uni-axial tension tests. This is an overstress model without hardening. The third model is the Bodner–Partom [1975] model. This is a model disregarding the yield stress. The model is σij 3 , ε˙pij = p˙ ) 2 IIσ (σrs 2 − 1 ( R+D )2n n+1 n p˙ = √ D0 e 2 IIσ (σrs ) , 3 σij p , R˙ = m1 (R1 − R)σij ε˙ij , D = Xij IIσ (σrs ) σij 3 p D1 − X X˙ ij = m2 ij σkl ε˙kl , ) 2 IIσ (σrs

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

204

Dynamic Plasticity

Fig. 4.5.6

Conical shape of the plate.

where the material parameters n, D0 , D1 , R1 , m1 , and m2 have to be identiﬁed from tension tests. These three models are applied by Stoﬀel for the motion of a thin (thickness 2 mm) circular membrane of 138 mm and 553 mm. The motion of such a plate at various times is shown in Fig. 4.5.6. Trying to describe the motion of such plates the author was obliged to consider the elastic material properties in the simulations. Using the Chaboche model elastic, hardening and viscous material properties can be separated from each other. This allows in the material parameter identiﬁcation procedure a precise adaptation of the viscoplastic law to the uni-axial tension tests. In the Bodner–Partom model elastic properties are not assumed and hardening as well as viscous behaviors are combined with each other. In the Tanimura model the hardening is neglected. With this described advantage in the case of the elasticviscoplastic Chaboche model simulations using this law lead to the most precise results. A novel technique for time-resolved detection and tracking of interfacial and matrix fracture in layered materials is due to Minnaar and Zhou [2004]. The measurements at multiple locations allow the speeds at which interfacial crack front or matrix cracking/delamination front propagates to be determined. The results show that the speed of delamination or the speed of matrix cracking/delamination increases linearly with impact velocity. In another paper Colak [2004] consider small strain, isotropic, viscoplasticity theory based on overstress, modiﬁed to model the complex cyclic hardening behavior under proportional and non-proportional loading. The theory is without yield

dynamic

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

Rate Inﬂuence

dynamic

205

surface and no loading/unloading conditions. The theory consists of two tensors valued state variables, which are in equilibrium stress and the kinematic stress, and a scalar isotropic stress with a ﬂow law. The propagation of stress pulses is studied by Ostoja-Starzewski [1995] in one-dimensional piecewise constant microstructure of grains with power-law elastic response, having randomness present in constitutive moduli and grain lengths. A study is conducted of the sensitivity of loading and unloading shock waves. The ﬂow law is (see Krempl [1998], development of viscoplasticity theory based on overstress Krempl [1988], S¨ ut¸cu ¨ and Krempel [1989]): ε˙ = ε˙ E + ε˙ P =

1 + v 3 σ − g σ˙ + E 2 Ek[Γ]

where g is the deviatoric part of the equilibrium stress G, Γ2 =

3 (σ − g) : (σ − g) 2

and the viscosity function k = k1

Γ 1+ k2

−k3

with k1 , k2 and k3 material constants. The equilibrium stress is introduced to represent the defect structure of the material. The growth law for the equilibrium stress consists of elastic, inelastic, dynamic recovery term and kinematic hardening contributions: Ψ[Γ] ˙ σ − g Γ g − f Ψ[Γ] σ˙ + − + 1− f g˙ = E k k A E where Ψ is the shape function which aﬀects the transition between initial quasi elastic behavior and inelastic ﬂow. It is related as C2 − C1 Ψ[Γ] = C1 + exp[C3 Γ] where C1 , C2 and C3 are material constants. The positive, decreasing shape function Ψ is bounded by 1 > Ψ[Γ]/E > Et /E. The growth laws for the kinematic stress f is given by Et (σ − g) f˙ = E k[Γ] where Et is the tangent modulus at the maximum inelastic strain. The state variable A, with the dimension of stress, grows according to 2 ˙ p˙ A = Ac [Af − A] 3 where Ac and Af are material constants. The equivalent inelastic strain rate p˙ is √ p˙ = ε˙P : ε˙P .

January 12, 2007

206

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Dynamic Plasticity

Fig. 4.5.7 Uniaxial dual-amplitude step-up test using modiﬁed viscoplasticity. Further hardening is observed after the increase in strain amplitude. The strain rate is ε˙ = 1 × 10−5 s−1 .

Since an extra hardening is observed and that is rate independent, one is using the Krempel [1998] constitutive equation. Also to include the strain amplitude eﬀect as well as the loading path eﬀect, the non-proportionality measure deﬁned by Tanaka [1994] is used. The forth order tensor C˙ ijkl = cc (uij ukl − Cijkl ) p˙ ˙ and the non-proportionality with cc a material constant, is introduced. u = ε˙ P /p, measure is Cijkl Cijkl − uij Cklij Cklmn umn . Φ= Cprst Cprst The center of inelastic strain range, Y is modeled by Tanaka [1994], ˙ = ry (εP − Y) p˙ Y where ry is a material constant. The size of the memory surface q is q = |εP − Y| where | | indicates magnitude. The theory was applied to various loadings. For instance, for uniaxial dual amplitude step-up test is shown in Fig. 4.5.7. The mathematical study of the problem of unilateral contact between an elasticviscoplastic body and a rigid frictionless foundation is due to Sofonea [1997]. The constitutive law is σ˙ = E ε˙ + G(σ, ε)

dynamic

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Rate Inﬂuence

where E and G are constitutive functions. For −k1 F1 (σ − f (ε)) G(σ, ε) = 0 k2 F2 (g(ε) − σ)

dynamic

207

G one is using if σ > f (ε) if g(ε) ≤ σ ≤ f (ε) if σ < g(ε)

where k1 , k2 > 0 are viscosity constants and F1 , F2 are increasing functions with F1 (0) = F2 (0) = 0. The variation formulation of the problem is given and the existence and uniqueness result for the displacement and stress ﬁeld is obtained. A ﬁxed point method was used in order to obtain the existence and uniqueness of the solution. The continuous dependence of the solution with respect to the input data as well as the stability result is then analyzed. Matos and Dodds [2002] have considered the initiation of brittle fracture triggered by a transgranular cleavage mechanism typical of that exhibited by ferritic steels operating in the ductile-to-brittle transition region. The plastic strain is of the form γ q q D − 1 >1 σ σ e e vp ε˙ = q 0 ≤1 σe where D and γ denote material parameters, q denotes the rate-dependent uniaxial tensile stress and σe denotes the static uniaxial tensile stress.

Fig. 4.5.8 Stress–strain curves of samples cut from an HSLA-65 plate at indicated directions and locations.

January 12, 2007

208

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Dynamic Plasticity

Fig. 4.5.9 Comparison of PB-model predictions with experimental results at a strain rate of 3000/s and indicated initial temperatures.

A paper in which one is discussing the Hopkinson technique for the dynamic recovery experiments is due to Nemat-Nasser et al. [1991]. In a recent paper NematNaser and Guo [2005] study the thermomechanical response of high-strength lowalloy steel (HSLA-65) in uniaxial compression tests. True strains exceeding 60% are achieved in these tests, over the range of strain rates from 10−3 /s to about 8500/s, and at initial temperatures from 77 to 1000 K. To show the inﬂuence of the strain rate is given the Fig. 4.5.8. Even the elastic parameters seem to be inﬂuenced. They apply the Johnson–Cook model and their own (PB-model). For their own model, it is for T ≤ Tc : 1/2 &3/2 γ ˙ τ = 760γ 0.15 + 1450 1 − −10.6 × 10−5 T ln 4 × 108 !γ where T = T0 + 0.267 0 τ dγ and for T > Tc we have τ = 760γ 0.15 where −1 γ˙ −5 . Tc = −10.16 × 10 ln 4 × 108 Figure 4.5.9 is showing the theory adapted to the experimental data. The compressive stress–strain behavior of a NiTi shape memory alloy has been determinated by Chen et al. [2001], over strain rates of 10−3 –7.5 × 102 s−1 . A split Hopkinson pressure bar with a pulse shaping technique was used to perform valid dynamic tests. Experimental results show that, the plateau stress of the shape memory alloy is strain rate dependent. The material is returning to its original length upon unloading.

dynamic

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Rate Inﬂuence

dynamic

209

Forrestal et al. [2003] present a Hopkinson bar technique to evaluate the performance of accelerometers that measure large amplitude pulses, such as those experienced during projectile penetration tests. An aluminum striker bar impacts a thin Plexiglas or copper disk placed on the impact surface of an aluminum incident bar. The Plexiglas or copper disk pulse shaper produces a nondispersive stress wave that propagates in the aluminum incident bar and eventually interacts with a tungsten disk at the end of the bar. A quartz stress gage is placed between the aluminum bar and tungsten disk, and an accelerometer is mounted to the free end of the tungsten disk. An analytical model shows that the rise time of the incident stress pulse in the aluminum bar is long enough and the tungsten disk length is short enough that the response of the tungsten disk can be accurately approximated as rigid-body motion. They measure stress at the aluminum bar-tungsten disk interface with the quartz gage and they calculate rigid-body acceleration of the tungsten disk from Newtonian’s Second Law and the stress gage data. In addition they measure strain-time at two locations on the aluminum incident bar to show that the incident strain pulse is nondispersive and they calculate rigid-body acceleration of the tungsten disk from a model that uses this strain-time data. Thus, they can compare accelerations measured with the accelerometer and accelerations calculated with models that use stress gage and strain gage measurements. They show that all three acceleration-time pulses are in very close agreement for acceleration amplitudes to about 20,000 G. In a recent paper G´ omez-del R´ıo et al. [2005] have tested dynamic tensile composites at law temperature using split Hopkinson pressure bar. The temperature is 20 and −60◦ C. The results of the dynamic tests showed little inﬂuence of temperature and strain rate on the tensile strength of a unidirectional laminate loaded in the ﬁber direction; in contrast, the strength increases appreciably in the transverse direction at low temperature and high strain rate. Regarding strain rate, a slight increase in tensile strength was observed under dynamic loading. In another paper M¨ uller et al.[2002] have a repetitive thermodynamics on viscoplastic body, since moulding plastic deformation is accompanied by heating. They have three such loadings. They show that the deformation in time, and temperature, is tending towards a single loading. In the paper by Tsai and Prakash [2005] is studied the normal plate impact experiments on 2-D layered material targets to understand the role of material architecture and material inelasticity in governing the elastic precursor decay and late-time wave dispersion. In order to understand the eﬀects of layer thickness and the distance of wave propagation on elastic precursor decay and latetime dispersion several targets with various layer and target thicknesses are employed. Moreover, in order to understand the eﬀects of material inelasticity both elastic-elastic and elastic-viscoelastic bilaminates are utilized. The results of the study indicate that the structure of acceleration waves is strongly inﬂuenced by impedance mismatch of the layers constituting the laminates, density of interfaces,

January 12, 2007

210

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Dynamic Plasticity

distance of wave propagation, and material inelasticity. The speed of elastic precursor is independent of the impedance mismatch of the individual laminae constituting the bilaminates and is equal to the average wave speed within the bilaminates. The speed of the late-time dispersion wave is observed to decrease with an increase in impedance mismatch; however, it is found to be independent of the density of interfaces, i.e., the number of layers in a given thickness laminate. The decay of the elastic precursor is observed to increase with an increase in impedance mismatch, the density of interfaces, and the distance of wave propagation. The rise-time of the late-time dispersion wave increases with an increase in impedance mismatch; however, it is observed to decrease with an increase in the density of interfaces. The frequency of oscillations of the late-time dispersive wave is observed to decrease with an increase in impedance mismatch; however, it is observed to increase with an increase in the density of interfaces. A model is presented by Ubachs et al. [2005] to describe the mechanical behavior of microstructure dependent materials. The model describes the microstructure evolution using a phase ﬁeld approach and employs a constitutive model dependent on the phase ﬁeld to account for the underlying microstructure. It has been demonstrated by applying it to eutectic tin-led solder, a material whose mechanical characteristics are strongly inﬂuenced by its continuously evolving microstructure. For the constitutive behavior the elasto-viscoplastic Perzyna model has been adopted. The Perzyna model allows the use of diﬀerent hardening functions, which makes it suitable for a large variety of materials. It is coupled to the phase ﬁeld model through the model parameters which are taken dependent on the mass fraction ﬁeld resulting from the solution of the phase ﬁeld equations. In this way the microstructure is accounted for using a continuum mechanics approach. Mixed-mode open-notch ﬂexure, anti-symmetric loaded end-notched ﬂexure and center-notched ﬂexure specimens were used to investigate dynamic mixed I/II mode delamination fracture using a fracturing split Hopkinson pressure bar by Wosu et al. [2005]. An expression for dynamic energy release rate is formulated and evaluated. The experimental results show that dynamic delamination increases linearly with mode mixing. In several papers by Krempl and Ho [2001], Ho and Krempl [2001], [2002] is developed a complicated theory based on overstress, to describe the rate sensitivities inside and outside the dynamic strain aging regime. The compressible and incompressible, isotropic, small strain viscoplasticity theory based on overstress is given. An experimental paper by Bourne [2006], is devoted to the plate impact to load in uniaxial strain and to show that a lower threshold exists for the propagation of fracture from the impact face. This is 4GPa in soda-lime glass. The velocity of impact is 1.5–2.5 km/s.

dynamic

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Rate Inﬂuence

dynamic

211

Bibliography Altenhof W. and Ames W., 2002, Strain rate eﬀects for aluminum and magnesium alloys in ﬁnite element simulations of steering wheel armature impact tests, Fatigue Fract. Engng. Mater. Struct. 25, 1149–1156. Alter B. E. K. and Curtis C. W., 1956, Eﬀect of strain rate on the propagation of a plastic strain pulse along a lead bar, J. Appl. Phys. 27, 1079–1085. Auricchio F., 1997, A viscoplastic constitutive equation bounded between two generalized plasticity models, Int. J. Plasticity 13, 8–9, 697–721. Baroncea A., Cristescu and Glodeanu E., 1977, A model for the description of the deformation of rocksalt, St. Cerc. Mec. Appl. 36, 1, 31–40 (in Roumanian). B´eda G., 1962a, Acta. Tech. Acad. Sci. Hung. 38, 161–187. Bell J. F., 1951, Propagation of plastic waves in prestressed bars, U.S. Navy Tech. Rep. No. 5, Baltimore, The Johns Hopkins University. Bell J. F., 1968, The phisics of large deformation of crystalline solids, Springer Tracts in Natural Philosophy, Vol. 14, Springer-Verlag, Berlin. Bell J. F., 1973, The experimental foundations of solid mechanics, in Hadbuch der Physik (ed. S. Flugge), Vol. Via/1, Springer-Verlag, Berlin. Bell J. F. and Stein A., 1962, The incremental loading wave in the pre-stressed plastic ﬁeld, J. M´ecan. 1, 4, 395–412. Bertholf L. D. and Karnes C. H., 1975, Two-dimensional analysis of the split Hopkinson pressure bar system, J. Mech. Phys. Solids 23, 1–19. Bingham E. C., 1922, Fluidity and Plasticity, McGraw-Hill, New York. Bodner S. R. and Partom Y., 1975, Constitutive equations for elasto-viscoplastic strainhardening materials, ASME J. Appl. Mech. 42, 385–389. Bourne N. K., 2006, On the impact and penetration of soda-lime glass, Int. J. Imp. Engineering (in press). Campbell J. D., 1970, Dynamic Plasticity of Metals, Springer Verlag, 92 pp. Campbell J. D., 1973, Dynamic plasticity-macroscopic and microscopic aspects, Materials Science and Engineering 12, 1, 3–21. Cernocky E. P., 1982, An examination of four viscoplastic constitutive theories in uniaxial monotonic loading, Int. J. Solids Structures 18, 11, 989–1005. Chaboche J. L., 1989, Constitutive equations for cyclic plasticity and cyclic viscoplasticity, Int. J. Plasticity 5, 247–302. Chang K. C., Sugiura K. and Lee G. C., 1989, Rate-dependent material model for structural steel, J. of Engeenering Mach. 115, 3, 465–474. Chau O., Fern´ andez-Garc´ıa J. R., Han W. and Sofonea M., 2002, A frictionless contact problem for elastic-viscoplastic materials with normal compliance and damage, Com. Met. Appl. Mech. Engi. 191, 44, 5007–5026. Chen W. W., Wu Q. P., Kang J. H. and Winfree N. A., 2001, Compressive superelastic behaviour of a NiTi shape memory alloy at strain rates of 0.001–750 s−1 , Int. J. Solids Struct. 38, 8989–8998. Chhabildas L. C. and Swegle J. W., 1989, Dynamic pressure-shear loading of using anisotropic crystals, J. Appl. Phys. 51, 9, 4799–4807. Colak O. U., 2004, A viscoplasticity theory appied to proportional and non proportional cyclic loading at small strains, Int. J. Plasticity 20, 1387–1401. Cristescu C. and Cristescu N. D., 1973, A numerical method to describe unloading in dynamic plasticity, 2nd Int. Conf. on “Structural Mechanics in Reactor Technology”, Berlin. L 4/8, 1–14.

January 12, 2007

212

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Dynamic Plasticity

Cristescu N. D., 1963, On the propagation of elastic-plastic waves in metallic rods, Bull. Acad. Polon. Sci. 11, 129–133. Cristescu N. D., 1964, Some problems in the mechanics of extensible strings, in: Kolsky H. and Prager W. (eds.), Symp. IUTAM Stress Waves in Anelastic Solids, Providence, 1963 (Springer Verlag, Berlin–G¨ ottingen–Heidelberg) 118–132. Cristescu N. D., 1966, About the propagation of elastic/plastic waves in thin rods, in: Dynamics of Mashines, Proc. Conf. Liblice-Praga, 1963, 87–96. Cristescu N. D., 1967, Dynamic Plasticity, North Holland Pub., Amsterdam. Cristescu N. D., 1972a, Rate-Type Constitutive Equations in Dynamic Plasticity, Noordhof International Publishing, Leyden, 287–310. Cristescu N. D., 1972b, A procedure for determining the constitutive equations for materials exhibiting both time-dependent and time-independent plasticity, Int. J. Solids Structures 8, 511–531. Cristescu N. D., 1977, Speed inﬂuence in wire drawing, Rev. Roumaine de M´ ecanique Appliqu´ee 22, 3, 391–399. Cristescu N. D. and Bell J. F., 1970, On unloading in the symmetrical impact of two aluminum bars, in: In Elastic Behaviour of Solids, Kannienen M. F., Adler W. F., Rosenﬁeld A. R. and Jaﬀee R. I. (eds.), McGraw Hill, New York, 397–421. Cristescu N. D. and Suliciu I., 1982, Viscoplasticity, Martinus Nijhoﬀ Pub.,307 pp. Curr` o C. and Valenti G., 1996, A linearization procedure for quasi-linear non homogeneous and non-autonomous ﬁrst-order systems, Int. J. Non-Linear Mechanics 31, 3, 377–386. Daimaruya M. and Naitoh M., 1983, On the existence of a strain plateau in the strain-rate dependent theory of Malvern for plastic wave propagation, J. Appl. Mech., Trans. ASME 50, 3, 678–679. Dally J. W. and Riley W. F., 1965, Experimental Stress Analysis, McGraw Hill, New York. Dawson T. H., 1972, On the applicability of one-dimensional non-viscous dynamic plasticity theory, Int. J. Mech. Sci. 14, 43–48. Dioh N. N., Leevers P. S. and Williams J. G., 1993, Thickness eﬀects in split Hopkinson pressure bar tests, Polymer 34, 20, 4230–4234. Dioh N. N., Ivankovic A., Leevers P. S. and Williams J. G., 1995, Stress wave propagation eﬀects in split Hopkinson pressure bar tests, Proc. Roy. Soc. London 449, 187–204. Drˇ agˇ anescu Gh. E. and Cˇ apˇ alnˇ aa¸san V., 2003, Nonlinear relaxation phenomena in polycristalline solids, Int. J. Nonlinear Sci. Num. Sci. 4, 219–225. Fˇ aciu C. and Mihailescu-Suliciu M., 1987, The energy in one-dimensional rate-type semilinear viscoelastcity, Int. J. Solids Sructures 23, 11, 1505–1520. Faciu C. and Simion N., 2000, Energy estimates and uniqueness of the weak solutions of initial-boundary value problems for semilinear hyperbolic systems, Z. Angev. Math. Phys. 51, 792–805. Fern´ andez J. R., Hild P. and Via˜ no J. M., 2003, Numerical approximation of the elasticviscoplastic contact problem with non-matching meshes, Numer. Math. 94, 501–522. Fern´ andez L. R., 2004, Numerical analysis of a contact problem between two elastic viscoplastic bodies with hardening and nonmatching meshes, Finite Elements in Analysis and Design 40, 771–791. Filbey G. L., 1961, Intensive Plastic Waves Ph.D. dissertation, The Johns Hopkins University, Baltimore. Forrestal M. J., Togami T. C., Baker W. E. and Frew D. J., 2003, Performance evaluation of accelerometers used for penetration experiments, Experimental Mechanics 43, 1, 90–96. Francis P. H. and Lindholm U. S., 1968, Eﬀect of temperature gradients on the propagation of elastoplastic waves, J. Appl. Mech. Trans. ASME 35, 3, 441–448.

dynamic

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Rate Inﬂuence

dynamic

213

Fusco D. and Manganaro N., 1994a, Riemann invariants-like solutions for a class of rate-type materials, Acta Mechanica 105, 23–32. Fusco D. and Manganaro N., 1994b, A method for determining exact solutions to a class of nonlinear models based on introduction of diﬀerential constrains, J. Math. Phys. 35, 7, 3659–3669. Fusco D. and Manganaro N., 1996, A method for ﬁnding exact solutions to hyperbolic systems of ﬁrst-order PDEs, IMA J. Appl. Math. 57, 3, 223–242. Gilman J. J., 1960, Physical nature of plastic ﬂow and fracture, in: Lee E. H. and Symonds P. S. (eds.), Plasticity, Proc. Second. Symp. on Naval Structural Mechanics, Providence, 1960 (Pergamon Press, New York–Oxford–London–Paris) 44–99. Goldsmith W., 2001, Impact, the Theory and Physical Behavior of Colliding Solids, Dover, N.Y. G´ omez-del R´ıo T., Barbero E., Zaera R. and Navarro C., 2005, Dynamic tensile behaviour at low temperature of CFRP using a split Hopkinson pressure bar, Composites Science and Technology 65, 61–71. Gupta Y. M., 1976, Shear measurements in shock-loaded solids, Appl. Phys. Lett. 29, 11, 694–697. Hauser F. E., Simmons J. A. and Dorn J. E., 1961, Strain rate eﬀects in plastic wave propagation, in: Shewmon P. G. and Zackay V. F. (eds.), Response of Metals to High Velocity Deformation, Proc. Conf. Colorado (Interscience Publ., New York, London) 93–110. Ho K. and Krempl E., 2001, The modeling of unusual rate sensitivities inside and outside the dynamic strain aging regime, Trans. ASME, J. Engng. Mat. Tech. 123, 28–35. Ho K. and Krempl E., 2002, Extension of the viscoplasticity theory based on overstress (VBO) to capture non-standard rate dependence in soils, Int. J. Plasticity 18, 851–872. Hu Y. and Feng R., 2004, On the use of a Kolsky torsion bar to study the transient largestrain response of polymer melts at high shear rates J. Appl. Mech. 71, 441–449. Ilyushin A. A. and Lenskii V. S., 1959, Strength of Materials, Fizmatghiz, Moscow (in Russian). Ionescu I. and Sofonea M., 1993, Functional and Numerical Methods in Viscoplasticity, Oxford University Press, Oxford, 265 pp. Khaleel M. A., Zbib H. M. and Nyberg E. A., 2001, Constitutive modeling of deformation and damage in superplastic materials, Int. J. Impact Engn. 17, 277–296. Klepaczko J. R., 1998, Remarks on impact shearing, J. Mech. Phis. Solids 46, 10, 2139–2153. Kojic M., 1996, The Governing Parameter Method for implicit integration of viscoplastic constitutive relations for isotropic and orthotropic metals, Computational Mechanics 19, 49–57. Kolsky H., 1949, An investigation of the mechanical properties of materials at very high rates of loading, Proc. Phys. Soc. B 62, 676–700. Krempl E., 1988, Phenomenological modeling of viscoplasticity, Revue Phys. Appl. Phisics Abstracts 23, 331–338. Krempl E., 1998, Creep-Plasticity Interaction. Lecture Notes. CISM No. 187, Udine, Italy, p. 74. Krempl E. and Ho K., 2001, Inelastic Compressible and Incompressible, Isotropic, Small Strain Viscoplasticity Theory Based on Overstress (VBO), Lemaitre Handbook of Materials Behaviour Models, Sec. 5.6, 336–348. Kuriyama S. and Kawata K., 1973, Propagation of stress wave with plastic deformation in metal obeying the constitutive equation of the Johnston–Gilman type, J. Appl. Phys. 44, 8, 3445–3454.

January 12, 2007

214

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Dynamic Plasticity

Lawson J. E. and Nicholas T., 1972, The dynamic mechanical behavior of titanium in shear, J. Mech. Phys. Solids 20, 65–76. Li C. H. and Clifton R. J., 1982, Dynamic stress–strain curves at plastic shear strain rate, in Shock Waves in Condensed Matter — 1981, Nellis W. J., Seaman L. and Graham R. A. (eds.), American Institute of Physics, New York, 360–366. Lodygowski T. and Perzyna P., 1997, Numerical modeling of localized fracture of inelastic solids in dynamic loading processes, Int. J. Numer. Meth. Engng. 40, 4137–4158. Lubarda V. A., Benson D. J. and Meyers M. A., 2003, Strain-rate eﬀects in rheological models of inelastic response, Int. J. Plasticity 19, 8, 1097–1118. ¨ Ludwik P., 1909, Uber den Einﬂuss der Deformationsgeschwindigkeit bei bleibenden Deformationen mit besonderer Ber¨ ucksichtigung der Nachwirkungserscheinungen, Physik. Zeitschrift 10, 411–417. Luo Y., Mori T., Li S. and Luo S., 2003, Isothermal rheological forming of high strength alloying part with complicated curved surface, Materials Sci. Forum 437 438, 337–340. Malvern L. E., 1951a, Plastic wave propagation in a bar of metal exhibiting a strain rate eﬀect, Quart. Appl. Math. 8, 4, 405–411. Malvern L. E., 1951b, The propagation of longitudinal waves of plastic deformation in a bar of material exhibiting a strain rate eﬀect, J. Appl. Mech. 18, 2, 203–208. Manganaro N. and Valenti G., 1993, Group analysis and linearization procedure for a nonautonomous model describing rate-type materials, J. Math. Phys. 34, 4, 1360–1369. Manganaro N. and Meleshko S., 2002, Reduction procedure and generalized simple waves for systhems written in Riemann variables, Nonlinear Dynamics, 30, 87–102. Maranini E. and Yamaguchi T., 2001, A non-associated viscoplastic model for the behavior of granite in triaxial compression, Mech. of Mater. 33, 5, 283–293. Matos C. G. and Dodds R. H. Jr., 2002, Probabilistic modeling of weld fracture in steel frame connections Part II: seismic loading, Engineering Structures 24, 687–705. Mihailescu-Suliciu M. and Suliciu I., 1987, On tensile shock waves in rubber-like materials, J. Appl. Mech. 54, 498–502. Minnaar K. and Zhou M., 2004, A novel technique for time-resolved detection and tracking of interfacial and matrix fracture in layered materials, J. Mech. Phys. Solids 52, 2771–2799. Mortell M. and Seymour B. R., 1973, Pulse propagation in nonlinear viscoelastic rod of ﬁnite length, SIAM J. Appl. Math. 22, 2, 209–224. M¨ uller I., Sahota H.-S. and Villaggio P., 2002, On the thermodynamics of repetitive visco-plastic moulding, Z. Angew. Math. Phys. 53, 1139–1149. Nemat-Nasser S., Isaacs J. B. and Starrett J. E., 1991, Hopkinson techniques for dynamic recovery experiments, Proc. R. Soc. Lond. A 435, 371–391. Nemat-Nasser S., Choi J. Y., Guo W. G. and Isaacs J. B., 2005, Very high strain-rate response of a NiTi shape-memory alloy, Mechanics of Materials 37, 287–289. Nemat-Nasser S. and Guo W. G., 2005, Thermomechanical response of HSLA-65 steel plates: experiments and modeling, Mechanics of Materials 37, 379–405. Nicholas T., 1981, Tensile testing of materials at high rates of strain, Experimental Mechanics 21, 5, 177–185. Nicholas T., Rajendran A. M. and Grove D. J., 1987a, Analytical modeling of precursor decay in strain-rate dependent materials, Int. J. Solids Struct. 12, 1601–1614. Nicholas T., Rajendran A. M. and Grove D. J., 1987b, An oﬀset yield criterion from precursor decay analysis, Acta Mechanica 69, 1–4, 205–218.

dynamic

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Rate Inﬂuence

dynamic

215

Nicholson D. W. and Phillips A., 1978, On the impact end in logitudinal dynamic plastic wave propagation, Acta Mechanica 29, 75–92. Ostoja-Starzewski M., 1995, Wavefront propagation in a class of random microstructuresII, Non-linear elastic grains, Int. J. Non-Linear Mechanics 30, 6, 771–781. Pao Y. H. and Gilat A., 1989, Modeling 1100-0 aluminum over a wide range of temperatures and strain rates, Int. J. Plasticity 5, 183–196. Perzina P., 1963, The study of the dynamical behaviour of rate sensitive plastic materials, Arch. Mech. Stos. 15, 113–130. Ponomarev S. D., Biderman V. L., Likharev K. K., Makushin V. M., Malinin N. N. and Feodos’ev V. I., 1956, Resistance calculus in construction of machines, Mashigiz Moscow, Tom III, 553–580 (in Russian). Prandtl L., 1928, Ein Gedankenmodell zur kinematischen Theorie der festen K¨orper, Z. Angew. Math. Mech. 8, 85–106. Schmidt M. L. and Ross C. A., 1999, Shear strength of concrete under dynamic loads, ASME Pressure Vessel and Piping Conf. Boston, MS, August 1999. Shaw R. P. and Cozzarelli F. A., 1971, Wave-front stress relaxation in a one dimensional nonlinear inelastic material with temperature and position dependent properties, J. Appl. Mech. 38, 1, 47–50. Sofonea M., 1997, On a contact problem for elastic-viscoplastic bodies, Nonlinear Analysis, Theory, Methods & Applications 29, 9, 1037–1050. Sokolovskii V. V., 1948a, Propagation of elastic-visco-plastic waves in bars, Docl. Akad. Nauk SSSR 60, 5, 775–778 (in Russian). Sokolovskii V. V., 1948b, Propagation of elastic-visco-plastic waves in bars, Pricl. Mat. Meh. 12, 3, 261–280 (in Russian). Stoﬀel M., 2004, Evolution of plastic zones in dynamically loaded plates using diﬀerent elastic-viscoplastic laws, Int. J. Solids and Structures 41, 6813–6830. Stoﬀel M., 2005, Sensitivity of simultaneous depending on material parameter variations, Mech. Res. Com. 32, 332–336. Suliciu I., 1966, private comunication. Suliciu I., 1972, Additional coments on Suliciu, Malvern and Cristescu’s paper. “Remarks concerning the “plateau” in dynamic plasticity”, Archives of Mechanics 27, 4, 665–667. Suliciu I., 1974, Classes of discontinuous motions in elastic and rate-type materials, Arch. Mech. Stos. 26, 4, 675–699. Suliciu I., 1981, On the Savart–Masson eﬀect, J. Appl. Mech. Trans. ASME 48, 426–428. Suliciu I., Lee S. Y. and Ames W. F., 1973, Nonlinear traveling waves for a class of rate-type materials, J. Math. Anal. Appl. 42, 2, 313–322. Sundaram S. and Clifton R. J., 1998, The inﬂuence of a glassy phase on the high strain rate response of a ceramic, Mechanics of Materials 29, 233–251. S¨ ut¸cu ¨ M. and Krempel E., 1989, A stability analysis of the uniaxial viscoplasticity theory based on overstress, Computational Mechanics 4, 401–408. Tabov I., 1996, Riemann invariants for a class of partial diﬀerential systems, Diﬀerential Equations 32, 11, 1550–1553. Tanaka E., 1994, A nonproportionality parameter and a cyclic viscoplastic constitutive model taking into account amplitude dependencies and memory eﬀects of isotropic harden, European J. of Mechanics 13, 2, 155–173. Tanimoto N., 1994, One-dimensional propagation speed of an elastic-plastic viscoplastic stress wave, Nuclear Eng. and Design 150, 2–3, 275–280. Tanimoto N., Fukuoka H. and Fujita K., 1993, One-dimensional numerical analysis of a bar subjected to longitudinal impulsive loading, ISME International Journal, Series A, 36, 2, 137–145.

January 12, 2007

216

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Dynamic Plasticity

Tanimura S., 1979, A practical constitutive equation covering a wide range of strain rates, Int. J. Eng. Sci. 17, 997–1004. Thomsen E. G., Yang C. T. and Kobayashi S., 1968, Mechanics of Plastic Deformation in Metal Processing, Macmillan Co., London. Ting T. C. T. and Symonds P. S., 1964, Longitudinal impact on visco-plastic rods linear stress–strain rate law, J. Appl. Mech. 31, Ser. E, 199–207. Tsai L. and Prakash V., 2005, Structure of weak shock waves in 2-D layered material systems, Int. J. Solids Struct. 42, 724–750. Ubachs R. L. J. M., Schreurs P. J. G. and Geers M. G. D., 2005, Phase ﬁeld dependent viscoplastic behaviour of solder alloys, Int. J. Solids Sructures 42, 2533–2558. Uenishi A. and Teodosiu C., 2004, Constitutive modeling of the high strain rate behaviour of interstitial-free steel, Int. J. Plasticity 20, 915–936. Valanis K. C., 1972, Irreversible thermodinamics of continuous media, Internal Variable Theory, CISM Courses and Lectures No. 77, International Centre for Mechanical Sciences, Springer, Wien. Vyalov S. S., 1978, Rheological foundations for soil mechanics, Vysh. Shkola, Moscow (in Russian). Wosu S. N., Hui D. and Dutta P. K., 2005, Dynamic mixed-mode I/II delamination fracture and energy release rate of unidirectional graphite/epoxy composites, Eng. Fracture Mech. 72, 1531–1558. Yokoyama T., 2001, Finite element computation of torsional plastic waves in a thin walled tube, Archive of Applied Mechanics 71, 6–7, 359–370. Zhao H., 1997, A study of specimen thickness eﬀects in the impact tests on polymers by numeric simulations, Polymer 39, 5, 1103–1106. Zhao H., 2003, Material behaviour characterization using SHPB techniques, tests and simulations, Computers & Structures 81, 12, 1301–1310. Zhao H. and Gary G., 1996, On the use of SHPB techniques to determine the dynamic behavior of materials in the range of small strains, Int. J. Solids Structures 33, 23, 3363–3375. Ziegler F., 1992, Developments in structural dynamic viscoplasticity including ductile damage, ZAMM 72, 4, T5–T15.

dynamic

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

Chapter 5

Mechanics of Extensible Strings

5.1

Introduction

The problem was considered for a long time. But generally only static problems or problems involving nearly quasi static conditions were studied (various cables existing in applications). Rubber cables or synthetic strings are elongating very much when impacted, even with quite small forces. But in some modern textile machines the speed of operation is quite high (knitting, weaving, sewing, carding machines). Also in elastic cables used to break airplanes on ships, the speed is quite high. In dynamic problems the cables are inﬂuenced what concerns the yield limit, the work-hardening modulus, the breaking stress and the elastic modulus. Impact velocities of the order of some hundred meters per second or even a few kilometers per second, when the component of the impact velocity ranges between the velocities of propagation of transverse and longitudinal waves, occur less often in practice and lead to diﬃcult mathematical problems, as will be pointed out below. One must also take into account that textile materials cannot resist transverse impacts if the latter exceed a certain limit; for each textile yarn there is a certain limiting transverse impact velocity which at once breaks the string at the point of impact. These limiting velocities, generally, of the order of many hundred meters per second. From the mechanical point of view, that is the simplest problem in which two kind of waves propagate and reﬂect together, inﬂuencing one another at every moment. This motion can be studied both experimentally and theoretically, because both kinds of wave can be observed experimentally during their propagation. The problem can be studied experimentally very well, for the two waves propagating and inﬂuencing each other. On the other hand, the mechanics of strings closely resembles many other problems of dynamic plasticity from the mechanical and mathematical points of view. We are not giving here a complete literature. The beginning of the literature is given in Cristescu [1967]. Some other papers are mentioned in the exposure. The equations of motion of a string in plane motion are written by Rakhmatulin 217

dynamic

January 12, 2007

10:41

218

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Dynamic Plasticity

Fig. 5.1.1

Typical conﬁguration of a yarn specimen after transverse impact.

and Shapiro [1955] in order to determine the dynamic relation between stress and strain for strings. The impact of strings by punctual bodies of ﬁnite mass, when the velocity of impact is variable, was studied by Rakhmatulin [1951] and Riabova [1953], and by some other authors. In the paper by Smith et al. [1956] a textile yarn segment about half a meter long is clamped at each end and impacted transversely at midpoint with a velocity of about 70 m/sec. The stress–strain curve for this yarn is obtained by measuring a high speed photographic record of the motion of the yarn. A typical conﬁguration of the yarn specimen after transverse impact is indicated in Fig. 5.1.1. It is assumed that the transverse waves always propagate more slowly and in fact are reduced to a single shock wave which modiﬁes the shape of the yarn. By measuring the lengths deﬁned in Fig. 5.1.1 on the frames of the photograph record, the average strain as deﬁned by L1 + L2 − L ε¯ = L is used. This manner of deﬁning strain as an average strain, in the presence of wave propagation, is certainly a restrictive one. By measuring also the velocity of propagation of the transverse wave, dynamic stress–strain curves are obtained for high-tenacity nylon, fortisan, and ﬁberglass. The stress–strain curves for nylon obtained by Smith et al. [1956] are reproduced in Fig. 5.1.2 for various strain rate. The important conclusion is that for such materials the increasing rate of strain tends to steepen the slope of the stress–strain curve at the origin. A theory of these phenomena, assuming the yarn to be inﬁnitely long, has been developed by Smith et al. [1958], and Smith et al. [1960]. The velocities of impact range between 1400 m/sec for undrawn nylon to 5000 m/sec for high tenacity rayon and glass-ﬁber. In Fig. 5.1.3 is given the stress–strain curves for acetate yarns as obtained by Smith et al. [1961]. All these yarns show an appreciable rate inﬂuence. The most strongly

dynamic

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Mechanics of Extensible Strings

Fig. 5.1.2

Fig. 5.1.3

Stress–strain curves for Nylon.

Stress–strain curves for braided silk.

dynamic

219

January 12, 2007

220

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Dynamic Plasticity

Fig. 5.1.4 Stress–strain curves for kapron for the following strain rates: (1) 1.2 × 10−3 sec−1 , (2) 1.2 × (10−2 sec−1 , 3) 1.2 × 10−1 sec−1 , (4) (280 sec−1 .

inﬂuenced factor is the yield stress, but generally the whole stress–strain curve is rate dependent. Another experimental technique that of impacting yarns with riﬂe bullets, was developed by Smith et al. [1963]. The transverse velocity of impact is now bigger: up to 700 m/sec. The eﬀect of air drag on the motion of yarn is also analyzed by Smith et al. [1964]. In another paper Fenstermaker and Smith [1965] have described experiments in which transversely impacted ﬁlaments are observed by ﬂash photography. Polyester yarns are used. The strain distribution is obtained at various times after impact and at various impact velocities. These experiments revealed important time eﬀects (creep and relaxation eﬀects) within 50 sec after impact. See also the papers of Smith and Fenstermaker [1967], Smith et al. [1965]. Longitudinal impact with a bullet were performed by Lewis [1957]; the velocity of the bullet is 170 m/sec. Similar experiments are reported by Victorov et al. [1966] for kapron and other yarns, tested at room temperature for rate of strain ranging between 10−3 and 102 sec−1 . An increase of the rate of strain raises the stress–strain curve appreciably.

dynamic

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Mechanics of Extensible Strings

dynamic

221

Some other authors have also reported results on transverse impact of yarns by bullets. But impact grater than 460 m/sec produce a sudden rupture of the yarn and generally all yarns are strongly rate dependent.

5.2

Equations of Motion

In order to obtain the equations of motion (Cristescu [1967]) of an extensible string moving in three-dimensional space, we use a curvilinear coordinate s taken along the string and starting from an arbitrary coordinate origin. This Eulerian coordinate is sometimes called the “laboratory” coordinate or the “actual” coordinate, corresponding to the deformed string at the actual moment t. The tension or total force in the string is denoted by T. It is a variable factor, both along the string and in time. In extensible, perfectly ﬂexible strings, the tension in every point is always directed along the tangent to the string, which will be represented below as a line. Consider a portion of the string comprised between the curvilinear coordinates s1 and s2 (Fig. 5.2.1). This portion of the string will be subjected now only to the tension, but possibly also, to various external forces (X, Y, Z), which are proportional to the length of the portion of the string considered. For this portion we can write " " s2 s2 ∂x "" ∂2x ∂x "" − T + Xds = ρ ds T ∂s "s2 ∂s "s1 ∂t2 s1 s1 and two similar equations for y and z. Here ρ is the density of the string, which is function of the two variables s and t. The projection of T on the three considered axes are T (∂x/∂s), T (∂y/∂s) and T (∂z/∂s), T being the modulus of T. The previous equation can be written in the form

Fig. 5.2.1

Element of a string.

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

222

dynamic

Dynamic Plasticity

s2

s1

∂ ∂s

∂x ∂2x T + X − ρ 2 ds = 0 ∂s ∂t

or taking into account that s1 and s2 are arbitrary ∂x ∂2x ∂ T +X =ρ 2 , ∂s ∂s ∂t

(5.2.1)

and two similar equations for y and z. It is easy to replace the curvilinear coordinate s by a Lagrangean coordinate s0 . The unknown function x, y, z will depend on the variable s0 through the intermediary of s, and also on the time t: x(s(s0 ), t) etc. Thus for a ﬁxed value of t, the formulae ∂x ∂x ds = , etc. ∂s0 ∂s ds0 will apply. The strain of the string is deﬁned by 2 2 2 ∂x ∂y ∂z ds − ds0 = + + −1. ε= ds0 ∂s0 ∂s0 ∂s0

(5.2.2)

(5.2.3)

The last expression is obtained using the formulae (5.2.2). Thus these formulae can be written ∂x ∂x , = (1 + ε) ∂s0 ∂s

∂y ∂y , = (1 + ε) ∂s0 ∂s

∂z ∂z . = (1 + ε) ∂s0 ∂s

(5.2.4)

From the law of conservation of mass, it follows that ρ ds = ρ0 ds0 where ρ0 is the density of the string in the initial non-deformed state. Thus, the relation between the actual density ρ and the initial one ρ0 is ρ0 = ρ(1 + ε) .

(5.2.5)

Taking into account the relation ds = (1 + ε) ds0

(5.2.6)

as well as (5.2.4) and (5.2.5), the equations of motion (5.2.1) can be written as ∂2x T ∂x ∂ − ρ0 2 + (1 + ε)X = 0 (5.2.7) ∂s0 1 + ε ∂s0 ∂t with two similar equations for y and z. To these equations must be added the constitutive equation.

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

Mechanics of Extensible Strings

5.3

dynamic

223

The Finite Constitutive Equation: Basic Formulae

The constitutive equation used most in dynamic problems is the ﬁnite constitutive equation, of the form T = T (ε) .

(5.3.1)

This function is generally a monotonic (sometimes strictly monotonic) increasing function. Taking into account (5.3.1) together with the system (5.2.7) and the relation obtained from (5.2.3) by diﬀerentiating with respect to s0 , we obtain xs0

∂xs0 ∂ys0 ∂zs0 ∂ε + ys0 + zs0 − (1 + ε) = 0, ∂s0 ∂s0 ∂s0 ∂s0

T ∂xs0 ∂xt (1 + ε)dT /dε − T ∂ε + xs0 − ρ0 + (1 + ε)X = 0 , 1 + ε ∂s0 ∂t (1 + ε)2 ∂s0

(5.3.2)

with two similar relations for y and z. For the sake of simplicity the notations xs0 = ∂x/∂s0 , xt = ∂x/∂t, etc. has been used. In order to ﬁnd the type of the system, let us ﬁnd the type of the characteristic lines. For this purpose, the relations dxs0 =

∂xs0 ∂xs0 dt , ds0 + ∂s0 ∂t

dxt =

∂xt ∂xt dt , ds0 + ∂s0 ∂t

(5.3.3)

and similar ones for y and z, will be combined with (5.3.2). The system (5.3.2) contains four equations with four unknown functions x, y, z, and ε, and two independent variables s0 and t. It is clear that the strain ε can be eliminated using (5.2.3). However, to facilitate subsequent mechanical interpretation it is more advantageous to retain ε as an unknown function. The ten relations (5.3.2), (5.3.3) contain ten derivatives of the form ∂xs0 /∂s, ∂xs0 /∂t, etc. By solving with respect to these derivatives we obtain ∂ε ξxs0 + ηys0 + ζzs0 , = ∂s0 (1 + ε)[ρ0 (ds0 /dt)2 − dT /dε] ∂xs0 (1 + ε)3 [dT /dε − ρ0 (ds0 /dt)2 ]ξ =− ∂s0 (1 + ε)3 [ρ0 (ds0 /dt)2 − T /(1 + ε)][ρ0 (ds0 /dt)2 − dT /dε] +

(5.3.4)

xs0 [(1 + ε)dT /dε − T ](ξxs0 + ηys0 + ζzs0 ) , (1 + ε)3 [ρ0 (ds/dt)2 − T /(1 + ε)][ρ0 (ds0 /dt)2 − dT /dε]

and similar expressions for the other second order derivatives which occur in (5.3.2). In (5.3.4) the notations

January 12, 2007

224

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

dynamic

Dynamic Plasticity

ds0 1 − dxt + (1 + ε)X , ξ = ρ0 dxs0 dt dt ds0 1 η = ρ0 dys0 − dyt + (1 + ε)Y , dt dt ds0 1 ζ = ρ0 dzs0 − dzt + (1 + ε)Z dt dt

(5.3.5)

have been used. From (5.3.4) it follows (Cristescu [1954]) that the system (5.3.2) is totally hyperbolic since it has four distinct families of characteristic curves. Two of them are deﬁned by the diﬀerential relations 1/2 ds0 T =± , (5.3.6) dt ρ0 (1 + ε) while the other two by the relations 1/2 ds0 1 dT =± . (5.3.7) dt ρ0 dε Thus all the characteristic lines are generally curved lines whose slope depends on T and ε. From the mechanical point of view, the characteristics lines represent wave fronts. There will be two kinds of waves: the characteristic lines (5.3.6) represent wave fronts which propagate with the velocity 1/2 T , (5.3.8) cI (ε) = ρ0 (1 + ε) while the characteristic lines (5.3.7) represent wave fronts which propagate with a velocity 1/2 1 dT . (5.3.9) cII (ε) = ρ0 dε If (5.3.6) is taken into account, it follows from (5.3.4) (Cristescu [1960, 1961]) that the following diﬀerential relations 1 xs0 (±cI (ε) dε − dv) , dxt = ±cI (ε) dxs0 + [(1 + ε)X − xs0 F ] dt − ρ0 1+ε (5.3.10) and four similar relations for y and z, are satisﬁed on these lines. Along the characteristics (5.3.7) are satisﬁed the diﬀerential relations 1+ε F dt = 0 . (5.3.11) ±cII (ε) dε − dv + ρ0 Here the notations 1 (xs dxt + ys0 dyt + zs0 dzt ) , dv = 1+ε 0 (5.3.12) 1 (Xxs0 + Y ys0 + Zzs0 ) F = 1+ε

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Mechanics of Extensible Strings

dynamic

225

have been used, where v is the projection on the tangent to the string of the velocity of the corresponding particle of the string. The diﬀerential dv is computed along a non-speciﬁed characteristic line. F is the projection on the tangent to the string of the external forces which act on the portion of the string considered, of unit length. The upper and lower signs in (5.3.6) and (5.3.10) and in (5.3.7) and (5.3.11) correspond to each other. Let us write the “jump conditions”, by denoting by [A] the jump of the function A across a characteristic line. Writing the relations (5.3.3) for either side of a characteristic line, and taking into account that the diﬀerentials dxs0 , dxt , etc. are computed along a characteristic line and are in fact “interior derivatives” which are continuous across such a line, we obtain for the kinematics compatibility conditions: ∂xs0 ds0 ∂xs ∂xt ds0 ∂xt + = 0, + =0 (5.3.13) ∂s0 dt ∂t ∂s0 dt ∂t with four similar relations for y and z. In (5.3.13) the rate ds0 /dt must be replaced by one of the two expressions given by (5.3.6) or (5.3.7), depending of the characteristic line considered. If the equations of motion (5.3.2) are written for either side of a characteristic line and the diﬀerence is taken, and if (5.3.13) is also taken into account, we obtain ∂xs0 ∂ys0 ∂zs0 ∂ε + ys0 + zs0 − (1 + ε) = 0, xs0 ∂s0 ∂s0 ∂s0 ∂s0 (5.3.14) 2 & T ∂xs0 ds0 (1 + ε)dT /dε − T ∂ε − ρ0 + = 0, xs0 1+ε dt ∂s0 (1 + ε)2 ∂s0 with two other relations for y and z. These are the dynamic compatibility equations (Cristescu [1954]). In order to see what happens on each characteristic line, we combine (5.3.6) and (5.3.14), to get ∂xs0 ∂ys0 ∂zs0 ∂ε + ys0 + zs0 = 0 and = 0. (5.3.15) xs0 ∂s0 ∂s0 ∂s0 ∂s0 Similarly, from (5.3.7) and (5.3.14) [taking into account also (5.2.2) and (5.2.3)] we obtain: ∂xs0 /∂s0 ∂ys0 /∂s0 ∂zs0 /∂s0 ∂ε . (5.3.16) = = = xs ys zs ∂s0 From (5.3.15) follows that the waves which propagate with the velocity (5.3.8) are transverse waves which aﬀect only the shape of the string but do not aﬀect the longitudinal strain (because [∂ε/∂s0 ] = 0). The waves which propagate with the velocity (5.3.9) are longitudinal waves which produce only propagable elongations of the string, but do not change its shape. The jumps [∂xs0 /∂s0 ], etc. of the second derivatives of the coordinates are simply the projections on the coordinate axes of the discontinuity of ∂ε/∂s0; the relation

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

226

dynamic

Dynamic Plasticity

∂xs0 ∂s0

2

+

∂ys0 ∂s0

2

+

∂zs0 ∂s0

2

=

∂ε ∂s0

2

is also satisﬁed. Thus the projection of the discontinuity on the tangent to the string will propagate through longitudinal waves while the orthogonal component of this discontinuity will propagate through transverse waves. Both types of waves inﬂuence one another. The equation of motion of strings considered to be made of a phase-transforming material like a shape-memory alloy, was done by Purohit and Bhattacharya [2003]. They study the phase boundaries, the driving force acting on them and the kinetic relation governing their propagation. The paper presents also a numerical method for studying general initial and boundary value problems in strings. 5.4

The Order of Propagation of Waves

The order of propagation depends on the initial and boundary conditions, as well on the constitutive equation. Suppose that, at the end of the string, the strain increases monotonically and that at each moment of time both types of waves are generated. The order of propagation of waves in the string will be examined for a material whose constitutive equation is represented in Fig. 5.4.1 (Cristescu [1954, 1958]). Such constitutive equation does not correspond to any speciﬁc material and has been selected only by way of example. From (5.3.8) and (5.3.9) it follows that cI < cII for those tension and strain states which are represented by points on the segments OA or BC. In this case the transverse waves propagate more slowly than the longitudinal ones. On the segments AB and CD the inequality cI > cII holds and in this case the transverse waves propagate faster than the longitudinal waves. Finally there are certain points A, B, C on the diagram, and sometimes even certain segments on this diagram, where the diﬀerential relation (1 + ε)

dT =T dε

(5.4.1)

is satisﬁed. In these points, or portions of the diagram, cI = cII and hence both waves generated at the end of the string propagate with the same velocity. The relation (5.4.1) is satisﬁed over an entire portion of the tension–strain diagram for synthetic strings (Miklowitz [1947], Marshall and Thomson [1954]). Generally cI = cII and we will consider this case. If the slope of the diagram is zero in some portions (for example A B ) then for the corresponding states of tension and strain the propagation of longitudinal waves is no longer possible, and cII = 0. If at a certain moment, the tension at the end of the string begins to increase once more (for instance starting at the point

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Mechanics of Extensible Strings

dynamic

227

Fig. 5.4.1 Typical tension–strain curve. At points A, B, C the velocities of propagation of transverse and longitudinal waves are equal.

B ) the longitudinal waves can propagate again. The case when the longitudinal waves propagate ﬁrst and the transverse ones (which do not produce elongations) later, is the simplest case and has bee studied by many authors (see Rahmatulin and Demianov [1961]). All these authors considered strings which were initially rectilinear and in which the two types of waves propagate successively in distinct portions of the string. 5.5

Boundary and Initial Conditions

We shell now formulate the boundary and initial conditions for a general threedimensional motion of the extensible string (Cristescu [1964]). One can formulate the boundary conditions for ﬁxed or moving points of the string. For instance in problems concerning the impact of strings by moving bodies, the body which strikes the string can contact the same material point of the string permanently or can move along it (ﬂoating boundary). Thus both stationary and moving boundaries have to be considered. The initial conditions can also be formulated in various manners. In the case of a Cauchy problem, for t = 0 and 0 ≤ s0 ≤ l the following functions must be prescribed ε(s0 , 0), v(s0 , 0), x(s0 , 0), . . . , xs0 (s0 , 0), . . . , xt (s0 , 0), . . . ,

(5.5.1)

where l is the initial length of the string. Thus, at the initial moment, the position of the string, the velocity of each of its points, and the strain distribution along the string must be known. It is assumed that the functions (5.5.1) possess continuous ﬁrst order derivatives. In this case (Courant [1962] Ch. V), within a certain band

January 12, 2007

228

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

dynamic

Dynamic Plasticity

0 ≤ t ≤ h, the system (5.3.2) possesses a unique solution with continuous derivatives, provided that h is suﬃciently small and the coeﬃcients in (5.3.2) as well as the data are Lipschitz-continuous. The solution can be further extended for t > h as long as the continuity conditions, which must be satisﬁed by the coeﬃcients, hold. Not all the functions in (5.5.1) can be prescribed arbitrarily since these functions must satisfy certain compatibility conditions, the equations given in the previous paragraphs. If the boundary conditions always aﬀect the same material points of the string (stationary boundaries) the boundary conditions have to be prescribed in the s0 Ot plane along the straight lines s0 = 0 and s0 = l. If the bodies which strike the string, or move its ends, move along the string, then the boundary conditions must be prescribed along ﬂoating boundaries. Such a problems arises for instance, if a string is wrapped around a bobbin. Another example is the safety cables used in the Saturn V rockets which have sent people to the Moon. It is known that in this case, in order to avoid the danger of ﬁre, a cable was attached to the rocket, close to the top (about 100 m), and the other end was attached to a pole on the ground. On this cable was attached a cable, isolated against ﬁre. When testing the system, one has observed that when the cage was going down, that the cable is almost able to wrap up around the pulley. In other words, when going down, the pulley was approaching the velocity of the transverse waves traveling in the cable. In all those cases the motion along the string of the impacting body is smaller than the velocity of propagation of the transverse cI or longitudinal waves. Thus, in most cases, a mixed boundary problem must be solved. If the striking body moves along the string with a velocity higher than cII or cI then certain discontinuities of the shape or of the strain of the string propagate, and these would soon produce an entanglement or rupture of the string. The elastic string. If the string is elastic, the constitutive equation (5.3.1) becomes T = Eε ,

(5.5.2)

where E is an elastic constant. The velocities of propagation of the two waves are (Cristescu [1951]) 1/2 1/2 Eε E cI (ε) = and cII = . (5.5.3) ρ0 (1 + ε) ρ0 Thus, the longitudinal waves propagate with a constant velocity. The equality (5.4.1) is impossible and hence the two waves always propagate with distinct velocities. For each ε, cII > cI (ε). The linear work-hardening string. In this case the constitutive equation (5.3.1) consists of two relations T = Eε if T ≤ TY , (5.5.4) T = TY + E1 (ε − εY ) if T ≥ TY ,

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

Mechanics of Extensible Strings

dynamic

229

where TY is the yield tension of the material considered and E1 is the constant workhardening modulus. If the tension does not exceeds the yield tension the situation coincides with that described above. If T > TY the velocities of propagation become 1/2 1/2 TY + E1 (ε − εY ) E1 cI (ε) = and cII = . (5.5.5) ρ0 (1 + ε) ρ0 It should be noted that in the neighborhood of the yield point, the velocity cI varies continuously with ε, while cII suﬀers a jump from cII = (E/ρ0 )1/2 for T < TY , to cII = (E1 /ρ0 )1/2 for T > TY . Generally cII is smaller in the plastic domain than in the elastic one and is a constant throughout this ﬁrst domain. Depending on the sizes of E1 and TY , three possibilities arise E1

TY 1 + εY

and cII > cI .

(5.5.6)

All of these possibilities are encountered in practice. The last of them leads to certain diﬃculties since, in this case, longitudinal shock waves can appear. The second case has already been discussed above; it corresponds to the case when both types of waves propagate with the same velocity, when the characteristic curves (5.3.6) and (5.3.7) coincide and the last three equations of the system (5.3.2) reduce to ∂xs0 ∂xt + (1 + ε)X = 0 , − ρ0 E1 ∂s0 ∂t with similar equations for y and z. Through the intermediary of ε, this system of equations becomes a system of three partially coupled diﬀerential equations. If external forces are absent the three equations are no longer partially coupled and each of them can be integrated separately. Inextensible strings. Another possible case is that of a string which has suﬀered a former deformation. The strain is then generally distributed non-homogeneously along the string but remains constant in time in each section of the string. In this case the system (5.3.2) reduces to three semi-linear non-coupled equations Φ(s0 )

∂2x ∂2x ∂x dΦ(s0 ) − ρ + + (1 + ε(s0 ))X(s0 , t) = 0 , 0 2 2 ∂s0 ∂t ∂s0 ds0

with two similar ones for y and z. Here Φ(s0 ) = T (ε)/(1 + ε) is a known function of s0 . The integration of such equations do not entail special diﬃculties. If the strain is uniformly distributed along the string ε = const., and the equation reduces to an equation with constant coeﬃcients

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

230

Dynamic Plasticity

c2I

∂2x ∂2x 1 + ε − 2 + X(s0 , t) = 0 , ∂s20 ∂t ρ0

with two others for y and z. Here cI and ε are constants. The string behaves as an inextensible string which may possibly undergo appreciable transverse motions. 5.6

Numerical Examples

The numerical examples are obtained with integration along the four characteristic lines. Details are given in Cristescu [1967] and will not be given here. Examples are given for semi-inﬁnite string, for ﬁnite string, for ﬁnite elastic string. For the extensible cable used to break high speed moving bodies when at the impacted end we have M dV = ATdt where V is the velocity of the body, A is the area of the transverse section of the string and T is the stress at the end of the string (see Fig. 5.6.1):

Fig. 5.6.1

Impact of a rectilinear cable with a fast moving body.

The shape of the cable is shown in Fig. 5.6.2. Were given also vertical velocity, horizontal velocity, strain distribution, longitudinal velocity, and variation of strain along the ﬁrst transverse wave front and the length of the cable at various times.

Fig. 5.6.2

Shape of the cable at various times.

dynamic

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

Mechanics of Extensible Strings

dynamic

231

Fig. 5.6.3 Motion of two bodies connected by an extensible cable; Schematic representation of two positions of the system.

Fig. 5.6.4

Successive positions of the system for the case M ∗ = 2M .

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

232

dynamic

Dynamic Plasticity

The motion of two bodies connected by an extensible cable was also considered. The mass of the two bodies were M ∗ = 2M or 2M ∗ = M (Fig. 5.6.3). The successive positions of the system for the case M ∗ = 2M are given in Fig. 5.6.4. Were also given the strain proﬁle at various time, the characteristic ﬁeld showing the propagation of the ﬁrst longitudinal and the ﬁrst transverse wave fronts in the cable and several reﬂections from the two ends of the cable, the equalization of the vertical velocities of the two bodies, the strain proﬁles at various times and the variation of the length of the cable. 5.7

Rate Inﬂuence

Finite constitutive equations cannot be used to describe the mechanical properties of synthetic strings for which the rate inﬂuence is very large. Thus, in many cases, various classes of diﬀerential constitutive equations, which can be applied to different kinds of materials, must be considered. Some such diﬀerential constitutive equations will be analyzed below in connection with the problem of rapid motion of extensible strings (Cristescu [1965]). The ﬁrst constitutive equation which will be considered is that which is quasilinear both in the rate of strain and in the rate of tension: ∂T ∂ε = g(T, ε) + f (T, ε) , (5.7.1) ∂t ∂t where the functions f and g may possibly depend explicitly on s0 , t, as well as on various characteristic constants (yield tension, etc.). The function g(T, ε) describes the instantaneous response properties of the material, at a certain increment of the tension, while the function f (T, ε) describes the non-instantaneous response properties. Relations of the type (5.7.1) can be used both for loading processes and for non-linear unloading processes. Various special cases of the relation (5.7.1) will be considered below. The constitutive equation must be supplemented by the equations xs0

∂xs0 ∂ys0 ∂zs0 ∂ε + ys0 + zs0 − (1 + ε) = 0, ∂s0 ∂s0 ∂s0 ∂s0

∂xt T ∂xs0 xs0 ∂T xs0 T ∂ε + − ρ0 − + (1 + ε)X = 0 , 1 + ε ∂s0 ∂t 1 + ε ∂s0 (1 + ε)2 ∂s0

(5.7.2)

with two other ones for y and z. (5.7.1) and (5.7.2) represent the system of equations that describes the motion of a string which satisﬁes a constitutive equation of the type (5.7.1). This time, there is one more unknown function T , so that there is now ﬁve unknown quantities i.e. x, y, z, ε and T . In order to ﬁnd the type of this system (5.7.1) and (5.7.2) will be combined with the six equations (5.3.3) as well as the relations dε =

∂ε ∂ε dt , ds0 + ∂s0 ∂t

dT =

∂T ∂T dt . ds0 + ∂s0 ∂t

(5.7.3)

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Mechanics of Extensible Strings

dynamic

233

Taken together, these relations form a system of ten equations with ten unknown derivatives ∂xs0 /∂s0 , ∂xt /∂t, ∂ys0 /∂s0 , ∂yt /∂t, ∂zs0 /∂s0 , ∂zt /∂t, ∂ε/∂s0 , ∂ε/∂t, ∂T /∂s0 and ∂T /∂t. By solving this system with respect to these derivatives, we obtain: ∂ε f dt + gdT + (1 + ε)F gds0 − ρ0 g(ds0 /dt) dv = ∂t [1 − ρ0 g(ds0 /dt)2 ] dv ∂ε −(f dt + gdT − dε) + ρ0 g[dv − (ds0 /dt)dε] − ((1 + ε)/ρ0 )gF ds0 = ∂s0 [1 − ρ0 g(ds0 /dt)2 ] ds0 ∂T −[ρ0 (ds0 /dt)2 f + 1] dT − (1 + ε)F ds0 + ρ0 (ds0 /dt) dv = , ∂t [1 − ρ0 g(ds0 /dt)2 ] dt ∂xs0 [T /(1 + ε) − ρ0 (ds0 /dt)2 ](f dt + gdT − dε)xs0 = ∂s0 −(1 + ε)[T /(1 + ε) − ρ0 (ds0 /dt)2 ][1 − ρ0 g(ds0 /dt)2 ] ds0

(5.7.4)

+

(1 + ε)[1 − ρ0 g(ds0 /dt)2 ][(1 + ε)Xdt − ρ0 dxt + ρ0 (ds0 /dt) dxs0 ] ds0 /dt −(1 + ε)[T /(1 + ε) − ρ0 (ds0 /dt)2 ][1 − ρ0 g(ds0 /dt)2 ] ds0

−

xs0 [1 − T g/(1 + ε)][(1 + ε)F dt − ρ0 (dv − (ds0 /dt) dε)] ds0 /dt , −(1 + ε)[T /(1 + ε) − ρ0 (ds0 /dt)2 ][1 − ρ0 g(ds0 /dt)2 ] ds0

and similarly for the other six derivatives. Thus, in the case of the constitutive equation (5.7.1) the equations of motion of the problem possess ﬁve families of characteristic lines 2 ds 1 T = c2I (T, ε) , = (5.7.5) dt ρ0 1 + ε

ds0 dt

2 =

1 = c2II (T, ε) , ρ0 g

s0 = const.

(5.7.6) (5.7.7)

Along these characteristic lines the following diﬀerential relations ρ0 dxt = ±ρ0 cI dxs0 + (1 + ε)Xdt −

xs0 {(1 − ε)F dt − ρ0 (dv ∓ cI dε)} , 1+ε

± cII (f dt + gdT ) +

1+ε F dt − dv = 0 , ρ0

dε = gdT + f dt ,

(5.7.8) (5.7.9) (5.7.10)

are satisﬁed respectively. Thus there are two types of propagable waves, whose velocities of propagation are functions of both tension and strain. There are also stationary (non propagable) discontinuities (5.7.7). Certain information concerning the nature of the waves which appear in this case can be obtained from the dynamic and kinematics compatibility conditions which are

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

234

dynamic

Dynamic Plasticity

∂xs0 ∂ys0 ∂zs0 ∂ε + ys0 + zs0 − (1 + ε) = 0, xs0 ∂s0 ∂s0 ∂s0 ∂s0 2 & T ∂T ∂xs0 ds0 xs0 xs0 T ∂ε − ρ0 + − = 0, 1+ε dt ∂s0 1 + ε ∂s0 (1 + ε)2 ∂s0 .................. ∂ε ∂T −g = 0, ∂t ∂t −

∂xs0 ∂s0

ds0 dt

2

+

∂xt = 0, ∂t

.................. ∂ε ∂ε dt + ds0 = 0 , ∂t ∂s0

∂T ∂T dt + ds0 = 0 , ∂t ∂s0 (5.7.11)

and four equations for y and z. The ﬁrst ﬁve relations (5.7.11) are the dynamic compatibility equations while last ﬁve are the kinematics compatibility conditions. In (5.7.11) and in the following formulae, the square brackets are used to denote the jump of a certain function across a wave front. Across the characteristic lines (5.7.5), it follows from the second, third and fourth relation (5.7.11) that ∂ε T ∂T = . ∂s0 1 + ε ∂s0 From this relation, and taking into account the other relations (5.7.11) as well, it follows that across a line (5.7.5) ∂ε ∂ε ∂T ∂T = = 0, (5.7.12) = = ∂s0 ∂s0 ∂t ∂t if the relation cI = cII is satisﬁed. Moreover, from the ﬁrst relation (5.7.11), we obtain ∂xs0 ∂ys0 ∂zs0 + ys0 + zs0 = 0. (5.7.13) xs0 ∂s0 ∂s0 ∂s0 Thus from (5.7.12) and (5.7.13) it follows that (5.7.5) are transverse wave fronts which aﬀect only the shape of the string but not the tension nor the longitudinal strain. Both the equation (5.7.5) of the characteristic curves and the diﬀerential relations (5.7.8) satisﬁed on these characteristics formally coincide with those corresponding to the ﬁnite constitutive equation.

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

dynamic

Mechanics of Extensible Strings

235

If one takes into account (5.7.6), it follows from (5.7.11) that across a characteristic of this family the relations 1 ∂xs0 1 ∂ys0 1 ∂zs0 ∂ε = = = (5.7.14) xs0 ∂s0 ys0 ∂s0 zs0 ∂s0 ∂s0 are satisﬁed if cI = cII . Thus the discontinuities of the derivatives of the coordinates are directed along the tangent to the string. From (5.7.14) one obtains conclusions similar to those of (5.3.16) in the case of the ﬁnite constitutive equation. Thus, (5.7.6) represent longitudinal wave fronts which aﬀect the strain and tension but not the shape of the string. The diﬀerential relations (5.7.9) are diﬀerent from those corresponding to the ﬁnite constitutive equation. The characteristics (5.7.12) represent stationary discontinuities. Across such a line, all the derivatives with respect to the variable t (the interior derivatives) are continuous. From the second relation (5.7.11), it follows that: xs0 ∂T xs0 ∂ε ∂xs0 =− + , (5.7.15) ∂s0 T ∂s0 1 + ε ∂s0 with two similar relations for y and z. Introducing this relation into the ﬁrst relation (5.7.11), we obtain [∂T /∂s0 ] = 0, so that the derivatives of the tension are continuous across a line ds0 = 0. It follows that (5.7.15) reduces to (5.7.14) and therefore that the stationary discontinuities aﬀect only the strain. We can consider some special cases. The ﬁrst one is if the form ∂ε ∂T =E − G(T, ε) , ∂t ∂t

(5.7.16)

where the function G(T, ε) is often taken to depend linearly on the overstress G(T, ε) = k[σ − F (ε)] .

(5.7.17)

In (5.7.17) k is a speciﬁc constant of the material while σ = F (ε) is the static constitutive equation of the material considered. Constitutive equation of the form (5.7.16) corresponds to materials whose instantaneous response to a tension increment is purely elastic. A second special case of the constitutive equation (5.7.1) is the constitutive equation ∂ε = f (T, ε) , ∂t

(5.7.18)

which corresponds to materials which do not possess an instantaneous response to an increment of the tension. This case leads to very interesting mathematical problems. The particular case of the Voigt model has been mentioned by Cristescu [1952] while for a general discussion of a constitutive equation of the form T = T (ε, ε) ˙

(5.7.19)

January 12, 2007

236

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

dynamic

Dynamic Plasticity

the reader is referred to Cristescu [1957]. Combining the equations of motion with (5.7.18), one obtains the complete system describing the motion. The characteristics of the system are 2 ds0 1 T = c2 (T, ε) , = (5.7.20) dt ρ0 1 + ε dt = 0 ,

(5.7.21)

ds0 = 0 .

(5.7.22)

It should be noted that the two distinct characteristic lines (5.7.6) in the present special case are superposed and coincide with the family of straight linear dt = 0. The characteristics (6.7.5), which are transverse wave fronts, exist in this particular case too, as for the constitutive equation (5.7.1). Thus the system is of an intermediary type. The inﬂuence of the temperature inﬂuence has been considered by Manacorda [1958]. Let us denote by θ(s0 , t) the actual temperature of the points of the string, by θe the actual external temperature and by θ∗ the initial uniform temperature of both string and external media. We shell also use the notation π = θ − θ∗ and πe = θe − θ∗ . The equations of motion, also take into account the force due to the resistance of the medium in which the string moves. This is of the form −R(x2t + yt2 + zt2 )v with R ≥ 0 (this force is directed along the velocity of the point, but in the opposite sense). Thus ∂ ∂xt T ∂x = + (1 + ε)(X − Rxt ) (5.7.23) ρ0 ∂t ∂s0 1 + ε ∂s0 and two similar expressions for y and z. Attaching the Fourier law and the constitutive law of the form ˙ π) . T = T (s0 , ε, ε,

(5.7.24)

Manacorda showed that across the transverse wave fronts (5.3.6) the second order derivatives of the strain as well as those of the temperature do not suﬀer a jump. Thus, the transverse waves do not directly inﬂuence the strain and temperature variation. The inﬂuence of temperature on the dynamics of extensible strings which move in a resistive medium has also been considered by Dinca [1967], who ﬁrst considered a constitutive equation of the form T = T (ε, π) .

(5.7.25)

The system is of hyperbolic-parabolic type. Dinca [1967] has used also instead of the Fourier law the law proposed by Kaliski [1965] and the system again becomes hyperbolic.

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

Mechanics of Extensible Strings

5.8

dynamic

237

Shock Waves

In the previous sections the integration schemes have been given for cases when only ordinary waves propagate in the string. Thus at the end of the string, for t = 0, the values of the stress and of the particle velocity, prescribed according to boundary and initial conditions, must coincide. In some particular motions of the string, one should consider the possibility that shock waves might appear. Two types of shock waves can occur, i.e. longitudinal shock waves which are propagable discontinuities of ε, T and v, and transverse shock waves which are propagable discontinuities of the slope of the string. We shall examine the propagation of shock waves in strings which can move in space (Cristescu et al. [1966]). As before, it will be assumed that the strings are perfectly ﬂexible, although to neglect the rigidity of the string when considering transverse shock waves is a fairly rash assumption. The propagation of shock waves in various particular cases, when the string moves in a single plane, has been studied by Rakhmatulin (see Rakhmatulin and Dmianov [1961]), P´er`es [1953] Ch. XII, Craggs [1954], and Pavlenko [1959]. The conditions satisﬁed across a shock wave front can be obtained from the conditions of continuity of coordinates, from the conditions of conservations of mass and conservation of momentum. If c is used to denote the velocity of propagation of the shock wave, it follows from the conditions of continuity of coordinates that [xt ] + c[(1 + ε)xs ] = 0 ,

(5.8.1)

with two similar conditions for y and z. These are the kinematics compatibility conditions. The vector form of this relation is [v] + c[(1 + ε)τ ] = 0 .

(5.8.1a)

We shall denote by “+” the value of a certain function after the shock wave front has passed, and by “−” the value of the same function before this event. The law of conservation of mass can be written as follows ρ0 ds0 = ρ− ds− = ρ+ ds+ .

(5.8.2)

Sometimes it is useful to write this relation in the form ρ0 = ρ− (1 + ε− ) = ρ+ (1 + ε+ ) .

(5.8.3)

Considering the element of the string which is traversed by the shock wave front in time dt, and writing for this element, of mass ρ0 ds0 , the conditions of conservation of momentum yields: − − − + + ρ− (1 + ε− )c(x+ t − xt ) = T xs − T xs .

(5.8.4)

The relation (5.8.1) can be written − − − + + x+ t − xt = c{(1 + ε )xs − (1 + ε )xs } .

(5.8.5)

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

238

dynamic

Dynamic Plasticity

Introducing (5.8.5) into (5.8.4) we obtain − − + + − − ρ0 c2 {(1 + ε+ )x+ s − (1 + ε )xs } = T xs − T xs ,

or 2 − − − {ρ0 c2 {(1 + ε+ ) − T + }x+ s = {ρ0 c (1 + ε ) − T }xs ,

(5.8.6)

and similar relations for y and z. The relations (5.8.6) link the values of various functions before and after the shock wave front has passed. They involve both the functions which describe the longitudinal motion of the string, and those which refer to the transverse motion. By squaring the relations (5.8.6), summing, and taking into account that xs , ys , zs are direction cosines which cannot be simultaneously zero, we obtain ρ0 c2 {(1 + ε+ ) − T + = ρ0 c2 (1 + ε− ) − T − ,

(5.8.7)

which yields the velocity of propagation: c2II =

[T ] . ρ0 [ε]

(5.8.8)

The formula (5.8.7) was derived by P´er`es [1953] Ch. XI, and by Pavlenko [1959] for the case of plane motion; it can be used to calculate the velocity of propagation of longitudinal shock waves. This velocity is generally variable and does not coincide with the velocity of propagation of smooth waves. However, this coincidence occurs if the slope is constant on the portion of the tension–strain curve considered (elastic, linear work-hardening, etc.). If the curvature of the tension–strain curve and the jumps [T ] and [ε] are not too big, the velocity furnished by (5.8.8) does not diﬀer greatly from the velocity of propagation of longitudinal smooth waves c2II = (1/ρ0 )(dT /dε). If one introduces (5.8.7) into (5.8.6) it follows that [xs ] = [ys ] = [zs ] = 0 .

(5.8.9)

In this case, and taking (5.8.3) into account, the two kinds of relation (5.8.1) and (5.8.4) reduce to a single type of relation [xt ] = −cII [ε]xs .

(5.8.10)

Thus the shock waves which propagate with the velocity (5.8.8) are longitudinal waves which do not change the shape of the string, while the jump of the material velocity is directed along the tangent to the string. The component of this velocity which is normal to the string remains continuous. The conclusions developed from (5.8.7) hold only if both terms in (5.8.7) are diﬀerent from zero. Let us consider the case when both these terms are zero. This yields a velocity of propagation c furnished by c2 =

T− T+ − T− T+ = = . + − ρ0 (1 + ε ) ρ0 (1 + ε ) ρ0 (ε+ − ε− )

(5.8.11)

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Mechanics of Extensible Strings

dynamic

239

Fig. 5.8.1 The ﬁrst special case when longitudinal and transverse shock waves propagate with the same velocity.

These are shock waves which produce discontinuities for all the unknown functions involved in the problem, i.e. [ε] = 0, [T ] = 0, [xs ] = 0, [ys ] = 0, [zs ] = 0, [xt ] = 0, [yt ] = 0, [zt ] = 0. This case has been discussed by Pavlenco [1959]. Let us examine in what circumstances such waves are possible. A ﬁrst case when such waves may arise is that shown in Fig. 5.8.1, when a whole portion of the stress–strain curve is a segment of the straight line passing trough the point (−1, 0), and the jump of the tension is comprised in this segment. A second possible case has been represented in Fig. 5.8.2, which is selfexplanatory; this case is certainly not a stable one. From these special cases, one can conclude that a shock wave which simultaneously carries discontinuities for both strain and slope, occurs seldom (for very special constitutive equations and loading laws). A third case when (5.8.11) holds is the case when [ε] = 0

so that [T ] = 0 .

In this case the formula (5.8.11) can be written T . c2I = ρ0 (1 + ε)

(5.8.12)

(5.8.13)

Introducing (5.8.12) into (5.8.1) [or into (5.8.4)] it follows that [xt ] + cI (1 + ε)[xs ] = 0 .

(5.8.14)

These are transverse shock waves. Their velocity of propagation (5.8.13) always coincides with the velocity of propagation of smooth transverse waves (5.3.8). For the elastic strings the formula (5.8.13) was given by Cristescu [1951] and for the general extensible strings by P´er`es [1953] Ch. XI #19. Taking into account that the case of simultaneous propagation of discontinuities of strain and slope occurs only very seldom, in the special cases mentioned in

January 12, 2007

10:41

240

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Dynamic Plasticity

Fig. 5.8.2 The second special case (unstable) when longitudinal and transverse shock waves propagate with the same velocity.

Figs. 5.8.1 and 5.8.2, one can conclude that a shock produced at a point of the string will generally propagate by means of two kinds of shock waves, one transverse and the other longitudinal. The discontinuities of the velocity prescribed by the boundary conditions produce a jump of the strain [formula (5.8.19)] which propagates by means of a longitudinal shock wave, and a jump of slope [formula (5.8.14)] which propagates by means of a transverse shock wave. These waves propagate with the velocities (5.8.8) and (5.8.13) respectively.

5.9

Other Papers

The equations of the elastic strings were considered by many other authors. Disturbances produced by the motion of a driver which is rigidly bonded to the edge of a plate are used by Parker and Varley [1968], to motivate parameter expansion technique which, when applied to the equations of ﬁnite elasticity, generate approximating equations which describe law-frequency deﬂection and stretching waves traveling along stretched elastic plates and rods in the limit when bending forces are negligible compared with membrane forces. The structure of the boundary layer at the driven edge and shock layers, where the low-frequency or ﬁlament approximations are locally invalid, are also discussed. The low-frequency equations are used to discuss the interaction between progressing ﬁnite amplitude deﬂection and stretch waves in the limit when the stretch rate is small compared with the angular speed of the plate. The disturbance is locally that of a pure deﬂection simple wave whose amplitude and frequency are modulated by slow variations in the stretch. As the stretch increases the frequency increases while the amplitude

dynamic

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Mechanics of Extensible Strings

dynamic

241

decreases. The stretch wave is also modiﬁed by deﬂection of the plate: the speeds of wavelets carrying constant values of stretch are always less than their values in the pure stretch simple wave. Also, Parker [1970] considers the motion of a plane non-linearly elastic string. It is shown that extensional signals passing through a non-uniform disturbance are not carried along exact characteristics, but are carried at a considerable slower speed, even though the governing equations are non-dispersive. The impact of composites impacted with a body will not be discussed here. We mention only the damage observed in composites, as one is impacting them, the successive impact of various laminas, and the successive damage produced (Cristescu et al. [1975]). That was continued by several other papers as for instance Papanicolaou et al. [1998], Navarro [1998] and Kook et al. [2000]. In these papers the ﬁgures are very close to those from impacted strings. The Riemann and Goursat step data problems for extensible strings have been considered by Mihailescu and Suliciu [1975a, b]. They consider longitudinal discontinuities, for which [λ] = 0, [τ ] = 0, U = λτ (|τ |) = 1, and therefore [U] = [λ]τ ,

[V] + c[λ]τ = 0 ,

c2 =

[T ] , ρ[λ]

and transversal discontinuities, for which [λ] = 0, [τ ] = 0, therefore [U] = λ[τ ] ,

[V] + cλ[τ ] = 0 ,

They write the system to be solved as ∂ T ∂V U −ρ = 0, ∂r λ ∂t T = f (ε) ≥ 0 ,

c2 =

T . ρλ

∂U ∂V − =0 ∂t ∂r

λ = |U| ≥ 1 ,

ε=λ−1

with f (0) = 0 f (ε) > 0

for ε ≥ 0 ,

f (ε) < 0 where U = ∂x/∂r, V = ∂x/∂t, ρ = const. > 0 and x is a function. In order to ensure unique solutions for the problems considered in the paper, one is adopting the following principle. A shock discontinuity is possible only when a rarefaction fan is not possible (Suliciu [1973]). The Goursat problem in strains is solved as well as the problem in velocities and the Riemann problem. The transient response of an impulsively loaded plastic string on a plastic foundation was considered by Mihailescu-Suliciu et al. [1996]. The last authors consider the problem of an impulsive loading of a long rigid-plastic string resting on a rigid-plastic foundation. A closed form solution is obtained by disregarding the longitudinal motion and

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

242

Dynamic Plasticity

Fig. 5.9.1

Final string shape for diﬀerent I0 .

considering an arbitrary large transversal motion. Expressions for the ﬁnal shape of the string are derived in terms of magnitude of the applied impulse. It is found that the stress and the foundation reaction force are not uniquely determined, while the shape of the string is. The ﬁnal shape of the string is given in Fig. 5.9.1. Here w is a dimensionless displacement, ζ a dimensionless variable and I0 an impulse. A continuous initial or initial-boundary value problem for an elastic visco-plastic string on an elastic viscoplastic foundation is formulated by Suliciu [1996]. An energy identity/inequality is deduced. Bounds in energy of the solutions are derived and the stress deviation of the viscoplastic model from the plastic one is estimated. As a farther limiting case similar results are derived for the rigid perfect plastic case. In the paper by Jang et al. [1990] the response of advanced composites to low-velocity projectile loading was investigated. The impact failure mechanisms of composites containing various ﬁbers with diﬀerent strength and ductility were studied by a combination of static indentation testing, instrumented falling dart impact testing, acoustic emission monitoring, and scanning electron microscopy. The composites containing ﬁbers with both high strength and high ductility demonstrate a superior impact resistance as compared to those containing ﬁbers with high strength (graphite ﬁbers) or high ductility (nylon) but not both. Upon impact loading, the composites containing polyethylene ﬁbers usually exhibited a great degree of plastic deformation and some level of delamination. The paper by Wang and Vu-Khanh [1991] reports both experimental and numerical investigations on delamination mechanisms in [05 , 905 , 05 ] carbon ﬁber/poly laminate subjected to low-velocity impact. It was found that these

dynamic

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Mechanics of Extensible Strings

dynamic

243

composites exhibits the same damage mechanisms as epoxy-based composites, but superior delamination resistance. Thick glass-ﬁbre-reinforced laminates of various dimensions have been subjected to low-velocity impact with a ﬂat-ended impactor by Zhou [1995]. Post-impact examination of damage is carried out by visual inspection, diametric crosssectioning, and ultrasonic C-scanning. A number of damage mechanisms have been observed, and their inﬂuence on impact behavior is found to be generally dependent on the impact force or incident kinetic energy level. By replacing the ﬁrst-order law of motion (velocity given) with a second-order law (acceleration given), dynamics of e.g. ﬂexible and rigid elastic strings is described by Uby [1996] in a similar manner. A system of nine coupled partial diﬀerential equations results, but on eliminating longitudinal motion, a smaller system is obtained. Classic vibration equations are recovered as special cases. The free surface spalling phenomena is 2D carbon/carbon and carbon-polyimide laminates was studied by Gupta et al. [1996] by subjecting them to laser-produced nano-second rise-time compressive stress pulses. The compression pulse travels through the laminate normal to the plies and, upon reﬂection into a tension pulse from the sample’s front surface, leads to ﬁber/matrix debondings either in the bundles within a ply or at the interplay interface. Additional information on the attenuation and the dispersion characteristics associated with the propagation of such stress pulses was also obtained for both types of composite microstructures. High speed cine techniques have been used by Gellert et al. [1998] to examine the perforation of thin targets constructed of glass ﬁber reinforced plastic, Spectra and Kevlar composites as well as nylon and Kevlar fabrics. From the ﬁlm record the kinetic, strain and (for the composites only) delamination/surface energy terms were evaluated for the rear layer of material. Simple models for the deformation of the panels were used to compare these energies, summed for all layers, with the projectile energy loss. All the energy terms are shown to be signiﬁcant. The work highlights many of the features which need to be accounted for in modeling ballistic perforation of fabric and ﬁber reinforced composite materials. Karbhari and Rydin [1999] have shown that resin transfer molded composites exhibit impact induced damage mechanisms and sequences diﬀerent from those shown by laminated composites due to diﬀerences in layering and compaction of reinforcement. In addition to the classical modes of damage, mechanisms such as inter-bundle, inter-bundle and void pocket cracking are also seen. In a paper denoted to the Riemann problem, Hanche-Olsen et al. [2002] presents the problem of Riemann for an elastic string with a linear Hooke’s law. They are showing that the Riemann problem has a unique solution. A weak solution of the nonstrictly hyperbolic conservation law when the total variation of the initial data is suﬃciently small is due to Reiﬀ [2002], which examined an elastic string of inﬁnite length in three-dimensional space, restricted to possess non-simple eigenvalues of constant multiplicity.

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

244

Dynamic Plasticity

Fig. 5.9.2

Traveling wave in a whipped string with a phase boundary.

The paper of Purohit and Bhattacharya [2003] presents a theory to describe the dynamical behavior of a string made of a phase-transforming material like a shape-memory alloy. The study of phase boundaries, the driving force acting on them and the kinetic relation governing their propagation is of central concern. The paper proposes a qualitative experimental test of the notion of a kinetic relation, as well as a simple experimental method for measuring it quantitatively. It presents a numerical method for studying initial and boundary value problems in strings, and concludes by exploring the use of phase transforming strings to generate motion at very small scales. Figure 5.9.2 is showing one example of traveling waves in a whipped string; the grid size is 1.25 × 10−3 in this calculation. The string is ﬁxed at the right end, initially stretched horizontally and then whipped or impacted at the left end x = 0 with the following velocity: y˙ 1 = 0 and y˙ 2 = 100.0 m/s , y˙ 2 = −100.0 m/s , y˙ 2 = 0.0 ,

0 ≤ t < 1.6 × 10−4 , 1.6 × 10−4 ≤ t < 3.2 × 10−4 ,

3.2 × 10−4 ≤ t < 1.2 × 10−3 .

The traveling wave propagating through the length of the string is discernible. The breakdown of classical solutions of the planar motion of an elastic string was studied by Manfrin [2004]. The string is inﬁnite in length and having a planar motion, in the absence of external forces. One assumes strict hyperbolicity in the sense

dynamic

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Mechanics of Extensible Strings

T (r) >

dynamic

245

T (r) >0 r

for any r > 1. A novel experimental technique is developed by Minnaar and Zhou [2004] for time-resolved detection and tracking of damage in the forms of delamination and matrix cracking in layered materials such as composite laminates. The technique is non-contact in nature and uses dual or quadruple laser interferometers for high temporal resolution. Simultaneous measurements of diﬀerential displacement and velocity at individual locations are obtained to analyze the initiation and progression of interfacial fracture and/or matrix cracking/delamination in a polymer matrix composite system reinforced by graphite ﬁbers. The measurements at multiple locations allow the speeds or matrix cracking/delamination front propagates to be determined. The results show that the speed of delamination or the speed of matrix cracking/delamination increases linearly with impact velocity. An analytical model for studying the material failure in shear hinges formed during the dynamic plastic response of a circular plate under projectile impact is due to Chen et al. [2005]. Analytic solutions for the ballistic perforation performance of a fully clamped plate struck by a blunt projectile are obtained. It takes into account both the global response (plate bending) and the localized shear. Based on the estimations of the shear strain and the size of shear hinge, condition for the initiation of an adiabatic shear band is formulated. The eﬀectiveness of the present model is demonstrated by reasonable agreement between the theoretical predictions and the available experimental data for the perforation of steel plates. In another paper (Stoﬀel [2006]) an explanation for the development of conical shapes in the case of shock wave loaded plated is proposed based on the wave propagation phenomena. Impact damage processes in composite sheet and sandwich honeycomb materials, impacted with an impactor of 5 kg from a drop hight of 1 m, with a velocity of 4,4 m s−1 , was done by Dear et al. [2006]. Experiments were conducted on aluminum plates of 1 mm thickness by using a gas gun and projectiles with blunt and hemispherical noses (Gupta et al. [2006]). Ballistic limit velocity was found to be higher for hemispherical projectiles than for blunt projectiles. The ballistic impact of woven fabric was done by Naik et al. [2006]. Using the analytical formulation, ballistc limit, contact duration at ballistic limit, surface radious of the cone formed and the radious of the damaged zone have been predicted for typical woven fabric composites. The numerical results of ballistic impact and perforation of woven aramid fabric are presented by Tan et al. [2006]. The crimp is introduced in several ways. Inﬂuence of boundary conditions on the ballistc performance of high-strength fabric target were considered by Zeng et al. [2006]. Targets that are unclamped on two edges can absorb more impact energy than those with all four sides clamped. It

January 12, 2007

10:41

246

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Dynamic Plasticity

also observed that slippage at clamped edges contributes to higher energy absorption. The impact velocity is less than 500 m/s. In another paper (Tan and Ching [2006]) a FE model of woven fabric that reﬂects the orthotropic properties of the fabric, the viscoelastic nature of the yarns, the crimping of the yarns, the sliding contact betveen yarns and yarn breakage using an assembly of viscoelastic bar elements.

Bibliography Chen X. W., Li Q. M. and Fan S. C., 2005, Initiation of adiabatic shear failure in a clamped circular plate, Int. J. Impact Engn. 31, 877–893. Courant R., 1962, Methods of Mathematical Physics, Vol. II, Partial Diﬀerential Equations, Interscience Publi., New York. Craggs J., 1954, Wave motion in plastic-elastic strings, J. Mech. Phis. Solids 2, 4, 115–124. Cristescu N., 1951, Discontinuities in the motion of perfectly ﬂexible elastic strings, Commun. Acad. Rep. Populare Romane 1, 439–445. Cristescu N., 1952, Discontinuities in the motion of visco-elastic, perfectly ﬂexible strings, Rev. Univ. C.I. Parhon Politeh. Bucuresti, Ser. Stiint. Nat. 1, 68–81. Cristescu N., 1954, About the loading and unloading waves which can appear in the motion of elastic or plastic ﬂexible strings, Prikl. Mat. Meh. 18, 3, 257–264 (in Russian). Cristescu N., 1957, On the propagation of waves in rubber, Prikl. Mat. Meh. 21, 6, 797–800 (in Russian). Cristescu N., 1958, Dynamic problems in the theory of plasticity, Editura Tehnica (in Rumanian). Cristescu N., 1960, Elastic-plastic waves in strings, Arch. Mech. Stos. 12, 597–615. Cristescu N., 1961, Spatial motions of elastic-plastic strings, J. Mech. Phys. Solids 9, 165–178. Cristescu N., 1964, Some problems of the mechanics of extensible strings, Symp. IUTAM Stress Waves in Anelastic Solids, Providence, 1963 (Springer-Verlag, Berlin–G¨ otthingen–Heidelberg) 118–132. Cristescu N., 1965, Loading/unloading criteria for rate sensitive materials, Arch. Mech. Stos. 17, 291–305. Cristescu N., 1967, Dynamic Plasticity, North-Holland Pub. Comp., 614 pp. Cristescu N., Dinca G. and Suliciu I., 1966, On the propagation of shock waves in extensible strings, Analele Univ. Bucuresti, Ser. Stiint. Nat., Mat.-Mec. 15, 65–73. Cristescu N., Malvern L. E. and Sierakowski R. L., 1975, in Foreign Object Impact Damage to Composites, ASTM STP 568, American Society for Testing and Materials, pp. 159–172. Dear J. P., Lee H. and Brown S. A., 2006, Impact damage processes in composite sheet and sandwich honeycomb materials, Int. J. Impact Engineerig (in print). Dinca G., 1967, Some remarks about the thermodynamics of extensible strings, Studii Cercetari Matematice 19, 659–680. Fenstermaker C. A. and Smith J. C., 1965, Appl. Polymer Symposia 1, 125–146. Gellert E. P., Pattie S. D. and Woodward R. L., 1998, Energy transfer in ballistic perforation of ﬁber reinforced composites, J. Materials Sci. 33, 1845–1850. Gupta N. K., Iqbal M. A. and Sekhon G. S., 2006, Experimental and numerical studies on the behavior of thin aluminum plates subjected to impact by blunt- and hemisphericsal-nosed projectiles, Int. J. Imp. Engineering (in press).

dynamic

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Mechanics of Extensible Strings

dynamic

247

Gupta V., Pronin A. and Anand K., 1996, Mechanisms and quantiﬁcation of spalling failure in laminated composites under shock loading, J. Composite Mat. 30, 6, 722–747. Hanche-Olsen H., Holden H. and Risebro N. H., 2002, The Riemann problem for an elastic string with a linear Hooke’s law, Quart. Appl. Math. 60, 4, 695–705. Jang B. Z., Chen L. C., Hwang L. R., Hawkes J. E. and Zee R. H., 1990, The response of ﬁbrous composites to impact loading, Polymer Composites 11, 3, 144–157. Karbhari V. M. and Rydin R. W., 1999, Impact characterization of RTM composites II: Damage mechanisms and damage, J. Materials Sci. 34, 5641–5648. Kaliski S., 1965, Wave equation of thermoelasticity, Bull. Acad. Polon. Sci., Ser. Sci. Tech. 13, 211–219. Kook J. S., Yang I. Y. and Adachi T., 2000, Characteristics of delamination in graphite/epoxy laminates under static and impact loads, Key Engng. Materials 183 187, 731–736. Lewis G. M., 1957, Proc. Conf. Prop. Mater. At High Rates of Strain (Inst. Mech. Engrs., London) 190–194. Manacorda T., 1958, Riv. Mat. Univ. Parma 9, 13–19. Manfrin R., 2004, On the breakdown of classical solutions of the planar motion of an elastic string, Bull. Sci. Math. 128, 253–263. Marshall I. and Thomson A. B., 1954, The cold drawing of high polimers, Proc. Roy. Soc. A 221, 541–557. Mihailescu M. and Suliciu I., 1975a, Riemann and Goursat step data problems for extensible strings, J. Math. Anal. Appl. 52, 10–24. Mihailescu M. and Suliciu I., 1975b, Riemann and Goursat step data problems for extensible strings with non-convex stress–strain relation, Rev. Roumaine Math. Pures. Appl. 20, 551–559. Mihailescu-Suliciu M., Suliciu I., Wierzbicki T. and Fatt Hoo M. S., 1996, Transient response of an impulsively loaded plastic string on a plastic foundation, Quart. Appl. Math. 54, 2, 327–343. Miklowitz J., 1947, The initiation and propagation of the plastic zone along a tension specimen of nylon, J. Colloid Sci. 2, 193–215. Minnaar K. and Zhou M., 2004, A novel technique for time-resolved detection and tracking of interfacial and matrix fracture in layered materials, J. Mech. Phys. Solids 52, 2771–2799. Naik N. K., Shrirao P. and Reddy B. C. K., 2006, Ballistic impact behaviour of woven fabric composites: Formulation, Int. J. Impact Engineering (in press). Navarro C., 1998, Simpliﬁed modelling of of the ballistic behaviour of fabrics and ﬁbre reinforced polymeric matrix composites, Key Engin. Mat. 141 143, 383–400. Papanicolaou G. C., Blanas A. M., Pournaras A. V. and Stavropoulos C. D., 1998, Impact damage and residual strength of FRP composites, Key Engin. Mat. 141 143, 127–148. Parker D. F., 1970, Interacting waves in long stretched elastic strings, J. Mech. Phis. Solids 18, 331–342. Parker D. F. and Varley E., 1968, Interaction of ﬁnite amplitude deﬂection and stretching waves in elastic membranes and strings, Quart. Journ. Mech. and Applied Math. 21, Pt.3, 329–352. Pavlenko A. L., 1959, On the propagation of perturbations in a ﬂexible string, Izv. Akad. Nauk. SSSR, Otd. Tekhn. Nauk, Mekhn. Mashinostr. 4, 112–122. P´er`es J., 1953, M´ecanique G´en´erale, Masson, Paris. Purohit P. K. and Bhattacharya K., 2003, Dynamics of strings made of phase transforming materials, J. Mech. Phis. Solids 51, 3, 393–424.

January 12, 2007

248

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Dynamic Plasticity

Rakhmatulin H. A., 1951, Transverse shock with variable velocity on a ﬂexible string, Uch. Zap. Mosk. Univ. 4, 5, 154. Rakhmatulin H. A. and Shapiro G. S., 1955, Propagation of perturbations in non linear-elastic and nonelastic media, Izv. Akad. Nauk SSSR, Otd. Fekhn. Nauk 2, 68–89. Rahmatulin H. A. and Demianov Yu. A., 1961, Strength under intensive momentary loads, Moscow (in Russian). Reiﬀ A. M., 2002, Existence of weak solutions to the elastic string equations in three dimensions, Quart. Appl. Math. 60, 3, 401–424. Riabova E. H., 1953, Transverse shock with variable velocity on a ﬂexible string, Vestn. Mosk. Univ. 10, 85–91. Smith J. C., Blandford J. M. and Schiefer H. F., 1960, Stress–strain relationship of yarns subjected to rapid impact loading: 6. Velocities of strain waves resulting from impact, Textile Res. J. 30, 10, 752–769. Smith J. C., Crackin F. L. Mc and Schiefer H. F., 1958, Stress–strain relationship in yarns subjected to rapid impact loading: 5. Wave propagation in long textile yarns impacted transversely, J. Res. Nat. Std. 60, 5, 517–534. Smith J. C., Crackin F. L. Mc, Schiefer H. F., Sione W. K. and Towne K. M., 1956, Stress–strain relationship in yarns subjected to rapid impact loading: 4. Transverse impact tests, J. Res. Nat. Bur. Std. 57, 2, 83–89. Smith J. C. and Fenstermaker C. A., 1967, Strain-wave propagation in strips of natural rubber subjected to high-velocity transverse impact, J. Appl. Phys. 38, 11, 4218–4224. Smith J. C., Fenstermaker C. A. and Shouse P. J., 1964, Experimental determination of air drag on textile yarn struck transversely by high-velocity projectile, J. Res. Nat. Bur. Std. C 68, 177–181. Smith J. C., Fenstermaker C. A. and Shouse P. J., 1965, Stress–strain relationships in yarns subjected to rapid impact loading. 11. Strain distribution resulting from riﬂe bullet impact, Textile Res. J. 35, 743. Smith J. C., Fenstermaker C. A. and Shouse P. J., 1963, Experimental determination of air drag on textile yarn struck transversly by high-velocity projectile, Textile Res. J. 33, 919–934. Smith J. C., Shouse P. J., Blandford J. M. and Towne K. M., 1961, Textile Res. J. 31, 721–734. Stoﬀel M., 2006, Shape forming of shock wave loaded viscoplastic plates, Mec. Res. Comm. 33, 35–41. Suliciu I., 1973, Motions with discontinuit´es in solides — Nonlinear models, Stud. Cerc. Mat. 25, 53–170 (in Rumanian). Suliciu I., 1996, An energetic characterization of the constitutive equations for plastic strings on plastic foundations, Constitutive Relation in High/Very High Strain Rates, IUTAM Symposium, Noda, Japan, Oct. 16–19, 1995. Spriger Vlg. Tan V. B. C. and Ching T. W., 2006, Computational simulation of fabric armour subjected to ballistic impacts, Int. J. Impact Engineering (in press). Tan V. B. C., Shim V. P. W. and Zeng X., 2006, Modelling crimp in woven fabrics subjected to ballistic impact, Int. J. Impact Engineering (in print). Uby L., 1996, Strings, rods, vortices and wave equations, Proc. R. Soc. Lond. 452, 1531–1543. Victorov V. V., Dobrovolsckii I. P., Cristrescu N., Kovalenco T. S., Stepanov P. D. and Shapiro G. S., 1966, Study of some dynamic properties of some polymers, Proc. Symp. on the Prop. of Elastic-plastic Waves in Cont. Med., Baku, 1964, 103–108.

dynamic

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Mechanics of Extensible Strings

dynamic

249

Wang H. and Vu-Khanh T., 1991, Impact-induced delamination in [05 , 905 , 05 ] carbon ﬁber/polyetheretherketone composite laminates, Polymer Eng. Sci. 31, 18, 1301–1309. Zeng X. S., Shim V. P. W. and Tan V. B. C., 2006, Inﬂuence of boundary conditions on the ballistic performance of high-strength fabric targets, Int. J. Impact Engineering (in press). Zhou G., 1995, Damage mechanisms in composite laminates impacted by a ﬂat-ended impactor, Composites Sci. Tech. 54, 267–273.

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

This page intentionally left blank

dynamic

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

dynamic

Chapter 6

Flow of a Bigham Fluid

This chapter is devoted to the motion of a Bingham body through various devices; through a tube with or without friction at the wall, ﬂow in a viscosimeter, ﬂow in the ﬁeld of natural slopes, etc. Plastic ﬂow through conical converging dies will not be described (Cristescu [1975] [1976], Fu and Loo [1995]). For general concept on strain rate intensity factor see Aleksandrov et al. [2003].

6.1

Flow of a Bingham Fluid Through a Tube

We consider a tube of length l and of radius R (Buckingham [1921]). We work in cylindrical coordinates. At z = 0 we have (Fig. 6.1.1) σ = −p

(6.1.1)

that is a pressure is applied.

r

v(r)

2r0

R

z

0

l Fig. 6.1.1

The ﬂow in a tube.

251

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

252

dynamic

Dynamic Plasticity

We assume “telescopic ﬂow” i.e., vr = vθ = 0 ,

vz = v = f (r) .

(6.1.2)

The rate of deformation tensor in cylindrical coordinates are Drr

Drz

1 ∂vθ ∂vr vr ∂vz 1 , Dθθ = + , Dzz = , Dθz = = ∂r r r ∂θ ∂z 2 ∂vz vθ 1 ∂vr 1 ∂vr 1 ∂vθ + , Drθ = − + . = 2 ∂z ∂r 2 ∂r r r ∂θ

∂vθ 1 ∂vz + r ∂θ ∂z

,

From here for our problem we have Drr = Dθθ = Dzz = Dθz = Drθ = 0 ,

Drz =

1 f (r) . 2

(6.1.3)

The constitutive equation for a Bingham (viscoplastic/rigid) ﬂuid is: σij = σδij + kij + 2ηDij

(6.1.4)

with the plastic part Dij = 2λkij

if

kij kij = 2k 2 .

(6.1.5)

If only kij kij < 2k 2

we have Dij = 0 .

From (6.1.3) and (6.1.5) we obtain Drz = 2λkrz

2 and krz = k 2 = τY2 .

(6.1.6)

Thus for the only non zero component: krz = kzr = τY (sign Drz ), all other kij = 0 .

(6.1.7)

We observe now that f < 0 or (∂vz /∂r) < 0 since vz decreases with increasing r. = 0, besides Drz and σrz . We Therefore sign Drz = −1. Since all Dij = 0 all σij have thus σrr = σθθ = σzz = σ ,

σθz = σrθ = 0 ,

σrz = σzr = −τY + ηf (r) .

(6.1.8)

The equations of motion in cylindrical coordinates are: 1 ∂σrθ ∂σzr σrr − σθθ ∂σrr + + + + ρ(br − ar ) = 0 , ∂r r ∂θ ∂z r 1 ∂σθθ ∂σzθ 2σrθ ∂σrθ + + + + ρ(bθ − aθ ) = 0 , ∂r r ∂θ ∂z r 1 ∂σzθ ∂σzz σrz ∂σrz + + + + ρ(bz − az ) = 0 . ∂r r ∂θ ∂z r

(6.1.9)

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

Flow of a Bigham Fluid

dynamic

253

Introducing (6.1.8) in (6.1.9)1 and (6.1.9)2 , and by disregarding the body forces and the accelerations, we have: ∂σ ∂σrr =0⇒ = 0, ∂r ∂r

⇒ σ(z) ∂σ ∂σθθ =0⇒ = 0, ∂θ ∂θ thus σ depends on z alone. Introducing (6.1.8) in (6.1.9)3 we obtain: dσ τY f = −η f + + , dz r r

(6.1.10)

(6.1.11)

where σ depends on z alone and f depends on r alone. This by integrating with respect to z we get τY f + z+C (6.1.12) σ = −η f + r r with the boundary conditions at the end of the tube (independent on r, thus constant in the hole cross section): z = 0 : σ = σ0 ⇒ C = σ0 z = l : σl = 0 .

(6.1.13)

Thus for z = l, from (6.1.12), by integration with respect to r, we obtain: −ηf r + τY r +

σ0 r2 + C1 = 0 l 2

(6.1.14)

or C1 σ0 r + . l 2 r Comparing now this equation with the last (6.1.8) we get: ηf = τY +

C1 σ0 r + . l 2 r From the shearing ﬂow symmetry it follows that for σrz =

r = 0,

(6.1.15)

(6.1.16)

∂v = 0 ⇒ f = 0 ⇒ Drz |r=0 = 0 ⇒ σrz |r=0 . ∂r

Thus, around r = 0 exists a cylinder of radius r0 , where kij kij < 2k 2 , i.e., is rigid and for r = r0 : σrz = −τY

(6.1.17)

the condition kij kij = 2k 2 is just satisﬁed. Introducing (6.1.17) in (6.1.16) for r = r0 we have −τY =

C1 σ0 r0 + . l 2 r0

(6.1.18)

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

254

dynamic

Dynamic Plasticity

From the global equilibrium condition of rigid cylinder of radius r0 (the inner core): πr02 σ0 = −τY (2πr0 )l or r0 σ0 . (6.1.19) τY = − 2l Introducing (6.1.19) in (6.1.18) we get C1 = 0. Returning to (6.1.15) by integration: σ0 −ηv + τY r + r2 + C2 = 0 . (6.1.20) 4l Flow with wall adherence. We assume now that the material adheres on the wall, i.e., r = R : v = 0.

(6.1.21)

By introducing (6.1.21) in (6.1.20) we obtain τY R + (σ0 /4l)R2 = −C2 and from (6.1.20): σ0 ηv = τY (r − R) + (r2 − R2 ) . (6.1.22) 4l If we put here v = 0 we get for r two solutions r1 = R ,

r2 = −R + 2r0 .

The second solution is impossible, since we must have r0 > R. The velocity of the rigid internal nucleus is obtained from (6.1.22) for r = r0 : σ0 (r0 − R)2 . v0 = − (6.1.23) 4lη The radius of the nucleus is [from (6.1.19)]: r0 = −

2lτY 2lτY = σ0 ∆p

with

σ0 < 0 .

(6.1.24)

If τY → 0 from (6.1.20) follows r0 → 0 and (6.1.22) becomes a parabolic distribution of velocities of a viscous ﬂuid, i.e., for ﬁxed l and ∆p, r0 is a measure of “plasticity”. Some conclusions: • r0 increases with l; when r0 increases towards R, l increases towards lMAX = (R∆p/2τY ), and from (6.1.23) v0 → 0. • r0 increases with τY (decrease of temperature, decrease of humidity, irradiation, etc.) when τY increases its maximal value is τYMAX = (R∆p/2l), from (6.1.24) r0 → R, and from (6.1.23) v0 → 0. • r0 decreases with the increasing σ0 , i.e., the inner core radius decreases with increasing pressure. If σ0 ⇒ r0 , i.e., σ0 towards σ0min = −2lτY /R and from (6.1.24) r0 → R and from (6.1.23) v0 → 0. • The maximum value of r0 is R = (2lτY /∆p), when the whole body becomes rigid and from (6.1.23) v = 0 since the ﬂuid adhere on the wall and v0 → 0. • Flow is possible only if r0 < R or (2lτY /∆p) < R or ∆p > (2lτY /R) is the limit pressure diﬀerence for the ﬂow to take place.

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

dynamic

Flow of a Bigham Fluid

255

• ∆p must be bigger if: the tube is longer (bigger l) τY is bigger (lower temperature or dryer paste) smaller R If the ﬂuid does not adhere to the wall, i.e., the slip is possible, see below. Volume ﬂux. The volume ﬂux of the ﬂuid comprised between r0 and R is: 2 2 2 4 4 − R σ0 R − r0 + σ0 R − r0 R 4l 2 4l 4 dQ1 2π = v2πr dr = dt η r0 R3 − r03 R2 − r02 −τY R − 2 3

(6.1.25)

with v from (6.1.22), or

r 3 r 2 dQ1 πσ0 R4 4 r0 5 r0 4 0 0 =− 1− − . +4 −2 dt 8ηl 3R 3 R R R

(6.1.26)

The volume ﬂux Q2 of the portion which remain rigid is [with v from (6.1.23)]: r0 r0 2πσ0 πσ0 dQ2 2 v2πr dr = − r dr = − = (r0 − R) (r0 − R)2 r02 . dt 4lη 4lη 0 0 (6.1.27) If at t = 0, Q = 0, the total volume ﬂux is Q = Q1 + Q2 , and 4 r0 Q πσ0 R4 1 r0 4 1− =− + t 8lη 3R 3 R

(6.1.28)

and with r0 from (6.1.24):

# 4 $ Q πσ0 R4 4 2 lτY 1 2lτY =− 1+ + t 8lη 3 R σ0 3 Rσ0

or

# 2 $ 2 Q πσ0 R4 2 2lτY 2lτY 1 2lτY =− 1− 1+ + t 8lη 3 Rσ0 3 Rσ0 Rσ0

(6.1.29)

(6.1.30)

which is the formula of Buckingham [1921]–Reiner [1926]. For τY = 0 this formula reduces to the one for viscous ﬂuids. If we introduce variables which do not depend on the tube dimensions V = (6.1.30) is written V =

4 Q/t , R3 π

P =−

Rσ0 2l

2 τY 1 τY 2 τY 2 P 1− + 1− η 3 P 3 P P

(6.1.31)

(6.1.32)

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

256

dynamic

Dynamic Plasticity

Ne wt on V

=P /η

V

B 0

a gh in

m

P

τY

Fig. 6.1.2

The diﬀerence between the two formulas.

for τY → 0 we obtain the solution for Newtonian viscosity V =

P η

or

Q πR4 σ0 = t 8ηl

i.e., the Hagen–Poiseuille formula (Fig. 6.1.2). Flow with friction at the wall. Viscous friction. For a general Bingham material, the fact that for r0 → R the ﬂow is no more possible is a restriction which we have to remove. Generally, when r0 increases, v0 decreases. This could be accepted up to a certain limit. Let us assume that for r0 → R : v → vf

(6.1.33)

where vf would be a limit velocity due to friction between the Bingham body and the wall. In this case, by replacing (6.1.22) by (6.1.33) we get η(v − vf ) = τY (r − R) +

σ0 2 (r − R2 ) . 4l

(6.1.34)

An estimation of the friction shearing stress τf can be obtained by assuming r0 = R and considering the motion of the material as a rigid body: πR2 σ0 = 2πRlτf or τf =

Rσ0 . 2l

(6.1.35)

Let us further assume that the friction takes place in a “boundary layer” of thickness h, and that the property of this boundary layer can be approximated by a Newtonian linear viscous ﬂow σ = 2µD, where µ is a viscosity coeﬃcient for the boundary layer. For the σrz = τf component we get ∂vf vf vf ≈ (6.1.36) τf = µ h ∂r h

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

Flow of a Bigham Fluid

Fig. 6.1.3

dynamic

257

The ﬂow of a Bingham body with adherence at the wall.

where h is the thickness of the boundary layer (assumed to be 10−n cm, with n = 3 or 4, say). Combining (6.1.36) and (6.1.35): vf =

Rσ0 h 2lµ

(6.1.37)

which is to be introduced in (6.1.34). Examples are given in Fig. 6.1.3 for v = 0 at r = R and in Fig. 6.1.4 for v = vf at r = R. The examples are computed for R = 2 cm, l = 20 cm, τY = 20 kPa, h = 10−2 cm, σ0 = 1 Mpa, µ = 0.01 kPa s and η = 1 s−1 . Viscoplastic friction. Any other friction law could be considered, for instance the friction law proposed for metal plasticity (Cristescu [1975]) (6.1.38) τ = m IIσ where m is a “friction factor” 0 ≤ m ≤ 1, with m = 1 corresponding to adherence and m = 0 for no friction. For Bingham model this law becomes: τ = m(τY + 2η IID ) . (6.1.39)

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

258

dynamic

Dynamic Plasticity

Fig. 6.1.4

The ﬂow of a Bingham body with friction at the wall.

For our case we have τ = m(−τY + 2ηDrz ) . Thus the slide takes place when Drz at the wall reaches the value 1 1 σ0 σ0 τY + r , σrz = r, Drz = f (r) = 2 2η 2l 2l and at the wall the law (6.1.40) becomes: σ0 τ = m R = mσrz |R . 2l Thus the sliding starts when the applied pressure reaches the " " 2l τ 2l = σrz "" σ0 = mR R R

(6.1.40)

(6.1.41)

(6.1.42)

(6.1.43)

and, again: τ = mσrz |R .

(6.1.44)

Thus, more pressure is needed if the contact surface ﬂuid/tube is longer, if the tube is thinner, and if m is bigger.

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

Flow of a Bigham Fluid

Fig. 6.1.5

dynamic

259

Motion in the case of a viscoplastic friction.

In the case when a viscous layer does not exist any more, and r0 = R, σrz |R = (σ0 /2l)R, and σrz |R increases with σ0 . When σ0 reaches a certain limit, satisfying (6.1.44) the plug moves. Figure 6.1.5 is an example.

6.2

Flow of a Bingham Fluid Between Two Circular Concentric Cylinders (Reiner [1960])

Let us consider two circular concentric cylinders of height h. The inner one has the radius Ri and is either kept ﬁxed and a torque M is measured, or is rotating with angular velocity ω˙ i . The external cylinder, of radius Re > Ri is either rotating with the angular velocity ω˙ e or is ﬁxed. Let us consider the stationary motion of a ﬂuid between these two cylinders (Fig. 6.2.1). This is a typical motion taking place in viscometers. If ω˙ i = 0 the viscometer is of Couette–Hatschek type. If ω˙ e = 0 we get the principle of the Searle viscometer. The ﬁxed cylinder (or mobile) can be used also for the measurement of the torque induced by the rotating ﬂuid.

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

260

dynamic

Dynamic Plasticity

h

Ri

Re

r1

ω e

Fig. 6.2.1

Flow of Bingham body between two cylinders.

We use cylindrical spatial coordinates r, θ, z. We assume the ﬂow ﬁeld of the form vr = vz = 0 ,

vθ = v = f (r) .

(6.2.1)

The components of the rate of deformation tensor in cylindrical coordinates become in this case vθ 1 f 1 ∂vθ − = f − , Drθ = 2 ∂r r 2 r Drr = Dθθ = Dzz = Drz = Dθz = 0 .

(6.2.2)

Since every single particle is in motion v = f = rω(r) ˙

(6.2.3)

where the angular velocity ω˙ depends on r. The rate of deformation becomes r dω˙ . 2 dr The Newtonian viscous ﬂuid is the ﬁrst case to consider. Drθ =

σrθ = ηr

dω˙ dr

(6.2.4)

(6.2.5)

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

Flow of a Bigham Fluid

dynamic

261

and σrr = σθθ = σzz = −p and σzθ = σzr = 0 .

(6.2.6)

The equilibrium equations becomes for this case (disregarding the body forces and the accelerations): ∂p 1 ∂σrθ − + = 0, ∂r r ∂θ ∂σrθ 1 ∂p 2σrθ − + = 0, ∂r r ∂θ r ∂p = 0. (6.2.7) ∂z Taking into account that the problem is with axial symmetry (∂/∂θ = 0) it follows that p = const. (the atmospheric pressure). From (6.2.7)2 follows C1 σrθ = 2 (6.2.8) r and with (6.2.5): dω˙ C1 η = 2 (6.2.9) dr r i.e., C1 (6.2.10) η ω˙ = 2 + C2 . 2r The two constants are determined from the boundary conditions: −

t>0

r = Ri : ω˙ = ω˙ i ,

Thus

C1 = 2η(ω˙ e − ω˙ i )

C2 = 2η

(6.2.11)

r = Re : ω˙ = ω˙ e . 1 1 − 2 Ri2 Re

−1

ω˙ e Re2 − ω˙ i Ri2 . Re2 − Ri2

(6.2.12)

Introducing in (6.2.10) we get: ω˙ =

ω˙ i Ri2 (Re2 /r2 − 1) − ω˙ e Re2 (Ri2 /r2 − 1) Re2 − Ri2

while the tangential stress follows from (6.2.8): 2η ω˙ e − ω˙ i . σrθ = 2 r 1/Ri2 − 1/Re2

(6.2.13)

(6.2.14)

The torque exerted on a cylindrical surface of radius r and of height h can be estimated as M = σrθ (2πrh) r

(6.2.15)

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

262

dynamic

Dynamic Plasticity

i.e., with (6.2.14): M = 4ηπh

ω˙ e − ω˙ i . 1/Ri2 − 1/Re2

Thus the torque is independent on r. In the particular case when the internal cylinder is ﬁxed: ω˙ i = 0 , ω˙ = ω˙ e

Re2 (1 − Ri2 /r2 ) , Re2 − Ri2

M = 4ηπh

1/Ri2

ω˙ e . − 1/Re2

(6.2.16)

The torque is measured either on the internal (ﬁxed) cylinder, or on the external one. In the particular case when the external cylinder is ﬁxed; ω˙ e = 0 , ω˙ = ω˙ i

Ri2 (Re2 /r2 − 1) , Re2 − Ri2

M = 4ηπh

−ω˙ i . − 1/Re2

1/Ri2

(6.2.17)

The Bingham ﬂuid. The constitutive equation is now: dω˙ dr

for σrθ > τY ,

ω˙ = const. = 0

for σrθ ≤ τY .

σrθ = τY + ηr

(6.2.18)

The other stress components satisfy (6.2.6) with p = const. From (6.2.7)2 follows again (6.2.8) and therefore with (6.2.18): dω˙ C1 τY +η = 3 , r dr r

(6.2.19)

or after integration C1 − τY ln r + C2 . (6.2.20) 2r2 Let us assume now that the internal cylinder is ﬁxed and the other one rotates with the angular velocity ω˙ e prescribed. Thus for η ω˙ = −

t>0

r = Ri : ω˙ i = 0 , r = Re : ω˙ = ω˙ e .

From (6.2.21)1 and (6.2.20) follows C2 =

C1 + τY ln Ri 2Ri2

(6.2.21)

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Flow of a Bigham Fluid

and (6.2.20) becomes C1 η ω˙ = 2

1 1 − 2 Ri2 r

− τY ln

dynamic

263

r . Ri

(6.2.22)

The constant C1 can be determined if the torque M is measured on one of the cylinders. We have M , (6.2.23) 2πh where h is the height of the portion of the cylinder in contact with the ﬂuid. Thus (6.2.22) becomes, if M is known, 1 1 r M − τY ln − (6.2.24) η ω˙ = 4πh Ri2 r2 Ri C1 =

and for the outer cylinder: M η ω˙ e = 4πh

1 1 − 2 Ri2 Re

− τY ln

Re Ri

(6.2.25)

which is the formula due to Reiner and Riwlin [1927]. In the particular case τY → 0 we obtain again (6.2.17)3 for the viscous ﬂuid. From (6.2.15) follows that for a constant value of M , the tangential stress σrθ is bigger when r is smaller. On the other hand the ﬂow takes place only if σrθ > τY , i.e., [from (6.2.15)]: M > M0 = τY 2πRi2 h .

(6.2.26)

M < M0

(6.2.27)

If

the Bingham ﬂuid is stressed, but no ﬂow is possible. If however (6.2.26) is satisﬁed, then a portion of the material in the neighborhood of the inner cylinder is ﬂowing. If the value of the measured moment is M1 , the radius r1 of the portion of the material which is in motion can be obtained from (6.2.15) for σrθ = τY : M1 r1 = . (6.2.28) 2πhτY The condition that the whole material in Ri ≤ r ≤ Re be in motion (i.e., r1 = Re ) is M ≥ Me = 2πRe2 hτY .

(6.2.29)

If M1 and r1 are measured (6.2.28) can be used to determine τY . Afterwards from (6.2.25) follows η. If the material comprised between r1 ≤ r < Re rotates as a rigid, the formula (6.2.24) becomes 1 M1 1 r1 − τY ln − (6.2.30) η ω˙ 1 = 2 2 4πh Ri r1 Ri

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

264

dynamic

Dynamic Plasticity

4πhη τ Y Re ln 1/Ri2 − 1/Re2 η Ri

4ηπ

M=

M=

Ne wto

nia

Bin gha m

e

n fl uid h ω& e 1/R 2 i − 1/R 2

4π 1/R 2 hη i − 1/R 2 ω&1 + τ Y e η ln Re Ri

ω1

0 No flow

= M0 increa sin g r1

Me

M Ri < r < Re

r1 = Re

r1 = Ri

Ri < r < r1 − viscoplastic ri < r < Re − rigid Fig. 6.2.2

The relationship between M and ω. ˙

and for the torque M1 =

4πhη 1/Ri2 − 1/r12

r1 τY ln ω˙ 1 + . η Ri

(6.2.31)

In Fig. 6.2.2 is showing the diﬀerent relations between M and ω˙ which results from the formulae. 4πhη τY Re ln 1/Ri2 − 1/Re2 η Ri is a measure of the Bingham eﬀect. It is sometimes convenient to introduce dimensionless variables, independent on the geometry of the apparatus V =2

ω˙ i , 1 − Ri2 /Re2

P =

M . 2Ri2 πh

With these variables one can rewrite (6.2.24) to become P τY ln(Ri /Re )2 V = 1− . η P 1 − (Ri /Re )2

(6.2.32)

(6.2.33)

The relationship P ∼ V deﬁnes the properties of the material called consistency.

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Flow of a Bigham Fluid

dynamic

265

Re

δ Ri r1

ω e Viscoplastic fluid

ω w

Rigid Boundary layer Fig. 6.2.3

The motion with a boundary layer.

For τY → 0 the model becomes a viscous ﬂuid. For η → 0 the model becomes a perfectly plastic one. Boundary layer. Static/dynamic dry friction. As the torque or ω˙ e is increased, there is a limit value of r1 when the powder (the Bingham body) in contact with the wall, will slip (Fig. 6.2.3). This will happen when the shear transmitted to the cylindrical surface of radius r1 equals or surpasses the frictional shearing force exerted on the cylinder of radius Re : 2πr1 hτY = 2πRe hτf , where τf is the frictional shearing stress. Thus (see Fig. 6.2.4) r1 τY = Re τf .

(6.2.34)

So long as τf >

r1 τY Re

(6.2.35)

the ﬂuid will adhere to the wall. If however, when r1 is increasing towards r1f r1f τY τf ≤ (6.2.36) Re the rigid portion of the ﬂuid of thickness Re − r1f will slip along the wall. Let us assume that in a very thin layer of thickness δ (see Fig. 6.2.3) the friction law can be described by a relationship of the form (6.2.37) τf = m(τY − 2n IID )

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

266

dynamic

Dynamic Plasticity

ω

increase during dynamic friction

start of dynamic friction

ω e − ω w

end of dynamic friction initiation

M0

Ms Me

M

∆M Fig. 6.2.4

Explanation of the text.

where m is a “friction factor” with 0 ≤ m ≤ 1, IID is the second invariant of the rate of deformation tensor of the material in the boundary layer, and n is a “dynamic friction factor” expressing a measure between the “static” and “dynamic” frictions. If no slip takes place then IID = 0 and the “static” friction law is τf = mτY .

(6.2.38)

The value m = 0 corresponds to perfect lubrication, when τf = 0. From (6.2.34) follows r1 = 0 and therefore the whole volume of ﬂuid comprised between Ri ≤ r ≤ Re is not moving at all and remain rigid. For m = 1 we get the other extreme case; again from (6.2.34) follows r1 = Re , i.e., when ω˙ (or M ) increases it is ultimately possible that the thickness of the rigid layer be reduced to zero thickness, when M → Me (Fig. 6.2.5). In the general case the law (6.2.37) will be used to describe the friction when the slip takes place. Since in IID a single nonzero component is involved r dω˙ (6.2.39) 2 dr we will write this component for the thin layer of thickness δ as nonzero component is involved Re ω˙ w − ω˙ e (6.2.40) Drθ ∼ = 2 δ where ω˙ w is the angular velocity of the external viscometer cylinder, ω˙ e is the “external” angular velocity of the layer r = Re after sliding (Fig. 6.2.6). The Drθ =

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

Flow of a Bigham Fluid

dynamic

267

Rigid Viscoplastic Ri

ω1

Re r1

τY

τ f > τY Fig. 6.2.5

Velocity proﬁle for r1 < Re .

Viscoplastic

Ri Re

Fig. 6.2.6

Velocity proﬁle for r1 = Re .

friction law (6.2.37) becomes

ω˙ w − ω˙ e τf = m τY − nRe δ

from where follows

(6.2.41)

δ . (6.2.42) m nRe Here since during dynamic friction τf < mτY follows that ω˙ e < ω˙ w . δ depends on the material and ﬂuid/viscometer interface, and n is the measure of the diﬀerence ω˙ e = ω˙ w +

τ

f

− τY

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

268

Dynamic Plasticity

ω w

Rigid Viscoplastic

ω e

Ri

Re

r1 τY

τf Fig. 6.2.7

Velocity proﬁle for the case of sliding with dry dynamic friction.

between static and dynamic frictions. In the case of “static” friction, when (6.2.38) holds, from (6.2.42) follows ω˙ e = ω˙ w . (6.2.42) is giving the value of ω˙ e to be introduced in the boundary condition (6.2.21). The quantity δ τ f (6.2.43) ∆ω˙ = ω˙ e − ω˙ w = − τY m nRe is the sudden decrease of ω˙ e and as such produces a sudden decrease ∆M of M [see (6.2.31)]. From the value Ms reached just before slip have started, M decreases to Ms − ∆M during slip. The jump decrease of M produces a jump decrease of r1 [see (6.2.28)], i.e., a sudden increase of the thickness of the rigid portion of the ﬂuid (Fig. 6.2.7). If ω˙ or M are further increased, r1 will continue to increase again. If ∆M is measured, one can determine ∆ω˙ and thus δ/n, assuming that m is determined by other experimental procedures. If δ is obtained by physical considerations, n follows. Generally we need the ratio δ/n, only. 6.3

A Model for Slow Motion of Natural Slopes (Cristescu et al. [2002])

Introduction. Gravitational creep ﬂow, in the sense of deformation in time along a slope under gravitational forces, is often encountered in nature. Examples include: submarine landslides, debris ﬂow, coal slurries, drilling mud, etc. Bedrock landslides have long been recognized as signiﬁcant geomorphic processes in mountainous topography.

dynamic

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Flow of a Bigham Fluid

dynamic

269

Some landslides are deep-seated and involve long-term displacement at low strain rates. Landslide velocities extend from millimeters per year, to hundreds of kilometers per hour. Conventional stability analysis, which treats the geologic material in the slope as a rigid perfectly plastic body, may provide information on the safety factor of stable mass of soil. To describe this a variety of nonlinear viscous models have been considered. To overcome some of limitations of the viscous ﬂow models, Desai et al. [1995] developed an elasto-viscoplastic model. Based on ﬁeld observations, it was assumed that a shear zone exists up to a certain depth, while the bottom layer under the shear zone remains rigid and at rest. It was supposed that in the shear zone the material obeys an associated viscoplastic constitutive equation while the inﬂuence between the rigid bottom and the shearing zone was described by a non associated viscoplastic constitutive equation. The postulated thickness of each of these zones was based on ﬁeld observations. The “interface” model developed by Desai et al. [1995] was further reﬁned by Samtani et al. [1996]; ﬁnite element implementation of the interface element was described along with veriﬁcation of the model with respect to the ﬁeld behavior of a creeping natural slope. The model parameters are determined from laboratory tests. Below is presented a new model describing gravitational motion along a slope. First, an analysis of gravitational consolidation is performed using an elasticviscoplastic constitutive equation for dry sand (Cristescu [1991]). Based on this analysis, it can be concluded that the assumption of a linear variation of density with depth applies. This hypothesis is supported by most experimental data (see for example Desai et al. [1995]). Next, a non homogeneous Bingham model, with yield stress depending on the current density, is considered for the geologic material in the slope. Although the density could be considered to be linearly dependent on depth, it is shown that a linear variation of the yield stress with depth is physically unacceptable. Here we give a procedure for the determination of all of the material parameters involved in the proposed model from in situ measurements. More speciﬁcally, we use only density measurements and measured displacement of the upper boundary of the shear zone corresponding to any time interval ∆t, with all of the other available inclinometer records being further used for validation purposes. Formulation of the problem. A granular material deposited on an inclined slope compacts slowly in time due to its own weight. The geometry of the natural slope and the related coordinate system is shown in Fig. 6.3.1. θ is the slope angle, the x-axis along the slope direction, y-axis normal to the x-axis and situated in the slope plane. The compaction characteristic can be described with a non associated viscoplastic constitutive equation of the form (see Ch. 2): W (t) ∂F 1 1− (6.3.1) D= 2η H(σ) ∂σ

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

270

Dynamic Plasticity

Fig. 6.3.1

Schematic ﬂow along a slope.

where D is the irreversible strain rate tensor, H(σ) is the yield function, F (σ) is !t the viscoplastic potential, σ is the Cauchy stress tensor, W (t) = t0 σ · Ddt is the irreversible stress work per unit volume, which is used here as an internal state variable, η is a viscosity coeﬃcient and the bracket A denotes the positive part of function A, i.e., A = A if A > 0 and A = 0 if A ≤ 0. If we assume that the gravitational stress state to which the granular material is subjected on the slope is essentially constant in time, Eq. (6.3.1) can be easily integrated to give the variation in time of the volumetric strain εv as 1 − W (t0 )/H(σ) ∂F/∂σ 1 ∂F t0 − t 1 − exp (6.3.2) εV (t) = ·σ (1/H) (∂F/∂σ) · σ H ∂σ 2η where t0 is an initial reference time, t is the current time, and σ is the mean stress. Since the density is related to the volumetric strain through ρ(t0 ) (6.3.3) ρ(t) = 1 − εV (t) we can determine at each depth the variation with time of the density. However, to obtain the density variation from Eq. (6.3.3), we need to estimate the stress distribution within the layer of bulk material. Consider a layer of material of constant depth h deposited horizontally (θ = 0 in Fig. 6.3.1). At an arbitrary depth y, the vertical stress is y ρ(t)gdy = −ρ(t0 )g(h − y) − ph (6.3.4) σyy (t) = h

where ph stands for the pressure exerted at the top surface y = h. For bodies of large lateral extent, assuming a plane strain state, Hooke’s law and isotropy, give the other stress components v σyy σxx = σzz = (6.3.5) 1−v

dynamic

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Flow of a Bigham Fluid

dynamic

271

where v is the Poisson’s ratio. The stress given by Eq. (6.3.5) correspond to t = t0 in Eq. (6.3.2) [i.e., the initial data for the viscoplastic Eq. (6.3.1)]. Next we give an example of application of Eqs. (6.3.2)–(6.3.5) for dry sand. The explicit expressions of the yield function, H, and viscoplastic potential, F , used in Eq. (6.3.2) are for dry sand. The material parameters involved in the expressions of these constitutive functions were determined from triaxial compression data reported in Hettler et al. [1984]. From Eq. (6.3.2) it follows that the density at any depth is an increasing function of time and tends asymptotically towards a limit value, say ρ(∞). Figure 6.3.2 shows the variation of the bottom density with time for h = 6 m, v = 0.36, and η = 20 Poise. Figure 6.3.3 shows the plot of the ultimate limit values of the density versus the depth y corresponding to v = 0.3. A linear law of variation of the limit density ρ(∞) with depth approximates the data well ρ h − ρ0 y + ρ0 (6.3.6) ρ= h where ρ0 = ρ(0) is the density at the bottom, y = 0 after compaction and ρh = ρ(h) is the density at the top, y = h. To capture the inﬂuence of the compaction history on the creep ﬂow of the material deposited on the slope, a non homogeneous Bingham model is proposed. if IIσ ≤ k 2 (ρ) 0 (6.3.7) D= k(ρ) 1 √ 1− σ if IIσ > k 2 (ρ) 2η(ρ) IIσ where D is the irreversible strain rate tensor, Dij = 1/2(vi,j + vj,i ), v the the σij is velocity ﬁeld, σ = σ − 1/3(trσ)1 is the stress deviator, and IIσ = (1/2)σij the second invariant of the stress deviator.

Fig. 6.3.2

Evolution in time of the bottom. Density as predicted by (6.3.3).

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

272

dynamic

Dynamic Plasticity

Fig. 6.3.3 Variation of the ultimate density (i.e., density at t → ∞) with depth as predicted by Eq. (6.3.3) (η = 20 Poise, h = 6 m).

In this model both the yield stress k(ρ) and the viscosity coeﬃcient η(ρ) are considered to be functions of the actual density; k is given in stress units and η in Poise. We make the usual kinematics assumption that the particles move in the slope direction (see Fig. 6.3.1) with a velocity depending on depth only, i.e., vx = V (y) , hence, the strain rate tensor is

vy = 0 ,

vz = 0

0 0. 0

0 1 ∂V D= 1 2 ∂y 0

1 0 0

(6.3.8)

(6.3.9)

We assume also that the depth, h, of the stratum is constant. Using Eqs. (6.3.9) and (6.3.7), we obtain (stresses are negative in compression) the following: σxx = σyy = σzz − p and σxz = σyz = 0

(6.3.10)

where −p is the mean pressure. Substituting Eq. (6.3.10) in Cauchy equilibrium equations we ﬁnd −

∂p ∂σxy + + ρg sin θ = 0 , ∂x ∂y

−

∂p ∂σxy + − ρg sin θ = 0 , ∂y ∂x ∂p = 0. ∂z

(6.3.11)

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

Flow of a Bigham Fluid

Fig. 6.3.4

dynamic

273

Variation of shearing stress with depth.

In the proposed constitutive Eq. (6.3.7), the yield stress is a function of the actual density. Since the density varies with depth, we further assume that the yield stress is a function of depth only. Thus the model exhibits transverse isotropy, i.e., the material is isotropic in any plane, y = constant (the group of symmetry of the material consists of all of the rotations about the y direction). Because the yield limit is assumed to depend solely on depth, it follows that the shear stress σxy is a function of y only. Hence, y ρ(y) dy (6.3.12) p(y) = −g cos θ h

and the shear stress is

y

σxy = −g sin θ

ρ(y) dy .

(6.3.13)

h

For the speciﬁc law of linear variation of ρ with depth, Eq. (6.3.6), and the boundary condition σxy |y=h = 0, we further obtain (ρh − ρ0 )(h + y) . (6.3.14) σxy = g sin θ (h − y) ρ0 + 2h Figure 6.3.4 shows the variation of σxy with depth corresponding to θ = 20◦ , h = 6 m, ρ0 = 1.4 g/cm3 , and ρh = 1.002 g/cm3 . The minimum value of σxy is reached at a point that is outside the interval 0 ≤ y ≤ h, while the maximum value is reached at the bottom ρ 0 − ρh hg sin θ . (6.3.15) σxy (0) = 2

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

274

dynamic

Dynamic Plasticity

This value is an increasing function of the stratum thickness h, and of the stratum slope θ. Similarly, we obtain ρ h − ρ0 2 (h − y 2 ) + ρ0 (h − y) . (6.3.16) p(y) = g cos θ 2h Its maximum value is reached at the bottom: ρ 0 + ρh gh cos θ . p(0) = 2 We note that p is a decreasing function of θ. Incipient shear ﬂow. According to the constitutive law Eq. (6.3.7), ﬂow takes place if and only if σxy (y) > k(y) i.e., when the shear stress surpasses the yield limit. The threshold condition for the ﬂow initiation is therefore σxy (y) = k(y). While most data support a linear variation of density with depth [see Eq. (6.3.6)], a linear variation of the yield stress with depth is physically unacceptable. A rigorous proof of this statement is presented in the next section. For the time being, we will postulate a power law variation of the yield stress with depth y n + kh (6.3.17) k(y) = (k0 − kh ) 1 − h where k0 = k(0) is the yield stress at the bottom, kh = k(h) the yield stress at the top, and n > 1 is a material constant. As an illustration of the capabilities of the model, in the following we describe the theoretical pattern of movements corresponding to n = 2 in the power law Eq. (6.3.17). The condition for ﬂow initiation σxy (y) = k(y) is G kh − k0 2 2 (ρ0 − ρh ) + (k y y + − k ) − Gρ 0 h 0 2h h2 h 1 + Gh(ρ0 + ρh ) − k0 = 0 2

(6.3.18)

where G = g sin θ. The case (G/2h)(ρ0 − ρh ) − (kh − k0 )/h2 = 0 corresponding to an overall depth of the moving slope given by h = 2(kh − k0 )/G(ρ0 − ρh ) is physically unacceptable and will not be considered. For h < 2(kh − k0 )/G(ρ0 − ρh ), the discriminant of Eq. (6.3.18), considered as a second order polynomial in y, is 1 ∆ = 2 [h2 G2 ρ2h + 2hG(ρ0 − ρh )kh + 4kh (kh − k0 )] . (6.3.19) h For h = const., the discriminant of ∆(θ) = 0, as a second order polynomial in h is ∆1 = 4kh h2 [kh (ρ0 − ρh )2 + 4(k0 − kh )ρ2h ] .

(6.3.20)

Since ρ0 ≥ ρh and k0 ≥ kh , it follows that ∆1 ≥ 0 and that the equation ∆(θ) = 0 has only one positive root. Furthermore, the equation ∆(θ) = 0 has a solution in (0, π/2) if and only if: h > H, where −(ρ0 − ρh )kh + kh [kh (ρ0 − ρh )2 + 4ρ2h (k0 − kh )] . (6.3.21) H= gρ2h

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

Flow of a Bigham Fluid

dynamic

275

In conclusion, if h < H, then σxy (y) < k(y) for any y ∈ [0, h], i.e., no shear ﬂow is possible. If h > H then: • Incipient shearing motion initiates at the depth hY I =

gρ0 sin θi − (2/h)(k0 − kh ) 2[((ρ0 − ρh )/2h) g sin θi − (k0 − kh )/h2 ]

where θi is the unique solution in (0, π/2) of the equation ∆(θ) = 0; σxy (y) < k(y) for any y = hY I ; the top stratum 0 < y < hY I is a rigid plug in motion, while the bottom stratum is rigid and at rest. • For slope inclination, θ > θi , ∆(θ > 0), Eq. (6.3.18) has two distinct solutions hY B and hY T . In this case, σxy (y) > k(y) for hY B < y < hY T and σxy (y) < k(y) otherwise. The pattern of movement of the slope is as depicted in Fig. 6.3.1. There is a shear zone hY B < y < hY T , its lower and upper boundaries being the solutions of Eq. (6.3.18), i.e., √ −ρ0 g sin θ + (2/h)(k0 − kh ) − ∆ , hY B = 2[((ρ0 − ρh )/2h)g sin θ − (k0 − kh )/h2 ] √ −ρ0 g sin θ + (2/h)(k0 − kh ) + ∆ . (6.3.22) hY T = 2[((ρ0 − ρh )/2h)g sin θ − (k0 − kh )/h2 ] As an example, Figs. 6.3.5(a)–6.3.5(c) show the variation of the shear stress σxy (y) and of the yield limit k(y) with depth corresponding to a slope inclination θ = θi /2, θ = θi and θ = 1.2θi , respectively; h = 20 m, k0 = 48 kPa, kh = 8 kPa, ρ0 = 1.3 g/cm3 , and ρh = 1.2 g/cm3 . For this set of values of the constitutive parameters: θi = 8.4◦ . The thickness of the top rigid stratum depends strongly on the magnitude of the yield stress kh . If kh is very small, the thickness of this stratum becomes very small (i.e., if kh → 0 then hY T → 0). The top rigid stratum hY T ≤ y ≤ h moves with the velocity v(hY T ) of the layer y = hY T (“plug ﬂow”), while the bottom rigid stratum 0 ≤ y ≤ hY B is at rest. The case when this bottom layer may slide along the bottom bedrock will be discussed in the section “Slip with friction at the bottom”. Note that from Eq. (6.3.18) it follows that there is an inclination, θ = θC , such that the lower boundary of the shearing zone coincides with the bottom layer y = 0, sin θC =

k0 ((ρh + ρ0 )/2)gh

(6.3.23)

the upper boundary y = hY T of the shearing zone being k0 ρh . hY T = 2h 1 − 2k0 ρh − kh (ρ0 + ρh ) Let us brieﬂy analyze some limit cases. If the yield stress at the bottom of the stratum is excessively high, then the incipient shear ﬂow takes place at the free surface. Indeed, if in Eq. (6.3.22) k0 → ∞ then hY i → h. Note that if the ﬂow condition σxy (y) = k(y) is satisﬁed at y = h, i.e., motion starts at the free surface,

January 12, 2007

276

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Dynamic Plasticity

(a)

(b) Fig. 6.3.5 Variation of the shear stress σxy and yield stress k (n = 2) with depth for diﬀerent slope inclination θ: (a) θ < θi , the yield condition is not satisﬁed; no shear or rigid motion is possible. (b) θ = θi , shear is possible at depth y = hY I ; the layer hY I < y < h is in a rigid body motion. (c) θ > θi , in the layer hY B < y < hY I , |σxy (y)| > k(y) so the material is shearing; for y > hY B the material is at rest.

dynamic

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Flow of a Bigham Fluid

dynamic

277

(c) Fig. 6.3.5

(Continued ).

then the yield stress at the free surface approaches zero and the material is free ﬂowing. Generally, even after ﬂow has initiated, the material will further compact if the stress to which it is subjected is below the compressibility/dilatancy boundary of the material. Compaction results in an increase of the yield limit, which causes a decrease in the displacement rate to extremely low values. Conversely, a decrease in yield stress and an increase in the unit weight of the soil may be caused, for instance, by heavy rainfalls or sudden snow melting, water-level change, volcanic eruption, or earthquake shaking. This in turn, results in a higher displacement rate. Another possible trigger of shear ﬂow may be an additional pressure added in a short time interval to the top boundary of the stratum (a thick layer of snow, for instance), which will raise the curve σxy = σxy (y) is such that it will intersect k = k(y). In our analysis, we have assumed that the depth h of the stratum is constant and θ is steadily increased. However, a similar solution can be obtained if the inclination θ of the slope is constant, and the thickness h is steadily increased. Determination of k(y). Several methods can be used to determine k. A procedure based on in situ measurements will be given in the section “Example of slow motion of a natural slope”.

January 12, 2007

278

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Dynamic Plasticity

Fig. 6.3.6 Floating boundaries between the rigid and viscoplastic domains when the slope θ ranges from θi (slope angle corresponding to incipient shear ﬂow) to θC (corresponding to viscoplastic motion up to the bottom of stratum).

In the following, we present an inverse method based on laboratory measurements of the motion of the stratum for diﬀerent chute inclinations θ. Speciﬁcally, the necessary data are: • the measured value of the depth hY i , where the shear motion initiates and the corresponding inclination θi ; • hYB and hY T for successive increasing values of θ (θ > θi ), [see Eq. (6.3.22)]. Obviously, the slope of σxy as well as the locations of the vertical lines y = hYB (θ) and y = hY T (θ) (see Fig. 6.3.6) is changing with increasing θ; and • the critical value θC (or of hY T ) corresponding to the case when the whole stratum is in motion [see Eq. (6.3.23)]. Using the measured values of hYB (θ) and hY T (θ), respectively, we then compute σxy (hYB (θ)) and σxy (hY T (θ)) to get k(hYB ) and k(hY T ), respectively. These data points are then used to approximate k(y). Once k(y) is determined, the evolution in time of the boundaries between the domains of rigid motion and of viscoplastic deformation corresponding to a given law of variation of the chute angle with time can be obtained using Eqs. (6.3.22) and (6.3.23). As an example, Fig. 6.3.6 shows the variation with θ of the upper rigid-viscoplastic boundary hY T (θ) and lower rigid-viscoplastic boundary hYB (θ) for θ ∈ (θi , θC ) and the following set of values of the constitutive parameters: k0 = 48 kPa, kh = 8 kPa, n = 2, ρ0 = 1.3 g/cm3 ,

dynamic

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Flow of a Bigham Fluid

dynamic

279

Fig. 6.3.7 Variation of the shear stress σxy and yield stress k(y) for three values of the exponent n [see Eq. (6.3.17)]; only n > 1 is physically possible.

ρh = 1.2 g/cm3 . The initial common point of these boundaries is at h = hY I and θ = θi , hY T (θ) is an increasing function (i.e., the thickness of the rigid stratum is decreasing) while hYB (θ) is a decreasing function (i.e., the thickness of the lower rigid stratum decreases). Note that the stress distribution σxy (y) given by Eq. (6.3.14) is general and does not involve any constitutive assumptions. We have postulated a power law variation (n > 1) of the yield stress k(y) with depth [see Eq. (6.3.17)]. In the following we show that a linear variation (n = 1) or n < 1 is physically unacceptable. Indeed, for the non homogeneous Bingham material Dxy is proportional to the overstress σxy − k and thus reaches a maximum value at a location that corresponds to a maximum in overstress. If a linear dependence is assumed (see Fig. 6.3.7, case n = 1) then for h = const., and θ gradually increased, σxy (y) intersects k(y) always at y = 0. Thus, shear ﬂow would always initiate at the bottom. Though this is a possible particular case, generally it is expected that incipient shear ﬂow would start at some other depth, mainly if h were very large. The same arguments hold against the choice of a power law variation with n < 1 (see Fig. 6.3.7). Only for n > 1 (see Fig. 6.3.7), incipient shear ﬂow can start anywhere between 0 and h. Generally, the yield stress may depend on other parameters such as humidity, temperature, and particle size. Here we assume that all of these parameters inﬂuence ρ, which in turn aﬀects k.

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

280

dynamic

Dynamic Plasticity

Velocity ﬁeld. According to the proposed model Eq. (6.3.7), in the shear zone (IIσ > k 2 ), 2η(y)Dxy = [σxy − k(y)](sign σxy )

(6.3.24)

and since from Eq. (6.3.14) we have sign σxy = +1, we obtain Dxy =

1 [σxy (y) − k(y)] 2η(y)

Dxy = 0 for 0 ≤ y ≤ hYB

for hYB < y < hY T , (6.3.25) and hY T ≤ y ≤ h ,

σxy (y) − k(y) being the “overstress”. Substituting Eqs. (6.3.9), (6.3.14), (6.3.15) in (6.3.17) we obtain 1 ρ h − ρ0 2 k0 − kh dV 2 n = g sin θ (h − y ) + ρ0 (h − y) − (h − y) − kh . dy η 2h hn (6.3.26) For simplicity, we assume that the viscosity η is constant. If there is no slip at the bottom, i.e., V (hYB ) = 0, then after integration we obtain the velocity ﬁeld in the viscoplastic zone hYB < y < hY T 1 2 1 1 3 ρ h − ρ0 2 g sin θ h y − y + ρ0 hy − y V (y) = η 2h 3 2 k0 − kh n+1 (h − y) − kh y + C (6.3.27) + (n + 1)hn where

1 3 1 2 ρ h − ρ0 2 g sin θ h hYB − hYB + ρ0 hhYB − hYB 2h 3 2 k0 − kh (h − hYB )n+1 − kh hYB . + (n + 1)hn

1 C=− η

For the particular case when hYB = 0, C = −(1/η)((k0 − kh )/(n + 1))h. As an example Fig. 6.3.8 shows the velocity proﬁle Eq. (6.3.27) after ∆t = 100 days for: θ = 10.81◦ , h = 20 m, k0 = 48 kPa, kh = 8 kPa, ρ0 = 1.3 g/cm3 , ρh = 1.2 g/cm3 , and η = 1.48 × 106 Poise. The bottom layer 0 ≤ y ≤ hYB of the granular material remains rigid and at rest (V = 0). The top layer hY T ≤ y ≤ hYB moves as a rigid with the velocity V (hY T ) of the layer y = hY T . Note that if velocity data are available and if no slip takes place at the bottom, η can be estimated from Eq. (6.3.27). Both the exponent n in the expression of k(y) and the viscosity coeﬃcient η inﬂuence the velocity proﬁles. Setting θ = 10.81◦ , h = 20 m, k0 = 48 kPa, kh = 8 kPa, 3

3

ρ0 = 1.3 g/cm , ρh = 1.2 g/cm , n = 2, η = 1.48 × 106 Poise,

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

Flow of a Bigham Fluid

dynamic

281

Fig. 6.3.8 Computed velocity proﬁle corresponding to θ = 10.81◦ ; viscoplastic ﬂow develops in the layer hYB < y < hY T (hYB = 6.32 m, hY T = 13.9 m).

Fig. 6.3.9

Inﬂuence of the parameter n on the velocity proﬁle.

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

282

dynamic

Dynamic Plasticity

for the lower η we obtain a larger shear deformation zone, a thinner rigid layer, and more severe displacements (see Fig. 6.3.8). Figure 6.3.9 shows the inﬂuence of n when all of the other constitutive parameters are ﬁxed (same numerical values as in the previous example). Using Eq. (6.3.27) we can also compute the total volume of granular material moving down the slope. The total volume of granular material moving down between hYB ≤ y ≤ hY T in a width interval ∆z in the z-direction and in a unit time interval (the ﬂux) is hY T QS = ∆z u(y) dy (6.3.28) hY B

to which we have to add the material that is in rigid body motion in the zone hY T ≤ y ≤ h, i.e., h QT = ∆z u(hY T ) dy = (∆z)u(hY T )(h − hT ) . (6.3.29) hY T

Thus, for a unit width interval in the z-direction (∆z = 1), and n = 2, we obtain "hT 2 2 " ρ h − ρ0 y4 y3 y 2y " g sin θ h − + ρ − h 0 " h 2 12 2 6 1 " QS = " + C y|hhTY " η 2 + k0 − kh (y − h)4 − kh y "" 12h2 2 hY 2 2 ρ h − ρ0 h4T h3T hT 2 hT g sin θ h − + ρ0 h − h 2 12 2 6 1 + ChT = η 2 + k0 − kh (hT − h)4 − kh hT 12h2 2 2 2 ρ h − ρ0 hY h4Y h3Y 2 hY g sin θ h + ρ0 h − − h 2 12 2 6 1 − ChY . − η 2 + k0 − kh (hY − h)4 − kh hY 12h2 2 (6.3.30) Slip with friction at the bottom. In the following, we further examine how frictional eﬀects at the interface inﬂuence the pattern of movement. Most authors consider Coulomb friction at the interface, τ = µσn .

(6.3.31)

According to Eq. (6.3.31), the tangential stress τ , at any point, is proportional to the normal pressure σn , and is directed opposite to the relative motion between the soil and the bedrock. The coeﬃcient of friction µ is taken as a constant for a given soil and is considered to be independent of the velocity. It is worthwhile

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Flow of a Bigham Fluid

dynamic

283

to note that Coulomb’s law describes correctly the mechanics of friction between two rigid bodies. To accurately reproduce friction between a rigid body and a deformable body, diﬀerent friction law should be considered. To describe friction between a rigid and a perfectly plastic body, the following law was proposed on a great number of tests (Levanov et al. [1976]): σ τ (6.3.32) = ks 1 − exp a τY σY where a < 0, 0 ≤ ks ≤ 1, and τY and σY are the yield stress in simple shear and uniaxial compression, respectively. Generally, ks characterize the rugosity of the hard surface and ranges from 0 to 1. The limit ks = 1 corresponds to very high rugosity when no slip is possible, and a viscoplastic deformation takes place up to the rigid surface. The limit value ks = 0 corresponds to ideal smooth contact and “perfect” lubrication, when sliding is taking place at the smallest applied shearing stress. Note that for normal pressures much lower than σY , the law Eq. (6.3.32) reduces to Coulomb’s law Eq. (6.3.31), while for high pressures (generally for σ > σY ) when the material is fully plastic Eq. (6.3.32) reduces to τ = mτY

(6.3.33)

with m constant, i.e., a constant shear stress is assumed at the interface, irrespective of the normal pressure. Since the maximum shear a material can withstand according to the von Mises yield criterion is τY , it follows that 0 ≤ m ≤ 1: (i) for no friction, m = 0; (ii) for the case of complete adherence to the wall (no slip), m = 1, the material in contact with the wall is deforming plastic. The friction law Eq. (6.3.33) is widely used in plastic forming of metals to describe friction between the die (rigid body) and deforming material (Avitzur [1968]). A generalization of the friction law Eq. (6.3.33) to the case of contact between a rigid body and a viscoplastic material was proposed by Cristescu [1975] (6.3.34) τ = m IIσ where IIσ is the second invariant of the stress deviator. In the case where the viscoplastic material is of Bingham type, the friction law Eq. (6.3.34) becomes (6.3.35) τ = m(k + 2η IID ) where k is the yield stress of the material, η is the viscosity, IID is the second invariant of the stretching tensor D and 0 ≤ m ≤ 1. In the following, we consider friction law Eq. (6.3.35) between the material in the slope and the bedrock (assumed to be a rigid body). This law reproduces the fact that the frictional shear stress is identical with the shearing yield stress. Let as assume that the maximum shear stress that the bottom surface, y = 0 can hold without relative motion is mk0 , m < 1, then σxy |y=0 = mk0 is ﬁrst reached at θ = θs 2mk0 (6.3.36) sin θs = (ρ0 + ρh )hg

January 12, 2007

284

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Dynamic Plasticity

Fig. 6.3.10 The angle at which sliding initiates and the extent of the shear zone for diﬀerent friction conditions at the interface y = 0.

[see Eq. (6.3.15)] and the thickness of the rigid plug sliding along the bottom surface, y = 0 is hYB (θs ) [see Eq. (6.3.22)]. In conclusion, if the friction law Eq. (6.3.35) is assumed at the interface and θ ≥ θs , then there will be a rigid plug at the bottom (see Fig. 6.3.10), i.e., the viscoplastic deformation zone cannot extend to the bottom. If m → 1 (very rough bottom surface) it follows that the sliding velocity Vs → 0 and the zone of viscoplastic ﬂow extends to the bottom. In the case where θ is ﬁxed and h is steadily increased, the depth at which sliding starts is hs =

2mk0 . (ρ0 + ρh )g sin θ

Similar arguments hold, if somewhere in the stratum 0 ≤ y ≤ h there exists a weaker plane y = ys along which the maximum shear stress is much smaller than in the neighborhood layers. In other words, there exists a plane y = ys of yield stress k(ys ) smaller than that of the stress above it. As an example, see the case study reported by Alonso et al. [1993] where a thin marl layer has weaker shear properties than all of the other materials in the moving stratum. Example of slow motion of a natural slope. Laboratory experiments are far from being representative of long-term in situ behaviors. Hence, we propose a procedure for the identiﬁcation of the model parameters based on in situ measurements: density measurements and inclinometer recordings.

dynamic

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

Flow of a Bigham Fluid

dynamic

285

The coeﬃcients of the proposed model are: the viscosity η, the densities ρ0 and ρh , as well as the parameters involved in the law of variation of the yield stress with depth: k0 , kh and n. From measurements of the density of the slope material at the surface and at two other depths we can estimate ρh and the slope of the density line. One inclinometer record gives the values of the upper limit, hY T , the lower limit of the shear zone hYB and h (the extent of the domain of interest). Given the slope angle θ, ρ0 , and ρh from Eq. (6.3.14), we calculate σxy (hY T ) and σxy (hYB ). Since the yield condition is satisﬁed at hY T and hYB , it follows that k(hY T ) = σxy (hY T ) and k(hYB ) = σxy (hYB ). Next, using Eq. (6.3.17) we calculate ln[(kh − k(hYB ))/(kh − kY T )] , n= ln[(h − hYB )/(h − hY T )] k(hYB ) − k(hY T ) , (1 − (k(hYB )/h)n − (1 − (k(hY T )/h)n n k(hYB ) − (k0 − kh ) 1 − . h

k0 = kh + kh = kYB

(6.3.37)

Further, the measured displacement of the upper boundary of the stress zone, u(hY T ), corresponding to any time interval ∆t, permits the determination of the viscosity coeﬃcient η. Indeed, assuming V (hYB ) = 0 (i.e., the strata below the shear zone are at rest) from Eq. (6.3.27) we obtain ρ h − ρ0 2 1 3 3 h (hY T − hYB ) − (hY T − hYB ) 2h 3 g sin θ − h ) h(h Y T YB ∆t η= +ρ 0 1 u(hY T ) 2 2 (h − − h ) YT YB 2 k0 − kh n+1 n+1 + [(h − hY T ) − (h − hYB ) ] − kh (hY T − hYB ) (n + 1)hn (6.3.38) with u(hY T ) the measured displacement of the upper boundary of the shear zone. Hence, all of the material parameters are obtained from exact formulae. In the following, we apply the proposed model to the description of the slow movement of a natural slope, the Villarbeney landslide in Switzerland (data after Samtani et al. [1996]). Creep ﬂow data over one year were recorded at two locations E1 and E2 about 250 m apart. At both locations it was observed that there is a top layer, which is moving essentially as a rigid body. Under this layer, another layer exists where shearing ﬂow takes place. At even deeper layers no motion was recorded. Taking the origin of the y axis at the bottom.

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

286

dynamic

Dynamic Plasticity Table 6.3.1 Model parameter n at location E1 . kh (kPa) 10 20

n 1.14 1.31

30

1.55

42.5

2

At location E1 hY T (= 6m) ≤ y ≤ h(= 18m)

top layer in rigid motion

hYB (= 1m) ≤ y ≤ hY T (= 6m)

slow creep shearing takes place

0 ≤ y ≤ hYB (= 1m)

rigid at rest.

(6.3.39)

At location E2 hY T (= 2m) ≤ y ≤ h(= 8m)

top layer in rigid motion

hYB (= 0.5m) ≤ y ≤ hY T (= 2m)

slow creep shearing takes place

0 ≤ y ≤ hYB (= 0.5m)

rigid at rest.

(6.3.40)

At the location of borehole E1 , the base slope angle is θ = 14◦ , while at location E2 , the base slope angle is θ = 17◦ . Samtani et al. [1996] also give an empirical linear law for the variation with depth of the unit weight of the form γ(h − y) = γh + ζ(h − y)

(6.3.41)

where γ(h − y) is the unit weight at the depth h − y below the surface, γh is the unit weight at the surface, and ζ is a material parameter. At borehole E1 , γh = 21.85 kN/m3 and ζ = 0.0024 kN/m4 , while at borehole E2 : γ = 21.6 kN/m3 and ζ = 0.024 kN/m4 . The data thus support the linear law of variation of density with depth Eq. (6.3.6) that we have obtained using the constitutive Eq. (6.3.2). Using Eqs. (6.3.39) and (6.3.41), we obtain k(hYB ) = 90.637 kPa and k(hY T ) = 63.824 kPa at E1 , and k(hYB ) = 47.989 kPa and k(hY T ) = 38.281 kPa at E2 . The exponent n and k0 in the power law variation of yield stress with depth can be estimated using Eq. (6.3.37). However, the ground yield stress kh at both locations was not available. As an example in Table 6.3.1, we give the values of this experiment corresponding to several values of the ground yield stress kh . We assume kh = 30 kPa at location E1 and using Eq. (6.3.37) we obtain n = 1.55. Next, we calculate the viscosity coeﬃcient η using Eq. (6.3.38) and the measured displacement of the upper boundary of the shear zone u(hY T ) = 17.5 mm corresponding to ∆t = 100 days. We obtain η = 1.523 × 109 Poise. All of the other available inclinometer records at location E1 are further used for validation purposes. Figures 6.3.11(a)–6.3.11(d) show a comparison between the data (symbols) and the predicted displacement proﬁles (lines) at location E1 corresponding to time intervals 148, 196, 260, and

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Flow of a Bigham Fluid

dynamic

287

Fig. 6.3.11 Villaberney landslide. Experimental displacement proﬁles (symbols) and model predictions (dashed lines) at location E1 after a period of: ∆t = 148, 196, 260 and 356 days. The displacement after ∆t = 100 days, which was used for the determination of the model parameters, is not shown.

356 days. At location E2 we assume that kh = 22 kPa, and to calculate η we use the measured displacement of the upper boundary of the shear zone, u(hY T ) = 6.3 mm, corresponding to ∆t = 100 days. The obtained values are: η = 3.852×108 Poise and n = 2. The model predictions versus the data, which was not used for identiﬁcation

January 12, 2007

288

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Dynamic Plasticity

Fig. 6.3.12 Villaberney landslide. Experimental displacement proﬁles (symbols) and model predictions (dashed lines) at location E2 after a period of: ∆t = 148, 196, 260 and 356 days. The displacement proﬁle after ∆t = 100 days, which was used for the determination of the model, is not given.

of the model parameters (readings at ∆t = 148, 196, 260 and 365 days), are shown in Figs. 6.3.12(a)–6.3.12(d). The model predictions seem reasonable; however for an accurate determination of the exponent n, we would have needed the value of the yield stress kh at the surface.

dynamic

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Flow of a Bigham Fluid

dynamic

289

Conclusion. The non homogeneous Bingham model proposed accounts for the eﬀect of gravitational consolidation on the material response and allows for a variation of density and yield stress with depth. A criterion for shear ﬂow initiation is formulated and the ensuing motion is described. Generally, at a certain depth there is a shear region; the top layer above it is in rigid motion (unless the cohesion is zero). The layer below the shear region is either rigid and at rest or in rigid body motion (plug sliding along the bedrock). Velocity proﬁles for several slip conditions at the interface with the bedrock are given. A procedure for determining the constitutive parameters using only the measured displacement of the upper boundary of the shear zone, u(hY T ), corresponding to any time interval ∆t, and density measurements was given. Finally, the model was used to predict the observed ﬁeld behavior of the natural slope from the Villarbeney landslide in Switzerland, and Fosso San Martino (inclinometers readings after Bertini et al. [1984]) (Cazacu and Cristescu [2000]). Let as note that records of a single inclinometer were used for the determination of the model, whereas all the other available records were utilized to test the predictive capabilities of the model. Laboratory tests have been undertaken by Petley and Allison [1997] to elucidate the behavior of deep-seated landslides. In deep-seated failures deformation has been reported at depths of up to 250 m. In the movement zone, owing to the weight of the overburden and the surrounding stress environment, conventional soil mechanics cannot be used to explain eﬀectively associations between the landslip activity and the deformation mechanisms operating within the mowing mass. A number of tests were undertaken, the most signiﬁcant focusing on the transition between ductile and brittle behavior. The results presented in this paper identify a transitional phase of behavior in which creep-like movement will manifest itself at the base of a deep-seated landslide as growth of microcracks. In the Mount Stuart batholith, Washington, Paterson and Miller [1998] have examined magmatic fabrics patterns around stopped blocks in tonalite located near the pluton roof and completed 1:1 scale, three-dimensional mapping of fabric patterns around stopped blocks in diorite located ≈ 1000 m below the roof. There are many places in the world where we have a sliding of several millimeters in 100 days, say. They are producing a recurrent instability phenomenon. Slow motion develops along a deep-seated sliding surface, involving a volume of rock between 22 and 35 million cubic meters. For instance, at Rosone in Italy, such a slide was studied by Forlati et al. [2001]. This rock slope is aﬀected by recurrent instability phenomena. The slow movement develops along a deep-seated sliding surface, involving a volume of rock between 22 and 35 million cubic meters. A series of non-linear, time dependent analyses has been carried out through the ﬁnite element method. A visco-plastic constitutive law, allowing for strain softening eﬀects.

January 12, 2007

10:41

290

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Dynamic Plasticity

The ﬂow of a Bingham ﬂuid taking into account inhomogeneous yield limit of the ﬂuid was considered by Hild et al. [2002]. After setting the general three dimensional problem, the blocking property is introduced. Then they focus on necessary and suﬃcient conditions such that blocking of ﬂuid occurs. The anti-plane ﬂow in two dimensional and one dimensional cases is considered. More ﬁne properties dealing with local stagnant regions as well as local regions where the ﬂuid behaves like a rigid body are obtained in dimension one. Some other ˙ n were variants of Bingham bodies including non-linear Bingham as τ = τy + K(γ) considered by Talmon and Huisman [2005] to describe the ﬂow of drilling ﬂuids.

6.4

How to Measure the Viscosity and Yield Stress

Introduction. There are many apparatuses used today to measure the viscosity of ﬂuids and/or yield stress. Their principles and theories are presented in many books, as for instance in Bird et al. [1987]. Generally all these devices need a signiﬁcant volume of liquid in order to determine its viscosity. However, for some applications like biomedical, ﬂuid supply can be extremely limited. For that reason, we have recently developed a falling cylinder viscometer that requires only a tiny amount of ﬂuid (about 20 µl) in order to measure viscosity. This viscometer is based on a falling ball viscometer of Tran-Son-Tay et al. [1988]. The advantage of falling cylinder versus the falling ball is that the generated shear rate is better deﬁned. Falling cylinder viscometers have been used for over 75 years, but remarkably the problem of a cylinder of ﬁnite length falling inside a cylindrical tube has not been solved yet in simple closed form solution, involving a magnetic ﬁeld as well. It appears that Pochettino [1914] was the ﬁrst to study experimentally the passage from “solid state” to the “ﬂuid state” using a method of falling cylinder in order to study the mechanical properties of tar. Bridgman [1926] used a falling cylinder to determine the “relative viscosities” of ﬂuids subjected to high pressures. He devised the apparatus and analyzed the various possible experimental errors, mainly related to the “inertia eﬀect”, i.e., the time needed for the cylinder to reach a steady-state falling velocity. His apparatus did not give the absolute viscosity, but only the relative viscosity. The relative viscosities for a variety of ﬂuids, for several temperatures and pressures were determined. It was found that viscosity increases with pressure. Using a falling cylinder type viscometer, viscosities of methane and propane at low temperatures and high pressures were determined by Huang et al. [1966], and viscosities of methane, ethane, propane and n-butane by Swift et al. [1960]. A theoretical analysis of the laminar ﬂuid in the annulus of a falling cylinder viscometer was made by Lohrenz et al. [1960]. The falling cylinder viscometer was analyzed by Ashare et al. [1965] for both Newtonian and non-Newtonian ﬂuids; approximate expression for axial

dynamic

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Flow of a Bigham Fluid

dynamic

291

non-Newtonian ﬂow in the annuli was developed. They assumed that, since annular slit is small, it can be regarded as a plane slit. A theoretical analysis for the falling cylinder viscometer for Bingham ﬂuid and power law model, is due to Eichstadt and Swift [1966], while the inﬂuence of the eccentricity on the terminal velocity of the cylinder was considered by Chen et al. [1968]. A falling magnetic stainless steel slug was developed by Mc Duﬃe and Barr [1969] to measure viscosities between 1 and 104 P at pressure up to 3500 Kg/cm2 and temperature between −60◦ and 100◦ C. The motion of the slug was determined with a diﬀerential transformer that moved along the tube. An automatic falling cylinder viscometer for high pressures was also developed by Irving and Barlow [1971]; the sinker was either a solid cylinder or one with a central hole, and the fall time is detected inductively by a series of coils along the viscometer tube. Viscosity in the range 0.01–3000 P was determined. Another kind of falling coaxial cylinder viscometer for lower viscosity ﬂuids as paints, was constructed by Chee et al. [1976], where a weighted rod is falling into a closed-end concentric cylinder. A laser Doppler technique was used to measure the velocity of a falling-slug in a high pressure viscometer by Dandridge and Jackson [1981]; the viscosities of two polyisobutenes have been determined as function of pressure. Viscosities in excess of 107 Pa s have been determined by this method. An improved version of the viscometer was presented by Chan and Jackson [1985]. Measurements of the relative viscosity of aqueous solutions for various temperatures and pressures up to 120 MPa are due to Tanaka et al. [1988]; they found that viscosity increases almost linearly with pressure. Tanaka et al. [1994] later used a laser beam that passed through a pair of sapphire windows to a phototransistor to determine the falling time of the cylinder. A special designed falling cylinder viscometer was used by Kiran and Sen [1992] to measure high-pressure viscosities in the 10 to 70 MPa range and temperatures from 310 to 450 K, of n-butane, n-pentane, n-hexane and n-octane (see also Kiran and Sen [1995]). Kiran and Gokmenoglu [1995] also published viscosity values for Polyethylene solutions subjected to high pressures. Chen and Swift [1972] analyzed the “entrance” and “exit” eﬀects in a falling cylinder viscometer for creeping and non-creeping ﬂow, giving a numerical correction for incompressible Newtonian ﬂuid. End eﬀects occurring in the falling cylinder viscometer were also analyzed by Wehbeh and Hussey [1993]; experimental data for closed and open tubes were also presented. A theoretical and experimental study allowing for the prediction of end eﬀects is due to Gui and Irvine [1994]; the ﬂow ﬁeld is obtained numerically (see also Gui and Irvine [1996]). A superposition technique was utilized by Park and Irvine [1995] to account for the end eﬀects of a ﬂat ends falling cylinder viscometer; the technique is applicable for Newtonian ﬂuids. Park and Irvine [1997] also gave a method to simultaneously determine the density and viscosity of the liquid by using needles of three distinct densities. The derivation of the “exact” solution for the motion of a liquid ﬂowing past a falling cylinder with a frontal spherical end was analyzed by Borisov [1998] with some assumptions concerning the front shape of the cylinder and liquid velocity. The ﬁnite element

January 12, 2007

292

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Dynamic Plasticity

study of a uniform ﬂow past a needle in a cylindrical tube for materials having diﬀerent constitutive equations is due to Phan-Thien et al. [1993]. In the chapter we present a simple theory of the ﬂow of a viscous ﬂuid in a falling cylinder viscometer according to Cristescu et al. [2002], and Cristescu [2005]. The velocity proﬁle is obtained in ﬁnite form for both open tube and closed tube. Also in ﬁnite form is obtained a formula for the determination of the viscosity coeﬃcient. These formulae contain also a term describing the inﬂuence of a magnetic ﬁeld on the motion of the falling cylinder and of the ﬂuid. How this term is used in viscosity measurements will be described in future papers. Since all the obtained formulae are in ﬁnite form, a parametric study (determination of the inﬂuence of various factors involved) of the ﬂuid ﬂow in the falling cylinder viscometer can be done quite easily. The comparison of the determination of the viscosity parameter according to the present theory with viscosity determined with a cone-plate viscometer is quite good. Microrheometer. The most common viscometers and rheometers presently in use are those based on the measurement of stress on a ﬁxed surface while a parallel or opposing surface is moved with a known applied strain rate. However, as already mentioned, these devices require fairly large sample volumes. Often it is diﬃcult, if not impossible, to collect large volumes of samples for testing. In response to this chalange, Tran-Son-Tay et al. [1988] developed an acoustically tracked falling ball

Fig. 6.4.1 Schematic of Microrheometer (a-sample tube, b-cylinder, c-piezoelectric crystal, d-ultrasound transducer, e-water jacket, f-electromagnet).

dynamic

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Flow of a Bigham Fluid

dynamic

293

rheometer (Microrheometer). The Microrheometer (Fig. 6.4.1) is a unique device that was designed to measure the viscosity and viscoelasticity of small samples of biological ﬂuids by using a spherical steel ball that is concentrically located in a small cylindrical tube with a volume of about 20 µl. The ball falls either under the force of gravity or is levitated and oscillated with a force produced by a magnetic ﬁeld. The position of the ball is tracked by ultrasonic pulse-echo method. Furthermore, the small volume permits accurate temperature control and rapid temperature changes to be eﬀected in the sample under study. Modiﬁcations have been made to the original setup so that a constant shear rate will be exhibited across the ﬂuid, that is, a falling cylinder is used in place of a ball. A 20 µl sample is loaded, by retrograde injection, into a disposable glass tube with an inner diameter of 1.6 mm and a height of 10 mm. Once loaded, the tube is centered inside a cylindrical, Plexiglas, water-jacket chamber. The ultrasonic transducer is housed at the bottom center of the Plexiglas chamber. An O-ring forms a watertight seal with the base of the sample tube and with the transducer. A plastic cap is screwed into place at the top of the chamber and provides a seal that completely protects the sample. A schematic of the Microrheometer is given in Fig. 6.4.1. The exact size of the tube and falling cylinder are given in Fig. 6.4.2. One can see that the falling cylinder is very large, as compared with the tube. That is very important for the approach. A small electromagnet coupled with a micromanipulator is used to position and drop a 1.215 mm diameter cylinder in the center of the tube, where the strongest echo occurs. The pulse-echo mode is used to locate and track the falling cylinder. A single sound pulse is transmitted into the ﬂuid medium by pulsing an ultrasound

Fig. 6.4.2 The dimensions of the falling cylinder and tube; CD-cylinder diameter 1.215 mm, CHcylinder height 4.90 mm, TID-tube inner diameter 1.61 mm, TOD-tube outer diameter 2.21 mm, IH-tube height 10.0 mm.

January 12, 2007

294

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Dynamic Plasticity

transducer that also acts as a receiver. Any returning echoes from the cylinder cause a voltage rise across the transducer that is ampliﬁed by the ultrasonic pulse/receiver unit. The time for the sound waves to travel to and back from the cylinder, and the speed of sound in the ﬂuid are measured. From that information, the distance between the transducer and the cylinder, i.e., the location of the falling cylinder is determined. Two types of measurements can be performed with our Microrheometer: (1) a speed-of-sound evaluation, and (2) a steady-state viscosity. The parameters of interest are c, the local speed of sound in the medium and η, the bulk suspension viscosity. In order to measure the speed of sound in the ﬂuid, the instrument needs to be calibrated. To accomplish this, the sample chamber is ﬁrst ﬁlled to the top with distilled water and then capped with a glass cover slip to assure a ﬁxed sample height h. Once the chamber height is determined, the water is removed and replaced by the ﬂuid sample. The local speed of sound in the medium c, is then determined. The ﬂuid viscosity is determined from the speed of sedimentation of the falling cylinder. Details of the theory, including the use of a magnetic force to pull on the

Fig. 6.4.3 Main bang in the large signal on the left, the echo of the cylinder is the smaller signal on the right (at 3).

dynamic

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Flow of a Bigham Fluid

dynamic

295

Fig. 6.4.4 Falling of the cylinder with constant velocities (on 3). The measurements starts at point 1 and end at 3, where the cylinder reaches the bottom.

Fig. 6.4.5 Three approaches of the theory: falling in an inﬁnite tube, moving up or down under a pressure gradient, and falling in a closed tube.

cylinder, are provided in the following section. The main bang followed by the pulse reﬂected from the top of the cylinder is shown in Fig. 6.4.3. The time for the sound waves to travel to and back from the cylinder, and the speed of sound in the ﬂuid is measured. That is shown also in Fig. 6.4.4 where is shown that on the portion considered, the reading is quite linear. That is shown in Fig. 6.4.5. That is why the theory is based on three successive approaches. First we study the ﬂow in an inﬁnite open tube (see the ﬁrst Fig. 6.4.5). Then is studied the ﬂow in an inﬁnite tube under a pressure gradient (second Fig. 6.4.5). Finally at the end we study the ﬂow in a ﬁnite tube, having in mind that a part of the ﬂuid is ﬂowing up while some is ﬂowing down with the cylinder (last Fig. 6.4.5). Theory. In what follows we use cylindrical coordinates (see Fig. 6.4.6) and the notation shown in this ﬁgure. We use: ρc -cylinder density, ρ-ﬂuid density, v1 -velocity of the cylinder.

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

296

dynamic

Dynamic Plasticity

Fig. 6.4.6

Schematic of the falling cylinder viscometer and notations used.

Assumptions made are: A1. The ﬂow is laminar and telescopic; the velocity components are vr = vθ = 0 , vz = v = f (r) with r = x2 + y 2 . A2. The boundary conditions at the cylinder wall:

(6.4.1)

r = R1 : v(R1 ) = −v1

(6.4.2)

t ≥ 0,

i.e. the ﬂuid adders to the cylinder wall. A3. The boundary condition at the tube wall t ≥ 0,

r = R2 : v(R2 ) = 0

i.e., the ﬂuid adheres to the tube wall.

(6.4.3)

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

Flow of a Bigham Fluid

dynamic

297

A4. The ﬂuid is a Newtonian viscous ﬂuid Tij = 2ηDij

(6.4.4)

where Tij is the Cauchy stress deviator, and η is the viscosity coeﬃcient, which may depend on z, if the ﬂuid is non-homogeneous. Taking into account (6.4.1) the only non-zero strain rate is Drz =

1 f (r) 2

(6.4.5)

and from (6.4.4) we get for the stresses Trr = Tθθ = Tzz = σ ,

Tθz = Tθr = 0 ,

Trz = η(z)f (r) .

(6.4.6)

Since v is varying with r and assuming that this variation is of the kind shown in Fig. 6.4.6, we expect for Trz : positive if R1 < r < r0 ∂v (6.4.7) Trz = η(z) negative if r0 < r < R2 ∂r 0 for r = r0 if at r = r0 the velocity reaches a maximum and the stress Trz is zero. From the equilibrium equations written in cylindrical coordinates, since the problem is with cylindrical symmetry, follows for our case ∂σ ∂σ = = 0, ∂r ∂θ

∂Trz ∂σ Trz + + + ρbz = 0 ∂r ∂z r

(6.4.8)

where bz is the body force component. Thus σ(z) depends on z alone, and from the last equation (6.4.8) and (6.4.6) we get dσ d(rf ) + + ρbz r = 0 . (6.4.9) η dr dz Integrating once with respect to r, we get r C1 dσ + ρbz + . Trz = − dz 2 r Integrating a second time with respect to r we obtain 2 dσ r ηf + + ρbz = C1 ln r + C2 . dz 4

(6.4.10)

(6.4.11)

The integration constants can be determined from the boundary conditions A2 and A3 ηv1 + (dσ/dz + ρbz )(R22 − R12 )/4 , ln(R2 /R1 ) 2 ηv1 + (dσ/dz + ρbz )(R22 − R12 )/4 R2 dσ C2 = + ρbz − ln R2 . dz 4 ln(R2 /R1 ) C1 =

(6.4.12)

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

298

dynamic

Dynamic Plasticity

Thus the velocity distribution is obtained as 2 2 1 r R2 − r2 R2 − R12 dσ dσ + ρbz + ηv1 + + ρbz ln ηv = dz 4 ln(R2 /R1 ) dz 4 R2 (6.4.13) if the viscosity coeﬃcient is known and dσ/dz is the pressure gradient along the tube. Let us write now a global equilibrium condition for the cylinder: the projections on the z-axis of all forces acting on the cylinder are zero; i.e., gravitational force + buoyancy force + shearing force on the cylinder wall = 0. Thus R1 g(ρc − ρ + m) (6.4.14) 2 with m the “local density” of the magnetic force. With (6.4.9) this relation becomes 2 R 2 R2 R22 − R12 R1 R2 dσ + ρbz ln + 1 ln − [g(ρc − ρ + m)] ηv1 = dz 2 R1 4 2 R1 Trz |R1 =

(6.4.15) which is a relation between ηv1 , (dσ/dz) + ρbz and m. We can examine now the velocity proﬁle for open tube. First let us consider an open vertical tube (or an “inﬁnite” tube) in which can move a heavy cylinder

1.0E-03

Velocity of Fluid (m/s)

8.0E-04

6.0E-04

4.0E-04

2.0E-04

0.0E+00 5.1E-04 R1

5.6E-04

6.1E-04

6.6E-04

Radius (m)

7.1E-04

7.6E-04

8.1E-04 R2

Fig. 6.4.7 Velocity of the ﬂuid moving upward under the pressure gradient (6.4.16) which keeps the cylinder stationary.

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Flow of a Bigham Fluid

dynamic

299

and a pressure gradient exists. Let us assign various values to the pressure gradient dσ/dz in order to ﬁnd out the various possible velocity proﬁles. Example 1. From (3.14) follows that if the pressure gradient satisﬁes the relation dσ −(R12 /2) ln(R2 /R1 )[g(ρc − ρ + m)] + ρbz = dz (R12 /2) ln(R2 /R1 ) − (R22 − R12 )/4 the cylinder is stationary (v1 = 0). In other words under this pressure gradient the shearing forces of the ﬂuid ﬂowing upwards will keep stationary the cylinder. Figure 6.4.7 shows an example computed for η = 0.1014 N s/m2 (101.4 P) and dσ + ρbz = 9.36 × 104 Pa m−1 . dz The velocity distribution shown was obtained with (6.4.12).

(6.4.16)

Example 2. If the pressure gradient is greater than that obtained from (3.16), the shearing force of the ﬂuid ﬂowing up is able to move upwards the cylinder. In order to give an example, Fig. 6.4.8 is showing the velocity proﬁle of the ﬂuid for (dσ/dz) + ρbz = 1.2 × 105 Pa × m−1 . If this term reaches the value 1 × 106 Pa × m−1 the velocity of the ﬂuid in contact with the cylinder is equal with that of the cylinder itself. This case can be obtained from (3.12) by putting the condition that the maximum velocity of the ﬂuid be reached for r = R1 . Example 3. This example considers the most common case when term (dσ/dz) + ρbz has a smaller value than that obtained from (3.15). Figure 6.4.9 shows an example obtained with the value (dσ/dz) + ρbz = 8.0 × 104 Pa m−1 and same η as before. In this case most of the ﬂuid is moving upwards, but a thin layer of ﬂuids neighboring the cylinder, the ﬂuid is moving downwards. In the present example |v1 | = 0.000528 m/s (down) is obtained from (6.4.14). Example 4. The last example corresponds to very small values for (dσ/dz) + ρbz . Let us consider the case when the pressure gradient is zero dσ/dz = 0. Introducing this value in (6.4.14) together with ρg = 9.807 × 103 (kg/m2 s2 ) and same value for η as above, we get v1 = −0.00363 m/s (down). The velocity proﬁle follows from (6.4.12). This time the falling cylinder induces into the ﬂuid a shearing stress which will put it to ﬂow downwards (see Fig. 6.4.10). The velocity of the ﬂuid in contact with the tube is certainly zero. Velocity proﬁle for closed tube. Let us consider now the case when the bottom of the tube is closed and the pressure gradient is generated by the falling cylinder. We can write down the condition that the volume of the ﬂuid displaced by the falling cylinder is equal to the volume of the ﬂuid ﬂowing (up and down) between the cylinder and the tube: R2 v2πr dr = v1 πR12 . (6.4.17) R1

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

300

dynamic

Dynamic Plasticity

Fluid Velocity (m/s)

1.6E-03

1.2E-03

8.0E-04

4.0E-04

0.0E+00 5.1E-04 R1

5.6E-04

6.1E-04

6.6E-04

7.1E-04

7.6E-04

Radius (m)

8.1E-04 R2

(a)

4.0E-02

Fluid Velocity (m/s)

3.0E-02

2.0E-02

1.0E-02

0.0E+00 5.1E-04 R1

5.6E-04

6.1E-04

6.6E-04

Radius (m)

7.1E-04

7.6E-04

8.1E-04 R2

(b) Fig. 6.4.8 Velocity proﬁle from the ﬂuid ﬂowing upwards under a pressure gradient greater than (6.4.16); the ﬂuid pushing the cylinder upwards: (a) the pressure gradient slightly bigger than (6.4.17); (b) pressure gradient bigger than (6.4.16) when the velocity of the cylinder is equal with the maximum velocity of the ﬂuid (and a small plateau exists).

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

dynamic

Flow of a Bigham Fluid

301

Fluid Velocity (m/s)

6.7E-04

2.7E-04

-1.3E-04

-5.3E-04 5.1E-04

5.6E-04

6.1E-04

R1

6.6E-04

7.1E-04

7.6E-04

8.1E-04 R2

Radius (m)

Fig. 6.4.9 Under a small pressure gradient, part of the ﬂuid is moving up, but part is moving down with the falling cylinder.

Fluid Velocity (m/s)

-7.0E-04

-1.7E-03

-2.7E-03

-3.7E-03 5.1E-04 R1

Fig. 6.4.10 zero).

5.6E-04

6.1E-04

6.6E-04

Radius (m)

7.1E-04

7.6E-04

8.1E-04 R2

The velocity proﬁle in the ﬂuid generated by the falling cylinder (pressure gradient is

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

302

dynamic

Dynamic Plasticity

Fig. 6.4.11

Schematic of the ﬂuid ﬂow in the case of closed tube.

Introducing here v(= f ) from (6.4.11) we get 3 dσ r 2 R2 + ρbz + C1 r ln r + C2 r dr = v1 R12 − η R1 dz 4

(6.4.18)

with the values of C1 and C2 from (3.14) and the notations R22 − R12 1 1 ln R2 ln R1 R24 − R14 2 2 + R2 − − R1 − Σ=− 16 4 ln(R2 /R1 ) 2 4 2 4 (R22 − R12 )2 R22 R22 − R12 − ln R2 4 2 8 ln(R2 /R1 ) 1 1 ln R2 ln R1 1 R22 − − R12 − V =− ln(R2 /R1 ) 2 4 2 4 +

+

R2 ln R2 R22 − R12 + 1 ln(R2 /R1 ) 2 2

(6.4.19)

we ﬁnally obtain dσ V + ρbz = η|v1 | dz Σ

(6.4.20)

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

Flow of a Bigham Fluid

dynamic

303

which established another relationship between η v1 and (dσ/dz) + ρbz , obtained from a kinematic assumption. However, the term η v1 as obtained from (6.4.20) and from (6.4.15) must be equal. From this condition follows (R12 /2) ln(R2 /R1 )[g(ρc − ρ + m)] dσ + ρbz = . dz V /Σ − (R12 /2) ln(R2 /R1 ) + (R22 − R12 )/4

(6.4.21)

This relation determines (dσ/dz) + ρbz . The magnetic force is involved as a “local density”, i.e., if pushing down it is equivalent with a heavier cylinder. After calibration, this observation will be used to speed up some tests with very viscous ﬂuids, and using the very same magnetic cylinder. Introducing this value into (6.4.20) we obtain a formula for the determination of the viscosity coeﬃcient η: dσ Σ + ρbz . (6.4.22) η= V |v1 | dz We can consider the expression α=

(R12 /2)g ln(R2 /R1 ) Σ β 2 V Σ/V − (R1 /2) ln(R2 /R1 ) + (R22 − R12 )/4

(6.4.23)

to be a viscometer constant. We have introduced β as a correction parameter, mainly because the cylindrical magnet has sometimes no perfect cylindrical shape, and also to take into account the end eﬀects. Thus the formula for the determination of the viscosity coeﬃcient (6.4.22) writes η=α

ρc − ρ + m . |v1 |

(6.4.24)

Shearing stress distribution. The shearing stress distribution in the layer of ﬂuid is obtained from (6.4.10) with (6.4.12), as r ηv1 + ((dσ/dz) + ρbz )(R22 − R12 )/4 1 dσ + ρbz + . (6.4.25) Trz = − dz 2 ln(R2 /R1 ) r The stress becomes zero there where the ﬂuid velocity is maximum; Trz = 0 or v = vmax for r = r0 . That is obtained from 1 r0 dσ + ρbz + C1 = 0 − dz 2 r0 i.e.,

r0 =

2C1 (dσ/dz) + ρbz

(6.4.26)

which determines r0 . From the numerical examples given in this paper one can see that r0 depends strongly on the pressure gradient. Example 5. In order to check the prediction of the above formulae, we have performed experiments with a variety of standardized ﬂuids available in our laboratory.

January 12, 2007

304

10:41

Fluid

Number of Falling Cylinder samples

Average Falling Cylinder Velocity (m/s)

Average Viscosity as determined from the Theory (cp)

Standard deviation of Theoretical Value

Accuracy % (theoretical value-Brookﬁeld value)/Brookﬁeld value)

Variability % (standard deviation/ Measured value)

1

1005

16

5.25E-04

1067

87

6.169154229

8.153701968

2 3

3085 9549

17 37

1.71E-04 6.05E-05

3274 9442

241 1564

6.126418152 −1.120536182

7.361026268 16.56428723

Dynamic Plasticity

Viscosity as measured on the Brookﬁeld (cp)

Summary statistics of all samples computed both experimentally and theoretically.

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Table 6.4.1

dynamic

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

Flow of a Bigham Fluid

dynamic

305

The tests were done with a custom made falling cylinder viscometer. The viscometer data are: R1 = 0.000505 m (cylinder radius) R2 = 0.000805 m (container inner radius) 3

ρc = 7228 kg/m (cylinder density) ρf = 1000 kg/m3 (ﬂuid density) . A sample of standard 1000 cP calibration ﬂuid was measured to verify its viscosity using a cone-plate viscometer (Brookﬁeld, MA). We have tested 17 samples of this calibration ﬂuid and determined a coeﬃcient of viscosity µ = 1067 ± 87 cP compared with 1005 cP as determined by the cone-plate viscometer. The experimental viscosity coeﬃcient is 6.17% higher than the cone-plate value. Though the matching is quite good, the existing diﬀerence may be due either to the disregarding in the theory of the end eﬀects, or/and to the non-perfect cylindrical shape of the falling cylinder. However, for all practical measurements of viscosities, the accuracy is quite good. The data for all sample ﬂuids is summarized in Table 6.4.1. In order to make another check of the prediction of the above formulae, we use the experimental data given by Park and Irvine [1997] for the Canon S-60 standard

0.01 0.005 0

Fluid velocity (m/s)

-0.005 -0.01

-0.015 -0.02 -0.025

R1 -0.03 2

R2 4

6

Radius (m) Fig. 6.4.12

8 -3

x 10

Velocity proﬁle obtained for v1 = 0.02903 m/s.

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

306

Dynamic Plasticity

0.02 0.01 0

Fluid velocity (m/s)

-0.01 -0.02 -0.03 -0.04 -0.05 -0.06 2

R2

R1 4

6

Radius (m) Fig. 6.4.13

8 -3

x 10

Velocity proﬁle for v1 = 0.05251 m/s.

ﬂuid. The tests done for the falling needle viscometer are: R1 = 1.99 × 10−3 m (needle diameter); R2 = 9.525 × 10−3 m (container diameter); L = 10.2 cm (needle length); ρ = 0.8589 × 103 kg/m3 (ﬂuid density). For the needle density ρc = 1.1019 × 103 kg/m3 the terminal falling velocity recorded was v1 = 0.02903 m/s. We have determined a coeﬃcient of viscosity η = 115 cP as compared with 101.4 cP given in the Cannon speciﬁcations. It is 13% higher. The ﬂow of the ﬂuid is shown in Fig. 6.4.12. For the needle density ρc = 1.2998 kg/m3 the terminal falling velocity was found v1 = 0.05251 m/s. The determined viscosity coeﬃcients is η = 116 cP to be compared with 101.4 cP. The velocity proﬁle is shown in Fig. 6.4.13. Thus the determined viscosity coeﬃcients are about 14% higher than the Cannon speciﬁcation value. Conclusion. A simple theory is presented in which the solution of the ﬂow of a viscous ﬂuid in a falling cylinder viscometer is expressed in a closed form. The formula giving the viscosity of the ﬂuid is also obtained in ﬁnite form. Since all the formulae are obtained in ﬁnite forms, one can easily study the inﬂuence of all parameters involved [as densities (maybe variable), geometry of cylinder-tube, pressure gradient,

dynamic

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

dynamic

Flow of a Bigham Fluid

307

magnetic force, etc.] on the cylinder-ﬂuid motion. The comparison of the viscosity coeﬃcients, as determined by our experiments with the falling cylinder microrheometer and using the present theory, and as determined with a classical coneplate viscometers is quite good. It is important to note that the formulae for velocity, stress, viscosity, etc. contain a term that describes the inﬂuence of a magnetic ﬁeld on the motion of the cylinder and thus on the ﬂow of the ﬂuid. However, the inﬂuence and use of a magnetic ﬁeld in viscometer studies will be treated in a future paper. An extension of the analysis to nonhomogeneous ﬂuids, viscoplastic materials, and to the case when the ﬂuid slides along the tube and/or cylinder is to be considered in the future. Further developments. An extension of the theory for Non-Newtonian ﬂuids was done by Tigoiu and Cipu [2005]. They have in mind that some biological ﬂuids are of this kind. The velocity, in physical cylindrical components is: vr = 0 ,

vθ = 0 ,

vz = V1 f (r) ,

r ∈ [R1 , R2 ] .

(6.4.27)

The corresponding boundary conditions on both the falling cylinder and the pipe are vz (R1 ) = −V1 ,

vz (R2 ) = 0 .

(6.4.28)

It is well known that the velocity ﬁeld (6.4.27) is associated to a viscometric motion and therefore Cauchy’s stress tensor is given by ˜ 1 , A2 ) . T(x, t) = −pI + T(A

(6.4.29)

Here p is the pressure ﬁeld, I is the identity tensor, A1 , A2 are the ﬁrst two Rivlin– ˜ should be given in explicit forms in Ericksen tensors. The eﬀective stress tensor T next sections. After some calculi we obtain from (6.4.27) (A1 )rz = V1 f , (A2 )rr = 2V12 f 2 , (A1 A2 + A2 A1 )rz = 2V13 f 3 ,

(6.4.30)

A3 = 0 and all other components of A1 , A2 are null. We pass to non-dimensional variables and functions by z = H z¯ ,

r = R1 r¯ ,

f = f¯ ,

p = p0 p¯ ,

σz = ρ1 g¯ σz

and T˜ = T0 T¯ (6.4.31)

where we denote T0 ≡ η0 (V1 /R1 ). Here η0 is a characteristic shear viscosity. We remark that the velocity ﬁeld (6.4.28) satisﬁes the continuity equation and then the ﬂow problem can be written, after using (6.4.31), as

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

308

dynamic

Dynamic Plasticity

h (r) =

1 1 d ˜ (rTrr (r)) , Re r dr

1 d (rTrz (r)) = Re σz , r dr R2 f (1) = −1 , f = 0, R1

(6.4.32)

where Re ≡ (ρ1 gR12 /η0 V1 ) is a modiﬁed Reynolds number, described by means of characteristic quantities of our problem (ρ1 being the ﬂuid mass density) and where we have suppressed the overlines. For this end we remark that (∂p/∂θ) = 0. At this level of generality, the arguments are given by (6.4.29), (6.4.30) and Wang’s representation theorem for isotropic functions. Consequently p = C0 z + h(r). In (6.4.32) we have denoted σz = (p0 /ρ1 gH)(∂p/∂z) + 1 the “modiﬁed pressure gradient”. We remark that equation (6.4.32)1 leads to the determination of the pressure ﬁeld, once the eﬀective stress tensor components are known. The above mentioned components will be determined after solving the boundary value problem (6.4.32)2 –(6.4.32)3 . For this, a ﬁrst integral is simply obtained from (6.4.32) and leads to the determination of the shear stress component which, in dimensional variables, is 1 V1 C1 1 ∂p C1 η0 = + ρ1 g r + η0 V1 . (6.4.33) T˜rz (r) = σz r + 2 r 2 ∂z r The dimensional constant C1 will be independently determined for each investigated model. We remark here that the necessary condition of having a constant velocity (for the falling cylinder) is given by the global equilibrium of forces acting on the cylinder (gravitational force, buoyancy force, shearing force and magnetic force). Some elementary calculi lead to the following formula (ρc being the mass density of the falling cylinder) 1 T˜rz (R1 ) = (ρc − ρ1 + fm ) gR1 . 2

(6.4.34)

Employing (6.4.33) and (6.4.34) we obtain η0 V1 =

1 (ρc − ρ1 + fm ) g − σz } R12 . 2C1

(6.4.35)

This formula is a compatibility condition between the geometry, material and ﬂow parameter (connecting V1 , fm , η0 and σz ) and which leads to the determination of the necessary magnetic ﬁeld density fm . We remind, that the shear viscosity η on viscometric ﬂows is given by η(k) =

τ (k) , k

(6.4.36)

where k stands for the shear rate and τ (k) for the shear stress. Formula (6.4.36) is the support for the T0 expression in (6.4.31).

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

Flow of a Bigham Fluid

dynamic

309

The Third Grade Fluid Case. For the third grade ﬂuid we employ the eﬀective ˜ and constitutive restrictions as obtained in Tigoiu [1987] stress tensor T ˜ 1 , A2 , A3 ) = µA1 + α1 (A2 − A21 ) + β1 A3 T(A + β2 (A1 A2 + A2 A1 ) + β3 (trA21 )A1 , µ ≥ 0,

β1 < 0 ,

(6.4.37)

β1 + 2(β2 + β3 ) ≥ 0 ,

where µ, α1 and βi , i = 1, 2, 3 are constant constitutive moduli. Use of (6.4.37) in ﬂow equation (6.4.32)2 leads, after a ﬁrst integration, to the following non-dimensional problem f + βf 3 =

1 1 Reσz r + C1 , 2 r

f (1) = −1 ,

f (R2 /R1 ) = 0 ,

(6.4.38)

where the left term in equation (6.4.37)1 is the non-dimensional shear component of Cauchy’s stress tensor. We see that this problem has a unique solution 3 3 1 4 4 2+ 2+ + C + C C − C , (6.4.39) f (r) = 27β 27β (2β)1/3 where C ≡ C(r) ≡ ar +

C1 , r

a≡

1 Reσz 2

and β ≡

2(β2 + β3 ) 2 V1 . µR12

We remark here that, the normal force acting on the outer cylinder is given, in non-dimensional form, by Trr (R2 /R1 , z) = −Re p(R2 /R1 , z) + αf 2 (R2 /R1 ) .

(6.4.40)

The explicit formula for Trr is obtained if we introduce p(r, z) = C0 z + h(r) where h(r) is obtained from h (r) =

α 1 ∂ (rf 2 (r)) Re r ∂r

(6.4.41)

and (6.4.39). In formulae (6.4.40), (6.4.41) α stands for the non-dimensional constitutive moduli α1 , α ≡ (α1 V1 /µR1 ). The solution f (r) is ﬁnally obtained from (6.4.39) + (6.4.38)2 , after applying a shooting method (for determination of the constant C1 ), by numerical integration. The results are plotted. The Second Order Fluid Case. We consider now a falling cylinder viscometer ﬁlled with a second order ﬂuid with the shear viscosity depending on the shear rate. The corresponding constitutive law for the eﬀective stress is given by ˜ 1 , A2 ) = η(tr A21 )A1 + α1 (A2 − A21 ) , T(A

(6.4.42)

January 12, 2007

310

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Dynamic Plasticity

where we generally suppose that η is a positive, bounded and decreasing C 2 function (deﬁned on a compact set of positive numbers). For the numerical application we consider ' 2 &( 1 2 2 log(f ) + 1.7897 . η(trA1 ) = η0 exp −A(ln 10) 2 Here η0 = 102.8 Pa s is supposed to be the zero shear rate viscosity. Equation (6.4.32)1 is now given in dimensional form by 1 ∂ (rf 2 (r)) . h (r) = V12 α1 (6.4.43) r ∂r After obtaining f from the corresponding boundary value problem for (6.4.32)2 – (6.4.32)3 , the pressure ﬁeld will be determined from (6.4.43). We consider, as in the previous section, the non-dimensional ﬂow problem ∂ σ ¯z [rη(tr A21 )f (r)] = r , f (1) = −1 ; f (R2 /R1 ) = 0 . (6.4.44) ∂r Wi In (6.4.44) we denote with W i the corresponding Weissenberg number given by W i = (V1 η0 /ρ1 gR12 ). Similar to the third grade ﬂuid case, a ﬁrst integral is obtained from (6.4.44)1 as: σz C1 Trz (r) ≡ η(tr A21 )f (r) = r+ . (6.4.45) Wi r With the above mentioned properties for η, we can easily see that the equation η(X 2 )X − g(r) = 0

(6.4.46) ¯ has a unique solution X = X(r). Consequently we can uniquely express from (6.4.45) the derivative of f as a continuously diﬀerentiable function of r. Finally it results that the considered problem (6.4.44) has a unique twice continuously diﬀerentiable solution. To obtain the ﬁnal solution we will numerically solve the problem (6.4.44) for the mentioned solution of a polyisobutylene in decline. Closed Domain Case. In this section we consider the case of a third grade ﬂuid model. However, in the case of a linear viscous ﬂuid the velocity ﬁeld is analytically obtained. In almost all other cases we can not expect any analytical solutions. In order to put into evidence end eﬀects (i.e., in a closed pipe), we simulate such eﬀects by a kind of “volumetric ﬂow rate” equilibrium. The result leads to the determination of a modiﬁed pressure gradient σz necessary for the above mentioned equilibrium. With this σz the characteristics of the velocity ﬁeld (as solution of the new boundary value problem) are diﬀerent from those of the velocity ﬁeld which has been obtained in previous section. In order to do this, we write the balance of the volume of ﬂuid (per unit time) pushed downwards by the falling cylinder with the volume of ﬂuid (per unit time) ﬂowing upwards and downwards between the pipe and the cylinder. Therefore we have R2 rf (r) dr . πR12 V1 = 2πV1 R1

dynamic

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Flow of a Bigham Fluid

dynamic

311

Fig. 6.4.14 Velocity ﬁelds for a closed domain for diﬀerent values of computed apparent modiﬁed pressure gradient σz .

For a third grade ﬂuid, the obtained values for σz (corresponding to V1 = 0.00007 m s−1 , 0.000528 m s−1 and 0.00363 m s−1 , respectively) are |σz | = 90.91, 685.5 and 4713.5, respectively. The corresponding graphics for the velocity ﬁelds are shown in Fig. 6.4.14. In all graphics it is put into evidence a domain in neighborhood of the pipe in which an inverse ﬂow occurs. The three domains have practically similar dimensions, that is the point of cut oﬀ with the axe vz = 0 is almost the same in the three cases. However, the dimension of the domain is diﬀerent from the case of a linear viscous ﬂuid.

Bibliography Aleksandrov S. E., Goldshtein R. V. and Lyamina E. A., 2003, Developing the concept of the strain rate intensity factor in plasticity theory, Doklady Physics 48, 3, 131–133. Alonso E. E., Gens A. and Lloret A., 1953, The landslide of Cortes de Pallas, Spain, G´eotechnique 43, 507–521. Ashare E., Bird R. B. and Lescarboura J. A., 1965, Falling cylinder viscometer for non Newtonian ﬂuids, AIChE Jour. 11, 5, 910–916. Avitzur B., 1968, Metal Forming: Processes and Analysis, Mc Graw Hill, New York. Bertini T., Cugusi F., D’Elia B. and Rossi-Doria M., 1984, Climatic conditions and slow movements of colluvial covers in Central Italy, Proc. IV Int. Symp. on Landslaides, Toronto, Vol. I, 367–376.

January 12, 2007

312

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Dynamic Plasticity

Bird B. R., Armstrong R. C. and Hassager O., 1987, Dynamics of Polymeric Liquids, Wiley, New York. Borisov V. B., 1998, The equation for a falling-cylinder viscometer, High Temperature 36, 2, 293–298. Bridgman P. W., 1926, The eﬀect of pressure on the viscosity of forty-three pure liquids, Proc. Amer. Acad. Arts Sci. 61, 56, 57–99. Buckingham E., 1921, On plastic ﬂow through capillary tubes, Proc Amer. Soc. Testing Materials 117, 1154–1161. Cazacu O. and Cristescu N., 2000, Constitutive model and analysis of creep ﬂow of natural slopes, Rev. italiana di geotecnica 3, Luglio-Settembre, 44–54. Chan R. K. Y. and Jackson D. A., 1985, An automated falling-cylinder high pressure Laser-Doppler viscometer, J. Phys. E: Sci. Instrum. 18, 510–515. Chee K. K., Sato K. and Rudin A., 1976, Falling coaxial cylinder viscometer for polymer solutions, Journal of Applied Polymer Science 20, 1467–1474. Chen M. C. S., Lescarboura J. A. and Swift G. W., 1968, The eﬀect of eccentricity on the terminal velocity of the cylinder in a falling cylinder viscometer, AIChE Journal 14, No. 1, 123–127. Chen M. C. S. and Swift G. W., 1972, Analysis of entrance and exit eﬀects in a falling cylinder viscometer, AIChE Journal 18, No. 1, 146–149. Cristescu N., 1975, Plastic ﬂow through conical converging dies using a viscoplastic constitutive equation, Int. J. Mech. Sci. 17, 425–433. Cristescu N., 1976, Drawing through conical dies. An analysis compared with experiments, Int. J. Mech. Sci. 18, 1, 45–49. Cristescu N., 1991, Nonassociated elastic/viscoplastic constitutive equations for sand, Int. J. Plasticity 7, 41–64. Cristescu N. D., 2005, Theory of Falling Cylinder Viscometers (in print). Cristescu N. D., Conrad B. P. and Tran-Son-Tay R., 2002, A closed form solution for falling cylinder viscometers, Int. J. Engn. Sci. 40, 605–620. Cristescu N. D., Cazacu O. and Cristescu C., 2002, A model for slow motion of natural slopes, Canadian Geotech. Journal 39, 4, 924–937. Dandridge A. and Jackson D. A., 1981, Measurements of viscosity under pressure: a new method, J. Phys. D: Appl. Phys. 14, 829–831. Desai C. S., Samtani N. C. and Vulliet L., 1995, Constitutive modeling and analysis of creeping slopes, J. of Geotehnical Eng., ASCE 121, 43–56. Mc Duﬃe G. E. and Barr T., 1969, Pressure viscometer for viscosities between 1 and 104 P, The Review of Scientiﬁc Instruments 40, No. 5, 653–655. Eichstadt F. J. and Swift G. W., 1966, Theoretical analysis of the falling cylinder viscometer for power law and Bingham plastic ﬂuids AIChE Journal 6, 1179–1183. Forlati F., Gioda G. and Scavia C., 2001, Finite element analysis of a deep-seated slope deformation, Rock Mech. and Rock Engineering 34, 2, 135–159. Fu M. and Loo Z. J., 1995, J. Materials Proc. Tech. 55, 442–447. Gui F. and Irvine T. F. Jr., 1994, Theoretical and experimental study of the falling cylinder viscometer, Int. J. Heat Mass Transfer. 37, 1, 41–50. Gui F. and Irvine T. F. Jr., 1996, An absolute falling tube viscometer, Experimental Thermal and Fluid Science 12, 325–337. Hettler A., Gudehus G. and Vardoulakis I., 1984, Stress–strain behaviour of sand in triaxial tests, in Results of the International Workshop on Constitutive Relations for Soils, Grenoble, France, September 1982, Gudehus G., Darve F. and Vardulakis I. (eds.), A.A. Balkema, Rotterdam, The Nederlands, 55–66.

dynamic

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Flow of a Bigham Fluid

dynamic

313

Hild P., Ionescu I. R., Lachand-Robert T. and Ro¸sca I., 2002, The blocking of an inhomogeneous Bingham ﬂuid. Applications to landslides, Mat. Modelling and Num. Anal. 36, 6, 1013–1026. Huang E. T. S., Swift G. W. and Kurata F., 1966, Viscosities of methane and propane at low temperatures and high pressures, AIChE. 12, 5, 932–936. Irving J. B. and Barlow A. J., 1971, An automatic high pressure viscometer, Journal of Physics E: Scientiﬁc Instruments 4, 232–236. Kiran E. and Sen Y. L., 1992, High-pressure viscosity and density of n-alkanes, International Journal of Thermophysics 13, No. 3, 411–442. Kiran E. and Sen Y. L., 1995, Viscosity of polymer solutions in near-critical and supercritical ﬂuids. Ch. 9 in Viscosity of Polymer Solutions in Fluids, Kiran E. and Brennecke J. F. (eds.), ACS Symposium Series 514, Am. Ch. Soc. 1993, 104–120. Kiran E. and Gokmenoglu Z., 1995, High-pressure viscosity and density of polyethylene solutions in n-pentane, Journal of Applied Polymer Science 58, 2307–2324. Levanov A. N., Kolmogorov V. L., Burkin S. P., Katak B. R., Ashpur Iu. V. and Spasskii Iu. M., 1976, Contact Friction in the Metal Working Processes, Metallurgia Publisher, Moscow (in Russian). Lohrenz J., Swift G. W. and Kurata F., 1960, An experimentally veriﬁed theoretical study of the falling cylinder viscometer, AIChE Journ. 6, 4, 547–550. Park N. A. and Irvine T. F. Jr., 1995, Falling cylinder viscometer end correction factor, Rev. Sci. Instrum. 66, 3982–3984. Park N. A. and Irvine T. F. Jr., 1997, Liquid density measurements using the falling needle viscometer, Int. Comm. Heat Mass Transfer. 42, 3, 303–312. Paterson S. R. and Miller R. B., 1998, Stoped blocks in plutons: paleo-plumb bobs, viscometers, or chronometers? J. of Structural Geology 20, 9/10, 1261–1272. Petley D. N. and Allison R. J., 1997, The mechanics of deep-seated landslides, Earth Surface Processes and Landforms 22, 747–758. Phan-Thien N., Jin H. and Zheng R., 1993, On the ﬂow past a needle in a cylindrical tube, Journal of Non-Newtonian Fluid Mechanics 47, 137–155. Pochettino A., 1914, Su le propriet` a dei corpi plastici, Il Nuovo Cimento 8, 6th Ser., 77–108. ¨ Reiner M. and Riwlin R., 1927, Uber die Str¨ omung einer elastichen Fl¨ ussigkeit im Couette Apparat, Kolloid. Z. 43, 1–5. ¨ Reiner M., 1926, Uber die Str¨ omung einer elastichen Fl¨ ussigkeit durch eine Kapillare, Kolloid Z. 39, 80–87. Reiner M., 1960, Deformation, Strain and Flow, Wiley-Interscience, New York. Samtani N. C., Desai C. S. and Vulliet L., 1996, An interface model to describe viscoplastic behavior, Int. Jour. of Numerical and Analyt. Meth. in Geomech. 20, 4, 231–252. Swift G. W., Lohrenz J. and Kurata F., 1966, Liquid viscosities above the normal boiling point for methane, ethane, propane, and n-butane, AIChE Jour. 6, 3, 415–419. Talmon A. M. and Huisman M., 2005, Fall velocity of particles in shear ﬂow of drilling ﬂuids, Tunnelling and Underground Space Technology 20, 2, 193–201. Tanaka Y., Ohta K., Kybota H. and Makita T., 1988, Viscosity of aqueous solutious of 1, 2-ethanediol and 1,2-propanediol under high pressures, International Journal of Thermophysics 9, 4, 511–523. Tanaka Y., Xiao Y. F., Matsuo S. and Makita T., 1994, Density, viscosity and dielectric constant of HCFC-225ca and HCFC-225cb at temperatures from 293 to 323 K and pressures up to 80 Mpa, Fluid Phase Equilibria 97, 155–165. Tigoiu V., 1987, Wave propagation and thermodynamics for third grade ﬂuids, St. Cerc. Mat. 29, 4, 279–347.

January 12, 2007

314

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Dynamic Plasticity

Tigoiu V. and Cipu C., 2005, Non-Newtonian ﬂuid ﬂows in a falling cylinder viscometer, trends in applications of mathematics to mechanics, Wang Y. and Hutter K. (eds.), Proc. Of the XIVth Int. Simp. on Trends in Appl. of Math. to Mech., Seeheim, Germany, 22–28 Aug., 2004, Shaker Verlag. Tran-Son-Tay R., Beaty B. B., Acker D. N. and Horchmuth R. M., 1988, Rev. Sci. Instrum. 59, 1399–1404. Wehbeh E. G., Ui T. J. and Hussey R. G., 1993, End eﬀects for the falling cylinder viscometer, Phys. Fluids A 5, 1, 25–33.

dynamic

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

Chapter 7

Axi-Symmetrical Problems

7.1

Introduction

In previous sections we have considered cases when the boundary and initial conditions conform to the assumption that only a single component of stress and a single component of velocity occur. Sometimes, in these cases, a constitutive equation is not used at all and the procedure is somehow similar to that used in some static problems, i.e., the equation of motion and continuity condition are only combined with a yield condition but not a constitutive equation. Using this procedure a suﬃcient number of equations is obtained for the number of unknown quantities required. Sometimes else, a constitutive equation is used, but this is in fact a onedimensional stress–strain relation, and therefore as a rule, the methods used do not greatly diﬀer from those used for the study of the propagation of longitudinal waves in thin bars. In all the cases examined the propagation of a single type of wave has been considered if the equation of motion is of the hyperbolic type. Otherwise, propagation is assumed to occur by diﬀusion according to an equation of parabolic type. First let as present shortly the static, plane stress, problem (Sokolovski [1969]) when at the oriﬁce one is given a pressure. For a Mises type of yield condition 1 1 2 2 (σ − σx σy + σy2 ) + σxy = k 2 = σY2 3 x 3 the problem is hyperbolic close to the oriﬁce, but elliptic at farther distances Fig. 7.1.1. √ The characteristics are logarithmic spiral lines. The ﬁgure corresponds to p = 3k when b ≈ 5.13a. On this circle the problem is parabolic. For greater distances the problem is elliptic. For the Tresca condition, written in cylindrical coordinates σθ + σr = 2k the characteristics are logarithmic spirals up to b = a exp(p/2k), where p is the applied pressure at the oriﬁce. The Fig. 7.1.2 is obtained for p = 2k when the logarithmic spirals are until the circle r = b is reached. Further on the problem we have a single family of straight lines, the problem being parabolic. 315

dynamic

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

316

Dynamic Plasticity

Fig. 7.1.1

The characteristics for the plane stress problem satisfying a Mises condition.

Fig. 7.1.2

The characteristics for the Tresca condition.

dynamic

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Axi-Symmetrical Problems

dynamic

317

The simple problem of enlargement of circular holes in thin inﬁnite plate taking into account variations in geometry, material properties, and loading conditions, was considered by several authors. Upadhyay and Stokes [1977] have used for that a Ramberg–Osgood constitutive equation: n ' ˙ ( II II T 2n + 1 T Tij T˙ij = 2Ge˙ ij − 2 2 k IIT combined with a Mises yield condition. As remarked by Bernstein and Shokooh [1980], when subjected to creep test, aluminum exhibits characteristics which are analogous to those of thermorheologically simple material in the sense that, on a plot of logarithm of creep function versus logarithm of time, the curves corresponding to diﬀerent stresses have the same shape so that they all could be shifted to form a master curve. Based on this observation and in analogy with the idea of time-temperature superposition, a theory for viscoelastic materials is developed in which the natural time appearing explicitly in the argument of relaxation or creep function is replaced by a suitable scalar-valued function of stress tensor. A comparison between the Perzyna viscoplastic model and the Consistency viscoplastic model is due to Heeres et al. [2002]. If, in the problem considered, there occur two or three components of velocity and therefore several components of stress and strain, and the problem is dynamic, one is obliged to consider a complete constitutive equation. Several types of constitutive equations are used in theory of plasticity. This set of constitutive equations can be divided into several group, each group of constitutive equations is characterized by certain dynamic properties. In problems in which several components of velocity, stress and strain are involved, several kind of plastic waves are present. Thus, depending on the theory of plasticity used, the plastic waves are coupled (Cristescu [1956], [1967], Nowachi [1974]). The coupling of plastic waves was ﬁrst discussed many years ago. Some authors have used for this purpose constitutive equations written in ﬁnite form. First were discussed axi-symmetrical problems. That will be discussed also below. In order to analyze such problems, without overcomplicating the writing, we analyze a case in which the whole problem depends only on a single spatial coordinate, although many components of stress and strain are involved. 7.2

Enlargement of a Circular Oriﬁce

The simplest possible case is the one in which two velocity components are involved. It is assumed that along a cylindrical hole of radius r = R the radius is enlarged and rotated. Thus the radius is enlarged (velocity u) and rotated (velocity v) (see Fig. 7.2.1). It is question of sudden motion, so that the inertia forces are involved. From all the stresses involved we assume that σr , σθ , and σrθ are diﬀerent of zero, but σz = σrz = σθz = 0. There are two velocity components distinct of zero; the radial one u, and the circumferential one v.

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

318

dynamic

Dynamic Plasticity

σθ

σ rθ

0

σr

r v

r

u

Fig. 7.2.1

Enlargement of a circular hole in a plate.

We apply the Hencky–Nadai constitutive equation. For our case we have: S S σr = εr and σθ = εθ . E E The strain components are: ∂u u 1 ∂v v , εθ = , εrθ = − . (7.2.1) εr = ∂r r 2 ∂r r If we assume incompressibility we have: εr + εθ + εz = 0 , from where we obtain εz if the other two components are known. The Hencky–Nadai constitutive equation is for our case: ∂u u ∂v v S S 2 + , σrθ = − , σr = E ∂r r 2E ∂r r where E 2 = IIε = ε2r + ε2θ + εr εθ + ε2rθ ,

(7.2.2)

(7.2.3)

(7.2.4)

and the work-hardening law is written: S = F (E) .

(7.2.5)

The equation of motion, with Xr and Xθ the two body forces per unit volume are: σr − σθ ∂ 2 u ∂σr = + Xr , ρ 2 − ∂t ∂r r ρ

2σrθ ∂ 2 v ∂σrθ = + Xθ . − 2 ∂t ∂r r

(7.2.6)

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

dynamic

Axi-Symmetrical Problems

319

Introducing here (7.2.3) we get: ρ

∂ 2u ∂2v ∂2u − L − P = Φ, ∂t2 ∂r2 ∂r2

(7.2.7)

∂ 2u ∂2v ∂2v ρ 2 −P 2 −M 2 = Ψ, ∂t ∂r ∂r where L= M = P =

ES − S 2S + (2εr + εθ )2 , E 2E 3 ES − S 2 S + εrθ , 2E 2E 3

(7.2.8)

ES − S (2εr + εθ )εrθ , 2E 3

and Φ=

ES − S S εr − εθ + (2εr + εθ )[(εr − εθ )(2εθ + εr ) − 2ε2rθ ] + Xr , E r 2E 3 r

2S ES − S εrθ + εrθ [(εr − εθ )(2εθ + εr ) − 2ε2rθ ] + Xθ . Er 2E 3 r There are two waves propagating with the velocities: & c21 M + L ± (M − L)2 + 4P 2 . = 2ρ c22 Ψ=

(7.2.9)

Both are real (the expressions at the right hand side are positive). Also, c21 > c22 .

(7.2.10)

The diﬀerential relations satisﬁed on the characteristic lines are: {Φ(M − ρc2 ) − ΨP } dt − ρ(M − ρc2 )(cdur − dut ) − ρP (cdvr − dvt ) = 0 (7.2.11) where c is either c1 or c2 , and we denote ur = (∂u/∂r), etc. Let us write now the jump conditions. First the kinematics jump conditions are 2 2 ∂ u ∂ u dr = 0 , dt + ∂t2 ∂r∂t 2 2 ∂ u ∂ u dt + dr = 0 . ∂r∂t ∂r2 From here we obtain easy the kinematics jump conditions, for u and v are similar: 2 2 ∂ u ∂ u 2 (dt) − (dr)2 = 0 , 2 ∂t ∂r2 2 2 ∂ v ∂ v 2 (dt) (dr)2 = 0 . − (7.2.12) 2 ∂t ∂r2

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

320

dynamic

Dynamic Plasticity

The dynamic jump conditions are [from (7.2.7)]: 2 2 2 ∂ u ∂ v ∂ u −L −P = 0, ρ ∂t2 ∂r2 ∂r2 2 2 2 ∂ u ∂ v ∂ v − P − M = 0. ρ 2 2 ∂t ∂r ∂r2 From (7.2.12) and (7.2.13) we get easily 2 2 2 ∂ v ∂ u ∂ u 2 ρc − L −P = 0, 2 2 ∂r ∂r ∂r2 2 2 2 ∂ v ∂ v ∂ u 2 ρc − P −M = 0, 2 2 ∂r ∂r ∂r2 or we can write also:

2 ∂ v ∂2u −P = 0, (ρc − L) 2 ∂r ∂r2 2 2 ∂ u ∂ v − P = 0. (ρc2 − M ) 2 ∂r ∂r2

(7.2.13)

(7.2.14)

2

(7.2.15)

These relations are valid for both waves; we have to precise only the velocity. It is easy to show by direct computation that P ρc22 − L = − . ρc21 − L P

(7.2.16)

From (7.2.16) and (7.2.15) we get [∂ 2 u/∂r2 ]1 [∂ 2 v/∂r2 ]2 P ρc22 − L = − , = = − [∂ 2 v/∂r2 ]1 ρc21 − L [∂ 2 u/∂r2 ]2 P or,

∂2u ∂r2

1

∂ 2u ∂r2

∂2v + ∂r2 2

1

∂2v ∂r2

(7.2.17)

= 0.

(7.2.18)

2

Thus at each point the jumps are orthogonal. Both waves are coupled, i.e., they are both dilatational and shearing [see (7.2.11), (7.2.15), (7.2.17)]. Both involve the stresses σr and σrθ and also both components of the velocity u and v. From (7.2.15), if the ratio between jumps is eliminated, it follows P M − ρc2 . = 2 L − ρc P

(7.2.19)

If M > L from (7.2.19) we have (P/(ρc2 − L)) > 1, or from (7.2.17) we obtain [∂ 2 u/∂r2 ]1 > [∂ 2 v/∂r2 ]1 that is the wave “one” is mainly a dilatational one. If M < L from (7.2.19) follows (P/(ρc2 − L)) < 1, and from (7.2.17) we obtain [∂ 2 u/∂r2 ]1 < [∂ 2 v/∂r2 ]1 that is the wave “one” is primarily a shearing wave. If M ∼ = L, then both waves are equally dilatant and shearing.

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

dynamic

Axi-Symmetrical Problems

321

The coupling coeﬃcient is P , that is if P = 0 an uncoupling takes place. That can happen if: • εrθ = 0 or v = 0. The wave “one” is pure dilatational and the only propagable, with the velocity: 1 3S 2 S ∗ c1 = ε + ρ 2E 3 θ 2E 2 which becomes smaller i.e., c∗1 < c1 . • u = 0, i.e., εr = εθ = 0; the only wave which exists is the wave “two” which becomes pure shearing. For the velocity of propagation we have: c∗2 =

S 2ρε2rθ

and we have c∗2 > c1 . Therefore we have c2 < c∗2 < c∗1 < c1 . • The third case is the elastic body, i.e., ES − S = 0. The coupling factor is P . If it is present one has coupling. And we have to integrate two equations separately, as if they are not inﬂuencing each other. If it is question what is coupling the waves it is the work hardening condition (7.2.5).

7.3

Thin Wall Tube

Let us consider now the problem of a thin wall tube, loaded at one of its end by tension and torque. Thus we have two loadings, and we expect a combined load. The boundary conditions are: at x = 0 a combined loading at x = l0 the end is ﬁxed . We are using cylindrical coordinates x, r, and θ, and the displacements are u, v and w = 0. Thus the velocity components are ut , vt , and 0. The stress components

v u

l0 Fig. 7.3.1

Thin wall tube subjected to tension and torque.

x

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

322

dynamic

Dynamic Plasticity

are σr , σrθ , and σrx are assumed to be small, at least compared with σxx = σ and σθx = τ , which are dominant. We assume also axial-symmetry thus (∂/∂θ) = 0. The equations of motion are: ∂σ ∂ut + Fx = ρ , ∂x ∂t

(7.3.1) ∂vt ∂τ + Fθ = ρ , ∂x ∂t where Fx and Fθ are the corresponding body forces, and ρ is the constant density. The strains are: ∂w w ∂u εrr = = 0, εθθ = = 0, εxx = = ε, ∂r r ∂x v 1 ∂v 1 ∂u ∂w 1 ∂v = γ , εrx = + = 0 , εrθ = − = 0. εθx = 2 ∂x 2 ∂r ∂x 2 ∂r r (7.3.2) We use also the noticing 1 σ2 σ : σ = + τ2 . (7.3.3) 2 3 We introduce now the constitutive equations. We introduce one in very general form and we particularize it later on. Thus, assuming small strains, IIσ =

ε˙ = ε˙ E + ε˙ P .

(7.3.4)

For the elastic we assume the Hooke’s law:

2Gε˙ E = σ˙ , σ˙ m = 3K ε˙m .

(7.3.5)

The plastic part of the strain rate, satisfy a general constitutive equation of the form: ε˙ P = Aσ˙ + B where A is a fourth order tensor and B a second order tensor. For our case we have ε˙P ˙ xx + ϕ12 σ˙ θx + ψ1 , xx = ϕ11 σ ˙ xx + ϕ22 σ˙ θx + ψ2 . ε˙P θx = ϕ21 σ

Introducing here the Hooke’s law, these equations becomes: ∂ut 1 2 = ϕ11 + σ˙ + ϕ12 τ˙ + ψ1 , ∂x 3 E ∂vt 4 1 = ϕ21 σ˙ + 2ϕ22 + τ˙ + 2ψ2 , ∂x 3 G

(7.3.6)

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

Axi-Symmetrical Problems

dynamic

323

where σ 9KG , and σm = . 3K + G 3 In order to simplify the problem, we introduce the new notation: 1 1 1 2ϕ11 + + , α12 = ϕ12 , β1 = ψ1 , α11 = 3 G 3K E=

4 1 ϕ21 , α22 = 2ϕ22 + , 3 G with whom the constitutive equation becomes: α21 =

β2 = 2ψ2 ,

∂ut = α11 σ˙ + α12 τ˙ + β1 , ∂x ∂vt = α21 σ˙ + α22 τ˙ + β2 . (7.3.7) ∂x This is the general form of the constitutive equation. Until now we have not said what is α11 , . . . . . . etc. In order to make a discussion we consider now several particular cases. P1. Elastic. In the elastic case, we have: ϕ11 = ϕ12 = ϕ21 = ϕ22 = ψ1 = ψ2 = 0 . The constitutive equation becomes: ∂vt ∂ut = σ˙ , G = τ˙ . ∂x ∂x The two equations are completely separated and we have two kinds of waves which propagate independently. E

P2. Rate semi linear (the constitutive equation is of Malvern type). For such equations we have: ϕ11 = ϕ12 = ϕ21 = ϕ22 = 0 . The constitutive equation can be written: k σ˙ 1 1− √ σ, ε˙ = + E 3η IIσ 1 k τ˙ + 1− √ τ, γ˙ = 2G 2η IIσ

(7.3.8)

where k is the yield stress, assumed constant or not, and η is a viscosity coeﬃcient, assumed also possibly variable. P3. Piece-wise work-hardening (separated for the two components). In this case we have ϕ12 = ϕ21 = 0 .

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

324

dynamic

Dynamic Plasticity

The constitutive equations are:

1 2 σ˙ + ψ1 , ϕ11 + 3 E ∂vt 1 = 2ϕ22 + τ˙ + ψ2 . ∂x G

∂ut = ∂x

(7.3.9)

P4. The Prandtl–Reuss constitutive equation. In this case we have: ψ1 = ψ2 = 0 . The constitutive equation is in general: σ˙ ij 2G σij σij , H σmn σmn . σij σij = H σkl dεP kl 2Gε˙ij = σ˙ ij +

and

This constitutive equation particularized for the problem is: 2 1 4 1 1 2 σ σ˙ + στ τ˙ , ε˙ = + E 27 H IIσ 3 H IIσ 1 2 1 1 2 + γ˙ = τ˙ . στ σ ˙ + τ 9 H IIσ 2G H IIσ

(7.3.10)

P5. Rate quasi-linear. In this case, assuming that the strains are small, we have to start with:

P VP ε˙ij = ε˙E , ij + ε˙ij + ε˙ij σ˙ ij 1 k F (IIσ ) + 1− √ σij + σ σ˙ σij , ε˙ij = 2G 2η 2IIσ kl kl IIσ

and for the work-hardening:

P ε˙ij = F (IIσ )σkl σ˙ kl . σij

For the problem considered this law is reduced to 4 F (IIσ ) 2 k 2 F (IIσ ) 1 1 + 1− √ σ, σ σ˙ + στ τ˙ + ε˙ = E 27 IIσ 3 IIσ 3η IIσ 2 F (IIσ ) F (IIσ ) 2 k 1 1 γ˙ = + 1− √ τ. στ σ˙ + τ τ˙ + 9 IIσ 2G IIσ 2η IIσ

(7.3.11)

From here for F = 0 we obtain the rate semi linear constitutive equation, while if η → ∞ we obtain the classic plasticity theory. The velocity of propagation for P5 and P4 are variable and equal to: & c2T L α11 + α22 ± (α11 − α22 )2 + 4α12 α21 (7.3.12) = 2ρ(α11 α22 − α12 α21 ) c2LT

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

dynamic

Axi-Symmetrical Problems

325

and cT L > cLT . For the particular case P3 we have: c2L3 =

1 , ρα11

and c2T 3 =

1 , ρα22

and these velocities are also variable. For the particular cases P1 and P2 the velocities are constant and equal to: c2L1 = c2L2 =

E , ρ

c2T 1 = c2T 2 =

G . ρ

Let us consider two particular cases. If everywhere we have vt = 0, then considering again the initial equations (with ϕ12 = 0) we have a single kind of longitudinal wave which propagates with the velocity c2L0 =

3E 1 , ρ 2Eϕ11 + 3

which for the special cases P1 and P2 reduce to the elastic bar velocity. In a similar case if ut = 0 the only existing wave is the one propagating with the velocity c2T 0 =

1 G ρ 2Gϕ22 + 1

which are shearing waves and the formula is reduced to that from elastic waves in the case ϕ22 = 0. Let us consider now the diﬀerential relations along the characteristics. We have for the general case: ∓ρc(1 − ρα22 c2 ) dut ∓ ρ2 α12 c3 dvt + (1 − ρα22 c2 ) dσ + ρα12 c2 dτ + {ρβ1 c2 (1 − ρα22 c2 ) + β2 α12 ρ2 c4 ∓ (1 − ρα22 c2 ) Fx ∓ ρc3 α12 Fθ } dt = 0 . (7.3.13) Here we have to replace c by one of the four expressions (7.3.12). For the particular case P3 the diﬀerential relations are: ∓ρcL3 dut + dσ + (ρβ1 c2L3 ∓ cL3 Fx ) dt = 0 , ∓ρcT 3 dvt + dτ + (ρβ2 c2T 3 ∓ cT 3 Fθ ) dt = 0 .

(7.3.14)

For the particular case P2 they are: ( ' E Fx dt = 0 , ∓ ρEdut + dσ + β1 E ∓ ρ ∓ ρGdvt + dτ +

' β2 G ∓

G Fθ ρ

( dt = 0 .

(7.3.15)

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

326

dynamic

Dynamic Plasticity

For the particular case P1 they are: ∓ ρEdut + dσ ∓

∓

E Fx dt = 0 , ρ G Fθ dt = 0 . ρ

ρGdvt + dτ ∓

(7.3.16)

Let us write now the coupling jump conditions. We have from the constitutive equations (the brackets stand for the “jumps” of the function considered): ∂σ ∂τ ∂ut = α11 + α12 , ∂x ∂t ∂t

∂vt ∂σ ∂τ = α21 + α22 . ∂x ∂t ∂t

From the equation of motion we get: ∂σ ∂ut = , ρ ∂t ∂x Finally, we have also the relation ∂ψ ∂ψ = −c , ∂t ∂x From here we obtain:

ρ

∂vt ∂τ = . ∂t ∂x

for ψ = ut , vt , σ, τ .

∂ut 2 2 ∂vt (1 − ρα11 c ) = ρα12 c , ∂x ∂x ∂vt 2 2 ∂ut (1 − ρα22 c ) = ρα21 c . ∂x ∂x

From all those relations we conclude that α12 and α21 are the coeﬃcients that couple the wave. They are introduced by the yield condition, which are relating all stresses in a single condition. Thus we have:

P5

&

instantaneous response

non-instantaneous response

α12 = 0 ← coupling

← coupling

α21 = 0 ← P3 α =0← 12 ← P2 α 21 = 0 ← P1 P4

coupling

← no coupling

partially coupling or uncoupling ← coupling uncoupled

← coupling

uncoupled

← no coupling

A combined tension–torsion impact testing apparatus and an experimental study in the incremental wave propagation is due to Tanimura [1978]. The apparatus can realize a tension–torsion loading. To obtain a practical form of the general equation, the methods to examine the existence of the instantaneous plastic property and to

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Axi-Symmetrical Problems

dynamic

327

obtain directly the coeﬃcients of the general equation, through the experiments in which the incremental torsional impact or the incremental combined impact is applied to the tubular specimens, have been presented. By a special mechanism for clamping and quick releasing of the input bar, a combined impulse could be generated easily with a short rise time. Through an experiment in which the torsional incremental impact was applied to the tubular specimens of commercial pure aluminum and copper, it could be observed that the incremental wave velocity, just after passing through the partial unloading, was clearly smaller than the elastic wave velocity. A general study is given by Ting [1970] of plane and cylindrical wave propagation of combined stress in an elastic-plastic medium. The relations between the stresses on both sides of an elastic-plastic boundary are derived. Also presented are the restrictions on the speed of an elastic-plastic boundary. The combined longitudinal and torsional plastic waves in thin-walled tube of rate-independent isotropic workhardening material are used by Ting [1973] to illustrate the problems involved when the speeds are equal. Plastic wave speeds in materials whose elastic response is linear and isotropic while the plastic ﬂow is incompressible and isotropically workhardening are obtained also by Ting [1977]. One of the three plastic wave speeds is identical to the elastic shear wave speed regardless of the form of the yield condition. The other two plastic wave speeds are determined for materials obeying the von Mises yield condition. See also Mandel [1974]. The propagation of waves in thin tubes, subjected to longitudinal and torsional loading, was also considered by Myers and Eisenberg [1974], [1975]. They ﬁnd that the fast and slow wave speeds are 1/2 1/2 1 1 {b + (b2 − 4aA4 )1/2 } {b − (b2 + 4aA4 )1/2 } , cs = cf = 2aρ 2aρ for a constitutive equation sij 3 s, ∆)s¯˙ ] ε˙P ij = [φ(¯ 2 s¯ % s¯ 3 2 P s¯ = sij sij , ∆ = . ε˙P ij ε˙ ij dt + 2 3 E All the other coeﬃcients are variable. Integration along characteristics is also done, for solutions with or without radial inertia. The thin-walled tube was considered also by Yokoyama [2001]. He has considered various models to describe the propagation only of simple torsional waves in tubes. These were elasto-plastic, elasto-viscoplastic and elasto-viscoplastic-plastic with linear work-hardening. The constitutive equation is of the form 1 k 1 + G H τ˙ + G τ − g(γp ) τ˙ > 0 , h γ˙ = τ ˙ k + τ − g(γ ) τ˙ < 0 . p G G

January 12, 2007

328

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Dynamic Plasticity

with Hh = dh(γp )/dγp and the function h(γp ) denotes the limiting maximum dynamic shear stress-plastic shear strain curve. When τ˙ → ∞ from the ﬁrst equation we have G (γ < γY ) 1 dτ = = dγ 1/G + 1/Hh Ht (γ ≥ γY ) which is the instantaneous response curve. The integration is numerical using ﬁnite element formulation. Then one compares the velocity of propagation of the shearing strain with the tests of Yew and Richardson [1969]. One is not ﬁnding a good coincidence, since none of the considered theories, considered by the author, could predict that plastic shear strains along the axis of the thin-walled tube decrease with increasing distance from the impacted end. However one is ﬁnding that the rate dependent models give an overall better agreement with the experimental data than the rate-independent models. The smaller plastic strains are propagated with higher velocity in the torsional wave-propagation experiments than predicted by the rate-independent plastic wave theory, whereas the situation is reversed for larger plastic strains. Assuming a one-dimensional rate independent theory of combined longitudinal and torsional plastic wave propagation in thin-walled tube, restrictions are obtained on the possible speeds of elastic-plastic boundaries by Clifton [1968]. A laser-induced deformation modes in thin metal targets is considered by O’Keefe et al. [1973]. An analogy with dilatational and transverse plastic waves in a thin membrane is considered. Some experimental data are due to Hsu and Clifton [1974a] for longitudinal plastic waves propagating in thin-walled tubes of alpha-titanium. Strain-time proﬁles recorded in these experiments show evidence of (i) stress levels considerably above quasistatic values at the same strain, (ii) decay of the amplitude of the elastic precursor, and (iii) variation with distance of propagation of the speed at which a given level of strain propagates. These features of the strain-time proﬁles are interpreted as indicating that a strain-rate dependent theory is necessary to describe the observed wave phenomena. Numerical solutions based on such a theory agree reasonably well with experimental results. In another paper Hsu and Clifton [1974b] present experiments in which combined longitudinal and torsional plastic waves are generated in thin-walled tubes of alpha-titanium by subjecting pre-torque tubes to longitudinal impact. Longitudinal and torsional strain-time proﬁles are recorded at several stations along the specimen. These strain-time proﬁles exhibit features which cannot be explained within the framework of a strain-rate independent theory. The latter theory requires the wave generated under the loading employed to consist of, successively, a fast simple wave, an intermediate constant state region, a slow simple wave, and a ﬁnal constant-state region. The experiments, done by the authors, show no evidence of an intermediate constant-state region; furthermore, a ﬁnal constant-state region is not observed even though the latest times of observation are greater than the time at which, according to a strain-rate independent

dynamic

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

Axi-Symmetrical Problems

dynamic

329

theory, a constant strain-rate region is expected. Straightforward generalization of the rate-dependent theory to allow for combined stress state leads to a theory which predicts the observed strain-time proﬁles with good accuracy. The theory applied by the authors is τ˙ ∂ τ¯ ∂ τ¯ σ˙ + Φ(¯ τ , γ¯ p ) , γ˙ = + Φ(¯ τ , γ¯ p ) , ε˙ = E ∂σ G ∂τ which are giving such results. In another paper Abou-Sayed and Clifton [1976] consider the oblique impact of fused-silica target plates by A1 6061-T6 projectile plates. The equations of motion are ∂σ ∂u ∂v ∂τ = ρ0 , = ρ0 . ∂X ∂t ∂X ∂t The present analysis of the propagating waves in the fused-silica plates indicates that the main features of the normal velocity proﬁles at the free surface will be the same as for the case of uniaxial strain. The predicted velocity-time proﬁle and the rise time for the normal velocity agree closely with those measured experimentally. The predicted eﬀect of the combined loading on the normal component of the particle velocity is a shift in the ﬁnal plateau value due to the interaction between the longitudinal wave reﬂected from the free surface and the on-coming shear wave. The eﬀect of this interaction propagates back towards the free surface at the longitudinal wave speed so that the disturbance reaches the rear surface, before the arrival of the shear wave front. The shear wave front propagating in the shear-strain-free compressed region of the specimen remains non-dispersive. The initial jump in the transverse acceleration maintains its strength as it propagates inside the body. A numerical solution is presented by Abou-Sayed and Clifton [1977a] for the case of symmetric impact of two skewed plates, modeled to represent 6061-T6 Aluminum. One is considering a Perzina [1966] type of constitutive equation ε˙ij =

1+v v ∂f σ˙ ij − δij σ˙ kk + Φ(¯ τ , γ¯ p ) . E E ∂σij

The main features of the solution are, except near the impact face, the same as in previous solutions based on a rate-independent theory. Free-surface velocity-time proﬁles are obtained for the target rear surface. Results are reported by Abou-Sayed and Clifton [1977b] for experiments employing two types of oblique-plate-impact conﬁgurations. One, a symmetric conﬁguration, uses 6061-T6 Aluminum plates for both targets and projectiles. The second, an asymmetric conﬁguration, uses a 6061-T6 Aluminum projectile and a fused silica target. The experimental results are compared to analytical solutions based on an elastic-viscoplastic model for the aluminum alloy and a hyperelastic model for fused silica. The normal velocity-time proﬁle for the symmetric conﬁguration shows close agreement with the predicted one. The plastic deformation of circular membranes of strain-rate dependent, work-hardening metal is analyzed based on the strain increment theory by

January 12, 2007

330

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Dynamic Plasticity

Tobe et al. [1979]. Numerical solutions for aluminum membranes are obtained under various types of loading as well as impulsive pressure, pulses caused by underwater wire explosions. When the duration of the loading pulse is less than one-third of the time required to ﬁnish the deformation of the membrane, the deﬂection of a deformed membrane depends almost only on the impulse of the loading pulse and the instantaneous proﬁle of the membrane is found to be trapezoidal during deformation. The relation between impulse of loading and deﬂection is calculated and illustrated. The neglect of strain-rate dependency of material leads to a notable underestimation of the forming limit. In a paper written by Kim and Clifton [1980] one is using the plate impact experiment to study the material behavior at high strain rates. The results show that the transverse velocity proﬁle is clearly more sensitive to the constitutive relations than is the longitudinal velocity proﬁle. In addition, the transverse velocity proﬁle gives the relatively long time history of the ﬂow characteristics of solids, whereas the longitudinal one does not because the plastic strain rate decreases as the stress state becomes more nearly that of hydrostatic pressure. Improved agreement between theoretical predictions and results of pressure shear impact experiments appears to require improved constitutive models for plastic ﬂow. Comparisons presented here suggest that models are required which characterize plastic ﬂow characteristics accurately along loading trajectories with sharp changes in direction. The computed transverse velocity-time proﬁles have regions of steeper slope than observed in the experiments. This discrepancy appears to be mainly due to the inadequacy of the assumption of isotropic hardening and the yield function. Comparison of the various strain-time proﬁles reveals qualitative agreement in the main features, but with several characteristic diﬀerences (G¨ uldenpfennig and Clifton [1980]). First, the solution based on self-consistent slip models does not show a constant state region between the fast and slow simple waves. Such intermediate constant states regions are predicted by theories based on smooth yield surfaces, but are not observed in experiments. Second, the decrease in shear strain in early part of the wave proﬁle is greater for the self-consistent slip models than for the experiments or for the predictions of an isotropic work-hardening, smooth yield surface model. Third, for small strains, the slip-models with independent and latent hardening predict the experimental results appreciably better than either of the other models. Fourth, all models predict the late-arriving, large amplitude strains would arrive earlier than observed in the experiments. In a paper written by Chhabilidas and Swegle [1980] an experimental technique is described which uses anisotropic crystals to generate dynamic pressure-shear loading in materials. The technique has been successfully used to detect a 0.2 GPa shear wave in 6061-T6 aluminum at 0.7 GPa longitudinal stress. A viscoplastic constitutive equation of Bingham type was used by Tayal and Natarajan [1981] together with ﬁnite element method to analyze the extrusion of rate sensitive aluminum through a conical die, extrusion of superplastic alloy

dynamic

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Axi-Symmetrical Problems

dynamic

331

through a tube of uniform diameter under complete sticking conditions and extrusion of a Pb-Sn eutectic alloy through a conical die. The results are compared with experimentally measured values. A good agreement is found. Gilat and Clifton [1985] compared experimental results with predictions based on elastic/viscoplastic models of the form τ , γ¯ p ) ε˙vp ij = Φ(¯

∂f . ∂σij

The eﬀective shear stress τ¯ was taken to have the value of the plastic potential f . Two ﬂow potentials were used: 1/2 1 σ σ , f (σij ) = 2 ij ij 1/2 1 (σ − αij )(σij − αij ) f (σij , αij ) = , 2 ij where αij denotes the coordinates of the center of a yield surface that translates in ˙ γ p )nij where nij = ∂f /∂σij = (σij − αij )/2¯ τ is the direction according to α˙ ij = µ(¯ determined by unloading at various stages of, for example, a simple shear experiment in order to determine the extent of the elastic region. The plastic strain rate function Φ(¯ τ , γ¯ p ) characterizes the material’s response in simple shear. Its value during such an experiment is equal to the current value of the plastic shear strain rate. The yield surfaces are 1 (σ σ ) = k 2 (¯ γ p) for isotropic hardening , 2 ij ij 1 (σ − αij )(σij − αij ) = k02 for kinematic hardening , 2 ij where k(¯ γ p ) is the quasi-static ﬂow stress in pure shear at a plastic shear strain γ¯ p , and k0 is the initial yield stress in shear. For these models the transverse velocity predicted at the free surface is less for kinematic hardening than for isotropic hardening; such a diﬀerence was observed in all symmetric impact experiments. Better determination of Φ(¯ τ , γ¯ p ) especially for the small plastic strains that occur in symmetric impact experiments, would be helpful. The ﬂow stress increases strongly with increasing plastic strain rate at strain rates above 104 s−1 . Hydrostatic pressure up to 2 GPa appears to have no signiﬁcant eﬀect on plastic ﬂow in 6061-T6 aluminum and at most a minor eﬀect on plastic ﬂow in alpha titanium. In plate impact experiments, the elastic precursor is attenuated as it propagates through the shocked specimen due to plastic straining at the shock front. However, the plastic strain rates (Meir and Clifton [1986]) required to explain the observed precursor decay are much higher than the strain rates that are predicted for known initial dislocation densities in the unshocked specimen, regarded as homogeneous. When dislocation generation at the surfaces is included in the computations, the calculated precursor amplitudes are comparable with measurements only for thin

January 12, 2007

10:41

332

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Dynamic Plasticity

(3 mm) specimens. When subgrain boundaries are included as additional sources for dislocation generation, the computed velocity-time proﬁles at 3 and 6.6 mm are in good agreement with measured proﬁles. An analysis is presented by Klopp and Clifton [1990] concerning the eﬀect of the inclination of the waves due to the tilt, on the calculation of stress, strain, and strain rate in the specimen. The errors seem to be small. Frutschy and Clifton [1997] present some modiﬁed pressure-shear plate impact experiment to test materials at high temperatures (up to 700◦ C). The high strain rate experiment is up to 106 s−1 . In another paper Frutschy and Clifton [1998] present the dynamic response of copper at strain rates of 105 –106 s−1 and temperatures up to 700◦ C. They show that the ﬂow stress increases with increasing strain rate, and decreases with increasing temperature. They compare the experiment with some popular models, but they show that the models do not predict the softening that is observed at large strains.

7.4 7.4.1

Wire Drawing Introduction

The processes of metal extrusion or drawing have been considered within the framework of classical time-independent plasticity theory (see Avitzur [1968]). The theory considered here is to describe the inﬂuence of the speed of the process (of the order of 100 m/s) on all the other involved parameters (Cristescu [1975], [1976]). We consider mainly wires which are very thin, less than 0.5 mm in diameter. Let us assume that the main mechanical properties of the material can be described with a viscoplastic constitutive equation. Since the elastic part of the strain will be neglected the simplest possible model is a Bingham-type constitutive equation of the form σm 1 1− √ √ σij (7.4.1) Dij = 2η 3 IIσ where σm is the mean yield stress which depends on reduction and is an approximation of the isotropic work-hardening law σ ¯ = f (¯ ε) of the material, and is the positive part. Thus the model is viscoplastic rigid. A second assumption is that the circular conical die remains rigid during plastic ﬂow and that in the domain where plastic ﬂow takes place (domain II) the process is axi-symmetric. Assuming volume incompressibility the following velocity ﬁeld components in spherical co-ordinate r, θ, ϕ can be obtained cos θ 2 , vθ = vϕ = 0 , (7.4.2) v = vr = −vf rf r2 in the domain II deﬁned by r0 ≤ r ≤ rf , 0 ≤ θ ≤ α, 0 ≤ ϕ ≤ 2π. According to (7.4.2) the material particles are moving radially towards the apex 0. Since in the domain I (for r > r0 ) the whole rod is moving as a rigid body with the absolute

dynamic

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Axi-Symmetrical Problems

Fig. 7.4.1

dynamic

333

Geometry of wire drawing.

velocity v0 and since in the domain III the rod is moving again as a rigid body with the absolute velocity vf , the spherical surfaces r = r0 and r = rf are discontinuity surfaces for the velocity ﬁeld. Along the surface Γ2 (r = r0 ) the tangential discontinuity of the velocity ﬁeld is obtained from (7.4.2) as ∆v = −v0 sin θ along r = r0 ,

0≤θ≤α

(7.4.3)

while along the surface Γ1 (r = rf ) the tangential discontinuity of the velocity is ∆v = −vf sin θ along r = rf ,

0 ≤ θ ≤ α.

(7.4.4)

Another evident formulae is R . (7.4.5) sin α From (7.4.2) the following components of the rate of strain result, in spherical coordinates, cos θ cos θ ∂v v v = 2vf rf2 3 , Dθθ = = −vf rf2 3 , Dϕϕ = , Drr = ∂r r r r r (7.4.6) sin θ 1 1 ∂v Drθ = = vf rf2 3 , Drϕ = Dθϕ = 0 2r ∂θ 2 r and obviously v0 R02 = vf Rf2 ,

r=

Drr + Dθθ + Dϕϕ = 0 .

(7.4.7)

Therefore, according to the kinematical velocity ﬁeld chosen, plastic deformation takes place in region II only, while regions I and III remain rigid. Dissipation is

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

334

dynamic

Dynamic Plasticity

calculated in region II, and dissipation due to the velocity discontinuity along Γ1 and Γ2 , while along Γ3 the dissipation is produced by the friction existing there. Γ5 is stress free. The surface Γ6 (x = r0 ) at the entrance and Γ4 (x = r0 cos α) at the exit of the die are used for the computation of the balance of forces. The semiangle of the die is denoted by α, the drawing stress by σf and a possible back-stress by σb . 7.4.2

Basic Equations

For the problem under consideration, taking into account the spherical symmetry and (7.4.6), the constitutive equation can be written as σm 2 1 1− √ √ (σrr − σθθ ) , Drr = 2η 3 IIσ 3 σm 1 1 1− √ √ (σθθ − σrr ) , Dθθ = 2η 3 3 IIσ σm 1 1− √ √ σrθ . (7.4.8) Drθ = 2η 3 IIσ The second invariant of the stress deviator is 1 2 IIσ = (σrr − σθθ )2 + σrθ . (7.4.9) 3 Using (7.4.6) and (7.4.8) the expression for this invariant can be written as vf rf2 σm IIσ = √ + 3 η 11 cos2 θ + 1 . (7.4.10) r 3 Another group of equations are the equilibrium equations. Since we have σrϕ = σθϕ = 0, σθθ = σϕϕ and since the problem is axially symmetric with respect to ϕ, the set of equilibrium equations reduces to two 1 ∂σrθ 2(σrr − σθθ ) + σrθ cot gθ ∂σrr + + = 0, ∂r r ∂θ r ∂σrθ 1 ∂σθθ 3σrθ + + = 0. ∂r r ∂θ r From (7.4.6), (7.4.8)3 and (7.4.10) we get σrθ = √

σm sin θ sin θ √ + ηvf rf2 3 r 11 cos2 θ + 1 3

(7.4.11)

(7.4.12)

which satisﬁes the requirement that σrθ = 0 for θ = 0. Introducing (7.4.12) in (7.4.11)2 a diﬀerential equation is obtained, which after integration yields # $ √ 3σm 1 2 ln cos θ + σθθ = √ (7.4.13) + cos θ + C(r) 11 11 where C is a undetermined function depending on r alone.

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

dynamic

Axi-Symmetrical Problems

335

Any one from the two equations (7.4.8) taken together with (7.4.6), (7.4.10) and (7.4.13) now yields $ # √ 3σm 1 + C(r) ln cos θ + cos2 θ + σrr = √ 11 11 √ + 2 3σm √

cos θ cos θ + 6vf rf2 η 3 . (7.4.14) 2 r 11 cos θ + 1 To determine the function C for θ = 0, we obtain 4 1 σm 168 C(r) = − vf rf2 η 3 − √ ln r + C1 (7.4.15) 3 r 3 123/2 where C1 is an integration constant, which is determined from the condition r = r0 ,

θ = 0 we have σrr = σxb .

Thus it is found for C1 , $ # √ 2 3σm 14 vf rf η σm 1 − ln 1 + 1 + + √ 4.04145 ln r0 − σm , C1 = σxb − √ 11 3 r03 11 3 and for σθθ we get $ # √ vf rf2 η 4 3σm 1 14 2 σθθ = √ − ln cos θ + cos θ + + 3 11 3 r3 r0 11 $ # √ 3σm r0 1 σm − σm ln 1 + 1 + + √ 4.04145 ln + σxb − √ r 11 3 11

(7.4.16)

and a similar procedure can be used to determine σrr . This is an approximate value since we have not taken into account the friction. We have to compute now the stress power per unit volume 2σm IID + 4ηIID , (7.4.17) σij Dij = √ 3 where 1 1 2 2 2 2 2 2 IID = Dij Dij = (Drr + Dθθ + Dϕϕ ) + Drθ + Dθϕ + Dϕr . (7.4.18) 2 2 Using (7.4.6) in (7.4.17) and (7.4.18) we get v 2 r4 η 2σm vf rf2 2 θ + 1 + f f (11 cos2 θ + 1) . 11 cos σij Dij = √ r6 3 2r3 After integrating over the volume of zone II, and using (7.4.5): ˙ = 2πσm vf Rf2 ln R0 f (α) + 2 πvf2 Rf η W Rf 3 sin α # $ 3 Rf 11 × 1− 1 − cos α + (1 − cos3 α) , R0 3

(7.4.19)

January 12, 2007

10:41

336

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

dynamic

Dynamic Plasticity

where

# $ √ 11 1 1 1 1 + ln cos α + cos2 α + (cos α) cos2 α + −f (α) = √ 11 11 11 2 3 sin2 α # $& 12 12 1 − ln 1 + . (7.4.20) − 11 11 11

The ﬁrst term is the time independent while the second term in (7.4.19) corresponds to the time dependent term. 7.4.3

Friction Laws

We ﬁrst consider a Coulomb friction law τ = µσθθ .

(7.4.21)

Here µ is the constant friction coeﬃcient and σθθ is the stress normal to the die surface. Since the velocity along the surface is cos α v = −vf rf2 2 r the rate of the work done by the stress vector on conical die surface Γ3 (r0 ≥ r ≥ rf , θ = α) is rf cos α ˙ σθθ vf rf2 2 2πr sin α dr . WΓ3 = −µ r r0 Introducing here (7.4.16) and after some algebra, we get # 3 $ 2 σm R 4 sin α R0 f 2 ˙ Γ3 = −2µπvf R cot α √ v 1 − − η 2.0207 ln W f f 9 Rf R0 Rf 3 ( #√ ' 2 3σm 14 1 sin α Rf 2 √ − vf η ln cos α + cos α + + σxb 11 3 R0 R0 11 ( $& ' √ 3σm 1 − σm . (7.4.22) ln 1 + 1 + − √ 11 11

Rf + ln R0

Another law in metal plasticity is that the modulus of shearing stress due to √ friction is proportional to the yield stress τY = σY / 3. For viscoplastic materials this law is generalized as (7.4.23) τ = m IIσ where m is a constant friction coeﬃcient and 0 ≤ m ≤ 1. m = 0 means no friction, while m = 1 means adherence on the wall. Using (7.4.10) (7.4.23) can be written $ # vf rf2 σm (7.4.24) τ = m √ + 3 η 11 cos2 α + 1 . r 3

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

Axi-Symmetrical Problems

dynamic

337

With this law the rate of work done on the conical die surface is # $& 3 cos α η sin α σ R v R m f f f ˙ Γ3 = 2πmvf R2 √ ln + 11 cos2 α + 1 −1 . W f sin α 3Rf R0 3 R0 (7.4.25) Let us observe that both expressions are variable depending on vf , η and α. The dependency on r is distinct; in the law (7.4.21) it decreases with decreasing r, while in the law (7.4.23) it increases with increasing r. We assume all the other parameters to stay constants. 7.4.4

Drawing Stress

We apply now the theorem of powder expanded, extended to the volume V of the viscoplastic domain. We have σij Dij dV + σi [vi ] dS + σi [vi ] dS = σi vi dS , (7.4.26) Γ1

V

Γ2

∂V

where σi is the component of the stress vector on Γ1 , Γ2 or ∂V while [v] is the jump of the particle velocity at the crossing of the surface Γ1 or of the surface Γ2 . The term on the right-hand side of (7.4.26) represents the rate of work done by the stress vector on the surface bounding the volume V . This term can be decomposed into ﬁve parts. On the plane Γ6 where x = r0 we have ˙ Γ6 = −πR02 v0 σxb , W

(7.4.27)

˙ Γ4 = πR2 vf σxf . W f

(7.4.28)

while on Γ4 where x = rf ,

Along Γ5 the rate of work is zero since this surface is stress free. Along the surfaces where a friction law exists the integral is already computed. Let us consider now the last term from right. The velocity discontinuity is [v] = v0 sin θ. The surface element is dA = rj2 sin θ dθ dϕ . Thus

σi [vi ] dA =

Γ2

α

σi τi sin2 θ dθ

2πv0 r02

(7.4.29)

0

where τi is the vector tangent to Γ2 in the meridian plane. From the global condition of equilibrium of the forces which act on the domain I of the bar we have dA = 0 −πσ0 R02 + σ0∗ Γ2

we determine σ0∗ =

σ0 σ0 R02 = (1 + cos α) . − cos α) 2

2r02 (1

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

338

dynamic

Dynamic Plasticity

Introducing this value in (7.4.29) we get 2 σi [vi ] dA = −(1 + cos α)πv0 r0 σ0 Γ2

or

σi [vi ] dA = − Γ2

α

sin3 θ dθ

0

− cos α + 1/3 cos3 α + 2/3 πv0 R02 σ0 . 1 − cos α

Similar for the surface Γ4 we get 1 2 3 σi [vi ] dA = πvf rf σf (1 + cos α) (1 − cos α) + (1 − cos α) . 3 Γ4

(7.4.30)

(7.4.31)

Combining all these formulae, for the second friction law, we have − cos2 α + (1/3) cos3 α + 2/3 sin2 α σf σb 1 + 2 = σm 2 cos α − cos2 α − (2/3) cos3 α − 1/3 σm sin2 α # 3 $ 1 Rf 11 2 ηvf R0 1− 1 − cos α + (1 − cos3 α) + + 2f (α) ln Rf 3 σm Rf sin α R0 3 # 3 $&& R0 ηvf sin α R 2 f √ + 11 cos2 α + 1 1 − + √ mctgα ln Rf σm Rf R0 3 3 +

2 L σY m 3 Rf σm

(7.4.32)

where

' ( √ 11 1 1 1 1 + ln cos α + cos2 α + −f (α) = √ (cos α) cos2 α + 11 11 11 2 3 sin2 α −

' (& 12 12 1 − ln 1 + . 11 11 11

and N=

ηvf σm Rf

(7.4.33)

is a “speed eﬀectiveness parameter” expressing the inﬂuence of the speed on the energy dissipated in the domain of viscoplastic deformation. Further the term containing the factor m expresses the energy dissipation due to friction; in this term a component due to the speed inﬂuence is also present. The ﬁnal term in Eq. (7.4.32) is due to the friction along the die land of length L. In the same equation the dissipation term due to the presence of discontinuity surfaces Γ1 and Γ2 is also involved, but not additively. Since the rates of deformation involved in viscoplastic deformation in region II are very high, the resultant heating was also considered (Cristescu [1980]), in order

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Axi-Symmetrical Problems

dynamic

339

to be able to choose the values of the various constants from the constitutive equation correctly. It was assumed that the heating is adiabatic, that is " dT "" ρc " = σij Dij dV (7.4.34) dt med V where c is the speciﬁc heat (assumed constant), T is the temperature and dT /dt|med is the mean temperature gradient over the volume V , deﬁned by " dT dT "" 1 dV. = " dt V dt med

V

On the right-hand side of (7.4.34) is the stress power over the volume V , which is given by the above formula. This equation becomes # 3 $ R N R 2 0 f " 2f (α) ln 1− + 2 " R σ πv dT " f f m Rf 3 sin α R0 . = " dt med V ρc 11 3 × 1 − cos α + (1 − cos α) 3 This equation was used to estimate the mean rise of temperature due to fast viscoplastic deformation. For steel wire and R0 = 0.5 mm, vf = 1 m/s, α = 6◦ , η = 0.34 Nmm−2 s, ρc = 3.60 Nmm−2 (◦ C)−1 , r% = 20%, an approximate mean temperature rise of ∆Tmed = 84.0◦ C (28.2◦ C due to plastic deformation and 55.8◦ C due to the speed eﬀect), is obtained, estimating that the particles cross region II in a time interval less than 5 × 10−4 s. For vf = 50 m/s and η = 0.023 Nmm−2 s, the mean temperature rise due to viscolastic deformation is ∆Tmed = 121◦ C (29.6◦ C due to plastic deformation and the remaining due to the speed eﬀect). Another estimation of temperature rise was done by integrating numerically the equation (7.4.34). This is no more done since the temperature rise is less than 150◦ C at the most and thus do not change the constants of the materials signiﬁcantly. 7.4.5

Comparison with Experimental Data

We have chosen the experimental data by Wistreich [1955] for copper wires with Rf = 1.27 mm and mean yield stress of σY = 349.7 MN/m2 have been drawn at a speed of vf = 33 mm/sec, the friction coeﬃcient is µ = 0.025. The viscosity coeﬃcient for copper was taken from Lindholm and Bessey [1969] η = 2.78 MN/m−2 from where N = 0.2069. For these values of the constants, the results shown in Fig. 7.4.2 were obtained. For various reductions in area deﬁned by # 2 $ Rf r% = 100 1 − R0 the variation of the drawing stress with semi-cone angle α is plotted. The discrepancy with experimental data existing for α relatively big and/or r small is due to the bulging phenomenon.

January 12, 2007

10:41

340

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Dynamic Plasticity

Fig. 7.4.2 Variation of drawing stress with semi-cone angle for various reductions in area: comparison between theory and experiment.

Fig. 7.4.3

Total drawing force for various reductions and area and three semi-cone angles.

dynamic

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Axi-Symmetrical Problems

dynamic

341

Fig. 7.4.4 Variation of relative drawing stress and optimum die angle with the speed eﬀectiveness parameter N , for diﬀerent degrees of reduction.

Another comparison with experimental data has been done for the total drawing force as measured by Wistreich for semi-cone die angles equal to: 2.29◦ , 8.02◦ and 15.47◦. These experimental results are shown in Fig. 7.4.3 together with the theory. For mild steel Manjoine (see Lindholm and Bessey [1969]) and Cristescu [1977] give D ≈ 10−1 –1 s−1 , η ≈ 104 kNm−2 s, for D ≈ 1–10 s−1 , η ≈ 1700 kNm−2 s, for D ≈ 10–102 s−1 , η ≈ 200 kNm−2 s, and for D ≈ 102 –103 s−1 , η ≈ 24 kNm−2 s. For higher rates of deformation Campbell [1973] suggests η ≈ 2 kNm−2 s and it is varying very little. Let us observe that an increase of vf does not imply an increase on N , since η may decrease signiﬁcantly with the increase of vf . In the example given below, σb = 0 and L = 0, the consideration of these two parameters can be done very easily. In Fig. 7.4.4 are given for three reductions, the optimum relative drawing stress for diﬀerent values of N (full lines). From this ﬁgure it can be seen that the drawing stress increases with reduction and become large for very thin wires. A comparison with the experiments was done also by Cristescu [1977] for copper of diameter wires 2R0 = 0.94 mm and steel wires of 2R0 = 1.02 mm, tested slowly.

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

342

Dynamic Plasticity

Fig. 7.4.5

Drawing forces for copper wires.

For the die semi-angle α = 8◦ , the length of the land L = 0.5 mm, friction coeﬃcient on the land m = 0.08, friction on the conical surface µ = 0.09, and viscosity of the copper η = 2.94 Nmm−2 s. Figure 7.4.5 shows some results for α = 8◦ (smaller ﬁgures) and α = 7◦ . That is because α = 8◦ is closer to the optimum die angle. The lines are the theoretical ones. The ﬁgure corresponds to L = 0.5 mm, µ = 0.06, m = 0.08, and η = 2.94 Nmm−2 s. Similar results for steel wires. 7.4.6

Other Papers

A visio-plastic method, for big deformations, was developed by Dahan and Le Nevez [1983]. First some extrusion pieces are obtained and measured. Then by a ﬁnite diﬀerence one is obtaining for a rigid work-hardening and isotropic material, the stress deviator and the strain. Also a Bingham model was used by Ionescu and Vernescu [1988], to describe numerically the wire drawing. The friction conditions are of two types: a Coulomb friction law and a viscoplastic one. The drawing speeds is low, with the viscosity coeﬃcient 2.94 Ns/mm2 .

dynamic

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

Axi-Symmetrical Problems

dynamic

343

The same theory was presented in a book devoted to “Mathematical Models in Working Metals” by Camenschi and S ¸ andru [2003]. The book contains much more than drawing of bars but this theory is presented. In reality the book presents some papers published since 1978. For instance the drawing of bars with asymptotic developments was ﬁrs published in Camenschi et al. [1979] for a friction law of the form (7.4.23) and in Camenschi et al. [1983] for a Coulomb friction law. Concerning the drawing theory one is assuming N < 1, that is slow processes. The solution is obtained for the incompressibility condition by introducing the ﬂow function ψ = ψ(r, θ) = R22 vf ψ 0 (r0 , θ), and vr0 = − where the upper index ments one is writing

0

r02

∂ψ 0 1 , sin θ ∂θ

vθ0 = −

r0

1 ∂ψ 0 sin θ ∂r0

is for dimensionless magnitudes. For asymptotic develop-

ψ 0 (r0 , θ) = ψ00 (θ) + N ψ10 (r0 , θ) + O(N 2 ) , p0 (r0 , θ) = p00 (r0 , θ) + N p01 (r0 , θ) + O(N 2 ) . and the solution is obtained in dimension quantities with a formula for the stress as well. One is obtaining the drawing force as # $ 3 R1 R23 2 |σf | 1 − 3 F (α, m) + N ln =√ G(α, m) σY R1 R2 3N where one have used the friction law (7.4.23) and m , γ= √ 1 − m2 α sin2k−1 θdθ % Ik = , 0 1 − sin2 θ(λ1 − λ2 sin2 θ)

k = 1, 2, 3

√ 3γ( 3 sin 2α − 3γ cos 2α + 2γ) √ , λ1 = sin2 α( 3 cos α + 3γ sin α)2 6γ 2 √ , sin α( 3 cos α + 2γ sin α)2 √ (cos3 α/2)(2γ + 3 sin 2α) √ F (α, m) = , γ(sin α/2)(1 + 2 cos α) + 3 cos α cos(α/2) √ (m/3) cos α sin2 α − sin α(γ sin α − (2/ 3) cos α)I1 √ G(α, m) = (1 − cos α)[sin 2α − (γ/ 3)(1 − cos α)(1 + 2 cos α)] √ √ (γ( 3 sin 2α + 6γ cos 2α − 4γ)I2 + 4γ 2 I3 )/( 3 sin 2α + 6γ sin2 α) √ − . (1 − cos α)[sin 2α − (γ/ 3)(1 − cos α)(1 + 2 cos α)] λ2 =

2

January 12, 2007

344

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Dynamic Plasticity

The authors have determined also several optimum angles for the drawing, depending on friction, reduction and N . They have also considered a Coulomb friction law in Camenschi et al. [1983]. The same authors, S¸andru and Camenschi [1979] have considered the rolling of a material, by assuming that the rolls can be approximated by two straight lines. They apply an asymptotic series development. The kinetic and dynamic eﬀects, on the upper bound loads in metal forming processes, are due to Tirosh and Kobayashi [1976]. It is question of forging, extrusion and piercing. The same kind of approach was applied for rolling of viscoplastic materials (Tirosh et al. [1985]). Since the arc of contact area is practically small (α ≈ 5 deg) and the thickness of the sheet is small with respect to the roller diameter, the authors replace the arc of the contact area by a straight line. The strains are σm σrr − σθθ 1 1− √ √ , Drr = 2η 2 3 IIσ σm 1 1− √ √ τrθ , Drθ = 2η 3 IIσ and repeat the theorem of powder expansion and also with the same friction laws. The comparison with the tests seems good. Comparisons with experiments and with FEM are done. For instance in Fig. 7.4.6 a comparison with the data by Shida and Awazuhara [1973] and the FEM method by Li and Kobayashi [1982] are done. In another paper by Iddan and Tirosh [1996] one renounces at this assumption. The dynamic fracture by spallation in metals was considered by Gilman and Tuler [1970]. The stress state associated with plane strain is described, and the eﬀect of the initial conditions and the time dependent conditions of the material on spallation is discussed. Fu and Luo [1995] consider the rigid-viscoplastic FEM to analyze the viscoplastic forming process. The general rigid-viscolastic FEM formulation is given and speciﬁc formulations of isothermal forging processes and superplastics forming are listed also. As an application, the combined extension process of pure lead, which is strain-rate sensitive at room temperature, is analyzed. The simulated results reveal the variation of the forming load with the stroke and its dependence on conditions. On the basis of the metal ﬂow patterns deﬁned by the rigid-viscoplastic ﬁniteelement method, the change of the position of the neutral layer is given and it is found that the occurrence of folding at the ﬂange may be attributed mainly to an abnormal ﬂow pattern. Moreover, the calculated results bring to light the rule of deformation distribution and its dependence on strain rate. Alexandrov and Alexandrova [2000], assuming a rigid viscoplastic material model, show that the velocity ﬁelds adjacent to the surfaces of maximum friction must satisfy sticking conditions. This means that the stress boundary conditions, the maximum friction law, may be replaced by the velocity boundary condition.

dynamic

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Axi-Symmetrical Problems

Fig. 7.4.6 for steel.

dynamic

345

Comparisons between measured, predicted, and computed roll force versus reduction

For planar ﬂows, they show that plastic deformation in the vicinity of maximum friction surfaces is possible. The metal forming processes of aluminum-alloy wheel forging at elevated temperature are analyzed by the ﬁnite element method by Kim et al. [2002]. A coupled thermo-mechanical model for the analysis of plasic deformation and heat transfer is adapted in the ﬁnite element formulation. The rolling problem is not mentioned in the present book. We would like to mention the paper by Angelov [2004] in which a variational analysis of a rigidplastic rolling problem was considered. The material is rigid-plastic, strain-rate sensitive and incompressible. A nonlinear friction law is considered.

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

346

7.5 7.5.1

Dynamic Plasticity

Floating Plug Formulation of the Problem

In the present text the geometry of the ﬂoating plug is studied in order to optimize the tube drawing process, i.e., in order to increase the drawing speed, to increase the reduction per pass, to reduce the consumption of energy used, etc. For this purpose the theory of fast tube drawing with ﬂoating plug is formulated and a formula is given expressing the drawing stress as function of various parameters involved in the drawing process (drawing speed, semi-cone die angle α, tube geometry, mechanical properties of the material, friction coeﬃcients and plug geometry). Some data, mainly of experimental character and of industrial practice can be found in Bisk and Shveikin [1963] and Perlin [1957]. From the experiments described in these books it results that when the drawing speed is increased from 20 m/min to 60 m/min the drawing force increases several times (two or even three times). The signiﬁcant inﬂuence of the speed on the wire drawing process was mentioned. Since the rates of strains are higher than 102 s−1 , one has to describe theoretically this process with a viscoplastic constitutive equation (Cleja and Cristescu [1979]). Due to the geometrical symmetry of the die, plug and of the tube the problem can be considered to be axisymmetrical. For this reason the geometry of the deformation process was represented in Fig. 7.5.1 in a symmetry plane. The tube of initial thickness R1 − R3 enter in the die with the speed v0 and leaves it with the speed vf . The thickness of the tube at the exit is R2 −R4 . Three domains can be distinguished: in domains I and III the material is assumed rigid, while in domain II the viscoplastic deformation takes place and a Bingham type of constitutive equation

Fig. 7.5.1

Geometry of ﬂoating plug.

dynamic

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

Axi-Symmetrical Problems

dynamic

347

σm 1− √ √ σij (7.5.1) 3 IIσ is satisﬁed. Here again σm is the “mean” yield stress, i.e., the area under the universal stress–strain curve divided by the equivalent strain, while 1 Dij = 2η

Z =

Z

if Z > 0

0

if Z ≤ 0 .

(7.5.2)

It is assumed that the domains previously mentioned are separated by the discontinuity surfaces Γ1 and Γ2 . Generally it is assumed that one of the two curves Γ1 or Γ2 has a prescribed shape and the second one is then determined accordingly. In what follows Γ2 is taken as an arc of a circle of radius r2 . It will be assumed that in the domain II the material ﬂows radially towards the pole 0 situated at the distance x from the symmetry axis; in what follows x is to be determined. Here we will determine the semi-angle γ of the ﬂoating plug. From the point of view of the optimization of the drawing process, this angle is a fundamental parameter of the geometry of the ﬂoating plug. Let V be the domain ﬁlled up with the viscoplastic material and Γ = Γσ ∪ Γv = ∂V , where Γσ is the portion of the boundary where the stress vector is prescribed and Γv the one on which the velocity ﬁeld is prescribed. Let v be a kinematic admissible ﬁeld (i.e., div v = 0 in V and v|Γv = v0 ). We denote by D the set of kinematic admissible ﬁelds on V . Then the functional 2 ) 1 σm σ ij Dij + √ IID dV + [t · v] dσ J(v) = 2 3 V j=1 Γj

X · v dV −

−

t · v dσ

(7.5.3)

Γσ

V

is minimized. Here [f ] = f + − f − is the jump of f at the crossing of the considered surface. Let Dγ ⊂ D0 be a family of kinematic admissible ﬁelds depending on a parameter γ. The kinematic ﬁeld which corresponds to that value of γ for which J(v) on Dγ is minimum will be determined. 7.5.2

Kinematics of the Deformation Process

From r2 sin α = R2 − x ,

r2 sin γ = R4 − x

(7.5.4)

the following expression for x x= and for r2

R2 sin γ − R4 sin α sin γ − sin α

(7.5.5)

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

348

dynamic

Dynamic Plasticity

r2 =

R2 − R4 R2 − x = sin α sin α − sin γ

(7.5.6)

are obtained. The relation between the velocities v0 at the entrance and vf at the exit is obtained as R2 − R42 vf . (7.5.7) v0 = 22 R1 − R32 Writing now the condition of equal rates of ﬂow for a circular annulus comprised at the entrance between radii r1 (θ) sin θ + x and R3 and at the exit between r2 sin θ + x and R4 , the equation of the discontinuity surface Γ1 & 2 − R2 1 R 1 3 r1 (θ) = [(r2 sin θ + x)2 − R42 ] 2 + R32 − x (7.5.8) sin θ R2 − R42 is obtained. Here r1 (θ) can be either a decreasing or increasing function of θ. In order to determine a kinematic admissible velocity ﬁeld we introduce the curvilinear coordinates θ, r, ϕ by X = (r sin θ + x) cos ϕ ,

Y = (r sin θ + x) sin ϕ ,

Z = −r cos θ

(7.5.9)

where X, Y, Z are the Cartesian coordinates of a point P belonging to the domain II, the OZ axis is the symmetry axis, and θ ∈ [γ, α], r ∈ [r2 , r1 [θ]], ϕ ∈ [0, 2π] (see Fig. 7.5.1 which corresponds to ϕ = 0). Denoting by vr , vθ and vϕ the components of the particle velocity in the curvilinear coordinates chosen, and taking into account that due to symmetry vθ = vϕ = 0, from the incompressibility condition, we get C(θ) vr = r(r sin θ + x) where the function C(θ) is determined from the continuity of the normal component of the velocity at the crossing of the surface Γ2 , i.e., for r = r2 : vr = vf cos θ. The following velocity ﬁeld is thus found r2 (r2 sin θ + x) vr = vf cos θ , θ ∈ (γ, α) , r ∈ (r2 , r1 (θ)) r(r sin θ + x) vθ = vϕ = 0 .

(7.5.10)

The components of the rate of strain are Drr = −vf r2 (r2 sin θ + x) cos θ

2r sin θ + x , [r(r sin θ + x)]2

Dθθ = vf r2

r2 sin θ + x cos θ , r2 (r sin θ + x)

Dϕϕ = vf r2

r2 sin θ + x cos θ sin θ , r(r sin θ + x)2

Dθr = −vf r2

r(r2 sin θ + x) + x2 sin θ − xr2 cos 2θ , 2r2 (r sin θ + x)2

Dθϕ = Dϕr = 0 .

(7.5.11)

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

dynamic

Axi-Symmetrical Problems

With these formulas the second invariant of the rate of strain tensor is 2 vf r2 (Ar2 + Br + C) , 2IID = Dij Dij = 2 r (r sin θ + x)2

349

(7.5.12)

where 1 A = 6 cos2 θ sin2 θ(r2 sin θ + x)2 + (r2 sin3 θ + x)2 , 2 B = 6x sin θ cos2 θ(r2 sin θ + x)2 + x(r2 sin3 θ + x)(x sin θ − r2 cos 2θ) , x2 [x sin θ − r2 cos 2θ]2 . (7.5.13) 2 With the help of the invariant IIε for the Bingham model the stress power can be expressed as 2σm σij Dij = √ IID + 4IID , (7.5.14) 3 C = 2x2 cos2 θ(r2 sin θ + x)2 +

where σij are the stress components. For the whole volume V of the domain II deﬁned by θ ∈ (γ, α), r ∈ (r2 , r1 (θ)), ϕ ∈ [0, 2π], using (7.5.12)–(7.5.14) we get 4πσm σij Dij dv = √ vf r2 I1 (γ, α; r2 , r1 (θ)) + 4πη(vf r2 )2 I2 (γ, α; r2 , r1 (θ)) , 6 V (7.5.15) where the following notations

α

r1 (θ)

I1 (γ, α) = γ

and

r2

α

r1 (θ)

I2 (γ, α) = γ

r2

√ Ar2 + Br + C drdθ r(r sin θ + x) Ar2 + Br + c drdθ r3 (r sin θ + x)3

(7.5.16)

(7.5.17)

were used, together with the Jacobian of (7.5.9). 7.5.3

Friction Forces

Friction forces are involved at the interfaces between the tube and die and between the tube and the plug. On the conical surface of the plug it will be assumed that the friction between the rigid surface of the plug and the viscoplastic body, can be described by |tτ | = m IIσ = k + 2η IID . (7.5.18) The friction force T2 between the tube and the plug land at exit, Γ9 (see Fig. 7.5.1) has the direction k and the modulus |T2 | = 2πm2 τ2 lR4

(7.5.19)

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

350

dynamic

Dynamic Plasticity

where m2 is the friction factor, τ2 is the actual shearing yield stress of the tube at the exit while l is the length of the plug land at the exit. The resultant of the normal forces on the conical portion of the ﬂoating plug (θ = γ) has the modulus r1 (γ)−ε Tθθ |θ=γ (r sin γ + x) dr , (7.5.20) Nγ = 2π r2

Tθθ being the normal component on the conical portion of the plug. The contact between the tube and the plug, on the conical portion, is expressed by a relationship between r2 and r1 (γ) − ε with a = ε sin γ, representing the clearance between the maximum diameter of the plug and the inside diameter of the tube at entrance. The magnitude of Tθθ will be obtained assuming that the friction law (7.5.18) is giving the same tangential stress with the one given by a law of Coulomb type |tτ | = µ|Tθθ |, µ being the corresponding friction factor. Thus µTθθ = m4 IIσ . (7.5.21) This suggestion is done by the computations done at the bar. On the conical portion of the plug the modulus of the friction force is r1 (γ)−ε Tγ = 2πm4 IIσ |θ=γ (r sin γ + x) dr . (7.5.22) r2

The equilibrium condition of all the forces which act on the ﬂoating plug is Nγ + T2 + Tγ = 0

(7.5.23)

since the cylindrical portion of the plug, of radius R3 , is not in contact with the interior of the tube. Projecting now (7.5.18) on the symmetry axes of the plug and using (7.5.19), (7.5.20) and (7.5.22), we obtain the following equation which determine m4 τ2−1 sin γ − cos γ I3 (γ; r2 , r1 (γ) − ε) (7.5.24) l= m2 R4 µ with the notation

I3 (γ; r2 , r1 (γ) − ε) =

r1 (γ)−ε

IIσ |θ=γ (r sin γ + x) dr

r2

=

1 k sin γ[(r1 (γ) − ε)2 − r22 ] + xk(r1 (γ) − ε − r2 ) 2 r1 (γ)−ε + 2η IID |θ=γ (r sin γ + x) dr . (7.5.25) r2

In the next paragraph we ﬁrst determine the value of γ which minimize the functional J(v) and which is used to determine the length l of the cylindrical part of the plug.

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

Axi-Symmetrical Problems

7.5.4

dynamic

351

Determination of the Shape of the Floating Plug

For the problem considered here the functional J(v) on Uad (γ) becomes a function of γ j(γ) = 2πvf

√ 1 π(R12 − R32 ) σ0 (R22 − R42 ) − I5 + 2kr2 I1 (γ, α) 2 A(S1 )

+ km3 r2 R2 ln + ηvf r22

r1 (α) r1 (γ) − ε cos α + km4 r2 R4 ln cos γ r2 r2

*√ 2m3 R2 I4 (α, r2 , r1 (α)) cos α

+ √ + 2m4 R4 I4 (γ, r2 , r1 (γ) − ε) + I2 (γα) + m2 τ2 lR4 + m1 τ1 LR2

(7.5.26)

with the notations Ij introduced by the formulae (7.5.16) and (7.5.17) and A(S1 ) is the area of the surface S1 . Proof. For the computation of J(v) on Uad (γ) we use the formula divσ + ρb = 0 and we observe that the integrals on the volume are computed by (7.5.15)–(7.5.17), with the remark that I2 is now multiply with 1/2. The surfaces Sj involved, correspond to the values j = 3, 5–12, while the surfaces Sk , correspond to the value k = 1, 4. S2 is not involved in the computation of J(v) since on this surface the stress vector is not known. On the surface S3 — since Γ3 is a ﬂow line — the speed has the tangential component equal to vr , and the modulus of the tangential vector of the stress is given by (7.5.18). Thus r1 (α) t · v dA = −2πm3 vr IIσ |θ=α (r sin α + x) dr . (7.5.27) S3

r2

With (7.5.10) this relation becomes t · v dA = −2πm3 vf r2 R2 I6 (α; r2 , r1 (α)) cos α

(7.5.28)

S3

with the notation

r1 (α)

I6 (α; r2 , r1 (α)) = r2

IIσ |θ=α dr . r

(7.5.29)

Using now (7.5.18), (7.5.29) is now written I6 (α; r2 , r1 (α)) = k ln

r1 (α) √ + 2ηvf r2 I4 (α; r2 , r1 (α)) r2

(7.5.30)

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

352

dynamic

Dynamic Plasticity

where

r1 (α)

I4 (α; r2 , r1 (α)) = r2

√ " Ar2 + Br + C "" dr . r3 (r sin θ + x) "θ=α

(7.5.31)

In a similar way we compute the integral on S4 which becomes r1 (α)−ε t · v dA = −2πm4 vr IIσ |θ=γ (r sin α + x) dr S4

r2

= −2πm4 vf r2 R4 I6 (γ; r2 , r1 (γ) − ε) cos γ

(7.5.32)

while I6 is computed with (7.5.29)–(7.5.31), with the integral limits taken correspondingly. The surface S4 is a surface of discontinuity for the vector ﬁeld, [v]|S4 = −v. The integral S6 is t · v dA = −πv0 σ0 (R12 − R32 ) . (7.5.33) S6

The integral S1 will be computed from the term [v] · t, where t is the stress vector which act on this surface. In the symmetry plane considered, the tangent and normal unit vectors on S1 , deﬁned by the equation r = r1 (θ), deﬁned by (7.5.8), are 1 [(−r1 cos θ + r1 sin θ)k + (r1 sin θ + r1 cos θ)i] τ = 2 r1 + (r1 )2 1 [−(r1 sin θ + r1 cos θ)k + (r1 sin θ − r1 cos θ)i] . (7.5.34) n= 2 r1 + (r1 )2 The tangential components of the velocity are: v0 vτ+ = v0 · τ = (r1 sin θ − r1 cos θ) (r1 )2 + r12 vr r vτ− = vr · τ = (vr cos θ k − vr sin θ i) · τ = − 1 2 . (r1 )2 + r1

(7.5.35)

The normal component of the velocity is continuous at the crossing of S1 , and is vn = v0 · n = −v0

r1 sin θ + r1 cos θ . (r1 )2 + r12

(7.5.36)

The traction vector which act on the surface S1 (as a part of the boundary of III, thus of normal n) is determined from a mean formula, obtained from the equilibrium forces which act on the domain III: −π(R12 − R32 )σ0 k + σ0∗ A(S1 )k = 0 .

(7.5.37)

For the computation of the area A(S1 ) we take care of the element of the surface: % (7.5.38) dA = (r1 sin θ + x) (r1 )2 + r12 dθdϕ

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

dynamic

Axi-Symmetrical Problems

with r = r1 (θ) given by (7.5.8) and thus α % (r1 sin θ + x) (r1 )2 + r12 dθ . A(S1 ) = 2π

353

(7.5.39)

γ

From (7.5.37) and (7.5.39) we obtain: π(R12 − R32 ) σ0 . σ0∗ = A(S1 ) The stress vector on the surface S1 is given by the formula: t = t(x, n) = −σ0∗ k .

(7.5.40)

(7.5.41)

Thus from (7.5.35), (7.5.40), (7.5.41) and (7.5.34) we ﬁnd: α v0 (r1 sin θ − r1 cos θ) + vr r1 π(R12 − R32 ) σ0 2π [v] · t dA = A(S1 ) (r1 )2 + r12 S1 γ × (−r1 cos θ + r1 sin θ)(r1 sin θ + x) dθ .

(7.5.42)

We introduce notation: the v0 α vr (r1 sin θ − r1 cos θ)(r1 sin θ + x) (r1 sin θ − r1 cos θ) + r1 dθ I5 = vf γ v0 (r1 )2 + r12 (7.5.43) and the relation (7.5.42) becomes: π(R12 − R32 ) 2πσ0 vf I5 . t · [v] dA = − (7.5.44) A(S1 ) S1 On the surfaces S9 and S11 , taking into account the friction forces on the plug, we have: t · v dA = −2πm2 τ2 vf lR4 ,

S9

(7.5.45) t · v dA = −2πm1 τ1 vf LR2 ,

S11

where τj (with j = 1, 2) are the plasticity limits at shearing, corresponding to the surfaces, and l the cylindrical lengths of the plug at the exit is given by (7.5.24). The integral S4 is computed with (7.5.32): t · [v] dA = − t · v dA . (7.5.46) S4

S4

Introducing the integrals already computed we get: √ π(R12 − R32 ) J(v) = 2 2πkvf r2 I1 (γ, α) + 2πη(vf r2 )2 I2 (γ, α) − 2πσ0 vf I5 A(S1 ) r1 (α) √ + 2ηvf r2 I4 (α, r2 , r1 (α)) + 2πm3 vf r2 R2 cos α k ln r2 r1 (γ) − ε √ + 2πm4 vf r2 R4 cos γ k ln + 2ηvf r2 I4 (γ, r2 , r1 (γ) − ε) r2 + πv0 σ0 (R12 − R32 )

(7.5.47)

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

354

dynamic

Dynamic Plasticity

which will be denoted by j(γ) and which by minimization will determine a value which will be denoted γ ∗ = γopt ; because the value of the functional J(v) computed on real ﬁelds towards the pole O, in the plane of symmetry, (in the deforming ﬁeld) becomes a function of γ. The shape of the plug is given by the value γopt and the lengths l computed from (7.5.24), for this value of γ. With these values of γ and l we will compute the drawing force. 7.5.5

The Drawing Force

The drawing stress will be determined from the theorem of powder expanded applied to the domain V bounded by the boundaries S3 –S13 and which contains the discontinuity surfaces S1 and S2 : σ · D dx + V

2 ) k=1

Sk

t · [v] dA =

t · v dA ,

(7.5.48)

∂V

,13 (with ∂V = j=3 Sj ). In this formula ε˙ will be computed with the kinematics admissible ﬁeld (7.5.10) using γ = γopt , while the stress ﬁeld σ must be considered a static admissible ﬁeld (i.e., satisfying the equilibrium equations and the boundary conditions). Since we were unable to ﬁnd such a ﬁeld, we compute the power σ · D with the formula (7.5.15) with D found previously. Therefore we found the approximate values for the velocity by a minimization procedure. The integral on the volume from (7.5.48) is given by (7.5.15). The integral on S2 is computed with a similar procedure with the one which was used to get (7.5.43) and (7.5.44). The unit vectors on the tangent and normal at Γ2 are τ = sin θ k + cos θ i and n = − cos θ k + sin θ i and therefore vτ+ = 0 ,

vr− = vf k · τ = vf sin θ .

(7.5.49)

The stress vector on S2 will be computed from a global condition of equilibrium of the forces which act on the rigid domain III of the tube: dA k , (7.5.50) 0 = −2π(m1 τ1 LR2 + m2 τ2 lR4 ) + πσf (R22 − R42 ) − σf∗ S2

since we assume that σf∗ k is a mean stress on the surface. With the expression dA = r2 (r2 sin θ + x) dθdϕ of the element of the surface S2 , with (7.5.49) and (7.5.50), the integral on S2 is computed from "α " x sin 2θ cos3 θ " + θ− t · [v] dA = −2πr2 vf σf∗ r2 − cos θ + " 3 2 2 S2 γ

(7.5.51)

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

dynamic

Axi-Symmetrical Problems

355

or if we replace σf∗ from (7.5.50)

# cos3 θ πvf r2 − cos θ + t · [v] dA = r2 (cos γ − cos α) + x(α − γ) 3 S2 x + 2

$""α sin 2θ " θ− " [2(τ1 m1 LR2 + m2 τ2 lR4 ) − σf (R22 − R42 )] . " 2 γ

(7.5.52) The integrals on the surfaces S9 and S11 are computed in (7.5.45) taking into account the friction forces between the tube at exit and the plug. The integral on S13 is t · v dA = πvf σf (R22 − R42 ) . (7.5.53) S13

Introducing now in (7.5.48) the formulae (7.5.15), (7.5.44), (7.5.52), (7.5.28)– (7.5.33), (7.5.45) and (7.5.53) and taking into account the integrals on Sj with j = 5, 7, 8, 10, 12 are zero, we obtain: √ π(R12 − R32 ) 2kr2 I1 (γ, α) + 2ηvf r22 I2 (γ, α) − σ0 I5 A(S1 ) m1 τ1 LR2 + m2 τ2 lR4 + (1/2)σf (R22 − R42 ) r2 (cos γ − cos α) + x(α − γ) "α " x sin 2θ cos3 θ " + θ− × r2 − cos θ + " 3 2 2 γ +

= −m3 r2 R2 cos αI6 (α, r2 , r1 (α)) − m4 r2 R4 cos γI6 (γ, r2 , r1 (γ) − ε) −

v0 σ0 2 σf 2 (R2 − R42 ) . (R1 − R32 ) − m2 τ2 lR4 − m1 τ1 LR2 + 2vf 2

(7.5.54)

We use now (7.5.26) and (7.5.30), and grouping the terms which contain vf we obtain from (7.5.54) the following expression for the drawing force σf =

τ2 m2 lR4 + m1 τ1 LR2 R22 − R42 + x + 2

# "α cos3 θ "" R22 − R42 r2 − cos θ + " 2[r2 (cos γ − cos α) + x(γ − α)] 3 γ &−1 "α $ " " sin 2θ "" R22 − R42 min J(v) 2 " θ− + + ηv r I (γ, α) . f 2 2 " " 2 2 2πvf γ=γ ∗ γ (7.5.55)

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

356

dynamic

Dynamic Plasticity

In this formula, the terms which contains vf will describe the speed inﬂuence on the drawing force. We note that all the integrals I1 , I2 , I4 , I5 do not depend on vf . At the end, we will make precise how to make these computations, which are involved in the drawing force σf [the formula (7.5.55) as well as in J(v) — the formula (7.5.47)]. Let cos2 θ 2 2 2 2 (7.5.56) δ = x cos θ(r2 sin θ + x) 2 sin θ + 2 √ √ √ √ Ax + δ Ax + δ , x2 = (7.5.57) x1 = sin θ sin θ and the variable t: √ t = Ar2 + Br + C − Ar . (7.5.58) Then for I1 (γ, α) we obtain the formula: I1 (γ − α) " √ " √ √ "( " " α '√ √ " t − x1 " "r1 (θ) C "" t − C "" A δ " " √ "− ln " ln |2 At − B| − ln " dθ = " t + C " sin θ x x sin θ " t − x2 " "r2 γ (7.5.59) while for I2 (γ, α) — formula (7.5.17) — follows: " " α# " b " r e "− − a ln "" I2 (γ − α) = " r sin θ + x r sin θ(r sin θ + x) γ 1 − 2

c f + 2 r sin θ(r sin θ + x)2

$""r1 (θ) " dθ " "

(7.5.60)

r2

where

3B sin θ 6C sin2 θ + A− , x x2 C 3C sin θ 1 , c= 3, b= 3 B− x x x 2B sin θ 3C sin2 θ sin θ − −A + , e= 2 x x x2 B sin θ C sin2 θ sin θ −A + − . f = x x x2 The integral (7.5.31) for θ ∈ [γ, α] is computed according to: " " ' " t − √C " b1 b2 c1 " " √ "− √ − √ − √ I4 (θ, r2 , r1 (θ)) = a1 ln " "t + C " t − C t+ C (t − C)2 (" " " "r1 (θ) " t − x1 " f c2 f 1 2 "− " √ − + e1 ln "" − t − x2 " t − x1 t − x2 "r2 (t + C)2 a=

1 x3

(7.5.61)

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

Axi-Symmetrical Problems

where

B sin θ 3C sin θ B2 − + A− , 8C x x2 √ √ (B − 2 AC) B − 2 AC − 8C sin θ/x

dynamic

357

1 a1 = √ Cx2 b1 =

8Cx2 √ √ (B + 2 AC)(B + 2 AC − 8C sin θ/x) , b2 = 8Cx2

,

(x21 − C) sin2 θ (x22 − C) sin2 θ , f = , 2 2x4 2x4 √ (B − 2 AC)2 √ , c1 = a Cx2 ' √ ( √ sin θ (x21 − C) sin2 θ 3 δ √ , − A+ e1 = 3 − x x 2x δ √ (B + 2 AC)2 √ c2 = . 8 Cx2

f1 =

The integral I3 (γ, r2 , r1 (γ) − ε) — the formula (7.5.25) — needs the following computation: r1 (γ)−ε IID |θ=γ (r sin γ + x) dr r2

√ " Ar2 + Br + C "" = dr r2 (r sin γ + x) "θ=γ r2 " # √ " √ 1 B − 2C sin γ "" t − C "" B − 2 AC √ √ "− √ = ln " 2 " " 2x 2x C t+ C t− C √ √ " $"r (θ)−ε " " " δ "" t − x1 "" "" 1 1 B + 2 AC " √ + 2 ln " . − " " " 2x x t − x2 t+ C θ=γ r2

r1 (γ)−ε

(7.5.62) The integral I5 , given by formula (7.5.43), which is involved in the computation of the functional is computed numerically. The same with the integrals with respect to θ, from the relations (7.5.59) and (7.5.60), one compute them numerically. 7.5.6

Numerical Examples

In order to show how the previously established formula can be used several numerical examples will be given. In choosing the constants involved in the constitutive equation, some experimental data obtained for mild steel was used. For this

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

358

dynamic

Dynamic Plasticity

material some mechanical properties which can be described by a Bingham model were already given previously. We stress however, that the numerical examples given here have a qualitative character only. Drawing stress. Several reductions in area were considered. By deﬁnition the reduction in area is R2 − R42 (7.5.63) r% = 100 1 − 22 R1 − R32 while λ=

1 R12 − R32 = R22 − R42 1 − r/100

(7.5.64)

is called the coeﬃcient of extension. In order to give more general examples, the inﬂuence of the speed will be described with the parameter ηvf which is called “speed factor”, or by the dimensionless number ηvf (7.5.65) N= σY 0 R1 which is called the “parameter of speed inﬂuence”. Here σY 0 is the initial limit of plasticity. For big speeds, η decreases very little. We remind that in order to establish from one dimensional test a relation between η and the speed, we deﬁne a mean value for the strain rate √ 3πvf 2r2 1 √ I1 (γ, α) IID dV = (7.5.66) Dm = V V V 6 extended over the whole viscoplastic domain of volume V estimated by 3 r12 − r22 r1 − r23 (cos γ − cos α) − x(α − γ) V = 2π 3 2

(7.5.67)

where r1 is a mean value r1 (mean) = (1/2)(r1 (α)+r1 (γ)). The term from the square bracket from (7.5.66) is computed numerically. The formula (7.5.67) introduces √ ¯ = 2Dm / 3 was used as the mean errors in the estimation of Dm of 1%. Then D equivalent speed of deformation. The coeﬃcient of viscosity in the Bingham model was chosen from the experi¯ From the mental data which correspond to the speed of deformation D1 = D. experimental data of Manjoine [1944] and Cristescu [1977] was establish the empi¯ in s−1 . ¯ + 0.000204, with η in kgf mm−2 s and D rical formula η = (0.74/D) Another parameter involved in the theory of tube drawing is the reduction in diameter deﬁned by the ratio R3 /R4 . The thickness of the wall is expressed by R3 /R1 . Thus in order to characterize the geometry of the tube drawing we use: • the reduction in area r% or λ; • the reduction in diameter expressed by R3 /R4 ; • the reduction of the wall thickness expressed by R3 /R1 .

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Axi-Symmetrical Problems

dynamic

359

In all examples given below the radius R4 was maintained constant and all the other radius were varied in order to obtain various reductions in areas, various reduction in diameter and various wall thicknesses. Most computations were done for the angle α = 12◦ , but other cases were also considered. Concerning the free surface a, in most of the cases it was taken a = 0.5 mm, and sometimes a = 1 mm. Generally this free surface must be small, and for tubes with thin walls and carefully prepared drawing, a can be chosen smaller than 0.5 mm. In the following examples several values for the friction factor m were considered. In the computation of the land l according to the formula (7.5.24) the friction coeﬃcient µ is also involved. After choosing m, the value for µ was obtained from the empirical formula µ = (3/4)m, which was obtained for drawing of wires. The optimum γ angle. We observe also that J(v) increases faster when γ increases than when γ decreases. That suggests for the practice the idea that the ﬂoating plug is to be computed for higher speeds and that will be good for smaller speeds as well. In Fig. 7.5.2 is given a ﬁgure showing the contribution of various terms in the minimum of the functional. The ﬁrst curve is the friction ﬂoating plug-tube, the second the friction matrix-tube and the third the internal dissipation. The inﬂuence of the speed and of the friction factors on the value of the functional. One can see a signiﬁcant inﬂuence on the functional of the speed and of the friction factors (Fig. 7.5.3).

Fig. 7.5.2

Contribution of various terms contained in the functional for α = 13◦ .

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

360

Dynamic Plasticity

Fig. 7.5.3

Speed inﬂuence and friction inﬂuence on the functional J(v).

Fig. 7.5.4

Inﬂuence of the die angle on the drawing stress.

dynamic

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

Axi-Symmetrical Problems

dynamic

361

The inﬂuence of the die angle. The inﬂuence of the die angle on the drawing stress and corresponding plug angle is shown on Fig. 7.5.4 for two sets of friction factors and three sets of velocity factors. One can see that the increase of the drawing stress with speed is more signiﬁcant at small die angles. On the same ﬁgure by dotted or interrupted lines are given the values of the plug angle corresponding to various frictions, speeds and die angles. When the die angle is increased, the corresponding plug angle must also be increased. The diﬀerence α − γ increases slightly when α increases. The drawing stress is decreasing when the die angle is increasing. The optimum angle γ decreases with the increase of the speed. That is more important at small speeds. For higher speeds this decrease is smaller. Our solution does not allow a too much increase of α, since in this case we have some other phenomena (Bramley and Smith [1976]). The shape of the ﬂoating plug is deﬁned essentially by the angle γ and the length l of the land. While γ is uniquely deﬁned, l is not. Here the maximum value for l was computed, that is the value which would keep the ﬂoating plug in its most advanced position there where the whole conical surface of the plug is in contact with the inner surface of the tube. For practical purposes l is to be reduced with one third or even with one half of this computed length. Figure 7.5.5 gives the values of γ and l for various die angles and three drawing speeds. It is shown that l

Fig. 7.5.5

Computation of γ and l, for three drawing speeds.

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

362

Dynamic Plasticity

increases with α, but decreases when the drawing speed is increased. For a certain high speed and/or certain small α, l can decrease even to zero, i.e., the ﬂoating plug can be kept in equilibrium without any cylindrical land. A further increase of the drawing speed or a further decrease of the die angle is certainly impossible since the plug cannot be maintained in equilibrium any more. There are also some other limit drawing regimes which may occur when the drawing stress equals the current yield stress of the material; these limit drawing regimes can also be found quite easily using the main formula (7.5.55) with the condition σf < σY . Thus another limitation for the drawing speed and die angle is found. It is also found that if the friction coeﬃcient is higher, then the angle γ is only slightly reduced but l is reduced signiﬁcantly. The inﬂuence of the tube geometry on the drawing process with ﬂoating plug can be considered easily using formulas (7.5.47), (7.5.24) and (7.5.55). One of the geometrical parameters of signiﬁcance for the tube drawing is the wall thickness expressed by the ratio R3 /R1 . Generally, when the wall thickness decreases stress increases (more signiﬁcantly at high reductions in area and high drawing speeds) (Fig. 7.5.6), the plug angle increases and l also increases (Figs. 7.5.7 and 7.5.8).

Fig. 7.5.6

Variation of wall thickness for various speeds.

dynamic

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Axi-Symmetrical Problems

Fig. 7.5.7

dynamic

363

Variation of plug angle and of length l.

Another important drawing parameter is the diameter reduction expressed by the ratio R3 /R4 . Generally an increase of this ratio decreases γ, increases l maximal, increase σf , etc. Signiﬁcant diameter reductions are impossible with thin wall tubes, high reductions in area or high drawing speeds. All these limit drawing regimes can be easily computed. The clearance a, is of less importance in the whole process. Certainly an increase of a, decreases the drawing stress and therefore allows an increase of the drawing speed. Conclusions. The most important conclusions are: (1) The drawing stress for tube drawing with ﬂoating plug is obtained from formula (7.5.55). It gives the drawing stress as function of the drawing speed, die angle, tube geometry, and mechanical properties of the material, friction coeﬃcients and plug geometry. (2) The optimum geometry of the ﬂoating plug is obtained for various drawing conditions. (3) The optimum semi-cone plug angle is decreasing with decreasing semi-cone die angle, increasing speed, increasing friction, increasing tube wall thickness, increasing diameter reduction.

January 12, 2007

364

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Dynamic Plasticity

Fig. 7.5.8 Nomogram for the computation of ﬂoating plugs for drawing of small tubes. There are three programs: initial diameter × initial thickness of the wall → ﬁnal diameter × the ﬁnal thickness of the wall. Various angles α and various drawing stress are given.

(4) The plug land is increasing with α. Also l is increasing when the friction decreases and when the speed decreases. The plug land increases signiﬁcantly with the increase of the diameter reduction, and increases when the wall thickness is decreasing. (5) There are limit drawing regimes which cannot be surpassed; these correspond to cases when the drawing stress reaches the actual yield stress of the tube or when the plug land decreases to zero. Another theory of drawing with ﬂoating plug is due to S ¸ andru and Camenschi [1988] (see also Ioan and Ioan [1999]). They are assuming again slow processes so that N < 1, and asymptotic developments follows. The drawing stress is

dynamic

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

Axi-Symmetrical Problems

dynamic

365

σf R22 2 R2 LmL 2 √ = √ + σY N 3(R22 − R42 )(R12 − R32 ) 3 R22 − R42 $ # R2 (R22 − R12 ) R2 (R32 − R22 ) + R1 (R12 − R32 ) F (α) + F (γ) × R1 R3 A R32 (R12 − R22 ) G(α, γ) + √ −√ 2 2 2 2 2 3(R2 − R4 )(R1 − R3 ) 3(R1 − R32 )(R22 − R42 ) R1 R3 + R32 (R22 − R12 ) ln × R12 (R32 − R22 ) ln R2 R1 were all the constants are determined from other equations. Here u(θ) = a + bp(θ) + q(θ) , A + Bp(θ) + Dq(θ) + K1 (θ)p(θ) + K2 (θ)q(θ) , 6 α 9 K1 (θ) = − f (t)q(t) sin t dt , 16 γ α 9 f (t)p(t) sin t dt , K2 (θ) = 16 γ v(θ) =

1 + cos 2θ , 3 1 θ q(θ) = + cos 2θ ln tan − (1 − 3 cos θ)(1 + cos θ) , 3 2

p(θ) =

F (α) = [2a sin α − u (α) cos α] sin2 α , F (γ) = [2a sin γ − u (γ) cos γ] sin2 γ , G(α, γ) = mα cot α + mγ cot γ − 4[v(α) − v(γ)] − v (α) cot α + v (γ) cot γ tan α/2 + [A cos γ + v (γ) sin γ + mγ sin γ] ln tan γ/2 # α u (t) α −2 dt + 6 ln tan 2 3u2 (t) + u2 (t)/4 γ × γ

α

u(t) sin t

dt − 3u2 (t) + u2 (t)/4

γ

α

$ u(t) sin t ln(tan t/2) dt . 3u2 (t) + u2 (t)/4

Several examples are given for the determination of the drawing stress and all the other unknown quantities.

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

366

7.6 7.6.1

Dynamic Plasticity

Extrusion Formulation of the Problem

Let us consider now a mathematical model for hot tube extrusion, taking into account the inﬂuence of the working speed, when melted glass is used as a lubricant. We consider the problem of being stationary and isothermal. The working speed is considered variable during the process but for a certain magnitude of this velocity it is assumed that it is maintained constant for certain time interval so that during this time the process is considered “stationary”. Therefore, the variation of the working speed is described by a set of stationary cases (Cleja-Tigoiu and Cristescu [1985]). The extrusion problem considered with classical plasticity theory was considered by many authors. We mention here only Avitzur [1968], Blazynski [1976], Maneghin et al. [1980], Medvedev et al. [1980], Hartley [1971], etc. to mention just a few. The cylindrical billet of annular cross-section with outer radius R1 , inner radius R3 and length l is pushed out from a cylindrical container using a ram which is moving with the speed v0 (Fig. 7.6.1). In the interior of the billet a cylindrical plug of radius R3 and moving together with the ram is used to control the ﬁnal inner radius of the tube. In front of the billet, between the billet and container, is placed a glass ring which at the beginning of the process melts and forms a dead zone which during the extrusion process is an extrusion of the die. All other surfaces of the billet are also glass lubricated. As is well known, glass lubrication allows higher working speeds and therefore high rates of deformation are involved (of the order of 102 s−1 ). Due to the symmetry of the process the considered problem is axial symmetric and the geometry of the process is shown in Fig. 7.6.1 (not to

Fig. 7.6.1

Geometry of extrusion process.

dynamic

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Axi-Symmetrical Problems

dynamic

367

scale). The mathematical problem reduces to the determination of the velocity ﬁeld v and the stress ﬁeld σ, smooth in V , which must satisfy the equilibrium condition, incompressibility condition and a constitutive equation of Bingham type: k 1 1− √ σ (7.6.1) divσ = 0 , div v = 0 , D = 2η IIσ where the same notation as given previously are used. η is the viscosity coeﬃcient and k is the mean yield stress in pure shear, both η and k being temperature dependent. A prime denotes “deviator”. Boundary conditions, which will be given below, have also to be satisﬁed. The kinematic velocity ﬁeld is obtained from the following assumptions. There are two subdomains I and III, of V where the material is assumed to be in a rigid state and moving with velocity v0 k and vf k, respectively. Thus the incompressibility condition yields the following relationship between v0 and vf : vf (R22 − R32 ) = v0 (R12 − R32 ) .

(7.6.2)

Further it is assumed that in the domain II viscoplastic deformation takes place. In the interior of V the velocity ﬁeld is assumed to be smooth. Thus the surfaces S0 and Sf (the rigid-viscoplastic interfaces) are continuity surfaces for the velocity ﬁeld. We assume also that the melted glass forms a dead zone, the billet-melted glass interface surface, denoted by S4 , is a ﬂow surface (ﬂow line tube) which can be considered to be a surface of velocity discontinuity. The shape of this surface changes during the extrusion process. Finally we assume that the plug-billet interface S3 is also a ﬂow surface. On these surfaces friction takes place which will be described by the law: (7.6.3) |tτ | = m IIσ where tτ is the friction stress and 0 ≤ m ≤ 1 is the constant friction factor. On the surfaces Sj (j = 5, . . . , 8) there is a friction between the rigid material and rigid tool surface, while the velocities on S1 and S2 are known and related by Eq. (7.6.2). To solve the problem the velocity ﬁeld and the ram pressure have to be determined. The velocity ﬁeld is chosen from the range of kinematically admissible velocity ﬁelds as being the one for which the functional J(v) related to the Bingham model takes the smallest value. Starting from the equation of the ﬂow lines in V a smooth kinematic admissible velocity ﬁeld is derived which satisﬁes the incompressibility condition, and takes given values on S1 and S2 . This velocity ﬁeld depends on the functions g0 and gf which are involved in the deﬁnition of the surfaces S0 and Sf . The velocity ﬁeld which approximates the real one corresponds to the values g0∗ and gf∗ for which J(v), considered a functional of g0 and gf , takes the smallest value. The ram pressure is obtained from the theorem of power expanded written for the approximate velocity ﬁeld previously determined. The approximate velocity

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

368

dynamic

Dynamic Plasticity

ﬁeld and the ram pressure can be determined numerically only. Since signiﬁcant computing time is involved, several simplifying assumptions concerning the shape of the surfaces S0 and Sf will be made. Thus the functional J(v) is transformed into a real function depending on a certain number of real parameters. The inﬂuence of the working speed on the process (ram pressure, dead zone shape, etc.) is obtained numerically for cases suggested by practical applications, assuming that the mechanical properties of the material, the lubrication conditions and the geometry of the process (i.e., Ri ) are known. 7.6.2

Kinematics of the Process

Due to the axial symmetry of the problem, cylindrical coordinates (r, θ, z) will be used. The equation of the ﬂow surfaces are r = G(z, α)

(7.6.4)

with α ∈ [R3 , R2 ]. The cylindrical surfaces r = α are the ﬂow surfaces in domain III. Let us assume that the surfaces S0 and Sf of equations surfaces are z = Γ0 (r) ,

z = Γf (r)

(7.6.5)

have unique intersections with the ﬂow surfaces α = const. for any α ∈ [R3 , R2 ]. It follows that the equations of these surfaces can be written as function of r = f0 (α) ,

r = ff (α)

(7.6.6)

where f0 yields from the incompressibility condition written in the form v0 [f02 (α) − R32 ] = vf (α2 − R32 ) or

f0 (α) =

R12 − R32 2 (α − R32 ) + R32 R22 − R32

(7.6.7) 1/2 (7.6.8)

if Eq. (7.6.2) is also used. From Eqs. (7.6.5) and (7.6.6) the equations of the surfaces S0 and Sf can be written as z = Γ0 (f0 (α)) ≡ g0 (α) ,

z = Γf (α) ≡ gf (α) .

Thus the equations of the ﬂow surface are f0 (α) , r = G(z, α) ≡ F (z, α) , α,

(7.6.9)

z ≤ g0 (α) g0 (α) ≤ z ≤ gf (α)

(7.6.10)

z ≥ gf (α) ,

for α ∈ [R3 , R2 ]. Since the velocity ﬁeld is smooth in V , the derivative of the function F (z, α), with respect to z must satisfy the conditions lim Fz (z, α) = 0 ,

lim Fz (z, α) = 0 .

z g0 (α)

z gf (α)

(7.6.11)

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

dynamic

Axi-Symmetrical Problems

369

Fα (z, α)Fz (z, α) = 0

(7.6.12)

It will be assumed also that in the interior of II and that it is ﬁnite. Since the inner cylindrical surface of the tube is α = R3 we have F (z, R3 ) = R3

(7.6.13)

for any z ∈ [g0 (α), gf (α)]. From (7.6.12) we conclude that through any point P of II passes a unique ﬂow line. Therefore, the family β = const. of orthogonal lines to the ﬂow lines exists; their equation in the plane (z, r) is Φ(z, r) = β ,

(7.6.14)

with β a real number belonging to a certain interval. The orthogonally condition of the curves (7.6.10) and (7.6.14) is Φz = Fz Φr .

(7.6.15)

Since Φr (z, α) = 0 in II, (7.6.14) can be solved, with respect to r. From (7.6.10) and (7.6.14) written as f1 (z, r; α, β) = r − F (z, α) = 0 ,

(7.6.16)

f2 (z, r; α, β) = Φ(z, α) − β

and using the theorem of implicit functions we get the nonsingular mapping r = u(α, β) ,

z = v(α, β)

(7.6.17)

because 1 + Fz2 Fz is ﬁnite and non-zero in the interior of II. Further the formulae Fα Fα Fz ∂z ∂r = =− , , ∂α 1 + Fz2 ∂α 1 + Fz2 ∆ = Φr

(7.6.18)

(7.6.19)

∂r Fz2 ∂z Fz = , = , ∂β Φr (1 + Fz2 ) ∂β Φr (1 + Fz2 ) yield from Eqs. (7.6.16) and (7.6.17). Thus x = u(α, β) cos θ ,

y = u(α, β) sin θ ,

z = v(α, β)

(7.6.20)

deﬁne a nonsingular mapping from (x, y, z) → (q = α, q = θ, q = β), since the Jacobian " " " ∂z ∂r ∂z ∂r "" √ − (7.6.21) g ≡ r "" ∂α ∂β ∂β ∂α " 1

computed with Eq. (7.6.19)

is non-zero.

" " F (z, α) "" Fα Fz "" √ g= 1 + Fz2 " Φr "

2

3

(7.6.22)

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

370

dynamic

Dynamic Plasticity

In the new system of coordinates the incompressibility condition is 3 1 ) ∂ √ i ( gv ) = 0 div v = √ g i=1 ∂q i

(7.6.23)

with v i the contravariant components of the velocity. Since q 1 = α = const. are ﬂow lines it yields v = v β eβ

(no summation)

with eβ directed along the ﬂow lines in the ﬂow sense. From Eqs. (7.6.23) and (7.6.24) and the axial symmetry we get √ β gv = C(α) .

(7.6.24)

(7.6.25)

The function C(α) is determined from the condition lim r=F (z,α) zg0 (α)

v(r, z) = v0 k .

Thus the kinematic velocity ﬁeld considered is C(α) ∂r ∂z eβ ir + k , v = C(α) √ = √ g g ∂β ∂β

(7.6.26)

(7.6.27)

where ir and k are unit vectors (see Fig. 7.6.1). By inverting the relations (7.6.17) and using (7.6.21) we get r ∂z ∂α = √ , ∂r g ∂β

∂α r ∂r = −√ . ∂z g ∂β

(7.6.28)

From (7.6.27) and (7.6.24) the components of the kinematic velocity ﬁeld in the cylindrical coordinates are ∂α ∂α 1 1 vr = − C(α) , vθ = 0 , vz = C(α) , (7.6.29) r ∂z r ∂r where α is considered to be a function of z and r according to Eq. (7.6.10): α = H(z, r)

(7.6.30)

so that r = F (z, H(z, r)). To get the explicit expression of C(α) involved in Eqs. (7.6.26) and (7.6.27) the following limits are necessary: from (7.6.19)1 and (7.6.11)1 yields ∂r = Fα (g0 (α), α) , r=F (z,α) ∂α

∂z = 0; r=F (z,α) ∂α

zg0 (α)

zg0 (α)

lim

lim

(7.6.31)

from (7.6.19)2 , (7.6.22) and (7.6.11)1 we have lim sign(Φr Fz )r=F (z,α) 1 ∂z zg0 (α) = lim √ g ∂β F (g0 (α), α)|Fα (g0 (α), α)| r=F (z,α) zg0 (α)

(7.6.32)

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

dynamic

Axi-Symmetrical Problems

371

1 ∂r = 0. √ g ∂β r=F (z,α)

(7.6.33)

and lim

zg0 (α)

Thus C(α) = v0 F (g0 (α), α)|Fα (g0 (α), α)| .

(7.6.34)

Using (7.6.34) in (7.6.29) and (7.6.10) the kinematic velocity ﬁeld expressed as a function of z, r is vr = −v0 f0 (α)|Fα (g0 (α), α)| vz = v0 f0 (α)|Fα (g0 (α), α)|

1 ∂α , r ∂z

∂α , ∂r

(7.6.35)

vθ = 0 , with α = H(z, r). By diﬀerentiation of Eq. (7.6.10) ∂α 1 = , ∂r Fα (z, α)

∂α Fz (z, α) = , ∂z Fα (z, α)

(7.6.36)

is obtained. From (7.6.36), (7.6.35) and (7.6.10), another form of the velocity ﬁeld, this time as function of z and α, can be obtained vr =

v0 f0 (α) |Fα (g0 (α), α)| Fz (z, α) , F (z, α) Fα (z, α)

vz =

v0 f0 (α) |Fα (g0 (α), α)| , F (z, α) Fα (z, α)

(7.6.37)

vθ = 0 . The previous formulae will be written in a particular form for the case when the ﬂow lines are sinusoidal lines, deﬁned by r = F (z, α) = A(α){sin[a(α)z + b(α)] + 1} + α ,

(7.6.38)

with 1 [f0 (α) − α] , 2 where a(α) and b(α) are determined by (7.6.11) as A(α) =

a(α) =

π , gf (α) − g0 (α)

b(α) =

π gf (α) − 3g0 (α) . 2 gf (α) − g0 (α)

(7.6.39)

(7.6.40)

Condition (7.6.13) is satisﬁed since (7.6.8) yields A(R3 ) = 0. Formulae (7.6.38) to (7.6.40) yield vf α . (7.6.41) F (g0 (α), α) = f0 (α) ≡ v0 f0 (α)

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

372

dynamic

Dynamic Plasticity

In this particular case the velocity ﬁeld is written as α ∂α α ∂α , vz = vf , vθ = 0 , (7.6.42) r ∂z r ∂r with α = H(z, r) obtained from Eq. (7.6.39) by inversion, with respect to α. In what follows we will need the expression of the second invariant IID in cylindrical coordinates, which, using the incompressibility condition, becomes vr = −vf

2 2 2 IID = Drr + Dθθ + Drz + Drr Dθθ .

(7.6.43)

The components of the rate of deformation tensor corresponding to the ﬁeld (7.6.42) are α ∂α α ∂ 2 α 1 ∂α − 2 + , Drr = −vf r ∂r r ∂z r ∂r∂z α ∂α , r2 ∂z & 2 2 ∂α ∂2α 1 vf ∂2α ∂α α ∂α −α 2 . =− +α 2 − + 2 r ∂z ∂z ∂r r ∂r ∂r

Dθθ = −vf Drz

(7.6.44)

In forming the partial derivatives of the function α = H(z, r), (7.6.38) is used. Thus the second invariant IID can be considered either as a function of z and r if α = H(z, r) is used, or a function of z and α if r is represented by F (z, α). The latter version will be used further on. 7.6.3

The Approximate Velocity Field

The functional attached to the Bingham model, for the case considered here is ) ) IID dV + 2k IID dV − t · v dσ + t · [v] dσ , J(v) = 2η V

V

j

Sj

i

Si

(7.6.45) where Sj with j = 2 and 5–8 are the surfaces on which the velocity is prescribed and Si with i = 3, 4 are the discontinuity surfaces for the velocity ﬁeld and on which it is assumed that the stress vector t is known. The approximate velocity ﬁeld for the extrusion problem is determined by minimizing on the kinematical velocity ﬁeld (7.6.42) using (7.6.38) to form the appropriate expression of J(v) [in the sense that in this functional on surfaces S4 and S3 the stress vector is replaced by Eq. (7.6.3)]. On the family of kinematic admissible velocity ﬁelds J becomes a functional of g0 and gf . The values g0∗ and gf∗ for which J takes the smallest value deﬁne the approximate solution of the problem. The geometry of the viscoplastic domain is known if the surfaces S4 , S0 and Sf are known. The volume integrals from (7.6.45) are calculated with (7.6.43) and (7.6.44) by assuming that IID depends on α and z alone. Passing from the variables (z, r, θ) to (z, α, θ) with r = F (z, α), we obtain for instance for the ﬁrst integral

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

dynamic

Axi-Symmetrical Problems

R2

gf (α)

IID dV = 2π V

IID (z, α)F (z, α)|Fα (z, α)| dzdα . R3

373

(7.6.46)

g0 (α)

On the boundaries S3 and S4 the tangential component of the stress vector, according to (7.6.3) is given by (7.6.47) |tτ | = mi IIσ = mi 2η( IID + k) , where mi (i = 3, 4) is the constant friction factor on the corresponding surface. The equation of the surface S4 deﬁned by α = R2 is x = F (z, R2 ) cos θ , y = F (z, R2 ) sin θ ,

(7.6.48)

z = z, with θ ∈ [0, 2π] and z ∈ [g0 (R2 ), gf (R2 )]. The element of area is dσ = F (z, R2 ) 1 + Fz2 (z, R2 ) dθdz . The velocity ﬁeld is tangent to the surface S4 and from (7.6.42) yields 2 2 R2 ∂α ∂α + , |vτ | = vf F (z, R2 ) ∂r ∂z

(7.6.49)

(7.6.50)

where ∂α/∂r and ∂α/∂z are computed with (7.6.36). Thus from (7.6.47)–(7.6.49), the integral on S4 is obtained with gf (R2 ) 1 + Fz2 (z, R2 ) dz . t · v dσ = −2πm4 vf R2 (2η IID (z, R2 ) + k) |Fα (z, R2 )| S4 g0 (R2 ) (7.6.51) On the cylindrical surface S3 (α = R3 ) the velocity is tangent to the surface and from (7.6.42), (7.6.36) and (7.6,13) we get the relative velocity between the billet and the plug: v0 1 − k. (7.6.52) v3 = vf Fα (z, R3 ) vf The integral over S3 is computed with (7.6.47) and (7.6.52) as gf (R3 ) t · v dσ = −2πm3 R3 (2η IID (z, R3 ) + k)|v3 | dz . S3

(7.6.53)

g0 (R3 )

The integral over S2 is zero since this surface is stress free. On the surface Sj with j = 5–8 friction between rigid tool walls and billet takes place and is prescribed by the law |tτ | = mj τj

(no summation) ,

(7.6.54)

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

374

dynamic

Dynamic Plasticity

where τj is the constant shearing yield stress of the material along the wall Sj . The law (7.6.54) is a particular version of (7.6.3). Denoting by Lj the length of the cylindrical surfaces Sj , the integrals over these surfaces are t · v dσ = −2πm5 L5 τ5 R1 v0 , S5

t · v dσ = −2πm7 L7 τ7 R2 vf ,

(7.6.55)

S7

t · v dσ = −2πm8 L8 τ8 R3 |vf − v0 | , S8

while the integral on S6 is zero. With the expression of all these integrals, the functional which has to be minimized, with respect to g0 and gf becomes R2 gf (α) (ηIID + k IID )F (z, α)|Fα (z, α)| dzdα J(v) = 4π R3

g0 (α)

+ 2πm5 L5 τ5 R1 v0 + 2πm7 L7 τ7 R2 vf + 2πm8 L8 τ8 R3 |vf − v0 | " " gf (R3 ) " 1 v0 " + 2πm3 R3 vf − "" dz (2η IID (z, R3 ) + k) "" Fα (z, R3 ) vf g0 (R3 )

gf (R2 )

+ 2πm4 R2 vf

(2η

IID (z, R2 ) + k)

g0 (R2 )

1 + Fz2 (z, R2 ) dz , |Fα (z, R2 )|

(7.6.56)

where F (z, α) given by (7.6.38) depends on g0 and gf . 7.6.4

The Extrusion Pressure

The extrusion pressure is determined from the theorem of power expanded σ · D dV = t · v dσ (7.6.57) V

S

with S=

8 -

Sj

j=1

and in which the internal dissipation and those on various surfaces are computed for the approximate velocity ﬁeld already determined. The dissipation on the surface S1 is t · v dσ = π(R12 − R32 )v0 p (7.6.58) S1

in which p is the extrusion pressure.

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

dynamic

Axi-Symmetrical Problems

375

For the Bingham model (7.6.1) the stress power is σij Dij dV = 4η IID dV + 2k IID dV V

V

(7.6.59)

V

with the volume integrals calculated according to the same procedure as for (7.6.46). Taking into account in (7.6.57) the integral on S1 as given by (7.6.58), the integral on S4 and S5 furnished by (7.6.51) to (7.6.53), the integrals on S5 , S7 and S8 given by (7.6.55) (the integrals on S2 and S6 are zero) we get the ram pressure 1 1 p= 2 2 R1 − R3 πv0

σ · D dV + 2m3 R3

V gf∗ (R2 )

gf∗ (R3 )

g0∗ (R3 )

(2η

IID (z, R3 ) + k)|v3 | dz

1 + Fz2 (z, R2 ) dz |Fα (z, R2 )| g0∗ (R2 ) vf vf + 2m5 L5 τ5 R1 + 2m7 L7 τ7 R2 + 2m8 L8 τ8 R3 −1 . v0 v0 + 2m4 R2

vf v0

(2η

IID (z, R2 ) + k)

(7.6.60)

In this formula g0∗ and gf∗ are the functions which deﬁne the surfaces S0 and Sf . From (7.6.60) the ram pressure can be determined if either the velocity of the ram or the velocity vf at the exit of the container is known. The value of the extrusion pressure depends on the parameters deﬁning the geometry (Rj , g0∗ and gf∗ ), on the mechanical properties of the billet (η and k), on the friction factors (mi ) on various interface surfaces, and certainly on v0 or vf . The mechanical parameters and the friction conditions are strongly temperature dependent. 7.6.5

Numerical Examples

In order to determine numerically the ram pressure and the inﬂuence of the working velocity on this pressure, we have to ﬁnd ﬁrst g0∗ and gf∗ . Since signiﬁcant computing time is necessary in order to ﬁnd g0∗ and gf∗ by minimizing the functional J, simplifying assumptions concerning the shape of these surfaces are necessary. These simpliﬁcations, suggested by experimental evidence, must keep the formulae involved in the problem as simple as possible. In a ﬁrst particular case the surfaces S0 and Sf are assumed to be conical, i.e., straight lines in the symmetry plane. These straight lines pass trough the points Q(0, R2 ) and P (−L, R1 ), respectively r − R1 = m0 (z − L) r − R2 = mf z .

(7.6.61)

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

376

dynamic

Dynamic Plasticity

If m0 and mf are ﬁnite, (7.6.61) and (7.6.6) yield α − R2 ≡ gf (α) = z mf f0 (α) − R1 + m0 L ≡ g0 (α) = z . (7.6.62) m0 With these expressions for g0 and gf the functional J becomes a function of the real parameters γ0 , γf and L. These parameters may vary in the intervals R1 R2 , π , γf ∈ arctan ,π , (7.6.63) L ∈ (0, l) , γ0 ∈ arctan L0 L0 where l is the initial length of the billet, m0 = tan γ0 and mf = tan γf . Another case in which simpliﬁcations are possible is the one in which it is assumed that gf (α) − g0 (α) = L .

(7.6.64)

Equations (7.6.40), (7.6.41) and (7.6.64) then yield π 2g0 (α) π 1− a= , b= L 2 L in which the function g0 and the real parameter L are arbitrary. In another particular case we can assume that g0 and gf are chosen so that the surfaces S0 and Sf are circles in the plane of symmetry: for instance circles with centers at the points C0 (Z0 , R0 ) and Cf (Zf , Rf ) and passing through P and Q, respectively. Then we have % z = Z0 − ρ20 − [f0 (α) − R0 ]2 ≡ g0 (α) z = Zf −

% (R2 − Rf )2 + Zf2 − (α − Rf )2 ≡ gf (α) .

(7.6.65)

In this case the real parameters on which the function J depends are R0 , Z0 , ρ0 , Rf and Zf . Some combinations of the particular cases given above can be imagined. The mechanical properties of the billet at high temperatures are described by choosing appropriate values for the viscosity coeﬃcient η and the mean yield stress k. In the numerical examples we have taken into account the dependence of η on the mean rate of deformation Dm deﬁned by 2 2 1 ¯ D = √ Dm = √ IID dV , (7.6.66) 3 3V V ¯ is computed for each particular where V is the volume of the viscoplastic domain. D ¯ case of extrusion considered. From the graphical plot of the function η = η(D) obtained from experimental data, the corresponding value of the viscosity coeﬃcient is obtained.

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Axi-Symmetrical Problems

dynamic

377

For high temperatures the value of k was determined from uniaxial experiments. The geometry of the extrusion process will be characterized by the reduction in area R2 − R32 (7.6.67) r% = 100 1 − 22 R1 − R32 and the geometry of the billet. In the numerical examples given below the data for steel AISI 304 as given by Polukhin et al. [1976] have been used. Thus for the temperature range of 1100– √ ◦ −2 1200 C, the mean yield stress is k = 3.5 kgf mm and σY f = 3τ7 = 8 kgf mm−2 . For the working speed v0 ranging between 200 mm s−1 and 400 mm s−1 and ¯ takes values between 38.12 s−1 and 58.40 s−1 . reductions of 96.14% and of 97%, D The corresponding values for η are 2.2 × 106 Poise and 1.5 × 106 Poise. For the reduction mentioned, the radii Ri are: R1 = 74 mm, R2 = 28.5 mm, R3 = 25 mm and R1 = 74 mm, R2 = 23.5 mm, R3 = 20 mm, respectively. On the billet-plug and billet-container interfaces, the lubricant used is powdered glass, which at high pressure and temperature melts forming a thin ﬁlm with the thickness of a few microns (5–17 µm). On the surface S4 the interface between the melted glass and the billet, the friction factor is very small. From the experimental data by Maneghin et al. [1980] the friction factor at all surfaces lubricated by melted glass was taken m = 0.02 and in one single case m = 0.04. For the particular shape of the surfaces S0 and Sf described by formulae (7.6.62) the numerical values of the parameters γ0 , γf and L for which the functional J(v) — now a function J(L, γ0 , γf ) of real variables — takes a minimal value, have been determined. This is done for various prescribed values of v0 , various geometries of the billet and product, prescribed mechanical properties of the metal and those of the lubricant, by a trial and error procedure. Then the value of L for which the function J(L, γ0 , γf ) has a minimum is found. With this value of L, the parameter γ0 is varied and its value which minimizes J is found. We return now and with this new value of γ0 kept constant vary again L, etc. After several iterations the parameter γf is varied also. The ﬁnal values of the tree parameters obtained by this trial and error procedure are denoted by (L∗ , γ0∗ , γf∗ ). We start with prescribed values of γ0 and γf in the neighborhood of 90◦ . On Fig. 7.6.2 for v0 = 300 mm s−1 is shown the dependence of J(L, γ0∗ , γf∗ ) on L for ﬁxed values of γ0∗ and γf∗ . The dependence of J(L∗ , γ0 , γf∗ ) on γ0 is shown on Fig. 7.6.3 while that of J(L∗ , γ0∗ , γf∗ ) on γf is on Fig. 7.6.4. If the reduction in area is increased by a few per cent the minimum value of J increases. The values of γ0∗ and γf∗ do not change signiﬁcantly but the value of L∗ increases when reduction is increased. With an increase of the friction factor, the minimum value of J increases, L∗ slightly increases but γ0∗ and γf∗ are practically the same. For each ﬁxed value of v0 , geometry conditions, mechanical proprieties and lubrication conditions, using the determined values of L∗ , γ0∗ , γf∗ , the ram pressure is

January 12, 2007

378

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Dynamic Plasticity

Fig. 7.6.2 Dependence of functional J on the length L for various reductions and friction factors, showing the minimum.

Fig. 7.6.3 Dependence of functional J on angle γ0 , for various reductions and friction factors, showing the minimum.

dynamic

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Axi-Symmetrical Problems

Fig. 7.6.4

dynamic

379

Dependence of functional J on the angle γf ; the minimum is close to 90◦ .

Fig. 7.6.5 The inﬂuence of working speed on the length L of the viscoplastic domain and on the extrusion pressure.

obtained from formula (7.6.60). On Fig. 7.6.5 is shown the working speed inﬂuence on the extrusion pressure: the extrusion pressure increasing with increasing v0 . The inﬂuence of v0 on L∗ is also shown on this ﬁgure: L∗ increases signiﬁcantly with v0 . The signiﬁcant increase of L∗ with v0 is accompanied by an increase of the volume Vg of the melted glass. It has been shown that the geometry of the viscoplastic domain, and therefore of the melted glass, is strongly dependent on the working speed. During the extrusion process, the melted glass is a self-adjusting die. A control volume of the melted glass during extrusion may ensure the optimal working conditions.

January 12, 2007

10:41

380

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Dynamic Plasticity

Bibliography Abou-Sayed A. S. and Clifton R. J., 1976, Pressure shear waves in fused silica, J. Appl. Phys. 47, 5, 1762–1770. Abou-Sayed A. S. and Clifton R. J., 1977a, Analysis of combined pressure-shear waves in an elastc/viscoplastic material, J. Appl. Mech. Trans. ASME 44, 79–84. Abou-Sayed A. S. and Clifton R. J., 1977b, Pressure-shear waves in 6061-T6 aluminum due to oblique-plate-impact, J. Appl. Mech. Trans. ASME 44, 1, 85–88. Alexandrov S. and Alexandrova N., 2000, On the maximum friction law in viscoplasticity, Mech. Time-Dependent Materias 4, 99–104. Angelov T. A., 2004, Variational analysis of a rigid-plastic roling problem, Int. J. Engng. Sci. 42, 1779–1792. Avitzur B., 1968, Metal Forming: Processes and Analysis, McGraw-Hill, New York. Bernstein B. and Shokooh A., 1980, J. Rheology 24, 2, 189–211. Bisk M. B. and Shveikin V. V., 1963, Tube drawing with ﬂoating plugs, Metalurgya, Moscow (in Russian). Blazynski T. Z., 1976, Metal Forming. Tool Proﬁles and Flow, Macmillan, London. Bramley A. N. and Smith D. J., 1976, Metals Technology, 322. Camenschi G. and S ¸ andru N., 2003, Mathematical Models in Metal Working, Bucharest, 188 pp. (in Roumanian). Camenschi G., Cristescu N. and S ¸ andru N., 1979, High speed wire drawing, Archives of Mechanics 31, 5. Camenschi G., Cristescu N. and S ¸ andru N., 1983, Developments of high speed viscoplastic ﬂow through conical converging dies, Trans. ASME, J. Appl. Mech. 50. Campbell J. D., 1973, Dynamic plasticity — macroscopic and microscopic aspects, Materials Science and Engineering 12, 1, 3–21. Chhabildas L. C. and Swegle J. W., 1980, Dynamic pressure-shear loading of materials using anisotropic crystals, J. Appl. Phys. 51, 9, 4799–4807. Cleja S. and Cristescu N., 1979, Inﬂuence of the drawing speed on the optimum shape of the ﬂoating plug, Rev. Roum. Sci.-Mec. Appl. 24, 3, 357–377. Cleja-Tigoiu S. and Cristescu N., 1985, A ﬂow analysis of rigid-viscoplastic body through annular oriﬁce, Int. J. Mech. Sci. 27, 5, 291–301. Clifton R. J., 1968, Elastic-plastic boundaries in combined longitudinal and torsional plastic wave propagation, J. Appl. Mech. Trans. ASME 35, 4, 782–786. Cristescu N., 1956, Some remarks concerning the case of plane axial symmetrical deformation in dynamic problems of plasticity, Comm. Acad. Rep. Pop. Rom. 6, 19–28 (in Romanian). Cristescu N., 1967, Dynamic Plasticity, North-Holland Pub. Co., 614 pp. Cristescu N., 1975, Plastic ﬂow through conical converging dies, using a viscoplastic constitutive equation, Int. J. Mech. Sci. 17, 425–433. Cristescu N., 1976, Drawing through conical dies — an analysis compared with experiments, Int. J. Mech. Sci. 18, 45–49. Cristescu N., 1977, Speed inﬂuence in wire drawing, Rev. Roum. Sci. Techn. Mec. Appl. 22, 3, 391–399. Cristescu N., 1980, On the optimum die angle in fast wire drawing, J. Mech. Working Tech. 3, 275–287. Dahan N. and Le Nevez P., 1983, M´ethode de calcul des grandes d´eformations plastiques et endommagement dans les pi`eces extrudees, M´emoire et Etudes Scientiﬁques Revue de M´etallurgie 80, 10, 557–566.

dynamic

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Axi-Symmetrical Problems

dynamic

381

Frutschy K. J. and Clifton R. J., 1997, High-temperature pressure-shear plate impact experiments using pure tungsten carbide impactors, Experimental Mechanics 38, 2, 116–125. Frutschy K. J. and Clifton R. J., 1998, High-temperature pressure-shear plate impact experiments on OFHC copper, J. Mech. Phys. Solids 46, 19, 1723–1743. Fu M. and Luo Z. J., 1995, The simulation of the viscoplastic forming process by the ﬁnite element method, J. Materials Process. Tech. 55, 442–447. Gilat A. and Clifton R. J., 1985, Pressure-shear waves in 6061-T6 aluminum and alpha titanium, J. Mech. Phys. Solids 33, 3, 263–284. Gilman J. J. and Tuler F. R., 1970, Dynamic fracture by spallation in metals, Int. J. Fracture Mech. 6, 2, 169–182. G¨ uldenpfennig J. and Clifton R. J., 1980, Plastic waves of combined stress based on self consistent slip models, J. Mech. Phys. Solids 28, 3–4, 201–219. Hartley C., 1971, Int. J. Mech. Sci. 17, 651–663. Heeres O. M., Suiker A. S. J. and de Borst R., 2002, A comparison between the Perzyna viscoplastic model and the Consistency viscoplastic model, Europ. J. Mech. A/Solids 21, 1–12. Hsu J. C. C. and Clifton R. J., 1974a, Plastic waves in a rate sensitive material-I. Waves of uniaxial stress, J. Mech. Phys. Solids 22, 233–253. Hsu J. C. C. and Clifton R. J., 1974b, Plastic waves in a rate sensitive material-II. Waves of combined stress, J. Mech. Phys. Solids 22, 255–266. Ioan S. and Ioan R., 1999, A mathematical model of bimetallic tube drawing with ﬂoating plug, Rev. Roum. Sci. Tech.-Mec. Appl. 44, 1, 49–72. Iddan D. and Tirosh J., 1996, Analysis of high-speed rolling with inertia and rate eﬀects, J. Appl. Mech. Trans. ASME 63, 27–37. Ionescu I. R. and Vernescu B., 1988, A numerical method for viscoplastic problem. An application to wire drawing, Int. J. Engng. Sci. 26, 6, 627–633. O’Keefe J. D., Skeen C. H. and York C. M., 1973, Laser-induced deformation modes in thin metal targets, J. Appl. Phys. 44, 10, 4622–4626. Kim K. S. and Clifton R. J., 1980, Pressure-shear impact of 6061-T6 aluminum, J. Appl. Mech. 47, 1, 11–16. Kim Y. H., Ryou T. K., Choi H. J. and Hwang B. B., 2002, An analysis of the forging processes for 6061 aluminum-alloy wheels, J. Materials Process. Tech. 123, 279–276. Klopp R. W. and Clifton R. J., 1990, Analysis of tilt in the high-strain-rate pressure-shear plate impact experiment, J. Appl. Phys. 67, 11, 7171–7173. Li G. J. and Kobayashi S., 1982, Rigid-plastic ﬁnite-element analysis of plane-strain roling, ASME, J. Eng. for Industry 104, 1, 55–64. Lindholm U. S. and Bessey R. L., 1969, A survey of rate dependent strength properties of metals, Rept. AFML-TR-69-119. Mandel J., 1974, Introduction a la mecanique des milieux continues deformables, PWN, Warszawa. Maneghin I. V., Pritomanov A. E., Shpittel T. and Knauschner A., 1980, Hot extrusion of tubes and proﬁles, Metallurgya, Moscow (in Russian). Manjoine M. J., 1944, The inﬂuence of rate of strain and temperature on yield stresses in mild steel, J. Appl. Mech. 66, A-211. Medvedev M. I., Laskutov P. A. and Ratner A. G., 1980, Metallurgya, Moscow (in Russian). Meir G. and Clifton R. J., 1986, Eﬀects of dislocation generation at sursaces and subgrain boundaries on precursor decay in high-purity LiF., J. Appl. Phys. 59, 1, 124–148.

January 12, 2007

382

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Dynamic Plasticity

Myers C. D. and Eisenberg M. A., 1974, The eﬀect of radial inertia on combined plastic stress wave propagation in thin-walled tubes, J. Appl. Mech. Trans. ASME 41, 3, 619–624. Myers C. D. and Eisenberg M. A., 1975, The eﬀect of radial inertia on the plastic stress wave speeds in thin-walled tubes under combined stress, Acta Mechanica 22, 163–170. Nowachi W. K., 1974, Stress Waves in Non-Elasic Solids, Pergamon Press, Oxford. Perlin I. A., 1957, Drawing Theory, Metalurghizdat (in Russian). Perzina P., 1966, Fundamental problems in viscoplasticity, Advances in Appied Mechanics, Academic Press, New York, 9, 243–377. Polukhin P. I., Gun G. Y. and Galkin A. M., 1976, Plastic deformation strength of metals and alloys, Reference Book, Metallurgya, Moscow (in Russian). S ¸ andru N. and Camenschi G., 1979, Viscoplastic ﬂow through inclined planes with applications to the strip drawing, Lett. Appl. Engng. Sci. 17, 773–784. S ¸ andru N. and Camenschi G., 1988, Mathematical model of the tube drawing with ﬂoating plug, Int. J. Engng. Sci. 26, 6, 567–585. Shida S. and Awazuhara H., 1973, J. Japan Soc. Tech. Plasticity 14, 267–272. Sokolovski V. V., 1969, Theory of plasticity, Iz. Vashaia Skola (in Russian). Tanimura S., Igaki H., Majima H. and Tada M., 1978, Combined tension–torsion impact testing apparatus and an experimenal study in the incremental wave propagation, Bulletin of the JSME 21, 160, 1455–1461. Tayal A. K. and Natarajan R., 1981, Extrusion of rate-sensitive materials using a viscoplastic constitutive equation and the ﬁnite element method, Int. J. Mech. Sci. 23, 89–98. Ting T. C. T., 1970, Elastic-plastic boundaries in the propagation of plane and cylindrical waves of combined stress, Quart. Appl. Math. 27, 4, 441–449. Ting T. C. T., 1973, On wave propagation problems in which cf = cs = c2 occurs, Quart. Appl. Math. 31, 3, 275–286. Ting T. C. T., 1977, Plastic wave speeds in isotropically work-hardening materials, J. Appl. Mech. Trans. ASME 44, 1, 68–72. Tirosh J. and Kobayeski S., 1976, Kinetic and dynamic eﬀects on the upper-bound loads in metal-forming processes, J. Appl. Mech. Trans. ASME 43, 2, 314–318. Tirosh J., Iddan D. and Pawelski O., 1985, The mechanics of high-speed rolling of viscoplastic materials, J. Appl. Mech. Trans. ASME 52, 309–318. Tobe T., Kato M. and Obara H., 1979, Metal forming by underwater wire explosion 1. An analysis of plastic deformation of circular membranes under impulsive loading, Bulletin JSME 22, 164, 271–278. Upadhyay P. C. and Stokes V. K., 1977, On the dynamic expansion of a circular hole in an inﬁnite plate, J. Appl. Mech. Trans. ASME 44, 577–582. Wistreich J. G., 1955, Proc. Inst. Mech. Engng. London 169, 654. Yew C. H. and Richardson H. A. Jr., 1969, Strain-rate eﬀect and incremental plastic wave in copper, Exp. Mech. 9, 8, 366–373. Yokoyama T., 2001, Finite element computation of torsional plastic waves in a thin walled tube, Archive of Appl. Mech. 71, 6–7, 359–370.

dynamic

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

Chapter 8

Plastic Waves. Perforation

8.1

Introduction

Problems of plastic waves were considered by a lot of authors from variety points of view. Some restrictive relations for possible constitutive equations are due to B´eda [1997]. Problems of plastic waves, problems of perforation etc. were considered; for a review of the subject see Davids [1960], Shewmon and Zackay [1961], Kolsky and Prager [1964], Cristescu [1967], Campbell [1972], Burke and Weiss [1971], Ezra [1973], Rinehart [1975], Cristescu et al. [2003], Zukas [2004] and the papers Backman and Goldsmith [1978], Zhu et al. [1992], Fomin and Kiselev [1997], Cheeseman and Bogetti [2003]. Chernyshov [1966] has shown that the structure of shock waves is practically the same as for gases. A suﬃcient condition is established by Lee [1975] for uniqueness of the dynamic path of an elastic-plastic body subject to prescribed kinematic boundary conditions on a part of the surface and prescribed time-dependent Lagrangian tractions on the remainder. The problems considered until now are of some importance for civil engineering, mechanical engineering, seismology, military applications, etc. The history of soil history is older than that of theory of plasticity. In the last times the theory of plasticity has developed faster, since the experimental facts are easier than in the soils or rock mechanics. Also it is more diﬃcult to interpret the results of soil and rock mechanics. While the plastic deformation in metallic bodies is studied in more than half a century, the experiments with soils and rock mechanics are done only in the last decades. The physics is also quite complex: the soils is considered a continuous medium where solid bodies, ﬂuids and gas are mixed together in a complex manner in what is called a three-phase medium. Sometimes one of these tree medium is absent and the body becomes a two-phase medium. If α1 , α2 , α3 denote the relative proportions by volume of gas, liquid and solid constituents of the soil, so that α1 + α2 + α3 = 1 , (8.1.1) 3 and if ρ1 , ρ2 and ρ3 are the corresponding densities (in g/cm ), the density ρ of the soil considered as a three-phase medium will be ρ = α1 ρ1 + α2 ρ2 + α3 ρ3 . (8.1.2) 383

dynamic

January 12, 2007

10:41

384

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

dynamic

Dynamic Plasticity

The density of air is ρ1 = 1.2 × 10−3 g/cm3 of water ρ2 = 1 g/cm3 , while for the solid an average value ρ3 = 2.65 g/cm3 is used. One is introducing also the concept of porosity as the ratio between the volume of the pores and that of the soil itself. Various constitutive equations have been established for soils and rocks (see Ch. 2). Sometimes Eulerian methods were used since “big” strains are involved. In hydrostatic tests the compressibility of the soil is considered. The compaction property is highly dependent on the water content of the body and is diﬀerent under dynamic and static loadings. In static experiments it is the solid skeleton of the body that generally supports most of the pressure if the sample is drained, because there is suﬃcient time for the water to drain away from the pores during the experiment. In dynamic experiments the situation is quite diﬀerent. The mixture of water and air, if the sample is drained, there is not suﬃcient time for the water to escape during a dynamic experiment. In dynamic loading experiments it is the water–air mixture that supports most of the applied pressure. However if the water–air mixtures, the total volume of air is larger than that of the water, then the mixture is much more compressible than the solid skeleton: in these cases the skeleton supports most of the pressure. For very high pressures however, skeleton compressibility plays an important role in the overall compressibility of the body. 8.2

Various Theories

In the previous sections we have discussed the laws of variation of the volume as well as various possible critical stress conditions. In the present section we present several old stress–strain relations which have played a role in the development of the theory. They are very similar to the classic theories of plasticity. S. S. Grigorian [1959, 1960b, 1967] assumes that the Prandtl–Reuss theory can be used to describe the mechanical properties of soft soils. If vi are the velocity components, and 1 ∂vi ∂vj (8.2.1) + Dij = 2 ∂xj ∂xi are the components of the rate of strain, and xi are the Cartesian coordinates, then the constitutive equations are ˜ dσ ij + λσij , dt where the derivatives are taken in the sense of Jauman ˜ ∂σij dσ ∂σij ij = + vk − Ωik σjk − Ωjk σik , dt dt ∂xk = 2GDij

(8.2.2)

(8.2.3)

and 2Ωij =

∂vi ∂vj − . ∂xj ∂xi

(8.2.4)

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

Plastic Waves. Perforation

dynamic

385

The factor λ in (8.2.2) plays the same role as in classical plasticity theory. The elastic behavior of the material corresponds to λ = 0, and the plastic state to λ > 0. This factor can be expressed in terms of invariants following the usual and summation, we obtain procedure: by multiplying (8.2.2) by σij 4GW ≡ 2Gσij Dij = σij

˜ dσ ij + λσij σij . dt

(8.2.5)

Since IIσ = F (p) and σij

˜ dσ dIIσ ij = , dt dt

it follows from (8.2.5) that λ=

4GW − F (p)(∂p/∂t + vi ∂p/∂xi ) . 2F (p)

(8.2.6)

This formula is used only if

4GW > F (p)

∂p ∂p + vi ∂t ∂xi

,

otherwise λ = 0. To the constitutive equation one is adding the equation of motion and the continuity equation. The Prandtl–Reuss constitutive equation is proposed for dynamic problems for soils since soils being dispersed media, there is not a single reference conﬁguration for them. The system of equation was analyzed also from the thermodynamic point of view. There are three functions (Grigorian [1960a]) to be determined from tests: p = f (ρ, ρm , H) ,

Hσ = F (p, H) ,

G = G(ρm , H) .

(8.2.7)

Here H is the humidity, i.e., the ratio between the volume of the water and that of the mineral particles, per unit mass of soil. Since in dynamic problems there is no time for water to drain away from the pores dH/dt = 0. If H = Hmax , that is the soil is fully saturated, in dynamic experiments such soils behave as barotropic liquids. Thus for small or moderate values of H the soil is irreversible compressible. The other functions involved in (8.2.7) are determined as usual for compressible materials. The Coulomb ﬂow rule was used by Chadwick et al. [1964], as associated ﬂow rule. They have assumed that the soil obeys Hooke’s law within the elastic range and the Coulomb’s criterion and the associated ﬂow rule during yielding under the restriction of perfectly plastic ﬂow. According to the rule mentioned, if f (σij ) = 0 denotes the yield function and the elastic domain corresponds to f < 0, then the plastic part of the rate of strain is furnished by ∂f ε˙pij = λ˙ , ∂σij

(8.2.8)

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

386

dynamic

Dynamic Plasticity

˙ where λ(x, t) is a scalar function satisfying the condition λ ≥ 0. The elastic strain rates satisfy a Hookean law. The authors consider only spherical-symmetry problems and therefore spherical polar coordinates r, θ, ϕ are used. The principal components of the stress are σr , σθ and σϕ . If ∂v v , ε˙θ = ε˙ϕ = ∂r r are the components of the strain rate then the associated ﬂow rule is ∂f ∂f ∂f ε˙pr = λ˙ , ε˙pθ = λ˙ , ε˙pϕ = λ˙ , ∂σr ∂σθ ∂σϕ ε˙r =

(8.2.9)

(8.2.10)

where f is one of the six expressions involved in the Coulomb yield condition. At singular points the generalized ﬂow rule proposed by Koiter [1953] and Prager [1953] is used. The “plastic gas” model was considered by Rakhmatulin and Stepanova [1958]. It was used for soils in one-dimensional problems. By deﬁnition a “plastic gas” is a continuous body whose density changes during loading (increasing pressure) according to a prescribed law, while during unloading (decreasing pressure) the density remains constant and equal to the maximum density reached during loading. On repeated loading the density does not change as long as the pressure does not exceed the value reached previously. This model was proposed for the use in problems in which high pressures are involved. Since experiments have shown that for such pressures the temperature rise is negligible, temperature changes are generally disregarded. Very many problems have been solved using the model mentioned above (Rakhmatulin et al. [1964]). Let us see what Sagomonian [1961] has to say about this problem. The problem is one-dimensional and cylindrically symmetrical. In cylindrical Lagrange coordinates r and θ, the equation of motion and the equation of mass conservation are ∂2u ∂σr ∂ + (σr − σθ ) (r + u) , ρ0 r 2 = (r + u) ∂t ∂r ∂r 1 ∂ ρ0 (r + u)2 = r. 2 ∂r ρ Assuming that σr = σθ = −p, the ﬁrst equation becomes

(8.2.11)

r + u ∂p ∂2u . (8.2.12) =− ∂t2 r ∂r The problems to be solved are the following. An inﬁnitely long cylindrical explosive of initial radius r0 is exploded in an inﬁnite medium. It is assumed that the explosion products expand as a polytrophic gas whose adiabatic exponent is γ. Since in most cases the maximum pressure is reached just behind the shock wave front, Sagomonian assumes that the density of the plastic gas changes only on the front (in the transition zone). Thus, behind the shock wave front the density is a function only of r, and the motion is that of a non-homogeneous incompressible medium. ρ0

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

Plastic Waves. Perforation

To the equation (8.2.11) one attaches the law of soil compressibility 1 ρ0 (σr + σθ + σz ) = F 1 − , 3 ρ

dynamic

387

(8.2.13)

and the Coulomb condition is written in the form σr − σθ = −τ0 + µ(σr + σθ )

(8.2.14)

with τ0 = 2k cos ϕ and µ = sin ϕ and assuming that σr > σθ . The ﬁrst case considered is µ = 0, i.e., the case of frictionless soils. The Eq. (8.2.11) becomes ∂ ∂2u ∂σr − τ0 (r + u) , = (r + u) ∂t2 ∂r ∂r or, by formal integration with respect to r, r∗ r ∂2u σr (r, t) = ρ0 dr + τ0 {ln(r + u) − ln R} − pk (t) . 2 r0 r + u ∂t ρ0 r

(8.2.15)

(8.2.16)

Here r0 is the radius of the charge hole at the moment of explosion, pk (t) is the pressure at r = r0 , while the radius of the hole at a certain moment is R(t) = r0 + u(r0 , t). The relation (8.2.16) holds for all points between the hole and the shock wave front. Thus denoting by an asterisk the values of any function on this front, we have r∗ r ∂2u ∗ dr + τ0 {ln r∗ − ln R} − pk (t) . (8.2.17) σr = ρ0 2 r0 r + u ∂t From (8.2.16) and (8.2.17), it follows that r∗ r ∂2u ∗ σr − σr = −ρ0 dr − τ0 {ln r∗ − ln(r + u)} . 2 r0 r + u ∂t

(8.2.18)

If, in (8.2.14) µ = 0, then the ﬁrst equation (8.2.11) becomes (r + u)

∂ ∂2u τ0 ∂ ∂σr + v (r + u)σr = ρ0 r 2 + (r + u) , ∂r ∂r ∂t 1 + µ ∂r

(8.2.19)

with v = 2µ/(1 + µ). By multiplying both sides of (8.2.19) by (r + u)v−1 and integrating with respect to r, we obtain r ∂2u v (r + u) σr (r, t) = ρ0 (r + u)v−1 r 2 dr ∂t r0 +

τ0 1 [(r + u)v − Rv ] − Rv pk (t) . 1+µv

Hence, on the shock wave front we have r∗ ∂2u τ0 1 ∗v (r − Rv ) − Rv pk (t) . (r + u)v−1 r 2 dr + r∗v σr∗ = ρ0 ∂t 1+µv r0

(8.2.20)

(8.2.21)

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

388

dynamic

Dynamic Plasticity

Thus, from the last two formulae it follows that r∗ ∂2u v ∗v ∗ (r + u) σr − r σr = −p0 (r + u)v−1 2 rdr ∂t r τ0 {r∗v − (r + u)v } . v(1 + µ)

−

For cohesionless soils (τ0 = 0) this formula becomes r∗ ∂2u v ∗v ∗ (r + u) σr − r σr = −ρ0 (r + u)v−1 r 2 dr . ∂t r

(8.2.22)

(8.2.23)

As has already been mentioned, it is assumed that the density change occurs only in the transition zone, and therefore, that behind the shock wave front, the density is a function only of the Lagrangiann coordinate r. Thus, from the second equation (8.2.11), by integration with respect to r, it follows that (r + u)2 = 2ψ(r) + ϕ(t) with

r

ψ(r) = r0

ρ0 r¯d¯ r. ρ(¯ r)

(8.2.24)

The arbitrary function ϕ(t) is determined by the boundary conditions r = r0 : ψ(r0 ) = 0 ,

ϕ(t) = {r0 + u(r0 , t)}2 = R2 (t)

so that (r + u)2 = 2ψ(r) + R2 (t)

(8.2.25)

r∗2 = 2ψ(r∗ ) + R2 (t) .

(8.2.26)

or, on the shock wave front

From (8.2.25), we obtain the velocity and acceleration as RR˙ ∂u = , ∂t 2ψ(r) + R2 ¨ ˙ 2 ∂2u R˙ 2 + RR (RR) = − . ∂t2 [2ψ(r) + R2 ]3/2 2ψ(r) + R2

(8.2.27)

Across the shock wave front the jump conditions ρ0 D = ρ(D − u˙ ∗ ) ,

ρ0 Du˙ ∗ = −σr∗ − pa

are satisﬁed. In these conditions, D is the velocity of the displacement of the wave, u˙ ∗ the material velocity just behind the shock front, and pa is the pressure ahead of the shock wave. We therefore obtain dψ 1 ρ0 u˙ ∗2 u˙ ∗ ρ0 ∗ ∗ + pa , D = , b(r ) = = . −σr = 1 − b(r∗ ) 1 − b(r∗ ) ρ(r∗ ) dr r r=r∗ (8.2.28)

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

dynamic

Plastic Waves. Perforation

389

Introducing (8.2.25)–(8.2.28) into (8.2.18), (8.2.22) and (8.2.23), we obtain r∗ r∗ rdr rdr ¨ + R˙ 2 )ρ0 ˙ 2 ρ0 −σr (r, t) = (RR − (R R) 2 2ψ + R (2ψ + R2 )2 r r +

˙ 2 ρ0 (RR) r∗ + pa , + τ ln 0 1 − b r∗2 r+u

¨ + R˙ 2 )ρ0 −(r + u) σr = (RR

r∗

v

r

r

∗

˙ 2 ρ0 − (RR) r

rdr (2ψ + R2 )1−(v/2)

˙ 2 rdr ρ0 (RR) + ∗ 2 2−(v/2) 1 − b (r )2−v (2ψ + R )

τ0 (r∗v − (r + u)v ) + pa r∗v , + v(1 + µ) ¨ + R˙ 2 )ρ0 −(r + u)v σr = (RR r

˙ 2 ρ0 − (RR) r

+

r

∗

(8.2.29)

r∗

(8.2.30)

rdr (2ψ + R2 )1−(v/2)

rdr (2ψ + R2 )2−(v/2)

˙ 2 ρ0 (RR) + pa r∗v . ∗ 1 − b (r )2−v

(8.2.31)

From the relations (8.2.27)–(8.2.31) it follows that all the quantities required to describe the motion can be expressed by two functions, i.e., a function only of the Lagrangean coordinate ψ(r) and another one function only of time R(t). A ﬁrst solution is obtained, assuming that behind the shock wave front the density is a constant ρ1 and that ρ0 /ρ1 = b1 .

(8.2.32)

From (8.2.24) and (8.2.6) it then follows that ψ(r) =

1 b1 (r2 − r02 ) , 2

r∗2 =

R2 (t) − b1 r02 . 1 − b1

(8.2.33)

With this expression for ψ(r), one can compute the integrals in (8.2.29)–(8.2.31) and thus express the solution in terms of the function R(t) and its ﬁrst two derivatives. The case when the density is not constant behind the shock wave front has also been considered by an iterative method. In the same paper by Sagomonian [1961], solutions for the cases of polar symmetry and of the propagation of plane waves were also given. Many other problems were solved using the previously mentioned model for the soils concerned. For instance, the penetration of sharp, rotationally symmetrical bodies into the ground was examined by Rachmatulin et al. [1964] in Ch. IV, where a bibliography of the problem is also given.

January 12, 2007

390

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Dynamic Plasticity

The propagation of spherical collapsing waves which propagate in an elasticbrittle material was studied by Aliev [1963]. The same problem for an elastic-plastic medium, which is incompressible both during loading and unloading and satisﬁes a Tresca yield condition during loading, was considered by Shemiankin [1961]. In another paper, Medvedeva and Shemiankin [1961] have examined the propagation of spherical waves in a medium satisfying a Coulomb yield condition, for a compaction law written in the form n ρ0 , −σ = K 1 − ρ where K and n are positive constants. The model is applied to various rocks. The locking medium was considered by many authors. The main idea is: once the density of the medium reaches a certain limit value, characteristic of the medium, no further density increase is possible. During unloading, the density remains constant and equal to the limiting density. There has also been proposed a model known as an ideal locking medium, which is deﬁned by most authors as follows. The material, of a certain initial density, does not at ﬁrst oﬀer any resistance to compression, but once the limiting density ρ∗ is reached, this remains constant during any subsequent motion and Coulomb’s yield condition is satisﬁed. In a certain sense, the ideal locking medium is a model corresponding to the perfectly plastic/rigid model of plasticity theory. It seems that the idea of locking medium was ﬁrst used in the paper by Ishlinskii et al. [1954] and Salvadori et al. [1955]. These authors start from the experimental observation that if a cylindrical hole some ten meters deep and of diameter 10 to 15 cm is made in a soil (of clay type) and if an explosion is produced in this hole, the density of the soil to a distance of 1 m around the hole increases considerably (approximately 30 per cent). This experiment is described mathematically. Ishlinskii [1954] established the equations of plane motion of certain materials like sand. He made four hypothesis: the medium is non-elastic and incompressible, the stress do not depend on the rate of strain, the directions of principal axes of stresses coincide at each point with the directions of the principal axes of strain, the state of stress satisﬁes the same yield condition as in the static case. The propagation of spherical shock waves in sandy type medium was considered by Kompaneets [1956]. He assumed that initially the medium is of density ρ0 and has a small resistance to shear. When reaching the density ρ1 , the medium becomes incompressible and plastic, and satisﬁes a plasticity condition of the Coulomb form σr − σθ = k + m(σr + σθ + σϕ ) . He also assumes that shock waves are produced by an explosion detonated in a small sphere. Andriankin and Koryavov [1959] consider that the soil compaction along the shock wave front is not constant. They assumed that the compaction produced by the shock wave front depends on the amplitude of the wave; a power law of compaction of the form

dynamic

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Plastic Waves. Perforation

dynamic

391

p = p0 β 1−n εn , is proposed. Here n and β are constants, p0 is the pressure ahead of the wave front and ε = 1 − ρ0 /ρ. A viscous model for plug formation in plates is due to Pytel and Davids [1963]. The paper presents the analysis of a viscous model for the study of impact of plates by projectiles under conditions which would lead to failure of the plate by the formation of a plug. The impact is represented by a velocity uniformly distributed over a circular area on the plate surface. Only the vertical shearing stress is considered and it is assumed to depend only on the radial coordinate. The stress, velocity and displacement proﬁles are calculated for the viscous model. The calculated displacement proﬁles are compared with experimental proﬁles. Spherical elastic-plastic boundaries due to loading were considered by Srinivasan and Ting [1974]. They have considered spherical waves in an elastic-plastic, isotropically work-hardening medium generated by radial stress uniformly applied at a spherical cavity. The radial stress and its time derivative at the cavity may be discontinuous at time t0 . If the applied radial stress is continuous while its time derivative is not, the discontinuity propagates into r > r0 along the characteristics and/or the elastic-plastic boundaries. If the applied radial stress itself is discontinuous, the discontinuity may propagate into r > r0 in the form of a shock wave, or a centered simple-wave, or a combination of both. In any case, the solutions in the neighborhood of (r0 , t0 ) are obtained for all possible combinations of discontinuous loadings applied at r = r0 . This is a systematic study on the nature of the solution near (r0 , t0 ) where the applied load is discontinuous. Solutions for specials materials, such as linearly work-hardening or ideally-plastic ones, and for special applied loadings at the cavity obtained by other workers, in which the nature of the solutions near (r0 , t0 ) are assumed a priori rather than determined, are compared with the results obtained here. Wave propagation in elastic circular membrane is considered by Hutton and Counts [1974]. One is starting from the problem given in Cristescu [1967] Ch. 5. The equations of motion for meridian line of the membrane are ∂2η ξη σ1 ∂η p ∂ω ∂ σ2 − (1 + ε1 ) ξ + η0 2 = η ∂τ p0 ∂η0 ∂η0 1 + ε1 p0 ∂η0 p0 p ∂η ∂ ∂2ω ξ σ1 ∂ω − −η0 2 = η ∂τ p0 ∂η0 ∂η0 1 + ε1 p0 ∂η0 where η and η0 are the actual and initial radial coordinates, ω is the axial coordinate, ε1 , ε2 , ε3 are the meridional, circumferential, normal strains, and σ1 , σ2 , σ3 are the corresponding stress components, p/p0 is the ratio of instantaneous pressure to maximum pressure, τ is the nondimensional time, and ξ = 1 + ε2 . The totally hyperbolic equations are integrated along characteristics. Strain and inertia waves propagate with constant velocities during elastic deformation.

January 12, 2007

392

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Dynamic Plasticity

The buckling problem. Dynamic axisymmetric buckling of circular cylindrical shells struck axially by a mass is studied by Karagiozova and Jones [2000] in order to clarify the initiation of buckling and to prove some insight into the buckling mechanism as a transient process. It is assumed that the material is elastic-plastic with linear strain hardening and displaying the Bauschinger eﬀect. The deformation process is analyzed by a numerical simulation using a discrete model. It is found that the development of the buckling shape depends strongly on the inertia properties of the striker and on the geometry of the shell. A new concept is presented by Karagiozova and Jones [2001], [2002] for the dynamic elastic-plastic axisymmetric buckling of circular cylindrical shells under axial impact. The phenomena of dynamic plastic buckling and dynamic progressive buckling are analyzed from the viewpoint of stress wave propagation resulting from an axial impact. The conditions for the development of dynamic plastic buckling are obtained. It is concluded that shells made of strain rate insensitive materials can respond either by dynamic plastic buckling or dynamic progressive buckling, depending on the inertia properties of the shell, while those shells made of strain rate sensitive materials respond always by dynamic progressive buckling. It is shown that the prediction for the peak load depends on the particular yield criterion used in the analysis. The speeds of the stress waves that can propagate in an elastic-plastic medium with isotropic linear strain hardening in a plane stress state are obtained by Karagiozova [2004] to analyze the inﬂuence of the transient deformation process on the initiation of buckling in square tubes under axial impact. The kinematic conditions across a surface of discontinuity were employed to obtain the stress wave propagation speeds for an initial condition. It is shown that the plastic wave speeds depend on the stress state and on the direction of wave propagation. The material hardening properties have a stronger eﬀect on the speed of the slow plastic wave, while the shear stress aﬀects both the speeds of the fast and slow plastic waves. The magnitude of the instantaneously applied in-plane load at t = 0, which results from an impact in the direction “one”, is obtained as a function of the initial velocity when using the diﬀerential relationship along the characteristics. A general non-dimensional formula based on the dynamic cavity-expansion model is proposed buy Chen and Li [2002] to predict penetration depth into several mediums subjected to a normal impact of a non-deformable projectile. The proposed formula depends on two dimensionless numbers and shows good agreement with penetration tests on metal, concrete and soil for a range of nose shapes and impact velocities. The validity of the formula requires that the penetration depth is larger than the projectile diameter and the projectile nose length while projectile remains rigid without noticeable deformation and damage. A theoretical investigation of plane waves in granular soils is presented by Osinov [1998]. Dynamic equations are derived with the use of the hypoplasticity theory for granular materials. For numerical calculations the material parameters of Karlsruhe sand are used. Wave speeds slopes of characteristics of dynamic equations are calculated for various stresses and densities.

dynamic

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Plastic Waves. Perforation

8.3

dynamic

393

Perforation with Symmetries

For perforation ﬁrst to be seen is the paper by Backman and Goldsmith [1978]. This big paper presents the problem until 1978, characteristics of the projectile and the targets, semi-inﬁnite targets, thin plate penetration and perforation, and thick plates. The problem was considered also by Demiray and Eringen [1978]. By means of a nonlocal viscous ﬂuid model, an investigation is carried out of the problem of penetration of a cylindrical projectile into a plate leading to a failure of the plate by a plug formation. The eﬀect of impact is represented by a uniform initial velocity distribution over a circular region on the surface of the plate. The behavior of this plate material is assumed to be viscous and spatially nonlocal, and only the eﬀects of vertical shearing stress are considered. The expression of stress, velocity and displacement are obtained and the calculated displacement proﬁles are compared with some existing experimental proﬁles. The problem of impact of a liquid cylinder on an elastic-plastic solid was considered by Lush [1991]. He has modiﬁed the model to incorporate the unloading of the plastic wave which is produced by multiple reﬂections of the elastic release wave. In general the agreement between penetration rate, contact pressure and depth of penetration is good. Afterwards, the ballistic strengths of composites are considered mainly in Cheeseman and Bogetti [2003]. First is described a single ﬁber subjected to transverse impact (see Ch. 5). Then is described the mechanisms inﬂuencing ballistic performance. The ﬁbers are Kevlar or Spectra laminates which are impacted with impact velocities up to 1000 m/s. If the cover factors of the fabrics are from 0.6 to 0.95 they are eﬀective in ballistic applications. The crimp that is the undulation on the yarns due to their interlacing in the woven structure is also discussed. Generally is discussed all the factors which have collaboration in the perforation. An oblique penetration was considered by Macek and Duﬀey [2000]. A spherical cavity expansion is assumed with the local velocity normal equal to the penetrator surface VN (see Fig. 8.3.1). Incompressible kinematics is also assumed. The incompressible condition is r∗3 − ri∗3 = r3 − ri3 ,

(8.3.1)

where ∗ refer to the deformed conﬁguration, the other radii to the undeformed conﬁguration. The subscript i refer to the inner surface of the ith layer. The radial displacement is ur = r∗ − r = (ri∗3 + r3 − ri3 )1/3 − r .

(8.3.2)

The radial velocity distribution is obtained from (8.3.2) Vr =

ri∗2 Vi , r∗2

(8.3.3)

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

394

dynamic

Dynamic Plasticity

Fig. 8.3.1

Spherical cavity expansion idealization.

with V the velocity. The radial acceleration is determined by diﬀerentiation: ∗ 2 ∗3 ri ˙ i + 2ri∗ Vi2 1 − ri . (8.3.4) V ar = r∗ r∗2 r∗5 The corresponding spherically symmetric strain ﬁeld as a result of incompressibility is obtained from (8.3.2): εθ =

r∗ r∗ ur = − 1 = ∗3 −1, ∗3 r r (r − ri + ri3 )1/3

(r∗3 − ri∗3 + ri3 )2/3 dur = −1. dr r∗2 The approximated eﬀective strain ﬁeld is εr =

εθ − εr =

R3 r∗3 − r3 r∗3 − r3 = ∗2 ∗3 i ∗3 i 3 1/3 ≈ i ∗3 i . 3 r r r (r − ri + ri )

(8.3.5)

(8.3.6)

(8.3.7)

For a Hooke’s material with spherically symmetry and incompressible, the eﬀective stress is 2 (8.3.8) σe = σθ − σr = E(εθ − εr ) . 3 If the material has yielded and a Mohr–Coulomb yield criterion with damage is used then Y0 (8.3.9) Y = σθ − σr = Y0 + λP , P ≥ − , εθ ≤ εut , λ Y = σθ − σr = λD P ,

εθ > εut ,

(8.3.10)

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Plastic Waves. Perforation

dynamic

395

where εut is the tensile failure strain, P is the pressure, Y0 is the yield stress at zero pressure, λ is the Mohr–Coulomb slope, and λD denotes the slope after failure. The equilibrium equation in the deformed conﬁguration is dσr 2 + ∗ (σr − σθ ) = ρar = ρV˙ r . dr∗ r Combining (8.3.4) and (8.3.11) ∗ 2 dσr 1 2 ri ri∗3 ∗ ˙ . + (σ − σ ) = ρ + 2ρr − V r θ i 1 dr∗ r∗ r∗ r∗2 r∗5

(8.3.11)

(8.3.12)

The governing equation for an elastic sub-layer is found from (8.3.7), (8.3.8) and (8.3.12): ∗ 2 dσr 1 4E ri ri∗3 ∗ 2 ˙ =ρ ∗ − ∗5 + ∗4 (ri∗3 − ri3 ) . (8.3.13) Vi + 2ρri Vi ∗ ∗2 dr r r r 3r The eﬀective stress is 2 ri∗3 − ri3 E . (8.3.14) 3 r∗3 Integrating (8.3.13) with σr = σr0 at r∗ = r0∗ on the outer surface layer, ∗ 1 ri 1 ri∗3 ri∗3 ri∗ ∗ ˙ + ρr − + − − σr (r∗ ) = σr0 + 2ρri∗ Vi2 V i i r0∗ r∗ 4r∗4 4r0∗4 r0∗ r∗ ri3 ri∗3 4E ri∗3 1 − . (8.3.15) − + 9 r0∗3 r∗3 ri∗3 σe =

Putting r¯ = ri∗ /r∗ and r¯0 = ri∗ /r0∗ this equation becomes r¯4 − r¯04 + ρri∗ V˙ i (¯ σr (¯ r ) = σr0 + 2ρVi2 r¯0 − r¯ + r0 − r¯) 4 ri3 4E 3 3 (¯ r − r¯ ) 1 − ∗3 . + 9 0 ri

(8.3.16)

The equivalent pressure is σr + 2σθ . (8.3.17) 3 Using (8.3.7), (8.3.8), (8.3.16) in (8.3.17) the pressure for an elastic layer is ri3 4 P (¯ r ) = −σr − E r¯3 1 − ∗3 9 ri r¯4 − r¯04 + ρri∗ V˙ i (¯ r0 − r¯) = − σr0 + 2ρVi2 r¯0 − r¯ + 4 ri3 4E r¯03 1 − ∗3 . (8.3.18) − 9 ri P (¯ r) = −

The radial stress distribution and pressure depend also on the acceleration term.

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

396

dynamic

Dynamic Plasticity

For a plastic sub-layer the eﬀective stress σe can be written using (8.3.8), (8.3.9), and (8.3.17) as α σe = σθ − σr = Y0 + λP = Y0 − ασr , (8.3.19) λ where α = 3λ/(3 + 2λ). From (8.3.19) we get also α 2 Y0 + σr . (8.3.20) P =− λ 3 Using (8.3.19) in (8.3.12) we get for the plastic sub-layer: ∗ 2 dσr 1 2αY0 2α ri ri∗3 ∗ 2 ˙ + + σ = ρ + 2ρr V − . V r i i i dr∗ r∗ r∗ r∗2 r∗5 λr∗

(8.3.21)

Multiplying with the integrating factor r2α we get: ∗2α−1 r∗3 r∗2α−4 ρr∗2 V˙ i ∗2α−1 Y0 ∗2α r − i + i r σr r∗2α = 2ρRVi2 + r +K. 2α − 1 2α − 4 2α − 1 λ (8.3.22) Applying the boundary condition σr = σrx at the elastic-plastic boundary r∗ = rx∗ we get: # ∗ 2α $ ∗ 2α ri∗3 Y0 rx rx 1 ∗ 2 1− − + σ + 2ρr V σr (r) = rx i i λ r∗ r∗ r∗ (2α − 1) r∗4 (2α − 4) − 2ρri∗ Vi2

rx∗ r∗

2α

ri∗3 ρri∗2 V˙ i 1 1 rx∗2α−1 − + . − ∗2α rx∗ (2α − 1) rx∗4 (2α − 4) 2α − 1 r∗ r (8.3.23)

By non-dimensionalizing the radius r¯x = ri∗ /rx∗ we obtain # 2α $ 2α r¯ r¯ Y0 1− + r) = σrx σr (¯ λ r¯x r¯x

r /¯ rx )2α r /¯ rx )2α r¯4 − r¯x4 (¯ r¯ − r¯x (¯ − 2α − 1 2α − 4 # $ 2α r¯ ρri∗ V˙ i r¯ − r¯x . + 2α − 1 r¯x

+ 2ρVi2

(8.3.24)

Three possible stress states are possible: elastic σe < Y0 + λP , plastic σe = Y0 + λP or pressure-failed P < −Y0 /λ. To determine if the material yields ﬁrst or pressurefails ﬁrst, the expanded radius at which yielding occurs Ry can be compared to the expanded radius at which failure occurs Rf . Setting (8.2.14) equal to the yield stress produces 3 Ry 2 σe = E = Y0 + λP . (8.3.25) 3 r∗

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

dynamic

Plastic Waves. Perforation

397

Using (8.3.18) in (8.3.25) yields Ry3 =

9(Y0 − λσr )r∗3 . (6 + 4λ)E

(8.3.26)

The failure radius Rf is found by setting the pressure given by (8.3.18) equal to the failure pressure: P = −σr −

4ERf3 Y0 =− . ∗3 9r λ

(8.3.27)

Solving for Rf3 : 9r∗3 (Y0 − λσr ) . (8.3.28) 4λE From (8.3.26) and (8.3.28) the material will yield before pressure-failing Ry3 < Rf3 if 1 1 < (8.3.29) 6 + 4λ 4λ because σr < 0. Any real Mohr–Coulomb material 0 < λ < ∞ will yield before pressure-failing. The materials will not pressure-fail after yielding if Y0 α 2 Y0 + σr > − (8.3.30) P =− λ 3 λ or if Y σr < . (8.3.31) λ Since σr < 0 pressure-failure cannot occur. The elastic-plastic interface r¯x is found from the condition that the eﬀective stress σe in the elastic region equals the current yield stress, Y = Y0 + λP . From (8.3.14) and (8.3.18) # 2 3 ri3 r¯x4 − r¯04 2 E r¯ 1 − ∗3 = Y0 + λP = Y0 + λ − σr0 + 2ρVi r¯0 − r¯x + 3 x ri 4 Rf3 =

+ ρri∗ V˙ i (¯ r0

$ ri3 4E r¯03 1 − ∗3 . − r¯x ) − 9 r1

(8.3.32)

Simplifying (8.3.32) we ﬁnd the following equation for r¯x : C1 where

r¯x4 − C¯1 r¯x + C2 r¯x3 − C3 = 0 , 4

(8.3.33)

ri3 2 , C2 = E 1 − ∗3 , C1 = 3 ri 4 ri3 r¯0 4λE r¯03 − r¯0 − λρri∗ V˙ i r¯0 − 1 − ∗3 . C3 = Y0 − λσr0 + 2λρVi2 4 9 ri 2λρVi2

C¯1 = 2λρVi2 + λρri∗ V˙ i ,

Equation (8.3.33) is solved by Newton iteration for 0 < r¯x < 1.

January 12, 2007

398

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

dynamic

Dynamic Plasticity

Further is described a damaged sub-layer, damage-undamaged interface location, stress-based failure, multilayer systems, etc. A comparison with the experiments (data by Longcope and Forrestal [1983]): 162 kg penetrator, 1.56 m long, 0.156 m diameter ogival nose shape (6.0 caliber radius head), impact velocity 520 m/s, impact angle 90◦ , angle of attack of 0◦ , ρ = 1.62×10−9 Mg/mm3 , E = 3.192×103 MPa, Y = 10.0 MPa, λ = 1.00, λd = 1.00. The comparison is very good. Some other comparisons with experimental data are also given. Another spherical cavity-expansion and comparison with experiment is due to Forrestal and Tzou [1997]. A spherically symmetric cavity is expanded from zero initial radius at constant velocity V . For slow enough V , there are three regions of response: an elastic region, a region with radial cracks (the material reaches its tensile strength), and a plastic region (the material reaches its shear strength). The plastic region is bounded by r = V t and r = ct, the cracked region is bounded by r = ct and r = c1 t, and the elastic region is bounded by r = c1 t and r = cd t where r is the radial Eulerian coordinate, t is time and c, c1 , and cd are velocities. In the plastic region a linear pressure-volumetric strain relation and a Mohr–Coulomb yield criterion are satisﬁed: pK(1 − ρ0 /ρ) = Kη p = (σr + σθ + σφ )/3 ; σr − σθ = λp + τ ;

σθ = σφ

(8.3.34)

τ = [(3 − λ)/3]Y

with Y the uniaxial compressive strength, and σr and σθ are the Cauchy stress, positive in compression. In the cracked region σθ = 0. For the elastic incompressible material we have: ∂v 2v ∂σr 2 ∂v ∂v + = 0, + (σr − σθ ) = −ρ0 +v (8.3.35) ∂r r ∂r r ∂t ∂r with v the particle velocity. From (8.3.34) and (8.3.35) we have ∂σr αλσr ατ ∂v ∂v + + = −ρ0 +v ∂r r r ∂t ∂r

(8.3.36)

where α = 6/(3 + 2λ). With dimensionless variables S = σr /τ , U = v/c, ε = V /c and the similarity transformation ξ = r/ct where c is he elastic-plastic interface velocity we have: 2U dS αλS α ρ 0 c2 dU dU dU + = 0, + =− + ξ −U . (8.3.37) dξ ξ dξ ξ ξ τ dξ dξ The boundary condition at the cavity surface is U (ξ = ε) = ε and (8.3.37a) is U = ε3 /ξ 2 . Introducing in (8.3.37b) and multiplying with ξ αλ , we get: d αλ 2ρ0 c2 ε3 αλ−2 2ρ0 c2 ε6 αλ−5 (ξ S) = −αξ αλ−1 − ξ ξ + dξ τ τ

(8.3.38)

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

Plastic Waves. Perforation

dynamic

399

which can be integrated 2ρ0 c2 ε3 1 2ρ0 c2 ε6 1 1 − + + Cξ −αλ (8.3.39) λ τ (αλ − 1) ξ τ (αλ4) ξ 4 where C is the integration constant. Particle velocity is obtained by diﬀerentiating displacement: S=−

3τ 2 3ρ0 c2 , U= + . 3 3ξ Eξ 2Eξ 2 At the elastic and plastic interface the Hugoniot jump conditions hold: S=

ρ2 (v2 − c) = ρ1 (v1 − c) ,

σ2 + ρ2 v2 (v2 − c) = σ1 + ρ1 v1 (v1 − c)

(8.3.40)

(8.3.41)

where 1 and 2 represent the quantities in elastic and plastic regions. For incompressible material ρ1 = ρ2 = ρ0 and radial stress and particle velocity are continuous. From (8.3.41b) we get for 1/3 3τ V = ξ=1:ε= c 2E and 2 −αλ 1 2ρ0 V 2 ε4 ε − + S= ξ − αλ λ τ (1 − αλ)ξ (4 − αλ)ξ 4 2ε3 2ε6 ρ0 c2 3τ + − ξ −αλ . + τ E αλ − 1 αλ − 4 Or the radial stress at the cavity surface: ρ0 V 2 6 2αλ 1−αλ 2 −αλ 1 2ε4αλ ε − ε S(ε) = − + + αλ λ τ (1 − αλ)(4 − αλ) 1 − αλ 4 − αλ (8.3.42) In the elastic-cracked-plastic response σθ = σφ = 0 and the radial stress is ε3 ε6 3 + 2λ −αλ 1 2ρ0 c2 ξ − − − S= λ(3 − λ) λ τ (αλ − 1)ξ (αλ − 4)ξ 4 2ρ0 c2 ε3 ε6 ξ −αλ . (8.3.43) + − τ αλ − 1 αλ − 4 For a compressible target the equations are: ∂σr 2v ∂ρ ∂ρ 2(σr − σθ ) ∂v ∂v ∂v =− , ρ + +v + = −ρ +v ∂r r ∂t ∂r ∂r r ∂t ∂r (8.3.44) Eliminating σθ and ρ we get 2v α ∂σr ∂v ∂σr + =− +v , ∂r r 2K(1 − η) ∂t ∂r ∂σr αλσr ατ ρ0 ∂v ∂v + + =− +v ∂r r r 1 − η ∂t ∂r

(8.3.45)

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

400

dynamic

Dynamic Plasticity

where 6 , α= 3 + 2λ

ατ η= 2K

σr 2 − τ 3

.

Introducing the dimensionless variables S = σr /τ, U = v/c, ε = V /c, β = c/cp , β1 = c1 /cp , βε = V /cp , c2p = K/ρ0 , ξ = r/ct the system of equations becomes dU 2U/ξ + (τ α2 /2Kξ)[(ξ − U )/(1 − η)](λS + 1) = , dξ (αβ 2 /2)[(ξ − U )/(1 − η)]2 − 1 dS α/ξ + αλS/ξ + (2β 2 KU/τ ξ)[(ξ − U )/(1 − η)] = dξ (αβ 2 /2)[(ξ − U )/(1 − η)]2 − 1

(8.3.46)

which are to be solved with the Runge–Kutta method. The radial stress and particle velocity are continuous at the elastic-plastic interface. Thus at ξ = 1 we have S1 = S 2 =

2[(1 − 2v)(1 + γβ) + (1 + v)(γβ)2 ] , 3(1 − 2v)(1 + γβ) − 2λ(1 + v)(γβ)2

3τ (1 + v)(1 − 2v)(1 + γβ) , E[3(1 − 2v)(1 + γβ) − 2λ(1 + v)(γβ)2 ] 2 cp 1+v E(1 − v) γ2 = , c2d = = cd 3(1 − v) (1 + v)(1 − 2v)ρ0

U1 = U2 =

(8.3.47)

with S2 and U2 known, one can calculate the dimensionless radial stress and particle velocity in the plastic region. Further the elastic-cracked-plastic response is calculated and a cavity-expansion numerical results is given for K = 6.7 GPa, Y = 130 MPa, λ = 0.67, E = 11.3 GPa, v = 0.22, f = 13 NPa, ρ0 = 2260 kg/m3 . The penetration equations and comparison with data are reasonable. Dynamic cavity expansion of ceramic materials when subjected to cavity expansion at constant velocity was considered by Satapathy and Bless [2000], Satapathy [2001]. All ﬁve zones are considered: cavity, comminuted zone, radially cracked zone, elastic zone and undisturbed zone (Fig. 8.3.2). For spherical symmetry the conservation equations for mass and momentum in Eulerian coordinates are: 1 ∂ ∂ρ + 2 (ρr2 v) = 0 , ∂t r ∂r σr − σθ ∂σr +2 = −ρ ∂r r The stresses are positive in compression.

∂v ∂v +v ∂t ∂r

.

(8.3.48)

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

Plastic Waves. Perforation

Fig. 8.3.2

dynamic

401

Dynamic response regions in a spherical cavity.

In the elastic region due to spherical symmetry the stresses are ∂u u E (1 − v) + 2v , σr = − (1 + v)(1 − 2v) ∂r r ∂u u E σθ = − v + . (1 + v)(1 − 2v) ∂r r

(8.3.49)

Since the particle velocity is negligible in the elastic region, it is ignored and the equation to be integrated is ∂ 2 u 2 ∂u 2u 1 ∂2u − + = , ∂r2 r ∂r r2 Ce2 ∂t2 where Ce is the dilatational elastic wave seed, and with ξ1 = r/Cc t and u¯1 = u/Cc t this equation becomes 2 ¯ u ¯ d2 u 2 d¯ 2¯ u 2 2d u + − = α ξ , 2 2 dξ1 ξ1 dξ1 ξ1 dξ12

(8.3.50)

with α = Cc /Ce . Forrestal and Luk [1988] have shown that this equation has the solution 1 − 3α2 ξ12 , u ¯ = Aαξ1 − B 3α2 ξ12 where A and B are constants of integration, with 3 α2 (1 − v) 2σf B = − A, A = . 2 ρ0 Cc2 2v(α3 − 1) + 2α3 − 3α2 + 1 In the cracked region only radial stresses are transmitted ∂σr 2σr ∂2u + = −ρ 2 . ∂r r ∂t

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

402

dynamic

Dynamic Plasticity

Since σr = −E

∂u , ∂r

and ξ2 =

r , Cpt

u ¯2 =

u , Cp t

this equation becomes ¯2 u2 d2 u ¯2 d2 u 2 d¯ + = β 2 ξ22 2 , 2 dξ2 ξ2 dξ2 dξ2

Cp β= , Ccr

Ccr =

E ρ

with the following solution u ¯2 = −c1

1 + β 2 ξ22 + c2 ξ2

and c1 =

Y − 1)

E(β 2

,

c2 =

(1 − v)(2α3 − 3α2 + 1) σf γ Y β2γ2 + 1 + . 2 2 γE β − 1 ρ0 Ce 2v(α3 − 1) + 2α3 − 3α2 + 1

For the passage to the next domain the conditions ρ1 (v1 − C) = ρ2 (v2 − C) ,

σ2 − σ1 = ρ1 (C − v1 )(v2 − v1 )

are used. Denoting the volumetric strain in the elastic side η=

α2 (α − 1)(1 − v) ρ0 6σf P =1− =− 2 3 , K ρ ρCe 2α (1 + v) − 3α2 + 1 − 2v

the following relation between α and β is obtained # 2 $ ρ0 Cc − V1 2 2 + σ1 β 2 γ 2 − γ 2 Y (1 − β γ ) 1 − 3K 1 − η1 γ2 =

=

α Ce β Ccr

2

Y (1 − β 2 γ 2 )[1 −

ρ0 Cc −V1 2 3K ( 1−η1 ) ]

+ σ1 β 2 γ 2 − η1 β 2 γ 2 ρ0 [(Ce − V1 )/(1 − η)]2

σ1 − η1 ρ0 [(Ce − V1 )/(1 − η1 )]2

.

The product βγ is function of α only. One assumes that the shear strength increases linearly with the conﬁning pressure σr + 2σθ σr − σθ = λ1 . 2 3 Using this equation in the equation of motion (8.3.48)2 we obtain ∂σr σr ∂v ∂v + 2α ¯ = −ρ +v , (8.3.51) ∂r r ∂t ∂r where α ¯ = 6λ1 /(3 + 4λ1 ). Using the similarity transformation v r u , u ¯3 = and U = , ξ3 = Vt Vt V in the comminuted region, (8.3.51) becomes

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

Plastic Waves. Perforation

dynamic

403

σr dσr dU + 2α ¯ = −ρV 2 (U − ξ3 ) . (8.3.52) dξ3 ξ3 dξ3 One is disregarding dilatancy and compaction and from the mass conservation D1 v= 2 , r where D1 is the constant of integration. This is in non-dimensional quantities 1 (8.3.53) U= 2. ξ3 Inserting it in the Eq. (8.3.52) and integrating, we get 2 D2 ρV 2 2 2α−4 ¯ 2α−1 ¯ ξ ξ + 2α¯ , + σr = − 2α¯ − ξ3 2α ¯−1 3 2α ¯−1 3 ξ3 where D2 is the integration constant. The density for this region is the same as that at the cracked-comminuted boundary ρ = ρ0 /(1 − Y /3K). Denoting the pressure at the cavity surface by Pc , the stress required to maintain the constant cavity expansion velocity is: " 2α−4 ¯ " 2δ 2α−1 3 δ ¯ − + . (8.3.54) Pc ≡ σr "" = Y δ 2α¯ + ρ0 V 2−α ¯ 1 − 2α ¯ (1 − 2α ¯ )(2 − α ¯) ξ3 =1

The quantity δ is related to α and β by 1 . 3[c2 − c1 (1 + β 2 )] The equation in the saturated region becomes dσr dU 4τ + = −ρV 2 (U − ξ3 ) . dξ3 ξ3 dξ3 Integrating this equation with (8.3.53) yields 1 2τ ρV 2 4 Pc = + 4τ ln δ1 + 3+ 4 − . α ¯ 2 δ1 δ1 The application is for the alumina ceramic Coors AD995, for which we have E = 373.14 GPa, K = 231.8 GPa, ρ = 3890 kg/m, and the quasi-static compressive strength Y = 2.62 GPa, and the tensile strength σf = 0.262 GPa. The tungsten projectile for impact velocities up to 3.5 km/s are shown in Fig. 8.3.3. A dynamic spherical cavity expansion in a pressure sensitive elastoplastic medium was considered also by Durban and Masri [2004]. The material behavior is described by the hypoelastic model of the Drucker–Prager material with a nonassociated ﬂow rule, with arbitrary strain-hardening. Simple analytical solutions are given for the fully incompressible elastic/perfectly plastic material with a nonassociated ﬂow rule. A numerical analysis is given for the fully incompressible strain-hardening solid with a non-associated ﬂow rule. In another paper by Gao et al. [2004] one considers the same problem and comparison with experiments, perforation of concrete. The following nine assumptions are given and argued. The medium of concrete can be considered as ideal ﬂuid for high-velocity impact, where the shear modulus is zero, which can satisfy δ3 =

January 12, 2007

10:41

404

Fig. 8.3.3 levels.

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Dynamic Plasticity

Cavity expansion pressure versus penetration velocity for diﬀerent shear-saturation

the needs of engineering analysis for the case of high-velocity and high-pressure. To be compared with the compressive strength, the tensile strength is very little. For high-velocity and high-pressure impacting, the tensile strength can be neglected. During the impact or penetration, the elastic ultimate stress of concrete can be neglected while the wave velocity of elastic stress is very high. There is an ultimate density for concrete during the impact pressing, to which the density of concrete medium can not be increased again for further compressing. A series of experiments had proved that the ultimate density had almost no changes for the higher pressure. During the compressing until ultimate density, the concrete medium subjects to ideal plastic deformation. There is no change of stress. In this process, the air voids are gradually compressed out of the concrete. The wave velocity of stress is zero. The region of medium response will expand in the external normal direction of the projectile surface. In the compressed region, the density and volume of the concrete material have not any more changes. Therefore, the stress wave is constant-volume wave. The thermal conduction can be neglected during impacting. The projectile is non-deformable. The dynamic penetration of the projectile is studied by writing the mass conservation, the momentum conservation and the energy conservation. One is studying the penetration equation and the scabbing produced. The criteria for scabbing is σ ∗ − σ ≥ σs where σ ∗ is the front peak value of the attenuation stress wave, σ is the compressing stress where crack is caused and σs is the tensile stress of concrete. For a parabola nose projectile and concrete with density of ρ = 2400 kg/m3 , with ultimate (the highest) density of ρ∗ = 2640 kg/m3 , the compressive strength

dynamic

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Plastic Waves. Perforation

Fig. 8.3.4

dynamic

405

The measurement and calculation deceleration curves of a projectile in the second test.

σc = 3.0 × 107 N/m2 , mass of the projectile mp = 7.63 kg, the moment of inertia Jp = 0.162 kg/m2 , the friction coeﬃcient µf = 0.1 and the thickness of one target plate is 0.3 m. The plates were 1 m apart and the striking velocity of the projectile is 532 m/s in the ﬁrst series of test and 580 m/s in the second. One has measured the deceleration curve and also the scabbing. The case of three cement plates is shown in Fig. 8.3.4. A new constitutive model for cold compaction of metal powders is developed by Gu et al. [2001]. The plastic ﬂow of metal powders at the macroscopic level is assumed to be representable as a combination of a distortion mechanism, and a consolidation mechanism. For the distortion mechanism the model employs a pressure-sensitive, Mohr–Coulomb type yield condition, and a new physically based non-associated ﬂow rule. For the consolidation mechanism the model employs a smooth yield function which has a quarter-elliptical shape in the mean-normal pressure and the equivalent shear stress plane, together with an associated ﬂow rule. The constitutive model has been implemented in a ﬁnite element program. The material parameters in the constitutive model have been calibrated for MH-100 iron powder by ﬁtting the model to reproduce data from true triaxial compression experiments, torsion ring-shear experiments, and simple compression experiments. The predictive capability of the constitutive model and computational procedure is checked by simulating two simple powder forming processes: (i) a uniaxial strain compression of a cylindrical sample, and (ii) forming of a conical shaped-charge liner. In both cases the predicted load-displacement curves and density variations in the compacted specimens are shown to compare well with corresponding experimental measurements.

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

406

Dynamic Plasticity

The transverse cracks in glass/epoxy cross-ply laminates impacted by projectiles was considered by Takeda et al. [1981]. They started from the glass/epoxy cross-ply laminates impacted by cylindrical projectiles with diﬀerent impactor nose shapes and lengths, a sequential delamination mechanism is dominant, initiated by a generator strip, of with approximately equal to the impactor diameter, cut from the ﬁrst lamina by two through-the-thickness cracks parallel to the ﬁbers of the ﬁrst lamina Cristescu et al. [1975]. They have continued the tests and the impactor velocity for the development of the transverse cracks appears to be independent of the impactor type and to be about 23 m sec−1 . Above this threshold velocity, the mean transverse crack distance decreases sharply as the impactor velocity increases. The curves are eventually ﬂattened out at higher velocities. Another paper about damage of composites is due to Nemes and Sp´eciel [1995]. The problem is mathematically well-posed wave propagation problem, with an unique and stable solution. A big new paper, devoted to a new membrane model for ballistic impact response and V50 performance of multi-play ﬁbrous systems was written by Phoenix and Porwal [2003]. They started with Rakhmatulin and Dem’yanov [1961] equations * u +⊕ 1 ∂2u 1 ∂ (ε = r cos γ) − (8.3.55) t a0 ∂t2 r ∂r r2 and 1 ∂2v 1 ∂ (εt r sin γ) =− (8.3.56) 2 a0 ∂t r ∂r where a0 is reduced to a0 = E/ρ, the symbol [ ]⊕ means the quantity is kept only if positive, and 2 2 ∂u ∂v 1+ + −1 εt = ∂r ∂r is the strain. These equations are discussed and integrated. Ultimately one expresses the threshold projectile velocity V50 above which the membrane fails by perforation 50% of the time, in terms of Cunniﬀ’s dimensionless scaling parameters √ 3 2 3/4 V50 / Ω = 21/3 ε1/12 y max (1 + θ Γ0 )/Kmax where Kmax is accurately represented by 4θ2 Γ0 2 (ψ − 1) Kmax ≈ exp − 3(1 + θ2 Γ0 ) max

1/3 × ψmax

ψmax /εy max (ψmax − 1) ln[1 + ψmax /εy max (ψmax − 1)]

and ψmax ≈

(1 + θ2 Γ0 )/(2θ2 Γ0 )

&2/3

dynamic

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Plastic Waves. Perforation

with

dynamic

407

√ 3 Ω a normalizing velocity and Ω is expressed in yarn (ﬁber) properties as % Ω = (1/2)(σy max εy max /ρy ) Ey /ρy .

The comparison with Kevlar 29, Kevlar KM2, PBO and Spectra 1000 are good. For Kevlar 29, we have σy max ≈ 2.9 GPa, εy max ≈√ 0.034, Ey ≈ 74 GPa, ρy = 3 1440 kg/m3 and producing the normalizing velocity Ω ≈ 624 m/s.. Warren et al. [2004], document the results of a combined experimental, analytical, and computational research program that investigates the penetration of steel projectiles into limestone targets at oblique angles. The striking velocities were 0.4 to 1.3 km/s. In several papers, one have studied the eﬀect of preliminary strain hardening on the ﬂow stress of titanium and a titanium alloy during shock compression by Razoreniv et al. [2005]. The eﬀect of preliminary strain hardening of titanium and a titanium alloy on their mechanical properties under quasi-static and highrate (> 105 s−1 ) loading is studied. Preliminary hardening is accomplished using equal-channel angular pressing and shock waves. High-rate deformation is attained via shock-wave loading of samples. The experimental results show that structural defects weaken the dependence of the yield strength on the strain rate. The diﬀerence in the rate dependence can be so high that the eﬀect of these defects on the ﬂow stress can change sign when going from quasi-static to high-rate loading. The ﬂyer plates were launched at velocities of 0.1–1.23 km/s.

8.4

Modeling of the Taylor Cylinder Impact Test. Anisotropy

The anisotropy of the impact bar was also considered, starting from a simpliﬁed description of the Taylor impacting bar. One has considered the simpliﬁed theory by Hawkyard et al. [1968], Hawkyard [1969], Hutchings [1979] and Jones et al. [1987]. The projectile is deformed by the impact and, from geometrical measurements made before and after impact, the yield stress of the specimen is deduced. Copper and mild steel were ﬁrst considered at various temperatures. The proﬁles predicted of the specimen, after the tests, were afterwards approximated in various ways. A comparison with the measured shape of the specimen after the test is afterwards done. Polymers were also considered with projectiles measured before and after impact. New equation was developed. But again with a schematic illustration of the projectile. In another paper Jones et al. [1991] a simple theoretical analysis of the old problem is presented. The analysis is more complete, but retains the mathematical simplicity of the earlier versions. The major thrust is to separate the material response into two phases. The ﬁrst phase is dominated by strain rate eﬀects and has a variable plastic wave speed. The second phase is dominated by strain hardening eﬀects and has a constant plastic wave speed. Estimates for dynamic yield stress, strain, strain-rate, and plastic wave speed during both phases

January 12, 2007

408

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Dynamic Plasticity

are given. In the paper an example of a cooper specimen impacting a steel anvil with an initial speed of 187 m/s, is given. Experimental techniques are described and illustrated by Nemat-Nasser et al. [1994] for direct measurement of temperature, strain-rate, and strain eﬀects on the ﬂow stress of metals over a broad range of strains and strain rates. Taylor anvil tests are performed, accompanied by high-speed photographic recording of the deformation, and the results are compared with those obtained by ﬁnite-element simulations, leading to ﬁne tuning of parameters in the material’s ﬂow stress. Constitutive models and solution algorithms for anisotropic elastoplastic material strength are developed by Maudlin and Schiferl [1996] for use in the high-rate explicit multi-dimensional continuum mechanics codes. The constitutive modeling is posed in an unrotated material frame using the polar decomposition theorem. Continuous quadratic and discontinuous piecewise yield functions obtained from polycrystal simulations for metallic hexagonal-close-paked and cubic crystal structures are utilized. Associative ﬂow formulations incorporating these yield functions are solved using various solution algorithms; explicit, semi-explicit and geometric normal return schemes are assessed for stability, accuracy and eﬃciency. Isotropic scaling (hardening) of the anisotropic yield surface shapes is included in the modeling. An explosive forming application involving large strain was selected to investigate the eﬀect of using anisotropic materials. Axisymmetric two-dimensional forming simulations were performed for both crystal structures producing resultant formed shapes that are unique to the material’s initial yield anisotropy, and are distinct from isotropic results. Initial axisymetric geometry of a simple explosive forming problem for titanium simulated with the EPIC code, is given. In another paper a new one-dimensional simpliﬁed analysis of the Taylor impact test is presented by Jones et al. [1996]. This analysis diﬀers from any previously presented in that the wave mechanics are separated from the calculation of dynamic stress. The new results utilize post test measurements to estimate key parameters in the plastic wave propagation. However, these measurements are incorporated into the analysis in a very unconventional way. A comparison with continuum code calculations shows very good agreement has been achieved. Simple conservation relationships (jump conditions) in conjunction with postulated material constitutive behavior are applied by Maudlin et al. [1997] to steady plastic strain waves propagating in problems of uniaxial stress and Taylor Cylinder Impact. These problems are simulated with a two-dimensional Lagrangian continuum mechanics code for the purpose of numerically validating the jump relationships as an accurate analytical representation of plastic wave propagation. The constitutive behavior used in this eﬀort assumes isotropy and models the thermodynamic response with a Mie-Grunisen Equation-of-State and the mechanical response with the rate-dependent Johnson-Cook and MTS ﬂow stress models. The jump relationships successfully replicate the results produced by continuum code simulations of plastic wave propagation and provide a methodology for constructing mechanical constitutive models from experimental plastic wave speed information.

dynamic

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Plastic Waves. Perforation

dynamic

409

Comparison are also presented between experimental speeds from Taylor Cylinder Impact tests with jump relationships and continuum code predictions, indicating that the above mentioned ﬂow stress models may not accurately capture plastic wave propagation speeds in annealed and hardened copper. Taylor cylinder impact testing is used by Maudlin et al. [1999] to validate anisotropic elastoplastic constitutive modeling by comparing polycrystal-computed yield-surface shapes (topography) with measured shapes from post-test Taylor specimens and quasi-static compression specimens. Measured yield-surface shapes are extracted from the experimental post-test geometries using classical r-value deﬁnitions modiﬁed for arbitrary stress state and specimen orientation. Rolled tantalum (body-centered-cubic metal) plate and clock-rolled zirconium (hexagonalclose-packed metal) plate are both investigated. The results indicate that an assumption of topography invariance with respect to strain rate is well justiﬁed for tantalum. However, a strong sensitivity of topography with respect to strain rate for zirconium was observed, implying that some accounting for a deformation mechanism rate dependence associated with lower-symmetry materials should be included in the constitutive modeling. Discussion of the importance of this rate dependence and texture evolution in formulating constitutive models appropriate for ﬁnite-element model applications is provided. In another paper by Maudlin et al. [1999] Taylor impact tests using specimens cut from a rolled plate of tantalum were conducted. The tantalum was experimentally characterized in terms of ﬂow stress and crystallographic texture. A piece-wise yield surface was interrogated from an orientation distribution function corresponding to this texture assuming two slip system modes, in conjunction with an elastic stiﬀness tensor computed from the same orientation distribution function and single crystal elastic properties. This constitutive information was used in a code of a Taylor impact test. A forged and round-rolled pure tantalum bar stock was observed by Maudlin et al. [2003] to exhibit large asymmetry in bulk plastic ﬂow response when subjected to large strain Taylor cylinder impact testing. This low-symmetry behavior was analyzed experimentally investigating both the initial stock and the impactdeformed material via x-ray crystallographic texture measurements and automated electron back-scatter diﬀraction scans to establish spatial micro structural uniformity. Polycrystal simulations based upon the 110 measured duplex texture and experimentally inferred deformation mechanisms were performed to project discrete yield surface shapes. Subsequent least squares ﬁtting and eigensystem analysis of the resulting quadratic forth-order tensors revealed strong normal/shear coupling in the yield surface shape. This mixed-mode coupling produces a shearing deformation in the 1–2 impact plane of a Taylor specimen whose axis is coincident with the compressive 3-axis. The resultant deformation generates an unusual rectangular-shaped impact footprint that is conﬁrmed by ﬁnite-element calculations compared to experimental post-test geometries.

January 12, 2007

410

8.5

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Dynamic Plasticity

Analysis of the Steady-State Flow of a Compressible Viscoplastic Medium Over a Wedge (Cazacu et al. [2006])

Penetration mechanics has a long and rich history. Information concerning the stress-time response in the target during penetration is lacking. A comprehensive review of empirical equations for maximum penetration depth in rock, concrete, soil, ice, and marine sediments can be found in Batra [1987], Heuze [1990], Zukas et al. [1990], etc. The maximum penetration depth is expressed as a function of initial impact velocity, penetrator cross-sectional area, penetrator weight, and/or nose geometry. However, in these equations the only target material properties considered are the initial density and unconﬁned strength. A large number of semi-analytical models where penetration is idealized as uniform expansion of a spherical or cylindrical cavity into a semi-inﬁnite target have been proposed. These cavity expansion analyses provide the radial stress at the cavity surface as a function of the cavity velocity and acceleration. This radial stress is considered to be the load on the penetrator and subsequently used in conjunction with equations of motion to calculate the maximum depth of penetration. As emphasized in recent contributions, good agreement between model and data could be expected only if the compressibility and rate sensitivity of the target material are accounted for. In the present section (Cazacu et al. [2006]) I present a new model for calculating the resistance to penetration into geological or geologically derived materials. In the analyses it is assumed that the rate of penetration and all ﬂow ﬁelds are steady as seen from the tip of the penetrator. This hypothesis is supported by penetration tests into cementitious materials (grout, concrete) for impact velocities below 1000 m/s. The shear response of the target material is modeled by a modiﬁed Bingham type viscoplastic equation proposed by Cazacu and Cristescu [2000], Cristescu et al. [2002]. The rationale for adopting such a model is that it accounts for both strain rate and compaction eﬀects on yielding, which are key properties of any porous/brittle material. In the law-pressure regime, a non-linear pressurevolume relationship is considered. Based on experimental observations which show that in the high-pressure regime a very large increase in pressure is necessary to produce even a very small change in density, the hypothesis of a “locking medium” is adopted: the density cannot exceed a critical value. The penetrator is wedgeshaped with high length-over-diameter ratio. Contact between the projectile nose and target is considered to be of Coulomb type with constant friction coeﬃcient, whereas the frictional contact between the remainder of the projectile and target is considered to be slip-rate dependent. Resistance to penetration is calculated for diﬀerent interface conditions between the target and wedge. It is shown that for low to intermediate impact velocities, accounting for friction alters the optimal wedge geometry for penetration performance by blunting the nose. Furthermore, the higher the velocity, the greater the inﬂuence of the nose geometry (wedge semi-angle) on penetration.

dynamic

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Plastic Waves. Perforation

dynamic

411

The deviatoric response of the target material is modeled by a non-homogeneous Bingham type rigid/viscoplastic equation: if IIS ≤ k 2 (ρ) , 0 D = (8.5.1) 1 k(ρ) 1− √ s if IIS > k 2 (ρ) , 2η IIs with the Macauley bracket. The inﬂuence of the degree of compaction on the behavior is modeled through the dependence of the yield limit in shear, k, on the current density ρ. Thus, for stress states satisfying IIS ≤ k 2 (ρ) the model response is rigid, otherwise the model response is viscoplastic. A power law variation of the yield limit with the current density is assumed n ρ0 , (8.5.2) k(ρ) = k0 + β 1 − ρ where ρ0 and k0 = k(ρ0 ) are the density and yield stress of the undeformed medium, respectively, while n and β are material constants. The yield stress k is given in stress units and η in Poise. The stress-volume relationship adopted reﬂects the following experimental observations (see Schmidt [2003]): • in the low to moderate pressure regime, most cementitious materials show a highly non-linear mean stress-volumetric strain response, the reversible decrease in volume being very small, • in the high-pressure regime, a very large increase in pressure is necessary in order to produce even a very small change in volume. Thus, the hypothesis of a “locking medium” applies, i.e., the density cannot exceed a critical value. This critical density, called locking density, is the density at which no volume change occurs under hydrostatic conditions. It will be denoted by ρ∗ and the pressure level at which this density is ﬁrst reached, called locking pressure, is denoted by p∗ . Hence, ρ = ρ0 for p > p∗ while for ρ ≤ ρ∗ , the pressure vs. density relationship p = p(ρ) is assumed to be of the form m ρ p(ρ) = p∗ (8.5.3) ρ∗ where m is a material constant. The relationships (8.5.1)–(8.5.3) could be inverted, to give: k(ρ) p(ρ)I + 2η + √ D for D = 0 , IID σ= (8.5.4) p(ρ)I for D = 0 . Note that the model accounts for both rate dependency and compaction eﬀects on yielding, which are key properties of any cementations or geologic materials. Generally post-test observations of penetration experiments in geologic or cementations materials (grout, concrete) indicate that there are four stages of the

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

412

dynamic

Dynamic Plasticity

Fig. 8.5.1

Schematic of the ﬂow over the wedge.

penetration event. The ﬁrst stage corresponds to nose penetration when the target material is restrained from large movements; the second stage corresponds to chipping and cratering at the point of impact; the third stage occurs when the projectile is fully embedded and the pusher plate hits the target and strips oﬀ while the forth stage occurs when the full length of the projectile is in the penetration channel or tunnel created by the penetrator. The analyses presented here concerns the steady-state ﬂow of the target material over a projectile fully embedded in the target (i.e., forth stage of penetration). The penetrator is considered to be rigid and wedge-shaped. Post-test observations indicate that for impact velocities up to 1000 m/s, penetration paths are relatively straight and stable with regard to the original shotline. Thus, we can assume that the problem is axi-symmetric with respect to the wedge centerline. Let us denote by D = D0 ∪ Dvisco ∪ Df the domain occupied by the penetrator and the target material around it (see Fig. 8.5.1). The lateral extent of this domain is F × R, where R is the wedge semi-height and F is a number estimated from post-test observations. In the domains D0 and Df (i.e., in front of and behind the penetrator), it is assumed that the target material is in rigid body motion while in the domain Dvisco the material undergoes viscoplastic deformation. We further suppose that in Dvisco the ﬂow lines are centered at a certain pole O. Hence, the viscoplastic domain Dvisco is bounded by the nose surface, Γ1 , MP, and the two surfaces S0 and Sf . The surface Sf is of radius OP ≡ rf = (R/sin α)F , while the surface S0 is of radius OM ≡ r0 (R/sin α)(1 + F ) (see Fig. 8.5.1). We assume that there exists velocity discontinuities tangent to the surfaces S0 and Sf , while the components of velocity normal to these surfaces are continuous. Since across S0 ] · n = 0 , [V (8.5.5) with n the outward normal unit vector, it follows that in the viscoplastic domain, Dvisco , the only non-zero velocity component is the radial component, Vr = V cos θ ,

0≤θ≤α

(8.5.6)

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

dynamic

Plastic Waves. Perforation

413

and consequently the only non-zero components of the rate of deformation are Dθθ =

V cos θ r

and Drθ = −

V sin θ 2r

(8.5.7)

The continuity equation reduces to: ∂ (rρ) = 0 . (8.5.8) ∂r Since ρ = ρ0 on S0 , in the viscoplastic domain, r0 (8.5.9) ρ = ρ0 . r Obviously, the compaction law (8.5.9) could also be obtained by imposing that the velocity be the same in the domains D0 and Df (debit compatibility). In the following, we estimate the resistance to penetration based on energy considerations. The wedge semi-angle that minimizes the resistance to penetration is then determined for diﬀerent interface conditions between the wedge and the target. Along the surface of the wedge signiﬁcant friction arises. The mechanics of friction at high sliding speeds is very complex. Much of the work reported is at lower speeds or pressures than those occurring during a penetration event. In view of this, in our analysis we assume that Coulomb friction law applies along Γ1 , the surface area of contact between the nose of the rigid projectile and the target, i.e. τ = µσn ,

(8.5.10)

where τ is the shear stress in the deformed material, µ is a friction coeﬃcient taken as constant, and σn is the normal pressure between the nose and the target material. In plastic forming of metals, when one body is fully plastic and the other is rigid, it is often assumed a friction law of the form (see Avitzur [1968]): √ (8.5.11) τ = µr σY / 3 , where τ is the shear stress in the deformed material, µr is a friction coeﬃcient taken constant and σY is the yield limit of the material. In general, 0 ≤ µr ≤ 1, the case µr = 0 corresponds to “no friction”, while µr = 1 corresponds to adherence of the plastic body to the rigid die wall. Hence, according to the friction law (8.5.11) irrespective of the normal pressure between the two bodies, the shear stress is constant. The density of the target material behind the penetrator is: ρ = ρf √ where ρf = ρ|r=rf while the state of stress is such that IIS = k(ρf ) (i.e., on the yield surface) (see Cristescu [1975]). Thus, it can be assumed that the contact between the rigid penetrator and the compacted material behind the penetrator is described by a law similar to (8.5.11), i.e. τ = µr k(ρf ) .

(8.5.12)

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

414

dynamic

Dynamic Plasticity

The theorem of power expanded is used to compute the resistance to penetration. In the domains D0 and Df no deformation occurs and therefore no internal power dissipation is involved. In the viscoplastic domain, the stress power per unit volume, σ : D can be expressed as (8.5.13) σ : D = σij Dij = 4ηIID + 2k(ρ) IID + p · tr D . Using the work-hardening law (8.5.2) in conjunction with the radial compaction law (8.5.8), we obtain n V 3 + cos2 θ V 2 3 + cos2 θ r + k0 + β 1 − σ:D=η 2 r 3 r0 r 3 m ρ0 r0 m V cos θ . (8.5.14) + p∗ ρ r r Integrating over Dvisco , we arrive at: r0 α ˙ σ : D dV = (σ : D) rdθdr , W = Dvisco

rf

0

or

2 ˙ = η V (7α + sin α cos α) ln r0 W 6 rf # n+1 $ rf r0 V 1− + √ F (α) k0 (r0 − rf ) + β n+1 r0 3 $ m # m−1 V sin α ρ0 r0 r0 −1 (8.5.15) + p∗ m − 1 ρ∗ rf !α√ where F (α) = 0 3 + cos2 θdθ. The surfaces S0 and Sf are surfaces of velocity ˙ !discontinuity. The ! power dissipated at the crossing of these surfaces is: WS0 ,Sf = t · [v ]dA + t · [v ] dA, where t is the stress vector while [v ] is the jump in S0 Sf velocity across the respective surface. Since the magnitude of the tangential jump is V sin θ, we obtain: α ˙ σrθ V sin θr0 dθ t · [v ] dA = WS0 = 0

S0

√ ηV (α − sin α cos α) − r0 k0 V 3F1 (α) , 2 α = −σrθ V sin θrf dθ t · [v ] dA = 2

=− ˙S W f

0

S0

n √ rf ηV (α − sin α · cos α) + k0 + β 1 − V 3F1 (α) 2 r0 2

= where

F1 (α) = 0

α

sin2 θ √ dθ . 3 + cos2 θ

(8.5.16)

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

Plastic Waves. Perforation

dynamic

415

Assuming Coulomb friction [see (8.5.10)] along Γ1 , the surface area of contact between the nose of the rigid projectile and the target, the dissipation due to friction is: rf ˙ (V cos α · σθθ |θ=α ) dr WΓ1 = µ r0

4 V cos α + η ln = µV cos α 3 #

r0 × k0 (r0 − rf ) + β n+1 p∗ + µV cos α m−1

ρ0 ρ∗

r0 rf

+

cos α 4 √ 3 3 + cos2 α

n+1 $ & rf 1− r0 #

r0

r0 rf

m−1

$ −1 .

(8.5.17)

Assuming that the friction law (8.5.11) applies along Γ2 , the surface area of contact between the penetrator and the compacted target material behind it (see Fig. 8.5.1), then ˙ k(ρf )V ds = µr k(ρf )V L , (8.5.18) WΓ2 = µr Γ2

where L is the length of the shank. Next, the resistance to penetration can be computed from energy balance. Consider the control volume V = D0 ∪ Dvisco ∪ Df i.e., in the domain comprised between the planes x = 0 and x = OS and y = 0 and y = F · R, (see Fig. 8.5.1). At steady state, the stress power theorem writes: ˙ S0 + W ˙S +W ˙ Γ1 + W ˙ Γ2 σ : D dV + W f Dvisco

(σb V − σf V ) dA .

=

(8.5.19)

∂V

In (8.5.19), σb denotes the magnitude of the stress vector acting along the direction of the velocity on the boundary of the domain D0 (i.e., in front of the penetrator) while σf is the magnitude of the stress vector acting on the boundary of Df . We may assume that σf = k(ρf ), where ρf is the density of the compacted target material behind the penetrator. Substituting (8.5.14) to (8.5.18) into (8.5.19), we obtain the expression of σb , the resistance to penetration, as: σb =

1 ˙ +W ˙ S0 + W ˙S +W ˙ Γ1 + W ˙ Γ2 + k(ρf )V F R) . (W f V (F + 1)R

(8.5.20)

To illustrate the predictive capabilities of the model, we will apply it to concrete for impact velocities of 300 m/s to 1000 m/s. In an attempt to study the inﬂuence of the frictional contact at the penetrator/target interface on the resistence to penetration for various impact velocities, the friction coeﬃcient µ between the tip of the projectile and target was varied between 0.001 and 0.2. The coeﬃcient of friction

January 12, 2007

416

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Dynamic Plasticity

between the body of the wedge and the target was set to µr = 0.6. The target material parameters involved in Eqs. (8.5.1)–(8.5.3) were assigned numerical values for conctrete material of initial density ρ0 = 2 g/cm3 and unconﬁned compressive strength is of 42.2 MPa. This implies that the pressure range of interest varies from tents of Mega-Pascals (MPa) to the order of a Giga-Pascal (GPa) for a case involving a high-strength steel penetrator. Thus, to characterize the behaviour of the concrete material for pressures representative for the in situ material, quasi-static compression tests were conducted for conﬁning pressures in the range 0–450 MPa using a standard fully automated MTS testing machine at a strain rate of approximately 0.77 · 10−6 /s. To better characterize the time and history eﬀects on the behaviour of the material, in each quasi-static test the loading path considered of several loadingcreep-unloading-reloading cycles. As already mentioned, before passing from loading to unloading, the load was held constant for 10–20 minutes in order to separate viscous eﬀects from unloading. As an example, in Figs. 8.5.2(a) and (b) are shown the results of a tests under σ3 = 200 MPa conﬁnement. The variation of the axial strain rate, ε˙1 with time during the third creep cycle is presented in Fig. 8.5.3 showing that within the load was held constant until the time rate of change of the axial strain approached zero. Note that hysteresis eﬀects were very much reduced thus allowing a rather accurate determination of the elastic parameters from the slopes of the unloading curves. No Hugoniot shock test data were available for

Fig. 8.5.2 Cyclic quasi-static test results under σ3 = 200 MPa: (a) principal stress diﬀerence versus axial strain; (b) principal stress diﬀerence versus radial strain.

dynamic

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Plastic Waves. Perforation

Fig. 8.5.3 pressure.

dynamic

417

Axial strain rate versus time during this 3rd creep cycle under σ3 = 300 MPa conﬁning

this material. Thus, the licking pressure was considered to be p∗ = 0.5 GPa, a value which is based on post-test data on cementious materials. The corresponding locking density ρ∗ is estimated using the relationship 1 ρ∗ = ρ0 1 − εfV where εfV = 0.068 corresponds to the volumetric deformation at failure under conﬁnement 450 MPa. For sake of simplicity, we assume a quadratic dependence of pressure on density [i.e., we set m = 2 in (8.5.3)]. We take the yield limit of the undisturbed medium k(ρ0 ) to be equal to the unconﬁned yield limit, i.e., k(ρ0 ) = 10 MPa. One of the challenges associated with modeling penetration is that the only information that could be gathered during penetration concerns the projectile trajectory and deceleration. To date, there is no in-target instrumentation for measuring deformation during penetration, there is no data from which the yield limit k(ρf ) may be inferred. Thus, we will assume that k(ρf ) = F F · k(ρ0 ), F F being a parameter, which depends on the impact velocity. Setting n = 2 in the law of variation of k(ρ), we estimate the parameter β as k(ρ0 )(F F − 1) . β= (1 − ρ0 /ρf )2 The wedge dimensions are set at: R = 6.35 mm, L = 89 mm. As an example, in Fig. 8.5.4 is shown (σb /p∗ ), the resistance to penetration normalized by the locking pressure, versus the projectile semi-angle α for an impact

January 12, 2007

418

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Dynamic Plasticity

Fig. 8.5.4 Resistance to penetration σb normalized by the locking pressure p∗ as a function of projectile semi-angle α for diﬀerent values of the friction coeﬃcient between the target and the wedge tip; impact velocity V = 300 m/s.

velocity V = 300 m/s. Calculations were done for 4 diﬀerent values of the coeﬃcient of friction between the wedge tip and target material. The yield stress of the compacted target k(ρf ) was considered to be 2.5 k(ρ0 ). Note that irrespective of the contact conditions between the wedge and target, there exists a critical angle for which the resistance to penetration is minimal. All the others parameters being kept the same, the more friction that is present, the blunter the nose required to achieve minimum resistance to penetration (of course, assuming that no erosion takes place and that the nose does not fail). This trend was observed for all impact velocities. The plots of the optimal wedge-angle vs. impact velocity for diﬀerent values of the friction coeﬃcient between the tip and target are presented in Fig. 8.5.5. Since compaction ratios were not available, in the calculations it was assumed that for an impact velocity of 1000 m/s k(ρf )/k(ρ0 ) is double than at 300 m/s impact velocity. The results indicate that at higher impact velocities a sharper nose is required for optimum performance. However, for modest friction (µ = 0.01), the sharpening is minimal. Figure 8.5.6 shows the resistance to penetration corresponding to optimum wedge angle versus the coeﬃcient µ between the wedge tip and target for diﬀerent impact velocities. Irrespective of the contact conditions, an increase in resistance to penetration occurs with increased impact velocity. In an attempt to study the inﬂuence of the frictional contact at the penetrator/target interface on the resistance to penetration for various impact velocities,

dynamic

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Plastic Waves. Perforation

dynamic

419

Fig. 8.5.5 Optimum projectile semi-angle versus impact velocity for various contact conditions between the wedge tip and viscoplastic target.

Fig. 8.5.6 Normalized resistance to penetration corresponding to the optimum projectile semiangle versus the coeﬃcient of friction between the wedge tip and viscoplastic target for various impact velocities.

January 12, 2007

10:41

420

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Dynamic Plasticity

the friction coeﬃcient µ between the tip of the projectile and target was varied between 0.001 and 0.2. The coeﬃcient of friction between the body of the wedge and the target was set to µr = 0.6. It was found that irrespective of the contact conditions between the penetrator and target, there exists a critical angle for which the resistance to penetration is minimal. All the other parameters being kept the same, the more friction that is present, the blunter the nose required to achieve minimum resistance to penetration (of course, assuming that no erosion takes place and that the nose does not fail). This trend was observed for all impact velocities in the range considered 300–1000 m/s. The resistance to penetration at optimal nose angle was found to be greater for higher impact velocity. An theory of optimal nose geometry for a rigid penetrator is due to Jones et al. [1998]. A net force on the nose of a rigid projectile normally penetrating a compliant target is given. The frictional eﬀects are neglected. A comparison of experimental results with simulations over a wide range of stiking velocities (less than 1000 m/s) is giving accurate prediction (Waren and Tabbara [2000]). Bibliography Aliev H. M., 1963, Dokl. Akad. Nauk. SSSR 151, 80–83 (in Russian). Andriankin E. I. and Koryavov V. P., 1959, Shock wave in a plastic medium of variable density, Dokl. Akad. Nauk. SSSR 128, 257–260 (in Russian). Avitzur B., 1968, Metal Forming: Processes and Analysis, Mc Graw Hill, New York. Backman M. E. and Goldsmith W., 1978, The mechanics of penetration of projectile into targets, Int. J. Engng. Sci. 16, 1–99. Batra R. C., 1987, Steady-state penetratration of viscoplastic targets, Int. J. Engng. Sci. 24, 9, 1131–1141. B´eda G., 1997, Constitutive equations and nonlinear waves, Nonlinear Analysis, Theory, Methods & Applications 30, 1, 397–407. Burke J. J. and Weiss V. (eds.), 1971, Shock Waves and the Mechanical Properties of Solids, Syracuse University Press, 417 pp. Campbell J. D. 1972, Dynamic Plasticity of Metals, Springer-Verlag, Wien, 92 pp. Cazacu O. and Cristescu N. D., 2000, Constitutive model and analysis of creep ﬂow of natural slopes, Italian Geo. Journal 34, 3, 44–54. Cazacu O., Ionescu I. R. and Perrot T., 2004, Penetration of a rigid body into a viscoplastic compressible ﬂuid, ECCOMAS 2004, Jyv¨ askyl¨ a, 24–28 July, 2004. Cazacu O., Cristescu N. D. and Schmidt M. J., 2006, Analysis of steady-state ﬂow of a compressible viscoplastic medium over a wedge, Int. J. Num. Anal. Meth. Geomechanics 30, 489–499. Chadwick P., Cox A. D. and Hopkins H. G., 1964, Phil. Trans. Roy. Soc. London A 256, 235–300. Cheeseman B. A. and Bogetti T. A., 2003, Ballistic impact into fabric and compliant composite laminates, Comp. Structures 61, 161–173. Chen X. W. and Li Q. M., 2002, Deep penetration of a non-deformable projectile with diﬀerent geometrical characteristics, Int. J. Impact Engng. 27, 619–637.

dynamic

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Plastic Waves. Perforation

dynamic

421

Chernyshov A. D., 1966, On the character of strong jumps in certain complex media, PMM J. Appl. Math. Mech. 30, 6, 1226–1232 (in Russian). Cristescu N., 1967, Dynamic Plasticity, North-Holland, 614 pp. Cristescu N., 1975, Plastic ﬂow through conical converging dies, using a viscoplastic constitutive equation, Int. J. Mech. Sci. 17, 425–433. Cristescu N., 1980, On the optimum die angle in fast wire drawing, J. Mech. Working Tech. 3, 275–287. Cristescu N. D., 2000, A model of stability of slopes, in Slope Stability 2000. Proceedinds of Sessions of Geo-Denver 2000, Griﬃths D. V., Fenton G. A. and Martin T. R. (eds.), Geotechnical Special Publication 101, 86–98. Cristescu N., Malvern L. E. and Sierakowski R. L., 1975, Failure mechanisms in composite plates impacted by blunt-ended penetrators, foreign object impact damage to composites, American Society for Testing and Materials, ASTM, STP 568, 159–172. Cristescu N. D., Craciun E. M. and So´ os E., 2003, Mechanics of Elastic Composites, Chapman & Hall/CRC, 682 pp. Cristescu N. D., Cazacu O. and Cristescu C., 2002, A model for slow motion of natural slopes, Canadian Geotechnical Journal 39, 4, 924–937. Davids N. (ed)., 1960, International Symposium on Stress Wave Propagation in Materials, Interscience Pub., 337 pp. Davids N. (ed)., 1969, Stress Wave Propagation in Materials, Intern. Sympo., Pennsylvania, Inter. Sci., New York–London. Demiray H. and Eringen A. C., 1978, A nonlocal model for plug formation in plates, Int. J. Engng. Sci. 16, 287–297. Durban D. and Masri R., 2004, Dynamic spherical cavity expansion in a pressure sensitive elastoplastic medium, Int. J. Solids Struct. 41, 5697–5716. Ezra A. A., 1973, Principles and Practice of Explosive Metalworking, Industrial Newspapers Limited, 270 pp. Fomin V. M. and Kiselev S. P., 1997, Elastic-Plastic Waves in Porous Materials, in High-Pressure Shock Compression of Solids IV, Davison L., Horie Y. and Shahinpoor M. (eds.), Springer, 205–232. Forrestal M. J. and Luk V. K., 1988, Dynamic spherical cavity-expansion in a compressible elastic-plastic solid, J. Appl. Mech. 55, 2, 275–279. Forrestal M. J. and Tzou D. Y., 1997, A spherical cavity-expansion penetration model for concrete targets, Int. J. Solids Struct. 34, 31–32, 4127–4146. Gao S., Jin L. and Liu H., 2004, Dynamic response of a projectile perforating multi-plate concrete targets, Int. J. Solids Struct. 41, 4927–4938. Grigorian S. S., 1959, On the general equations of the dynamics of soils, Dokl. Acad. Nauk. SSSR 124, 285–288 (in Russian). Grigorian S. S., 1960a, On the ﬁnal deﬁnition on the motion of soils, Prikl. Mat. Mech. 24, 651–662 (in Russian). Grigorian S. S., 1960b, On the fundamental representation of the dynamics of soils, Prikl. Mat. Mech. 24, 6, 1057–1072 (in Russian). Grigorian S. S., 1967, Some problems of mathematical theory of deformation and failure of solid soils, Prikl. Mat. Mech. 31, 643–669 (in Russian). Gu C., Kim M. and Anand L., 2001, Constitutive equations for metal powders: application to powder forming processes, Int. J. Plasticity 17, 147–209. Hawkyard J. B., 1969, A theory for the mushrooming of ﬂat-ended projectiles impinging on a ﬂat rigid anvil, using energy considerations, Int. J. Mech. Sci. 11, 313–333.

January 12, 2007

422

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Dynamic Plasticity

Hawkyard J. B., Eaton D. and Johnson W., 1968, The mean dynamic yield strength of cooper and low carbon steel at elevated temperatures from measurements of the “mushrooming” of ﬂat-ended projectiles, Int. J. Mech. Sci. 10, 929–948. Heuze F. E., 1990, An overview of projectile penetration into geological-materials, with emphasis on rocks, Int. J. Rock Mech. Min. Sci. 27, 1–14. Hutchings I. M., 1979, Estimation of yield stress in polymers at high strain-rates using G. I. Taylor’s impact technique, J. Mech. Phys. Solids 26, 289–301. Hutton D. V. and Counts J., 1974, Wave propagation in an elastic circular membrane subjected to impulsive pressure loading, J. Appl. Mech. Trans. ASME 41, 1, 290–291. Ishlinskii A. Yu., 1954, Ukr. Mat. Zh. 6, 430–441 (in Russian). Ishlinskii A. Yu., Zvolinskii N. V. and Stepanenko I. A., 1954, Dokl. Akad. Nauk. SSSR 95, 729–731 (in Russian). Johnson G. R. and Holmquist T. J., 1988, Evaluation of cylinder-impact test data for constitutive model constants, J. Appl. Phys. 64, 8, 3901–3910. Jones S. E., Gillis P. P. and Foster J. C. Jr., 1987, On the equation of motion of the undeformed section of a Taylor impact specimen, J. Appl. Phys. 61, 2, 499–502. Jones S. E., Gillis P. P., Foster J. C. Jr and Wilson L. L., 1990, A one-dimensional, two-phase ﬂow model for Taylor impact specimens, Trans. ASME, J. Engn. Mat. Tech. 113, 228–235. Jones S. E., Maudlin P. J. and Foster J. C. Jr, 1996, An engineering analysis of plastic wave propagation in the Taylor test, Int. J. Impact Engng. 19, 2, 95–106. Jones S. E., Rule W. K., Jerome D. M. and Klug R. T., 1998, On the optimal nose geometry for a rigid penetrator, Comp. Mech. 22, 413–417. Karagiozova D., 2004, Dynamic buckling of elastic-plastic square tubes under axial impact — I: stress wave propagation phenomenon, Int. J. Impact Engng. 30, 143–166. Karagiozova D. and Jones N., 2000, Dynamic elastic-plastic bucling of circular cylindrical shell under axial impact, Int. J. Solids Struct. 37, 2005–2034. Karagiozova D. and Jones N., 2001, Inﬂuence of stress waves on the dynamic progressive and dynamic plastic buckling of cylindrical shell, Int. J. Solids Struct. 38, 6723–6749. Karagiozova D. and Jones N., 2002, On dynamic buckling phenomena in axially loaded elastc-plastic cylindrical shells, Int. J. Non-Lin. Mech. 37, 1223–1238. Koiter W. T., 1953, Stress–strain relations, uniqueness and variational theorems for elastic-plastic materials with a singular yield surface, Quart. Appl. Math. 11, 350–354. Kolsky H. and Prager W., 1964, Stress Waves in Anelastic Solids, Springer-Verlag, 342 pp. Kompaneets A. S., 1956, Dokl. Akad. Nauk. SSSR 109, 49–52 (in Russian). Lee L. H. H., 1975, Bifurcation and uniqueness in dynamics of elastic-plastic continua, Int. J. Engng. Sci. 13, 1, 69–76. Longcope D. B. and Forrestal M. J., 1983, Penetration of targets describet by a Mohr Coulomb failure criterion with a tension cutoﬀ, J. Appl. Mech. 50, 327–333. Lush P. A., 1991, Comparison between analytical and numerical calculations of liquid impact on elastic-plastic solid, J. Mech. Phys. Solids 39, 1, 145–155. Macek R. W. and Duﬀey T. A., 2000, Finite cavity expansion method for near-surface eﬀects and layering during earth penetration, Int. J. Impact Engng. 24, 239–258. Maudlin P. J. and Schiferl S. K., 1996, Computational anisotropic plasticity for high-rate forming applications, Comput. Methods Appli. Mech. Engrg. 131, 1–30. Maudlin P. J., Foster J. C. Jr. and Jones S. E., 1997, A continuum mechanics code analysis of steady plastic wave propagation in the Taylor test, Int. J. Impact Engng. 19, 3, 231–256.

dynamic

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Plastic Waves. Perforation

dynamic

423

Maudlin P. J., Gray III G. T., Cady C. M. and Kaschner G. C., 1999, High-rate material modelling and validation using the Taylor cylinder impact test, Phil. Trans. R. Soc. Lond. A 357, 1707–1729. Maudlin P. J., Bingert J. F., House J. W. and Chen S. R., 1999, On the modeling of the Taylor cylinder impact test for orthotropic textured materials: experiments and simulations, Int. J. Plasticity 15, 139–166. Maudlin P. J., Bingert J. F. and Gray III G. T., 2003, Low-symmetry plastic deformation in BCC tantalum: experimental observations, modeling and simulations, Int. J. Plasticity 19, 483–515. Medvedeva N. S. and and Shemiankin E. I., 1961, J. Appl. Mech. Tech. Phys. 6, 78–87. Nemat-Nasser S., Li Y.-F. and Isaacs J. B., 1994, Experimental/computational evaluation of ﬂow stress at high strain rates with application to adiabatic shear banding, Mech. of Mat. 17, 111–134. Nemes J. A. and Sp´eciel E., 1995, Use of a rate-dependent continuum damage model to describe strain-softening in laminated composites, Comp. Structures 58, 6, 1083–1092. Osinov V. A., 1998, Theoretical investigation of large-amplitude waves in granular soils, Soil Dynamics Earthquake Engn. 17, 13–28. Phoenix S. L. and Porwal P. K., 2003, A new membrane model for the ballistic impact response and V50 performance of multi-play ﬁbrous systems, Int. J. Solids Struct. 40, 6723–6765. Prager W., 1953, On the use of singular yield conditions and associated ﬂow rules, J. Appl. Mech. 20, 3, 317–320. Pytel A. and Davids N., 1963, A viscous model for plug formation in plates, J. Franklin Inst.-Engineering Appl. Math. 276, 5, 394–406. Razorenov S. V., Savinykh A. S., Zaretsky E. B., Kanel G. I. and Kolobov Yu. R., 2005, Eﬀect of preliminary strain hardening on the ﬂow stress of titanium and titanium alloy during shock compression, Physics of the Solid State 47, 4, 663–669. Rakhmatulin Kh. A. and Dem’yanov Yu. A., 1961, Strength under High Transient Loads (English translation, Israel Program for Scientiﬁc Translations, 1966). Rakhmatulin H. A. and Stepanova L. I., 1958, On the propagation of explosion shock waves in sols, in: The Problems of Destruction of Rocks by Explosion (Moscow) 149–159 (in Russian). Rakhmatulin H. A., Sagomonian A. Yu. and Alekseev N. A., 1964, The Problems of Dynamics of Soils (Izv. MGU, Moscow) (in Russian). Rinehart J. S., 1975, Stress Transients in Solids, HyperDynamics, 230 pp. Sagomonian A. Yu., 1961, One-dimensional motion of soils with spherical, cylindrical and plane waves, in: Dynamics of Soils, No. 44 (Moscow), 43–87 (in Russian). Salvadori M. G., Skalak R. and Weidlinger R., 1955, Trans. N.Y. Acad. Sci. Ser. II 21, 427–434. Satapathy S., 2001, Dynamic spherical cavity expansion in brittle ceramics, Int. J. Solids Struct. 38, 5833–5845. Satapathy S. S. and Bless J. S., 2000, Cavity expansion resistance of brittle materials obeying a two-curve pressure-shear behavior, J. Appl. Phys. 88, 7, 4004–4012. Schmidt M. J., 2003, High Pressure and High Strain Rate Behaviour of Cementitious Materials: Experiments and Elastic/Viscoplastic Modeling, PhD dissertation, University of Florida. Schmidt M. J., Cazacu O., Ross C. A. and Cristescu N. D., 2001, Dynamic behaviour of mortar: experimental data and modeling, Proceedings of the 10th International Conference on Computer Methods and Advances in Geomechanics, Tucson, Arizona.

January 12, 2007

424

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Dynamic Plasticity

Shemiankin E. I., 1961, J. Prikl. Mech. Tech. Fiz. 5, 91–99 (in Russian). Shewmon P. G. and Zackay V. F., 1961, Response of Metals to High Velocity Deformation, Intersience Publishers, 491 pp. Srinivasan M. G. and Ting T. C. T., 1974, Initiation of spherical elastic-plastic boundaries due to loading at a spherical cavity, J. Mech. Phys. Solids 22, 415–435. Takeda N., Sierakowski R. L. and Malvern L. E., 1981, Transverse cracks in glass/epoxy laminates impacted by projectiles, J. Material Sci. 16, 7, 2008–20011. Warren T. L. and Tabbara M. R., 2000, Simulations of the penetration of 6061-T6511 aluminum targets by spherical-nosed VAR 4340 steel projectiles, Int. J. Solids Struct. 37, 4419–4435. Warren T. L., Hanchak S. J. and Poormon K. L., 2004. Penetration of limestone targets by ogive-nosed VAR 4340 steel projectiles at oblique angles: experiments and simulations, Int. J. Imp. Engineering 30, 1307–1331. Zhu G., Goldsmith W. and Dharan C. K. H., 1992, Penetration of laminated Kevlar by projectiles — I. Experimental investigation. Int. J. Solids Struct. 29, 4, 399–420. Zukas J. A., Nichols T., Greszczuk L. B. and Curran D. R., 1990, Impact Dynamics, Wiley, New York, 155–214. Zukas J. A., 2004, Introduction to Hydrocodes, Elsevier.

dynamic

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

Chapter 9

Hypervelocity Impact (Information)

9.1

Introduction

Several papers were published in the last years about hypervelocity impact. It seems that the beginning is a big paper by Al’tshuler [1965]; it is a review paper containing everything which was done up to this year (shock adiabats and their experimental registration, methods of obtaining semiempirical equation of state, shock adiabats, speed of sound and isentropic elasticity of shock-compressed bodies, on the composition of the earth’s core and the mantle, dynamic strength of materials, etc.). A paper by Alekseevskii [1966] is devoted to penetration of a rod with high velocity; the main ideas and schemes are given an example is computed for the velocity of 1470 m/s. Then is the paper by Tate [1967]. A modiﬁed hydrodynamic theory which takes some account of strength eﬀects is used to predict the deceleration of a long rod after striking a target. The results are then compared with experimental data from X-ray observation. The Bernoulli equation is used. The theory of long rod penetration as given in a previous paper is extended by Tate [1969] to take into account of the deformation of a soft rod against a rigid target and the penetration of a rigid projectile into a soft target. It is shown that it is theoretically possible to have a decrease in depth of penetration with increasing impact velocity, and a method for deducing the average radius of the hole is given. The Bernoulli equation is again given for materials which behave as a ﬂuid. A semi-inﬁnite solenoid in a uniform velocity ﬂow ﬁeld is used by Tate [1986], as a model for the quasisteady primary phase of long rod penetration. Assumptions: the materials to be incompressible, to obey a Mises yield criterion, when yielding the materials are perfectly plastic, the Levy–Mises ﬂow law applies, the materials are eitherelastic or plastic, a modiﬁed Bernoulli equation is established. In another paper Tate [1990] is proposing a segmented rod to explain penetration; the projectile is ﬁred up to 1800 m/s. Allen and Rogers [1961] study the penetration of metal rods into semi-inﬁnite metal targets. They have investigated experimentally at velocities up to 0.3 cm/µs. Results are compared with predictions from the hydrodynamic theory of jet penetration. Experimental results indicate that the eﬀective yield strength is relatively 425

dynamic

January 12, 2007

426

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Dynamic Plasticity

independent of the strength of the rod. The hydrodynamic theory of penetration was determined to be generally acceptable except where the density of the jet is much greater than that of the target. The impact ﬂash jet initiation phenomenology was considered by several authors. Shaped charge theory predicts that a jet will form when the impact angle between two colliding surfaces is greater than an initiation angle criterion which is a function of material properties and impact velocity. Because the eﬀective impact angle continuously sweeps over a range of values as a spherical particle impacts a ﬂat target, this jet initiation angle criterion is satisﬁed at some point during the penetration process. A simple model has been developed by Ang [1990] which predicts the jet initiation from either the target or the particle material. The hypervelocity impact of a projectile upon a thin metal plate and subsequent formation of back-surface debris is reviewed by Anderson et al. [1990]. At suﬃciently high impact velocities, roughly greater than 3.0 km/s, shock formation and interaction dominate and control the overall response of both the projectile and the target plate. The authors focus upon the importance of shock heating, melting, and vaporization in the application. They also assess the current status of computational modeling of this kind of impact event, speciﬁcally addressing recent work bearing on the sensitivity of such modeling to the equations of state and certain numerical issues. More accurate data in multi-dimensional experiments may be able to resolve the question of what are the major causes of diﬀerences between calculations and experiments. The theory is summarized and the origins of the target resistance term are examined by Anderson and Walker [1991]. Numerical simulations were performed of a tungsten-alloy, long-rod projectile into a semi-inﬁnite hardened steel target at three impact velocities suﬃciently high to result in projectile erosion (impact velocity apt to 1.5 km/s). The constitutive responses of the target and projectile were varied parametrically to assess the eﬀects of strain hardening, strain-rate hardening, and thermal softening on penetration response. The results of one of the numerical simulations were selected to compare and contrast in detail with the predictions of the Tate model. A computational study was performed by Anderson et al. [1993a] to quantify the eﬀects of strain rate on replica-model experiments of penetration and perforation. The impact of a tungsten-alloy, long-rod projectile into an armor steel target at 1.5 km/s was investigated. It was found that over a scale factor of 10, strain-rate eﬀects change the depth of penetration, for semi-inﬁnite targets, and the residual velocity and length of projectile, for ﬁnite-thickness targets, by an order of 5%. Although not modeled explicitly in the present study, the time-dependence of damage was examined. Damage accumulation is a strong function of absolute time, not scaled time. At homologous times, a smaller scale will have less accumulated damage than a larger scale; therefore, the smaller scale will appear stronger, particularly in situation where the detailes of damage evolution are important.

dynamic

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Hypervelocity Impact (Information)

dynamic

427

The penetration resistance of hard layers, such as ceramics and hardened steels, struck by high velocity long rod projectiles can be characterized by the depth of penetration tests (Bless and Anderson [1993]). The depth of penetration tests can be used to calculate average penetration resistance. The tests can also be used to compute diﬀerential eﬃciency. Implications for the eﬀectiveness of hypervelocity penetration (for 2–5 km/s) are that the optimum velocity for energy eﬃcient penetration will be much higher for hard materials than for conventional armor steel. Furthermore, ceramics will continue to substantially outperform armor steels, while high hardness steels will lose their relative advantages against long rod projectiles above 3 km/s. Numerical simulations are used by Anderson et al. [1993b] to examine long-rod penetration as a function of impact velocity. Similarities and diﬀerences between the penetration histories are analyzed, including penetration and tail velocities, penetration depths, crater radii, centerline interface pressures, and the extends of plastic ﬂow in the projectile and target. The Tate’s Bernoulli equation is used 1 1 ρp (v − u)2 + Yp = ρt u2 + Rt 2 2 where Yp is the ﬂow stress of the projectile, and Rt is deﬁned as the target resistance in the one-dimensional formulation, v is the projectile (tail) velocity, u is the penetration (interface) velocity. The one-dimensional modiﬁed Bernoulli theory is often used to examine long-rod penetration into semi-inﬁnite targets, and integral to the theory is a term that describes the resistance of the target to penetration. It is shown that the hydrodynamic theory gives smaller penetration velocities. The impact velocities are 1.5–4.5 km/s. One is also observing that the target resistance decreases with impact velocity, and it is shown that this is a consequence of both the residual phase of penetration and variations in the size of the plastic zone ﬁeld. Calculations of steel target penetration by L/D ≤ 1 tungsten and tungsten alloy projectiles have been extended to L/D = 1/32 over the velocity range 1.5 to 5 km/s by Orphal et al. [1993]. L is the projectile length and D the projectile diameter. The ratio of crater to projectile diameter tends to 1 as L/D decreases over this entire velocity range. For impact velocities of 1.5 and 3 km/s, penetration depth normalized by projectile length increases with decreasing projectile L/D up to a maximum value and then decreases for still lower L/D. Experiments at impact velocities of 2 and 3 km/s conﬁrm these results. For 5 km/s impact velocity, the calculations show P/L increasing (P depth of penetration) with decreasing projectile L/D over the entire range 1/32 ≤ L/D ≤ 1. Comparison with the experiments by Bjerke et al. [1992] is also done. Walker and Anderson [1995] found that in general the time histories of penetration predicted by the Tate model can be in good agreement with those computed from numerical simulations. However, discrepancies exist between the model and numerical simulations at the beginning and at the end of penetration. From insights provided by numerical simulations, assumptions are made concerning the velocity

January 12, 2007

428

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Dynamic Plasticity

and stress proﬁles in the projectile and the target. Using these assumptions, the time-dependent, cylindrically-symmetric, axial momentum equation is explicitly integrated along the centerline of the projectile and target to provide the equation of motion. The model requires the initial interface velocity — which can be found, for example, from the shock jump conditions — and material properties of the projectile and target to compute the time history of penetration. Agreement between the predictions of this one-dimensional, time-dependent penetration model is in good agreement with experimental results and numerical simulations. Analytic penetration modeling usually relies on either a momentum balance or an energy-rate balance to predict depth of penetration by a penetrator based on initial geometry and impact velocity. Based on the ﬂow ﬁeld and constitutive assumptions it is then possible to derive a momentum or an energy-rate balance. In another paper Walker et al. [1995] is presented the results of impact tests, as well as discusses the shaped charge design modiﬁcations for the nickel and molybdenum launchers. Radiographs are presented of impacting projectiles, as are post test photographs of various targets. The data are unique in that they represent low L/D projectile impacts into both monolithic blocks and spaced plates at velocities above 10 km/s. The aluminum projectiles are being launched at 11.25±0.20 km/s, the molybdenum projectiles at 11.72 ± 0.10 km/s, and the nickel projectiles at 10.81 ± 0.10 km/s. The impact data for aluminum agree well with trends seen at lower velocity light gas gun testing and scaled approaches. The paper by Walker [2001] examines the use of assumed ﬂow ﬁelds within a target created by impact and then examines the resulting predicted behavior based on either momentum conservation or energy conservation. It is shown that for the energy rate balance to work, the details of energy transfer mechanisms must be included in the model. In particular, how the projectile energy is initially transferred into target kinetic energy and elastic compression energy must be included. As impact velocity increases, more and more energy during the penetration event is temporarily deposited within the target as elastic compression and target kinetic energy. This energy will be dissipated by the target at a later time, but at the time of penetration it is this transfer of energy that deﬁnes the forces acting on the projectile. Thus, for an energy rate balance approach to successfully model penetration, it must include the transfer of energy into kinetic energy within the target and the storage of energy by elastic compression. Understanding the role of energy dissipation in the target clariﬁes the various terms in analytic models and identiﬁes their origin in terms of the fundamental physics. Understanding the modes of energy transfer also assists in understanding the hypervelocity result that penetration depth only slowly increases with increasing velocity even through the kinetic energy increases as the square of the velocity. At ordnance velocities (1.0–1.9), there is a pronounced decrease in penetration eﬃciency, as measured by P/L, when projectiles of larger L/D are used, as mentioned by Anderson et al. [1995b]. The inﬂuence of L/D on penetration is

dynamic

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Hypervelocity Impact (Information)

dynamic

429

refered to the L/D eﬀect. They numerically examine the L/D eﬀect at higher velocities, from 2.0 km/s to 4.5 km/s. It is found that as the velocities increases, there is a change in mechanism for the L/D eﬀect. At ordnance velocities the L/D eﬀect is mostly due to the decay in penetration velocity during the steady-state region of penetration. At higher velocities, the steady-state region of penetration shows no L/D dependence, and the L/D eﬀect is due primarily to the penetration of the residual rod at the end of the penetration event. This change in mechanism is related to the change in slope of the penetration-versus-impact velocity for eroding projectiles. Anderson et al. [1995a] study in a paper the penetration behavior of tungsten alloy, long-rod penetrators into high-hard steel, at two impact velocities 1.25 km/s and 1.70 km/s. The positions of the nose and tail of the projectile were measured by means of a 600 kV ﬂash X-ray system at diﬀerent times during penetration. The experiments were numerically simulated. The computational results are in very good agreement with the experimental position-time data. The computational results by Lawrence et al. [1995] are discussed and compared with new experimental observations obtained at an impact velocity of ∼ 10 km/s. In the experiment, the debris cloud was generated by the impact of a plate-shaped titanium projectile with a thin titanium shild. When 0.76 mm diameter tungsten rods impact AD995 Alumina at velocities up to 3.5 km/s, Subramanian and Bless [1995] show that penetration and consumption velocities are approximately linear functions of impact velocity. At 3.5 km/s, the penetration falls below the hydrodynamic limit by 15%. Neither the primary penetration nor the total penetration (i.e., ﬁnal depth of penetration) reached the limiting value of 2.23 suggested by hydrodynamic theory. The residual penetration, which is the diﬀerence between the total and primary penetration, was almost zero at 3 to 3.5 km/s. This suggests that the ceramic retains considerable strength ahead of the penetrator/target interface. Primary penetration approaches 75% of the hydrodynamic limit. A systematic study is decribed by Chhabildas et al. [1995], has led to the successful launch of thin ﬂier plates to velocities of 16 km/s. The energy required to launch a ﬂier plate to 16 km/s is approximately 10 to 15 times the energy required to melt and vaporize the plate. In the experiments by Brannon and Chhabildas [1995], a thin plate of zinc is impacted by a tantalum ﬂier plate at speeds ranging from 8 to 10.1 km/s, producing pressures from 3 Mbar to over 5,5 Mbar and temperatures as high as 39000 K. Such high pressures produce essentially full vaporization of the zinc. Trucano and Chhabildas [1995] used the Sandia Hypervelocity Launcher to get velocities in excess of 10 km/s. In the ﬁrst experiment the launch of an intact 0.33 gram titanium alloy chunk ﬂier to a velocity of 10.2 km/s. In a paper by Anderson et al. [1996a] one is considering the ballistic impact experiments which were performed on ceramic laminate targets at three scale sizes,

January 12, 2007

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

10:41

430

Dynamic Plasticity

normally 1/3, 1/6 and 1/12, to quantify the eﬀects of scale on various responses, in particular, the ballistic limit velocity. Some of the measured quantities showed little or no dependence on scale size, whereas other quantities, particularly the ballistic limit velocity, were found to vary with scale size. The impact velocities are up to 2.69 km/s. The ballistic limit velocity VBL is Vr =

0 ≤ Vs ≤ VBL

0, a(Vsp

−

p 1/p VBL )

,

Vs > VBL

where Vr , Vs and VBL are the residual, striking (impact), and limit velocities. In another paper by Orphal et al. [1996] a series of 26 terminal ballistics experiments was performed to measure the penetration of simple conﬁned aluminum nitride targets by a long tungsten rod. Impact velocities ranged from 1.5 to about 4.5 km/s. Penetrator diameter D was 0.762 mm. From the data u = dp/pt = speed of penetration into the target and vc = d(L − Lr )/dt = speed of “consumption” of the long rod were obtained. In a paper by Anderson et al. [1996], a common measure of penetration eﬃciency is given by the depth of penetration P into a semi-inﬁnite target normalized by the original length of the projectile L. It has been known for many years that P/L depends upon the aspect ratio L/D for projectiles with relatively small aspect ratios, e.g. 1 ≤ L/D ≤ 10. This inﬂuence of L/D on penetration is referred to as the L/D eﬀect. Although observed, the L/D eﬀect for large aspect ratio rods is not as well documented. Further, published penetration equations have not included the L/D eﬀect for high aspect ratio rods. The authors have compiled a large quantity of experimental data that permits the quantiﬁcation of the L/D eﬀect for projectiles with aspect ratios of 10 ≤ L/D ≤ 30. Numerical simulations reproduce the observed experimental behavior; thus, no new physics is required to explain the phenomenon. The numerical simulations allow investigation of the fundamental mechanics leading to a decrease in penetration eﬃciency with increasing aspect ratio. In a paper by Piekutowski et al. [1996] one is studying the perforation experiments of 26.3 mm thick aluminum plates and 12.9 mm diameter, 88.9 mm long, ogive-nose steel rods. For normal and oblique impacts with striking velocities between 280 and 860 m/s, one is measuring the residual velocities and displayed the perforation process with X-ray photographs. They have developed perforation equations that accurately predict the ballistic limit and residual velocities. Forty terminal ballistics experiments were performed by Orphal et al. [1997] to measure the penetration of simple conﬁned boron carbide targets by long tungsten roads. Impact velocities ranged from 1.5 to about 5.0 km/s. For tests with velocities 1.493 ≤ v ≤ 2.767 km/s, the penetrator diameter was 1.02 mm. For tests with impact velocities v ≥ 2.778 km/s the penetrator diameter was 0.762 mm. For tests in the velocity range 2.335 < v < 2.761 km/s both penetrator sizes were used. The penetration velocity u is found to depend linearly on the impact velocity u = 0.757v − 0.406.

dynamic

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Hypervelocity Impact (Information)

dynamic

431

The shock-wave compression of brittle solids was studied by Grady [1998]. Extensive experimental investigation in the form of large-amplitude, nonlinear wave-proﬁle measurements which manifest the shock strength and equation-of-state properties of brittle solids has been performed. The results of experiments performed to determine a complete set of independent elasic constants and the eﬀect of shock-induced shear strain on the delamination strength of a glass-ﬁber-reinforced plastic composite is due to Dandecar et al. [1998]. Two analytical models for the crater size generated by long-rod and thick-walled tube projectiles are presented by Lee and Bless [1998]. The ﬁrst is based on energy; in a steady-state penetration, the kinetic energy loss of a projectile is related to the total energy deposited in the target. This simple approach provides an upper bound for the crater size. The second approach is based on the observation that two mechanisms are involved in cavity growth due to long projectiles: ﬂow of projectile erosion products, which exerts radial stress on the target and opens a cavity, and radial momentum of the target as it ﬂows around the projectile nose. The speed of impact is less than 5 km/s. This analysis includes the centrifugal force exerted by the projectile, radial momentum of the target, and the strength of the target. Thus, it can estimate the extent of cavity growth due to projectile mushrooming, which cannot be predicted by other analyses. This model is shown to be in good agreement with experimental data. Yaw has been known to generally inﬂuence the penetration performance of long-rod projectiles. Experiments have shown that even small angles of yaw can signiﬁcantly degrade performance. The experiments by Bless et al. [1999] have shown that even small angles of yaw can signiﬁcantly degrade performance. The authors show that a critical feature of a yawed impact is the transverse load on the penetrator. Transverse loads tend to decrease the misalignment of rod axis and velocity vector. They use classical cavity expansion theory to quantify the impact transients and determine the magnitude of the transverse load. Then, a steady-state slot-cutting model is used to calculate the shape and orientation of a projectile that exits a ﬁnite plate. They found that this is contrary to the ﬁndings of some previous studies considered. The strength pf the projectile may be ignored compared to the inertial loads even at the relatively high impact velocities. The theory agrees well with reverse impact experimental data on ﬁnite plate. Two and three-dimensional numerical simulations have been conducted by Anderson et al. [1999b] to help better understand the penetration and perforation of chemical submunition targets by tungsten-alloy long-rod projectiles. In particular, the computational results are analyzed to assess modeling assumptions in the application of the modiﬁed Bernoulli model of Tate to this class of problems. For the study, the chemical submunitions were treated as long steel cylinders ﬁlled with water. Impacts near the submunitions ends were neglected. Many of the simulations conducted looked at rod penetration through two successive submunitions. For

January 12, 2007

432

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Dynamic Plasticity

purposes of the computational study, the cylinders were idealized as ﬂat plates. The study considered three impact obliquities (60◦ , 70◦ and 80◦ ) and two impact velocities (2.0 and 4.0 km/s). Penetration velocities, erosion rates, and the eﬀects of a ﬁnite projectile diameter were investigated as a function of obliquity and impact velocity. Experimental data by Anderson et al. [1999a] show that penetration velocities and instantaneous penetration eﬃciencies fall below that expected from hydrodynamic theory, even at impact velocities as high as 4.0 km/s. For steel rod impacting an aluminum target, the hydrodynamic penetration velocity is achieved only at impact velocity of about 4 km/s. Numerical simulations, using appropriate strength values, are in excellent agreement with the experimental data. Parametric studies demonstrate that both projectile and target strength have a measurable eﬀect even at such high impact velocities. The ballistic performance of 17 penetrator materials, representing 5 distinct steel alloys treated to various hardnesses along with one tungsten alloy, has been investigated by Anderson et al. [1999]. Residual length and velocities, as well as the ballistic limit velocities, were determined experimentally for each of the alloy types for length to diameter (L/D) ratio 10 projectiles against ﬁnite-thick armor steel targets. An equation for the residual velocity VR in terms of the impact velocity VP and ballistic limit is m 1/m VR VP =a −1 VBL VBL were VBL is the ballistic limit velocity, was used. The target thickness normalized by the projectile diameter (T/D) was 3.55. For some of the projectile types, a harder target, with the same thickness, was also used. It was found that the ballistic limit velocity decreases signiﬁcantly when the projectile hardness exceeds that of the target. Numerical simulations are used to investigate some of the observed trends. It is shown that the residual projectile length is sensitive to projectile hardness; the numerical simulations reproduce this experimental observation. The results of experiments showed that the residual velocity either increased or remained approximately constant as the projectile strength was increased. It is assumed that the plastic work per unit volume is approximately a constant, that is, there is a trade oﬀ between strength and ductility. An Eulerian wave code was used by Anderson et al. [1999d] to simulate the impact, penetration, and detonation of a 23-mm highexplosive projectile into a water-ﬁlled tank. The pressure-time response is compared with results from an experiment. Computed peak pressures and impulses compare well with the experimental values. Orphal and Anderson [1999] report a direct observation of the streamline reversal of eroded rod material proposed by Allen and Rogers [1991]. Allen and Rogers suggested that the turning of high-velocity long-rod penetrator material at the target interface could be viewed as a reversal of the direction of a streamline with

dynamic

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Hypervelocity Impact (Information)

dynamic

433

only a change of sign in the velocity. Allen and Rogers’ streamline reversal model has two important consequences. First the eroded debris has a speed of vd = 2u − v relative to the target, where v is the impact velocity and u is the speed of penetration of the rod relative to the target. Secondly, a consequence of this formula is that the length of the rod debris, is given by the diﬀerence in the initial length of the rod and the remaining length of the rod. Results of a time-resolved experiment for a tungsten penetrator into a polycarbonate target at 3.61 km/s and a corresponding numerical simulation are consistent with streamline reversal. Numerical simulations are then used in a parametric study to investigate the eﬀects of various density relations between penetrator and target materials. The dimensions of holes produced by the impact of aluminum spheres with various thicknesses and aluminum sheets are presented and analyzed by Piekutowski [1999]. The sphere diameters ranged from 3.18 mm to 19.05 mm and the bumper sheet thickness to projectile diameter ratio, ranged from 0.026 to 0.504 with the majority of the tests having this ratio of less than 0.234. Impact velocities ranged from 1.98 km/s to 7.23 km/s. As this ratio is increased the holes tended to be less circular. Piekutowski et al. [1999] performed a series of depth of penetration experiments using 7.11 mm diameter, 71.12 mm long ogive-nose steel projectiles and 254 mm diameter aluminum targets. The projectiles had a nominal mass of 0.021 kg and were launched with striking velocities between 0.5 and 3.0 km/s. Post test radiographs of the targets showed three diﬀerent regions of penetrator response as the striking velocity increased: (1) the projectiles remained rigid and visibly undeformed; (2) the projectiles deformed during penetration without nose erosion, deviated from the target centerline, and exited the side of the target of turned severely within the target; and (3) the projectiles eroded during penetration and lost mass. Similar experiments have been done with spherical nose steel projectiles by Forestal and Piekutowski [2000]. Goldsmith [1999] has published a very big review paper on the subject. Everything published until 1999 is mentioned: background and scope, oblique impact, yaw impact, impact with yaw and obliquity, moving targets, rotating penetrators, tumbling impact, impingement of jets or long rods with relative target motion, ricochet, and conclusions-status on non-standard projectile impact. He is also mentioning the rate of the impact velocities: subordnance v0 < 500 m/s, ordnance 500 < v0 < 1500 m/s, ultraordnace 1.5 < v0 < 3 km/s, and hypervelocity v0 > 3 km/s. The references are also quite big, starting with Euler and continuing to 367 references. See also Batra and Lin [1988]. Powder guns or a two-stage, light-gas launched the projectiles at normal impacts to striking velocities between 0.4 and 1.9 km/s, by Frew et al. [2000]. In addition, an analytical penetration equation that described the target resistance by its density and a strength parameter determined from depth of penetration versus striking velocity data, is also done.

January 12, 2007

10:41

434

9.2

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Dynamic Plasticity

Further Studies

The process of long-rod penetration into thick metallic targets is examined by Rosenberg and Dekel [2001] through a series of two-dimensional simulations. The aim of the research presented, is to uncover the inherent material similarities in this process. In particular, the search is for non-dimensional parameters which account for the depth of penetration, such as the density ratio, and the relative strengths of penetrator and target. The velocity of impact is less than 7 km/s. The simulation results are in accord with existing empirical data, shedding more light on the penetration process and emphasizing the diﬃculties in achieving an overall normalization procedure for this process. Target hole sizes and geometries were measured for a series of highly oblique hypervelocity impacts of steel spheres against thin laminated targets by Orphal and Anderson [2001]. The impact velocity was nominally 4.6 km/s for most of the experiments with a few tests conducted at 7.3 km/s. Impact obliquity ranged from 60◦ to 80◦ from the normal to the target plane. Projectiles were stainless steel spheres with masses of 222 g, 25 g, and 1 g. Targets were laminated MX-2600 silica phenolic bonded to a 2024-T3 substrate. Target thickness was varied to give thickness to projectile diameter 0.6 and 0.3 for each projectile. The normal penetration of a deformable projectile into an elastic-plastic target is considered by Roisman et al. [2001]. The force imposed on the projectile by the target is generally a complex function of the strength of the target material, the projectile velocity, its diameter and shape, as well as the instantaneous penetration depth. When this force exceeds a certain critical value the projectile begins to deform. At moderate to high values of the impact velocity, the projectile’s tip material ﬂows plastically with large deformations causing the formation of a mushroom-like conﬁguration. This process is accompanied by erosion of the projectile material. In the rear, elastic, part of the projectile the deformation remain small and the region can be approximated as a rigid body being decelerated by the projectile’s yield stress. The general model allows one to predict the penetration depth, the projectile’s eroded length and the crater diameter. It has been shown that in the limit of very high impact velocities the present model reduces to the well-known form of the hydrodynamic theory of shaped-charge jet. Also, a simpliﬁed asymptotic formula for the crater radius has been derived which includes the eﬀect of the target’s yield stress and compares well with experimental data for very high impact velocities. The paper by Lynch et al. [2001] presents scale size ﬁrings of two novel shape KE penetration into a steel/ceramic/steel target at four velocities between 1.8 and 2.9 km/s. The two novel shapes were a three piece segment rod and a telescopic rod/tube. Two unitary rod designs were also included in the assessment. All the penetrators had a similar mass of 60 grams. Test data against semi-inﬁnite rolled homogeneous armor was used to obtain the mass eﬀectiveness of the ceramic target

dynamic

January 12, 2007

10:41

Book Title: Dynamic Plasticity (9.75 in × 6.5 in)

Hypervelocity Impact (Information)

dynamic

435

for each rod shape and velocity. The performance rankings of the penetrators against the ceramic target were found to be similar to those for semi-inﬁnite rolled homogeneous armor. Hydrocode analysis of the experiments gave some valuable insights into the penetration processes of the two novel penetrator designs. Predicted depth of penetration compared very well with experimental values, but enhancements to the physics of the ceramic model are needed in order to simulate cover plate eﬀects. Tests surpassing 11 km/s have been reported by Reinhart et al. [2001]. The temperature, and hence the density of the ﬂyer-plate is also well known prior to impact. In a paper by Hari Manoj Simha et al. [2002] is described the computational modeling of the penetration response of a high-putity ceramic, namely the AD99.5 alumina. This material is the most widely investigated ceramic, and extensive materials testing and ballistic data are available. The model development is based on constitutive relationships inferred from bar impact and plate impact data. A novel element removal scheme for ceramics is presented, and the code is then used to investigate the penetration response of AD-99.5 alumina in the depth of penetration and semi-inﬁnite conﬁgurations. The computations are found to be in excellent agreement with the experimental results. The impact velocities are smaller than 3.5 km/s. A pulse shaping techniques to obtain compressive stress–strain data for brittle materials with the split Hopkinson pressure bar apparatus is presented by Frew et al. [2002]. The conventional split Hopkinson pressure bar apparatus is modiﬁed by shaping the incident pulse such that the samples are in dynamic stress equilibrium and have nearly constant strain rate over most of the test duration. A thin disk of annealed or hard copper is placed on the impact surface of the incident bar in order to shape the incident pulse. Analytical models and data that show a wide variety of incident strain pulses are produced by varying the geometry of the copper disks and the length and striking velocity of the striker bar. A model that corrects for the added sabot mass and shows good agreement with experiments conducted with high-strength steel striker and incident bars is presented by Forrestal et al. [2002]. They point out that this added sabot mass eﬀect will be even more pronounced with titanium, aluminum or magnesium bars. In another paper Piekutowski [2003] study the impact tests using aluminum bumper sheets ranging from 0.076 mm to 4.80 mm thick and impact velocities ranging from 1.98 to 7.19 km/s used to determine the fragmentation initiation threshold for aluminum spheres impacting at hypervelocity. Tests using 0.53 mm and 12.70 mm diameter aluminum spheres indicated that the fragmentation initiation threshold velocity scaled with the bumper-thickness projectile diameter ratio. When a conventional split Hopkinson pressure bar is used to investigate the dynamic ﬂow behavior of ductile metals, Chen et al. [2003] observe that the results at small strain (ε

Our partners will collect data and use cookies for ad personalization and measurement. Learn how we and our ad partner Google, collect and use data. Agree & close